MECHANICS OF SOLIDS AND MATERIALS Mechanics of Solids and Materials intends to provide a modern and integrated treatmen...
298 downloads
1994 Views
6MB Size
Report
This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!
Report copyright / DMCA form
MECHANICS OF SOLIDS AND MATERIALS Mechanics of Solids and Materials intends to provide a modern and integrated treatment of the foundations of solid mechanics as applied to the mathematical description of material behavior. The book blends both innovative topics (e.g., large strain, strain rate, temperature, timedependent deformation and localized plastic deformation in crystalline solids, and deformation of biological networks) and traditional topics (e.g., elastic theory of torsion, elastic beam and plate theories, and contact mechanics) in a coherent theoretical framework. This, and the extensive use of transform methods to generate solutions, makes the book of interest to structural, mechanical, materials, and aerospace engineers. Plasticity theories, micromechanics, crystal plasticity, thin ﬁlms, energetics of elastic systems, and an overall review of continuum mechanics and thermodynamics are also covered in the book. Robert J. Asaro was awarded his PhD in materials science with distinction from Stanford University in 1972. He was a professor of engineering at Brown University from 1975 to 1989, and has been a professor of engineering at the University of California, San Diego since 1989. Dr. Asaro has led programs involved with the design, fabrication, and fullscale structural testing of large composite structures, including highperformance ships and marine civil structures. His list of publications includes more than 170 research papers in the leading professional journals and conference proceedings. He received the NSF Special Creativity Award for his research in 1983 and 1987. Dr. Asaro also received the TMS Champion H. Mathewson Gold Medal in 1991. He has made fundamental contributions to the theory of crystal plasticity, the analysis of surface instabilities, and dislocation theory. He served as a founding member of the Advisory Committee for NSF’s Ofﬁce of Advanced Computing that founded the Supercomputer Program in the United States. He has also served on the NSF Materials Advisory Committee. He has been an afﬁliate with Los Alamos National Laboratory for more than 20 years and has served as consultant to Sandia National Laboratory. Dr. Asaro has been recognized by ISI as a highly cited author in materials science. Vlado A. Lubarda received his PhD in mechanical engineering from Stanford University in 1980. He was a professor at the University of Montenegro from 1980 to 1989, Fulbright fellow and a visiting associate professor at Brown University from 1989 to 1991, and a visiting professor at Arizona State University from 1992 to 1997. Since 1998 he has been an adjunct professor of applied mechanics at the University of California, San Diego. Dr. Lubarda has made signiﬁcant contributions to phenomenological theories of large deformation elastoplasticity, dislocation theory, damage mechanics, and micromechanics. He is the author of more than 100 journal and conference publications and two books: Strength of Materials (1985) and Elastoplasticity Theory (2002). He has served as a research panelist for NSF and as a reviewer to numerous international journals of mechanics, materials science, and applied mathematics. In 2000 Dr. Lubarda was elected to the Montenegrin Academy of Sciences and Arts. He is also recipient of the 2004 Distinguished Teaching Award from the University of California.
Mechanics of Solids and Materials ROBERT J. ASARO University of California, San Diego
VLADO A. LUBARDA University of California, San Diego
cambridge university press Cambridge, New York, Melbourne, Madrid, Cape Town, Singapore, São Paulo Cambridge University Press The Edinburgh Building, Cambridge cb2 2ru, UK Published in the United States of America by Cambridge University Press, New York www.cambridge.org Information on this title: www.cambridge.org/9780521859790 © Robert Asaro and Vlado Lubarda 2006 This publication is in copyright. Subject to statutory exception and to the provision of relevant collective licensing agreements, no reproduction of any part may take place without the written permission of Cambridge University Press. First published in print format isbn13 isbn10
9780511147074 eBook (NetLibrary) 0511147074 eBook (NetLibrary)
isbn13 isbn10
9780521859790 hardback 0521859794 hardback
Cambridge University Press has no responsibility for the persistence or accuracy of urls for external or thirdparty internet websites referred to in this publication, and does not guarantee that any content on such websites is, or will remain, accurate or appropriate.
Contents
Preface
page xix
PART 1: MATHEMATICAL PRELIMINARIES
1 Vectors and Tensors 1.1. Vector Algebra 1.2. Coordinate Transformation: Rotation 1.3. 1.4. 1.5. 1.6. 1.7. 1.8. 1.9. 1.10. 1.11. 1.12. 1.13. 1.14. 1.15. 1.16. 1.17. 1.18. 1.19.
1.20. 1.21. 1.22. 1.23.
of Axes SecondRank Tensors Symmetric and Antisymmetric Tensors Prelude to Invariants of Tensors Inverse of a Tensor Additional Proofs Additional Lemmas for Vectors Coordinate Transformation of Tensors Some Identities with Indices Tensor Product Orthonormal Basis Eigenvectors and Eigenvalues Symmetric Tensors Positive Deﬁniteness of a Tensor Antisymmetric Tensors 1.16.1. Eigenvectors of W Orthogonal Tensors Polar Decomposition Theorem Polar Decomposition: Physical Approach 1.19.1. Left and Right Stretch Tensors 1.19.2. Principal Stretches The Cayley–Hamilton Theorem Additional Lemmas for Tensors Identities and Relations Involving ∇ Operator Suggested Reading
1 1 4 5 5 6 7 7 8 9 10 10 11 12 14 14 15 15 17 19 20 21 21 22 23 23 25 v
vi
Contents
2 Basic Integral Theorems 2.1. Gauss and Stokes’s Theorems 2.1.1. Applications of Divergence Theorem 2.2. Vector and Tensor Fields: Physical Approach 2.3. Surface Integrals: Gauss Law 2.4. Evaluating Surface Integrals 2.4.1. Application of the Concept of Flux 2.5. The Divergence 2.6. Divergence Theorem: Relation of Surface to Volume 2.7. 2.8.
Integrals More on Divergence Theorem Suggested Reading
3 Fourier Series and Fourier Integrals 3.1. Fourier Series 3.2. Double Fourier Series 3.2.1. Double Trigonometric Series 3.3. Integral Transforms 3.4. Dirichlet’s Conditions 3.5. Integral Theorems 3.6. Convolution Integrals 3.6.1. Evaluation of Integrals by Use of Convolution 3.7. 3.8. 3.9. 3.10.
Theorems Fourier Transforms of Derivatives of f (x) Fourier Integrals as Limiting Cases of Fourier Series Dirac Delta Function Suggested Reading
26 26 27 27 28 29 31 31 33 34 35 36 36 37 38 39 42 46 48 49 49 50 51 52
PART 2: CONTINUUM MECHANICS
4 Kinematics of Continuum 4.1. Preliminaries 4.2. Uniaxial Strain 4.3. Deformation Gradient 4.4. Strain Tensor 4.5. Stretch and Normal Strains 4.6. Angle Change and Shear Strains 4.7. Inﬁnitesimal Strains 4.8. Principal Stretches 4.9. Eigenvectors and Eigenvalues of Deformation Tensors 4.10. Volume Changes 4.11. Area Changes 4.12. Area Changes: Alternative Approach 4.13. Simple Shear of a Thick Plate with a Central Hole 4.14. Finite vs. Small Deformations 4.15. Reference vs. Current Conﬁguration 4.16. Material Derivatives and Velocity 4.17. Velocity Gradient
55 55 56 57 58 60 60 61 62 63 63 64 65 66 68 69 71 71
Contents
4.18. 4.19. 4.20. 4.21. 4.22. 4.23. 4.24. 4.25. 4.26. 4.27. 4.28. 4.29.
vii Deformation Rate and Spin Rate of Stretching and Shearing ˙ vs. D Material Derivatives of Strain Tensors: E Rate of F in Terms of Principal Stretches 4.21.1. Spins of Lagrangian and Eulerian Triads Additional Connections Between Current and Reference State Representations Transport Formulae Material Derivatives of Volume, Area, and Surface Integrals: Transport Formulae Revisited Analysis of Simple Shearing Examples of Particle and Plane Motion Rigid Body Motions Behavior under Superposed Rotation Suggested Reading
5 Kinetics of Continuum 5.1. Traction Vector and Stress Tensor 5.2. Equations of Equilibrium 5.3. Balance of Angular Momentum: Symmetry of σ 5.4. Principal Values of Cauchy Stress 5.5. Maximum Shear Stresses 5.6. Nominal Stress 5.7. Equilibrium in the Reference State 5.8. Work Conjugate Connections 5.9. Stress Deviator 5.10. Frame Indifference 5.11. Continuity Equation and Equations of Motion 5.12. Stress Power 5.13. The Principle of Virtual Work 5.14. Generalized Clapeyron’s Formula 5.15. Suggested Reading 6 Thermodynamics of Continuum 6.1. First Law of Thermodynamics: Energy Equation 6.2. Second Law of Thermodynamics: Clausius–Duhem 6.3.
6.4.
6.5. 6.6. 6.7.
Inequality Reversible Thermodynamics 6.3.1. Thermodynamic Potentials 6.3.2. Speciﬁc and Latent Heats 6.3.3. Coupled Heat Equation Thermodynamic Relationships with p, V, T, and s 6.4.1. Speciﬁc and Latent Heats 6.4.2. Coefﬁcients of Thermal Expansion and Compressibility Theoretical Calculations of Heat Capacity Third Law of Thermodynamics Irreversible Thermodynamics 6.7.1. Evolution of Internal Variables
74 75 76 78 81 82 83 84 85 87 88 89 90 92 92 94 95 96 97 98 99 100 102 102 107 108 109 111 111 113 113 114 116 116 118 119 120 121 122 123 125 127 129
viii
Contents
6.8. Gibbs Conditions of Thermodynamic Equilibrium 6.9. Linear Thermoelasticity 6.10. Thermodynamic Potentials in Linear Thermoelasticity 6.10.1. Internal Energy 6.10.2. Helmholtz Free Energy 6.10.3. Gibbs Energy 6.10.4. Enthalpy Function 6.11. Uniaxial Loading and Thermoelastic Effect 6.12. Thermodynamics of Open Systems: Chemical 6.13. 6.14. 6.15. 6.16. 6.17. 6.18.
Potentials Gibbs–Duhem Equation Chemical Potentials for Binary Systems Conﬁgurational Entropy Ideal Solutions Regular Solutions for Binary Alloys Suggested Reading
7 Nonlinear Elasticity 7.1. Green Elasticity 7.2. Isotropic Green Elasticity 7.3. Constitutive Equations in Terms of B 7.4. Constitutive Equations in Terms of Principal Stretches 7.5. Incompressible Isotropic Elastic Materials 7.6. Elastic Moduli Tensors 7.7. Instantaneous Elastic Moduli 7.8. Elastic Pseudomoduli 7.9. Elastic Moduli of Isotropic Elasticity 7.10. Elastic Moduli in Terms of Principal Stretches 7.11. Suggested Reading
129 130 132 132 133 134 135 136 139 141 142 143 144 145 147 148 148 150 151 152 153 153 155 155 156 157 158
PART 3: LINEAR ELASTICITY
8 Governing Equations of Linear Elasticity 8.1. Elementary Theory of Isotropic Linear Elasticity 8.2. Elastic Energy in Linear Elasticity 8.3. Restrictions on the Elastic Constants 8.3.1. Material Symmetry 8.3.2. Restrictions on the Elastic Constants 8.4. Compatibility Relations 8.5. Compatibility Conditions: Cesaro ` Integrals 8.6. Beltrami–Michell Compatibility Equations 8.7. Navier Equations of Motion 8.8. Uniqueness of Solution to Linear Elastic Boundary Value Problem
8.8.1. 8.8.2. 8.9.
Statement of the Boundary Value Problem Uniqueness of the Solution Potential Energy and Variational Principle 8.9.1. Uniqueness of the Strain Field
161 161 163 164 164 168 169 170 172 172 174 174 174 175 177
Contents
8.10. Betti’s Theorem of Linear Elasticity 8.11. Plane Strain 8.11.1. Plane Stress 8.12. Governing Equations of Plane Elasticity 8.13. Thermal Distortion of a Simple Beam 8.14. Suggested Reading 9 Elastic Beam Problems 9.1. A Simple 2D Beam Problem 9.2. Polynomial Solutions to ∇ 4 φ = 0 9.3. A Simple Beam Problem Continued 9.3.1. Strains and Displacements for 2D Beams 9.4. Beam Problems with Body Force Potentials 9.5. Beam under Fourier Loading 9.6. Complete Boundary Value Problems for Beams 9.6.1. Displacement Calculations 9.7. Suggested Reading 10 Solutions in Polar Coordinates 10.1. Polar Components of Stress and Strain 10.2. Plate with Circular Hole 10.2.1. Far Field Shear 10.2.2. Far Field Tension 10.3. Degenerate Cases of Solution in Polar Coordinates 10.4. Curved Beams: Plane Stress 10.4.1. Pressurized Cylinder 10.4.2. Bending of a Curved Beam 10.5. Axisymmetric Deformations 10.6. Suggested Reading 11 Torsion and Bending of Prismatic Rods 11.1. Torsion of Prismatic Rods 11.2. Elastic Energy of Torsion 11.3. Torsion of a Rod with Rectangular Cross Section 11.4. Torsion of a Rod with Elliptical Cross Section 11.5. Torsion of a Rod with Multiply Connected Cross Sections 11.5.1. Hollow Elliptical Cross Section 11.6. Bending of a Cantilever 11.7. Elliptical Cross Section 11.8. Suggested Reading 12 SemiInﬁnite Media 12.1. Fourier Transform of Biharmonic Equation 12.2. Loading on a HalfPlane 12.3. HalfPlane Loading: Special Case 12.4. Symmetric HalfPlane Loading 12.5. HalfPlane Loading: Alternative Approach 12.6. Additional HalfPlane Solutions
ix 177 178 179 180 180 182 184 184 185 186 187 188 190 193 196 198 199 199 201 201 203 204 206 209 210 211 213 214 214 216 217 221 222 224 225 227 228 229 229 230 232 234 235 237
x
Contents
12.6.1. Displacement Fields in HalfSpaces 12.6.2. Boundary Value Problem 12.6.3. Speciﬁc Example 12.7. Inﬁnite Strip 12.7.1. Uniform Loading: −a ≤ x ≤ a 12.7.2. Symmetrical Point Loads 12.8. Suggested Reading 13 Isotropic 3D Solutions 13.1. DisplacementBased Equations of Equilibrium 13.2. Boussinesq–Papkovitch Solutions 13.3. Spherically Symmetrical Geometries 13.3.1. Internally Pressurized Sphere 13.4. Pressurized Sphere: StressBased Solution 13.4.1. Pressurized Rigid Inclusion 13.4.2. Disk with Circumferential Shear 13.4.3. Sphere Subject to Temperature Gradients 13.5. Spherical Indentation 13.5.1. DisplacementBased Equilibrium 13.5.2. Strain Potentials 13.5.3. Point Force on a HalfPlane 13.5.4. Hemispherical Load Distribution 13.5.5. Indentation by a Spherical Ball 13.6. Point Forces on Elastic HalfSpace 13.7. Suggested Reading 14 Anisotropic 3D Solutions 14.1. Point Force 14.2. Green’s Function 14.3. Isotropic Green’s Function 14.4. Suggested Reading 15 Plane Contact Problems 15.1. Wedge Problem 15.2. Distributed Contact Forces 15.2.1. Uniform Contact Pressure 15.2.2. Uniform Tangential Force 15.3. DisplacementBased Contact: Rigid Flat Punch 15.4. Suggested Reading 16 Deformation of Plates 16.1. Stresses and Strains of Bent Plates 16.2. Energy of Bent Plates 16.3. Equilibrium Equations for a Plate 16.4. Shear Forces and Bending and Twisting Moments 16.5. Examples of Plate Deformation 16.5.1. Clamped Circular Plate 16.5.2. Circular Plate with Simply Supported Edges
238 239 240 242 243 244 245 246 246 247 248 249 251 252 253 254 254 255 256 257 258 259 261 263 264 264 264 268 270 271 271 274 275 277 277 279 280 280 281 282 285 287 287 288
Contents
xi
16.5.3. Circular Plate with Concentrated Force 16.5.4. Peeled Surface Layer 16.6. Rectangular Plates 16.6.1. Uniformly Loaded Rectangular Plate 16.7. Suggested Reading
288 288 289 290 291
PART 4: MICROMECHANICS
17 Dislocations and Cracks: Elementary Treatment 17.1. Dislocations 17.1.1. Derivation of the Displacement Field 17.2. Tensile Cracks 17.3. Suggested Reading
293 294 295 298
18 Dislocations in Anisotropic Media 18.1. Dislocation Character and Geometry 18.2. Dislocations in Isotropic Media 18.2.1. Inﬁnitely Long Screw Dislocations 18.2.2. Inﬁnitely Long Edge Dislocations 18.2.3. Inﬁnitely Long Mixed Segments 18.3. Planar Geometric Theorem 18.4. Applications of the Planar Geometric Theorem 18.4.1. Angular Dislocations 18.5. A 3D Geometrical Theorem 18.6. Suggested Reading
299 302 302 303 303 305 308 311 312 314
19 Cracks in Anisotropic Media 19.1. Dislocation Mechanics: Reviewed 19.2. Freely Slipping Crack 19.3. Crack Extension Force 19.4. Crack Faces Loaded by Tractions 19.5. Stress Intensity Factors and Crack Extension Force 19.5.1. Computation of the Crack Extension Force 19.6. Crack Tip Opening Displacement 19.7. Dislocation Energy Factor Matrix 19.8. Inversion of a Singular Integral Equation 19.9. 2D Anisotropic Elasticity – Stroh Formalism 19.9.1. Barnett–Lothe Tensors 19.10. Suggested Reading 20 The Inclusion Problem 20.1. The Problem 20.2. Eshelby’s Solution Setup 20.3. Calculation of the Constrained Fields: uc , ec , and σ c 20.4. Components of the Eshelby Tensor for Ellipsoidal Inclusion 20.5. Elastic Energy of an Inclusion 20.6. Inhomogeneous Inclusion: Uniform Transformation Strain 20.7. Nonuniform Transformation Strain Inclusion Problem 20.7.1. The Cases M = 0, 1
293
299
315 315 316 319 320 322 323 325 325 328 329 332 334 335 335 336 338 341 343 343 345 349
xii
Contents
20.8. Inclusions in Isotropic Media 20.8.1. Constrained Elastic Field 20.8.2. Field in the Matrix 20.8.3. Field at the Interface 20.8.4. Isotropic Spherical Inclusion 20.9. Suggested Reading 21 Forces and Energy in Elastic Systems 21.1. Free Energy and Mechanical Potential Energy 21.2. Forces of Translation 21.2.1. Force on an Interface 21.2.2. Finite Deformation Energy Momentum Tensor 21.3. Interaction Between Defects and Loading Mechanisms 21.3.1. Interaction Between Dislocations and Inclusions
21.3.2. Force on a Dislocation Segment 21.4. Elastic Energy of a Dislocation 21.5. InPlane Stresses of Straight Dislocation Lines 21.6. Chemical Potential 21.6.1. Force on a Defect due to a Free Surface 21.7. Applications of the J Integral 21.7.1. Force on a Clamped Crack 21.7.2. Application of the Interface Force to Precipitation
21.8. Suggested Reading 22 Micropolar Elasticity 22.1. Introduction 22.2. Basic Equations of CoupleStress Elasticity 22.3. Displacement Equations of Equilibrium 22.4. Correspondence Theorem of CoupleStress Elasticity 22.5. Plane Strain Problems of CoupleStress Elasticity 22.5.1. Mindlin’s Stress Functions 22.6. Edge Dislocation in CoupleStress Elasticity 22.6.1. Strain Energy 22.7. Edge Dislocation in a Hollow Cylinder 22.8. Governing Equations for Antiplane Strain 22.8.1. Expressions in Polar Coordinates 22.8.2. Correspondence Theorem for Antiplane Strain 22.9. Antiplane Shear of Circular Annulus 22.10. Screw Dislocation in CoupleStress Elasticity 22.10.1. Strain Energy 22.11. Conﬁgurational Forces in CoupleStress Elasticity 22.11.1. Reciprocal Properties 22.11.2. Energy due to Internal Sources of Stress 22.11.3. Energy due to Internal and External Sources of Stress
22.11.4. The Force on an Elastic Singularity
350 350 351 352 353 354 355 355 357 359 360 362 364 365 366 367 369 371 372 372 372 374 375 375 376 377 378 379 380 381 382 384 386 388 389 390 391 392 392 393 394 394 395
Contents
22.12. 22.13. 22.14. 22.15. 22.16. 22.17. 22.18.
xiii EnergyMomentum Tensor of a CoupleStress Field Basic Equations of Micropolar Elasticity Noether’s Theorem of Micropolar Elasticity Conservation Integrals in Micropolar Elasticity Conservation Laws for Plane Strain Micropolar Elasticity M Integral of Micropolar Elasticity Suggested Reading
396 398 400 403 404 404 406
PART 5: THIN FILMS AND INTERFACES
23 Dislocations in Bimaterials 23.1. Introduction 23.2. Screw Dislocation Near a Bimaterial Interface 23.2.1. Interface Screw Dislocation 23.2.2. Screw Dislocation in a Homogeneous Medium 23.2.3. Screw Dislocation Near a Free Surface 23.2.4. Screw Dislocation Near a Rigid Boundary 23.3. Edge Dislocation (bx ) Near a Bimaterial Interface 23.3.1. Interface Edge Dislocation 23.3.2. Edge Dislocation in an Inﬁnite Medium 23.3.3. Edge Dislocation Near a Free Surface 23.3.4. Edge Dislocation Near a Rigid Boundary 23.4. Edge Dislocation (by ) Near a Bimaterial Interface 23.4.1. Interface Edge Dislocation 23.4.2. Edge Dislocation in an Inﬁnite Medium 23.4.3. Edge Dislocation Near a Free Surface 23.4.4. Edge Dislocation Near a Rigid Boundary 23.5. Strain Energy of a Dislocation Near a Bimaterial Interface 23.5.1. Strain Energy of a Dislocation Near a Free Surface
23.6. Suggested Reading 24 Strain Relaxation in Thin Films 24.1. Dislocation Array Beneath the Free Surface 24.2. Energy of a Dislocation Array 24.3. StrainedLayer Epitaxy 24.4. Conditions for Dislocation Array Formation 24.5. Frank and van der Merwe Energy Criterion 24.6. Gradual Strain Relaxation 24.7. Stability of Array Conﬁgurations 24.8. Stronger Stability Criteria 24.9. Further Stability Bounds 24.9.1. Lower Bound 24.9.2. Upper Bound 24.10. Suggested Reading 25 Stability of Planar Interfaces 25.1. Stressed Surface Problem 25.2. Chemical Potential
407 407 407 409 409 409 410 410 415 417 417 418 419 420 422 422 423 423 426 427 428 428 430 431 432 434 436 439 439 441 441 443 446 447 447 449
xiv
Contents
25.3. 25.4. 25.5. 25.6. 25.7.
Surface Diffusion and Interface Stability Volume Diffusion and Interface Stability 2D Surface Proﬁles and Surface Stability Asymptotic Stresses for 1D Surface Proﬁles Suggested Reading
450 451 455 457 459
PART 6: PLASTICITY AND VISCOPLASTICITY
26 Phenomenological Plasticity 26.1. Yield Criteria for Multiaxial Stress States 26.2. Von Mises Yield Criterion 26.3. Tresca Yield Criterion 26.4. Mohr–Coulomb Yield Criterion 26.4.1. Drucker–Prager Yield Criterion 26.5. Gurson Yield Criterion for Porous Metals 26.6. Anisotropic Yield Criteria 26.7. ElasticPlastic Constitutive Equations 26.8. Isotropic Hardening 26.8.1. J2 Flow Theory of Plasticity 26.9. Kinematic Hardening 26.9.1. Linear and Nonlinear Kinematic Hardening 26.10. Constitutive Equations for PressureDependent Plasticity 26.11. Nonassociative Plasticity 26.12. Plastic Potential for Geomaterials 26.13. RateDependent Plasticity 26.14. Deformation Theory of Plasticity 26.14.1. RateType Formulation of Deformation Theory 26.14.2. Application beyond Proportional Loading 26.15. J2 Corner Theory 26.16. RateDependent Flow Theory 26.16.1. Multiplicative Decomposition F = Fe · Fp 26.17. Elastic and Plastic Constitutive Contributions 26.17.1. RateDependent J2 Flow Theory 26.18. A Rate Tangent Integration 26.19. Plastic Void Growth 26.19.1. Ideally Plastic Material 26.19.2. Incompressible Linearly Hardening Material 26.20. Suggested Reading 27 Micromechanics of Crystallographic Slip 27.1. Early Observations 27.2. Dislocations 27.2.1. Some Basic Properties of Dislocations in Crystals 27.2.2. Strain Hardening, Dislocation Interactions, and Dislocation Multiplication
27.3. Other Strengthening Mechanisms 27.4. Measurements of Latent Hardening 27.5. Observations of Slip in Single Crystals and Polycrystals at Modest Strains
461 462 463 465 467 468 470 470 471 473 474 475 477 478 480 480 482 484 485 486 487 489 489 491 492 493 495 497 498 501 502 502 508 511 514 517 519 523
Contents
xv
27.6. Deformation Mechanisms in Nanocrystalline Grains 27.6.1. Background: AKK Model 27.6.2. Perspective on Discreteness 27.6.3. Dislocation and Partial Dislocation Slip Systems 27.7. Suggested Reading 28 Crystal Plasticity 28.1. Basic Kinematics 28.2. Stress and Stress Rates 28.2.1. Resolved Shear Stress 28.2.2. RateIndependent Strain Hardening 28.3. Convected Elasticity 28.4. RateDependent Slip 28.4.1. A Rate Tangent Modulus 28.5. Crystalline Component Forms 28.5.1. Additional Crystalline Forms 28.5.2. Component Forms on Laboratory Axes 28.6. Suggested Reading 29 The Nature of Crystalline Deformation: Localized Plastic Deformation 29.1. Perspectives on Nonuniform and Localized Plastic Flow 29.1.1. Coarse Slip Bands and Macroscopic Shear Bands in Simple Crystals
525 530 535 535 537 538 538 541 542 544 545 547 548 550 553 555 555
557 557 558
29.1.2. Coarse Slip Bands and Macroscopic Shear Bands in 29.2.
29.3.
29.4.
29.5.
Ordered Crystals Localized Deformation in Single Slip 29.2.1. Constitutive Law for the Single Slip Crystal 29.2.2. Plastic Shearing with NonSchmid Effects 29.2.3. Conditions for Localization 29.2.4. Expansion to the Order of σ 29.2.5. Perturbations about the Slip and Kink Plane Orientations 29.2.6. Isotropic Elastic Moduli 29.2.7. Particular Cases for Localization Localization in Multiple Slip 29.3.1. Double Slip Model 29.3.2. Constitutive Law for the Double Slip Crystal Numerical Results for Crystalline Deformation 29.4.1. Additional Experimental Observations 29.4.2. Numerical Observations Suggested Reading
30 Polycrystal Plasticity 30.1. Perspectives on Polycrystalline Modeling and Texture Development
30.2. Polycrystal Model 30.3. Extended Taylor Model
559 560 560 560 563 565 567 570 571 576 576 576 580 580 582 584 586 586 588 590
xvi
Contents
30.4. Model Calculational Procedure 30.4.1. Texture Determinations 30.4.2. Yield Surface Determination 30.5. Deformation Theories and PathDependent Response 30.5.1. Speciﬁc Model Forms 30.5.2. Alternative Approach to a Deformation Theory 30.5.3. Nonproportional Loading 30.6. Suggested Reading 31 Laminate Plasticity 31.1. Laminate Model 31.2. Additional Kinematical Perspective 31.3. Final Constitutive Forms 31.3.1. RigidPlastic Laminate in Single Slip 31.4. Suggested Reading
592 593 594 596 597 598 598 600 601 601 604 604 605 607
PART 7: BIOMECHANICS
32 Mechanics of a Growing Mass 32.1. Introduction 32.2. Continuity Equation 32.2.1. Material Form of Continuity Equation 32.2.2. Quantities per Unit Initial and Current Mass 32.3. Reynolds Transport Theorem 32.4. Momentum Principles 32.4.1. RateType Equations of Motion 32.5. Energy Equation 32.5.1. Material Form of Energy Equation 32.6. Entropy Equation 32.6.1. Material Form of Entropy Equation 32.6.2. Combined Energy and Entropy Equations 32.7. General Constitutive Framework 32.7.1. Thermodynamic Potentials per Unit Initial Mass 32.7.2. Equivalence of the Constitutive Structures 32.8. Multiplicative Decomposition of Deformation Gradient 32.8.1. Strain and StrainRate Measures 32.9. Density Expressions 32.10. Elastic Stress Response 32.11. Partition of the Rate of Deformation 32.12. Elastic Moduli Tensor 32.12.1. Elastic Moduli Coefﬁcients 32.13. Elastic Strain Energy Representation 32.14. Evolution Equation for Stretch Ratio 32.15. Suggested Reading 33 Constitutive Relations for Membranes 33.1. Biological Membranes 33.2. Membrane Kinematics
609 609 610 610 612 612 614 615 615 616 617 618 619 619 620 621 622 623 624 625 626 627 629 629 630 631 633 633 634
Contents
33.3. 33.4. 33.5. 33.6.
xvii Constitutive Laws for Membranes Limited Area Compressibility Simple Triangular Networks Suggested Reading
637 638 639 640
PART 8: SOLVED PROBLEMS
34 Solved Problems for Chapters 1–33
641
Bibliography Index
833 853
Preface
This book is written for graduate students in solid mechanics and materials science and should also be useful to researchers in these ﬁelds. The book consists of eight parts. Part 1 covers the mathematical preliminaries used in later chapters. It includes an introduction to vectors and tensors, basic integral theorems, and Fourier series and integrals. The second part is an introduction to nonlinear continuum mechanics. This incorporates kinematics, kinetics, and thermodynamics of a continuum and an application to nonlinear elasticity. Part 3 is devoted to linear elasticity. The governing equations of the threedimensional elasticity with appropriate speciﬁcations for the twodimensional plane stress and plane strain problems are given. The applications include the analyses of bending of beams and plates, torsion of prismatic rods, contact problems, semiinﬁnite media, and threedimensional isotropic and anisotropic elastic problems. Part 4 is concerned with micromechanics, which includes the analyses of dislocations and cracks in isotropic and anisotropic media, the wellknown Eshelby elastic inclusion problem, energy analyses of imperfections and conﬁgurational forces, and micropolar elasticity. In Part 5 we analyze dislocations in bimaterials and thin ﬁlms, with an application to the study of strain relaxation in thin ﬁlms and stability of planar interfaces. Part 6 is devoted to mathematical and physical theories of plasticity and viscoplasticity. The phenomenological or continuum theory of plasticity, single crystal, polycrystalline, and laminate plasticity are presented. The micromechanics of crystallographic slip is addressed in detail, with an analysis of the nature of crystalline deformation, embedded in its tendency toward localized plastic deformation. Part 7 is an introduction to biomechanics, particularly the formulation of governing equations of the mechanics of solids with a growing mass and constitutive relations for biological membranes. Part 8 is a collection of 180 solved problems covering all chapters of the book. This is included to provide additional development of the basic theory and to further illustrate its application. The book is transcribed from lecture notes we have used for various courses in solid mechanics and materials science, as well as from our own published work. We have also consulted and used major contributions by other authors, their research work and written books, as cited in the various sections. As such, this book can be used as a textbook for a sequence of solid mechanics courses at the graduate level within mechanical, structural, aerospace, and materials science engineering programs. In particular, it can be used for xix
xx
Preface
the introduction to continuum mechanics, linear and nonlinear elasticities, theory of dislocations, fracture mechanics, theory of plasticity, and selected topics from thin ﬁlms and biomechanics. At the end of each chapter we offer a list of recommended references for additional reading, which aid further study and mastering of the particular subject. Standard notations and conventions are used throughout the text. Symbols in bold, both Latin and Greek, denote tensors or vectors, the order of which is indicated by the context. Typically the magnitude of a vector will be indicated by the name symbol unbolded. Thus, for example, a or b indicate two vectors or tensors. If a and b are vectors, then the scalar product, i.e., the dot product between them is indicated by a single dot, as a · b. Since a and b are vectors in this context, the scalar product is also ab cos θ, where θ is the angle between them. If A is a higher order tensor, say secondorder, then the dot product of A and a produces another vector, viz., A · a = b. In the index notation this is expressed as Ai j a j = bi . Unless explicitly stated otherwise, the summation convention is adopted whereby a repeated index implies summation over its full range. This means, accordingly, that the scalar product of two vectors as written above can also be expressed as a j b j = φ, where φ is the scalar result. Two additional operations are introduced and deﬁned in the text involving double dot products. For example, if A and B are two secondrank tensors, then A : B = Ai j Bi j and A · · B = Ai j Bji . For higher order tensors, similar principles apply. If C is a fourthrank tensor, then C : e ⇒ Ci jkl ekl = {...}i j . . In ﬁnite vector spaces we assume the existence of a convenient set of basis vectors. Most commonly these are taken to be orthogonal and such that an arbitrary vector, say a, can be expressed wr t its components along these base vectors as a = a1 e1 + a2 e2 + a3 e3 , where {e1 , e2 , e3 } are the orthogonal set of base vectors in question. Other more or less standard notations are used, e.g., the left or righthand side of an equation is referred to as the lhs, or r hs, respectively. The commonly used phrase with respect is abbreviated as wr t, and so on. We are grateful to many colleagues and students who have inﬂuenced and contributed to our work in solid mechanics and materials science over a long period of time and thus directly or indirectly contributed to our writing of this book. Speciﬁcally our experiences at Stanford University, Brown University, UCSD, Ford Motor Company (RJA), Ohio State University (RJA), University of Montenegro (VAL), and Arizona State University (VAL) have involved collaborations that have been of great professional value to us. Research funding by NSF, the U.S. Army, the U.S. Air Force, the U.S. Navy, DARPA, the U.S. DOE, Alcoa Corp., and Ford Motor Co. over the past several decades has greatly facilitated our research in solid mechanics and materials science. We are also most grateful to our families and friends for their support during the writing of this book La Jolla, California July, 2005
Robert J. Asaro Vlado A. Lubarda
PART 1: MATHEMATICAL PRELIMINARIES
1 Vectors and Tensors
This chapter and the next are concerned with establishing some basic properties of vectors and tensors in real spaces. The ﬁrst of these is speciﬁcally concerned with vector algebra and introduces the notion of tensors; the next chapter continues the discussion of tensor algebra and introduces Gauss and Stokes’s integral theorems. The discussion in both chapters is focused on laying out the algebraic methods needed in developing the concepts that follow throughout the book. It is, therefore, selective and thus far from inclusive of all vector and tensor algebra. Selected reading is recommended for additional study as it is for all subsequent chapters. Chapter 3 is an introduction to Fourier series and Fourier integrals, added to facilitate the derivation of certain elasticity solutions in later chapters of the book.
1.1 Vector Algebra We consider threedimensional Euclidean vector spaces, E, for which to each vector such as a or b there exists a scalar formed by a scalar product a · b such that a · b = a r eal number in R and a vector product that is another vector such that a × b = c. Note the deﬁnitions via the operations of the symbols, · and ×, respectively. Connections to common geometric interpretations will be considered shortly. With α and β being scalars, the properties of these operations are as follows a · b = b · a,
∀ a, b ∈ E,
(αa + βb) · c = α(a · c) + β(b · c), a · a ≥ 0,
with a · a = 0
iff
(1.1)
∀ a, b, c ∈ E, a = 0,
(1.2) (1.3)
a × b = −b × a,
(1.4)
(αa + βb) × c = α(a × c) + β(b × c).
(1.5)
a · (a × b) = 0,
(1.6)
(a × b) · (a × b) = (a · a)(b · b) − (a · b)2 .
(1.7)
Also,
1
2
1. Vectors and Tensors
b
a
Figure 1.1. Geometric meaning of a vector triple product. The triple product is equal to the volume of the parallelepiped formed from the three deﬁning vectors, a, b, and c.
c
The magnitude of a is a ≡ a = (a · a)1/2 .
(1.8)
a · b = 0.
(1.9)
Two vectors are orthogonal if
From the above expressions it follows that if a × b = 0, then a and b are linearly dependent, i.e., a = αb where α is any scalar. A triple product is deﬁned as [a, b, c] ≡ a · (b × c).
(1.10)
It is evident from simple geometry that the triple product is equal to the volume enclosed by the parallelepiped constructed from the vectors a, b, c. This is depicted in Fig. 1.1. Here, again, the listed vector properties allow us to write [a, b, c] = [b, c, a] = [c, a, b] = −[b, a, c] = −[a, c, b]
(1.11)
= −[c, b, a] and [αa + βb, c, d] = α[a, c, d] + β[b, c, d].
(1.12)
[a, b, c] = 0
(1.13)
Furthermore,
iff a, b, c are linearly dependent. Because of the ﬁrst of the properties (1.3), we can establish an orthonormal basis (Fig. 1.2) that we designate as {e1 , e2 , e3 }, such that 1, if i = j, ei · e j = δi j = (1.14) 0, otherwise. The δi j is referred to as the Kronecker delta. Using the basis {ei }, an arbitrary vector, say a, can be expressed as a = a 1 e1 + a 2 e2 + a 3 e3
(1.15)
a = ai ei ,
(1.16)
or
1.1. Vector Algebra
3
υ
e2
Figure 1.2. A vector υ in an orthonormal basis.
e
e1 3
where the repeated index i implies summation, i.e., a = ai ei =
3
ai ei .
(1.17)
i=1
We can use (1.14) to show that ai = a · ei = ar er · ei = ar δri .
(1.18)
The properties listed previously allow us to write e1 = e2 × e3 ,
e2 = e3 × e1 ,
e3 = e1 × e2 .
(1.19)
We note that these relations can be expressed as ei × e j = i jkek, where the permutation tensor is deﬁned as ⎧ ⎪ ⎪ ⎨+1, if i, j, k are an even permutation of 1, 2, 3, i jk = −1, if i, j, k are an odd permutation of 1, 2, 3, ⎪ ⎪ ⎩ 0, if any of i, j, k are the same.
(1.20)
(1.21)
Some useful results follow. Let a = a p e p and b = br er . Then, a · b = (a p e p ) · (br er ) = a p br (e p · er ) = a p br δ pr .
(1.22)
Thus, the scalar product is a · b = a p bp = ar br .
(1.23)
a × b = a p e p × br er = a p br e p × er = a p br pri ei = i pr (a p br )ei .
(1.24)
Similarly, the vector product is
Finally, the component form of the triple product, [a, b, c] = [c, a, b] = c · (a × b),
(1.25)
c · (i pr a p br ei ) = i pr a p br ci = pri a p br ci = i jkai b j ck.
(1.26)
is
4
1. Vectors and Tensors
e' 2
e2
e' 1 Figure 1.3. Transformation via rotation of basis.
e
1
e3 e' 3
1.2 Coordinate Transformation: Rotation of Axes Let υ be a vector referred to two sets of basis vectors, {ei } and {ei }, i.e., υ = υi ei = υi ei .
(1.27)
We seek to relationship of the υi to the υi . Let the transformation between two bases (Fig. 1.3) be given by ei = αi j e j .
(1.28)
ei · e j = αis es · e j = αis δs j = αi j .
(1.29)
Then
It follows that υs = υ · e s = υ · αsp e p = υ p αsp = αsp υ p and thus υi = αi j υ j .
(1.30)
For example, in the twodimensional case, we have e 1 = cos θe1 + sin θe2 , e 2 = − sin θe1 + cos θe2 , with the corresponding transformation matrix cos θ α= − sin θ
sin θ . cos θ
(1.31)
(1.32)
Another way to describe the transformation in (1.28) is to set e = β · e.
(1.33)
A straightforward manipulation, however, shows that β and α are related by β = αT , where the transpose, αT , is deﬁned in the sequel.
(1.34)
1.4. Symmetric and Antisymmetric Tensors
5
1.3 SecondRank Tensors A vector assigns to each direction a scalar, viz., the magnitude of the vector. A secondrank tensor assigns to each vector another (unique) vector, via the operation A · a = b.
(1.35)
A · (αa + βb) = αA · a + βA · b.
(1.36)
More generally,
Secondrank tensors obey the following additional rules (A + B) · a = A · a + B · a, (αA) · a = αA · a, (A · B) · a = A · (B · a), A + B = B + A,
(1.37)
α(A · B) = (αA) · B, A · (B + C) = A · B + A · C, A · (B · C) = (A · B) · C. Each tensor, A, has a unique transpose, AT , deﬁned such that a · (AT · b) = b · (A · a).
(1.38)
Because of (1.36)–(1.38), we can write (αA + βB)T = αAT + βBT ,
(1.39)
(A · B)T = BT · AT .
(1.40)
and
1.4 Symmetric and Antisymmetric Tensors We call the tensor A symmetric if A = AT . A is said to be antisymmetric if A = −AT . An arbitrary tensor, A, can be expressed (or decomposed) in terms of its symmetric and antisymmetric parts, via A=
1 1 (A + AT ) + (A − AT ), 2 2
(1.41)
where 1 (A + AT ), 2 1 skew (A) ≡ (A − AT ). 2 sym (A) ≡
(1.42)
6
1. Vectors and Tensors
1.5 Prelude to Invariants of Tensors
Let f, g, h and {l, m, n} be two arbitrary bases of E. Then it can be shown that χ1 = ([A · f, g, h] + [f, A · g, h] + [f, g, A · h]) /[f, g, h] = ([A · l, m, n] + [l, A · m, n] + [l, m, A · n]) /[l, m, n], χ2 = ([A · f, A · g, h] + [f, A · g, A · h] + [A · f, g, A · h]) /[f, g, h] = ([A · l, A · m, n] + [l, A · m, A · n] + [A · l, m, A · n]) /[l, m, n], χ3 = [A · f, A · g, A · h]/[f, g, h] = [A · l, A · m, A · n]/[l, m, n]. In proof of the ﬁrst of the above, consider the ﬁrst part of the lhs, [A · f, g, h] = [A · ( f p e p ), gq eq , hr er ] = [ f p (A · e p ), gq eq , hr er ] = f p gq hr [A · e p , eq , er ].
(1.43)
Thus the entire expression for χ1 becomes χ1 =
f p gq hr ([A · e p , eq , er ] + [e p , A · eq , er ] + [e p , eq , A · er ]) . [f, g, h]
(1.44)
The term in (. . .) remains unchanged if p, q, r undergo an even permutation of 1, 2, 3; it reverses sign if p, q, r undergo an odd permutation, and is equal to 0 if any of p, q, r are made equal. Thus set p = 1, q = 2, r = 3, and multiply the result by pqr to take care of the changes in sign or the null results just described. The full expression becomes ( f p gq hr ) pqr ([A · e1 , e2 , e3 ] + [e1 , A · e2 , e3 ] + [e1 , e2 , A · e3 ]) [f, g, h]
(1.45)
= [A · e1 , e2 , e3 ] + [e1 , A · e2 , e3 ] + [e1 , e2 , A · e3 ]. Since [e1 , e2 , e3 ] = +1, the quantity ([A · f, g, h] + [f, A · g, h] + [f, g, A · h]) /[f, g, h]
(1.46)
is invariant to changes of the basis {f, g, h}. Given the validity of the expressions for χ1 , χ2 , and χ3 , we thereby discover three invariants of the tensor A, viz., IA = ([A · f, g, h] + [f, A · g, h] + [f, g, A · h]) /[f, g, h], I IA = ([A · f, A · g, h] + [f, A · g, A · h] + [A · f, g, A · h]) /[f, g, h], I I IA = [A · f, A · g, A · h]/[f, g, h]. The commonly held descriptors for two of these are IA = trace of A = tr (A), I I IA = determinant of A = det(A) = A.
(1.47)
1.7. Additional Proofs
7
1.6 Inverse of a Tensor If A = 0, A has an inverse, A−1 , such that A · A−1 = A−1 · A = I,
(1.48)
where I, the identity tensor, is deﬁned via the relations a = I · a = a · I.
(1.49)
Useful relations that follow from the above are αA = α 3 A,
(1.50)
A · B = AB. Thus, it follows that A · A−1  = I = 1 = AA−1 , A−1  =
(1.51)
1 = A−1 . A
1.7 Additional Proofs We deferred formal proofs of several lemmas until now in the interest of presentation. We provide the proofs at this time. LEMMA 1.1: If a and b are two vectors, a × b = 0 iff a and b are linearly dependent.
Proof: If a and b are linearly dependent then there is a scalar such that b = αa. In this case, if we express the vector product a × b = c in component form, we ﬁnd that ci = i jka j αak = αi jka j ak. But the summations over the indices j and k will produce pairs of multiples of aβ aγ , and then again aγ aβ , for which the permutator tensor alternates algebraic sign, thus causing such pairs to cancel. Thus, in this case a × b = 0. Conversely, if a × b = 0, we ﬁnd from (1.3) to (1.8) that a × b = ±ab. If the plus signs holds, we have from the second of (1.3) (ba − ab) · (ba − ab) = 2a2 b2 − 2aba · b = 0.
(1.52)
Because of the third property in (1.3) this means that ba = ab. When the minus sign holds, we ﬁnd that ba = −ab. In either case this leads to the conclusion that b = αa. Next we examine the relations deﬁning properties of the triple product when pairs of the vectors are interchanged. Use (1.26) to calculate the triple product. This yields [a, b, c] = i jkai b j ck. Next imagine interchanging, say a with b; we obtain [b, a, c] = i jkbi a j ck = i jka j bi ck = − jika j bi ck = −i jkai b j ck, where the last term involved merely a reassignment of summation indices. Thus [a, b, c] = −[b, a, c]. Proceeding this way all members of (1.11) are generated. We now examine the triple product property expressed in (1.12). LEMMA 1.2: If a, b, c, and d are arbitrary vectors, and α and β arbitrary scalars, then
[αa + βb, c, d] = α[a, c, d] + β[b, c, d],
∀ a, b, c, d ∈ E,
α, β ∈ R.
(1.53)
8
1. Vectors and Tensors
Proof: Begin with the property of scalar products between vectors expressed in (1.2) and replace c with c × d. Then, (αa + βb) · (c × d) = αa · (c × d) + βb · (c × d) = α[a, c, d] + β[b, c, d].
(1.54)
Of course, the ﬁrst term in the above is the triple product expressed on the lhs of the lemma.
1.8 Additional Lemmas for Vectors LEMMA 1.3: If
v = αa + βb + γ c,
(1.55)
where a, b, c, v are all vectors, then α=
i jkvi b j ck , pqr a p bq cr
i jkai v j ck , pqr a p bq cr
β=
γ =
i jkai b j vk . pqr a p bq cr
(1.56)
Proof: The three relations that express the connections are v1 = αa1 + βb1 + γ c1 , v2 = αa2 + βb2 + γ c2 ,
(1.57)
v3 = αa3 + βb3 + γ c3 . By Cramer’s rule v1 v2 v 3 α= a1 a2 a 3
b1 c1 b2 c2 b3 c3 . b1 c1 b2 c2 b3 c3
(1.58)
Thus, the lemma is proved once the two determinants are expressed using the permutation tensor. LEMMA 1.4: Given a vector a, then for arbitrary vector x,
a × x = a iff a = 0.
(1.59)
Proof: Express the i th component of a × x as i jka j xk,
(1.60)
and then form the product a · a to obtain i jka j xkir s ar xs = (δ jr δks − δ js δkr )a j xkar as = a 2 x 2 − (a · x)2 = a 2 . The expression just generated is zero as may be seen, for example, by letting x be equal to e1 , e2 , e3 , respectively. Note that the third equation of (1.70) below has been used.
1.9. Coordinate Transformation of Tensors
9
LEMMA 1.5: Suppose that for any vector p, p · q = p · t, then we have
p · q = p · t ⇒ q = t.
(1.61)
Proof: The relation p · q = p · t can be rewritten as p · (q − t) = p1 (q1 − t1 ) + p2 (q2 − t2 ) + p3 (q3 − t3 ) = 0.
(1.62)
As in the previous lemma, letting p be systematically equal to e1 , e2 , e3 shows that p1 = p2 = p3 = 0. We reexamine now the operation of the cross product between vectors to develop two additional lemmas of interest. LEMMA 1.6: Given the vectors p, q, r we have
p × (q × r) = q(p · r) − r(p · q).
(1.63)
Proof: The proof is most readily done by expressing the above in component form, i.e., r si ps i jkq j rk = r si i jk ps q j rk = ir s i jk ps q j rk.
(1.64)
Use the identity given by the third equation of (1.70) and write ir s i jk ps q j rk = qr ( ps rs ) − rr ( ps qs )
(1.65)
to complete the proof. A simple extension of the last lemma is that (p × q) × r = q(p · r) − p(r · q).
(1.66)
The proof is left as an exercise.
1.9 Coordinate Transformation of Tensors Consider coordinate transformations prescribed by (1.28). A tensor A can be written alternatively as A = Ai j ei e j = Ai j ei e j = Ai j αir er α js es .
(1.67)
Since e p · A · eq = A pq , performing this operation on (1.67) gives A pq = e p · Ai j ei e j · eq = α pi αqj Ai j . Transformation of higher order tensors can be handled in an identical manner.
(1.68)
10
1. Vectors and Tensors
1.10 Some Identities with Indices The following identities involving the Kronecker delta are useful and are easily veriﬁed by direct expansion δii = 3, δi j δi j = 3, δi j δikδ jk = 3,
(1.69)
δi j δ jk = δik, δi j Aik = Ajk. Useful identities involving the permutation tensor are i jkkpq = δi p δ jq − δiq δ j p , pqs sqr = −2δ pr ,
(1.70)
i jki jk = 6.
1.11 Tensor Product Let u and v be two vectors; then there is a tensor B = uv deﬁned via its action on an arbitrary vector a, such that (uv) · a = (v · a)u.
(1.71)
Note that there is the commutative property that follows, viz., (αu + βv)w = αuw + βvw, u(αv + βw) = αuv + βuw.
(1.72)
By the deﬁnition of the transpose as given previously, we also have (uv)T = vu.
(1.73)
The identity tensor, I, can be expressed as I = e pe p,
(1.74)
if e1 , e2 , e3 are orthonormal. Indeed, (e p e p ) · a = (a · e p )e p = a p e p = a = I · a. LEMMA 1.7: If u and v are arbitrary vectors, then
uv = 0,
and
tr (uv) = u · v.
(1.75)
Proof: Replace A in (1.47) with uv, and use {a, b, c} as a basis of E. Then the third equation from (1.47) becomes [(uv) · a, (uv) · b, (uv) · c] = I I Iuv [a, b, c],
1.12. Orthonormal Basis
11
where I I Iuv = uv. But, (uv) · a = (v · a)u u, and similarly (uv) · b = (v · b)u u,
(uv) · c = (v · c)u u.
Consequently, uv = 0.
(1.76)
Next, we note that the ﬁrst equation from (1.47), with A = uv, leads to [(uv) · a, b, c] + [a, (uv) · b, c] + [a, b, (uv) · c] = Iuv [a, b, c],
(1.77)
where Iuv = tr (uv). But the lhs of the relation (1.77) can be rearranged as v · a[u, b, c] + v · b[a, u, c] + v · c[a, b, u]. Since {a, b, c} is a basis of E, u can be expressed as u = αa + βb + γ c,
(1.78)
which, when substituted into the above, yields for the various bracketed terms [αa + βb + γ c, b, c] = α[a, b, c], [a, αa + βb + γ c, c] = β[a, b, c],
(1.79)
[a, b, αa + βb + γ c] = γ [a, b, c]. But, the ﬁrst of (1.47) gives (αa · v + βb · v + γ c · v) [a, b, c] = tr (uv)[a, b, c], so that tr (uv) = u · v.
(1.80)
1.12 Orthonormal Basis Let us now refer the tensor A to an orthonormal basis, {e1 , e2 , e3 }. The ei are unit vectors in this context. Let Ai j be the components of A relative to this basis. Then A · e j = Apj e p
and
Ai j = ei · A · e j .
Now form A = Apq e p eq and look at its operation on a vector a = ar er . We have (Apq e p eq ) · ar er = Apq ar e p eq · er = Apr ar e p = ar Apr e p .
(1.81)
12
1. Vectors and Tensors e
n
2
2 n
1
θ
Figure 1.4. Coordinate system (axes) of the principal directions.
e
1
e3 n3
But, A · a = A · ar er = ar A · er = ar Apr e p .
(1.82)
Thus, A can be expressed as A = Apq e p eq ,
with
Apq = e p · A · eq .
(1.83)
Note if A = uv, then Ai j = ui v j , because A = ui v j ei e j and u = ui ei , v = v j e j . By using an orthonormal basis {ei }, the invariants of a secondrank tensor A can be expressed from (1.47) as follows. First, consider IA = [A · e1 , e2 , e3 ] + [e1 , A · e2 , e3 ] + [e1 , e2 , A · e3 ] = [Ap1 e p , e2 , e3 ] + [e1 , Ar 2 er , e3 ] + [e1 , e2 , As3 es ].
(1.84)
To evaluate the above, use Ap1 e p = A11 e1 + A21 e2 + A31 e3 and, for example, [A11 e1 + A21 e2 + A31 e3 , e2 , e3 ] = [A11 e1 , e2 , e3 ] = A11 [e1 , e2 , e3 ] = A11 . Likewise, [e1 , Ar 2 er , e3 ] = A22 ,
[e1 , e2 , As3 es ] = A33 .
Thus, IA = A11 + A22 + A33 = tr A.
(1.85)
Similar manipulations yield I IA =
1 2 (A − Apq Aqp ), 2 pp
I I IA = det A = A = pqr Ap1 Aq2 Ar 3 .
(1.86) (1.87)
1.13 Eigenvectors and Eigenvalues Let σ be a symmetric tensor, i.e., σi j = σ ji in any orthonormal basis, {ei }. Examine the “normal components” of σ, e.g., σnn = n · σ · n = ni σi j n j . Look for extremum values for
1.13. Eigenvectors and Eigenvalues
13
σnn wr t the orientation of n. Let θ be the angle between n and e1 (Fig. 1.4). We require that ∂σnn /∂θ = 0 = ∂ni /∂θ (σi j n j ) + ni ∂(σi j n j )/∂θ = ∂ni /∂θ σi j n j + ni σi j ∂n j /∂θ = 2∂ni /∂θ (σi j n j ) = 2(∂n/∂θ ) · T(n) = 0, (n)
where T(n) = σ · n and Ti = σi j n j . Since ∂n/∂θ is orthogonal to n, we conclude that T(n) = σ · n must be codirectional with n. Hence, T(n) = σ · n = λ(n) n. This leads to the homogeneous set of equations (σi j − λ(n) δi j )n j = 0.
(1.88)
σ · n − λ(n) n = 0
(1.89)
In dyadic notation these are
or A · n = 0,
A = σ − λI.
(1.90)
Conditions need to be sought whereby (1.89) can have nontrivial solutions. LEMMA 1.8: Recall (1.5) viz. det A = [A · f, A · g, A · h], where {f, g, h} is an arbitrary
basis of E. If [A · f, A · g, A · h] = 0, then {A · f, A · g, A · h} must be linearly dependent. That is, [a, b, c] = 0 iff {a, b, c} are linearly dependent. Proof: If one of {p, q, r} are zero, [p, q, r] = p · (q × r) = 0. Next, if {a, b, c} are linearly dependent, there exist α, β, γ (not all zero) such that αa + βb + γ c = 0.
(1.91)
[αa + βb + γ c, b, c] = 0 = α[a, b, c].
(1.92)
But, such triple products are
The converse result follows from the fact that a × b = 0 iff a and b are linearly dependent. Return now to the possible solution of the equation A · n = 0. Suppose A = 0, then if {f, g, h} form a basis of E, they are linearly dependent, i.e., α(A · f) + β(A · g) + γ (A · h) = 0, which leads to A · (αf + βg + γ h) = 0. Thus, n = αf + βg + γ h.
(1.93)
Conversely, if n satisﬁes A · n = 0, then we can choose two vectors l and m that together with n form a basis of E. Then det A = [A · l, A · m, A · n] = 0,
14
1. Vectors and Tensors
because A · n = 0. Thus, if A · n = λ(n) n is to have a solution for n with λ(n) , then det(A − λ(n) I) = 0.
(1.94)
Using an arbitrary basis {a, b, c}, we obtain [A · a − λ(n) a, A · b − λ(n) b, A · c − λ(n) c] = 0,
(1.95)
λ3 − IA λ2 + I IA λ − I I IA = 0.
(1.96)
which becomes
Equation (1.96), referred to as a characteristic equation, has three solutions.
1.14 Symmetric Tensors Symmetric tensors, e.g., S, possess real eigenvalues and corresponding eigenvectors, {λ1 , λ2 , λ3 } and {p1 , p2 , p3 }, respectively. We may write S in the various forms such as S = S · I = S · (pr pr ) = S · pr pr = λ(r ) pr pr . Thus the spectral representation of S is S = λ(r ) pr pr (sum on r).
(1.97)
The invariants of S are I I IS = λ1 λ2 λ3 , I IS = λ1 λ2 + λ2 λ3 + λ1 λ3 ,
(1.98)
IS = λ1 + λ2 + λ3 .
1.15 Positive Deﬁniteness of a Tensor If for any arbitrary vector a, a · A · a ≥ 0, the tensor A is said to be positive semideﬁnite. If a · A · a > 0, A is said to be positive deﬁnite. Let S be a symmetric, positive semideﬁnite tensor with the associated eigenvectors and eigenvalues, pi and λi . Then, as before, S = λr pr pr (sum on r).
(1.99)
Now form the double products indicated above and note that a · S · a = a · λr pr pr · a = λr (a · pr )2 ≥ 0.
(1.100)
Since a is arbitrary, λr ≥ 0 for all r = 1, 2, 3. It follows that S1/2 = λr1/2 pr pr .
(1.101)
S−1 = λr−1 pr pr ,
(1.102)
Also,
1.16. Antisymmetric Tensors
15
which is readily veriﬁed via S · S−1 = λr pr pr · λ−1 s ps ps (sum on r,s) −1 = λr λ−1 s pr ps pr · ps = λr λs pr ps δr s
= pr pr = I. LEMMA 1.9: If A is an arbitrary tensor, then AT · A and A · AT are positive semideﬁnite.
Proof: Clearly, (AT · A)T = AT · (AT )T = AT · A = symmetric, (A · AT )T = (AT )T · AT = A · AT = symmetric. Thus,
and
a · (AT · A) · a = a · AT · (A · a) = (a · AT ) · (A · a) = (A · a) · (A · a) ≥ 0,
(1.103)
a · (A · AT ) · a = (a · A) · (AT · a) = (a · A) · (a · A) ≥ 0.
(1.104)
1.16 Antisymmetric Tensors If WT = −W,
(1.105)
the tensor W is said to be antisymmetric. Let a and b be arbitrary vectors, then b · (W · a) = a · (WT · b) = −a · (W · b).
(1.106)
Thus, for example, if a = b, a · W · a = 0. Furthermore,
⎧ ⎪ if i = j, ⎨ 0, Wi j = ei · W · e j = Wi j , if i = j, ⎪ ⎩ −Wji , if i =
j.
(1.107)
(1.108)
1.16.1 Eigenvectors of W Examine W · p = λp,
(1.109)
where p is a unit vector. Form the product p · W · p = λ = 0. Thus λ = 0 and W · p = 0.
(1.110)
16
1. Vectors and Tensors
Let {q, r, p} be a unit orthonormal basis; then p = q × r,
q = r × p,
r = p × q,
[p, q, r] = 1.
(1.111)
Recall that if {i, j} is a pair of unit vectors from the set {q, r}, then Wi j = i · W · j,
W = Wi j ij.
(1.112)
Thus W = ω(rq − qr),
(1.113)
W · p = ω(rq − qr) · p = 0.
(1.114)
which is readily veriﬁed via
The scalar ω is then obtained as ω = r · W · q = −q · W · r.
(1.115)
Now set w = ωp, and let a be an arbitrary vector. We have W · a − w × a = ω(rq − qr) · a − ωp × a.
(1.116)
a = (a · p)p + (a · q)q + (a · r)r,
(1.117)
Next, write
and form W·a−w×a = ω [(rq) · a − (qr) · a − p × (a · p)p − p × (a · q)q − p × (a · r)r] = ω [(q · a){r − p × q} − (r · a){q + p × r}] . But the two terms in the {. . .} above are equal to zero, and so W · a − w × a = 0.
(1.118)
So associated with W there is an axial vector w ≡ ωp such that W · a = w × a,
(1.119)
W · p = 0.
(1.120)
where
It is readily deduced from the above that IW = tr W = 0, I IW = ω2 ,
(1.121)
I I IW = det W = 0. Also, if u and v are arbitrary vectors, then the tensor L deﬁned as L ≡ uv − vu
(1.122)
1.17. Orthogonal Tensors
17
is an antisymmetric tensor and w=v×u
(1.123)
is its axial vector.
1.17 Orthogonal Tensors An orthogonal tensor Q has the property of preserving scalar products, i.e., (Q · a) · (Q · b) = a · b.
(1.124)
This property has the following effect (Q · a) · (Q · b) = (a · QT ) · (Q · b) = a · (QT · Q) · b = a · b. Thus, we deduce that QT · Q = I, or Q−1 = QT .
(1.125)
QT · (Q − I) = −(Q − I)T .
(1.126)
Note that
Since QT · Q = I and det QT = det Q, we have (det Q)2 = 1.
(1.127)
Thus, for a proper orthogonal (rotation) tensor, det Q = 1.
(1.128)
The proper orthogonal tensor has one real eigenvalue, which is equal to 1. The corresponding eigenvector, p, is parallel to the axis of rotation associated with Q, i.e., Q · p − 1p = 0.
(1.129)
Now introduce q and r as before, viz., p = q × r, q = r × p, r = p × q.
(1.130)
Then, Q · p = p = QT · p ,
(because QT = Q−1 ).
(1.131)
In addition, we may deduce q · (Q · p) = 0 = r · (Q · p) = p · (Q · q) = p · (Q · r)
(1.132)
p · Q · p = 1.
(1.133)
and
Some other results that may be straightforwardly deduced are (Q · q) · (Q · r) = q · r, (Q · q) · (Q · q) = (q · QT ) · (Q · q) = q · q = 1, Q · q = Q · r = 1.
(1.134)
18
1. Vectors and Tensors p
x
Figure 1.5. Geometric interpretation of an orthogonal tensor in terms of the rotation of a material ﬁber.
θ
Q x r
q
Thus, the pairs (q, r) and (Q · q, Q · r) are orthogonal to p. Because of this property, we then can write Q · q = αq + βr,
Q · r = γ q + δr,
(1.135)
γ 2 + δ 2 = 1.
(1.136)
and α 2 + β 2 = 1, The determinant of Q is det(Q) = [Q · p, Q · q, Q · r] = [p, αq + βr, γ q + δr] = αδ − βγ = 1.
(1.137)
Note also, since (Q · q) · (Q · r) = 0, that αγ + βδ = 0.
(1.138)
In addition, α 2 + β 2 = 1,
γ 2 + δ 2 = 1,
αδ − βγ = 1,
αγ + βδ = 0.
(1.139)
These are satisﬁed by the following assignments α = δ = cos θ,
β = −γ = sin θ.
(1.140)
Therefore, −q · Q · r = r · Q · q = sin θ, q · Q · q = r · Q · r = cos θ,
(1.141)
and thus Q = pp + cos θ(qq + rr) − sin θ(qr − rq).
(1.142)
This last result is depicted in Fig. 1.5, which shows the result of operating on a typical vector, x. As shown, the effect of the tensor operation is to rotate x about the eigenvector p by the angle θ. That is, the result of operating with Q is to produce a rotated vector, x = Q · x, as shown in the ﬁgure. As expected, orthogonal tensors enter the discussion of material motion prominently with respect to describing rotations of bodies and material ﬁbers. This will, for example, appear explicitly in our consideration of the the polar decomposition theorem introduced in the next section.
1.18. Polar Decomposition
19
As an example, with respect to the basis e = {e1 , e2 , e3 }, let Q11 = Q22 = cos θ, Q12 = −Q21 = − sin θ, Q33 = 1, and Qi j = 0 otherwise. Equations (1.129) then become cos θ p1 + sin θ p2 = p1 , − sin θ p1 + cos θ p2 = p2 ,
(1.143)
p3 = p3 , with p = pi ei . The solution to this set is trivially p1 = p2 = 0 and p3 = 1; thus p = e3 . Next choose q = e1 and r = e2 to satisfy the requirement of a righthanded triad basis, {p, q, r}. Clearly then Qqq = q · Q · q = cos θ = r · Q · r = Qrr , Qrq = r · Q · q = sin θ = −(q · Q · r) = −Qqr , and hence Q = pp + cos θ(qq + rr) − sin θ(qr − rq).
(1.144)
But x = xs es = (x · ξ s )ξ s , where ξ s = {p, q, r} and where x1 = cos α, x2 = sin α and x3 = 0. The relationship x = Q · x leads to x = [pp + cos θ(qq + rr) − sin θ(qr − rq)] · (cos αq + sin αr) = cos(θ + α)q + sin(θ + α)r. The result is exactly what was expected, namely that the ﬁber x inclined by θ to the e1 base vector is now rotated by α so that its total inclination is θ + α.
1.18 Polar Decomposition Theorem Let A be an arbitrary tensor that possesses an inverse A−1 . The following theorem, known as the polar decomposition theorem, will be useful in the analysis of ﬁnite deformations and the development of constitutive relations. THEOREM 1.1: An invertible secondorder tensor A can be uniquely decomposed as
A = Q · U = V · Q,
(1.145)
where Q is an orthogonal tensor and U and V are symmetric, positive deﬁnite tensors. Proof: Recall that the forms AT · A and A · AT are positive semideﬁnite, symmetric tensors. If A is invertible, i.e., A−1 exists, then det A = 0 and A · n = 0 if n = 0; also by this AT · n = 0. Recall also, that AT · A and A · AT have unique, positive square roots. Let U be the square root of AT · A and V be the square root of A · AT . But then U and V have unique inverses, U−1 and V−1 . Consequently, if A = Q · U, then Q = A · U−1 ,
(1.146)
A = V · R, then R = V−1 · A.
(1.147)
and if
20
1. Vectors and Tensors
>
T dX
dx R
Figure 1.6. Decomposition of motions into a rotation and translation followed by a deformation.
dx
V
Now, QT · Q = (A · U−1 )T · (A · U−1 ) = (U−1 )T · AT · A · U−1 = U−1 · U2 · U−1 = I · I = I. Similarly, we ﬁnd that RT · R = I, and thus that Q and R are orthogonal tensors. With U = (AT · A)1/2 and V = (A · AT )1/2 we have established that A = Q · U = V · R.
(1.148)
The question is now, are Q and R unique? Suppose we proposed another decomposition, A = Q · U . Then AT · A = (Q · U )T · (Q · U ) = (U · Q T ) · (Q · U ) = (U )2 . But (U )2 = U2 and thus U = U. This means that Q = A · U−1 = Q
(1.149)
is unique! A similar consideration establishes the uniqueness of R. Finally, we ask if Q = R? To address this, write A = Q · U = (R · RT ) · (V · R) = R · (RT · V · R) = R · (V1/2 · R)T · (V1/2 · R) = R · (RT · V · R) = Q · U. Therefore, R = Q and U = RT · V · R. COROLLARY 1.1: If A is an invertible tensor and A = Q · U = V · Q, then
U has eigenvectors pi and eigenvalues λi , V has eigenvectors qi and eigenvalues µi , where λi = µi
and
qi = Q · pi .
1.19 Polar Decomposition: Physical Approach It is illustrative to view the motions involved in the polar decomposition discussed above as a sequential set of motions. This is schematically shown in Fig. 1.6.
1.19. Polar Decomposition: Physical Approach
21
1.19.1 Left and Right Stretch Tensors ˆ such that In the ﬁrst motion the element dX → dx, dxˆ = R · dX + T,
(1.150)
where T is a translation vector and R is an orthogonal tensor representing a rotation. This gives for a deformation gradient, ˆ Fˆ = ∂ x/∂X = R.
(1.151)
Since there is no deformation in this ﬁrst step, we have ˆ = Fˆ T · Fˆ = I = RT · R ⇒ R is orthogonal. C
(1.152)
Next, let dxˆ be deformed into the element dx via a pure deformation, dx = V · dxˆ = V · (R · dX + T) = (V · R) · dX + V · T, which yields F = V · R.
(1.153)
This is the left form of the polar decomposition. The tensor V is the left stretch tensor. Note that C = FT · F = (V · R)T · V · R = RT · VT · V · R = RT · V2 · R.
(1.154)
Alternatively, the total motion may be viewed as occurring ﬁrst via a pure deformation given so that dxˆ = U · dX,
(1.155)
followed by a rotation, R, and a translation, T. Theses motions result in dx = R · dxˆ + T = (R · U) · dX + T,
(1.156)
F = R · U.
(1.157)
and
The tensor U is the right stretch tensor. 1.19.2 Principal Stretches Write, again, dx = F · dX,
dX = NdS,
dx = nds,
(1.158)
where all quantities should have obvious meanings. Then the principal stretches can be expressed as (N)n = F · N
or
λ(n)n = F · N,
(1.159)
where (N) = λ(n) = ds/dS. Since N and n are unit vectors, N is transformed into n via n = R · N.
(1.160)
22
1. Vectors and Tensors
This relation implies that R = nN.
(1.161)
Thus, noting that F = R · U = V · R, we have (N)R · N = (R · U) · N = F · N or R · [U − (N)I] · N = 0.
(1.162)
[U − (N)I] · N = 0
(1.163)
For arbitrary R this leads to
for the principal stretch ratios, (N), in the unrotated principal directions, N. Similarly, we ﬁnd that λ(n)n = (V · R) · N = V · n,
(1.164)
[V − λ(n)I] · n = 0
(1.165)
which yields
for the principal stretch ratios in the rotated principal directions, n.
1.20 The Cayley–Hamilton Theorem LEMMA 1.10: Let f (λ) be a real polynomial and A an arbitrary tensor, and let λ be an
eigenvalue of A. Then if f (A) is the tensor obtained from the polynomial function of A constructed from the appropriate multiples (i.e., dot products) of A, then f (λ) is an eigenvalue of f (A). Also an eigenvector of f (A) associated with eigenvalue f (λ) is an eigenvector of A associated with λ. Proof: The proof is obtained using simple induction. Let p be an eigenvector of A associated with λ via the equation A · p = λp. Then, Ar · p = λr p
(1.166)
holds for r = 1. Assume that this relation holds for r = n. If we prove that it also holds for r = n + 1, we would have shown that it holds by induction for all r . Therefore, An+1 · p = A · (An · p) = A · (λn p) = λn+1 p,
(1.167)
and thus the relation holds for all r . Further, since f (A) is a linear combination of powers of A, it follows that f (λ) will be an eigenvalue of f (A) and p will be its associated eigenvector. THEOREM 1.2: Let A be an arbitrary tensor and the set of three λ’s be its associated eigen
values. Then, since the λ’s satisfy (1.96), we have λ3 − IA λ2 + I IA λ − I I IA = 0.
(1.168)
1.22. Relations Involving ∇ Operator
23
Apply Lemma 1.10 to this characteristic polynomial. This leads to the result that the tensor A3 − IA A2 + I IA A − I I IA I = 0 has three eigenvalues each equal to 0. The Cayley– Hamilton theorem states that for arbitrary A this tensor is 0. This means that the tensor, A, satisﬁes its own characteristic equation, i.e., (1.96).
1.21 Additional Lemmas for Tensors LEMMA 1.11: Consider the quadratic form
λ = A : (xx) = Ai j xi x j .
(1.169)
Then ∂λ/∂x = 2 sym (A) · x, ∂ λ/∂x ∂x = 2 sym (A), 2
(1.170)
or, in component form, ∂λ/∂ xi = (Ai j + Aji )x j , ∂ λ/∂ xi ∂ x j = Ai j + Aji . 2
(1.171)
Proof: Consider ∂λ/∂ xk = Ai j (∂ xi /∂ xk)x j + Ai j xi (∂ x j /∂ xk).
(1.172)
Since ∂ xi /∂ xk = δik, the substitution into the above, proves the ﬁrst assertion. The rest is proved simply by continuing the argument. LEMMA 1.12: If r 2 = x · x = xi xi and f (r ) is an arbitrary function of r , then
∇ f (r ) = f (r )x/r.
(1.173)
Proof: The components of ∇ f (r ) are ∂ f/∂ xi . Thus, ∂f ∂ f ∂r = ∂ xi ∂r ∂ xi
(1.174)
and since r 2 = x j x j and ∂r 2 /∂ x j = 2r ∂r/∂ x j = 2x j , it follows that ∂r/∂ x j = x j /r . Thus, ∂ f (r ) ∂ f ∂r ∂ f xi . = = ∂ xi ∂r ∂ xi ∂r r
(1.175)
1.22 Identities and Relations Involving ∇ Operator In this section several useful and illustrative results involving the gradient, and divergence, operation are given. They are listed as a collection of lemmas as follows.
24
1. Vectors and Tensors
LEMMA 1.13: Let r be a position vector and thus r = x1 e1 + x2 e2 + x3 e3 . Then
∇ · r = 3, ∇ × r = 0, r ∇ · 3 = 0. r
(1.176)
Proof: The proof of the ﬁrst assertion is straightforward, since ∂ xi /∂ x j = δi j and ∇·r=
∂ xi = 3. ∂ xi
(1.177)
The curl of r is taken so that its i th component is i jk∂ xk/∂ x j . But ∂ xk/∂ x j = δkj and this leads to i jkδkj = 0, because i jk = −ikj and δkj = δ jk. This proves the second assertion. The third equation is expressed as ∇·
r ∂ xi ∂r −3 1 = = 3 3 + xi . 3 3 r ∂ xi r r ∂ xi
(1.178)
Since r 2 = xi xi , we ﬁnd r
∂r = xi , ∂ xi
∂r ∂r −3 = −3r −4 = −3r −5 xi . ∂ xi ∂ xi
(1.179)
Substituting this result in the expression for ∇ · (r/r 3 ) given above proves the lemma. LEMMA 1.14: Let f (u, v) be a scalar function of u and v, where u = u(x) and v = v(x).
Then the gradient of f may be expressed as ∇ f (x) =
∂f ∂f ∇u + ∇v. ∂u ∂v
(1.180)
Proof: First write the gradient of f as ∇f =
∂f ei . ∂ xi
(1.181)
By the chain rule of calculus, ∂f ei = ∂ xi
∂ f ∂u ∂ f ∂v + ∂u ∂ xi ∂v ∂ xi
ei .
(1.182)
When this expression is expanded, and its terms reassembled, it is found that ∇ f (x) =
∂f ∂f ∇u + ∇v, ∂u ∂v
(1.183)
as desired. LEMMA 1.15: Let f (x) be a scalar ﬁeld and G a vector ﬁeld. Then
∇ · ( f G) = ∇ f · G + f ∇ · G.
(1.184)
1.23. Suggested Reading
25
Proof: We again use the chain rule of calculus to write ∇ · ( f G) =
∂( f Gi ) ∂f ∂Gi = Gi + f ∂ xi ∂ xi ∂ xi
(1.185)
= ∇ f · G + f ∇ · G. LEMMA 1.16: If u is a vector ﬁeld then,
∇ · (∇ × u) = 0,
(1.186)
or, in other words, the divergence of the curl vanishes. Proof: When expressed in component form, this is ∂ ∂uk ∂ 2 uk i jk = i jk . ∂ xi ∂xj ∂ xi ∂ x j
(1.187)
But this will vanish because the second derivatives of u are symmetric, whereas i jk is antisymmetric in i j, so that i jkuk,i j = 0.
1.23 Suggested Reading There are a number of excellent texts and reference books concerned with vector and tensor algebra in physics and applied mathematics. Those that are speciﬁcally concerned with or provide a framework directly relevant to applications to solid mechanics include Synge and Shild (1949), Ericksen (1960), Brillouin (1964), Wrede (1972), and Boehler (1987). The reader is also directed to Chadwick (1999) for an excellent summary of such results as applied to the analysis of deformation and forces. The following is a list of books recommended for additional reading. Boehler, J. P. (1987), Application of Tensor Functions in Solid Mechanics, SpringerVerlag, Wien. Brillouin, L. (1964), Tensors in Mechanics and Elasticity, Academic Press, New York. Chadwick, P. (1999), Continuum Mechanics: Concise Theory and Problems, Dover Publications, Mineola, New York. Ericksen, J. L. (1960), Tensor Fields. In Hanbuch der Physik (S. Flugge, ed.), Band III/1, SpringerVerlag, Berlin. Eringen, A. C. (1971), Tensor Analysis. In Continuum Physics (A. C. Eringen, ed.), Vol. 1, Academic Press, New York. Spencer, A. J. M. (1971), Theory of Invariants. In Continuum Physics (A. C. Eringen, ed.), Vol. 1, Academic Press, New York. Synge, J. L., and Schild, A. (1949), Tensor Calculus, University Press, Toronto. Wrede, R. C. (1972), Introduction to Vector and Tensor Analysis, Dover Publications, New York.
2 Basic Integral Theorems
2.1 Gauss and Stokes’s Theorems The divergence theorem of Gauss may be expressed as follows: THEOREM 2.1: If V is a volume bounded by the closed surface S and A is a vector ﬁeld that
possesses continuous derivatives (and is singled valued in V), then ∇ · A dV = A · n dS = A · dS, V
S
(2.1)
S
where n is the outward pointing unit normal vector to S. Note that we may extend this result to the case where A is a tensor ﬁeld with the same proviso’s. The basic theorem is proven below. Stokes’s theorem takes the following form: THEOREM 2.2: If S is an open, twosided surface bounded by a closed, nonintersecting curve C, and if A again has continuous derivatives, then A · dr = (∇ × A) · n dS = (∇ × A) · dS, (2.2) C
S
S
where C is measured positive if the motion along it is counterclockwise (then S would be on the left). A special case of Stokes’s theorem for the plane is THEOREM 2.3: If S is a closed region of the x − y plane bounded by a closed curve S, and if
M(x, y) and N(x, y) are two continuous functions having continuous derivatives in S, then ∂N ∂M − dS, (2.3) M(x, y) dx + N(x, y) dy = ∂x ∂y C S where C is traversed in the same positive direction. 26
2.2. Vector and Tensor Fields
27
2.1.1 Applications of Divergence Theorem A useful application of the divergence theorem involves the computation of the volume of a solid. Consider the integral r · n dS, (2.4) S
where r is the position vector and all other quantities have their obvious meanings as above. The divergence theorem states that r · n dS = ∇ · r dV S
V
=
∇ · (xi ei ) dV =
V
Next, consider the integral
V
∂ xi dV = 3V. ∂ xi
(2.5)
∇ϕ dV,
(2.6)
V
where ϕ is a scalar function of position. To interpret this, deﬁne a vector a = ϕb0 where b0 is an arbitrary constant vector. Then, ∇ · (ϕb0 ) dV = ϕb0 · n dS V
S
V
b0 · ∇ϕ dV
= =
(2.7)
b0 · (ϕn) dS. S
Now take the constant vector, b0 , out of the integrals and note that it was indeed arbitrary. Thus, what is established is ∇ϕ dV = ϕn dS. (2.8) V
S
Clearly other useful integral lemmas may be derived by similar manipulations of the Gauss or Stokes theorems.
2.2 Vector and Tensor Fields: Physical Approach Consider, as an example, ﬁelds that arise from electrostatics and Coulomb’s law. If f is the force between two charged points at distance r with charges q and q0 , its representation is given as f=
1 qq0 ˆ u. 4π 0 r 2
(2.9)
The permeability of the vacuum is 0 . As shown in Fig. 2.1, uˆ is the unit vector from charge q to charge q0 and r is the distance between them. Now introduce a vector ﬁeld E(x1 , x2 , x3 ) such that E(x1 , x2 , x3 ) = E(r) =
1 q ˆ u. 4π 0 r 2
(2.10)
28
2. Basic Integral Theorems q
x 2 e1
q
>
e 2
0
r
u
Figure 2.1. Interaction of point charges.
x 1 e 3 x
3
Thus the force exerted on charge q0 from the ﬁeld of charge q can be expressed as f = Eq0 .
(2.11)
Now let there be as many as n charges, each with a net charge qi . The force they exert on the test charge q0 is given by the linear superposition, n qi uˆ q0 . f(r) = (2.12) 4π 0 r − ri 2 i=1 Thus, we deﬁne the ﬁeld arising from this distribution of charges as E(r) =
n i=1
qi ˆ u. 4π 0 r − ri 2
Finally, if we deﬁne a continuous charge density by the limit ρ = limv→0 charge in volume V is ρ(x1 , x2 , x3 ) dV. Q=
(2.13) q , v
the total
(2.14)
V
The total ﬁeld arising from this continuous distribution of charge is, therefore, 1 ρ(x1 , x2 , x3 )uˆ E(r) = dV. 4π 0 V r − r 2
(2.15)
Such is an example of a simple vector ﬁeld.
2.3 Surface Integrals: Gauss Law We will be interested in integrals evaluated over a surface of the general form, such as arises in the Gauss law E(x) · n dS = q/ , (2.16) S
where n is the outward pointing unit normal vector to the surface S. The normal to the surface can be deﬁned as n = u × v,
(2.17)
where u and v are locally unit vectors, tangent to the surface element as sketched in Fig. 2.2. If u and v are not unit vectors, then n=
u×v . u × v
(2.18)
2.4. Evaluating Surface Integrals
29
C' v x3 x2
Figure 2.2. Deﬁning the local normal to a surface.
C u
x1
Let the surface be given by g(x1 , x2 , x3 ) = 0
⇒
x3 = f (x1 , x2 ).
(2.19)
Imagine following the curve over an arc C, along x1 . The corresponding displacement undergone would be u = u1 e1 + (∂ f/∂ x1 )u1 e3 .
(2.20)
Similarly, on an arc C , along x2 , we obtain v = v2 e2 + (∂ f/∂ x2 )v2 e3 .
(2.21)
Thus, N = u × v = (−∂ f/∂ x1 e1 − ∂ f/∂ x2 e2 + e3 )u1 v2 , n=
−∂ f/∂ x1 e1 − ∂ f/∂ x2 e2 + e3 u×v = . u × v [1 + (∂ f/∂ x1 )2 + (∂ f/∂ x2 )2 ]1/2
(2.22)
2.4 Evaluating Surface Integrals Examine the integral
G(x1 , x2 , x3 ) dS,
(2.23)
S
where G may be either a scalar or tensor ﬁeld. Such integrals may be considered as the limit of a summation over an inﬁnite number of inﬁnitesimal surface elements (Fig. 2.3), i.e., N G(x1 , x2 , x3 ) dS = lim G(x1i , x2i , x3i )Si . (2.24) N→∞
S
ni
Si →0 i=1
∆ Si
x
3
∆Si
S
x2 x1 Figure 2.3. Limiting approach to evaluating surface integrals.
∆ Ri
30
2. Basic Integral Theorems
We want to relate these surface elements to the projections they make on the x1 − x2 coordinate plane. Note that if Ri is the projection of Si , then Si = Ri /(n · e3 ).
(2.25)
Thus, G(x1 , x2 , x3 ) dS = lim
N→∞ Ri →0
S
which in the limit becomes
R
N
G(x1i , x2i , x3i )Ri /(n · e3 ),
(2.26)
i=1
G(x1 , x2 , x3 ) dx1 dx2 . n · e3
(2.27)
Since on S, x3 = f (x1 , x2 ), and recalling the result from (2.22) for n, (2.26) becomes
1/2 G(x1 , x2 , x3 ) dS = G(x1 , x2 , f ) 1 + (∂ f/∂ x1 )2 + (∂ f/∂ x2 )2 dx1 dx2 . (2.28) S
R
If, instead, we had used projections on the x1 − x3 plane, we would have
1/2 G(x1 , x2 , x3 ) dS = G[x1 , g(x1 , x2 ), x3 ] 1 + (∂g/∂ x1 )2 + (∂g/∂ x2 )2 dx1 dx3 , S
R
(2.29) where x2 = g(x1 , x3 ).
(2.30)
Alternatively, on the x2 − x3 plane,
1/2 G(x1 , x2 , x3 ) dS = G[h(x2 , x3 ), x2 , x3 ] 1 + (∂h/∂ x2 )2 + (∂h/∂ x3 )2 dx2 dx3 , S
R
(2.31) where x = h(x2 , x3 ). We are, however, even more interested in integrals of the form, F · n dS,
(2.32)
(2.33)
S
such as appears in (2.16). Replace G with F · n in (2.28) to obtain
1/2 F · n dS = F · n 1 + (∂ f/∂ x1 )2 + (∂ f/∂ x2 )2 dx1 dx2 . S
(2.34)
R
The substitution of (2.22) into the above gives
−F1 (∂ f/∂ x1 ) − F2 (∂ f/∂ x2 ) + F3 [x1 , x2 , f (x1 , x2 )] dx1 dx2 , F · n dS = S
or
R
−F1 [x1 , x2 , f (x1 , x2 )](∂ f/∂ x1 ) − F2 [x1 , x2 , f (x1 , x2 )](∂ f/∂ x2 )
F · n dS = S
R
+F3 [x1 , x2 , f (x1 , x2 )] dx1 dx2 ,
2.5. The Divergence
31
υ∆t ∆S Figure 2.4. Flux of ﬂuid through a cylinder.
θ n
where F = F1 e1 + F2 e2 + F3 e3 .
(2.35)
2.4.1 Application of the Concept of Flux The ﬂux of the vector ﬁeld F through the surface S is deﬁned by F · n dS ,
(2.36)
S
where n is a unit outward normal to S. For example, consider the ﬂow of ﬂuid through a cylinder, during a time increment t, as depicted in Fig. 2.4. With υ as the velocity, the distance travelled in time t is υt, where υ is the magnitude of υ. The volume of ﬂuid ﬂowing through the surface inclined as shown is equal to υt cos θ. The mass of ﬂuid ﬂowing through the inclined surface is, with ρ as the mass density, ρυt cos θ = ρtυ · n, and thus the rate of mass ﬂow through the inclined surface is ρυ · nS. As shown in the sketch, S is the area of the inclined surface element. Thus, if we deﬁne F ≡ ρυ(x1 , x2 , x3 ), we ﬁnd that
(2.37)
Rate of mass ﬂow through S =
F · n dS.
(2.38)
S
2.5 The Divergence Recall the Gauss law
E(x) · n dS = q/0 .
(2.39)
S
Let q = ρ¯V V, where ρ¯V is the average charge density in V. Then, E(x) · n dS = ρ¯V V/0 , 1 V
S
(2.40) E(x) · n dS = ρ¯V /0 .
S
Taking an appropriate limit, there follows 1 lim E(x) · n dS = ρ(x1 , x2 , x3 )/0 . V→0 V S
(2.41)
32
2. Basic Integral Theorems
Figure 2.5. A cuboid with edges aligned with the coordinate axes.
Now, deﬁne the divergence of F to be 1 V→0 V
div F ≡ lim
F · n dS.
(2.42)
S
The Gauss law then becomes div F = ρ/0 .
(2.43)
We next calculate div F over a cuboid whose volume shrinks to zero (Fig. 2.5). Calculate ﬁrst F · n dS, (2.44) S1±
on S1+ , where F · n = F · e1 = F1 (x1 , x2 , x3 ). Take the centroid of the cuboid at (x1 , x2 , x3 ). On S1+ we have F · n = F1 ≈ F1 (x1 , x2 , x3 ) + (∂ F1 /∂ x1 )dx1 /2,
(2.45)
F · n = −F1 ≈ −F1 (x1 , x2 , x3 ) + (∂ F1 /∂ x1 )dx1 /2.
(2.46)
while on S1− ,
Thus, we obtain + = [∂ F1 (x1 , x2 , x3 )/∂ x1 ] dx1 dx2 dx3 = [∂ F1 (x1 , x2 , x3 )/∂ x1 ]dx1 S1± , S1+
S1−
where S1± = dx2 dx3 . This also shows that 1 lim F · n dS = ∂ F1 /∂ x1 . V→0 V S± 1 By the same sort of argument we have 1 lim F · n dS = ∂ F2 /∂ x2 , V→0 V S± 2 and 1 V→0 V lim
(2.47)
(2.48)
S3±
F · n dS = ∂ F3 /∂ x3 .
(2.49)
2.6. Divergence Theorem
33
S V i i V ∆S ∆ e me fac u l r o u bv s su ith w
S
S S1
V
V2
n2
(a)
V1
n1
(b)
Figure 2.6. Limiting approach to evaluating surface integrals.
Consequently, div (F) = ∂ F1 /∂ x1 + ∂ F2 /∂ x2 + ∂ F3 /∂ x3 .
(2.50)
∇ ≡ ∂/∂ x1 e1 + ∂/∂ x2 e2 + ∂/∂ x3 e3 ,
(2.51)
Letting
we can write ∇ · F = (∂/∂ x1 e1 + ∂/∂ x2 e2 + ∂/∂ x3 e3 ) · (F1 e1 + F2 e2 + F3 e3 ) = ∂ F1 /∂ x1 + ∂ F2 /∂ x2 + ∂ F3 /∂ x3 .
(2.52)
This yields another expression of the Gauss law, namely ∇ · E = ρ/0 .
(2.53)
2.6 Divergence Theorem: Relation of Surface to Volume Integrals Assume that
F · n dS = S
N i=1
F · n dS,
(2.54)
Si
as sketched in Fig. 2.6. The two subsurface integrals over S1 and S2 include the integrals over the subsurface facet common to both small subelements. The value of F is the same at each point on this common facet (if F is continuous). But the outward pointing normals n on such a common facet are such that at each point, n1 = −n2 . Thus, the integrals over the facet cancel. With this in mind, rewrite (2.54) as N 1 F · n dS = F · n dS Vi . (2.55) Vi Si S i=1 Taking the limit as N → ∞, or as Vi → 0, we have N 1 F · n dS = lim F · n dS Vi . N→∞ Vi Si S i=1 Vi →0
(2.56)
34
2. Basic Integral Theorems
But the term within (. . .) in (2.56) is in fact ∇ · F and thus F · n dS = ∇ · F dV. S
(2.57)
V
This is the Gauss divergence theorem. To illustrate its application, consider the rate of ﬂow of mass through a surface S, i.e., ﬂow rate = ρυ · n dS. (2.58) S
Let the surface S be closed. Then we can write
amount of mass in V =
ρ dV,
(2.59)
∂ρ/∂t dV.
(2.60)
V
and change of mass within V = unit time
V
The conservation of mass requires that ∂ρ/∂t dV = − ρυ · n dS. V
Applying the divergence theorem to the second integral in (2.61), we obtain (ρυ) · n dS = ∇ · (ρυ) dV. S
Consequently,
(2.61)
S
(2.62)
V
∂ρ/∂t dV = − V
∇ · (ρυ) dV.
(2.63)
V
Since this is true for all V, we conclude that ∂ρ/∂t = −∇ · (ρυ),
(2.64)
which is known as a continuity equation.
2.7 More on Divergence Theorem Another form of the divergence theorem of interest for later application can be stated as follows. LEMMA 2.1: If S is the surface bounding the volume V, and n is its unit outward pointing
normal, and u(x) and T(x) are arbitrary vector and tensor ﬁelds in V, then T u T · n dS = [u∇ · T + (∇u) · T ] dV. S
(2.65)
V
Some special cases immediately follow. For example, if u is a ﬁxed vector, then T u T · n dS = u ∇ · T dV. (2.66) S
V
2.8. Suggested Reading
35
Because u is arbitrary, (2.66) implies that TT · n dS = ∇ · T dV. S
(2.67)
V
Suppose further that T = I. Then (2.66) becomes un dS = ∇u dV. S
By taking the trace of both sides of (2.68), we obtain u · n dS = ∇ · u dV. S
(2.68)
V
(2.69)
V
It should be noted that (2.65) can, in fact, be derived from (2.69) by setting u to be (u · a)(T · b), where a and b are arbitrary vectors.
2.8 Suggested Reading Malvern, L. E. (1969), Introduction to the Mechanics of a Continuous Medium, Prentice Hall, Englewood Cliffs, New Jersey. Marsden, J. E., and Tromba, A. J. (2003), Vector Calculus, 5th ed., W. H. Freeman and Company, New York. Truesdell, C., and Toupin, R. (1960), The Classical Field Theories. In Handbuch der Physik (S. Flugge, ¨ ed.), Band III/l, SpringerVerlag, Berlin. Wrede, R. C. (1972), Introduction to Vector and Tensor Analysis, Dover, New York.
3 Fourier Series and Fourier Integrals
3.1 Fourier Series Let f (x) be a continuous, integrable function deﬁned on the interval [−c, c]. Consider the Fourier series of f (x), viz., f (x) = (a0 /2) +
∞ [ak cos(kπ x/c) + bk sin(kπ x/c)].
(3.1)
k=1
The coefﬁcients, ak and bk, indexed by the integers k, can be identiﬁed as follows. Multiply each side of (3.1) by cos(nπ x/c), n being an integer, and integrate over [−c, c] to obtain c c f (x) cos(nπ x/c) dx = (a0 /2) cos(nπ x/c) dx −c
−c
+
∞ c
−c k=1
[ak cos(kπ x/c) cos(nπ x/c)
+ bk sin(kπ x/c) cos(nπ x/c)] dx. To proceed, we note that c cos(kπ x/c) cos(nπ x/c) dx = c/π −c
π
−π
cos(kλ) cos(nλ) dλ,
(3.2)
where λ = π x/c, Thus,
and
⎧ ⎪ ⎪ π ⎨0, k = n , cos(kλ) cos(nλ) dλ = π, k = n , ⎪ −π ⎪ ⎩2π, k = n = 0 ,
π
−π
36
dλ = (π/c) dx.
sin(kλ) cos(nλ) dλ = 0.
(3.3)
(3.4)
(3.5)
3.2. Double Fourier Series
37
Similarly,
π −π
sin(kλ) sin(nλ) dλ =
0,
k = n ,
π,
k = n,
(3.6)
as long as k = 0 and n = 0. Consequently,
⎧ ⎪ ⎪ c ⎨0, k = n , cos(kπ x/c) cos(nπ x/c) dx = c, k = n , ⎪ −c ⎪ ⎩2c, k = n = 0 ,
and
c
−c
Therefore, we obtain an =
1 c
c
−c
cos(kπ x/c) sin(nπ x/c) dx = 0.
f (x) cos(nπ x/c) dx. n = 0, 1, 2, . . . .
(3.7)
(3.8)
(3.9)
Likewise, if (3.1) were multiplied by sin(nπ x/c) and integrated over the interval [−c, c], it would be found that 1 c f (x) sin(nπ x/c) dx, n = 1, 2, . . . . (3.10) bn = c −c It is noted in passing that if f (x) were an odd function of x, such that f (−x) = − f (x), then an = 0 for all n. Likewise if f (−x) = f (x), that is if f (x) were an even function of x, then bn = 0.
3.2 Double Fourier Series Let R be a rectangle deﬁned by the region −a ≤ α ≤ a, −b ≤ β ≤ b, and let ϕn (α, β) be a set of continuous functions, none of which vanishes identically in R. Such a set is said to be orthogonal if ϕn (α, β)ϕm(α, β) dα dβ = 0, if n = m. (3.11) R
The number
1/2
ϕn = R
ϕn2 (α, β) dα dβ
(3.12)
is called the norm of ϕn . The set is said to be normalized if ϕn = 1, for n = 0, 1, 2, . . . . It is equivalent for normalization that ϕn2 (α, β)dα dβ = 1, for n = 0, 1, 2, . . . . (3.13) R
Of course, it is always possible to deﬁne constants, say µn , such that µn =
1 , ϕn
which can be used to normalize the members of the set ϕn .
(3.14)
38
3. Fourier Series and Fourier Integrals
As was done for a function of a single variable, it is possible to expand a function of two variables in terms of these orthogonal functions as f (α, β) = c0 ϕ0 (α, β) + c1 ϕ1 (α, β) + . . . + cn ϕn (α, β) + . . . .
(3.15)
The coefﬁcients are obtained by using the orthogonality property. This gives cn =
f (α, β)ϕn (α, β) dα dβ R 2 R ϕ (α, β) dα dβ
.
(3.16)
If it is assumed that the equality holds in (3.15), the series will converge uniformly.
3.2.1 Double Trigonometric Series Consider the orthogonal set consisting of the functions 1, cos(mx), sin(mx), cos(ny), sin(ny) , cos(mx) cos(ny), sin(mx) cos(ny) ,
(3.17)
cos(mx) sin(ny), sin(mx) sin(ny), . . . , (n, m = 1, 2, 3, . . .) . These are clearly orthogonal on the square deﬁned by −π ≤ x ≤ π and −π ≤ y ≤ π. For reference we note that the norms are 1 = 2π, cos(mx) = sin(mx) =
√ 2π ,
cos(mx) cos(ny) = sin(mx) sin(ny) = cos(mx) sin(ny) = π.
(3.18)
The above leads to the following system amn = bmn cmn dmn
1 π2
1 = 2 π 1 = 2 π 1 = 2 π
f (x, y) cos(mx) cos(ny) dx dy,
R
R
R
f (x, y) sin(mx) cos(ny) dx dy, (3.19) f (x, y) cos(mx) sin(ny) dx dy, f (x, y) sin(mx) sin(ny) dx dy, R
for m, n = 1, 2, . . . . For the cases where either m = 0 or n = 0, we have
f (x, y) cos(mx) dx dy cos(mx)2 1 = f (x, y) cos(mx) dx dy, (m = 1, 2, . . .), 2π 2 R
Am0 =
R
(3.20)
3.3. Integral Transforms
39
f (x, y) cos(ny) dx dy cos(ny)2 1 = f (x, y) cos(ny) dx dy, (n = 1, 2, . . .), 2π 2 R
A0n =
R
(3.21)
f (x, y) sin(mx) dx dy sin(mx)2 1 = f (x, y) sin(mx) dx dy, (m = 1, 2, . . .), 2π 2 R
Bm0 =
R
(3.22)
f (x, y) sin(ny) dx dy sin(ny)2 1 = f (x, y) sin(ny) dx dy, (n = 1, 2, . . .). 2π 2 R
B0n =
R
(3.23)
Note that for symmetry of expression we may deﬁne Am0 = 12 am0 , with similar deﬁnitions for the other A and B terms. Finally note that f (x, y) dx dy 1 = f (x, y) dx dy, (3.24) A00 = R 1 4π 2 R whereby we may deﬁne A00 = 14 a00 . When this is assembled, the series expansion may be written as ∞
f (x, y) =
λmn [amn cos(mx) cos(ny) + bmn sin(mx) cos(ny) (3.25)
m,n=0
+cmn cos(mx) sin(ny) + dmn sin(mx) sin(ny)], with 1 , for m = n = 0, 4 1 = , for m > 0, n = 0 or m = 0, n > 0, 2
λmn = λmn
λmn = 1 ,
(3.26)
for m, n > 0.
The rectangular domain of interest is easily transformed into the area deﬁned by −a ≤ α ≤ a and −b ≤ β ≤ b by the change in variables, x = π α/a, y = πβ/b.
3.3 Integral Transforms Let f (x) be a function that has a convergent integral over the domain [0, ∞]. Also let K(αx) deﬁne a function of (α, x). Then, if the integral ∞ f (x)K(αx) dx (3.27) I f (α) = 0
40
3. Fourier Series and Fourier Integrals
is convergent, then I f (α) is the integral transform of f (x) by the kernel K(αx). If for each I f (α), (3.27) is satisﬁed by only one f (x), then (3.27) has an inverse ∞ I f (α)H(αx) dα. (3.28) f (x) = 0
If H(αx) = K(αx), then K(αx) is a Fourier kernel. A Mellin transform of K(x) is deﬁned as ∞ K(x)x s−1 dx. K(s) =
(3.29)
0
LEMMA 3.1: If K(αx) is a Fourier kernel then K(s)K(1 − s) = 1.
Proof: By deﬁnition,
∞
K(s) =
K(x)x s−1 dx,
(3.30)
0
and thus, by implication, ∞ s−1 α I f (α) dα = 0
∞
α
f (x)K(αx) dx dα
0
∞
s−1 0
∞
=
∞
f (x) dx 0
(3.31) α
s−1
K(αx) dα.
0
Now let η ≡ αx, and write ∞ K(αx)α s−1 dα = x −s 0
∞
K(η)ηs−1 dη = x −s K(s).
(3.32)
0
Then,
∞
α
s−1
∞
I f (α) dα = I(s) =
0
x −s f (x) dx K(s) (3.33)
0
= K(s)F(1 − s). Furthermore, if
f (x) =
∞
I f (α)K(αx) dα,
(3.34)
0
we have
∞
f (x)x
s−1
dx =
0
∞
x
s−1
0
=
I f (α)K(αx) dα dx 0
∞
(3.35)
∞
I f (α) dα 0
x
s−1
K(αx) dx.
0
Thus, when compared with (3.33), ∞ I f (α)α −s dα F(s) = 0
∞
∞
ηs−1 K(η) dη = I(1 − s)K(s),
(3.36)
0
which shows that F(1 − s) = I(s)K(1 − s),
(3.37)
3.3. Integral Transforms
41
and, therefore, K(s)K(1 − s) = 1, as desired. For example, if
2/π cos(αx),
K(αx) =
the Fourier cosine transform of a function f (x) is ∞ f (x) cos(αx) dx, Fc (α) = 2/π
(3.38)
(3.39)
(3.40)
0
with its inverse f (x) =
2/π
∞
Fc (α) cos(αx) dα.
(3.41)
0
As another example, let K(αx) be deﬁned as K(αx) = 2/π sin(αx). The corresponding set of transform and inverse is ∞ f (x) sin(αx) dx, Fs (α) = 2/π
(3.42)
(3.43)
0
and
f (x) = 2/π
∞
Fs (α) sin(αx) dα.
(3.44)
0
By the lemma proved above, if
∞
I f (α) =
f (x)K(αx) dx,
(3.45)
I f (α)H(αx) dα,
(3.46)
0
then
∞
f (x) = 0
and K(s)H(1 − s) = 1,
(3.47)
where K(s) and H(s) are the Mellin transforms of K(x) and H(x), respectively. In short, what is desired is to show that if f (x) is deﬁned on [0, ∞], then it is possible that ∞ 2 ∞ dα f (η) cos(αη) cos(αx) dη, (3.48) f (x) = π 0 0 or, more generally, 1 f (x) = π
∞
−∞
dα
∞
−∞
f (η) cos(αη) cos(αx) dη.
(3.49)
Before exploring this, it is necessary to establish some integrability properties of f (x). This is done next.
42
3. Fourier Series and Fourier Integrals
f(x) Figure 3.1. Function with ﬁnite number of extrema and discontinuities.
a a1 a 2 ..... a0
ap b x a p+1
3.4 Dirichlet’s Conditions We say that the function f (x) satisﬁes Dirichlet’s conditions if (1) f (x) has only a ﬁnite number of extrema in an interval [a, b], and (2) f (x) has only a ﬁnite number of discontinuities in the interval [a, b] and no inﬁnite discontinuities. Let a0 = a, a p+1 = b and ai , i = 1, 2, . . . , p be the points where f (x) has either an extrema or a discontinuity, as depicted in Fig. 3.1. The satisfaction of Dirichelet’s conditions leads to the following lemmas. LEMMA 3.2: If f (x) satisﬁes Dirichlet’s conditions in the interval [a, b], then
b
lim
ω→∞ a
lim
ω→∞ a
b
f (x) sin(ωx) dx = 0, (3.50) f (x) cos(ωx) dx = 0.
Proof: From the deﬁnition of the ai above we may rewrite the ﬁrst of the integrals as a
b
f (x) sin(ωx) dx =
p k=0
ak+1
f (x) sin(ωx) dx.
(3.51)
ak
In each subinterval f (x) is monotone, either increasing or decreasing, and by the second mean value theorem of calculus we have ak+1 ζ f (x) sin(ωx) dx = f (ak + 0) sin(ωx) dx ak
ak
+ f (ak+1 − 0)
ζ
(3.52)
ak+1
sin(ωx) dx,
where ζ is a point in the subinterval [ak, ak+1 ]. When the integrations are performed, there results ak+1 cos(ωak) − cos(ωζ ) f (x) sin(ωx) dx = f (ak + 0) ω ak (3.53) cos(ωζ ) − cos(ωak+1 ) . + f (ak+1 − 0) ω
3.4. Dirichlet’s Conditions
43
f(x) f(x+0)
Figure 3.2. Values of a discontinuous function.
f(x0) x
Thus, lim
ω→∞ a
b
f (x) sin(ωx) dx = 0.
(3.54)
Since p is ﬁnite, we obtain
b
lim
ω→∞ a
f (x) sin(ωx) dx =
p k=0
lim
ak+1
ω→∞ a k
f (x) sin(ωx) dx = 0,
(3.55)
as proposed above. The proposal in the second of (3.50) is proved by a similar procedure. The same considerations lead to the following additional results that are proved in standard textbooks on integral transforms. LEMMA 3.3: If f (x) satisﬁes the Dirichlet conditions on the interval [a, b], then
lim
ω→∞ a
b
0, if a > 0, sin(ωx) dx = 1 f (x) x π f (0+ ), if a = 0. 2
(3.56)
More generally, LEMMA 3.4: If f (x) satisﬁes Dirichlet’s conditions on the interval [a, b], then
2 lim ω→∞ π
a
b
⎧ ⎪ f (x + 0) + f (x − 0), if a < 0 < b, ⎪ ⎪ ⎪ ⎨ f (x + 0), if a = 0 < b, sin(ωu) du = f (x + u) ⎪ x f (x − 0), if a < 0 = b, ⎪ ⎪ ⎪ ⎩ 0, if 0 < a < b or a < b < 0.
Proof: The proof of this lemma requires the following identity, which is demonstrated ﬁrst, viz., π f (x + 0) + f (x − 0) 1 sin(n + 1/2)u lim du = . (3.57) f (x + u) n→∞ π 2 sin(u/2) 2 −π It is, for this purpose, sufﬁcient to show that (Fig. 3.2) π f (x + 0) 1 sin(n + 1/2)u lim du = , f (x + u) n→∞ π 2 sin(u/2) 2 0 0 f (x − 0) 1 sin(n + 1/2)u lim du = . f (x + u) n→∞ π 2 sin(u/2) 2 −π
(3.58) (3.59)
44
3. Fourier Series and Fourier Integrals
Focus on the demonstration of the ﬁrst of these, as the proof of the second follows similar lines. It is readily shown that π 1 sin(n + 1/2)u 1 f (x + 0) = du, (3.60) f (x + 0) 2 π 0 2 sin(u/2) which leads to the strategy of proving that π 1 sin(n + 1/2)u lim du = 0. [ f (x + u) − f (x + 0)] n→∞ π 2 sin(u/2) 0
(3.61)
Consider the function of u deﬁned by ϕ(u) =
f (x + u) − f (x + 0) f (x + u) − f (x + 0) u = . 2 sin(u/2) u 2 sin(u/2)
(3.62)
Since this function has a derivative at x + 0, the ratio f (x + u) − f (x + 0)/u exists as u → 0. This means that this same ratio is absolutely integrable on the interval 0 ≤ x ≤ π. But the function u/2 sin(u/2) is bounded, and so the function deﬁned as ϕ(u) is integrable on 0 ≤ x ≤ π. We furthermore have that π π sin(n + 1/2)u du = [ f (x + u) − f (x + 0)] ϕ(u) sin(n + 1/2)u du. (3.63) 2 sin(u/2) 0 0 To continue with the proof, note that for any > 0, the inequality δ 1 1  f (x + u) du < π −δ 2
(3.64)
holds for sufﬁciently small δ. The function (1/u) f (x + u) is absolutely integrable over −∞ < u ≤ −δ and δ ≤ u < ∞. Therefore, by the previous lemma we have ∞ −δ 1 1 sin(u) sin(u) lim du = lim du = 0. f (x + u) f (x + u) →∞ π →∞ π u u δ −∞ Next consider the equality π f (x + 0) + f (x − 0) 1 sin(mu) lim du = , f (x + u) m→ ∞ π 2 sin(u/2) 2 −π
(3.65)
which has already been demonstrated, and where m = n + 1/2 for integer n. This can be rewritten as δ f (x + 0) + f (x − 0) 1 sin(mu) lim du = , (3.66) f (x + u) m→ ∞ π 2 sin(u/2) 2 −δ because the integrals on the intervals −π ≤ u ≤ −δ and δ ≤ u ≤ π vanish as m → ∞. Note that the integral on the lhs of (3.66) differs from δ 1 sin(mu) du (3.67) f (x + u) π −δ u by the quantity 1 π
δ −δ
1 1 − f (x + u) sin(mu) du, 2 sin(u/2) u
(3.68)
3.4. Dirichlet’s Conditions
45
where the function in [...] is continuous and where it is seen to be zero at u = 0 (by appropriate limits). But the integral in (3.68) vanishes in the limit as m → ∞, and (3.66) can be replaced by 1 lim m→ ∞ π
δ −δ
f (x + u)
sin(mu) f (x + 0) + f (x − 0) du = . u 2
(3.69)
Now, let m ≤ < m + 1, so that = m + ξ , where 0 ≤ ξ < 1. The mean value theorem of calculus gives sin(u) − sin(mu) = ( − m) cos(hu), u
(3.70)
where m ≤ h ≤ . Therefore, for any , 1 π
δ
−δ
f (x + u)
sin(u) du − u
δ
f (x + u)
−δ
1 δ = f (x + u)ξ cos(hu) du π −δ δ 1 ≤  f (x + u) du < . π −δ 2
sin(mu) du u (3.71)
For large and m, we have δ f (x + 0) + f (x − 0) 1 sin(mu) − du < . f (x + u) 2 π −δ u 2
(3.72)
Thus, combining the last two inequalities, we ﬁnd that δ f (x + 0) + f (x − 0) 1 sin(u) − du < , f (x + u) 2 π −δ u 2
(3.73)
for all sufﬁciently large . Finally, by (3.4), ∞ f (x + 0) + f (x − 0) 1 sin(u) − du < , f (x + u) 2 π −∞ u 2
(3.74)
for sufﬁciently large . This proves the lemma in question. LEMMA 3.5: If f (x) satisﬁes the Dirichlet conditions on the interval [a, b], then
1 1 [ f (x + 0) + f (x − 0)] = 2 π
∞
dα 0
∞
−∞
f (η) cos[α(η − x)] dη,
(3.75)
and, if f (x) is continuous, f (x) =
1 π
∞
dα 0
∞
−∞
f (η) cos[α(η − x)] dη.
(3.76)
This last lemma will be used below to demonstrate an integral inversion theorem.
46
3. Fourier Series and Fourier Integrals
Proof: We again suppose that f (x) is absolutely integrable on the entire x axis. Then, by the deﬁnition of an improper integral, we have 1 π
∞
dλ
∞
−∞
0
1 →∞ π
f (u)cosλ(u − x) du = lim
dλ
∞ −∞
0
f (u) cos λ(u − x) du.
(3.77)
The integral
∞
−∞
f (u) cos λ(u − x) du
(3.78)
is convergent for −∞ ≤ λ ≤ ∞, because  f (u) cos λ(u − x) ≤  f (u),
(3.79)
and f (u) is, as already stipulated, absolutely integrable on the entire axis. It follows from the previous lemmas that
∞
−∞
0
=
f (u) cos λ(u − x) du =
∞
−∞
∞
−∞
sin (u − x) du = f (u) u−x
du
f (u) cos λ(u − x) dλ
0
∞ −∞
sin(u) du, f (x + u) u
(3.80)
where an obvious substitution of variables has been made. But, from (3.77) we have 1 π
∞
dλ 0
∞
−∞
1 →∞ π
f (u) cos λ(u − x) du = lim
∞ −∞
f (x + u)
sin(u) du. u
(3.81)
If the function f (x) has lefthand and righthand derivatives at the point x, then the limit on the rhs exists and is equal to 12 [ f (x + 0) + f (x − 0)]. Thus, the integral on the lhs exists and is ∞ ∞ 1 1 (3.82) dλ f (u) cos λ(u − x) du = [ f (x + 0) + f (x − 0)], π 0 2 −∞ which proves the lemma.
3.5 Integral Theorems Let f (x) have a convergent integral over the interval [0, ∞] and satisfy the Dirichlet conditions described above. As f (x) is deﬁned for x ≥ 0, deﬁne f (x) in the interval [−∞, 0] as f (−x) = f (x), i.e., make f (x) an even function. Then we may construct the integral 1 π
∞
dα 0
∞
−∞
f (η) cos[α(η − x)] dη =
1 π
1 + π
∞
∞
f (η) cos[α(η − x)] dη
dα 0
0
∞
dα 0
0 −∞
(3.83) f (η) cos[α(η − x)] dη.
3.5. Integral Theorems
But,
47
0 −∞
f (η) cos[α(η − x)] dη =
∞
f (−η) cos[α(−η − x)] dη
0
=
(3.84)
∞
f (η) cos[α(η + x)] dη.
0
Consequently, 1 π
∞
dα 0
1 = π 2 = π
∞
−∞
f (η) cos[α(η − x)] dη
∞
∞
f (η) cos[α(η − x)] + cos[α(η + x)] dη
dα
0
0
∞
∞
cos(αx) dα 0
f (η) cos(αη) dη. 0
Therefore, with appeal to (3.76), if
2/π
Fc (α) =
∞
f (η) cos(αη) dη,
(3.85)
Fc (α) cos(αx) dα.
(3.86)
0
then
f (x) = 2/π
∞
0
On the other hand, if f (x) is deﬁned in the interval [−∞, 0] as f (−x) = − f (x), then ∞ Fs (α) = 2/π f (η) sin(αη) dη (3.87) 0
implies f (x) =
2/π
∞
Fc (α) sin(αx) dα.
(3.88)
0
Noting that
m
−m
m
cos[α(η − x)] dα = 2
cos[α(η − x)] dα,
0 m −m
(3.89)
sin[α(η − x)] dα = 0,
we have, as before, 1 f (x) = lim m→∞ π 1 m→∞ π
−∞
= lim or f (x) =
1 2π
∞
−∞
m
f (η) dη 0
∞
−∞
∞
f (η) dη
e−iαx dα
1 2
cos[α(η − x)] dα
m
−m ∞
−∞
eiα(η−x) dα,
f (η)eiαη dη.
(3.90)
48
3. Fourier Series and Fourier Integrals
Thus,
1 F(α) = √ 2π
∞
f (x)eiαx dx
(3.91)
F(α)e−iαx dα.
(3.92)
−∞
implies 1 f (x) = √ 2π
∞
−∞
3.6 Convolution Integrals The convolution of f (x) and g(x) is deﬁned as ∞ 1 g(η) f (x − η) dη. f g= √ 2π −∞ Since
∞
1 g(η) f (x − η) dη = √ 2π −∞
where 1 F(t) = √ 2π we have 1 √ 2π
−∞
g(η) dη
∞ −∞
∞
−∞
g(η) dη
∞
−∞
F(t)e−it(x−η) dt,
f (x)eit x dx,
(3.94)
∞ ∞ 1 F(t)e−it(x−η) dt = √ F(t)e−it x dt g(η)eitη dη 2π −∞ −∞ −∞ ∞ F(t)G(t)e−it x dt, =
∞
(3.93)
∞
−∞
with 1 G(t) = √ 2π
∞
−∞
g(x)eit x dx.
(3.95)
Therefore,
∞ −∞
F(t)G(t)e
−it x
dt =
∞
−∞
g(η) f (x − η) dη.
In a special case where x = 0, (3.96) becomes ∞ ∞ F(t)G(t) dt = g(η) f (−η) dη. −∞
−∞
(3.96)
(3.97)
If we replace F(t) with Fc (t), i.e., if f (x) is an even function, f (−x) = f (x), and if the same is done for g(x), the above becomes ∞ ∞ Fc (t)Gc (t) dt = f (η)g(η) dη. (3.98) 0
0
3.7. Transforms of Derivatives
49
3.6.1 Evaluation of Integrals by Use of Convolution Theorems The above results may be used to evaluate integrals. For example, let f (x) = e−bx , and let us evaluate two integrals, viz., I1 =
∞
(3.99)
e−bx cos(αx) dx,
0
I2 =
(3.100)
∞
e
−bx
sin(αx) dx.
0
We ﬁnd ∞ 1 α ∞ −bx 1 α I1 = − e−bx cos(αx) − e sin(αx) dx = − I2 , b b 0 b b 0 ∞ ∞ 1 α α I2 = − e−bx sin(αx) + e−bx cos(αx) dx = I1 . b b 0 b 0
(3.101)
When the above are solved, we obtain b b ⇒ F (α) = 2/π 2 , c α 2 + b2 α + b2 α α I2 = 2 ⇒ Fs (α) = 2/π 2 . 2 α +b α + b2 I1 =
(3.102)
But, from the deﬁnition of the Fourier cosine transform, ∞ b 2 ∞ f (x) = 2/π Fc (α) cos(αx) dα = cos(αx) dα 2 π 0 α + b2 0 2b ∞ cos(αx) = dα = e−bx . π 0 α 2 + b2 Imagine the same development for a companion function, g(x) = e−ax and substitute both results into (3.99). First, it is found that Fc (α) =
2/π
b α 2 + b2
and
Gc (α) =
2/π
a , α2 + a2
and then, after the substitution, ∞ 2ab ∞ dα 1 = . e−(a+b)x dx = π 0 (α 2 + b2 )(α 2 + a 2 ) a + b 0
(3.103)
(3.104)
3.7 Fourier Transforms of Derivatives of f (x) To obtain formulae for the transformations of derivatives of functions, ﬁrst deﬁne ∞ r d f (x) iαx 1 (r ) e dx (3.105) F (α) = √ 2π −∞ dxr
50
3. Fourier Series and Fourier Integrals
and then integrate by parts to obtain ∞ ∞ r −1 d f 1 dr −1 f iαx 1 (r ) F (α) = √ e −√ (iα)eiαx dx r −1 dx 2π 2π −∞ dxr −1 −∞ dr −1 f → 0 as x → ±∞. = −(iα)F (r −1) (α) , if dxr −1 In general, by repetitive application of this procedure, it is found that F (r ) (α) = (−iα)r F(α).
(3.106)
(3.107)
3.8 Fourier Integrals as Limiting Cases of Fourier Series It is useful to explore the existence of the above Fourier integrals as limiting cases of the Fourier series considered at in previous sections. Although the following is not as rigorous as the proof of the Fourier theorem given earlier, the discussion of the Fourier integral as a limiting case of a Fourier series is valuable as a connection between the two. As before, let f (x) be deﬁned for all real x, and let it be piecewise smooth (with a possible ﬁnite number of discontinuities) on every ﬁnite interval − ≤ x ≤ . Then f (x) can be expanded as a Fourier series ∞ nπ x nπ x a0 + + bn sin , (3.108) an cos f (x) = 2 n=1 where an =
1
1 bn =
− −
f (u) cos
nπ x du, n = 0, 1, 2, . . . ,
(3.109)
nπ x du, n = 1, 2, 3, . . . . f (u) sin
We note that at points where f (x) is discontinuous we must interpret the value as 12 [ f (x + 0) + f (x − 0)]. Now, substitute (3.109) into the above to obtain ∞ 1 nπ 1 (u − x) du. (3.110) f (u) du + f (u) cos f (x) = 2 − − n=1 Suppose that f (x) is absolutely integrable on the entire x axis, that is suppose that the integral ∞  f (x) dx (3.111) −∞
exists. Then, as → ∞, (3.110) becomes ∞ 1 nπ (u − x) du. f (x) = lim f (u) cos →∞ − n=1
(3.112)
Setting π 2π 3π , λ2 = , λ2 = , ..., π λn = λn+1 − λn = ,
λ1 =
(3.113)
3.9. Dirac Delta Function
51
and using this in the above, the sum takes the form ∞ 1 λn f (u) cos λn (u − x) du. π n=1 −
(3.114)
But for ﬁxed x this looks like the sum that would deﬁne the integral of the function ∞ 1 f (u) cos λ(u − x) du, (3.115) ζ (λ) = π −∞ and, therefore, it is natural to conclude that, as → ∞, ∞ ∞ 1 f (x) = dλ f (u) cos λ(u − x) du. π 0 −∞
(3.116)
3.9 Dirac Delta Function Consider the function 1 sin(υs) . π s
(3.117)
υ (s) ds = 1,
(3.118)
υ (s) ≡ It can be veriﬁed that
∞ −∞
and
∞
lim
υ→0 −∞
υ (s) f (s) ds = f (0).
(3.119)
To prove the latter, expand f (s) about the point s = 0, i.e., f (s) = f (0) + (∂ f/∂s)0 s + 1/2!(∂ 2 f/∂s 2 )0 s 2 + . . . .
(3.120)
Then, lim
∞
υ→0 −∞
υ (s) f (s) ds = lim
∞
υ→0 −∞
+ lim
sin υs 1 f (0) ds + lim υ→0 π s ∞
υ→0 −∞
∞
−∞
1 (∂ f/∂s)0 sin υs ds π
1 2 (∂ f/∂s 2 )0 s sin υs ds 2π
= f (0). We also explore the function, η(s − a), where η(s) is shown in Fig. 3.3. Clearly, ∞ 1 1 (3.121) η(s) ds = 2 = 1. 2 −∞ Then, by expanding f (s) about the point s = a, we deduce that ∞ a+1/2 1 lim η(s) f (s) ds = lim f (a) ds. →0 −∞ →0 a−1/2
(3.122)
52
3. Fourier Series and Fourier Integrals
η( s ) 1/ε
f(s) Figure 3.3. A step function as a generalized function.
a − 1/2ε
s
a a + 1/2ε
The f (a) here is, of course, just the ﬁrst term of a Taylor expansion of f (s) about the point s = a. The remaining terms in the Taylor expansion produce null results; for example, the next term in the expansion yields a a−1/2 1 1 (3.123) (s − a) ds + lim (s − a) ds = 0, lim →0 a−1/2 →0 a and so on. Thus,
∞
η(s) f (s) ds = f (a).
(3.124)
lim η(s − a) = ∞, at s = a,
(3.125)
lim
→0 −∞
We note that →0
and
lim
∞
→0 −∞
η(s) ds = 1.
(3.126)
Consequently, we deﬁne lim η(s − a) ≡ δ(s − a),
(3.127)
lim υ (s) ≡ δ(s).
(3.128)
→0
and υ→0
The so deﬁned Dirac delta function δ(s) is such that ∞ ∞, δ(s) ds = 1, δ(s) = 0, −∞ and
∞
−∞
if s = 0 , if s = 0 ,
f (s)δ(s − a) ds = f (a) .
(3.129)
(3.130)
3.10 Suggested Reading Brown, J. W., and Churchill, R. V. (2001), Fourier Series and Boundary Value Problems, 6th ed., McGrawHill, Boston. Goldberg, R. R. (1961), Fourier Transforms, Cambridge University Press, Cambridge, UK. Little, R. W. (1973), Elasticity, Prentice Hall, Englewood Cliffs, New Jersey.
3.10. Suggested Reading
53
Papoulis, A. (1962), The Fourier Integral and Its Application, McGrawHill, New York. Pinkus, A., and Samy, Z. (1997), Fourier Series and Integral Transforms, Cambridge University Press, New York. Sneddon, I. N. (1951), Fourier Transforms, McGrawHill, New York. Sneddon, I. N. (1961), Fourier Series, Routledge and Paul, London. Sneddon, I. N. (1972), The Use of Integral Transforms, McGrawHill, New York. Wolf, K. B. (1979), Integral Transforms in Science and Engineering, Plenum, New York.
PART 2: CONTINUUM MECHANICS
4 Kinematics of Continuum
4.1 Preliminaries Let φ(x) be a scalar ﬁeld which is a function of x1 , x2 , x3 (Fig. 4.1), i.e., φ = φ(x1 , x2 , x2 ) . The function φ is continuous if lim φ(x + αa) − φ(x) = 0, α→0
(4.1)
∀ x ∈ D, a ∈ E.
The ﬁeld φ is differentiable within D if there is a vector ﬁeld, w, such that lim w · a − α −1 [φ(x + αa) − φ(x)] = 0, ∀ x ∈ D, a ∈ E. α→0
(4.2)
(4.3)
The vector ﬁeld w is unique and is the gradient of φ, w = grad φ. If u is a vector ﬁeld, u(x), then its gradient is deﬁned by [grad u(x)]T · a = grad[u(x) · a],
∀ x ∈ D, a ∈ E.
(4.4)
The divergence of u(x), div u, or ∇ · u, is deﬁned by ∇ · u = tr [grad u(x)].
(4.5)
The curl is deﬁned by [curl u(x)] · a = ∇ · [u(x) × a],
∀ x ∈ D, a ∈ E.
(4.6)
The tensor ﬁeld, T(x), if differentiable, has its divergence deﬁned as div T(x) · a = ∇ · T(x) · a = div [T(x) · a].
(4.7)
It is readily shown that if φ, u, and T are scalar, vector, and tensor ﬁelds, respectively, then with reference to rectangular Cartesian unit base vectors {e1 , e2 , e3 }, we can write φ = φ(x), u(x) = u p (x)e p ,
(4.8)
T(x) = Tpq (x)e p eq . 55
56
4. Kinematics of Continuum
φ(x )
x2
e2 Figure 4.1. A scalar ﬁeld, φ(x).
e3
x1
e 1
x3
It is also readily shown from the discussion and deﬁnitions given above that, inter alia, grad φ(x) = ∇φ = ∂φ(x)/∂ x p e p , grad u(x) = ∇u(x) = ∂u p /∂ xq e p eq , div u(x) = ∇ · u(x) = ∂u p /∂ x p ,
(4.9)
curl u(x) = pqr ∂ur /∂ xq e p , div T(x) = ∇ · T(x) = ∂ Tpq /∂ x p eq .
4.2 Uniaxial Strain A uniaxial measure of strain should, at the minimum, quantitatively describe changes in length as depicted in Fig. 4.2. There are, however, an inﬁnite number of ways to do this. For example, nominal strain:
e = /0 = ( − 0 )/0 = /0 − 1.
(4.10)
The stretch associated with this change in length is λ ≡ /0 → e = λ − 1.
(4.11)
Other deﬁnitions of uniaxial strain follow, and as examples we deﬁne
natural strain:
η=
− 0 = 1 − 1/λ ,
(4.12)
Lagrangian strain:
E=
1 2 − 20 1 = (λ2 − 1) , 2 20 2
(4.13)
Eulerian strain:
E=
1 2 − 20 1 = (1 − 1/λ2 ) . 2 2 2
(4.14)
l Figure 4.2. Uniaxial stretch.
l0
∆l
4.3. Deformation Gradient
57
F dx
Figure 4.3. Kinematics of deformation, describing the motion of material particles from the “reference state” to the “deformed state.”
dX u(X)
X
x
"reference" or "deformed" or "undeformed" state "current" state
Still another measure is deﬁned by d = 0
0
d = = ln = ln λ. 0
(4.15)
Accordingly, this measure of strain is referred to as the logarithmic strain or true strain.
4.3 Deformation Gradient To provide a precise description of changes in the shape, size, and orientation of a solid body, we introduce various tensors that describe deformation of a body. The displacement ﬁeld u(x) describes the change in position, relative to a convenient coordinate system, of all points in the body. We shall assume this ﬁeld to be single valued and continuous for the present. The property of being single valued implies that there are no holes, gaps, or interpenetrations of matter in the body. The displacement ﬁeld is nonuniform if the body is deformed and is uniform only if the body has undergone rigid translations. To describe the picture above we need to describe how each “material point” is displaced, i.e., we want to associate a displacement, u, with each material point (Fig. 4.3). We identify material points by their positions in the reference state, X. Thus, X
is position in the reference state ,
x
is position in the current (deformed) state, and
x
is function of X, x = x(X) .
The gradient of x(X) is deﬁned as F = ∂x/∂X.
(4.16)
If {e1 , e2 , e3 } is a set of convenient base vectors in the current conﬁguration and {E1 , E2 , E3 } are base vectors in the reference conﬁguration, then an explicit, and most natural, representation of F is F = ∂ xi (X)/∂ Xj ei E j .
(4.17)
This is a socalled twopoint tensor, which relates dx and dX, such that dx = F · dX.
(4.18)
58
4. Kinematics of Continuum
s x2 Figure 4.4. Case of 2D simple shear.
h x1
Since F is invertible, dX = F−1 · dx.
(4.19)
In terms of displacement gradients we may express the above as follows. Since x = X + u,
(4.20)
∂u/∂X = ∂x/∂X − I = F − I,
(4.21)
∂u/∂x = I − ∂X/∂x = I − F−1 .
(4.22)
the displacement gradient is
or, in the current state,
For example, consider a simple shear deformation. Deﬁne a shear strain as γ = s/ h, as depicted in Fig. 4.4. Then, the deformation mapping is x1 = X1 + γ X2 ,
x2 = X2 .
The inplane deformation gradient has the components 1γ F= , 01 whereas the displacement gradient is
∂u 0γ = . 00 ∂X
(4.23)
(4.24)
(4.25)
4.4 Strain Tensor Let R0 and R be regions within the body in the reference (undeformed) conﬁguration and current (deformed) conﬁguration, respectively. Further, let N be a unit vector embedded within the body in the reference conﬁguration; the deformation transforms N to n in the deformed state (Fig. 4.5). The square of the stretch of N, λ(N), can be calculated as λ2 (N) = (F · N) · (F · N) = N · FT · F · N.
(4.26)
Deﬁne C ≡ FT · F as the right Cauchy–Green deformation tensor. Then the stretch, squared, is also given by λ2 (N) = N · C · N.
(4.27)
By using the polar decomposition theorem (1.145), we obtain F = R · U,
C = FT · F = U2 ,
λ2 (N) = N · U2 · N.
(4.28)
4.4. Strain Tensor
59
F n Figure 4.5. Stretch of an arbitrary ﬁber N in the reference state to n in the current, deformed state.
N
R
o R "reference" or "deformed" or "undeformed" state "current" state The tensor U is called the right stretch tensor. If we now deﬁne the strain in the direction N as
1 2 λ (N) − 1 = N · E · N, (4.29) E(N) = 2 we deduce the strain tensor 1 (4.30) E = (C − I), 2 which is known as the Green strain (or Lagrangian strain) tensor. An alternative approach to deﬁne this strain tensor is as follows. Let dS = length of dX , ds = length of dx. Then, dS2 = dX · dX = dX · I · dX , ds 2 = dx · dx = (F · dX) · (F · dX) = dX · FT · F · dX . Combining the last two results, we have ds 2 − dS2 = dX · (FT · F − I) · dX.
(4.31)
This leads to the deﬁnition of Green strain as 1 1 E = (FT · F − I) = (C − I), 2 2 because then ds 2 − dS2 = 2dX · E · dX. The Green strain is symmetric as may be seen via the manipulations 1 T (F Fs j − δi j ) , 2 is 1 E ji = (F jsT Fsi − δ ji ) 2 1 1 = (Fs j FisT − δi j ) = (FisT Fs j − δi j ) . 2 2 Ei j =
This is also obvious from (4.4), because FT · F and I are symmetric.
(4.32)
60
4. Kinematics of Continuum
α
Figure 4.6. Angle change during shearing deformation.
α/2
α/2
4.5 Stretch and Normal Strains Consider an inﬁnitesimal vector, dX, which is deformed by F into the vector element, dx. The magnitudes of the lengths of these vectors are, respectively, dS and ds. Then, ds 2 = dx · dx = dX · FT · F · dX = dX · C · dX.
(4.33)
ˆ = dX/dS, we can write By deﬁning the unit vector, N ˆ ·C·N ˆ = λ2 (N). ˆ ds 2 /dS2 = N
(4.34)
ˆ is the stretch of a ﬁber, initially of unit length, which was lying in the direction Thus, λ(N) ˆ N in the reference state. ˆ = e1 . Then, For example, consider a uniaxial stretching, and take N λ2 (e1 ) = C11 = 2E11 + 1 .
(4.35)
ds(e1 ) − dS(e1 ) = λ(e1 ) − 1 = 2E11 + 1 − 1. dS
(4.36)
ds − dS ≈ E11 , dS
(4.37)
Also,
If E11 1, we have
which is just the deﬁnition of a small uniaxial engineering (or nominal) strain measure. Clearly, by expanding (1 + 2E11 )1/2 , we obtain e11 =
ds − dS 1 2 ∼ E11 − E11 + ... . dS 2
(4.38)
4.6 Angle Change and Shear Strains We begin by examining Fig. 4.6. Note that a convenient measure of the obvious distortion would be the change in the 90◦ angle made between the horizontal and vertical sides of the square section. This angular change is α as shown. Thus one measure of the distortion is simply cos(π/2 − α), which is zero if α = 0 and is nonzero if α = 0, in which case cos(π/2 − α) = sin α = 0. We also note that the distortions in both ﬁgures are the same, and the displacements differ only by a rigid body rotation. Thus, cos(π/2 − α) is an acceptable measure of strain. Now let us consider two inﬁnitesimal vector elements, dX1
4.7. Inﬁnitesimal Strains
61
F >
n1 n2
X
>
N1
Figure 4.7. Angle change between two ﬁbers.
x
N2
"reference" or "deformed" or "undeformed" state "current" state
and dX2 , in the reference state; in the current state they become, respectively, dx1 and dx2 (Fig. 4.7). Unit vectors associated with these two can be deﬁned as ˆ 1 = dX1 /dX1 , N
nˆ 1 = dx1 /dx1 ,
(4.39)
ˆ 2 = dX2 /dX2 , N
nˆ 2 = dx2 /dx2 .
(4.40)
We can now form the cosine of the angle between them as cos(nˆ 1 , nˆ 2 ) = nˆ 1 · nˆ 2 =
dx1 · dx2 . dx1 dx2 
(4.41)
In view of the connections dx1 = F · dX1 ,
dx2 = F · dX2 ,
dx1 = dX1 · F ,
dx2 = dX2 · FT ,
T
the angle change can be expressed as cos(nˆ 1 , nˆ 2 ) =
dX1 · FT · F · dX2 . (dX1 · C · dX1 )1/2 (dX2 · C · dX2 )1/2
(4.42)
ˆ 1 dX1  and dX2 = N ˆ 2 dX2 , so that But, dX1 = N cos(nˆ 1 , nˆ 2 ) =
ˆ2 ˆ1·C·N N . ˆ 1 )λ(N ˆ 2) λ(N
(4.43)
ˆ 2 = e2 . Then, ˆ 1 = e1 and N As an example, let N cos(nˆ 1 , nˆ 2 ) =
C12 C12 =√ √ λ(e1 )λ(e2 ) C11 C22
2E12 . =√ √ 2E11 + 1 2E22 + 1
(4.44)
If all strains are small, Ei j  1, we have cos(nˆ 1 , nˆ 2 ) ≈ 2E12 .
(4.45)
4.7 Inﬁnitesimal Strains In general, the connection between positions in the reference and deformed states can be written as x(X) = X + u(X).
(4.46)
62
4. Kinematics of Continuum
Consider a particular component of strain, say E11 =
1 T F1s Fs1 − 1 . 2
(4.47)
Since Fi j = δi j + ∂ui /∂ Xj ,
FiTj = δi j + ∂u j /∂ Xi ,
(4.48)
we have E11 =
1 [(δ1s + ∂us /∂ X1 )(δs1 + ∂us /∂ X1 ) − 1] , 2
i.e., E11 =
1 [(∂u1 /∂ X1 + ∂u1 /∂ X1 ) + (∂us /∂ X1 )(∂us /∂ X1 )] . 2
(4.49)
In general, we obtain that Ei j =
1 [(∂ui /∂ Xj + ∂u j /∂ Xi ) + (∂us /∂ Xi )(∂us /∂ Xj )] . 2
(4.50)
If ∂u/∂X 1, the Ei j reduce to the inﬁnitesimal strain components, Ei j ≈ ei j =
1 (∂ui /∂ Xj + ∂u j /∂ Xi ). 2
(4.51)
4.8 Principal Stretches Consider the stretch of a ﬁber along the direction of the unit vector n. We have λ2 (n) = n · C · n.
(4.52)
We seek those n for which the stretch is extreme (principal stretch). To ﬁnd the extremum introduce a Lagrange multiplier, µ, via L = n · C · n − µ(n · n − 1).
(4.53)
Then, ∂L(n, µ)/∂n = 2(C · n − µn) = 0, which leads to C · n − µn = 0,
(4.54)
where the µ’s are the eigenvalues of C. By using the results from Chapter 1, we have µ3 − IC µ2 + I IC µ − I I IC = 0,
(4.55)
where the invariants of C are IC = tr (C), I IC = [e1 , C · e2 , C · e3 ] + [C · e1 , e2 , C · e3 ] + [C · e1 , C · e2 , e3 ], I I IC = [C · e1 , C · e2 , C · e3 ].
(4.56)
4.10. Volume Changes
63
4.9 Eigenvectors and Eigenvalues of Deformation Tensors The deformation gradient may be decomposed via the polar decomposition theorem as F = R · U, with C = UT · U = U2 . Thus, if C=
3
µ pn pn p,
(4.57)
µ1/2 p n pn p,
(4.58)
i=1
then U=
3 i=1
where the eigenvalues, µ p , are associated with eigenvectors, n p , via C · n p = µ pn p.
(4.59)
Consider the stretch of an eigenvector, λ(n p ). Its square is λ2 (n p ) = n p · C · n p = µ p .
(4.60)
If p = s, then n p · ns = 0. Indeed, C · n p = µ pn p,
(4.61)
ns · C · n p − n p · C · ns = 0.
(4.62)
and thus, since C is symmetric,
Also, ns · µ p n p − n p µs ns = 0, i.e., (µ p − µs )ns · n p = 0.
(4.63)
Thus, if µ p = µs , then n p · ns = 0. Now consider cos(F · n j , F · nk). We have
√ µk n j · C · nk n j · (µknk) = √ √ = √ n j · nk = 0. √ √ µ j µk µ j µk µj
(4.64)
Therefore, the eigenvectors of C undergo pure stretch, i.e., they are not rotated by the deformation.
4.10 Volume Changes Consider the volume element, δV as it is transformed into δv through F (Fig. 4.8). Clearly, δV = dX1 dX2 dX3 , and δv = dx1 dx2 dx3 .
(4.65)
δv = [F · dX1 , F · dX2 , F · dX3 ].
(4.66)
Also,
64
4. Kinematics of Continuum x2
F dX3
e2
dX2
e1
Figure 4.8. Changes in volume of a typical volume element.
x1 e3 x3
dX
1
Now, if dXi = ei , then δV = 1, and δv = (δv/δV) = I I IF = det F = F.
(4.67)
4.11 Area Changes The area element, bounded by the inﬁnitesimals dX and dY shown in Fig. 4.9, can clearly be ˆ ˆ is the unit normal to the described as NdS = dX × dY; dS is the magnitude of the area and N surface “patch.” The componental representation for the vectorial area of the undeformed surface patch is Nˆ i dS = i jkdXj dYk.
(4.68)
Likewise, for the deformed surface patch, nˆ i ds = i jkdx j dyk,
(4.69)
where ds is the area of the deformed surface patch and nˆ is its unit normal. Since dx = F · dX, we have nˆ i ds = i jk F js dXs Fkp dYp .
(4.70)
Now multiply both sides of (4.70) by Fit and perform the indicated summations to obtain nˆ i Fit ds = i jk F js Fkp Fit dXs dXp .
(4.71)
Note that within the rhs we ﬁnd the term tsp (det F) ∼ i jk F js Fkp Fit . This allows us to write nˆ i Fit ds = tsp (det F)dXs dYp = Nˆ t (det F)dS.
(4.72)
Taking a product with Ftr−1 gives nˆ i Fit Ftr−1 ds = Nˆ t Ftr−1 (det F)dS, i.e., (4.73)
>
nˆ r ds = (det F) Nˆ t Ftr−1 dS,
>
n
N
ds
dS dy dY F dX
dx
Figure 4.9. Area change of a surface patch (element) during a general deformation.
4.12. Area Changes: Alternative Approach
65
and thus ˆ · F−1 dS = (det F)F−T · NdS. ˆ ˆ = (det F)N nds
(4.74)
This is known as Nanson’s relation between the undeformed and deformed vectorial areas. By multiplying (4.74) with itself, and then taking a square root of the result, we obtain ˆ · C−1 · N) ˆ 1/2 dS , ds = (det F)(N
(4.75)
where C = FT · F is the right Cauchy–Green deformation tensor. Substituting this back ˆ into (4.74), we obtain an expression for the unit normal nˆ in terms of the unit normal N, i.e., nˆ =
ˆ F−T · N . −1 ˆ · C · N) ˆ 1/2 (N
(4.76)
Alternatively, if (4.74) is rewritten as ˆ NdS =
1 1 FT · nˆ ds = nˆ · F ds , det F det F
(4.77)
the multiplication with itself gives dS =
1 ˆ 1/2 ds , (nˆ · B · n) det F
(4.78)
where B = F · FT is the left Cauchy–Green deformation tensor. When (4.78) is substituted ˆ in terms of the unit normal back into (4.77), we obtain an expression for the unit normal N ˆ i.e., n, ˆ = N
FT · nˆ . ˆ 1/2 (nˆ · B · n)
(4.79)
Two identities can be observed from the above results, one for the ratio of the deformed and undeformed surface areas and another for the cosine of the angle between their unit normals. These are ds ˆ · C−1 · N) ˆ 1/2 , ˆ −1/2 = (det F)(N = (det F)(nˆ · B · n) dS ˆ = nˆ · N
ˆ · F−T · N ˆ N nˆ · FT · nˆ = . 1/2 ˆ · C−1 · N) ˆ 1/2 ˆ (nˆ · B · n) (N
(4.80)
(4.81)
4.12 Area Changes: Alternative Approach A secondorder tensor F has a dual tensor F∗ , such that F∗ · (a × b) = (F · a) × (F · b),
(4.82)
where a and b are arbitrary vectors. To see this and identify F∗ , let c be still a third arbitrary vector. Then, by using the result from Problem 1.7, we obtain [F∗ · (a × b)] · c = [(F · a) × (F · b)] · (F · F−1 · c) = (det F)(a × b) · F−1 · c.
66
4. Kinematics of Continuum x2
F dX3
e2
2 4
e1 e3 x3
dX2
4 3 x 1
r
Figure 4.10. Block with circular hole subject to a deformation involving a simple shear.
1 dX
1 1
Recalling that F−1 · c = c · F−T , and by invoking cyclic property of triple product and commutative property of scalar product, the above becomes c · F∗ · (a × b) = (det F)c · F−T · (a × b).
(4.83)
Since this holds for arbitrary trio of vectors a, b, c, we obtain F∗ = (det F)F−T .
(4.84)
Applying this result to the computation of area, we ﬁnd ˆ dx × dy = (F · dX) × (F · dY) = F∗ · (dX × dY) = (det F)F−T · NdS.
4.13 Simple Shear of a Thick Plate with a Central Hole A threedimensional state of simple shear, as depicted in Fig. 4.10, is prescribed by x1 = X1 + γ X2 , x2 = X2 ,
(4.85)
x3 = X3 . The corresponding deformation gradient and its inverse are ⎡
⎤ 1γ 0 F = ⎣0 1 0⎦ , 001
⎡
F−1
⎤ 1 −γ 0 = ⎣0 1 0⎦ . 0 0 1
(4.86)
Furthermore, ⎤ 1 00 = ⎣−γ 1 0⎦ , 0 01 ⎡
(F−1 )T = F−T
(4.87)
and ˆ ˆ = (det F)F−T · NdS. nds
(4.88)
ˆ = e1 , dS = dX3 dX2 , and det F = 1. Thus, On side 1 we have N ˆ = F−T · e1 dX3 dX2 . nds
(4.89)
4.13. Simple Shear of a Hollow Plate
67
This means that ˆ · nds ˆ dA21 = nds = F−T · e1 (dX3 dX2 )2 · (F−T · e1 ) = e1 · F−1 · F−T · e1 (dX3 dX2 )2 −T = F1s−1 Fs1 (dX3 dX2 )2
= (1 + γ 2 )(dX3 dX2 )2 , that is,
Thus, on all of side 1,
dA1 =
1 + γ 2 dX3 dX2 .
1
dA = side 1
Similarly, for side 3,
0
4
1 + γ 2 dX2 dX3 = 4 1 + γ 2 .
(4.90)
(4.91)
0
dA = 4 1 + γ 2 .
(4.92)
side3
ˆ = e2 , dS = dX1 dX3 . Thus, On side 2, we have N ˆ = F−T · e2 dX1 dX3 , nds
(4.93)
and ˆ · nds ˆ dA22 = nds = e2 · F−1 · F−T · e2 (dX1 dX3 )2 −1 T = F2s−1 (Fs2 ) (dX1 dX3 )2
= 1(dX1 dX3 )2 = no change! For side 4 we have the same result as for side 2. Now consider the circular hole. Its radius in the reference state is r . With the origin at the hole’s center, and using a polar coordinate system aligned with the x1 − x2 axes, we have that ˆ NdS = (cos θe1 + sin θe2 )r dθdX3 ,
(4.94)
and (Fig. 4.11) ˆ ˆ = (det F)F−T · NdS nds = (F1s−1 ) Nˆ s r dθ dX3 e1 + (F2s−1 )T Nˆ s r dθdX3 e2 = [cos θe1 + (sin θ − γ cos θ)e2 ]r dθ dX3 . Consequently, dA2 = nˆ · ds · nˆ · ds = [cos θe1 + (sin θ − γ cos θ)e2 ] · [cos θe1 + (sin θ − γ cos θ)e2 ]r 2 dθ 2 dX32 ,
68
4. Kinematics of Continuum
n
Figure 4.11. Normal to the hole’s surface. See Fig. 4.10 for a complete perspective of the geometry.
or dA2 = [cos2 θ + (sin θ − γ cos θ)2 ]r 2 dθ 2 dX32 = (cos2 θ + sin2 θ − 2γ sin θ cos θ + γ 2 cos2 θ)r 2 dθ 2 dX32 = (1 − γ sin 2θ + γ 2 cos2 θ)r 2 dθ 2 dX32 . Finally, dA =
1 − γ sin 2θ + γ 2 cos2 θ r dθ dX3 ,
(4.95)
which, when integrated, yields A= r 0
1
2π
1 − γ sin 2θ + γ 2 cos2 θ dθ dX3 .
(4.96)
0
4.14 Finite vs. Small Deformations It is worthwhile to explore the differences between ﬁnite and small deformations for the purpose of understanding how even seemingly qualitative effects can arise in the transition from inﬁnitesimal to ﬁnite deformation. We do this here via a simple example. Consider the deformation x1 = X1 − γ X2 + β X3 , x2 = γ X1 + X2 − α X3 ,
(4.97)
x3 = −β X1 + α X2 + X3 . What we show is that this deformation involves only a rigid body rotation if the α, β, γ are “small,” but a general deformation if they are “ﬁnite.” Indeed, the deformation gradient is ⎡
1 F=⎣ γ −β
−γ 1 α
⎤ β −α ⎦ , 1
(4.98)
whereas the corresponding Green strain is ⎡ 2 β + γ2 1 ⎣ E= −αβ 2 −αγ
−αβ α2 + γ 2 −βγ
⎤ −αγ −βγ ⎦ . α2 + β 2
(4.99)
4.15. Reference vs. Current Conﬁguration
69
F
u(X) Figure 4.12. Reference and current coordinate systems.
"reference" or "deformed" or "undeformed" state "current" state
x2 e2
X2 E2 X1
E3 X
E1 3
e x
3
e1 x 1
3
Clearly, the strains vanish to O(ξ ζ ) where ξ, ζ = α, β, γ . If, however, these quadratic terms are not negligible, the state is one that involves deformation. In any event, the rotations do not vanish. The rotation vector, w, can be calculated as 1 wi = − i jk Wjk, 2 which yields w1 = α, w2 = β, w3 = γ .
(4.100)
4.15 Reference vs. Current Conﬁguration We again begin by deﬁning the deformation commencing from the reference to the current states as shown in Fig. 4.12. We introduce two coordinate frames each belonging to one state or the other. In particular, the frame {E1 , E2 , E3 } is deﬁned in the reference state, and {e1 , e2 , e3 } is deﬁned in the current, i.e., deformed state. For clarity we will use Greek subscripts to denote components referred to the reference state and Latin subscripts for the current state. Thus a vector such as u is expressed as either u = uπ Eπ ,
or
u = us es .
(4.101)
or
us = u · es .
(4.102)
Their components are formed as uπ = u · Eπ ,
Higher order tensors can be handled similarly. For example, σ = σαβ Eα Eβ = σsr es er ,
(4.103)
where σαβ = Eα · σ · Eβ
σsr = es · σ · er .
(4.104)
Mixed representations are also possible, e.g., σ = σαi Eα ei = σsβ es Eβ ,
(4.105)
70
4. Kinematics of Continuum
where σαi = Eα · σ · ei ,
(4.106)
σsβ = es · σ · Eβ .
(4.107)
Some components are most naturally represented as mixed components, including those of the deformation gradient. Recall x = x(X, t),
(4.108)
where the possibility that the deformation mapping depends on time, t, has been explicitly included. Then the gradient is F = ∂x/∂X = Fiα ei Eα ,
(4.109)
because x “lives” in the current conﬁguration, and X in the reference state. We note that F is invertible and so F−1 exists – this is physically demandable from the various pictures of the deformation presented to date, and from the statements that the displacements involved are single valued. Thus each material point is, at this juncture, taken to originate from a unique point in the reference conﬁguration and is displaced to a unique point in the current conﬁguration. Thus, the process is “conceptually invertible,” and F−1 exists. Therefore, we can write F−1 = ∂(x, t)/∂x = ∂X/∂x.
X = (x, t),
(4.110)
For a component representation, we have −1 Eα er , F−1 = Fαr
−1 Fαr = ∂ Xα /∂ xr .
(4.111)
LEMMA 4.1: If φ is a scalar ﬁeld, then
Grad φ = ∂φ/∂X = FT · grad φ,
(4.112)
where grad φ = ∂φ/x. Proof: First we write Grad φ = ∂φ/∂X = ∂φ/∂ Xα Eα . Then, ∂φ/∂X = ∂φ/∂x · ∂x/∂X = (∂φ/∂ xi ei ) · (∂ x p /∂ Xα e p Eα ) = (∂ x p /∂ Xα Eα e p ) · (∂φ/∂ xi ei ) = FT · grad φ. COROLLARY 4.1: Similarly to Lemma 4.1 above, we ﬁnd that for a vector ﬁeld u,
Grad u = (grad u) · F ,
(4.113)
i.e.,
u∇0 = (u∇) · F,
∂ui ∂ui ∂ xk = . ∂ Xj ∂ xk ∂ Xj
(4.114)
For clarity, the arrow above the nabla operator is attached to indicate the direction in which the operator applies.
4.17. Velocity Gradient
71
4.16 Material Derivatives and Velocity Let t be a time like variable that increases monotonically with the deformation process. It is assumed that F evolves with t. Likewise all scalar or tensor ﬁelds may evolve with time. For a scalar ﬁeld then φ = scalar ﬁeld = φ(X, t).
(4.115)
We may deﬁne the “material derivative” of φ as ˙ φ(X, t) = ∂φ(X, t)/∂t,
(4.116)
that is, a derivative taken at constant reference position, X. Stated otherwise, this is a rate of change at a ﬁxed material point. Clearly X does not depend on time. But the current position of a material point, x, does depend on time, so that in the current conﬁguration where we have the representation, φ(x, t), the time rate of φ is ˙ φ(x, t) = ∂φ(x, t)/∂t + (∂φ/∂x) · (∂x/∂t).
(4.117)
Deﬁning the velocity as υ(x, t) = ∂x/∂t,
(4.118)
the rate of change of the scalar ﬁeld is ˙ φ(x, t) = ∂φ(x, t)/∂t + ∇φ · υ.
(4.119)
˙ φ(x, t) = ∂φ(x, t)/∂t + (grad φ) · υ.
(4.120)
But, ∇φ = grad φ, and so
4.17 Velocity Gradient The velocity gradient is deﬁned as L = grad υ = grad x˙ ,
(4.121)
i.e.,
L = υ∇ ,
Li j =
∂vi . ∂xj
(4.122)
By using (4.113), we obtain ˙ · F, Grad x˙ = (grad x)
(4.123)
˙ · F−1 . grad x˙ = grad υ = L = (Grad x)
(4.124)
Grad x˙ = F˙
(4.125)
L = grad υ = grad x˙ = F˙ · F−1 .
(4.126)
or
But,
and so
72
4. Kinematics of Continuum
Note that F · F−1 = I. Taking the time derivative of this identity, we obtain . F˙ · F−1 + F · (F−1 ) = 0
⇒
. (F−1 ) = −F−1 · F˙ · F−1 .
(4.127)
Thus, . L = F˙ · F−1 = −F · (F−1 ) .
(4.128)
LEMMA 4.2: If F is invertible and depends on a time like parameter, t, then
d d (detF) ≡ J = (detF) tr(F˙ · F−1 ). dt dt
(4.129)
Proof: Begin by writing det F = [F · a, F · b, F · c],
(4.130)
where {a, b, c} is a set of any convenient orthonormal unit vectors. Then, d dF dF dF (det F) = · a, F · b, F · c + F · a, · b, F · c + F · a, F · b, ·c . dt dt dt dt Since L=
dF −1 ·F , dt
(4.131)
we have d (det F) = [L · F · a, F · b, F · c] + [F · a, L · F · b, F · c] + [F · a, F · b, L · F · c]. dt Clearly, then, d (det F) = (tr L)(det F). dt
(4.132)
Recalling that (δv/δV) ≡ J = det F, this means that J˙ = dJ/dt = (δv/δV). = J tr (F˙ · F−1 ) = J (tr L).
(4.133)
But, L = grad υ = ∂υ/∂x, and we have tr L = div υ = ∇ · υ,
(4.134)
J˙ = J div (υ).
(4.135)
or
Let us return now to the rate of change of an inﬁnitesimal material ﬁber (Fig. 4.3), and recall that dx = F · dX.
(4.136)
(dx). = dx˙ = F˙ · dX = L · F · dX = L · dx.
(4.137)
Then,
4.17. Velocity Gradient
73
Consider dx = ds ,
(4.138)
where = a unit vector dx, ds = the arc length of dx. By taking the time derivative we obtain ˙ + ds. dx˙ = ds ˙
(4.139)
Recalling that L = F˙ · F−1 and dX = F−1 · dx, we obtain ˙ + ds˙ = L · ds. dx˙ = ds
(4.140)
It is noted that ·=1
⇒
· ˙ = 0.
Thus, ds˙ = · L · ds
(4.141)
˙ = L · − ( · L · ).
(4.142)
and
Consequently, the change in length per unit length of the material ﬁber, dx, is found to be ds/ds ˙ = · L · .
(4.143)
If we decompose L into its symmetric and antisymmetric parts as L=
1 1 (L + LT ) + (L − LT ), 2 2
(4.144)
1 (L + LT ), 2
(4.145)
ds/ds ˙ = · D · .
(4.146)
and call D= then
The symmetric tensor D is called the rate of deformation or simply the deformation rate. The term velocity strain is also in use. We next look at the rate of change of the included angle between two material ﬁbers, i.e., at rates of shear. Let dx and dy be two inﬁnitesimal ﬁbers in the current state (Fig. 4.13). Then, dx = F · dX = ds x ,
dy = F · dY = mds y .
(4.147)
As for the angle between them, in the current state we have cos θ = · m
(4.148)
74
4. Kinematics of Continuum
F dy
θ
dY X
dX
"reference" or "undeformed" state
dx
x
Figure 4.13. Stretch and angular change between arbitrary ﬁbers.
"deformed" or "current" state
and d ˙ (cos θ) = − sin θ θ˙ = ˙ · m + · m. dt
(4.149)
Now, identify sin θ =  × m, and use (4.142) to get θ˙ =
1 ( · L · + m · L · m)( · m) − · (L + LT ) · m .  × m
(4.150)
4.18 Deformation Rate and Spin Recall again the deﬁnitions of the symmetric and antisymmetric parts of L, viz., L=
1 1 (L + LT ) + (L − LT ). 2 2
(4.151)
We call D the symmetric part and W the antisymmetric part of L, i.e., 1 (L + LT ), 2 1 W = (L − LT ). 2 D=
(4.152) (4.153)
From the polar decomposition theorem F = R · U = V · R,
(4.154)
˙ ·U+R·U ˙ =V ˙ ·R+V·R ˙ F˙ = R
(4.155)
F−1 = (R · U)−1 = U−1 · RT = (V · R)−1 = RT · V−1 .
(4.156)
˙ · RT + R · U ˙ · U−1 · RT L = F˙ · F−1 = R
(4.157)
˙ · V−1 + V · R ˙ · RT · V−1 , L=V
(4.158)
it follows that
and
Therefore,
or
4.19. Rate of Stretching and Shearing
75
because ˙ · RT )T . ˙ · RT = −(R R
(4.159)
For D and W, we obtain 1 ˙ · U−1 + U−1 · U) ˙ · RT R · (U 2
(4.160)
1 ˙ · U−1 − U−1 · U) ˙ · RT + R ˙ · RT . R · (U 2
(4.161)
D= and W=
If the current state is taken as the reference state, i.e., if F = I, U = I, and R = I, then instantaneously D=
1 ˙ ˙ 0) = U ˙0 (U0 + U 2
(4.162)
and ˙ 0. W=R
(4.163)
The subscript 0 signiﬁes the assignment of reference to current state.
4.19 Rate of Stretching and Shearing Once again consider two inﬁnitesimal ﬁbers dx and dy in the current state, as sketched in Fig. 4.13. Recall the connections dx = F · dX and dy = F · dY, where dX and dY are the same ﬁbers in the reference state. Recall also the representation of dx and dy in terms of unit vectors along them and their respective lengths, viz., dx = ds x and dy = mds y . For the change in length per unit length of dx, we have ds˙ x /ds x = · L · = · D · .
(4.164)
Also, from (4.150), θ˙ =
1 ( · L · + m · L · m)( · m) − · (L + LT ) · m .  × m
(4.165)
If it happened that, instantaneously, · m = 0 in the current conﬁguration, then θ˙ = − · (L + LT ) · m = −2 · D · m.
(4.166)
This suggests a possible deﬁnition of shearing rate as 1 γ˙ = − θ˙ = · D · m. 2
(4.167)
Since D is symmetric, it can be represented via a spectral form D=
3 r =1
αr pr pr .
(4.168)
76
4. Kinematics of Continuum
We also have the relations pr · ps = 0,
if r = s,
(ds/ds) ˙ pr = αr ,
(4.169)
3 1 ˙ s , pq ) = ps · − θ(p αr pr pr · pq . 2 r =1
Note a property of the last relation, viz., 3 1 ˙ s , pq ) = ps · αr pr pr · pq = 0, − θ(p 2 r =1
if s = q.
(4.170)
Thus the principal directions of D do not undergo relative angular changes and consequently undergo only rigid body rotations as a triad of vectors. Indeed, recall (4.142) for the time derivative of a unit vector along a ﬁber in the current state, ˙ = L · − ( · L · ),
(4.171)
and apply it to a principal direction, pi . There follows p˙i = L · pi − (pi · L · pi )pi .
(4.172)
This can be reduced to p˙i = D · pi + W · pi − (pi · D · pi )pi
(no sum on i)
= αi pi + W · pi − αi pi = W · pi ⇒ a rigid rotation. Thus W can be thought of as the instantaneous spin of the principal directions of D.
4.20 Material Derivatives of Strain Tensors: E˙ vs. D Recall that E=
1 1 T F · F − I = (C − I). 2 2
(4.173)
Taking the time derivative, we ﬁnd ˙ = 1C ˙ = 1 F˙ T · F + FT · F˙ E 2 2 1 T T F · L · F + FT · L · F = 2
1 T F · (L + LT ) · F . = 2 Thus, ˙ = FT · D · F = 1 C. ˙ E 2
(4.174)
4.20. Material Derivative of Strain
77
r
r0
2
l0
1
Figure 4.14. Geometry of uniaxial tension.
l 3
Only when the reference state is taken as the current state, i.e., when F = I instantaneously, do we have ˙ 0 = D0 . E
(4.175)
As an example, consider a homogeneous uniaxial tension or compression test. The reference gauge length of the uniaxial specimen is taken as 0 , and its current length is (Fig. 4.14). The geometry of uniaxial tension, or compression, then dictates the following deformation map x1 = (1 +
r − r0 )X1 r0
− 0 )X2 0 r − r0 x3 = (1 + )X3 . r0
x2 = (1 +
(4.176)
The stretches are deﬁned as λ ∼ length/initial length, and so for the three principal directions, λ1 = r/r0 , λ2 = /0 , λ3 = r/r0 .
(4.177)
The radial stretch in both directions is assumed to be the same, e.g., as would be the case for an isotropic material. For the deformation gradient we obtain ⎡
λ1 F=⎣0 0
0 λ2 0
⎤ 0 0 ⎦, λ3
⎡
F−1
1/λ1 =⎣ 0 0
0 1/λ2 0
⎤ 0 0 ⎦. 1/λ3
(4.178)
Also, ⎡
λ1 F=R·U ⇒ U=⎣0 0
0 λ2 0
⎤ 0 0 ⎦, λ3
R = I.
(4.179)
Thus, ⎤ λ21 0 0 C = FT · F = U2 = ⎣0 λ22 0 ⎦ . 0 0 λ23 ⎡
(4.180)
78
4. Kinematics of Continuum
The strain tensor is E=
1 1 T (F · F − I) = (C − I) 2 2 ⎡ 2 λ −1 1⎣ 1 = 0 2 0
⎤ 0 0 ⎦. λ23 − 1
0 λ22 − 1 0
(4.181)
The velocity gradient is ⎡
L = F˙ · F−1
λ˙ 1 /λ1 =⎣ 0 0
0 λ˙ 2 /λ2 0
⎤ ⎡ r˙ /r0 0 0 ⎦=⎣ 0 λ˙ 3 /λ3 0
0 ˙ 0 / 0
⎤ 0 0 ⎦. r˙ /r0
(4.182)
It is clear that L = D,
W = 0.
(4.183)
The rate of strain is ⎡ 2λ1 λ˙ 1 1 ˙E = ⎣ 0 2 0
0 2λ˙ 2 λ2 0
⎤ 0 0 ⎦. 2λ˙ 3 λ3
(4.184)
As a check on the above, form ˙ = FT · D · F E ⎡ λ1 0 = ⎣ 0 λ2 0 0 ⎡ 2λ1 λ˙ 1 1 = ⎣ 0 2 0
⎤ ⎡ λ˙ 1 /λ1 0 ⎣ ⎦ 0 · 0 λ3 0 0 2λ˙ 2 λ2 0
0 λ˙ 2 /λ2 0 ⎤
⎤ ⎡ λ1 0 0 ⎦·⎣0 λ˙ 3 /λ3 0
0 0 ⎦, 2λ˙ 3 λ3
0 λ2 0
⎤ 0 0⎦ λ3 (4.185)
in agreement with the previous result.
4.21 Rate of F in Terms of Principal Stretches The right stretch tensor can be expressed in terms of its eigenvalues – principal stretches λi (assumed here to be different) and corresponding eigendirections Ni as U=
3
λi Ni Ni .
(4.186)
˙i . ˙ i Ni + Ni N λ˙ i Ni Ni + λi N
(4.187)
i=1
The rate of U is then ˙ = U
3 i=1
4.21. Rate of F in Terms of Principal Stretches
79
If ei0 (i = 1, 2, 3) are the ﬁxed reference unit vectors, the unit vectors Ni of the principal directions of U can be expressed as Ni = R 0 · ei0 ,
(4.188)
where R 0 is the rotation that carries the orthogonal triad {ei0 } into the Lagrangian triad {Ni }. Deﬁning the spin of the Lagrangian triad by ˙ 0 · R −1 , Ω0 = R 0
(4.189)
˙ 0 · e0 = Ω0 · Ni = −Ni · Ω0 , ˙i =R N i
(4.190)
it follows that
and the substitution into (4.187) gives ˙ = U
3
λ˙ i Ni Ni + Ω0 · U − U · Ω0 .
(4.191)
i=1
If the spin tensor Ω0 is expressed on the axes of the Lagrangian triad as Ω0 = i0j Ni N j ,
(4.192)
i = j
it is readily found that Ω0 · U = 012 (λ2 − λ1 ) N1 N2 + 023 (λ3 − λ2 ) N2 N3 + 031 (λ1 − λ3 ) N3 N1 . Consequently, Ω0 · U − U · Ω0 = Ω0 · U + (Ω0 · U)T =
i = j
i0j (λ j − λi ) Ni N j .
(4.193)
(4.194)
The substitution into (4.191) yields ˙ = U
3
λ˙ i Ni Ni +
i = j
i=1
i0j (λ j − λi ) Ni N j .
(4.195)
Similarly, the rate of the Lagrangian strain tensor is ˙ = E
3
λi λ˙ i Ni Ni +
i = j
i=1
i0j
λ2j − λi2 2
Ni N j .
(4.196)
The principal directions of the left stretch tensor V, appearing in the spectral representation V=
3
λi ni ni ,
(4.197)
i=1
are related to principal directions Ni of the right stretch tensor U by ni = R · Ni = R · ei0 ,
R = R · R0 .
(4.198)
80
4. Kinematics of Continuum
The rotation tensor R is the rotation from the polar decomposition of the the deformation gradient F = V · R = R · U. By differentiating the above expression for ni , there follows n˙ i = Ω · ni ,
(4.199)
where the spin of the Eulerian triad {ni } is deﬁned by ˙ · R −1 = ω + R · Ω0 · RT , Ω=R
˙ · R−1 . ω=R
On the axes ni , the spin Ω can be decomposed as Ω= i j ni n j .
(4.200)
(4.201)
i = j
˙ it follows that By an analogous derivation, as used to obtain the rate U, 3
˙ = V
λ˙ i ni ni +
i j (λ j − λi ) ni n j .
(4.202)
ni Ni
(4.203)
˙ i = Ω · R − R · Ω0 , n˙ i Ni + ni N
(4.204)
i = j
i=1
The rate of the rotation tensor R=
3 i=1
is ˙ = R
3 i=1
or ˙ = R
i = j
i j − i0j ni N j .
(4.205)
Finally, the rate of the deformation gradient 3
λi ni Ni
(4.206)
˙i . λ˙ i ni Ni + λi n˙ i Ni + ni N
(4.207)
F=
i=1
is F˙ =
3 i=1
˙ i = Ω0 · Ni , it follows that Since n˙ i = Ω · ni and N F˙ =
3
λ˙ i ni Ni + Ω · F − F · Ω0 ,
(4.208)
i=1
and F˙ =
3 i=1
λ˙ i ni Ni +
i = j
λ j i j − λi i0j ni N j .
(4.209)
4.21. Rate of F in Terms of Principal Stretches
81
4.21.1 Spins of Lagrangian and Eulerian Triads The inverse of the deformation gradient can be written in terms of the principal stretches as F−1 =
3 1 Ni ni . λ i=1 i
(4.210)
Using this and (4.209) we obtain an expression for the velocity gradient 3 ˙ λi λi 0 i j − ni ni + i j ni n j . L = F˙ · F−1 = λ λj i = j i=1 i
(4.211)
The symmetric part of this is the rate of deformation tensor, D=
3 ˙ λi i=1
λi
ni ni +
λ2j − λi2 i = j
2λi λ j
i0j ni n j ,
whereas the antisymmetric part is the spin tensor λi2 + λ2j 0 W= i j ni n j . i j − 2λi λ j i = j
(4.212)
(4.213)
Evidently, for i = j from (4.212) we have i0j =
2λi λ j Di j , λ2j − λi2
λi = λ j ,
(4.214)
which is an expression for the components of the Lagrangian spin Ω0 in terms of the stretch ratios and the components of the rate of deformation tensor. Substituting (4.214) into (4.213) we obtain an expression for the components of the Eulerian spin Ω in terms of the stretch ratios and the components of the rate of deformation and spin tensors, i.e., i j = Wi j +
λi2 + λ2j λ2j − λi2
Di j ,
λi = λ j .
(4.215)
The inverse of the rotation tensor R is R−1 =
3
Ni ni ,
(4.216)
i=1
so that, by virtue of (4.205), the spin ω can be expressed as ˙ · R−1 = ω=R i j − i0j ni n j .
(4.217)
i = j
Thus, ωi j = i j − i0j ,
(4.218)
where i0j are the components of Ω0 on the Lagrangian triad {Ni }, whereas i j are the components of Ω on the Eulerian triad {ni }. When (4.214) and (4.215) are substituted into (4.218), we obtain an expression for the spin components ωi j in terms of the stretch ratios
82
4. Kinematics of Continuum
and the components of the rate of deformation and spin tensors, which is ωi j = Wi j +
λ j − λi Di j . λi + λ j
(4.219)
4.22 Additional Connections Between Current and Reference State Representations LEMMA 4.3: If u is a vector ﬁeld and T is a tensor ﬁeld representing properties of a deforming
body, then Div u = J div (J −1 F · u),
Div T = J div (J −1 F · T).
(4.220)
Proof: The above relations depend on the result ∂ −1 J F pα = 0, ∂ xp which is justiﬁed from Lemma 4.1. In fact replacing t with Xα , we obtain ∂ Fqρ −1 ∂ 2 xq ∂F −1 =J ∂ J/∂ Xα = J tr ·F Fρq = J F −1 , ∂ Xα ∂ Xα ∂ Xα ∂ Xρ ρq where we note that Fαi−1 = ∂ xi /∂ Xα , and J = det F. Thus, ∂ Xπ ∂ −1 ∂ −1 J F pα = J F pα ∂ xp ∂ Xπ ∂ xp ∂ 2 xp ∂ 2 xq −1 = J −1 − J −1 Fρq F pα Fπ−1 p ∂ Xα ∂ Xπ ∂ Xπ ∂ Xρ 2 ∂ xq ∂ 2 xq −1 −1 = 0. = J −1 Fρq − δπ α Fρq ∂ Xα ∂ Xρ ∂ Xπ ∂ Xρ Furthermore, we obtain ∂uπ Div u − J div J −1 F · u = − J J −1 F pπ uπ ∂ Xπ =
∂uπ ∂uπ − F pπ ∂ Xπ ∂ xp
=
∂uπ ∂uπ ∂ x p − =0 ∂ Xπ ∂ x p ∂ Xπ
and ∂ Tπρ ∂ Div T − J div J −1 F · T = Eρ − J (J −1 F pπ Tπq )eq ∂ Xπ ∂ xp =
∂ Tπq ∂ Tπρ Eρ − F pπ eq ∂ Xπ ∂ xp
=
∂ (Tπρ Eρ − Tπq eq ) = 0. ∂ Xπ
(4.221)
(4.222)
4.23. Transport Formulae
83
4.23 Transport Formulae We now turn our attention to the rates of change of integrals over material curves, surfaces, and volume elements. We focus attention to the area or volume elements in the current state. LEMMA 4.4: Let C, S, and V represent a material line (curve), a surface, and a volume element, respectively in the current state; as usual, φ(x) is a scalar ﬁeld. Then, d φ dx = (φ˙ dx + φ L · dx), dt C C
d (φ˙ + φ tr L)n − φ LT · n da, φ n da = (4.223) dt S S d φ dv = (φ˙ + φ tr L) dv, dt V V
where n is the unit normal to the external surface, S, of the body. If u(x) is a continuous and differentiable vector ﬁeld, then the corresponding results are d u · dx = (u˙ + LT · u) · dx, dt C C d u · n da = (u˙ + u tr L − L · u) · n da, (4.224) dt S S d u dv = (u˙ + u tr L) dv. dt V V Proof: We focus on the second of the above relations, as the other relations follow by direct analogy. We have −T d d u · J F · N dA u · n da = dt S dt SR ∂ −T u · J F · N dA = SR ∂t ∂ (J F−1 · u) · N dA = SR ∂t −1
J F · u˙ + (J tr L) · F−1 · u + J (−F−1 · L) · u · N dA =
SR
(u˙ + u tr L − L · u) · (J F−T · N dA)
=
SR
(u˙ + u tr L − L · u) · n da.
= S
In developing the above use was made of the following . (F−1 ) = −F−1 · F˙ · F−1 ,
. L = F˙ · F−1 = −F · (F−1 ) ,
84
4. Kinematics of Continuum
and J˙ = tr L. Also, if dx = F · dX and dy = F · dY are vector elements in the current and reference states respectively, then nda = (F · dX) × (F · dY) = J F−T · NdA.
4.24 Material Derivatives of Volume, Area, and Surface Integrals: Transport Formulae Revisited We recall the results for the rate of change of a volume element, d ∂vi dV. (dV) = dt ∂ xi Examine integrals of the type
(4.225)
Ai j... (t) =
Ai j... (x, t) dV,
(4.226)
V
and, more particularly, their time derivatives d d Ai j... (t) = Ai j... (x, t) dV. dt dt V
(4.227)
Since this integral is taken over a ﬁxed amount of mass (i.e., material), we may interchange the order of differentiation and integration. This leads to d d Ai j... (x, t) dV = (4.228) [Ai j... (x, t) dV] , dt V dt V which on using (4.225) leads to dAi j... (x, t) ∂v p d + Ai j... (x, t) Ai j... (x, t) dV = dV. dt V dt ∂ xp V
(4.229)
We next recall the relation for the material derivative operator, viz., ∂ d ∂ = + vp . dt ∂t ∂ xp When this is used in the above it is found that ! ∂ Ai j... (x, t) ∂ d + Ai j... (x, t)dV = [v p Ai j... (x, t)] dV. dt v ∂t ∂ xp V The divergence theorem may be used on the second term on the rhs to obtain ∂ Ai j... (x, t) d dV + v p Ai j... (x, t)n p dS, Ai j... (x, t) dV = dt v ∂t V S
(4.230)
(4.231)
(4.232)
where n is the outward pointing unit normal to the surface S that bounds V and n p is its pth component. We next examine surface integrals of the form Bi j... (t) = Bi j... (x, t)n p dS, (4.233) S
and derivatives of the type d d Bi j... (x, t)n p dS = [Bi j... (x, t)n p dS] . dt S dt S
(4.234)
4.25. Analysis of Simple Shearing
85
Figure 4.15. Geometry of simple shear.
From the solved Problem 4.11 of Chapter 34, with dSp ≡ n p dS, we have dSp = (∂vq /∂ xq )dSp − (∂vq /∂ x p )dSq , dt
(4.235)
which describes the rate of change of surface area elements. Using this in (4.234), we obtain dBi j... (t) = dt
S
dBi j... (x, t) ∂vq ∂v p + Bi j... (x, t) dSp − Bi j... (x, t) dSp . dt ∂ xq ∂ xq S
Finally, consider line integrals of the type Li j... (t) = Li j... (x, t) p ds,
(4.236)
C
where ds is an element of arc length and is the running tangent at each point on the line; p is then the pth component of that tangent. Recall that p ds = dx p and ∂v p d (dx p ) = dxk. dt ∂ xk Then, d dt
Li j... (x, t) dx p =
C
and dLi j... (t) = dt
C
C
d [Li j... (x, t) dx p ] dt
dLi j... (x, t) dx p + dt
C
∂v p [Li j... (x, t)] dxk. ∂ xk
(4.237)
(4.238)
(4.239)
4.25 Analysis of Simple Shearing Consider the motion depicted in Fig. 4.15. The motion is associated with the deformation gradient, F = I + γ (t)m.
(4.240)
Let n be a third unit vector that along with and m form a righthanded triad and serve as a basis system. The deformation prescribed by the above F is volume preserving because det F = [F · , F · m, F · n] = [, m + γ , n] = [, m, n] = 1.
(4.241)
86
4. Kinematics of Continuum
We also note that F−1 = I − γ m, FT = I + γ m,
(4.242)
I = + mm + nn. Thus, C = FT · F = + (1 + γ 2 )mm + nn + γ (m + m).
(4.243)
Since C · n = n, the vector n is clearly an eigenvector with an eigenvalue of 1; let p1 and p2 be the other two eigenvectors of C. Then, C=
3
λi2 pi pi ,
(4.244)
i=1
where formally p3 = n. But since det F = λ1 λ2 λ3 = 1, and λ3 = 1, it is clear that λ1 = 1/λ2 . Recall that det C = det(FT · F) = (det F)2 . Thus, letting λ = λ1 , we write C = λ2 p1 p1 + λ−2 p2 p2 + nn.
(4.245)
Next, express the eigenvectors as p1 = cos θ + sin θm, p2 = − sin θ + cos θm.
(4.246)
We use these in (4.245), and then in (4.243), to form the equations C · p1 = λ2 p1 ,
C · p2 = λ−2 p2 .
(4.247)
Upon expanding, we obtain the set λ2 cos2 θ + λ−2 sin2 θ = 1, λ2 sin2 θ + λ−2 cos2 θ = 1 + γ 2 ,
(4.248)
(λ2 − λ−2 ) sin θ cos θ = γ , which has the solution 1 1 λ = (1 + γ 2 )1/2 + γ = cot ψ, 4 2 1 θ = π − ψ, 2 1 ψ = tan(2/γ ). 2
(4.249)
Thus, the principal stretches are λ1 = cot ψ, λ2 = tan ψ, λ3 = 1,
(4.250)
4.26. Examples of Particle and Plane Motion
87
with the corresponding principal directions p1 = sin ψ + cos ψm, p2 = − cos ψ + sin ψm,
(4.251)
p3 = n. But γ is a function of time and we note that F˙ = γ˙ m. Thus, the velocity gradient becomes L = γ˙ m · (I − γ m) = γ˙ m,
(4.252)
which, in turn, means that the velocity is υ = γ˙ (m) · x.
(4.253)
The rate of deformation and spin rates become 1 (m + m), 2 1 W = (m − m). 2 Consider the effect of W on an arbitrary vector a. We have D=
W·a=
1 1 γ˙ [(a · m) − (a · )m] = − γ˙ n × a, 2 2
(4.254)
(4.255)
and thus 12 γ˙ n is the axial vector of W.
4.26 Examples of Particle and Plane Motion Consider a deformation map prescribed by x1 = X1 + kt X3 , x2 = X2 + kt X3 ,
(4.256)
x3 = X3 − kt(X1 − X2 ), where the geometry is sketched in Fig. 4.16. The parameter k is a constant and t is time. We will show that the motion of an arbitrary particle is along a straight line always orthogonal to X, the vector from the origin to the initial position of the particle. Further, if there was a slab, as also depicted in the ﬁgure, lying with its faces perpendicular to the X1 axis, this slab would reorient such that, in the limit as t → ∞, the slab’s faces would lie inclined to the X1 axes at π/4. From (4.256) we ﬁrst form the components of the deformation gradient and the vector of material velocity. These are ⎤ ⎡ 1 0 kt (4.257) F=⎣ 0 1 kt ⎦ , −kt −kt 1 and υ = kX3 e1 + kX3 e2 − k(X1 + X2 )e3 .
(4.258)
88
4. Kinematics of Continuum
X2
X2
υ X Figure 4.16. (a) Position vector, X, of an arbitrary particle. (b) Slab with its initial faces perpendicular to the X1 axis.
e1
o X1 X3
X1
(a)
(b)
X3
Since the vector to the arbitrary material particle is X, the velocity is – and for all t is – orthogonal to X, because υ · X = [kX3 e1 + kX3 e2 − k(X1 + X2 )e3 ] · [X1 e1 + X2 e2 + X3 e3 ] = 0.
(4.259)
Next consider the two vectors that deﬁne the sides of the slab. In the current state they are F · e2 = Fq2 eq ,
F · e3 = Fr 3 er .
(4.260)
Thus, the normal to the slab’s face is n=
Fq2 e2 × Fr 3 e3 . Fq2 e2  Fr 3 e3 
(4.261)
A straightforward calculation shows that n · e1 = which, in the limit, becomes
1 − (kt)2 , [1 + (kt)2 ]1/2 [1 + 2(kt)2 ]1/2 √ lim n · e1 = 1/ 2,
t→∞
(4.262)
(4.263)
thus demonstrating the proposition.
4.27 Rigid Body Motions LEMMA 4.5: Let {e1 , e2 , e3 } and {e 1 , e 2 , e 3 } be two orthonormal unit bases systems. Then
P = e p e p
(4.264)
is an orthogonal tensor. Proof: If a and b are two arbitrary vectors and if P is an orthogonal tensor, then (P · a) · (P · b) = a · b. To verify this, write (P · a) · (P · b) = (e p e p · a) · (e p e p · b) = (a · P T ) · (P · b) = (a · e p e p ) · (e s es · b).
(4.265)
4.28. Behavior under Superposed Rotation
89
x Figure 4.17. Two material ﬁbers.
y
The last equality veriﬁes the proposition since e p · e s = δ ps and, of course, a p = a · e p and bs = b · es . Thus (P · a) · (P · b) = a · b, as P deﬁnes an orthogonal tensor. LEMMA 4.6: If the distance between every pair of material points is the same following a motion, the motion is said to be rigid. For this to be the case the mapping must be of the form
x(t) = c(t) + Q(t) · X,
(4.266)
where Q is an orthogonal tensor. Proof: Refer to Fig. 4.17 showing two material vectors, x and y. First note that the term c(t) simply represents a uniform translation of the body. This clearly produces no changes in the length of any ﬁbers or any changes in the relative angle between any two ﬁbers. Thus, we are concerned only with the remaining part of the transformation, i.e., x − c = Q · X.
(4.267)
We proceed as follows. Form the scalar product between the two vectors x − c and y − c, (x − c) · (y − c) = (Q · X) · (Q · Y) = (X · QT ) · (Q · Y) = X · Y, which is constant for given X and Y. Also, x − y = X − Y, because Q is orthogonal and x − y = Q · (X − Y). Furthermore, since x = c + Q · X, the velocity is ˙ · X. x˙ = υ = dx/dt = c˙ (t) + Q
(4.268)
X = QT · [x − c(t)],
(4.269)
˙ · QT · (x − c). υ = x˙ = c˙ (t) + Q
(4.270)
But,
and so
Conversely, ˙ · QT + Q · Q ˙T=0 ⇒ Q ˙ · QT = −Q · Q ˙ T. Q · QT = I ⇒ Q ˙ · QT = W is antisymmetric, and we so write Thus, Q υ = x˙ = c˙ + W · (x − c).
(4.271)
4.28 Behavior under Superposed Rotation If a timedependent rotation Q(t) is superposed to the deformed conﬁguration at time t, an inﬁnitesimal material line element dx becomes dx∗ = Q · dx,
(4.272)
90
4. Kinematics of Continuum
whereas in the undeformed conﬁguration dX∗ = dX.
(4.273)
Consequently, since dx = F · dX, we have F∗ = Q · F.
(4.274)
This implies that U∗ = U,
C∗ = C,
E∗ = E,
(4.275)
and V∗ = Q · V · QT ,
B∗ = Q · B · Q T .
(4.276)
The objective rate of the deformation gradient F transforms according to ∇
∇
F∗ = Q · F,
∇
F = F˙ − W · F .
(4.277)
The rotation R becomes R∗ = Q · R.
(4.278)
˙ · R−1 changes to The spin ω = R ω ∗ = Ω + Q · ω · QT ,
˙ · Q−1 . Ω=Q
(4.279)
The velocity gradient transforms as L∗ = Ω + Q · L · QT ,
(4.280)
whereas the rate of deformation and the spin tensor become D∗ = Q · D · QT , W∗ = Ω + Q · W · QT .
(4.281)
4.29 Suggested Reading Chadwick, P. (1999), Continuum Mechanics: Concise Theory and Problems, Dover, New York. Chung, T. J. (1996), Applied Continuum Mechanics, Cambridge University Press, Cambridge, UK. Eringen, A. C. (1967), Mechanics of Continua, Wiley, New York. Fung, Y.C. (1965), Foundations of Solid Mechanics, Prentice Hall, Englewood Cliffs, New Jersey. Hill, R. (1978), Aspects of Invariance in Solid Mechanics, Adv. Appl. Mech., Vol. 18, pp. 1–75. Hunter, S. C. (1983), Mechanics of Continuous Media, Ellis Horwood, Chichester, UK. Jaunzemis, W. (1967), Continuum Mechanics, The Macmillan, New York. Lai, W. M., Rubin, D., and Krempl, E. (1993), Introduction to Continuum Mechanics, Pergamon, New York. Malvern, L. E. (1969), Introduction to the Mechanics of a Continuous Medium, Prentice Hall, Englewood Cliffs, New Jersey.
4.29. Suggested Reading
91
Ogden, R. W. (1984), NonLinear Elastic Deformations, Ellis Horwood, Chichester, UK (2nd ed., Dover, 1997). Prager, W. (1961), Introduction of Mechanics of Continua, Ginn and Company, Boston. Sedov, L. I. (1966), Foundations of the NonLinear Mechanics of Continua, Pergamon, Oxford, UK. Spencer, A. J. M. (1992), Continuum Mechanics, Longman Scientiﬁc & Technical, London. Truesdell, C., and Toupin, R. (1960), The Classical Field Theories. In Handbuch der Physik (S. Flugge, ¨ ed.), Band III/l, SpringerVerlag, Berlin. Truesdell, C., and Noll, W. (1965), The Nonlinear Field Theories of Mechanics. In Handbuch der Physik (S. Flugge, ¨ ed.), Band III/3, SpringerVerlag, Berlin (2nd ed., 1992).
5 Kinetics of Continuum
5.1 Traction Vector and Stress Tensor There are two general types of forces we consider in the mechanics of solid bodies, viz., applied surface traction and body forces. Examples of body forces include, inter alia, gravitational forces (selfweight), electrostatic forces (in the case of charged bodies in electric ﬁelds), and magnetic forces. Body forces are usually described as a density of force and thus have units of newtons per cubic meter [N/m3 ]. Surface traction has, as expected, units of newtons per square meter [N/m2 ]. We then describe a body force density as b, so that the total body force acting on a volume element δv is bδv. Surface traction must be described in terms of the vector force involved and with respect to the surface element it acts on; this, in turn, is described by the unit normal, n, to the surface element that the traction acts on. Let Tn be the traction vector measured per unit area of the surface element involved. Then the total force acting on an area element with normal n and area ds is Tn ds. These are depicted in Fig. 5.1. Consider a thin “wafer” of material whose lateral dimensions are of O(h) and whose thickness is of O(); we will soon take the limit as lim/ h→0 . In any event, / h 1. Equilibrium for the wafer requires that T ds + Tn+ dA+ Tn− dA+ b dA = 0. (5.1)
Here is the total area of the wafer’s top and bottom sides and is the perimeter around its edge. The traction vectors, Tn+ and Tn− act on the “top” and “bottom” sides of the wafer, respectively. The wafer’s thickness is . If → 0, we have T ds → 0, b dA → 0, (5.2)
and we arrive at the notion of traction continuity Tn+ dA+ Tn− dA = 0.
(5.3)
Since is arbitrary, we must have Tn+ = −Tn− . 92
(5.4)
5.1. Traction Vector and Stress Tensor
93 n+
n
Γ
Tn+ Tn ds
Ω Figure 5.1. Traction vector over the surface element.
h
δv
ε
b δv
n
b Tn 
Consider next the tetrahedron shown in Fig. 5.2. This is known as the Cauchy tetrahedron. Let a1 , a2 , a3 be the areas of the three faces having normals in the e1 , e2 , e3 directions, respectively. The volume of the tetrahedron is v. Note that the edges of the oblique face make intercepts with the axes at locations marked a, b, c. The distances along the axes of these intercepts are 1 , 2 , 3 . Note also that the three faces aligned with the coordinate axes have unit normals along −e1 , −e2 , −e3 , respectively. Simple geometry reveals that 1 1 1 1 2 3 , a 2 = 1 3 , a 3 = 2 1 , v = 1 2 3 . (5.5) 2 2 2 6 We need to calculate the area of the oblique face, and for this purpose we deﬁne two convenient vectors that deﬁne the oblique surface element. If we call an the magnitude of the area of this oblique surface element, and n its unit normal, its vector area will be an n. Clearly, a1 =
1 (b − a) × (c − a), (5.6) 2 where a, b, and c are the edge vectors comprising the sides of the inclined face of the Cauchy tetrahedron. In terms of the intercepts and unit base vectors, this becomes an n =
1 (−1 e1 + 2 e2 ) × (−1 e1 + 3 e3 ) 2 1 = (3 1 e2 + 1 2 e3 + 2 3 e1 ). 2
an n =
(5.7)
Thus, an n = ai ei ⇒ ai = an (n · ei ). e3
e3
n
c a2 Te 2
ε3 ε1
a nTn
c
a1 Te 1
ε3
ε2
b υb
a e1
(5.8)
a3 Te 3
e2
ε1
a e1
Figure 5.2. The Cauchy tetrahedron.
ε2
b
e2
94
5. Kinetics of Continuum
n
σ22
σnn Tn
σ23 σ32
σns
σ33
x2
σ21
σ12
σ11 Figure 5.3. Rectangular stress components of Cauchy stress.
σ31 σ13
x1 x3
The equilibrium of the tetrahedron yields an Tn + a1 Te−1 + a2 Te−2 + a3 Te−3 + vb = 0,
(5.9)
Tn + (n · ei )Tei− + v/an b = 0.
(5.10)
or, more compactly,
In the limit when i → 0, or v/an → 0, we obtain Tn = −(n · ei )Tei− = (n · ei )Tei .
(5.11)
σ ≡ ei Tei ,
(5.12)
Tn = n · σ .
(5.13)
Tei = Tei j e j ,
(5.14)
σ = Tei j ei e j .
(5.15)
This suggests the deﬁnition
such that
But,
which suggests a further deﬁnition
This yields σ = σi j ei e j ,
σi j = Tei j .
(5.16)
With reference to Fig. 5.3, we can represent the normal and shear components of stress as σnn = n · σ · n, σns = n · σ · s.
(5.17)
5.2 Equations of Equilibrium Consider a loading system on a solid body consisting of body forces and applied surface traction. Equilibrium requires that Tn dS + b dV = 0, (5.18) S
V
5.3. Balance of Angular Momentum: Symmetry of σ
95
Tn n S r(x)
Figure 5.4. A portion of an equilibrated body under surface tractions and body forces.
V
0
Tn
b(x)
where dS is a surface area element and S the body’s surface as depicted in Fig. 5.4. Since Tn = n · σ, (5.18) can be written as n · σ dS + b dV = 0. (5.19) S
The divergence theorem gives
V
n · σ dS =
∇ · σ dV,
S
which, in turn, leads to
(5.20)
V
v
(∇ · σ + b) dV = 0.
(5.21)
Since V is arbitrary, we ﬁnd that at every point div σ + b = ∇ · σ + b = 0.
(5.22)
These are the equilibrium equations. Since σ = σi j ei e j ,
(5.23)
we can write, in component form, the three equilibrium equations as ∂σ ji + bi = 0, ∂xj
i = 1, 2, 3.
(5.24)
The components of the body force per unit current volume are bi .
5.3 Balance of Angular Momentum: Symmetry of σ The requirement of vanishing net torque on the solid body requires that r × Tn dS + r × b dV = 0, S
(5.25)
V
where r is a position vector within the body measured from an arbitrary point (Fig. 5.4). Using the fact that Tn = n · σ = σ T · n, the above becomes T r × (σ · n) dS + r × b dV = 0. (5.26) S
V
96
5. Kinetics of Continuum
The corresponding equation in the index notation is i jk x j σlknl dS + i jk x j bk dV = 0 . S
By the Gauss divergence theorem ∂ i jk x j σlknl dS = i jk (x j σlk) dV ∂ xl S V ∂σlk = i jk σ jk + x j dV . ∂ xl V Then, (5.27) becomes
i jk x j V
(5.27)
V
∂σlk + bk dV + i jkσ jk dV = 0 . ∂ xl V
The ﬁrst integral vanishes by equilibrium equations. Thus, i jkσ jk dV = 0 .
(5.28)
(5.29)
(5.30)
V
This holds for the whole volume V, or any part of it, so that we must have at every point i jkσ jk = 0 .
(5.31)
Since i jk is antisymmetric in jk, the stress tensor must be symmetric, σ jk = σkj . Alternatively, by multiplying (5.31) with mni and by using − δ relation mni jki = δmj δnk − δmkδnj ,
(5.32)
mni i jkσ jk = σmn − σnm = 0 .
(5.33)
there follows
Consequently, σmn = σnm,
or
σ = σT ,
(5.34)
establishing that the Cauchy stress tensor is a symmetric tensor.
5.4 Principal Values of Cauchy Stress To explore principal values, σi , of the Cauchy stress tensor, we consider the equation σ · n = σ n.
(5.35)
σi = ni · σ · ni
(5.36)
The eigenvalues
are the principal stresses, and the eigenvectors ni are the unit normals to principal planes of the stress tensor σ. Since σ · ni − σi ni = 0 ,
(5.37)
there is no shear stress on the principal planes. The principal stresses and principal planes are determined by solving the eigenvalue problem (5.35). If the three eigenvalues are
5.5. Maximum Shear Stresses
97
tn n
p 2
σns
σnn Figure 5.5. Coordinate system of the principal directions.
σ
2
σ1 p 1
σ3 p 3
different, there are three mutually orthogonal principal directions. If two eigenvalues are equal, e.g., σ1 = σ2 = σ3 , any direction in the plane orthogonal to n3 is the principal direction. If three eigenvalues are equal to each other, the stress state is said to be spherical; any direction is the principal direction, without shear stress on any plane.
5.5 Maximum Shear Stresses Imagine that the principal stresses have been determined along with the corresponding eigenvectors, i.e., the principal directions of the Cauchy stress tensor σ. Call them {p1 , p2 , p3 }. Call the three principal stresses {σ1 , σ2 , σ3 }, and assume without loss of generality that they are algebraically ordered as σ1 ≥ σ2 ≥ σ3 . Now consider an arbitrary area element within the body at a point with unit normal n. The traction acting on this area element is tn . The components of tn with respect to the principal directions are then t1n = σ1 n1 , t2n = σ2 n2 ,
(5.38)
t3n = σ3 n3 , where the components of the unit normal n are likewise referred to the principal directions of σ. The normal stress on the area element is σnn = n · σ · n = σ1 n21 + σ2 n22 + σ3 n23 .
(5.39)
The stress component σns , deﬁned in Fig. 5.5 is the shear stress acting in the area element resulting from the tangential force resolved from tn . Then since the magnitude of tn is 2 2 tn · tn = σnn + σns ,
(5.40)
2 2 σns = tn · tn − σnn .
(5.41)
we have
With the obvious substitutions, we obtain 2 σns = σ12 n21 + σ22 n22 + σ32 n23 − (σ1 n21 + σ2 n22 + σ3 n23 )2 .
(5.42)
Extremum values for σns are found using the Lagrangian multiplier. Let 2 L = σns − λ(ni n1 − 1),
(5.43)
5. Kinetics of Continuum
N
t n
>
n
T N
>
>
>
98
Figure 5.6. The traction vector in the reference and deformed states.
ds
dS F
subject to the constraint that ni ni = 1. Then ∂L/∂λ = 0 yields the system
n1 σ12 − 2σ1 (σ1 n21 + σ2 n22 + σ3 n23 ) + λ = 0,
n2 σ22 − 2σ2 (σ1 n21 + σ2 n22 + σ3 n23 ) + λ = 0,
n3 σ32 − 2σ3 (σ1 n21 + σ2 n22 + σ3 n23 ) + λ = 0.
(5.44)
These equations are solved for λ and the components of n, subject to the constraint that n21 + n22 + n23 = 1. There are two sets of solutions possible. The ﬁrst set is n1 = ±1, n2 = 0, n3 = 0, for which σns = 0, n1 = 0, n2 = ±1, n3 = 0, for which σns = 0, n1 = 0, n2 = 0, n3 = ±1, for which σns = 0. The shear stresses are zero because these solutions for n are just to align it with a principal direction; this yields minimum values for σns . Another set of solutions is √ √ n1 = 0, n2 = ±1/ 2, n3 = ±1/ 2, for which σns = (σ2 − σ3 )/2, √ √ n1 = ±1/ 2, n2 = 0, n3 = ±1/ 2, for which σns = (σ1 − σ3 )/2, √ √ n1 = ±1/ 2, n2 = ±1/ 2, n3 = 0, for which σns = (σ1 − σ2 )/2. The second expression gives the maximum shear stress, which is equal to half the difference between the maximum and minimum principal stress. Also, the maximum shear stress acts in the plane that bisects the right angle between the directions of the maximum and minimum principal stresses.
5.6 Nominal Stress Recall the connection between area elements in the deformed and the reference state, ˆ ˆ = (det F)F−T · NdS. nds
(5.45)
Deﬁne the nominal traction TNˆ acting on the area element in the reference state (Fig. 5.6) by TNˆ dS = tnˆ ds ,
(5.46)
5.7. Equilibrium in the Reference State
99
where tnˆ is the true traction acting in the corresponding area element in the deformed ˆ we have state. Since tnˆ = σ · n, ˆ ˆ = σ · (det F)F−T · NdS. TNˆ dS = σ · nds
(5.47)
This deﬁnes the nominal stress tensor, or the ﬁrst Piola–Kirchhoff stress tensor, P = (det F)σ · F−T ,
(5.48)
ˆ If we decompose the nominal stress on the bases in the undeformed such that TNˆ = P · N. and deformed conﬁguration, we have P = Pi j ei E j .
(5.49)
Thus, the nominal stress deﬁned in this way has the following interpretation Pi j = ei · P · E j = i th component of force acting on an area element that had its normal in the j direction and had a unit area in the reference state. The representation Pˆ is also used in the literature, where Pˆ = PT . This is associated with the relationship to nominal traction, viz., ˆ · Pˆ . TNˆ = N
(5.50)
Pˆ = Pˆi j Ei e j ,
(5.51)
In this case
so that Pˆi j = Ei · Pˆ · ei = j th component of force acting on an area element that had its normal in the i direction and had a unit area in the reference state. It is noted that ﬁrst Piola–Kirchhoff stress is not symmetric. Since σ=
1 P · FT , det F
(5.52)
the symmetry of the Cauchy stress (σ = σ T ) implies P · FT = (P · FT )T = F · PT , or P · FT = F · PT .
(5.53)
5.7 Equilibrium in the Reference State We had already established the concept of nominal stress based on the idea of traction equality, i.e., TN dS = tn ds.
(5.54)
100
5. Kinetics of Continuum
S0 N
T N
t n
n
Figure 5.7. Nominal and true traction in the reference and current states.
ds
dS
V
F
0
To establish equilibrium in the reference state, we recall the deﬁnition of the nominal stress, viz., P = (det F)σ · F−T . With this in mind, global equilibrium requires that TN dS0 + B dV0 = 0. (5.55) S0
V0
The body force per unit reference volume is B. With the understanding that Tn = P · N, where N is the unit normal to the body’s surface S0 (see Fig. 5.7), (5.55) becomes P · N dS0 + B dV0 = 0. (5.56) S0
V0
By the usual route, the divergence theorem leads to (Div PT + B) dV0 = 0,
(5.57)
V0
i.e., Div PT + B = 0. By taking the time derivative of (5.56) we ﬁnd that d (Div PT + B) dV0 = 0, dt V0
(5.58)
(5.59)
where we note that dV0 /dt = 0. Thus, in rate form, T ˙ = 0. Div P˙ + B
(5.60)
Such a simple rate form equation does not hold for the Cauchy stress and its rate. In component form (5.58) becomes ∂ Pi j + Bi = 0. ∂ Xj
(5.61)
∂ P˙i j + B˙ i = 0. ∂ Xj
(5.62)
whereas, in rate form,
5.8 Work Conjugate Connections Consider an increment of work performed during an incremental displacement, i.e., δw = (P · N) · δu dS0 . (5.63) S0
5.8. Work Conjugate Connections
101
The rate of such working, at ﬁxed imposed stress, is w˙ = (P · N) · u˙ dS0 .
(5.64)
S0
But the connection between positions in the current and reference states is x = X + u,
˙ x˙ = u.
(5.65)
˙ ˙ ˙ ∂ x/∂X = ∂ u/∂X = F,
(5.66)
Recalling also that F = ∂x/∂X, we can write
(u˙ · P) · N dS0 =
w˙ = S0
Div (u˙ · P) dV0 = V0
or
˙ dV0 , Div (PT · u) V0
˙ dV0 . (u˙ · Div PT + P : F)
w˙ =
(5.67)
V0
˙ = 0, Div PT = 0, and so Consider the case where B = B P : F˙ dV0 , w˙ =
(5.68)
V0
where P : F˙ = Pi j F˙i j . Note, if Pˆ = PT is used as a nominal stress, then P : F˙ = Pi j F˙i j = Pˆ ji F˙i j = Pˆ · · F˙ .
(5.69)
If R0 is the work rate per unit reference volume, then R0 =
work rate = P : F˙ = Pi j F˙i j . unit reference volume
(5.70)
Since P = (det F)σ · F−T , we have ˙ R0 = (det F)(σ · F−T ) : F,
(5.71)
and, since σ = σ T , R0 = (det F) σ :
1 ˙ F · F−1 + (F˙ · F−1 )T . 2
(5.72)
This is is equivalent to R0 = (det F) σ : D = τ : D,
(5.73)
where we deﬁne the Kirchhoff stress as τ = (det F) σ.
(5.74)
˙ = FT · D · F ⇒ D = F−T · E˙ · F−1 , E
(5.75)
Recalling that
102
5. Kinetics of Continuum
we can further write R0 = (det F) σ : (F−T · E˙ · F−1 ) −T ˙ −1 Esp F pi = (det F) σi j F js −T −1 ˙ = (det F) σi j F js F pi Esp −1 −T ˙ Esp . = (det F) F pi σi j F js
Thus, ˙ R0 = (det F) F−1 · σ · F−T : E,
(5.76)
from which we extract the stress measure S = (det F) F−1 · σ · F−T ,
(5.77)
which we call the second Piola–Kirchhoff stress. Thus, for the rate of working per unit initial volume we have ˙ R0 = P : F˙ = τ : D = S : E.
(5.78)
To summarize, we have introduced three measures of stress, each conjugate to a particular deformation measure vis`avis the work rate per unit reference volume, i.e., Nominal stress = P = (det F) σ · F−T , Kirchhoff stress = τ = (det F) σ,
(5.79)
2nd Piola–Kirchhoff stress = S = (det F) F−1 · σ · F−T . We can say that P is work conjugate to F, whereas S is work conjugate to E.
5.9 Stress Deviator The general tensor, such as σ, can be uniquely decomposed into a deviatoric part as σ = σ +
1 (tr σ)I. 3
(5.80)
In proof, assume there were two such decompositions, viz., σi j = λδi j + σi j = λ∗ δi j + σi ∗j , with σii = σii ∗ = 0. Then, σii = 3λ = 3λ∗ and from λδi j + σi j = λδi j + σi ∗j it follows that σi j = σi ∗j . Note also that the principal directions of σ and σ are coincident.
5.10 Frame Indifference Consider the scenario depicted in Fig. 5.8, i.e., a uniaxial tensile test with σ22 = σ, σi j = 0 otherwise.
(5.81)
For the simple case of linear elasticity, with Young’s modulus E, one is tempted to write ˙ 22 =
1 σ˙ 22 . E
(5.82)
5.10. Frame Indifference
103
σ
σ
e2 e1
σ
Figure 5.8. Rotating body with stress relative to a ﬁxed reference frame.
e3
σ
This relation in rate form, on the surface, looks innocent enough! But, imagine that the rod shown in the ﬁgure were to rotate, with the loading system attached to it as indicated. With respect to a ﬁxed basis such as {e1 , e2 , e3 } the components of σ would change. However, there are clearly no changes in stress state within the body that would cause any additional deformation. Thus a stress rate such as σ˙ would clearly be inappropriate for use in a constitutive law. We introduce the concept of an observer, i.e., a frame of observation. We say that two such frames are equivalent if (a) (b) (c) (d)
they measure the distance between any two arbitrary points to be the same; they measure the orientation between any two vectors to be the same; the time elapsed between any two events is the same; and the relative time between any two events is the same.
Let the two frames be called F and F , respectively. The two frames will satisfy the invariance conditions (a)–(d) above iff the spatialtime coordinates are connected via x = c(t) + Q(t) · x,
t = t − a,
(5.83)
where Q is an orthogonal tensor and a is a scalar constant (Fig. 5.9). Equation (5.83) can be inverted to yield x = QT (t + a)[x − c(t + a)],
t = t + a.
(5.84)
If a scalar ﬁeld φ, a vector ﬁeld u, and a tensor ﬁeld T are to be objective, they must transform according to φ (x , t ) = φ(x, t), u (x , t ) = Q(t) · u(x, t),
(5.85)
T (x , t ) = Q(t) · T(x, t) · QT (t). These transformation rules ensure that the directions of u and T are not altered by the transformation, relative to two rotated frames. To see this consider the two sets of
104
5. Kinetics of Continuum e 2
e1 e' 2
Q( t)
e 3
Figure 5.9. Rotated coordinate frame.
e' 1
e' 3
orthonormal bases, {e1 , e2 , e3 } and {e 1 , e 2 , e 3 }, where the {ei } bases, deﬁned in F, coincide with the {ei } bases deﬁned in F , and where according to (5.85), ei = Q(t) · ei .
(5.86)
Q(t) = e p (t)e p .
(5.87)
Thus,
Now, form the components of u as u (x , t ) · ei = ui (x , t ) = Q(t) · u(x, t) · ei = u(x, t) · QT (t) · ei = u(x, t) · (e p e p ) · ei = u(x, t) · e p δ pi = u(x, t) · ei = ui (x, t). A similar manipulation conﬁrms that Ti j (x , t ) = ei · T (x , t ) · e j = ei · T(x, t) · e j = Ti j (x, t).
(5.88)
Let us next obtain the relations for the velocity υ, acceleration a, the rate of deformation ˙ and the velocity gradient L, under an observer transformation e = Q · ei . As gradient F, i before, x = c(t) + Q · x and t = t − a. In frame F the motion is given as x = Ψ(X, t),
(5.89)
x = c(t + a) + Q(t + a) · Ψ(X, t + a) = Ψ (X, t ).
(5.90)
whereas in frame F
We obtain ∂x ∂Ψ (X, t ) = ∂t ∂t ˙ + a) · Ψ(X, t + a) = c˙ (t + a) + Q(t
υ (x , t ) =
+ Q(t + a) ·
∂Ψ(X, t + a) . ∂t
Since x = c + Q · x, there follows x = QT · (x − c), and ˙ · QT · (x − c). υ (x , t ) = c˙ + Q · υ + Q Furthermore, ∂x /∂X = Q(t + a) · ∂Ψ/∂X = Q · F(X, t) = F ,
(5.91)
5.10. Frame Indifference
105
so that F = Q · F,
(5.92)
˙ ˙ · F(X, t) + Q · F(X, t). F˙ (X, t) = Q(t)
(5.93)
and
For the velocity gradient, we can write ˙ · F · (Q · F)−1 L = F˙ · F −1 = Q · F˙ + Q ˙ · QT . = Q · F˙ · F−1 · QT + Q
(5.94)
Let ˙ · QT . Ω≡Q
(5.95)
Since Q · QT = I ⇒
Q · QT
.
= 0,
we have ˙T=− Q ˙ · QT T , ˙ · QT = −Q · Q Q
(5.96)
˙ · QT is antisymmetric. Furthermore, that is, Q D =
1 L + L T , 2
(5.97)
and D =
1 Q · L · QT + Q · LT · QT + Ω + ΩT . 2
Thus, D = Q · D · QT .
(5.98)
Finally, we show that if a vector u and a tensor T are objective, their socalled convected rates
u = u˙ + LT · u,
(5.99)
T = T˙ + LT · T + T · L.
(5.100)
and
are also objective. In frame F we have
u = u˙ + L T · u = (Q · u)· + Q · LT · QT − Ω · (Q · u) ˙ · QT − Ω · (Q · u) = Q · u˙ + LT · u + Q = Q · u˙ + LT · u = Q · u.
106
5. Kinetics of Continuum
e2 e'1 σ W
e1
Figure 5.10. Components of stress formed on spinning axes.
σ e3
Thus, u, as given by (5.99), is objective. Similarly, for the tensor T,
T = T˙ + L T · T + T · L
= (Q · T · QT )· + (Q · LT · QT − Ω) · (Q · T · QT ) + (Q · T · QT ) · (Q · L · QT + Ω), i.e.,
T = Q · T · QT .
(5.101)
Thus, T, as given by (5.100), is objective. Further results can be obtained by using the polar decomposition theorem, F = R · U. Then, ˙ ·U+R·U ˙ · U−1 · RT L = F˙ · F−1 = R ˙ · RT + R · U ˙ · U−1 · RT =R ˙ · U−1 · RT , Ω = R ˙ · RT . =Ω+R· U
(5.102)
Recall that the spin W is given by W=
1 ˙ · U−1 − U−1 · U ˙ · RT + R ˙ · RT . R· U 2
(5.103)
˙ = 0, then W = R ˙ · RT , i.e., W = Ω. Consequently, L = R ˙ · RT and W = L = R ˙ · RT , If U as well. It follows that
T = T˙ − W · T + T · W
(5.104)
is another objective rate of the tensor T, viz., the Jaumann rate. To better understand the Jaumann rate, consider the stress tensor σ. Its representation in the basis {ei } is σ = σi j ei e j .
(5.105)
5.11. Continuity Equation and Equations of Motion
107
We ask now about the precise character of the base vectors ei that are used to form the components of σ. Let the basis {ei } spin with the rate W (material spin), as sketched in Fig. 5.10. Then, σ˙ = σ˙ i j ei e j + σi j e˙ i e j + σi j ei e˙ j ,
(5.106)
e˙ i = W · ei = Wki ek .
(5.107)
σ˙ = σ˙ i j ei e j + Wikσkj ei e j − σik Wkj ei e j ,
(5.108)
σ˙ = σ˙ i j ei e j + W · σ − σ · W .
(5.109)
and
Consequently,
i.e.,
This leads to deﬁnition of corotational stress rate, observed in the frame that instantaneously rotates with material spin W, σ˙ i j ei e j = σ˙ − W · σ + σ · W.
(5.110)
The stress rate
σ = σ˙ − W · σ + σ · W
(5.111)
is known as the Jaumann stress rate.
5.11 Continuity Equation and Equations of Motion Consider an arbitrary material region that occupies V at time t. Let ρ be its mass density, and as such is a continuous, differentiable, scalar ﬁeld; thus the third equation of (4.223) applies. If diffusion or chemical reactions are neglected, the total mass in this region is conserved during deformation processes that may cause V to change, i.e., d ρ dV = 0. (5.112) dt V When the third equation of (4.223) is applied, this gives (ρ˙ + ρ div υ) dV = 0.
(5.113)
V
Since the region V is arbitrary, we have the continuity equation ρ˙ + ρ div υ = 0, at each point of the body. Using (5.114), we may also show that d ρφ dV = ρ φ˙ dV. dt V V
(5.114)
(5.115)
108
5. Kinetics of Continuum
tn n S
dV
Figure 5.11. The volume V of the body bounded by closed surface S. The body force per unit mass is b and the surface traction over S is tn . The velocity vector at an arbitrary point is v.
v v
dS
b
V
Indeed, d dt
[(ρφ). + ρφ tr L] dV
ρφ dV = V
V
V
ρ φ˙ + (ρ˙ + ρ div υ)φ dV
=
ρ φ˙ dV.
=
(5.116)
V
Let bˆ be the density of body force, measured per unit mass, as opposed to b, introduced earlier which was measured per unit current volume. Then conservation of linear momentum dictates that d ρυ dV = ρ bˆ dV + tn dS, (5.117) dt V V S where S is the bounding surface of the region in question, n is its outward pointing unit normal, and tn = σ · n is the traction vector. Now use (5.115) and the divergence theorem to obtain ˆ dV = 0. ρ υ˙ − (div σ + ρ b) (5.118) V
Because V is arbitrary, we obtain ˆ ρa = ρ υ˙ = ρ x¨ = div σ + ρ b.
(5.119)
These are the equations of motion.
5.12 Stress Power The rate at which external surface and body forces are doing work (the mechanical power input) on a body currently occupying the volume V bounded by the surface S is given by ρbi vi dV , (5.120) P = tin vi dS + S
V
where bi are the components of the body force (per unit mass), and tin are the components of the traction vector over the surface element with unit normal n (Fig. 5.11). Since by the Cauchy relation tin = σi j n j , the surface integral can be expressed, with a help of the Gauss divergence theorem, as ∂ tin vi dS = σi j vi n j dS = (σi j vi ) dV . (5.121) ∂ S S V xj
5.13. The Principle of Virtual Work
109
Thus, the mechanical power input is ∂σi j ∂vi + ρbi vi + σi j P= dV. ∂xj ∂xj V
(5.122)
Since, by the equations of motion, ∂σi j dvi , + ρbi = ρ ∂xj dt the ﬁrst integral in the expression for P becomes dvi 1 d 1 d dV = ρ (vi vi ) dV = ρ (vi vi ) dV . ρvi dt dt dt V 2 V V 2 This is evidently the rate of the kinetic energy 1 ρ (vi vi ) dV , K= V 2 so that the mechanical power input is dK + P= dt
σi j V
∂vi dV. ∂xj
(5.123)
(5.124)
(5.125)
(5.126)
But, the velocity gradient is the sum of the rate of deformation and spin tensors, ∂vi = Li j = Di j + Wi j , ∂xj
(5.127)
and because σi j Wi j = 0 (σi j being a symmetric and Wi j an antisymmetric tensor), we ﬁnally obtain dK + σi j Di j dV. (5.128) P= dt V The second term is the socalled stress power. Thus, the mechanical power input goes into the change of kinetic energy of the body and the stress power associated with the deformation of the body. The quantity σi j Di j is the stress power per unit current volume. The stress power per unit initial volume is τi j Di j , where τi j = (ρ0 /ρ)σi j is the Kirchhoff stress. The stress power per unit mass is (1/ρ)σi j Di j .
5.13 The Principle of Virtual Work Consider a body that is in a state of static equilibrium under the action of a system of body forces b and surface traction Tn ; the unit vector n is again the normal to the body’s surface S. The surface S is taken to be composed of two parts, ST and Su , where on ST traction boundary conditions are imposed and on Su displacement boundary conditions are imposed, as sketched in Fig. 5.12. Note that this assumes that a displacement ﬁeld, u, exists that gives rise to the equilibrium state of stress, such that the stresses satisfy the equations of static equilibrium, viz., ∇ · σ + b = 0. Now let us consider a displacement ﬁeld δu consistent with the constraints imposed on the body. Thus δu must vanish on Su , but is arbitrary on ST . Additionally, we take δu to be continuous and differentiable (as needed) and to be inﬁnitesimal. We assume that this virtual displacement does not affect static
110
5. Kinetics of Continuum
Tn
n
ST Figure 5.12. Virtual displacements atop boundary conditions.
Su equilibrium which continues to prevail during the imposition of δu on u. The increment of work done through these displacements is then δw = b · δu dV + Tn · δu dS, (5.129) V
or, in the component form,
S
δw =
bi · δui dV + V
Ti δui dS.
(5.130)
S
But Tn = σ · n or Ti = σi j n j , and the second integral in (5.129) becomes, via the divergence theorem, Tn · δu dS = (σ · n) · δu dS S
S
(σ · δu) · n dS =
=
S
∇ · (σ · δu) dV V
∇ · σ · δu dV +
=
σ : grad δu dV.
V
(5.131)
V
The equilibrium conditions allow us to write ∇ · σ · δu dV = − b · δu dV. V
(5.132)
V
Deﬁne a small strain measure corresponding to δu as 1 sym (grad δu). 2 Then, because of the symmetry of σ, (5.129) becomes b · δu dV + Tn · δu dS = σ : δe dV, δe =
V
ST
or, in the component form, bi δui dV + V
(5.133)
(5.134)
V
Ti δui dS = ST
σi j δei j dV.
(5.135)
V
This is a principle of virtual work. A similar development in terms of the nominal stress and an increment in δF yields the result P : δF dV0 = B · δu dV0 + δu · P · N dS0 , (5.136) V0
V0
S0
where V0 and S0 are the volume and surface of the body in the reference state.
5.15. Suggested Reading
111
5.14 Generalized Clapeyron’s Formula Let σi j be any statically admissible stress ﬁeld, in equilibrium with body forces bi prescribed within the volume V of the body and surface tractions Ti prescribed over the boundary S of V. Let uˆ i be any continuous and differentiable displacement ﬁeld within V, giving rise to strain ﬁeld eˆi j = (uˆ i, j + uˆ j,i )/2. The notation for partial differentiation is used such that uˆ i, j = ∂ uˆ i /∂ x j . Then, since Ti = σi j n j , where ni deﬁnes the unit outward normal to S, the application of the Gauss divergence theorem gives Ti uˆ i dS = σi j uˆ i n j dS = (σi j uˆ i ), j dV S
S
V
(5.137)
(σi j, j uˆ i + σi j uˆ i, j ) dV .
= V
But, σi j, j = −bi by equilibrium, and σi j uˆ i, j = σi j eˆi j by symmetry of σi j , and the substitution in above establishes a generalized Clapeyron’s formula σi j eˆi j dV = Ti uˆ i dS + bi uˆ i dV . (5.138) V
S
V
This remarkable formula clearly leads to the principle of virtual work. Suppose we take uˆ i to be the difference of any kinematically admissible displacement ﬁeld uik and the true displacement ﬁeld uit of the boundary value problem corresponding to prescribed body forces within V, surface tractions on ST , and displacements on Su = S − ST (if any). A kinematically admissible displacement ﬁeld is continuous and differentiable, and it satisﬁes the prescribed displacement conditions on Su . Call the displacement difference a virtual displacement ﬁeld, i.e., uˆ i = δui = uik − uit .
(5.139)
Clearly, δui = 0 over Su . The generalized Clapeyron’s formula then becomes σi j δei j dV = Ti δui dS + bi δui dV . V
S
(5.140)
V
This is the virtual work principle, previously established in (5.135). If (5.140) holds for any kinematically admissible virtual displacement ﬁeld δui , giving rise to virtual strain ﬁeld δei j by usual relations, then the stress ﬁeld σi j is in equilibrium with given body forces bi in V and surface tractions Ti on ST , i.e., σi j, j + bi = 0 in V,
and
σi j n j = Ti
on ST .
(5.141)
5.15 Suggested Reading Chadwick, P. (1999), Continuum Mechanics: Concise Theory and Problems, Dover, New York. Chung, T. J. (1996), Applied Continuum Mechanics, Cambridge University Press, Cambridge. Eringen, A. C. (1967), Mechanics of Continua, Wiley, New York. Fung, Y.C. (1965), Foundations of Solid Mechanics, Prentice Hall, Englewood Cliffs, New Jersey. Gurtin, M. E. (1981), An Introduction to Continuum Mechanics, Academic Press, New York.
112
5. Kinetics of Continuum
Hill, R. (1978), Aspects of Invariance in Solid Mechanics, Adv. Appl. Mech., Vol. 18, pp. 1–75. Malvern, L. E. (1969), Introduction to the Mechanics of a Continuous Medium, Prentice Hall, Englewood Cliffs, New Jersey. Prager, W. (1961), Introduction of Mechanics of Continua, Ginn and Company, Boston. Sedov, L. I. (1966), Foundations of the NonLinear Mechanics of Continua, Pergamon, Oxford, UK. Spencer, A. J. M. (1992), Continuum Mechanics, Longman Scientiﬁc & Technical, London. Truesdell, C., and Toupin, R. (1960), The Classical Field Theories. In Handbuch der Physik (S. Flugge, ¨ ed.), Band III/l, SpringerVerlag, Berlin. Truesdell, C., and Noll, W. (1965), The Nonlinear Field Theories of Mechanics. In Handbuch der Physik (S. Flugge, ¨ ed.), Band III/3, SpringerVerlag, Berlin (2nd ed., 1992).
6 Thermodynamics of Continuum
6.1 First Law of Thermodynamics: Energy Equation A deforming body, or a given portion of it, can be considered to be a thermodynamic system in continuum mechanics. The ﬁrst law of thermodynamics relates the mechanical work done on the system and the heat transferred into the system to the change in total energy of the system. The rate at which external surface and body forces are doing work on a body currently occupying the volume V bounded by the surface S is given by (5.128), i.e., d 1 ρ vi vi dV + σi j Di j dV. (6.1) P= dt V 2 V Let qi be a vector whose magnitude gives the rate of heat ﬂow by conduction across a unit area normal to qi . The direction of qi is the direction of heat ﬂow, so that in time dt the heat amount qi dt would ﬂow through a unit area normal to qi . If the area dS is oriented so that its normal ni is not in the direction of qi , the rate of outward heat ﬂow through dS is qi ni dS (Fig. 6.1). Let a scalar r be the rate of heat input per unit mass due to distributed internal or external heat sources (e.g., radiation and heating due to dissipation). The total heat input rate into the system is then ∂qi ρ r dV = + ρ r dV. (6.2) − Q = − qi ni dS + ∂ xi S V V First law of thermodynamics states that in any process the total energy of the system is conserved, if no work is done or heat transferred to the system from outside. Alternatively, the whole energy of the universe (system and its surrounding) is conserved. According to the ﬁrst law of thermodynamics there exists a state function of a thermodynamic system, called the total energy of the system Etot , such that its rate of change is E˙tot = P + Q.
(6.3)
Neither P nor Q is in general the rate of any state function, but their sum is. The total energy of the system consists of the macroscopic kinetic energy and the internal energy of the system, 1 ρ vi vi dV + Etot = ρ udV. (6.4) V 2 V 113
114
6. Thermodynamics of Continuum n
o
t fl
hea
ctio ire d w
n q
q dS
dS
Figure 6.1. (a) Heat ﬂow through the surface orthogonal to the direction of the heat ﬂow. (b) The heat ﬂow vector q through the surface element dS with a unit normal n.
The speciﬁc internal energy (internal energy per unit mass) is denoted by u. It includes the elastic strain energy and all other forms of energy that do not contribute to macroscopic kinetic energy (e.g., latent strain energy around dislocations, phasetransition energy, twinning energy, and energy of random thermal motion of atoms). Substituting (6.1), (6.2), and (6.4) into (6.3) and having in mind the general result for a scalar or tensor ﬁeld A, dA d dV, (6.5) ρ AdV = ρ dt V dt V gives ρ u˙ − σi j Di j + V
∂qi − ρ r dV = 0 . ∂ xi
(6.6)
This holds for the whole body and for any part of it, so that locally, at each point, we can write ρ u˙ = σi j Di j −
∂qi +ρr . ∂ xi
(6.7)
This is the energy equation in the deformed conﬁguration.
6.2 Second Law of Thermodynamics: Clausius–Duhem Inequality The ﬁrst law of thermodynamics is a statement of the energy balance, which applies regardless of the direction in which the energy conversion between work and heat is assumed to occur. The second law of thermodynamics imposes restrictions on possible directions of thermodynamic processes. A state function, called the entropy of the system, is introduced as a measure of microstructural disorder of the system. The entropy can change by interaction of the system with its surroundings through the heat transfer, and by irreversible changes that take place inside the system due to local rearrangements of microstructure caused by deformation. The entropy input rate due to heat transfer is r r 1 ∂(qi /T) qi ni dS + ρ dV = + − ρdV, (6.8) − T ρ ∂ xi T S T V V
6.2. Second Law of Thermodynamics
115
where T > 0 is the absolute temperature. The temperature is deﬁned as a measure of the coldness or hotness. It appears in the denominators of the above integrands, because a given heat input causes more disorder (higher entropy change) at lower than at higher temperature (state at lower temperature being less disordered and thus more sensitive to the heat input). An explicit expression for the rate of entropy change caused by irreversible microstructural changes inside the system depends on the type of deformation and constitution of the material. Denote this part of the rate of entropy change (per unit mass) by γ . The total rate of entropy change of the whole system is then ds r 1 ∂(qi /T) dV = (6.9) ρ + + γ ρdV . − dt ρ ∂ xi T V V Locally, at each point of a deformed body, the rate of speciﬁc entropy is s˙ = −
1 ∂(qi /T) r + +γ . ρ ∂ xi T
(6.10)
Because irreversible microstructural changes increase a disorder, they always contribute to an increase of the entropy. Thus, γ is always positive, and is referred to as the entropy production rate. The inequality γ >0
(6.11)
is a statement of the second law of thermodynamics for irreversible processes. Therefore, from (6.10), we can write s˙ ≥ −
1 ∂(qi /T) r + . ρ ∂ xi T
(6.12)
The equality sign applies only to reversible processes (γ = 0). Inequality (6.12) is known as the Clausius–Duhem inequality. Since ∂T 1 ∂qi 1 ∂(qi /T) = − 2 qi , ∂ xi T ∂ xi T ∂ xi
(6.13)
the inequality (6.12) can be rewritten as s˙ ≥ −
1 1 ∂qi ∂T r + + qi . 2 ρ T ∂ xi T ρT ∂ xi
(6.14)
The heat spontaneously ﬂows in the direction from the hot to cold part of the body, so that qi (∂ T/∂ xi ) ≤ 0. Since T > 0, it follows that 1 ∂T qi ≤ 0. ρ T 2 ∂ xi
(6.15)
Thus, a stronger (more restrictive) form of the Clausius–Duhem inequality is s˙ ≥ −
r 1 ∂qi + . ρ T ∂ xi T
(6.16)
Inequality (6.16) can alternatively be adopted if the temperature gradients are negligible or equal to zero. For the Caratheodory’s ´ formulation of the second law of thermodynamics and the resulting expression for the entropy production rate, see Boley and Wiener (1960) and Kestin (1979).
116
6. Thermodynamics of Continuum
6.3 Reversible Thermodynamics If deformation is such that there are no permanent microstructural rearrangements within the material (e.g., thermoelastic deformation), the entropy production rate γ is equal to zero. The rate of entropy change is due to heat transfer only, and T s˙ = −
1 ∂qi + r. ρ ∂ xi
(6.17)
Since 1 1 σi j Di j = Si j E˙ i j , ρ ρ0
(6.18)
the energy equation (6.7) becomes 1 Si j E˙ i j + T s. ˙ ρ0
u˙ =
(6.19)
Equation (6.19) shows that the internal energy is a thermodynamic potential for determining Si j and T, when Ei j and s are considered to be independent state variables. Indeed, by partial differentiation of u = u (Ei j , s) ,
(6.20)
we have ∂u ∂u E˙ i j + s, ˙ ∂ Ei j ∂s
u˙ =
(6.21)
and comparison with (6.19) gives Si j = ρ0
∂u , ∂ Ei j
T=
∂u . ∂s
(6.22)
In the theory of the socalled entropic elasticity, describing thermomechanical behavior of some elastomers, the internal energy depends only on temperature (i.e., there is no change of internal energy due to deformation at constant temperature); see Chadwick (1974) and Holzapfel (2000). 6.3.1 Thermodynamic Potentials The Helmholtz free energy is related to internal energy by φ = u − T s.
(6.23)
By differentiating and incorporating (6.19), the rate of the Helmholtz free energy is φ˙ =
1 ˙ Si j E˙ i j − s T. ρ0
(6.24)
This indicates that φ is the portion of internal energy u available for doing work at constant temperature (T˙ = 0), i.e., the change of φ is the increment of work done at constant T. The Helmholtz free energy is a thermodynamic potential for Si j and s, when Ei j and T are considered to be independent state variables. Indeed, by partial differentiation of φ = φ (Ei j , T) ,
(6.25)
6.3. Reversible Thermodynamics
117
we have φ˙ =
∂φ ∂φ ˙ T, E˙ i j + ∂ Ei j ∂T
(6.26)
and comparison with (6.24) gives Si j = ρ0
∂φ , ∂ Ei j
s=−
∂φ . ∂T
(6.27)
The Gibbs energy is deﬁned as a thermodynamic potential with stress and temperature as independent (controllable) variables, such that g (Si j , T) = φ (Ei j , T) −
1 Si j Ei j . ρ0
(6.28)
By differentiating (6.28) and using (6.24), it follows that g˙ =
∂g ∂g 1 ˙ S˙ i j + T˙ = − Ei j S˙ i j − s T, ∂ Si j ∂T ρ0
(6.29)
so that Ei j = −ρ0
∂g , ∂ Si j
∂g . ∂T
(6.30)
1 Si j Ei j + T s . ρ0
(6.31)
s=−
Note that u (Ei j , s) − g (Si j , T) =
Finally, the enthalpy function is introduced as a thermodynamic potential with stress and entropy as independent variables, such that h (Si j , s) = u (Ei j , s) −
1 Si j Ei j = g (Si j , T) + T s. ρ0
(6.32)
By either (6.19) or (6.29), the rate of change of enthalpy is h˙ =
1 ∂h ∂h S˙ i j + s˙ = − Ei j S˙ i j + T s. ˙ ∂ Si j ∂s ρ0
(6.33)
This demonstrates that the enthalpy is a portion of the internal energy that can be absorbed or released as heat, Tds, when stress Si j is held constant. For example, if we compress the solid adiabatically, it warms up. If we then keep the stress constant, the amount of heat that is conducted and/or convected away is the enthalpy change. Furthermore, (6.33) yields Ei j = −ρ0
∂h , ∂ Si j
T=
∂h . ∂s
(6.34)
The fourthorder tensors iejkl
=
∂ Si j ∂ Ekl
Miejkl
=
∂ Ei j ∂ Skl
= T
∂ 2 (ρ0 φ) , ∂ Ei j ∂ Ekl
(6.35)
∂ 2 (ρ0 g) ∂ Si j ∂ Skl
(6.36)
= T
118
6. Thermodynamics of Continuum
are the isothermal elastic stiffness and compliance tensors. The two fourthorder tensors are the inverse of each other. Being deﬁned as the the second partial derivatives of ρ0 φ and ρ0 g with respect to strain and stress, respectively, the tensors i jkl and Mi jkl possess reciprocal symmetries iejkl = ekli j ,
e Miejkl = Mkli j .
(6.37)
The adiabatic elastic stiffness and compliance tensors are deﬁned be the second derivatives of ρ0 u and ρ0 h with respect to strain and stress, respectively. 6.3.2 Speciﬁc and Latent Heats The ratio of the absorbed amount of heat and the temperature increase is called the heat capacity. Because the increment of heat is not a perfect differential, the speciﬁc heat depends on the path of transformation. The two most important kinds of transformations are those taking place at constant stress (pressure) and constant strain (volume). Speciﬁc heats at constant strain and stress are thus deﬁned by ∂s ∂s , cS = T , (6.38) cE = T ∂T E ∂T S where s = s¯ (Ei j , T) = sˆ (Si j , T) .
(6.39)
The latent heats of change of strain and stress are the secondorder tensors ∂s ∂s E S li j = T li j = T . ∂ Ei j T ∂ Si j T In view of the reciprocal relations ∂ Si j ∂s =− , ρ0 ∂ Ei j T ∂T E
ρ0
the latent heats can also be expressed as ∂ Si j 1 , liEj = − T ρ0 ∂T E
∂s ∂ Si j
liSj =
=− T
1 T ρ0
∂ Ei j ∂T
∂ Ei j ∂T
,
∂s ∂ Si j
dSi j + T
∂s ∂T
dT = S
(6.41)
S
.
(6.42)
S
The physical interpretation of the speciﬁc and latent heats follows from ∂s ∂s 1 E l dEi j + c E dT , ds = dEi j + dT = ∂ Ei j T ∂T E T ij ds =
(6.40)
1 S li j dSi j + c S dT . T
(6.43)
(6.44)
Thus, the speciﬁc heat at constant strain c E (often denoted by cv ) is the heat amount (T ds) required to increase the temperature of a unit mass for the amount dT at constant strain (dEi j = 0). Similar interpretation holds for c S (often denoted by c p ). The latent heat liEj is the secondorder tensor whose i j component represents the heat amount associated with a change of the corresponding strain component by dEi j , at ﬁxed temperature and ﬁxed values of the remaining ﬁve strain components. Analogous interpretation applies to liSj .
6.3. Reversible Thermodynamics
119
By partial differentiation, we have from (6.39) ∂ s¯ ∂ s¯ ∂ Ei j ∂ sˆ = + . ∂T ∂T ∂ Ei j ∂ T The multiplication by T and incorporation of (6.38)–(6.42) gives the relationship ρ0 S E l l . cS − c E = T ij ij Furthermore, since ∂ sˆ ∂ s¯ = Me , ∂ Si j ∂ Ekl i jkl
(6.45)
(6.46)
(6.47)
it follows that liSj = Miejkl lklE .
(6.48)
When this is inserted into (6.46), we obtain ρ0 e E E M l l . T i jkl i j kl For positive deﬁnite elastic compliance Miejkl , it follows that cS − c E =
cS > c E.
(6.49)
(6.50)
The change in temperature caused by adiabatic straining dEi j , or adiabatic stressing dSi j , is obtained by setting ds = 0 in (6.43) and (6.44). This gives dT = −
1 E l dEi j , cE i j
dT = −
1 S l dSi j . cS i j
(6.51)
6.3.3 Coupled Heat Equation Suppose that the heat conduction is speciﬁed by a generalized Fourier law qi = −Ki j
∂T , ∂xj
Ki j = K ji .
(6.52)
If the inequality applies in (6.15), the secondorder tensor of conductivities Ki j must be positivedeﬁnite, i.e., ∂T ∂T Ki j > 0. ∂ xi ∂xj
(6.53)
For simplicity it is assumed that Ki j is a constant tensor, although it could more generally depend on temperature and deformation. The nominal rate of heat ﬂow is qi0 = −Ki0j
∂T , ∂ Xj
−1 Ki0j = (det F) Fim Kmn Fnj−T ,
(6.54)
qi0 = (det F)Fi−1 j qj ,
(6.55)
which follows from qi0 ni0 dS0 = qi ni dS
⇒
and (6.52). Since 1 ∂qi 1 ∂qi0 = 0 , ρ ∂ xi ρ ∂ Xi
(6.56)
120
6. Thermodynamics of Continuum
we obtain from (6.17) T s˙ =
1 0 ∂2T K +r . ρ 0 i j ∂ Xi ∂ Xj
(6.57)
Combining this with (6.43) yields the heat equation 1 0 ∂2T ˙ K + r = liEj E˙ i j + c E T, ρ 0 i j ∂ Xi ∂ Xj
(6.58)
where liEj = T
∂ Si j ∂ 2φ ∂ s¯ 1 = −T , =− 0T ∂ Ei j ρ ∂T ∂ Ei j ∂ T
(6.59)
∂ 2φ ∂ s¯ = −T . ∂T ∂ T2
(6.60)
cE = T
Since (6.58) involves the rates of both temperature and strain, it is referred to as a coupled heat equation. The temperature and deformation ﬁelds cannot be determined separately, but simultaneously.
6.4 Thermodynamic Relationships with p, V, T, and s In many thermodynamic considerations in materials science it is the pressure and volume that, together with temperature and entropy, appear in the analysis. We thus list in this section the corresponding thermodynamic expressions, reckoned per one mole of the substance (i.e., ρ0 V0 is the mass of one mole). The energy equation is du = − pdV + Tds . Taking u = u(V, s), we obtain
p=−
∂u ∂V
, s
T=
∂u ∂s
(6.61) .
(6.62)
V
The Helmholtz free energy is φ = φ(V, T) = u(V, s) − Ts, which gives dφ = − pdV − sdT , and
∂φ p=− ∂V
, T
∂φ s=− ∂T
(6.63) .
(6.64)
V
The Gibbs energy is g = g( p, T) = φ(V, T) + pV, and dg = Vd p − sdT ,
(6.65)
indicating that s determines how fast g varies with T, and V how fast g varies with p. Furthermore, ∂g ∂g V= , s=− . (6.66) ∂p T ∂T p
6.4. Thermodynamic Relations with p, V, T, and s
121
Finally, the enthalpy is h = h( p, s) = u(V, s) + pV, which gives dh = Vd p + Tds , and
V=
∂h ∂p
,
T=
(6.67)
∂h ∂s
.
(6.68)
u = φ − g + h.
(6.69)
s
p
It is noted that g = h − Ts , The Maxwell relations are ∂p ∂s = , ∂T V ∂V T and
∂V ∂T
=− p
∂s ∂p
∂p ∂s
, T
V
∂V ∂s
∂T =− ∂V
= p
∂T ∂p
,
(6.70)
.
(6.71)
s
s
It may be noted that at constant V, dφ = −sdT ,
du = Tds ,
(6.72)
dg = −sdT ,
dh = Tds .
(6.73)
whereas at constant p,
A physicist by “free energy” usually means the Helmholtz free energy, whereas a chemist usually means Gibbs free energy (because they study their reactions at constant p or T). 6.4.1 Speciﬁc and Latent Heats The speciﬁc heats at constant volume and pressure are deﬁned by ∂s ∂s , cp = T . cv = T ∂T V ∂T p Similarly, the latent heats are deﬁned by ∂s , lv = T ∂V T Since s = s(V, T), we have
ds =
∂s ∂V
lp = T
dV + T
∂s ∂p
∂s ∂T
(6.74)
.
(6.75)
T
dT ,
(6.76)
V
and, upon multiplication with T, Tds = lv dV + cv dT .
(6.77)
In particular, at V = const., we have du = Tds = cv dT. On the other hand, by writing s = s( p, T), we obtain ∂s ∂s dp + dT (6.78) ds = ∂p T ∂T p
122
6. Thermodynamics of Continuum
and, upon multiplication with T, Tds = l p d p + c p dT .
(6.79)
In particular, at p = const., we have dh = Tds = c p dT. The relationship between c p and cv can be derived by partial differentiation of s = s[V( p, t), T], as follows ∂s ∂V ∂s ∂s = + . (6.80) ∂T p ∂V T ∂T p ∂T V The multiplication with T establishes c p = lv
∂V ∂T
+ cv .
(6.81)
p
Similarly, the relationship between l p and lv can be derived by partial differentiation of s = s[ p(V, t), T], 2 ∂s ∂s ∂p ∂ φ ∂s = =− . (6.82) ∂V T ∂p T ∂V T ∂ p T ∂ V2 T The last transition is made by using the relationship p = −(∂φ/∂ V)T . The multiplication with T then establishes 2 ∂ φ lp . (6.83) lv = − ∂ V2 T 6.4.2 Coefﬁcients of Thermal Expansion and Compressibility Coefﬁcient of volumetric thermal expansion and compressibility coefﬁcient are deﬁned by 1 ∂V 1 ∂V , β=− . (6.84) α= V ∂T p V ∂p T In view of one of the Maxwell relations, we also have 1 ∂V 1 ∂s α= =− . V ∂T p V ∂p T
(6.85)
The coefﬁcient of linear thermal expansion is α/3, whereas the modulus of compressibility is κ = 1/β. The coefﬁcients α and β appear in the expression for the increment of volumetric strain dV = αdT − βd p . (6.86) V This follows from the above deﬁnitions of α and β, and ∂V ∂V V = V(T, p) ⇒ dV = dT + dp. (6.87) ∂T p ∂p T An important relation for the pressure gradient of enthalpy at constant temperature can be derived by partial differentiation of h = h[ p, s( p, T)]. This gives ∂h ∂h ∂s ∂s ∂h = + =V+T , (6.88) ∂p T ∂p s ∂s p ∂ p T ∂p T
6.5. Theoretical Calculations of Heat Capacity
i.e.,
∂h ∂p
123
= V(1 − αT) .
(6.89)
T
To establish additional useful relationships involving speciﬁc heats and coefﬁcient of thermal expansion, we ﬁrst recall the following result from calculus. If z = z(x, y), then ∂z ∂x ∂y = −1 . (6.90) ∂ x y ∂ y z ∂z x Applying this to variables (T, V, p), we have ∂p ∂T ∂V = −1 . ∂T V ∂V p ∂p T
(6.91)
In view of the deﬁnitions (6.84) for α and β, this gives ∂p α = , ∂T V β
(6.92)
or, recalling the Maxwell relation (∂ p/∂ T)V = (∂s/∂ V)T , ∂s α = . ∂V T β Now, from (6.81) and (6.84), c p − cv =
∂V ∂T
(6.93)
lv = αVlv = αVT p
∂s ∂V
,
(6.94)
T
and, in view of (6.93), c p − cv =
α2 VT . β
Finally, we derive a useful expression for the entropy change. Since ∂s ∂V = −T = −TαV , lp = T ∂p T ∂T p
(6.95)
(6.96)
we obtain, from (6.79), ds = −αVd p + c p
dT . T
(6.97)
6.5 Theoretical Calculations of Heat Capacity In this section we give a brief summary of theoretical calculations of heat capacity cv from solidstate physics. We start with a monatomic gas. Each atom has three degrees of freedom, so that the mean kinetic energy of an atom is 3 · 12 kT, where k = 1.38062 × 10−23 J/K is the Boltzmann constant. Thus, the molar heat capacity cv of a monatomic gas is cv = 3R/2, where R = NAk = 8.314 J/K is the universal gas constant, NA = 6.02217 × 1023 mol−1 being the Avogadro’s number. For diatomic molecule there are additional energy contributions, one vibrational along the axis joining two atoms, and two rotational around the axes normal to common axis. Each translational and rotational degree
124
6. Thermodynamics of Continuum
Figure 6.2. Speciﬁc heat cv (J/mol K) of a solid as a function of temperature T (normalized by the Debye’s temperature θD ).
of freedom contributes on average an energy equal to 12 kT per molecule (principle of equipartition of energy among the active degrees of freedom). This gives a theoretical value cv = 5R/2. At higher temperature, one needs to include the vibrational (kinetic and potential) energy contributions and quantum mechanics effects. If this is done, it is found that " # 2 θ eθ/T hν 5 + . (6.98) , θ= cv = R 2 θ/T 2 T k − 1) (e The Planck’s constant is h = 6.62620 × 10−34 J s, and ν is a characteristic vibrational frequency of the Einstein harmonic oscillator. The corresponding result for a solid is cv = 3R
2 θ eθ/T . T (eθ/T − 1)2
(6.99)
At high temperature this gives a Dulong–Petit limit lim cv = 3R .
θ/T→0
(6.100)
The expression (6.99) is not satisfactory at low temperature, where it predicts an exponential decrease of cv with temperature, whereas a dependence on T 3 is generally observed. This is accomplished by Debye’s expression " # 3θD /T θD −3 θD /T x 3 dx − cv = 3R 12 , (6.101) T e x − 1 eθD /T − 1 0 where θD is the Debye’s temperature of a solid (the temperature of a crystal’s highest mode of vibration). The values of θD are tabulated; for example, θDCu = 343 K, whereas θDAl = 428 K. The plot of cv /R vs. T/θD for a typical solid is shown in Fig. 6.2. For many solids for which the room temperature is greater than θD , the Dulong–Petit limit cv = 3R is practically attained already at 298 K.
6.6. Third Law of Thermodynamics
125 Cp
7
(cal /°K mol)
Cp, Cv
6
Cv
5 4 3 2 1 0
0
200
400 T (°K)
600
800
1000
Figure 6.3. Speciﬁc heats c p and cv of copper vs. temperature T (from Lupis, 1983).
If the coefﬁcients of thermal expansion and compressibility are experimentally determined, then the plot for c p vs. temperature can be obtained from that for cv and the relationship c p − cv = (α 2 /β)VT. Typically, one obtains a plot as sketched in Fig. 6.3. Knowing the variation c p (T) is important to determine the entropy change associated with the change of temperature (at constant pressure). Since, at constant pressure, Tds = c p dT, we obtain s − s0 =
T
c p (T)dT .
(6.102)
T0
In a certain temperature range, the approximation c p (T) = a + bT + cT −2 may be satisfactory. The coefﬁcients a, b, and c are also tabulated for various materials and temperature ranges. For most metals, the entropy increases because of phase transformations (melting and boiling) are J K mol J sb0 ≈ 92 K mol
0 = 8.3 ÷ 12.6 sm
(Richard s rule), (6.103)
(Trouton s rule).
The superscript 0 indicates that the values are given at standard pressure of 1 atm. Better estimates of sm are possible by including into considerations the crystallographic structure of solid phase. Usually, 0 0 0 0 (h.c.p.) − sm (f.c.c.) = sm (f.c.c.) − sm (b.c.c.) ≈ 1 sm
J . K mol
6.6 Third Law of Thermodynamics It is ﬁrst assumed that there is a lower limit of temperature that the matter can exhibit. This is called the absolute zero of temperature. Now, if the entropy of each element in its perfect crystalline state (without vacancies, dislocations, or any disorder) is taken to be zero at the absolute zero of temperature, every substance composed of elements has
126
6. Thermodynamics of Continuum
a ﬁnite positive entropy, unless it is a perfect crystalline substance. All perfect substances have zero entropy at T = 0 K. This is the third law of thermodynamics. This law simpliﬁes the calculation of entropies. For example, if perfect iron and perfect carbon have zero entropies at 0 K, then the entropy of perfect cementite Fe3 C is also zero at 0 K. If we do not adopt the third law, we could take that the entropy of perfect iron is, say, 8 J/K mol , and of carbon 4 J/K mol, but then the entropy of the perfect cementite would be 28 J/K mol. Note also that, if we take that s = 0 at T = 0, then from dg = dh − Tds − sdT we obtain that at the absolute zero of temperature dg = dh. Furthermore, from statistical thermodynamics, we have s = k ln wmax , where wmax is the probability of the state with maximum number of quantum states (under given conditions of energy, volume, etc.). At the absolute zero of temperature, there would be a perfect order and only one state. Thus, wmax = 1 and s = 0. With the adopted third law, in a test at constant pressure the entropy of a perfect substance at the temperature T can be calculated from T cp dT . (6.104) s= T 0 Clearly, the ratio c p /T must remain ﬁnite as T → 0 K. Similarly, in a test at constant volume (leading to another state from that obtained in a test at constant pressure), the entropy of a perfect substance at the temperature T would be T cv dT . (6.105) s= 0 T The integrand is clearly not divergent at T = 0 K, because cv ∼ T 3 near the absolute zero of temperature. The entropy of a perfect substance at T = 0 K is equal to zero regardless of the pressure or volume there. Thus, ∂s = 0, (6.106) ∂ p T=0 and since, by the Maxwell’s relation and the deﬁnition of the coefﬁcient of thermal expansion, ∂V ∂s =− = −αV , (6.107) ∂p T ∂T p we conclude that (α)T=0 = 0 . Furthermore, since
and
∂s ∂V
∂s ∂V
= 0,
(6.109)
T=0
= T
(6.108)
∂p ∂T
= V
α , β
(6.110)
6.7. Irreversible Thermodynamics
127
we conclude that (β)T=0 = 0 ,
(κ)T=0 = ∞ .
i.e.,
(6.111)
The modulus of compressibility is κ = 1/β.
6.7 Irreversible Thermodynamics For irreversible thermodynamic processes (e.g., processes involving plastic or viscoelastic deformation) we can adopt a thermodynamics with internal state variables. A set of internal (structural) variables is introduced to describe, in some average sense, the essential features of microstructural changes that occurred at the considered place during the deformation process. These variables are denoted by ξ j ( j = 1, 2, . . . , n). For simplicity, they are assumed to be scalars (extension to include tensorial internal variables is straightforward). Inelastic deformation is considered to be a sequence of constrained equilibrium states. These states are created by a conceptual constraining of internal variables at their current values through imposed thermodynamic forces f j . The thermodynamic forces or constraints are deﬁned such that the power dissipation (temperature times the entropy production rate) due to structural rearrangements can be expressed as T γ = f j ξ˙ j .
(6.112)
The rates of internal variables ξ˙ j are called the ﬂuxes, and the forces f j are their afﬁnities. By the second law, γ > 0, and therefore f j ξ˙ j > 0. If various equilibrium states are considered, each corresponding to the same set of values of internal variables ξ j , the neighboring states are related by the usual laws of reversible thermodynamics (thermoelasticity), such as (6.17) and (6.19). If neighboring constrained equilibrium states correspond to different values of internal variables, then T s˙ = −
1 ∂qi + r + f j ξ˙ j . ρ ∂ xi
(6.113)
Combining this with the energy equation gives u˙ =
1 Si j E˙ i j + T s˙ − f j ξ˙ j . ρ0
(6.114)
Thus, the internal energy is a thermodynamic potential for determining Si j , T and f j , when Ei j , s and ξ j are considered to be independent state variables. Indeed, after partial differentiation of u = u (Ei j , s, ξ j ) ,
(6.115)
the comparison with (6.114) gives Si j = ρ0
∂u , ∂ Ei j
T=
∂u , ∂s
fj = −
∂u . ∂ξ j
(6.116)
The Helmholtz free energy φ = φ (Ei j , T, ξ j ) = u (Ei j , s, ξ j ) − Ts
(6.117)
128
6. Thermodynamics of Continuum
is a thermodynamic potential for determining Si j , s and f j , such that Si j = ρ0
∂φ , ∂ Ei j
s=−
∂φ , ∂T
fj = −
∂φ . ∂ξ j
(6.118)
This clearly follows because φ˙ =
1 Si j E˙ i j − s T˙ − f j ξ˙ j . ρ0
(6.119)
If the Gibbs energy g = g (Si j , T, ξ j ) = φ (Ei j , T, ξ j ) −
1 Si j Ei j ρ0
(6.120)
∂g . ∂ξ j
(6.121)
is used, we have Ei j = −ρ0
∂g , ∂ Si j
s=−
∂g , ∂T
fj = −
This follows because g˙ = −
1 Ei j S˙ i j − s T˙ − f j ξ˙ j . ρ0
(6.122)
It is noted that in (6.118) fk = f¯k (Ei j , T, ξ j ) ,
(6.123)
fk = fˆk (Si j , T, ξ j ) ,
(6.124)
whereas in (6.121)
indicating different functional dependences of the respective arguments. Finally, with the enthalpy h = h (Si j , s, ξ j ) = u (Ei j , s, ξ j ) −
1 Si j Ei j ρ0
(6.125)
∂h , ∂ξ j
(6.126)
as a thermodynamic potential, it is found that Ei j = −ρ0
∂h , ∂ Si j
T=
∂h , ∂s
fj = −
because h˙ = −
1 Ei j S˙ i j + T s˙ − f j ξ˙ j . ρ0
(6.127)
By taking appropriate crossderivatives of the previous expressions, we establish the Maxwell relations. For example, ∂ sˆ (Si j , T, ξ j ) ∂ Ekl (Si j , T, ξ j ) = ρ0 , ∂T ∂ Skl ∂ s¯ (Ei j , T, ξ j ) ∂ Skl (Ei j , T, ξ j ) = −ρ0 , ∂T ∂ Ekl
(6.128)
6.8. Gibbs Conditions of Thermodynamic Equilibrium
129
and ∂ fˆm (Si j , T, ξ j ) ∂ Ekl (Si j , T, ξ j ) = ρ0 , ∂ξm ∂ Skl ∂ Skl (Ei j , T, ξ j ) ∂ f¯m (Ei j , T, ξ j ) = −ρ0 . ∂ξm ∂ Ekl
(6.129)
6.7.1 Evolution of Internal Variables The selection of appropriate internal variables is a difﬁcult task, which depends on the material constitution and the type of deformation. Once internal variables are selected, it is necessary to construct evolution equations that govern their change during the deformation. For example, if the ﬂuxes are assumed to be linearly dependent on the afﬁnities, we may write ξ˙i = i j f j .
(6.130)
The coefﬁcients i j obey the Onsager reciprocity relations if i j = ji . For some materials and for some range of deformation, it may be appropriate to assume that at a given temperature T and given pattern of internal rearrangements ξ j , each ﬂux depends only on its own afﬁnity, i.e., ξ˙i = function ( fi , T, ξ j ) .
(6.131)
The ﬂux dependence on the stress Si j comes only through the fact that fi = fˆi (Skl , T, ξk). This type of evolution equation is often adopted in metal plasticity, where it is assumed that the crystallographic slip on each slip system is governed by the resolved shear stress on that system (or, at the dislocation level, the motion of each dislocation segment is governed by the local Peach–Koehler force on that segment).
6.8 Gibbs Conditions of Thermodynamic Equilibrium The system is in a thermodynamic equilibrium if its state variables do not spontaneously change with time. Theorem 1: In an isolated system, the equilibrium state is the state that has the maximum value of entropy. This is a direct consequence of the second law of thermodynamics. The increment of entropy is due to irreversible processes within the system, and its interaction with the surrounding, ds = ds irr + ds surr . By second law, ds irr > 0. Thus, for an isolated system (ds surr = 0), we must have ds > 0 ,
(6.132)
i.e., the entropy of an isolated system can only increase during a thermodynamic process. If the process comes to equilibrium, the entropy is greater than the entropy in any nearby nonequilibrium state. This, for example, indicates that the entropy of the whole universe (which is an isolated system) always increases.
130
6. Thermodynamics of Continuum
Theorem 2: At constant stress and temperature, the direction of a spontaneous change of the thermodynamic state is in the direction of decreasing Gibbs energy. This clearly follows from (6.122), which, at constant stress and temperature, reduces to g˙ = − f j ξ˙ j < 0 .
(6.133)
The inequality follows from the second law, requiring f j ξ˙ j > 0. Thus, a transformation from the thermodynamic state can occur at constant stress and temerature only if it is associated with a decrease of the Gibbs energy. Because there is no spontaneous change from the equilibrium state, the Gibbs energy is minimum at the equilibrium state (relative to all neighboring states at constant stress and temperature). Gibbs originally formulated his celebrated thermodynamic equilibrium condition as: Any virtual variation from the equilibrium state at constant pressure and temperature which does not involve irreversible processes would give δg ≥ 0; if the variation involves irreversible changes, then δg < 0. If the substance can be in either a or b phase (structure), at given pressure and temperature, a stable equilibrium phase is one that corresponds to lower Gibbs energy. Theorem 3: Among all neighboring states with the same strain and entropy, the equilibrium state is one with the lowest internal energy. This follows from (6.114), which, at constant strain and temperature, reduces to u˙ = − f j ξ˙ j < 0 .
(6.134)
Thus, when the system undergoing a thermodynamic process at constant strain and entropy comes to rest at its equilibrium, its internal energy attains its minimum. (It is hard to control entropy in the experiment; conceptually one would need to extract the heat from the internal dissipation, such that ds = 0). Theorem 4: Among all neighboring states with the same strain and temperature, the equilibrium state is one with the lowest Helmholtz free energy. This follows from (6.119), which, at constant strain and temperature, reduces to φ˙ = − f j ξ˙ j < 0 .
(6.135)
Theorem 5: Among all neighboring states with the same stress and temperature, the equilibrium state is one with the lowest enthalpy. This follows from (6.127), which, at constant strain and temperature, reduces to h˙ = − f j ξ˙ j < 0 .
(6.136)
6.9 Linear Thermoelasticity The structure of the constitutive equations relating the stress, strain, entropy and temperature in linear thermoelasticity is readily derived by assuming a quadratic representation of the Helmholtz free energy in terms of strain and temperature. The material parameters are speciﬁed in the accordance with observed isothermal elastic behavior and
6.9. Linear Thermoelasticity
131
measured coefﬁcients of thermal expansion and the speciﬁc heat. For isotropic materials, this yields φ(ei j , T) =
1 2 λT ekk + µei j ei j − κT α0 (T − T0 )ekk 2 c0 − V (T − T0 )2 − s0 (T − T0 ) + f0 , 2T0
(6.137)
where λT and µ are the isothermal Lame´ elastic constants, κT = λT + 2µ/3 is the isothermal 0 , and s0 are, respectively, the coefﬁcient of volumetric thermal bulk modulus, and α0 , cV expansion, the speciﬁc heat at constant strain, and the speciﬁc entropy (per unit volume), all in the reference state with temperature T0 . The inﬁnitesimal strain is ei j . The corresponding free energy (per unit volume) is φ(0, T0 ) = φ0 . The stress and entropy in the deformed state are the gradients of f with respect to strain and temperature, which gives ∂φ = λT ekkδi j + 2µei j − κT α0 (T − T0 )δi j , (6.138) σi j = ∂ei j T
∂φ s=− ∂T
= κT α0 ekk + e
0 cV (T − T0 ) + s0 . T0
(6.139)
The speciﬁc heat at constant strain, associated with (6.137) is cV = T
∂s ∂T
= −T e
∂ 2φ ∂ T2
0 = cV e
T . T0
(6.140)
Once the Helmholtz free energy is speciﬁed as a function of strain and temperature, the internal energy u = φ + Ts can be expressed in terms of the same independent variables by simple substitution of (6.137) and the corresponding expression for the entropy. This yields u(ei j , T) =
c0 1 2 λT ekk + µei j ei j + κT α0 T0 ekk + V (T 2 − T02 ) + u0 . 2 2T0
(6.141)
In the sequel, it will be assumed that the internal energy vanishes in the reference state, so that u0 = 0 ,
φ0 = −T0 s0 .
(6.142)
However, the internal energy is a thermodynamic potential whose natural independent state variables are strain and entropy, rather than strain and temperature. The desired representation u = u(ei j , s) can be obtained from u = φ + Ts by eliminating the temperature in terms of strain and entropy. The purely algebraic transition is simple, but little indicative of the underlying thermodynamics. An independent derivation, starting from the energy equation and utilizing the experimental data embedded in the Duhamel–Neumann extension of Hooke’s law and the assumed speciﬁc heat behavior, is desirable. The systematic procedure to achieve this, and to derive the expressions for other thermodynamic potentials, is presented in next section.
132
6. Thermodynamics of Continuum
6.10 Thermodynamic Potentials in Linear Thermoelasticity The four thermodynamic potentials are derived in this section in terms of their natural independent state variables. The derivation is in each case based only on the Duhamel– Neumann extension of Hooke’s law, and an assumed linear dependence of the speciﬁc heat on temperature. 6.10.1 Internal Energy The increment of internal energy is expressed in terms of the increments of strain and entropy by the energy equation du = σi j dei j + Tds .
(6.143)
Because u is a state function, du is a perfect differential, and the Maxwell relation holds ∂σi j ∂T = . (6.144) ∂s e ∂ei j s The thermodynamic potential u = u(ei j , s) is sought corresponding to the Duhamel– Neumann expression σi j = λT ekkδi j + 2µei j − κT α0 (T − T0 )δi j ,
(6.145)
and an assumed linear dependence of the speciﬁc heat on temperature 0 cV = cV
T . T0
By partial differentiation from (6.145) it follows that ∂σi j ∂σi j ∂T ∂T = = −κT α0 δi j , ∂s e ∂ T e ∂s e ∂s e so that the Maxwell relation (6.144) gives ∂T ∂T = −κT α0 δi j . ∂ei j s ∂s e The thermodynamic deﬁnition of the speciﬁc heat at constant strain is ∂s cV = T , ∂T e which, in conjunction with (6.146), speciﬁes the temperature gradient T0 ∂T = 0 . ∂s e cV The substitution into (6.148) yields ∂T κT α0 T0 =− δi j . 0 ∂ei j s cV
(6.146)
(6.147)
(6.148)
(6.149)
(6.150)
(6.151)
The joint integration of the above two equations provides the temperature expression T=−
κT α0 T0 T0 ekk + 0 (s − s0 ) + T0 . 0 cV cV
(6.152)
6.10. Thermodynamic Potentials in Thermoelasticity
133
When this is inserted into (6.145), we obtain an expression for the stress in terms of the strain and entropy, σi j = λ S ekkδi j + 2µei j −
κT α0 T0 (s − s0 )δi j . 0 cV
(6.153)
The adiabatic (isentropic) Lame´ constant λ S is related to its isothermal counterpart λT by λ S = λT +
α02 T0 2 κT . 0 cV
(6.154)
By using (6.152) and (6.153), the joint integration of ∂u ∂u , T= , σi j = ∂ei j s ∂s e
(6.155)
yields a desired expression for the internal energy in terms of its natural independent variables ei j and s. This is 1 κT α0 T0 2 λ S ekk + µei j ei j − (s − s0 )ekk 0 2 cV
u(ei j , s) =
+
T0 (s − s0 )2 + T0 (s − s0 ) . 0 2cV
(6.156)
6.10.2 Helmholtz Free Energy An independent derivation of the Helmholtz free energy φ = φ(ei j , T) again begins with the pair of expressions (6.145) and (6.146). The increment of φ is dφ = σi j dei j − sdT , with the Maxwell relation
∂σi j ∂T
=− e
∂s ∂ei j
(6.157)
.
(6.158)
T
By evaluating the temperature gradient of stress from (6.145), and by substituting the result into (6.158), we ﬁnd ∂s = κT α0 δi j . (6.159) ∂ei j T The integration of above, in conjunction with c0 ∂s = V, ∂T e T0
(6.160)
provides the entropy expression s = κT α0 ekk +
0 cV (T − T0 ) + s0 . T0
By using (6.145) and (6.161), the joint integration of ∂φ ∂φ , s=− , σi j = ∂ei j T ∂T e
(6.161)
(6.162)
134
6. Thermodynamics of Continuum
yields a desired expression for the Helmholtz free energy in terms of its natural independent variables ei j and T. This is 1 2 λT ekk + µei j ei j − κT α0 (T − T0 )ekk 2
φ(ei j , T) =
c0 − V (T − T0 )2 − s0 T . 2T0
(6.163)
6.10.3 Gibbs Energy The increment of the Gibbs energy is dg = −ei j dσi j − sdT , with the Maxwell relation
∂ei j ∂T
σ
=
∂s ∂σi j
(6.164)
.
(6.165)
T
To derive the function g(σi j , T), independently of the connection g = φ − σi j ei j and without tedious change of variables, we begin with the thermoelastic stressstrain relation and the expression for the speciﬁc heat, α0 1 νT (T − T0 )δi j , σi j − σkkδi j + (6.166) ei j = 2µ 1 + νT 3 c P (T) = c0P
T . T0
(6.167)
The ﬁrst one is a simple extension of Hooke’s law to include thermal strain, and the second one is the assumed linear dependence of the speciﬁc heat at constant stress on temperature. The thermodynamic deﬁnition of the speciﬁc heat c P is ∂s . (6.168) cP = T ∂T σ By differentiating (6.166) to evaluate the temperature gradient of strain, and by substituting the result into the Maxwell relation (6.165), we ﬁnd α0 ∂s δi j . = (6.169) ∂σi j T 3 The integration of this, in conjunction with ∂s c0 = P, ∂T σ T0
(6.170)
provides the entropy expression s=
α0 c0 σkk + P (T − T0 ) + s0 . 3 T0
Using (6.166) and (6.171), the joint integration of ∂g ∂g , s=− , ei j = − ∂σi j T ∂T σ
(6.171)
(6.172)
6.10. Thermodynamic Potentials in Thermoelasticity
135
yields a desired expression for the Gibbs energy in terms of its natural independent variables σi j and T. This is 1 νT α0 2 (T − T0 )σkk σ g(σi j , T) = − − σi j σi j − 4µ 1 + νT kk 3 (6.173) c0P 2 − (T − T0 ) − s0 T . 2T0 0 The relationship between the speciﬁc heats c0P and cV can be obtained in various ways. For example, by reconciling the entropy expressions (6.161) and (6.171), and by using the relationship
ekk =
1 σkk + α0 (T − T0 ) , 3κT
(6.174)
following from (6.164), it is found that 0 c0P − cV = κT α02 T0 .
(6.175)
dh = −ei j dσi j + Tds ,
(6.176)
6.10.4 Enthalpy Function The increment of enthalpy is
with the Maxwell relation
∂ei j ∂s
σ
∂T =− ∂σi j
.
(6.177)
s
To derive the function h(σi j , s), we again begin with the expressions (6.166) and (6.167). By partial differentiation from (6.166) it follows that ∂ei j ∂ei j ∂T α0 ∂ T = = δi j . (6.178) ∂s σ ∂ T σ ∂s σ 3 ∂s σ The substitution into the Maxwell relation (6.177) gives ∂T α0 ∂ T α0 T0 =− δi j = − 0 δi j . ∂σi j s 3 ∂s σ 3c P
(6.179)
The deﬁnition (6.168), in conjunction with (6.167), was used in the last step. The joint integration of the above equation and ∂T T0 = 0 , (6.180) ∂s σ cP provides the temperature expression T=−
T0 α0 T0 σkk + 0 (s − s0 ) + T0 . 0 3c P cP
When this is substituted into (6.166), there follows 1 νS α0 T0 ei j = σkkδi j + 0 (s − s0 )δi j . σi j − 2µ 1 + νS 3c P
(6.181)
(6.182)
136
6. Thermodynamics of Continuum
The adiabatic Poisson’s ratio ν S is related to its isothermal counterpart νT by νS =
νT + 2µ(1 + νT )a , 1 − 2µ(1 + νT )a
νT =
ν S − 2µ(1 + ν S )a , 1 + 2µ(1 + ν S )a
(6.183)
where a=
α02 T0 . 9c0P
(6.184)
The adiabatic and isothermal Young’s moduli are related by α 2 T0 1 1 − = 00 . ET ES 9c P
(6.185)
A simple relationship is also recorded κS c0P = . 0 κT cV
(6.186)
This easily follows by noting, from (6.152) and (6.181), that for adiabatic loading T0 − T =
κT α0 T0 α0 T0 ekk = σkk . 0 cV 3c0P
(6.187)
Since for adiabatic loading σkk = 3κ S ekk, the substitution into (6.187) yields (6.186). Returning to the enthalpy function, by using (6.181) and (6.182), the joint integration of ∂h ∂h , T= , (6.188) ei j = − ∂σi j s ∂s σ yields the expression for the enthalpy in terms of its natural independent variables σi j and s. This is 1 νS α0 T0 2 σ h(σi j , s) = − − 0 (s − s0 )σkk σi j σi j − 4µ 1 + ν S kk 3c P (6.189) T0 + 0 (s − s0 )2 + T0 (s − s0 ) . 2c P
6.11 Uniaxial Loading and Thermoelastic Effect The derived representations of thermodynamic potentials for arbitrary threedimensional states of stress and strain are greatly simpliﬁed in the case of uniaxial and spherical states of stress. The corresponding results are listed in Problems 6.1 and 6.2 of Chapter 34. To illustrate the use of some of the derived formulas, consider the uniaxial loading paths shown in Fig. 6.4. The path OAB is an adiabatic (fast loading) path, the path OC is an isothermal (slow loading) path, the path AC is a constant stress path, and the path BC is a constant longitudinal strain path. Along the adiabatic path OAB (see Problem 6.1) u = −h =
1 σ2 , 2ES
(6.190)
6.11. Uniaxial Loading and Thermoelastic Effect
137
σ σB
σA = σC
o
B
A
Figure 6.4. Uniaxial loading along isothermal path OC, and along adiabatic path OAB. The paths AC and BC are the constant stress and constant longitudinal strain paths, respectively.
C
e eA e B= e C
whereas along the isothermal path OC [see the expressions for φ(σ, T) and g(σ, T) from Problem 6.1] φ − φ0 = g0 − g =
1 σ2 , 2ET
φ0 = g0 = −T0 s0 .
(6.191)
The temperature drop along the adiabatic path is T − T0 = −
α0 T0 σ, 3c0P
(6.192)
in accord with Kelvin’s formula describing Joule’s thermoelastic effect. The entropy increase along the isothermal path is s − s0 =
α0 σ, 3
(6.193)
with the corresponding absorbed heat given by T0 (s − s0 ). The heat absorbed along the constant stress path AC is equal to the enthalpy change hC − h A =
α 2 T0 α0 T0 σ A − 0 0 σ A2 . 3 18c P
This is in agreement with the result following from TC c0 c P (T)dT = P (T02 − TA2 ) . 2T0 TA The heat absorbed along the constant longitudinal strain path BC is 1 1 α0 T0 2 σC − σ + σ2 , uC − u B = 2ET C 3 2ES B
(6.194)
(6.195)
(6.196)
which gives uC − u B =
α0 T0 ES α02 T0 2 σA − σ . 3 ET 18c0P A
This can be conﬁrmed by integrating sC sC T0 α0 σ ds , T0 + 0 s − s0 − Tds = 3 cP sB sB
(6.197)
(6.198)
138
6. Thermodynamics of Continuum
with the stress variation, along the path BC, given by σ =
ES α0 T0 σ A − 0 ES (s − s0 ) . ET 3c P
(6.199)
For metals, the second term on the righthand side of (6.197) is much smaller than the ﬁrst term, being associated with small departures of c P and cV from their reference values c0P 0 0 and cV , inherent in linear approximations c P = c0P T/T0 and cV = cV T/T0 , which are valid for sufﬁciently small temperature differences (T − T0 ). An alternative derivation of (6.197) proceeds by noting that along the path BC, dσ = −ET α0 dT/3 (because the longitudinal component of strain is ﬁxed along that path). The corresponding increment of entropy is ds =
c0 c0 ET α0 dσ + P dT = P dT . 3 T0 T0 ES
(6.200)
The relationship (6.185) between isothermal and adiabatic Young’s moduli was used. Therefore, TC c0 ET 2 T0 − TB2 . (6.201) Tds = P 2T E 0 S TB The incorporation of (6.192) reproduces (6.197). Yet another derivation is possible by starting from an expression for the heat increment in terms of the latent and speciﬁc heat, i.e., Tds = liej dei j + cV dT . The components of the latent heat tensor at constant strain are deﬁned by ∂s liej = T = κT α0 Tδi j , ∂ei j T
(6.202)
(6.203)
which gives Tds = κT α0 Tdekk + cV dT .
(6.204)
Because along the path BC, dekk =
2 (1 + νT )α0 dT , 3
(6.205)
the substitution into (6.204), and integration from TB to TC = T0 , gives (6.197). This derivation is facilitated by noting that, in view of (6.183), (1 + νT )
α02 T0 ν S − νT = . 0 ES 9c P
(6.206)
The individual contributions of the latent and speciﬁc heat to the total heat absorbed along the path BC are C 1 − 2ν S cV dT = (uC − u B) , (6.207) 1 − 2νT B
C B
liej dei j = 2
ν S − νT (uC − u B) . 1 − 2νT
(6.208)
6.12. Thermodynamics of Open Systems
139
The contribution given by (6.207) is smaller than (uC − u B), because ν S > νT . Since the lateral strain is not held constant along the path BC, there is a small but positive contribution to absorbed heat from the latent heat, and this is represented by (6.208). Both, (6.197) and (6.207) display in their structure simple combination of adiabatic and isothermal elastic constants, via the ratio terms ES /ET and 0 cV ES 1 − 2ν S = . 1 − 2νT c0P ET
(6.209)
6.12 Thermodynamics of Open Systems: Chemical Potentials In addition to heat and work transfer, an open thermodynamic system allows a mass transfer across its boundary. Consider a homogeneous system, consisting of one phase, made up from uniform mixture of k components. For example, an AlZn fcc phase consists of Al and Zn components. Let n1 , n2 , . . . , nk be the numbers of moles of these components. Let U, V, and S be the internal energy, volume, and entropy within the whole system (extensive properties; if u is the internal energy per unit current mass, then U = ρVu and S = ρVs, where ρ is the current mass density). Suppose U = U(V, S, n1 , n2 , . . . , nk) , then
dU =
∂U ∂V
dV + S,ni
∂U ∂S
dS + V,ni
(6.210)
k ∂U i=1
∂ni
dni .
(6.211)
S,V,n j =i
Since, at constant composition (all ni ﬁxed), the relationships from the thermodynamics of closed system apply, we have ∂U ∂U , T= , (6.212) p=− ∂ V S,ni ∂ S V,ni where p and T are the pressure and temperature (intensive properties). If V and S are held constant, (6.211) indicates that the internal energy changes because of the changes in composition alone. Thus, we introduce the socalled chemical potential of the ith component by ∂U . (6.213) µi = ∂ni V,S,n j =i Consequently, the overall increment of internal energy can be expressed as dU = − pdV + TdS +
k
µi dni .
(6.214)
i=1
This can be viewed as the energy equation for an open system. The term − pdV is the work done to the system, TdS is the heat transferred to the system, and each µi dni is the energy change due to an inﬁnitesimal change of the component i at ﬁxed V and S and ﬁxed number of moles of other components. (For example, the addition of interstitial atoms changes the internal energy of the system, and this change is governed by the corresponding chemical potential).
140
6. Thermodynamics of Continuum
The chemical potential can also be introduced as the gradient of other thermodynamic potentials, by holding their independent variables ﬁxed. For example, considering the Helmholtz free energy (V, T, n1 , n2 , . . . , nk) = U(V, S, n1 , n2 , . . . , nk) − TS ,
(6.215)
we have = − pdV − SdT +
d
k
µi dni ,
(6.216)
i=1
where
∂ p=− ∂V
∂ S=− ∂T
, T,ni
,
µi =
V,ni
∂ ∂ni
.
(6.217)
V,T,n j =i
With the Gibbs energy G( p, T, n1 , n2 , . . . , nk) =
(V, T, n1 , n2 , . . . , nk) + pV
(6.218)
as the thermodynamic potential, we obtain dG = Vd p − SdT +
k
µi dni ,
(6.219)
i=1
where
V=
∂G ∂p
,
S=−
T,ni
∂G ∂T
,
µi =
p,ni
∂G ∂ni
.
(6.220)
p,T,n j =i
Finally, if the enthalpy of the system H( p, S, n1 , n2 , . . . , nk) = U(V, S, n1 , n2 , . . . , nk) + pV
(6.221)
is used, we have dH = Vd p + TdS +
k
µi dni ,
(6.222)
i=1
with
V=
∂H ∂p
, S,ni
T=
∂H ∂S
, p,ni
µi =
∂H ∂ni
.
(6.223)
p,S,n j =i
If the stress state is not pure pressure, the stress and strain tensors are related by ∂ ∂G 1 1 Si j = , Ei j = , (6.224) V0 ∂ Ei j T,ni V0 ∂ Si j Ei j ,ni where V0 is the initial volume of the system. Similar relations hold if U and H are used as thermodynamic potentials. One can easily establish the Maxwell’s relations corresponding to each thermodynamic potential (or the set of independent state variables). For example, by using the Gibbs energy, i.e., p, T, and ni as independent state variables, there follows ∂µi ∂V = , (6.225) ∂ni p,T,n j =i ∂ p T,n j
6.13. Gibbs–Duhem Equation
141
∂S ∂ni
∂µi ∂n j
p,T,n j =i
∂µi =− ∂T
= p,T,nr = j
∂µ j ∂ni
,
(6.226)
p,n j
.
(6.227)
p,T,nr =i
For the two component system, G = G( p, T, n1 , n2 ), the last reciprocal relation reads 2 ∂µ1 ∂µ2 ∂ G = = . (6.228) ∂n2 p,T,n1 ∂n1 p,T,n2 ∂n1 ∂n2 p,T
6.13 Gibbs–Duhem Equation The Gibbs energy G = G( p, T, n1 , n2 , . . . , nk)
(6.229)
is a homogeneous function of degree 1 with respect to ni , so that G( p, T, λn1 , λn2 , . . . , λnk) = λG( p, T, n1 , n2 , . . . , nk) ,
(6.230)
and k ∂G i=1
∂ni
ni = G .
(6.231)
p,T,n j =i
Recalling a deﬁnition of the chemical potential ∂G µi = , ∂ni p,T,n j =i
(6.232)
we conclude that G=
k
µi ni .
(6.233)
i=1
Therefore, the Gibbs energy of the system is the weighted sum of the chemical potentials of its components. If the system consists of n1 moles of only one component, then G1 = n1 µ1 , i.e., the chemical potential of this component (associated with the change of energy of the system due to change of the amount of this component in the system at constant V and S) is µ1 = G1 /n1 (molar Gibbs energy). An additional important relationship can be derived by applying a total differential to (6.233). We obtain dG =
k i=1
µi dni +
k
ni dµi .
(6.234)
i=1
By equating this to (6.219), i.e., dG = Vd p − SdT +
k i=1
µi dni ,
(6.235)
142
6. Thermodynamics of Continuum
there follows −Vd p + SdT +
k
ni dµi = 0 .
(6.236)
i=1
This is known as the Gibbs–Duhem equation. In a test at constant pressure and temperature, it reduces to k
ni dµi = 0 .
(6.237)
i=1
Having established the representation of the Gibbs energy in terms of chemical potentials, it is straightforward to derive the expressions for other thermodynamic potentials. Indeed, since H = G + TS, we obtain H = TS +
k
µi ni .
(6.238)
i=1
Furthermore, since U = H − pV, U = − pV + TS +
k
µi ni ,
(6.239)
i=1
and, since
= U − TS, = − pV +
k
µi ni .
(6.240)
i=1
The last two can be generalized for the case of nonhydrostatic state of stress as U = V0 Si j Ei j + TS +
k
µi ni ,
= V0 Si j Ei j +
i=1
k
µi ni .
(6.241)
i=1
6.14 Chemical Potentials for Binary Systems Consider a binary system consisting of n1 moles of component 1 and n2 moles of component 2. By (6.233), its Gibbs energy is G = n1 µ1 + n2 µ2 ,
(6.242)
where µ1 and µ2 are the chemical potentials of two components in the system. The molar Gibbs energy is deﬁned by Gm =
G . n1 + n2
(6.243)
Denoting by X1 =
n1 , n1 + n2
X2 =
n2 n1 + n2
(6.244)
the concentrations of two components, we can write Gm = X1 µ1 + X2 µ2 .
(6.245)
6.15. Conﬁgurational Entropy
143
Consider a process at constant p and T. The Gibbs–Duhem equation (6.237) then gives n1 dµ1 + n2 dµ2 = 0
⇒
X1 dµ1 + X2 dµ2 = 0 .
(6.246)
Consequently, upon applying the differential to (6.245), we obtain dGm = µ1 dX1 + µ2 dX2 .
(6.247)
Since dX1 = −dX2 (because X1 + X2 = 1), the above reduces to dGm = (µ2 − µ1 )dX2 ,
(6.248)
i.e., µ2 − µ1 =
dGm . dX2
(6.249)
Solving (6.245) and (6.249) for µ1 and µ2 , there follows µ1 = Gm − X2
dGm , dX2
µ2 = Gm + (1 − X2 )
dGm , dX2
(6.250)
(6.251)
both being expressed in terms of the molar Gibbs energy Gm = Gm (X2 ) and the concentration X2 .
6.15 Conﬁgurational Entropy We derive in this section an expression for the conﬁgurational entropy that is often adopted in the thermodynamics of open systems and alloy solutions. The number of distinguished ways in which N1 particles of type 1 and N2 particles of type 2 can ﬁll the N1 + N2 available sites is given by the wellknown formula =
(N1 + N2 )! . N1 !N2 !
(6.252)
The conﬁgurational entropy is deﬁned as Sconf = k ln = k ln
(N1 + N2 )! , N1 !N2 !
(6.253)
where k is the Boltzmann’s constant. Recalling the Stirling’s formula from calculus √ m! = 2π m mme−m , (6.254) we have ln m! =
1 ln(2πm) + m ln m − m . 2
(6.255)
For large integers m, this is approximately equal to ln m! ≈ m ln m − m .
(6.256)
144
6. Thermodynamics of Continuum
Applying this approximation to (6.253), we now have Sconf = k [(N1 + N2 ) ln(N1 + N2 ) − (N1 + N2 )
(6.257)
−(N1 ln N1 − N1 ) − (N2 ln N2 − N2 )] , i.e.,
conf
S
N1 N2 = −k N1 ln + N2 ln N1 + N2 N1 + N2
.
(6.258)
If there is n1 moles of particles 1 and n2 moles of particles 2, then N1 = NA n1 and N2 = NA n2 , where NA is the Avogadro’s number, so that n1 N1 = = X1 , N1 + N2 n1 + n2
N2 n2 = = X2 N1 + N2 n1 + n2
(6.259)
are the concentration of two types of particles in the mixture. Therefore, by dividing (6.258) with the total number of moles n1 + n2 , we obtain conf = −R(X1 ln X1 + X2 ln X2 ), Sm
(6.260)
conf = Sconf /(n1 + n2 ) is the molar conwhere R = NA k is the universal gas constant, and Sm ﬁgurational entropy.
6.16 Ideal Solutions The above expression for the conﬁgurational entropy is adopted in the theory of solid solutions. The molar entropy of the solid solution is assumed to consists of two parts: a weighted sum of the entropies of pure components (at given p and T), and the entropy of the components’ mixing, i.e., Sm =
k
(i) mix Xi Sm + Sm =
i=1
k i=1
i Xi Sm −R
k
Xi ln Xi .
(6.261)
i=1 (i)
The molar entropy of pure component i at given p and T is denoted by Sm . Similarly, the molar Gibbs energy is taken to be Gm =
k i=1
mix Xi G(i) m + Gm ,
mix Gmix m = −TSm = RT
k
Xi ln Xi .
(6.262)
i=1
If these expressions are adopted, the solution model is referred to as an ideal solution. mix Note that for an ideal solution model, Hmmix = 0 and mix m = Gm . The chemical potentials of the components in an ideal solution can be readily calculated. For example, for a binary solution, (6.262) gives (2) Gm = X1 G(1) m + X2 Gm + RT(X1 ln X1 + X2 ln X2 ) (2) = (1 − X2 )G(1) m + X2 Gm + RT[(1 − X2 ) ln(1 − X2 ) + X2 ln X2 ],
so that dGm X2 (1) = G(2) . m − Gm + RT ln dX2 1 − X2
(6.263)
6.17. Regular Solutions for Binary Alloys
145
The substitution of this into (6.250) and (6.251) then gives µ1 = G(1) m + RT ln X1 ,
µ2 = G(2) m + RT ln X2 .
(6.264)
The logarithmic terms are the mixing contributions to chemical potentials.
6.17 Regular Solutions for Binary Alloys The regular solution model involves an additional parameter ω (representing in some average sense the relative energies of like and unlike bonds between the two components of the alloy), such that the molar enthalpy of mixing is Hm = ωX1 X2 .
(6.265)
The entropy of mixing is taken to be as in an ideal solution, mix Sm = −R(X1 ln X1 + X2 ln X2 ) ,
(6.266)
mix mix so that the Gibbs energy of mixing (Gmix m = Hm − TSm ) becomes
Gmix m = ωX1 X2 + RT(X1 ln X1 + X2 ln X2 ) .
(6.267)
The molar Gibbs energy is accordingly (2) mix Gm = X1 G(1) m + X2 Gm + Gm ,
(6.268)
whereas the chemical potentials of two components in the solution are, from (6.250) and (6.251), 2 µ1 = G(1) m + ωX2 + RT ln X1 , 2 µ2 = G(2) m + ωX1 + RT ln X2 .
(6.269)
The most distinguished feature of a regular solution model is that it can lead to a miscibility gap. Namely, whereas an ideal solution implies complete solubility of two components throughout the concentration range, a regular solution allows a possibility that two components at low temperature may not mix for some concentration, but form a mixture of two solution phases with different concentrations. Assuming that ω > 0, the temperature below which there may be a miscibility gap is obtained from the requirements d3 Gm d2 Gm = = 0. dX22 dX23
(6.270)
This speciﬁes the critical temperature Tcr =
ω . 2R
(6.271)
The miscibility boundary is deﬁned by dGm (1) = G(2) m − Gm , dX2
(6.272)
146
6. Thermodynamics of Continuum
Gm
G (2) m
Τ 0,
(8.48)
and the strong convexity condition e : C : e = Ci jk ei j ek > 0.
(8.49)
The convexity condition is the more severe of the two, which may be readily seen by noting that the dyadic product ab would represent a strain tensor that is singular; yet (8.49) is to be true for all admissible strain tensors, including those that are not. For isotropic materials (8.49) leads to λ(eii )2 + 2µ(ei j ei j ) > 0, 1 2 (λ + µ)(eii )2 + 2µ[ei j ei j − (eii )2 ] > 0. 3 3
(8.50)
These imply 2 λ + µ > 0, 3
µ > 0.
(8.51)
Since the connections between the modulii (E, ν) and (λ, µ) are λ=
Eν , (1 + ν)(1 − 2ν)
µ=
E , 2(1 + ν)
(8.52)
the conditions expressed in (8.50) become E > 0,
−1 < ν < 1/2.
(8.53)
8.4. Compatibility Relations
169
Another approach to establishing such restrictions, still based on the positivedeﬁnite nature of the elastic energy function, is as follows. If the elastic strain energy is assumed to be positivedeﬁnite function of strain ei j , then σi j ei j = λ(ekk)2 + 2µei j ei j > 0 .
(8.54)
Denoting by ei j the deviatoric part of strain tensor, such that 1 ei j = ei j + ekkδi j , 3
(8.55)
1 ei j ei j = ei j ei j + (ekk)2 . 3
(8.56)
we have
Consequently, the inequality (8.54) can be rewritten as 2µei j ei j + κ(ekk)2 > 0 ,
(8.57)
where 2 E κ =λ+ µ= , 3 3(1 − 2ν)
µ=
E . 2(1 + ν)
(8.58)
By taking ekk = 0 in (8.57), we deduce that µ > 0; by taking ei j = 0, we deduce that κ > 0. This implies from equations (8.58) that E > 0 and −1 < ν < 1/2. Since experience does not reveal any isotropic elastic material with negative Poisson’s ratio, the physical range of ν is 0 < ν < 1/2. Negative values of ν would imply negative values of λ, because λ = 2µν/(1 − 2ν). In the limit ν → 1/2, the material behaves as incompressible (λ and κ → ∞), and µ = E/3. If ν = 1/3, we have E = κ and λ = 2µ; if ν = 1/4, then E = 3κ/2 and λ = µ.
8.4 Compatibility Relations If the strains are derived from a continuous, single valued vector displacement ﬁeld u, then they must satisfy a particular set of differential equations. Conversely, if this set of differential equations is satisﬁed by the components of strain, the corresponding displacement ﬁeld is a continuous displacement ﬁeld. We derive the compatibility equations below, using the following convenient notation for partial derivatives ∂(..)/∂ x ≡ (..), ,
∂ 2 (..)/∂ x ∂ xr ≡ (..),r .
With this notation the components of the inﬁnitesimal strain tensor become ei j =
1 (ui, j + u j,i ). 2
(8.59)
Thus, by inspection, we observe that e,mm = u,mm ,
emm, = u,m ,
(8.60)
and em,m =
1 1 (u,mm + um,m) = (u,mm + um,m ). 2 2
(8.61)
170
8. Governing Equations of Linear Elasticity
Therefore, e,mm + emm, = 2em,m.
(8.62)
Similarly, e,mn = u,mn ,
em,n =
1 (u,mn + um,n ), 2
(8.63)
and en,m =
1 (u,nm + un,m) , 2
emn, =
1 (um,n + un,m ). 2
(8.64)
Consequently, em,n + en,m − emn, = e,mn .
(8.65)
In general, we may express six independent relations of this type as e11,22 + e22,11 = 2e12,12 , e22,33 + e33,22 = 2e23,23 , e33,11 + e11,33 = 2e31,31 ,
(8.66)
e12,13 + e13,12 − e23,11 = e11,23 , e23,21 + e21,23 − e31,22 = e22,31 , e31,32 + e32,31 − e12,33 = e33,12 , or, in more compact form, ei j,kl + ekl,i j = eik, jl + e jl,ik.
(8.67)
The above are called the SaintVenant’s compatibility equations for the strain components. In what immediately follows, we revisit the establishment of such equations from two different approaches.
8.5 Compatibility Conditions: Cesaro ` Integrals Consider two points of the deformed body, Aand B. Denoting their displacement components by uiA and uiB, we can write B uiB = uiA + dui . (8.68) A
If displacement components uiB are to be singlevalued in a simply connected region, the integral on the righthand side of the above equation must be pathindependent. By imposing this condition, we will again arrive at the SaintVenant’s compatibility equations. To demonstrate this, we proceed as follows. First, we have uiB
=
uiA +
B A
dui =
uiA +
B A
∂ui dx j = uiA + ∂xj
B A
ei j dx j +
B A
ωi j dx j ,
(8.69)
8.5. Cesaro ` Integrals
171
where ei j and ωi j are the inﬁnitesimal strain and rotation tensors (symmetric and antisymmetric parts of the displacement gradient ui, j ). By using the integration by parts, we then write B B B ∂ωi j B A A ωi j dx j = ωi j d(x j − x B ) = (x − x )ω − (x j − x B dxk . (8.70) j j j ij j ) ∂ xk A A A But, as can be easily veriﬁed by inspection, ∂ωi j ∂eik ∂e jk = − . ∂ xk ∂xj ∂ xi
(8.71)
Hence, by substituting (8.71) into (8.70), and then this into (8.69), we obtain B B A B A A ui = ui + (x j − x j )ωi j + fik dxk , A
where
fik = eik − (x j − x B j )
∂eik ∂e jk − . ∂xj ∂ xi
(8.72)
The above integral has to be path independent. Thus, fikdxk = fi j dx j = dgi has to be a perfect differential. The necessary and sufﬁcient condition for this is that ∂ fi j ∂ fik = , ∂xj ∂ xk
(8.73)
(both then being equal to ∂ 2 gi /∂ x j ∂ xk). Substituting (8.72) into (8.73) leads to ∂ 2 ei j ∂ 2 e jl ∂ 2 ekl ∂ 2 eik + − − = 0. ∂ xk∂ xl ∂ xi ∂ x j ∂ x j ∂ xl ∂ xi ∂ xk
(8.74)
There are 81 of these equations, but some of them are trivial identities, and some are repetitions due to symmetry in indices i j and kl. The contraction k = l yields six linearly independent SaintVenant’s equations ∂ 2 ei j ∂ 2 e jk ∂ 2 ekk ∂ 2 eik + − − = 0. ∂ xk∂ xk ∂ xi ∂ x j ∂ x j ∂ xk ∂ xi ∂ xk
(8.75)
They can be compactly rewritten as $i j = ikl jmn
∂ 2 eln = 0. ∂ xk∂ xm
(8.76)
The permutation tensor is denoted by i jk. Thus, for a given strain ﬁeld ei j , the necessary and sufﬁcient conditions for the existence of singlevalued displacement ﬁeld ui within a simply connected region (apart from the rigidbody motion) are the six SaintVenant’s compatibility equations $i j = 0. These equations are linearly independent, but differentially related by three Bianchi conditions ∂$i j = 0. ∂xj
(8.77)
These follow from the symmetry of the mixed partial derivative ∂ 2 /∂ xm∂ xn and the skewsymmetry of the permutation tensor i jk. If $i j = 0, the incompatibility tensor $i j represents a measure of the degree of strain incompatibility.
172
8. Governing Equations of Linear Elasticity
For (N + 1)tiply connected region, in addition to six SaintVenant’s compatibility equations (8.76), there are 3N Cesaro ` integral conditions for the existence of singlevalued displacements. They are fi j dx j = 0 , (8.78) Cα
where Cα (α = 1, 2, . . . , N) are any closed irreducible curves around N internal “cavities” and fi j = ei j − (xk − xk0 )(ei j,k − e jk,i ) .
(8.79)
xk0 . Since this point can be selected
The coordinates of a selected reference point on Cα are arbitrarily on each Cα , equations (8.78) and (8.79) give rise to 6N integral conditions (ei j − xkliklpq e pj,q )dx j = 0 , (8.80) Cα
i jl e jk,l dxk = 0 .
(8.81)
Cα
8.6 Beltrami–Michell Compatibility Equations By substituting the stressstrain relations ν 1+ν σkkδi j + σi j (8.82) E E into the SaintVenant’s compatibility equations (8.75), and by using the equilibrium equations ei j = −
σi j, j + bi = 0 ,
(8.83)
we can deduce six linearly independent compatibility equations expressed in terms of stresses. These are the Beltrami–Michell compatibility equations 1 ν σkk,i j = − bk,kδi j − bi, j − b j,i . 1+ν 1−ν In particular, it follows that the hydrostatic stress satisﬁes the Poisson’s equation σi j,kk +
1+ν bk,k . 1−ν If there are no body forces, the Beltrami–Michell equation reduce to 2 σkk = −
(8.84)
(8.85)
1 σkk,i j = 0 , (8.86) 1+ν whereas the hydrostatic stress becomes a harmonic function, satisfying the Laplace’s equation σi j,kk +
2 σkk = 0 .
(8.87)
8.7 Navier Equations of Motion The Cauchy equations of motion, in terms of stresses, are ∂σi j ∂ 2 ui + bi = ρ 2 , ∂xj ∂t
(8.88)
8.7. Navier Equations of Motion
173
where bi are the components of the body force per unit volume. By substituting the stressstrain relations ∂u j ∂ui ∂uk + δi j (8.89) +λ σi j = 2µei j + λekkδi j = µ ∂xj ∂ xi ∂ xk into (8.88), we obtain the Navier equations of motion, in terms of displacements, (λ + µ)
∂ 2u j ∂ 2 ui ∂ 2 ui +µ + bi = ρ 2 . ∂ xi ∂ x j ∂xj ∂xj ∂t
(8.90)
Since Ti = σi j n j , the boundary conditions over the bounding surface of the body ST , where tractions are externally prescribed, are ∂u j ∂ui ∂uk n j = Tiext , ni + µ + (8.91) λ ∂ xk ∂xj ∂ xi whereas ui = uiext ,
(8.92)
where displacements are prescribed (Su ). In the vector notation, the Navier equations are (λ + µ) ∇(∇ · u) + µ∇ 2 u + b = ρ
∂ 2u ∂t 2
λ (∇ · u)n + µ(u∇ + ∇u) · n = Text u = uext
in V , on ST ,
(8.93)
on Su .
The nabla operator expressed with respect to three typical sets of coordinates is ∇ = e1
∂ ∂ ∂ + e2 + e3 , ∂ x1 ∂ x2 ∂ x3
∇ = er
∂ 1 ∂ ∂ + eθ + ez , ∂r r ∂θ ∂z
∇ = er
(8.94)
∂ 1 ∂ 1 ∂ + eθ + eφ . ∂r r ∂θ r sin θ ∂φ
The corresponding Laplacian operators are, respectively, ∇2 = 1 ∂ ∇ = r ∂r 2
∇2 =
1 ∂ r 2 ∂r
∂2 ∂2 ∂2 + 2+ 2, 2 ∂ x1 ∂ x2 ∂ x3 ∂2 ∂ 1 ∂2 + , r + 2 ∂r r ∂θ 2 ∂z2
∂ ∂ ∂2 1 ∂ 1 . r2 + 2 sin θ + 2 ∂r r sin θ ∂θ ∂θ r 2 sin θ ∂φ 2
(8.95)
174
8. Governing Equations of Linear Elasticity
8.8 Uniqueness of Solution to Linear Elastic Boundary Value Problem 8.8.1 Statement of the Boundary Value Problem The boundary value problem of linear elasticity is speciﬁed by the equations σi j, j + bi = 0 , ei j =
1 (ui, j + u j,i ) , 2
(8.96)
ei j,kl + ekl,i j = eik, jl + e jl,ik , and the boundary conditions Ti = σi j n j ui
prescribed on ST ,
(8.97)
prescribed on Su .
The outward pointing normal to the bounding surface of the body is ni . Furthermore, if there exists a strain energy function W = W(ei j ), then σi j =
∂W . ∂ei j
(8.98)
W=
1 1 σi j ei j = Ci jkl ei j ekl . 2 2
(8.99)
For linear elasticity, σi j = Ci jkl ei j ,
If the elastic strain energy is assumed to be positivedeﬁnite function of strain, the elastic moduli tensor Ci jkl is a positivedeﬁnite tensor.
8.8.2 Uniqueness of the Solution The so speciﬁed boundary value problem of linear elasticity has a unique solution for the stress and strain ﬁelds. The proof is based on the assumption of the positivedeﬁniteness of the elastic strain energy. Suppose that two solutions exist that satisfy (8.8.1)–(8.99). (1) (1) (1) (2) Denote the corresponding displacement, strain, and stress ﬁelds by ui , ei j , σi j and ui , (2)
(2)
ei j , σi j . Let ui∗ = ui − u2 , (1)
(2)
ei∗j = ei j − ei j , (1)
(2)
σi∗j = σi j − σi j . (1)
(2)
(8.100)
Since (1)
σi j, j + bi = 0 ,
(2)
σi j, j + bi = 0 ,
(8.101)
we evidently have σi∗j, j = 0 .
(8.102)
8.9. Potential Energy and Variational Principle
175
Consequently, the ﬁelds ui∗ , ei∗j , σi∗j represent a solution to the homogeneous boundary value problem σi∗j, j = 0 and bi∗ = 0 in V ,
Ti∗ = σi∗j n j = 0 on ST ,
ui∗ = 0 on Su .
(8.103)
Clearly, at every point of the bounding surface S of the body the product ui∗ Ti∗ = 0, because either ui∗ or Ti∗ vanishes at the boundary. Thus, upon integration and the application of the Gauss divergence theorem, ∗ ∗ ∗ ∗ (8.104) 0 = ui Ti dS = ui σi j n j dS = (ui∗ σi∗j ), j dV . S
S
V
Performing the partial differentiation within the integrand, and using σi∗j, j = 0 and σi∗j ui,∗ j = σi∗j ei∗j , then gives 0= σi∗j ei∗j dV = 2 W(ei∗j )dV . (8.105) V
V
But W is a positivedeﬁnite function of strain and the integral of W(ei∗j ) over the volume V vanishes only if W = 0 at every point of the body. This is possible only if ei∗j = 0 at every point, i.e., (1)
(2)
ei j = ei j
(1)
(2)
and therefore σi j = σi j .
(8.106)
Thus the uniqueness of the solution to the boundary value problem of linear elasticity: there is only one stress and strain ﬁeld corresponding to prescribed boundary conditions and given body forces.
8.9 Potential Energy and Variational Principle Consider inﬁnitesimal deformation of an elastic material. In this section, for the sake of generality, we do not actually restrict to linearly elastic material, but the material that is characterized by the strain energy that is an arbitrary single valued function of a small strain, such that emn ∂W σi j dei j , σi j = . (8.107) W = W(emn ) = ∂ei j 0 The principle of virtual work (5.140) then gives δW dV = Ti δui dS + bi δui dV , V
S
(8.108)
V
because δW = σi j δei j = (∂ W/∂ei j )δei j . With body forces bi regarded as given in V and surface forces Ti given on ST , and recalling that δui = 0 on Su = S − ST , (8.108) delivers a variational principle Ti ui dS . (8.109) δ% = 0 , % = [W(emn ) − bi ui ] dV − V
ST
The functional % = %(ui ) is the potential energy of the elastic body. Since bi and Ti are regarded as ﬁxed, it is a functional of the displacement ﬁeld. For the true equilibrium displacement ﬁeld, % has a stationary value, because δ% = 0 for any kinematically admissible variation δui .
176
8. Governing Equations of Linear Elasticity
We next show the equilibrium displacement ﬁeld minimizes the potential energy among all kinematically admissible displacement ﬁelds. The following proof relies on the adoption of an incremental stability (stability in the small), according to which dσi j dei j > 0
(8.110)
for any set of strain and corresponding stress increments. Indeed, let uit be the true equilibrium displacement ﬁeld and uik an arbitrary kinematically admissible displacement ﬁeld (continuous and differentiable, satisfying the displacement boundary conditions on Su , if any). The difference in the potential energy associated with these two ﬁelds is
k t k t %(ui ) − %(ui ) = W(emn ) − W(emn ) − bi (uik − uit ) dV V
−
S
(8.111) Ti (uik − uit ) dS .
Note that uik − uit = 0 on Su , so that the above surface integral can be extended from ST to S. But the principle of virtual work gives σitj (eikj − eit j ) dV = Ti (uik − uit ) dS + bi (uik − uit ) dV . (8.112) V
S
V
When this is substituted in (8.111), there follows
k t k t ) − W(emn ) − σitj (eikj − eit j ) dV . W(emn %(ui ) − %(ui ) =
(8.113)
V
In view of (8.107), this can be rewritten as " emn k k t %(ui ) − %(ui ) = (σi j − σitj )dei j − V
0
" =
k emn
t emn
V
# (σi j −
σitj )dei j
t emn
0
# (σi j −
σitj )dei j
dV
dV .
The elastic deformation is pathindependent, and the value of the integral emn k (σi j − σitj )dei j
(8.114)
t emn
t k and emn . Thus, selecting a strain path that does not depend on the strain path between emn t corresponds to a straight line in stress space from σi j to σikj , the stress increment dσi j is codirectional with σi j − σitj . Consequently, if the material is incrementally stable, such that dσi j dei j > 0, we have
k emn
t emn
(σi j − σitj )dei j > 0 ,
(8.115)
and thus %(uik ) − %(uit ) > 0 .
(8.116)
Therefore, among all kinematically admissible displacement ﬁelds, the true (equilibrium) displacement ﬁeld minimizes the potential energy of the body.
8.10. Betti’s Theorem of Linear Elasticity
177
8.9.1 Uniqueness of the Strain Field (1)
(2)
and ui both minimize the potential energy, then # (2) " emn (1) (σi j − σi j )dei j dV = 0 .
If two displacement ﬁelds ui
V
(1)
(8.117)
emn
(1)
But, the incremental stability dσi j dei j > 0 implies that (σi j − σi j )dei j > 0 along the strain (1)
(2)
path that corresponds to a straight line in stress space from σi j to σi j . Consequently, the (2)
(1)
above integral can vanish if and only if emn = emn , which assures the uniqueness of the strain ﬁeld (possibly, to within a rigid body displacement).
8.10 Betti’s Theorem of Linear Elasticity This important theorem of linear elasticity follows from the generalized Claopeyron’s formula and the linearity between the stress and strain, σi j = Ci jkl ekl , where Ci jkl are the elastic moduli obeying the reciprocal symmetry Ci jkl = Ckli j . Indeed, the Clapeyron’s formula [see (5.138) from Chapter 5] gives σi j eˆi j dV = Ti uˆ i dS + bi uˆ i dV . (8.118) V
S
V
Let σˆ i j = Ci jkl eˆ kl be the true equilibrium stress ﬁeld associated with the displacement ﬁeld uˆ i . Then, σˆ i j ei j = Ci jkl ei j eˆ kl ,
(8.119)
σi j eˆi j = Ci jkl ekl eˆi j = Ckli j ei j eˆ kl = Ci jkl ei j eˆ kl .
(8.120)
σˆ i j ei j = σi j eˆi j .
(8.121)
and
Thus,
Consequently, from (8.118) it follows that ˆ Ti uˆ i dS + bi uˆ i dV = Ti ui dS + bˆ i ui dV . S
V
S
(8.122)
V
This is the Betti’s reciprocal theorem of linear elasticity. The work of the ﬁrst type of loading on the displacement due to the second type of loading, is equal to the work of the second type of loading on the displacement due to the ﬁrst type of loading. A classical illustration of the application of this theorem is as follows. Consider a uniform rod of length l and crosssectional area A. The rod is made of isotropic elastic material, with the elastic modulus E and Poisson’s ratio ν. Two types of loading applied to this rod are shown in Fig. 8.2. The ﬁrst loading is a uniform tensile stress σ applied to the ends of the rod, giving rise to axial force P = σ A. The second loading is a pair of two equal but opposite transverse forces F applied to the lateral surface of the rod, anywhere along the length of the rod. The transverse distance between the points of the application of two forces is h. The Betti’s theorem allows us to easily calculate the elongation of the rod due to this pair of forces, without solving the complicated boundary value problem. Indeed, the ﬁrst type of loading causes the lateral contraction of the rod of magnitude
178
8. Governing Equations of Linear Elasticity F
σ
σ
h
l
F
Figure 8.2. A uniform elastic rod under two types of loading.
h = ν(Ph/EA). By Betti’s theorem, the work of F on the displacement due to P = σ A, must be equal to the work of P on the displacement due to F, i.e., Fν
Ph = P . EA
(8.123)
Thus, the elongation of the rod due to the pair of forces F is =ν
Fh . EA
(8.124)
8.11 Plane Strain Plane deformations are deﬁned such that e33 = e13 = e23 = 0.
(8.125)
If we allow for the possibility of thermal strains, with the thermal expansion coefﬁcient α, the corresponding thermoelastic constitutive equations are 1 [σ11 − ν(σ22 + σ33 )] + αT, E 1 = [σ22 − ν(σ11 + σ33 )] + αT, E
e11 = e22
(8.126)
e33 = 0 ⇒ σ33 = ν(σ11 + σ22 ) − α ET, e12 = e21 =
1 σ12 . 2G
Suppose that we introduce body forces via a potential function, V(x1 , x2 ), such that b = −∂ V/∂x.
(8.127)
Using the compact notation for differentiation, the equations of equilibrium become σ11,1 + σ12,2 − V,1 = 0 σ21,1 + σ22,2 − V,2 = 0.
(8.128)
All of the compatibility equations (8.66) are identically satisﬁed except the ﬁrst one, which gives e11,22 + e22,11 = 2e12,12 .
(8.129)
8.11. Plane Strain
179
Introduce the Airy stress function, φ(x1 , x2 ), such that σ11 = φ,22 + V(x1 , x2 ) , σ22 = φ,11 + V(x1 , x2 ) ,
(8.130)
σ12 = −φ,12 . With such deﬁnitions the equilibrium equations (8.128) are identically satisﬁed. To determine the governing equations for φ we ﬁrst substitute (8.130) into the constitutive expressions (8.126) and demand the satisfaction of the compatibility relation (8.129). Thus, we substitute 1 {(1 − ν 2 )φ,22 − ν(1 + ν)φ,11 + [1 − ν(1 + 2ν)]V} + (1 + ν)αT, E 1 = {(1 − ν 2 )φ,11 − ν(1 + ν)φ,22 + [1 − ν(1 + 2ν)]V} + (1 + ν)αT, E 1 φ,12 =− 2G
e11 = e22 e12
into (8.129) to get ∇ 4φ = −
(1 − 2ν) 2 αE ∇ V− ∇ 2 T. (1 − ν) (1 − ν)
(8.131)
If there are no body forces and thermal gradients, or if ∇ 2 V = 0 and ∇ 2 T = 0, then φ satisﬁes the biharmonic equation ∇ 4 φ = 0,
∇ 4φ ≡
∂ 4φ 2∂ 4 φ ∂ 4φ + + . ∂ x14 ∂ x12 ∂ x22 ∂ x24
(8.132)
If the thermal ﬁeld is such that ∇ 2 T = 0, there would be no effect on φ, or on the stresses; there would, of course, be an effect on the strains. An example in Section 8.13 will illustrate these effects. For this purpose we consider thermal strains alone – linear superposition allows the addition of the effects of applied loads or displacements.
8.11.1 Plane Stress The governing equations for plane stress are similar. In that case we set σ33 = σ13 = σ23 = 0, and the constitutive equations are e11 = e33
1 1 (σ11 − νσ22 ), e22 = (σ22 − νσ11 ), E E ν 1 σ12 , = − (e11 + e22 ), e12 = E 2G
(8.133)
e13 = e23 = 0. In the absence of thermal ﬁelds, the governing equation for the stress potential is ∇ 4 φ = −(1 − ν)∇ 2 V(x1 , x2 ).
(8.134)
180
8. Governing Equations of Linear Elasticity
8.12 Governing Equations of Plane Elasticity In this section we summarize the governing equations of plane elasticity, simultaneously for both plane stress and plane strain. The stressstrain relations are 1 3−ϑ σkkδi j , (i, j = 1, 2), ei j = (8.135) σi j − 2µ 4 where ϑ is the Kolosov constant deﬁned by ⎧ ⎪ ⎨3 − 4ν , plane strain , ϑ = 3−ν ⎪ ⎩ , plane stress . 1+ν
(8.136)
Because the physical range of the Poisson ratio is 0 ≤ ν ≤ 1/2, the Kolosov constant is restricted to 0 ≤ ϑ ≤ 3 for plane strain, and 5/3 ≤ ϑ ≤ 3 for plane stress. The inverted form of (8.135) is 1 3−ϑ ekkδi j , (i, j = 1, 2) . σi j = 2µ ei j + (8.137) 2 ϑ −1 There are two Cauchy equations of motion ∂σi j ∂ 2 ui + bi = ρ 2 , ∂xj ∂t
(8.138)
and one SaintVenant’s compatibility equation ∂ 2 e11 ∂ 2 e22 ∂ 2 e12 + = 2 . ∂ x1 ∂ x2 ∂ x22 ∂ x12
(8.139)
The corresponding Beltrami–Michell comaptibility equation is ∇ 2 (σ11 + σ22 ) =
4 ∂bi , 1 + ϑ ∂ xi
(8.140)
where ∇ 2 is the twodimensional Laplacian operator. Finally, the two Navier equations of motion are µ∇ 2 ui +
2µ ∂ 2 u j ∂ 2 ui + bi = ρ 2 , ϑ − 1 ∂ xi ∂ x j ∂t
(i, j = 1, 2) .
(8.141)
8.13 Thermal Distortion of a Simple Beam As an illustration of the application of derived equations, consider the following thermoelastic beam problem. Let T(x2 ) be the temperature variation speciﬁed across the beam shown in Fig. 8.3. Our objective is to calculate the displacements of the beam, and as needed the stresses and strains caused by what amounts to purely thermal loading. For this case, ∇ 2 T = d2 T/dx22 , since the gradient is solely through the thickness of the beam, i.e., in its x2 direction. Equation (8.131) becomes ∇ 4φ = −
α E d2 T . (1 − ν) dx22
(8.142)
8.13. Thermal Distortion of a Simple Beam
181
x2 ∆T m1
L
Consistent with all the boundary conditions speciﬁed so far, we can set σ22 = σ12 = 0, which are typical assumptions of elementary beam theory. Then, ∂ 4 φ/∂ x14 = 0, (8.143)
∂ 4φ = 0. ∂ x12 ∂ x22
The integration of (8.143) is elementary, but illustrative. Toward that end, we write ∂ 2 ∂ 2φ α E d2 T . (8.144) = − (1 − ν) dx22 ∂ x22 ∂ x22 Since σ11 = φ,22 , this reduce to
αE ∂2 T(x2 ) = 0. σ11 + (1 − ν) ∂ x22
(8.145)
Two integrations later, we obtain σ11 +
αE T(x2 ) = C1 x2 + C2 . (1 − ν)
(8.146)
The integration constants, C1 and C2 , are determined from the requirement of static equilibrium h σ11 (x2 ) dx2 = 0,
−h
h
−h
(8.147)
σ11 (x2 )x2 dx2 = 0.
The integrations yield h h αE 1 x2 −T(x2 ) + T(η) dη + ηT(η) dη . σ11 (x2 ) = (1 − ν) 2h −h 2/3h3 −h The corresponding strains are e11 (x2 ) =
1 σ11 + αT(x2 ), E
e22 (x2 ) = −
ν σ11 + αT(x2 ), E
e12 = 0.
We now analyze the resulting deﬂection of the beam. With the usual assumptions of elementary beam theory, we approximate the beam’s curvature as 1/r ≈ −e11 /x2 .
182
8. Governing Equations of Linear Elasticity
Thus, (1/r )top ≈ −e11 (h)/ h ,
(1/r )bottom ≈ −e11 (−h)/(−h),
(8.148)
and so e11 (−h) − e11 (h) ∂ 2 u2 ≈ . 2h ∂ x12
(8.149)
T(x2 ) = (1/2)mT(1 − x2 / h)m,
(8.150)
1/r ≈ As a speciﬁc example, take
where T is a given difference in temperature between the bottom and top sides of the beam. The analysis is straightforward. In particular, the maximum deﬂection of the beam is found to be δmax ≈
L αT(L/ h)g(m), 16
(8.151)
6m . (m + 1)(m + 2)
(8.152)
with g(m) ≡
The result shows how the shape of the temperature variation is important in affecting the magnitude of the induced thermal distortion. For example, if m < 1, say m ≈ 1/3, then g ∼ 0.6, which represents an appreciable reduction in the maximum displacement at the midpoint of the beam. On the other hand, if m ≈ 3, then g ∼ 0.9, and the reduction in maximum displacement is far less. Thus manipulating the temperature proﬁle may provide a mechanism to mitigate intolerably large thermally induced deﬂections.
8.14 Suggested Reading Barber, J. R. (2002), Elasticity, 2nd ed., Kluwer, Dordrecht. FilonenkoBorodich, M. (1964), Theory of Elasticity, Noordhoff, Groningen, Netherlands. Fung, Y.C. (1965), Foundations of Solid Mechanics, Prentice Hall, Englewood Cliffs, New Jersey. Green, A. E., and Zerna, W. (1954), Theoretical Elasticity, Oxford University Press, London. Landau, L. D., and Lifshitz, E. M. (1986), Theory of Elasticity, 3rd English ed., Pergamon, New York. Little, R. W. (1973), Elasticity, Prentice Hall, Englewood Cliffs, New Jersey. Love, A. E. H. (1944), A Treatise on the Mathematical Theory of Elasticity, Dover, New York. Malvern, L. E. (1969), Introduction to the Mechanics of a Continuous Medium, Prentice Hall, Englewood Cliffs, New Jersey. Musgrave, M. J. P. (1970), Crystal Acoustics: Introduction to the Study of Elastic Waves and Vibrations in Crystals, Holdenday, San Francisco. Muskhelishvili, N. I. (1963), Some Basic Problems of the Mathematical Theory of Elasticity, Noordhoff, Groningen, Netherlands.
8.14. Suggested Reading
183
Shames, I. H., and Cozzarelli, F. A. (1997), Elastic and Inelastic Stress Analysis, Taylor & Francis, London. Sokolnikoff, I. S. (1956), Mathematical Theory of Elasticity, 2nd ed., McGrawHill, New York. Timoshenko, S. P., and Goodier, J. N. (1970), Theory of Elasticity, 3rd ed., McGrawHill, New York.
9 Elastic Beam Problems
9.1 A Simple 2D Beam Problem Approximate solutions can be developed for twodimensional boundary value problems in plane stress or plane strain by representing the Airy stress function as a polynomial in x1 and x2 . This general methodology is developed via several speciﬁc examples. To begin, recall the general form of the biharmonic equation for the case of plane strain, 1 − 2ν 2 ∇ V, 1−ν
(9.1)
∇ 4 φ = −(1 − ν)∇ 2 V.
(9.2)
∇ 4φ = − or, for plane stress,
Recall also the connections between φ and the stresses, viz., σ11 = φ,22 + V(x1 , x2 ) , σ22 = φ,11 + V(x1 , x2 ) ,
(9.3)
σ12 = −φ,12 . To illustrate how an approximate solution may be constructed consider the boundary value problem for the simple beam shown in Fig. 9.1. Here the boundary conditions are speciﬁed as σ12 = 0 on x2 = ±b, σ22 = 0 on x2 = ±b,
(9.4)
σ11 = 0 on x1 = 0, and
b
−b
σ12 dx2 = F on x1 = 0.
(9.5)
The last boundary condition is the socalled integral or global boundary condition, in contrast to point wise boundary conditions of (9.4). 184
9.2. Polynomial Solutions to ∇4 φ = 0
185
x2
F
b b
Figure 9.1. A cantilever beam under the end loading.
x1
In the subsequent analysis it is assumed that no potentials act, so that V = 0. Also plane stress prevails so that the governing equation for φ is simply ∇ 4 φ = 0. We then explore possible polynomial solutions to this biharmonic equation.
9.2 Polynomial Solutions to ∇4 φ = 0 Consider the general nth order polynomial pn (x1 , x2 ) = a0 x1n + a1 x1n−1 x2 + a2 x1n−2 x22 + · · · + an x2n =
n
(9.6)
ai x1n−i x2i .
i=0
If (9.6) is substituted into (9.2), with V = 0, a polynomial of the form qn−4 (x1 , x2 ) = ∇ 4 pn (x1 , x2 ) =
n−4
bi x1n−4−i x2i
(9.7)
i=0
is generated. For example, b0 = n(n − 1)(n − 2)(n − 3)a0 + 4(n − 2)(n − 3)a2 + 24a4 ,
(9.8)
and so on. For (9.6) to be a solution to (9.2), all the qn (x1 , x2 ) must be zero. This requires that bi = 0,
i = 0, 1, . . . , n − 4.
(9.9)
Thus, (9.9) are a set of (n − 3) linear equations among the (n + 1) ai ’s. Four ai ’s are unknown, i.e., are adjustable constants, so that (9.9) places constraints on the rest. Now consider what polynomial forms for φ(x1 , x2 ) give rise to associated forms for the σi j ’s. For example, consider the form φ2 (x1 , x2 ) = a0 x12 + a1 x1 x2 + a2 x22 ,
(9.10)
which yields σ11 = 2a2 ,
σ22 = 2a0 ,
σ12 = −a1 .
(9.11)
Consequently, (9.10) implies a state of uniform inplane stress. Next, consider the form φ3 (x1 , x2 ) = a0 x13 + a1 x12 x2 + a2 x1 x22 + a3 x23 ,
(9.12)
186
9. Elastic Beam Problems
which produces the stress components σ11 = 2a2 x1 + 6a3 x2 , σ22 = 2a1 x2 + 6a0 x1 ,
(9.13)
σ12 = −2a1 x1 − 2a2 x2 . Suppose the assignment a0 = a1 = a2 = 0 is made. Then σ11 = 6a3 x2 ,
(9.14)
which corresponds to a simple state of pure bending. Clearly additional perspective can be developed by conjuring up other simple polynomial forms and noting that (9.2) is a linear partial differential equation for φ(x1 , x2 ).
9.3 A Simple Beam Problem Continued Consider the polynomial form φ(x1 , x2 ) = c1 x1 x23 + c2 x1 x2 .
(9.15)
The fourthorder term, c1 x1 x23 , produces a bending stress of the form σ11 ∝ x1 x2 , which varies linearly with x1 . The second term, c2 x1 x2 , produces a uniform shear stress, σ12 = −c2 that can be used to cancel out any otherwise unwanted shear stress arising from other terms. In fact, (9.15) yields σ11 = 6c1 x1 x2 ,
σ22 = 0,
σ12 = −3c1 x22 − c2 .
(9.16)
The ﬁrst boundary condition of (9.4) states that σ12 (x2 = ±b) = 0 = −3c1 b2 − c2 ⇒ c2 = −3c1 b2 ,
(9.17)
σ12 = 3c1 (b2 − x22 ).
(9.18)
and thus
The integral boundary condition of (9.5) demands that
b
σ12 dx2 = F on x1 = 0,
(9.19)
3c1 (b2 − x22 ) dx2 = F ⇒ c1 = F/(4b3 ).
(9.20)
−b
i.e.,
b
−b
Therefore, we arrive at the result φ(x1 , x2 ) =
F(x1 x23 − 3b2 x1 x2 ) . 4b3
(9.21)
9.3. Simple Beam Problem
187
Consequently, 3F x1 x2 , 2b3 3F = 3 (b2 − x22 ), 4b
σ11 = σ12
(9.22)
σ22 = 0. Note that the boundary conditions for the beam at the end x1 = 0 are satisﬁed only on an integral level; point wise satisfaction is not possible with such a simple polynomial solution. However, by SaintVenant’s principle, the solutions that correspond to statically equivalent, although pointwise different, end loads differ appreciably only within the region near the end of the beam. 9.3.1 Strains and Displacements for 2D Beams The strains are calculated directly from the stresses as σ22 3F x1 x2 σ11 −ν = , E E 2Eb3 σ11 3Fνx1 x2 σ22 −ν =− = , E E 2Eb3
e11 = e22
(9.23)
3F(1 + ν)(b2 − x22 ) 1+ν σ12 = . E 4Eb3 The strains may be integrated to obtain the displacements as follows. First, we have e12 =
e11 =
∂u1 3F x1 x2 = , ∂ x1 2Eb3
3F x12 x2 u1 (x1 , x2 ) = + f (x2 ), 4Eb3
(9.24)
where f (x2 ) is an arbitrary integration function of x2 . Likewise, e22 =
∂u2 3Fνx1 x2 =− , ∂ x2 2Eb3
3Fνx1 x22 + g(x1 ), u2 (x1 , x2 ) = − 4Eb3
(9.25)
where g(x1 ) is another arbitrary integration function of x1 . Furthermore, we have 3F(1 + ν)(b2 − x22 ) 1 ∂u1 ∂u2 + . (9.26) e12 = = 2 ∂ x2 ∂ x1 4Eb3 When we substitute the expressions for u1 and u2 from above into (9.26) and rearrange terms, we ﬁnd that 3F x12 3Fνx22 3F(1 + ν)(b2 − x22 ) 1 1 g f + (x ) = − (x ) + . 1 2 8Eb3 2 8Eb3 2 4Eb3
(9.27)
Rearranged in this way, (9.27) reads R(x1 ) = S(x2 ),
(9.28)
188
9. Elastic Beam Problems x2 x1
b
Figure 9.2. A simple beam under selfweight.
b
2a
which is true only if R(x1 ) = S(x2 ) = C, where C is a constant. Thus, g (x1 , x2 ) = −
3F x12 + C, 4Eb3
3Fνx22 3F(1 + ν)(b2 − x22 ) + −C. f (x1 , x2 ) = 4Eb3 2Eb3
(9.29)
This in turn leads to g(x1 ) = −
F x13 + Cx1 + B, 4Eb3
Fνx23 F(1 + ν)(3b2 x2 − x23 ) + − Cx2 + A. f (x2 ) = 4Eb3 2Eb3
(9.30)
By substituting equations (9.30) into (9.24) and (9.25), it is found that u1 (x1 , x2 ) =
3F x12 x2 F(2 + ν)x23 3F(1 + ν)x2 − + + A− Cx2 , 4Eb3 2Eb 4Eb3
F x12 3Fνx1 x22 u2 (x1 , x2 ) = − − + B + Cx1 . 3 4Eb 4Eb3
(9.31)
Physically, the constants A, B, and C describe rigid body displacements in the x1 and x2 directions and a counterclockwise rotation about the x3 axis. Possible approximate boundary conditions that may be applied to determine these constants are u1 = u2 = ∂u2 /∂ x1 = 0 at x1 = a, x2 = 0, or
u1 = u2 = ∂u1 /∂ x2 = 0 at x1 = a, x2 = 0, or b b b u1 dx2 = u2 dx2 = x2 u1 dx2 = 0 at x1 = a.
−b
−b
(9.32)
−b
The choice of boundary condition here is motivated by additional consideration of the actual conditions that may prevail in the physical system.
9.4 Beam Problems with Body Force Potentials An example is now considered that involves a body force potential, in particular one that accounts for the gravitational potential associated with selfweight. The simple beam is illustrated in Fig. 9.2; the boundary conditions are described below. As throughout the text, ρ is the mass density, and we introduce g as the gravitational acceleration constant. Thus, the body force potential is V(x1 , x2 ) = ρgx2 ,
(9.33)
9.4. Body Force Potentials
189
where x2 may be reckoned from any convenient reference level. This gives rise to the body force density f=−
∂V = −ρge2 . ∂x
(9.34)
The governing equation for φ for the case of plane stress is, in this case, ∇ 4 φ = −(1 − ν)∇ 2 V = 0.
(9.35)
The boundary conditions can be phrased as σ12 (x1 , ±b) = σ22 (x1 , ±b) = 0,
σ11 (±a, x2 ) = 0, b
−b
σ12 (−a, x2 ) dx2 = −
(9.36) b −b
σ12 (a, x2 ) dx2 = −2ρgba.
At this point it is fruitful to consider the symmetry that is obvious in the system. For example, for the normal stresses, σnn (x1 , x2 ) ∼ σnn (−x1 , x2 ) ⇔ an even function of x1 , σnn (x1 , x2 ) ∼ −σnn (x1 , −x2 ) ⇔ an odd function of x2 .
(9.37)
With these considerations, a stress function of the form φ(x1 , x2 ) = c21 x12 x2 + c23 x12 x23 + c03 x23 + c05 x25 = odd in x2 , even in x1 ,
(9.38)
may be tried. Note the subscripting convention used for the coefﬁcients vis`avis the exponents of x1 and x2 . Since ∇ 4 (x12 x2 ) = ∇ 4 (x23 ) = 0,
(9.39)
the remaining part of (9.38) must satisfy ∇ 4 (c23 x12 x23 + c05 x25 ) = 0,
(9.40)
which leads to 24c23 x2 + 120c05 x2 = 0,
i.e.,
1 c05 = − c23 . 5
(9.41)
Consequently, the stresses are σ11 (x1 , x2 ) = ρgx2 + 6c23 x12 x2 + 6c03 x2 + 20c05 x23 , σ22 (x1 , x2 ) = ρgx2 + 2c21 x2 + 2c23 x23 ,
(9.42)
σ12 (x1 , x2 ) = −2c21 x1 − 6c23 x1 x22 . Next the boundary conditions are applied. For example, σ12 (x1 , b) = 0 = −2c21 x1 − 6c23 x1 b2 , σ22 (x1 , b) = 0 = ρgb + 2c21 b + 2c23 b3 .
(9.43)
190
9. Elastic Beam Problems
Observe the symmetry in σ12 and σ22 , viz., that σ12 is purely even in x2 and σ22 is purely odd in x2 . Thus, the boundary conditions applied on x2 = b above may be equally well applied on x2 = −b. Together they lead to 3 c21 = − ρg, 4 1 ρg c23 = , 4 b2 1 1 ρg c05 = − c23 = − . 5 20 b2
(9.44)
The boundary condition σ11 (±a, x2 ) = 0 cannot be satisﬁed point wise with a polynomial solution of the type considered here. Global equilibrium can, however, be guaranteed by setting
b
−b
σ11 dx2 = 0.
(9.45)
Because σ11 is an odd function of x2 , this condition supplies no information regarding the evaluation of the remaining coefﬁcient, c03 . However, equilibrium also requires that no net moment exist, and this leads to
b
−b
σ11 x2 dx2 = 0 on x1 = ±a.
(9.46)
Since σ11 is an even function in x1 , (9.46) can be applied at x1 = ±a. Doing so leads to 2 2 ρgb3 + ρga 2 b + 4c03 b3 − ρgb3 = 0, 3 5 1 1 2 + (a/b) . c03 = −ρg 15 4 The ﬁnal results for the stresses are then ρgb 2 2 2 3 2 2 b x2 − x2 + (x1 − a )x2 , σ11 (x1 , x2 ) = I 5 3 2 x23 b x2 ρgb + − , σ22 (x1 , x2 ) = I 3 3 σ12 (x1 , x2 ) =
(9.47)
(9.48)
ρgb 2 b x1 − x22 x1 , I
where I = 2b3 /3 is the crosssectional moment of inertia per unit thickness of the beam.
9.5 Beam under Fourier Loading The beam illustrated in Fig. 9.3 is to be subject to a general loading along its top surface (x2 = c) and along its bottom surface (x2 = −c). This loading is imagined to have been Fourier analyzed, as described in Chapter 3. Because of the linearity of the biharmonic
9.5. Fourier Loading
191
x2
x1
c
Figure 9.3. Fourier loading on a simple beam.
c
l
equation it sufﬁces to develop a general solution for the typical Fourier component. Thus, imagine the loading to be of the form σ22 (x1 , x2 = c) = −bm sin(αm x1 ), σ22 (x1 , x2 = −c) = −am sin(αm x1 ),
(9.49)
where αm = mπ/, m is an integer, and is the length of the beam, as indicated in Fig. 9.3. No body forces are considered and, therefore, solutions of the biharmonic equation ∇ 4φ = 0
(9.50)
are sought. Assume solutions of the form φm = sin(αm x1 ) f (x2 ).
(9.51)
When this is substituted into (9.50), the result, after cancelling a redundant sin(αmπ x1 ), is 4 2 αm f (x2 ) − 2αm f (x2 ) + f (x2 ) = 0.
(9.52)
In (9.52) another common convention has been used, namely that primes denote differentiation with respect to the obvious variable, e.g., f (x2 ) = d2 f/dx22 . General solutions to (9.52) are of the form f (x2 ) ∼ eαm x2 , e−αm x2 , x2 e±αm x2 .
(9.53)
It is efﬁcient to form solutions in the form of hyperbolic functions, i.e., f (x2 ) ∼ (eαm x2 + e−αm x2 ), (eαm x2 − e−αm x2 ),
(9.54)
f (x2 ) ∼ cosh αm x2 , sinh αm x2 .
(9.55)
or
A suitable stress function is φm = [C1m cosh(αm x2 ) + C2m sinh(αm x2 ) + C3m x2 cosh(αm x2 ) + C4m x2 sinh(αm x2 )] sin(αm x1 ).
(9.56)
This delivers the stresses as σ11 = ∂ 2 φ/∂ x22 2 2 = sin(αm x1 ){C1mαm cosh(αm x2 ) + C2mαm sinh(αm x2 )
+ C3mαm[2 sinh(αm x2 ) + αm x2 cosh(αm x2 )] + C4mαm[2 cosh(αm x2 ) + αm x2 sinh(αm x2 )]},
(9.57)
192
9. Elastic Beam Problems
σ22 = ∂ 2 φ/∂ x12 2 = −αm sin(αm x1 )[C1m cosh(αm x2 ) + C2m sinh(αm x2 )
(9.58)
+ C3m x2 cosh(αm x2 ) + C4m x2 sinh(αm x2 )], σ12 = −∂ 2 φ/∂ x1 ∂ x2 = −αm cos(αm x1 ){C1mαm sinh(αm x2 ) + C2mαm cosh(αm x2 ) + C3m[cosh(αm x2 ) + αm x2 sinh(αm x2 )]
(9.59)
+ C4m[sinh(αm x2 ) + αm x2 cosh(αm x2 )]}. The boundary condition σ12 (x1 , x2 = ±c) = 0 requires that C1mαm sinh(αmc) + C2mαm cosh(αmc) + C3m[cosh(αmc) + αmc sinh(αmc)]
(9.60)
+ C4m[sinh(αmc) + αmc cosh(αmc)] = 0, and −C1mαm sinh(αmc) + C2mαm cosh(αmc) + C3m[cosh(αmc) + αmc sinh(αmc)]
(9.61)
+ C4m[sinh(αmc) + αmc cosh(αmc)] = 0. When rearranged these provide the connections C3m = −C2m
αm cosh(αmc) , cosh(αmc) + αmc sinh(αmc)
αm sinh(αmc) . C4m = −C1m sinh(αmc) + αmc cosh(αmc)
(9.62)
On the other hand, the boundary condition given in (9.49) requires that 2 αm [C1m cosh(αmc) + C2m sinh(αmc)
+ C3mc cosh(αmc) + C4mc sinh(αmc)] = bm
(9.63)
and 2 αm [C1m cosh(αmc) − C2m sinh(αmc)
− C3mc cosh(αmc) + C4mc sinh(αmc)] = am.
(9.64)
Consequently, we obtain C1m =
am + bm sinh(αmc) + αmc cosh(αmc) , 2 αm sinh(2αmc) + 2αmc
C2m = −
am − bm cosh(αmc) + αmc sinh(αmc) , 2 αm sinh(2αmc) − 2αmc
αm cosh(αmc) am − bm , C3m = 2 αm sinh(2αmc) − 2αmc C4m = −
αm sinh(αmc) am + bm . 2 αm sinh(2αmc) + 2αmc
(9.65)
9.6. Complete BVP for Beams
193
Finally, for compactness of notation, deﬁne the functions χ1 = [αmc cosh(αmc) − sinh(αmc)] cosh(αm x2 ), χ2 = αm sinh(αmc)x2 sinh(αm x2 ), χ3 = [αmc sinh(αmc) − cosh(αmc)] sinh(αm x2 ), χ4 = αm cosh(αmc)x2 cosh(αm x2 ), χ5 = [αmc cosh(αmc) + sinh(αmc)] cosh(αm x2 ), χ6 = αm sinh(αmc)x2 sinh(αm x2 ), χ7 = [αmc sinh(αmc) + cosh(αmc)] sinh(αm x2 ), χ8 = αm cosh(αmc)x2 cosh(αm x2 ), χ9 = αmc cosh(αmc) sinh(αm x2 ), χ10 = αm sinh(αmc)x2 cosh(αm x2 ), χ11 = αmc sinh(αmc) cosh(αm x2 ), χ12 = αm cosh(αmc)x2 sinh(αm x2 ). With these deﬁnitions, the stresses become σ11 = (am + bm)
χ1 − χ2 sin(αm x1 ) sinh(2αmc) + 2αmc
− (am − bm)
σ22 = −(am + bm) + (am − bm)
σ12 = −(am + bm)
χ 3 − χ4 sin(αm x1 ), sinh(2αmc) − 2αmc χ5 − χ6 sin(αm x1 ) sinh(2αmc) + 2αmc χ 7 − χ8 sin(αm x1 ), sinh(2αmc) − 2αmc χ9 − χ10 cos(αm x1 ) sinh(2αmc) + 2αmc
χ11 − χ12 cos(αm x1 ). + (am − bm) sinh(2αmc) − 2αmc
(9.66)
(9.67)
(9.68)
9.6 Complete Boundary Value Problems for Beams In this section we consider a complete boundary value problem for a beam subject to a general Fourier loading, as illustrated in Fig. 9.4. The load applied to the upper surface is now σ yy = −q sin(nπ x/),
(9.69)
where is the length of the beam. Note that in this section coordinate notation has been changed from x1 , x2 to x, y. This is done to illustrate generality of common notations. The boundary conditions are as depicted in Fig. 9.4 and as applied explicitly below. As before,
194
9. Elastic Beam Problems
σyy
y 2h
Figure 9.4. Fourier component loading on a simple beam.
x
we require a stress potential φ satisfying the biharmonic equation ∇ 4 φ = 0.
(9.70)
As discussed in Chapter 3, trial solutions of the form φ ∼ eαx eβy , xeαx eβy , or yeαx eβy
(9.71)
are explored. When such terms are inserted into the biharmonic equation, there results the characteristic equation, α 4 + 2α 2 β 2 + β 4 = 0 ⇒ (α 2 + β 2 )2 = 0,
(9.72)
and thus α = ±iβ, where β can be either real or imaginary. Therefore, we obtain solutions of the form φ = eiβx Aeβy + Be−βy + Cyeβy + Dye−βy (9.73) + e−iβx A eβy + B e−βy + C yeβy + D ye−βy . Of course, the roles of x and y could be interchanged, i.e., x y, to obtain additional solutions. In addition, terms could be formed such as sinh(βy) = 1/2(eβy − e−βy ) or cosh(βy) = 1/2(eβy + e−βy ) by simply adding or subtracting exponential terms. At the end, we obtain φ = sin(βx)[Asinh(βy) + B cosh(βy) + Cβy sinh(βy) + Dβy cosh(βy)] + cos(βx)[A sinh(βy) + B cosh(βy) + C βy sinh(βy) + D βy cosh(βy)] + sin(αy)[E sinh(αx) + F cosh(αx) + Gαx sinh(αx) + Hαx cosh(αx)] + cos(αy)[E sinh(αx) + F cosh(αx) + G αx sinh(αx) + H αx cosh(αx)] + R0 + R1 x + R2 x 2 + R3 x 3 + R4 y + R5 y2 + R6 y3 + R7 xy + R8 x 2 y + R9 xy2 . The boundary conditions include σ yy (x, y = h) = −q sin(nπ x/),
σxy (x, y = h) = 0,
σ yy (x, y = −h) = σxy (x, y = −h) = 0, h 1 σxx (x = 0, y) = 0, σxy (x = 0, y) dy = − q sin(nπ x/) dx, 2 0 −h h 1 σxx (x = , y) = 0, σxy (x = , y) dy = q sin(nπ x/) dx. 2 0 −h
9.6. Complete BVP for Beams
195
These suggest for φ the following form φ = sin(βx) [Asinh(βy) + B cosh(βy) + Cβy sinh(βy) + Dβy cosh(βy)] . This form guarantees that σxx (x = 0, y) = 0. It will satisfy the boundary condition at x = , as well, if the values for β are determined as described below. For the stresses we obtain σ yy = −β 2 sin(βx) [Asinh(βy) + B cosh(βy) + Cβy sinh(βy) + Dβy cosh(βy)] ,
σxy = −β 2 cos(βx) Acosh(βy) + D[βy sinh(βy) + cosh(βy)]
− β 2 cos(βx) B sinh(βy) + C[βy cosh(βy) + sinh(βy)] . The terms have been arranged so that they are either odd or even in y. Thus, to meet the boundary condition σxy (x, y = ±h) = 0, we require Acosh(βh) + D[βh sinh(βh) + cosh(βh)] = 0, B sinh(βh) + C[βh cosh(βh) + sinh(βh)] = 0.
(9.74)
This leads to A = −D[βh tanh(βh) + 1] , B = −C [βh coth(βh) + 1] , and
σ yy = − Dβ 2 sin(βx) βy cosh(βy) − [βh tanh(βh) + 1] sinh(βy)
− Cβ 2 sin(βx) βy sinh(βy) − [βh coth(βh) + 1] cosh(βy) .
To ensure σ yy (x, y = −h) = 0, we set
D βh cosh(βh) − [βh tanh(βh) + 1] sinh(βh)
= C βh sinh(βh) − [βh coth(βh) + 1] cosh(βh) . Hence,
(9.75)
(9.76)
(9.77)
"
# βh cosh2 (βh) − βh sinh2 (βh) D − sinh(βh) cosh(βh) " # βh sinh2 (βh) − βh cosh2 (βh) − cosh(βh) . =C sinh(βh)
(9.78)
Since cosh2 (βh) − sinh2 (βh) = 1, we have C = − tanh(βh)
βh − sinh(βh) cosh(βh) D. βh + sinh(βh) cosh(βh)
(9.79)
Deﬁning, for compactness, the parameter ϒ ≡ tanh(βh)
βh − sinh(βh) cosh(βh) , βh + sinh(βh) cosh(βh)
(9.80)
196
9. Elastic Beam Problems
we can write σ yy = −Dβ 2 sin(βx) [βy cosh(βy) − (βh tanh(βh) + 1) sinh(βy)] + Dβ 2 sin(βx)ϒ [βy sinh(βy) − (βh coth(βh) + 1) cosh(βy)] .
(9.81)
Since σ yy (x, h) = −q sin(nπ x/), there follows q sin(nπ x/) = 2β 2 Dsin(βx)
βh − sinh(βh) cosh(βh) . cosh(βh)
(9.82)
For this to be true, we demand that β = nπ/
(9.83)
and D=
q cosh(nπ h/) , − sinh(nπ h/) cosh(nπ h/)]
2(nπ/)2 [nπ h/
C=−
q sinh(nπ h/) . 2(nπ/)2 [nπ h/ + sinh(nπ h/) cosh(nπ h/)]
(9.84)
It can be readily veriﬁed that indeed σxx (0, y) = σxx (, y) = 0. 9.6.1 Displacement Calculations Recall the connections between the stress potential and the stresses, viz., σxx =
∂ 2φ , ∂ y2
σ yy =
∂ 2φ , ∂ x2
σxy = −
∂ 2φ . ∂ x∂ y
(9.85)
For the two normal strains, and for the case of plane stress considered here, the straindisplacement relations are 1 ∂ 2φ ∂ux ∂ 2φ exx = = −ν 2 , ∂x E ∂ y2 ∂x (9.86) 2 ∂u y 1 ∂ φ ∂ 2φ = −ν 2 . e yy = ∂y E ∂ x2 ∂y When integrated, this yields
∂φ ∂ 2φ + f (y) , dx − ν ∂ y2 ∂x 2 1 ∂φ ∂ φ + g(x) , uy = dy − ν E ∂ x2 ∂y
ux =
1 E
(9.87)
where f (x) and g(y) are integration functions. Furthermore, for the shear strain, ∂u y ∂ux 2(1 + ν) ∂φ + =− . ∂y ∂x E ∂ x∂ y
(9.88)
Now, substitute (9.87) into (9.88) and use exponential forms for φ of the type φ ∼ eαx eβy , i.e., ignore polynomial like terms, to obtain 3 β /α + 2αβ + α 3 /β eαx eβy + f (y) + g (x) = 0. (9.89)
9.6. Complete BVP for Beams
Observe that
197
∂ 3φ ∂ 2φ + dx + 2 3 ∂y ∂ x∂ y
∂ 3φ dy + f (y) + g (x) = 0. ∂ x3
(9.90)
But, β 3 /α + 2αβ + α 3 /β = β 4 + 2α 2 β 2 + α 4 = 0,
(9.91)
f (y) + g (x) = 0 ⇒ f (y) = g (x) = −ω.
(9.92)
from (9.72), and thus
Therefore, we have f (y) = −ωy + u0x , g(x) = −ωx + u0y .
(9.93)
The displacements are accordingly ux (x, y) = −
1 β cos(βx){A(1 + ν) sinh(βy) + B(1 + ν) cosh(βy) E
+ C[(1 + ν)βy sinh(βy) + 2 cosh(βy)]
(9.94)
+ D[(1 + ν)βy cosh(βy) + 2 sinh(βy)]} − ω0 y + u0x , and u y (x, y) = −
1 β sin(βx){A(1 + ν) cosh(βy) + B(1 + ν) sinh(βy) E
+ C[(1 + ν)βy cosh(βy) − (1 + ν) sinh(βy)]
(9.95)
+ D[(1 + ν)βy sinh(βy) − (1 − ν) cosh(βy)]} + ω0 x + u0y . Now, referring to Fig. 9.4, set u y (0, 0) = u y (, 0) = ux (0, 0) = 0
(9.96)
ω0 = u0y = 0
(9.97)
to obtain
and u0x =
1 β[B(1 + ν) + 2C]. E
(9.98)
More general loading, speciﬁed by say k(x), may be analyzed by Fourier analysis and by applying linear superposition. If k(x) is an odd function, the solution just obtained will be sufﬁcient; if not, a similar solution involving a boundary condition such as σ yy (x, y = h) = q cos(nπ/) will be required. The generation of such a solution would follow precisely along the lines of the one obtained above.
198
9. Elastic Beam Problems
9.7 Suggested Reading Little, R. W. (1973), Elasticity, Prentice Hall, Englewood Cliffs, New Jersey. Sokolnikoff, I. S. (1956), Mathematical Theory of Elasticity, 2nd ed., McGrawHill, New York. Timoshenko, S. P., and Goodier, J. N. (1970), Theory of Elasticity, 3rd ed., McGrawHill, New York. Ugural, A. C., and Fenster, S. K. (2003), Advanced Strength and Applied Elasticity, 4th ed., Prentice Hall, Upper Saddle River, New Jersey.
10 Solutions in Polar Coordinates
10.1 Polar Components of Stress and Strain We introduce a polar coordinate system as illustrated in Fig. 10.1. The polar coordinates r, θ are related to the cartesian coordinates x, y by θ = tan−1 (y/x)
(10.1)
y = r sin θ.
(10.2)
r = (x 2 + y2 )1/2 , or, through their inverse, x = r cos θ, Thus, derivatives can be formed via
∂r ∂ ∂θ ∂ ∂ sin θ ∂ ∂ = + = cos θ − , ∂x ∂ x ∂r ∂ x ∂θ ∂r r ∂θ ∂ ∂r ∂ ∂θ ∂ ∂ cos θ ∂ = + = sin θ + . ∂y ∂ y ∂r ∂ y ∂θ ∂r r ∂θ
(10.3)
For second derivatives we obtain 1 ∂ sin θ ∂ 2 1 ∂2 ∂2 ∂ ∂2 2 2 − + 2 2 = cos θ = cos θ 2 + sin θ ∂ x2 ∂r r ∂θ ∂r r ∂r r ∂θ 1 ∂2 1 ∂ − , + 2 sin θ cos θ r 2 ∂θ r ∂r ∂θ 1 ∂ cos θ ∂ 2 1 ∂2 ∂2 ∂ ∂2 2 2 + + 2 2 = sin θ = sin θ 2 + cos θ ∂ y2 ∂r r ∂θ ∂r r ∂r r ∂θ 1 ∂ 1 ∂2 − − 2 sin θ cos θ , r 2 ∂θ r ∂r ∂θ ∂2 = sin θ cos θ ∂ x∂ y
∂2 1 ∂2 1 ∂ − − ∂r 2 r ∂r r 2 ∂θ 2
1 ∂ 1 ∂2 − − (cos θ − sin θ) 2 r ∂θ r ∂r ∂θ 2
2
.
199
200
10. Solutions in Polar Coordinates σ θθ
y
σ θr
eθ
σ rr
er
σ rr
σr θ
r θ x
σ θθ
σ rθ
Figure 10.1. The stress components in 2D polar coordinates.
σ θr
Another need is to express the components of stress, strain, and displacement in terms of the polar coordinates. This is done with the help of Fig. 10.1 that illustrates the deﬁnitions of the polar stress components. For example, σrr = σxx cos2 θ + σ yy sin2 θ + 2σxy sin θ cos θ = cos2 θ
∂ 2φ ∂ 2φ ∂ 2φ + sin2 θ 2 − 2 sin θ cos θ 2 ∂y ∂x ∂ x∂ y
(10.4)
1 ∂ 2φ 1 ∂φ + 2 2. r ∂r r ∂θ In an entirely similar fashion it is found that =
σθ θ =
∂ 2φ ∂r 2
and σr θ
1 ∂ 2φ ∂ 1 ∂φ − =− = 2 r ∂θ r ∂r ∂θ ∂r
(10.5)
1 ∂φ r ∂θ
.
(10.6)
We now need to construct the ﬁeld equations, in particular the biharmonic equation. The Laplacian, in this 2D (x, y) frame, is formed as 1 ∂2 ∂2 ∂2 ∂2 1 ∂ 2 + + = ∇ = + , ∂ x2 ∂ y2 ∂r 2 r ∂r r 2 ∂θ 2
(10.7)
and, thus, ∇ =∇ ∇ = 4
2
2
1 ∂2 ∂2 1 ∂ + + ∂r 2 r ∂r r 2 ∂θ 2
2 .
(10.8)
As for displacements, we appeal to the deﬁnitions of unit base vectors in the polar geometry er = cos θ ex + sin θ e y , eθ = − sin θ ex + cos θ e y ,
(10.9)
and write ux = ur cos θ − uθ sin θ, u y = ur sin θ + uθ cos θ.
(10.10)
For the strains we note, for example, that uθ ∂ur ∂uθ 1 ∂ur 1 ∂uθ ur ∂ux exx = = cos2 θ + − − + sin θ cos θ + sin2 θ. ∂x ∂r r ∂r r ∂θ r r ∂θ (10.11)
10.2. Plate with Circular Hole
201
τ y
τ a Figure 10.2. Plate with a central hole.
x τ τ
The use of such relations leads to the following expressions for the polar strain components ∂ur , ∂r ∂uθ uθ 1 1 ∂ur + − , = 2 r ∂θ ∂r r
err = er θ
eθ θ =
(10.12)
ur 1 ∂uθ + . r ∂θ r
10.2 Plate with Circular Hole 10.2.1 Far Field Shear As an example, consider an inﬁnite plate containing a circular hole, as illustrated in Fig. 10.2. The plate is assumed to be loaded by far ﬁeld shear, which would represent a uniform pure shear had it not been for the hole. Thus at inﬁnite distance from the hole the state of stress is to reduce to uniform pure shear, and the stress state is nonuniform near the hole. We seek solutions of the biharmonic equation that can account for this state of loading. Try solutions of the form φ(r, θ) =
∞ n=0
fn (r ) cos(nθ) +
∞
gn (r ) sin(nθ).
(10.13)
n=1
Substitution into the biharmonic equation ∇ 4 φ = 0 yields 2 2
d n2 1 d − 2 fn (r ), gn (r ) = 0. + 2 dr r dr r
(10.14)
Solutions are of two forms, i.e., fn (r ) = An1r n+2 + An2r −n+2 + An3r n + An4r −n ,
n = 0, 1,
(10.15)
and f0 (r ) = A01r 2 + A02r 2 ln r + A03 ln r + A04 ,
n = 0,
f1 (r ) = A11r 3 + A12r ln r + A13r + A14r −1 ,
n = 1.
(10.16)
Similar solutions exist for gn (r ). These solution forms may be used to construct the solution. Because the surface of the hole is traction free, the boundary condition there becomes σrr = σθr = 0 on r = a,
(10.17)
202
10. Solutions in Polar Coordinates
whereas far from the hole σxy → τ
as r → ∞,
(10.18)
where τ is the magnitude of the remotely applied shear stress. Because the far ﬁeld stress state is pure shear, σxx , σ yy → 0 as r → ∞.
(10.19)
The problem is most easily solved by using an elementary application of the principle of linear superposition. We imagine two problems, one of a homogeneous plate subject to pure far ﬁeld shear and that of a plate with a hole whose surface is subject to traction; the traction to be imposed in this second problem will be such as to precisely annihilate the traction that would exist on a circular surface of the same radius in the homogeneous plate of the ﬁrst problem. When the two solutions are added, the hole’s surface becomes traction free. Moreover, as will be seen, the stresses of the second problem vanish far from the hole, so that the far ﬁeld stress state for the combined problems becomes only the uniform pure shear of the ﬁrst problem. For problem (1), involving pure uniform shear, we take r2 τ sin(2θ), (10.20) 2 which clearly produces a simple state of uniform pure shear stress of magnitude τ . The corresponding stresses are φ (1) = −τ xy = −τr 2 sin θ cos θ = −
σrr(1) = τ sin(2θ),
(1)
σr θ = τ cos(2θ).
(10.21)
In problem (2) we apply the stresses σrr = −τ sin(2θ) and σr θ = −τ cos(2θ) to the surface of the hole. To accomplish this, consider potential of the form φ (2) (r, θ) = Asin(2θ) + Br −2 cos(2θ),
(10.22)
which is from the inventory listed in (10.15) and (10.16). The choice of functions involving sin(2θ) and cos(2θ) may be taken as arrived at by trial and error, but is clearly motivated by similar term in the boundary conditions. The stresses associated with this potential are 4A 6B σrr(2) = − + sin(2θ), r2 r4 2A 6B (2) (10.23) cos(2θ), + σr θ = r2 r4 (2)
σθ θ = (2)
6B sin(2θ). r4 (2)
Next, by evaluating σrr (r = a) and σr θ (r = a) and setting the results equal to −τ sin(2θ) and −τ cos(2θ), respectively, it is found that A = τ a 2 and B = −τ a 4 /2. The combined stresses, therefore, become σrr = σrr(1) + σrr(2) = τ 1 − 4a 2 /r 2 + 3a 4 /r 4 sin(2θ), (1) (2) (10.24) σr θ = σr θ + σr θ = τ 1 + 2a 2 /r 2 − 3a 4 /r 4 cos(2θ), (1) (2) σθ θ = σθ θ + σθ θ = −τ 1 + 3a 4 /r 4 sin(2θ).
10.2. Plate with Circular Hole
203
It is interesting to examine the implications of such solutions vis`avis stress concentrations. Of particular interest is the normal stress that occurs at a perimeter of the hole corresponding to θ = 3π/4, where sin(2θ) = −1. The maximum hoop stress there is σθ θ = 4τ . As the state of stress at this point is uniaxial tension, because σrr = σr θ = 0 on the hole’s surface, the maximum shear stress at this point is simply τmax = 2τ . 10.2.2 Far Field Tension The second problem of this type that is of interest involves an identical plate subject to far ﬁeld tension (or compression). Thus the boundary conditions are the same as (10.17) on the surface of the hole, but become σxx → σ
at r → ∞.
(10.25)
At r → ∞ all other components of stress vanish. The problem may be solved using an identical superposition approach. For the ﬁrst problem we imagine a homogeneous plate subject to uniform far ﬁeld tension; the potential corresponding to this state of stress is φ (1) =
1 2 1 1 σ y = σ r 2 sin2 θ = σ [r 2 − r 2 cos(2θ)]. 2 2 4
(10.26)
Consider a second potential prescribed as φ (2) = Aσ ln r + Bσ cos(2θ) + Cσ r −2 cos(2θ),
(10.27)
so that, when the two solutions are combined, φ=
1 σ [r 2 − r 2 cos(2θ)] + Aσ ln r + Bσ cos(2θ) + Cσ r −2 cos(2θ). 4
The stresses computed from this potential are A 4B cos(2θ) 6C cos(2θ) 1 cos(2θ) , + + 2− − σrr = σ 2 2 r r2 r4 sin(2θ) 2B sin(2θ) 6C sin(2θ) σr θ = −σ + + , 2 r2 r4 A 6C cos(2θ) 1 cos(2θ) − − 2+ . σθ θ = σ 2 2 r r4
(10.28)
(10.29)
In setting the boundary condition σrr (r = a) = 0, note that two equations are generated from the ﬁrst of (10.29), viz., A 1 + 2 = 0, 2 a 1 4B 6C − 2 − 4 = 0. 2 a a
(10.30)
These arise from the need to independently set the terms involving cos(2θ) to zero. The second traction free boundary condition gives rise to a single equation 1 2B 6C + 2 + 4 = 0. 2 a a
(10.31)
204
10. Solutions in Polar Coordinates
When the equations are solved, we ﬁnd A = −a 2 /2,
B = a 2 /2,
C = −a 4 /4.
(10.32)
The resulting stresses are 4a 2 σ cos(2θ) 3a 4 a2 − 2 +1 , 1− 2 + r 2 r4 r 4 σ sin(2θ) 3a 2a 2 = − −1 , 2 r4 r2 σ σ cos(2θ) 3a 4 a2 1+ 2 − = +1 . 2 r 2 r4
σ σrr = 2 σr θ σθ θ
(10.33)
Of particular interest is the stress concentration at the point on the hole’s surface at = 3σ . θ = ±π/2. The maximum hoop stress there is σθmax θ
10.3 Degenerate Cases of Solution in Polar Coordinates We again seek solutions to the equation ∇ φ= 4
∂2 1 ∂2 1 ∂ + + ∂r 2 r ∂r r 2 ∂θ 2
2 φ=0
(10.34)
in the form φ=
∞
fn (r ) cos(nθ) +
n=0
∞
gn (r ) sin(nθ).
(10.35)
n=1
We examine the terms involving cos(nθ) for the moment. This leads to
d2 n2 1 d − + dr 2 r dr r2
2 fn (r ) = 0.
(10.36)
In general, solutions exist of the type fn (r ) = An1r n+2 + An2r −n+2 + An3r n + An4r −n ,
(10.37)
as we have seen previously. But, if n = 0, two sets of solutions become degenerate, viz., (An1r n+2 , An2r −n+2 ) and (An3r n , An4r −n ). If, on the other hand, n = 1, two other solutions become degenerate, viz., (An2r −n+2 , An3r n ). In such cases we seek to ﬁnd a resolution in terms of alternative solutions to replace those that are degenerate. Let n = 1 + , that is relax the condition that n be an integer. Then the two potentially degenerate forms for n = 1 become f (r ) = Ar 1− + Br 1+ ,
(10.38)
and as → 0 the two forms become degenerate. Now, recast f (r ) as f (r ) = C(r 1+ + r 1− ) + D(r 1+ − r 1− ).
(10.39)
10.3. Degenerate Cases
205
In the limit as → 0, we clearly have lim C(r 1+ + r 1− ) → 2Cr,
→0
lim D(r 1+ − r 1− ) → 0.
(10.40)
→0
Take D = E −1 and form again the limit to ﬁnd that lim E −1 (r 1+ − r 1− ) → Er ln r.
(10.41)
f1 (r ) = A11r 3 + A12r ln r + A13r + A14r −1 .
(10.42)
→0
Thus, for n = 1,
For n = 0, we ﬁnd d(r n+2 ) = r 2 ln r, n→0 dn lim
d(r n ) = ln r, lim n → 0 dn
(10.43)
so that f0 (r ) = A01r 2 + A02r 2 ln r + A03 ln r + A04 .
(10.44)
There are, however, additional aspects of the analysis. When n = 0, there are solutions of the form φ = A, for which there are no stresses. We want instead solutions that give rise to stresses of the Fourier form, which would come about, say, from potentials of the type φ = Ar cos(θ ) + Br sin(θ ),
(10.45)
lim [Ar cos(θ ) + Br sin(θ )] = A.
(10.46)
with the limit →0
Furthermore, lim
→0
d [Ar cos(θ ) + Br sin(θ )] = Aln r + Bθ. d
(10.47)
The term Bθ yields stresses σrr = σθ θ = 0,
σr θ = B/r 2 .
(10.48)
When n = 1, the terms in r cos θ and r sin θ yield no stresses; a similar procedure uncovers the alternative solution φ = Br θ sin θ + Cr θ cos θ,
(10.49)
which has the associated stresses σr θ = σθ θ = 0,
σrr =
2B cos θ 2C sin θ − . r r
(10.50)
206
10. Solutions in Polar Coordinates
The general solution of interest is, therefore, φ(r, θ) = A01r 2 + A02r 2 ln r + A03 ln r + A04 θ + A11r 3 + A12r ln r + A14r −1 cos θ + A13r θ sin θ + B11r 3 + B12r ln r + B14r −1 sin θ + B13r θ cos θ +
∞
An1r n+2 + An2r −n+2 + An3r n + An4r −n cos(nθ)
(10.51)
n=2
+
∞
Bn1r n+2 + Bn2r −n+2 + Bn3r n + Bn4r −n sin(nθ).
n=2
It should not go unnoticed that terms r θ sin θ and r θ cos θ are not single valued. This is a feature we exploit in the next section.
10.4 Curved Beams: Plane Stress Consider the equations of equilibrium. In polar coordinates, for cases of plane stress, we have σrr − σθ θ 1 ∂σr θ ∂σrr + + + br = 0, ∂r r r ∂θ 2σr θ 1 ∂σθ θ ∂σr θ + + + bθ = 0. ∂r r r ∂θ
(10.52)
As before, if there are no body forces, the Airy stress function satisﬁes ∇ 4φ = ∇ 2∇ 2φ =
1 ∂2 ∂2 1 ∂ + + ∂r 2 r ∂r r 2 ∂θ 2
2 φ = 0.
(10.53)
The connections to the stress components are σrr =
1 ∂ 2φ 1 ∂φ + 2 2, r ∂r r ∂θ
∂ 2φ , ∂r 2 ∂ 1 ∂φ =− . ∂r r ∂θ
σθ θ = σr θ
(10.54)
The straindisplacement relations are ∂ur , ∂r ∂uθ uθ 1 1 ∂ur + − = , 2 r ∂θ ∂r r
err = er θ
eθ θ =
ur 1 ∂uθ + . r ∂θ r
(10.55)
10.4. Curved Beams
207
To complete the set of governing equations, the elastic constitutive relations for plane stress are used, 1 (σrr − νσθ θ ), E 1 = (σθ θ − νσrr ), E 1+ν σr θ . = E
rr = θ θ r θ
(10.56)
Consider solutions of a form that are dependent solely on r , i.e., φ = φ(r ) only. In this case, and using again the convention whereby a comma denotes differentiation, the biharmonic equation, in the absence of body forces, reduces to & 1 1 = 0. (10.57) r (r φ,r ),r r r ,r ,r
This equation may be integrated four times in a straightforward manner to yield
1 r (r φ,r ),r r
,r
= C1 ,
1 (r φ,r ),r = C1 ln r + C2 , r r φ,r = C1
r2 r2 ln r − 2 2
φ,r = C1 r ln r + C2 r + C3 /r, φ = C1
+ C2
C1 = C1 /2,
r2 r2 ln r − 2 2
+ C2
r2 + C3 , 2 C2 = (C2 − C1 )/2,
r2 + C3 ln r + C4 . 2
In a slightly simpler form, the last expression becomes φ = Aln r + Br 2 ln r + Cr 2 + D.
(10.58)
This form for φ gives rise to stresses σrr = A/r 2 + 2B ln r + 2C, σθ θ = −A/r 2 + 2B ln r + 3B + 2C,
(10.59)
σr θ = 0. As for the strains, ﬁrst note that er θ
1+ν 1 σr θ = = E 2
1 ∂ur ∂uθ uθ + − r ∂θ ∂r r
= 0.
(10.60)
208
10. Solutions in Polar Coordinates
The radial strain is err =
1 ∂ur = ∂r E
A(1 + ν) + 2C(1 − ν) + B(1 − ν)(2 ln r + 1) − 2ν B . r2
(10.61)
For the hoop strain we ﬁnd 1 ∂uθ ur + r r ∂θ 1 A(1 + ν) = + 2C(1 − ν) + B(1 − ν)(2 ln r − 1) + 2B . − E r2
eθ θ =
(10.62)
Equations (10.61) and (10.62) provide two paths for evaluating ur . Integrating (10.61) it is found that A(1 + ν) 1 + 2C(1 − ν)r + B(1 − ν)(2r ln r − r ) − 2ν Br + f (θ), − ur = E r where f (θ) is an arbitrary function of integration. Solving for ur in (10.62), on the other hand, gives A(1 + ν) 1 + 2C(1 − ν)r + B(1 − ν)(2r ln r + r ) + 2Br − ∂uθ /∂θ. − ur = E r For last two expressions to be both expressions for ur , it must be that f (θ) = −∂uθ /∂θ + 4Br/E.
(10.63)
∂uθ /∂θ = 4Br/E → uθ = 4Br θ/E.
(10.64)
If we take f (θ) = 0, we obtain
With this choice for f (θ), (10.60) shows that ∂ur /∂θ = 0, as expected and as is consistent with the original assumption that ur = ur (r ) only. Note also, if such nonsingle valued solutions as uθ = (1/E)(4Br θ) are disallowed, B = 0. The corresponding strains are 1 A(1 + ν) dur (10.65) = + 2C(1 − ν) + B(1 − ν)(2 ln r + 1) − 2ν B , err = dr E r2 and eθ θ =
1 ur A(1 + ν) = + 2C(1 − ν) + B(1 − ν)(2 ln r + 1) + 2B . − r E r2
(10.66)
To derive the radial displacement, integrate the ﬁrst of these and solve the second to obtain 1 A(1 + ν) + 2C(1 − ν)r + B(1 − ν)(2r ln r − r ) − 2ν Br + Y, ur = − E r where Y is a constant, and 1 A(1 + ν) + 2C(1 − ν)r + B(1 − ν)(2r ln r + r ) + 2Br . ur = − E r For these two expressions to be the same, we must have B = Y = 0.
10.4. Curved Beams
209
po b
p
a
Figure 10.3. Hollow cylinder subject to imposed internal and external pressure.
i
10.4.1 Pressurized Cylinder Consider the case of a hole in a thin plate subject to both external and internal pressure, as depicted in Fig. 10.3. The boundary conditions are σrr = − pi on r = a, σrr = − p0 on r = b.
(10.67)
Take for the potential φ = Aln r + Cr 2 + D,
(10.68)
which gives the stresses σrr = A/r 2 + 2C, σθ θ = −A/r 2 + 2C,
(10.69)
σr θ = 0. Setting the boundary conditions prescribed above gives σrr (r = a) = A/a 2 + 2C = − pi , σrr (r = b) = A/b2 + 2C = − p0 .
(10.70)
When these are solved for A and C, it is found that σrr = σθ θ
a 2 b2 p0 − pi a 2 pi − b2 p0 + , b2 − a 2 r2 b2 − a 2
a 2 b2 p0 − pi a 2 pi − b2 p0 =− 2 + . b − a2 r2 b2 − a 2
(10.71)
Some interesting special cases are obtained as follows. Let t = (b − a) and Rm = (b + a)/2; this means that, for example, b = Rm +
t , 2
a = Rm −
t , 2
b2 − a 2 = 2t Rm .
Now, let p0 = 0 and assume t/Rm 1. Then, 2 pi Rm t Rm 2 ). σθ θ = + O(t 2 /Rm 1+ 2 − 2t r Rm
(10.72)
(10.73)
210
10. Solutions in Polar Coordinates
β M
Figure 10.4. Curved beam under the bending moment M.
b M
a
Recall the simple membrane approximation, viz., σθ θ ≈ pi Rm /t for the nominal stress across the annulus wall of such a cylinder with a central hole. This may be obtained from (10.73) by neglecting the term t/Rm and evaluating the expression at r = Rm .
10.4.2 Bending of a Curved Beam Consider the curved beam shown in Fig. 10.4. The beam is loaded at its ends by a bending moment M. The boundary conditions to be imposed are σrr = σr θ = 0 on r = a, b, σθ θ dr = 0 at θ = ±β,
(10.74)
σθ θ r dr = −M at θ = ±β. As the beam does not close on itself, it is possible to accept solutions that are characterized by nonsingle valued displacements, uθ . Thus the coefﬁcient B in (10.58) may not be zero! Consequently, by using (10.58), evaluating the stresses, and setting the above boundary conditions, it is found that A/a 2 + 2B ln a + B + 2C = 0, A/b2 + 2B ln b + B + 2C = 0, b A/b2 + 2B ln b + B + 2C − a A/a 2 + 2B ln a + B + 2C = 0, − Aln(b/a) + B b2 ln b − a 2 ln a + C(b2 − a 2 ) = −M. Solving the above, we ﬁnd 4M 2 2 a b ln(b/a), D 2M 2 (b − a 2 ), B=− D M 2 [(b − a 2 ) + 2(b2 ln b − a 2 ln a)], C= D A= −
D = (b2 − a 2 )2 − 4a 2 b2 ln(b/a).
(10.75)
10.5. Axisymmetric Deformations
211
The corresponding stresses are 4M a 2 b2 2 2 ln(b/a) + b ln(r/b) + a ln(a/r ) , D r2 2 2 4M a b =− − 2 ln(b/a) + b2 ln(r/b) + (b2 − a 2 ) , D r
σrr = − σθ θ
(10.76)
σr θ = 0.
10.5 Axisymmetric Deformations We have already encountered geometries where polar coordinates are particularly suited, namely those where the geometry is symmetric about some axis – we call that, as before, the z axis. Here we explicitly consider some cases of such axisymmetry. Suppose that the displacements are independent of the polar coordinate θ. If it happens that the stress potential is also independent of θ, then the biharmonic equation for φ becomes
d4 2 d3 1 d2 1 d + − + 3 4 3 2 2 dr r dr r dr r dr
φ = 0.
(10.77)
General solutions to this reduced equation have already been developed, but an alternative approach is to introduce a change in coordinates to ξ , where ξ is deﬁned, via the polar coordinate r , as r = eξ .
(10.78)
In this case (10.77) is simpliﬁed to
d4 d3 d2 − 4 + 4 dξ 4 dξ 3 dξ 2
φ = 0.
(10.79)
The general solution, in terms of ξ and r , is φ = Aξ e2ξ + Be2ξ + Cξ + D = Ar 2 ln r + Br 2 + C ln r + D.
(10.80)
We next recall the connections between the polar components of stress and the stress potential, viz., relations (10.4), (10.5), and (10.6), which when specialized to the axisymmetric case considered here are σrr =
1 dφ , r dr
σθ θ =
d2 φ , dr 2
σr θ = 0.
(10.81)
212
10. Solutions in Polar Coordinates
Substituting (10.80) into (10.81), we obtain C + A+ 2B, r2 C = 2Aln r − 2 + 3A+ 2B, r
σrr = 2Aln r + σθ θ
(10.82)
σr θ = 0. For solutions of this type in a simply connected body, e.g., a solid cylinder, the constants A and C must be zero so that the stresses are bounded at r = 0. For a multiply connected body, e.g., a hollow cylinder, this is not required. For such cases, we must examine the displacement ﬁeld, as has been done earlier. For the case of axisymmetry, relations (10.12) reduce to dur , dr ur = , r
err = eθ θ
(10.83)
er θ = 0. The constitutive relations become, for the case of plane stress (σzz = 0), dur 1 = (σrr − νσθ θ ), dr E ur 1 = (σθ θ − νσrr ). r E
(10.84)
For plane strain, the moduli become 1/E ← (1 − ν 2 )/E and ν ← ν/(1 − ν 2 ), while σzz = ν(σrr + σθ θ ). Using relations (10.82) in (10.84), we ﬁnd from the ﬁrst of (10.84) that 1 C C dur = 2Aln r + 2 + A+ 2B − ν 2Aln r − 2 + 3A+ 2B . dr E r r When integrated, this becomes C 1 C 2Ar ln r − Ar + 2Br − − ν 2Ar ln r + Ar + 2Br + +H , ur = E r r where H is an integration constant. The second of (10.84), on the other hand, gives 1 ur C C = 2Aln r − 2 + 3A+ 2B − ν 2Aln r + 2 + A+ 2B . r E r r When the two expressions for ur are equated, there follows 4Ar − H = 0,
(10.85)
which leads to the conclusion that A = H = 0. For axisymmetric deformations, there is no circumferential displacement (uθ = 0), and the equations of equilibrium, in the absence of body forces, lead directly to ur d2 ur 1 dur − 2 = 0, + 2 dr r dr r
(10.86)
10.6. Suggested Reading
213
Figure 10.5. Hollow cylinder subject to an imposed displacement on its inner circular surface. The outer surface at r = b is ﬁxed.
which has the general solution 1 ur = Kr + S . (10.87) r As an example, consider the case of a hollow cylinder, as in Fig. 10.5, that is subject to an imposed displacement, u0 , on its inner surface. The outer surface is ﬁxed. Thus, the boundary conditions are ur = u0 on r = a, and ur = 0 on r = b. This leads from the above to the solution 2 b au0 −r . (10.88) ur = 2 b − a2 r The strains and stresses may now be calculated directly.
10.6 Suggested Reading Doghri, I. (2000), Mechanics of Deformable Solids, SpringerVerlag, Berlin. FilonenkoBorodich, M. (1964), Theory of Elasticity, Noordhoff, Groningen, Netherlands. Fung, Y.C. (1965), Foundations of Solid Mechanics, Prentice Hall, Englewood Cliffs, New Jersey. Little, R. W. (1973), Elasticity, Prentice Hall, Englewood Cliffs, New Jersey. Love, A. E. H. (1944), A Treatise on the Mathematical Theory of Elasticity, Dover, New York. Muskhelishvili, N. I. (1963), Some Basic Problems of the Mathematical Theory of Elasticity, Noordhoff, Groningen, Netherlands. Sokolnikoff, I. S. (1956), Mathematical Theory of Elasticity, 2nd ed., McGrawHill, New York. Timoshenko, S. P., and Goodier, J. N. (1970), Theory of Elasticity, 3rd ed., McGrawHill, New York.
11 Torsion and Bending of Prismatic Rods
In this chapter we present the SaintVenant’s theory of torsion and bending of prismatic rods. We ﬁrst consider torsion of the prismatic rod by two concentrated torques at its ends, and then analyze bending of a cantilever beam by a concentrated transverse force at its end.
11.1 Torsion of Prismatic Rods We consider here the torsional deformation of prismatic rods subject to a torque or imposed angle of twist per unit length along the rod. The coordinate system, as illustrated in Fig. 11.1, has the z axis along the rod and the rod’s cross section in the xy plane. The rod is deformed such that adjacent crosssectional planes are rotated with respect to each other about the z axis; the angle of rotation φ is such that dφ = θdz where θ is the socalled twist, or angle of rotation per unit length along the rod’s axis. The deformation is assumed to be inﬁnitesimal in that θr 1, where r represents a characteristic transverse dimension of the rod. If the rotation is small, the change in a typical radius vector r, laying in a transverse plane, is given by δr = δφ × r,
(11.1)
where δφ = δφez is a vector along the z axis (measured from the mid cross section of the rod) and has a magnitude equal to the amount of rotation. The vectors r and δr are, respectively, r = xex + ye y , δr = ux ex + u y e y .
(11.2)
Because δφ = θ z, the components of the inplane displacement vector are ux = −θ zy,
u y = θ zx.
(11.3)
The rod will undergo deformation in the z direction, as well; this is assumed small and proportional to the twist θ. The displacement in the z direction is then given as uz = θ ψ(x, y), 214
(11.4)
11.1. Torsion of Prismatic Rods
215
l
C
M,φ
M,φ
x
M A
z
Figure 11.1. Prismatic rod in torsion. The applied torque is M, and the angle of rotation, relative to the midsection of the rod, is φ.
y
y
where ψ is a function of x, y, referred to as the torsion function. Thus each cross section of the rod becomes warped as it was originally ﬂat. The components of strain can be calculated from ∂u j 1 ∂ui . (11.5) + ei j = 2 ∂xj ∂ xi When this is done, the nonzero components of strain are ∂ψ ∂ψ 1 1 − y , e yz = θ +x . exz = θ 2 ∂x 2 ∂y
(11.6)
The application of the isotropic linear elastic constitutive relations shows that the two nonzero components of stress are ∂ψ ∂ψ − y , σ yz = 2µe yz = µθ +x . (11.7) σxz = 2µexz = µθ ∂x ∂y Given that only σxz and σ yz are nonzero, the equations of equilibrium reduce to ∂σxz ∂σ yz + = 0, ∂x ∂y
(11.8)
which, after substituting (11.7), becomes ∇ 2 ψ = 0,
(11.9)
where ∇ 2 is the Laplacian with respect to x, y. It is convenient at this stage to introduce two new stress potentials; the ﬁrst is deﬁned via its connection to the stresses as ∂χ ∂χ , σ yz = −2µθ . (11.10) σxz = 2µθ ∂y ∂x If (11.10) is compared to (11.7), the relations between ψ and χ are found to be ∂ψ ∂χ = y+2 , ∂x ∂y
∂ψ ∂χ = −x − 2 . ∂y ∂x
(11.11)
If the ﬁrst of (11.11) is differentiated with respect to y, and the second with respect to x, and the resulting equations subtracted, it is found that χ must satisfy the Poisson’s equation ∇ 2 χ = −1.
(11.12)
It remains to specify the boundary conditions to be applied to χ . We assume that the side surfaces of the rod are traction free, as indicated in Fig. 11.1. Thus, on the rod’s surface we have σ · n = 0 ⇒ σxznx + σ yzn y = 0,
(11.13)
216
11. Torsion and Bending of Prismatic Rods
y n dy
α
α
Figure 11.2. The unit normal n = {nx , n y } to an inﬁnitesimal arc of length dl. By geometry, nx = cos α = dy/dl and n y = sin α = −dx/dl.
dl
 dx Ο
x
where n is the outward pointing normal to the rod’s side surface, and nx and n y are its x and y components. When (11.10) is substituted into the above it is found that ∂χ ∂χ nx − n y = 0. ∂y ∂x
(11.14)
If d is an increment of arc length around the circumference of the rod then the normal’s components are also given by the relations nx = dy/d and n y = −dx/d (Fig. 11.2). Using these in (11.14), it is found that ∂χ dχ ∂χ dx + dy = dχ = 0 = d. ∂x ∂y d
(11.15)
In other words, χ is a constant along the circumference. Since the stresses (and strains) are related to derivatives of χ , the constant in question may be taken as zero, χ = 0 on the edges of cross section.
(11.16)
This result holds for a simply connected rod, i.e., one possessing a single, continuous outer edge.
11.2 Elastic Energy of Torsion We examine here the elastic energy of torsion. The elastic energy density is given as W=
1 1 2 σi j ei j = σxzexz + σ yze yz = (σ 2 + σ yz ), 2 2µ xz
or, in terms of χ,
" W = 2µθ
2
∂χ ∂x
2
+
∂χ ∂y
(11.17)
2 # = 2µθ 2 (grad χ )2 ,
(11.18)
where grad is the gradient with respect to the inplane coordinates x, y. The total elastic energy is obtained by integration of W over the volume of the rod. The energy per unit length along the rod is 1 W = 2µθ 2 (grad χ )2 dA = Cθ 2 . (11.19) 2 A The constant C is the torsional rigidity, because the applied moment is linear in the twist, i.e., M ∝ θ, and thus 1 (11.20) W = M dθ = Cθ dθ = Cθ 2 . 2 This deﬁnes C as the torsional rigidity in the relation M = Cθ.
11.3. Rectangular Cross Section
217
But, there is a relation (grad χ )2 = div (χ grad χ ) − χ ∇ 2 χ = div (χ grad χ ) + χ , which may be veriﬁed by noting that ∇ 2 χ = −1, and ∂ ∂χ ∂χ ∂χ + χ ∇ 2χ . χ = ∂xj ∂xj ∂xj ∂xj Thus,
C = 4µ
(11.21)
(11.22)
(grad χ ) dA = 4µ
[div (χ grad χ ) + χ ] dA.
2
A
(11.23)
A
The ﬁrst integral contained in (11.23) vanishes, which can be be seen by transforming it using the divergence theorem, ∂χ d = 0, div (χ grad χ ) dA = χ ∂n A C because χ = 0 on C. Thus, C is given by
C = 4µ
χ dA.
(11.24)
A
Finally, we introduce the second stress potential, ϕ, in analogy with the function used in the previous section, viz., ϕ ≡ 2µθ χ . In terms of ϕ the above equations become σxz = ∂ϕ/∂ y,
σ yz = −∂ϕ/∂ x,
∇ ϕ = −2µθ, M = 2 ϕ dA, 2
(11.25)
A
1 C=2 θ
ϕ dA. A
The function ϕ is known as the Prandtl stress function. In the next section we will use the Prandtl stress function and (11.25) as the basis for solving two classic torsional boundary value problems.
11.3 Torsion of a Rod with Rectangular Cross Section Let H ≡ −2µθ so that the governing equation for ϕ becomes ∇ 2 ϕ = H, ϕ=0
within C, on C.
(11.26)
We are concerned with a rectangular cross section, as illustrated in Fig. 11.3, so that x ≤ a and y ≤ b. The boundary conditions for ϕ are ϕ = 0 on x = ±a, y ≤ b and
ϕ = 0 on y = ±b, x ≤ a.
(11.27)
Deﬁne the function ϕ˜ as ϕ˜ ≡
1 H(x 2 − a 2 ), 2
(11.28)
218
11. Torsion and Bending of Prismatic Rods
Figure 11.3. Rod of rectangular cross section.
such that ∇ 2 ϕ˜ = H
(11.29)
ϕ˜ = 0 on x = ±a.
(11.30)
1 ϕ(x, y) = ϕ1 (x, y) + H(x 2 − a 2 ). 2
(11.31)
and
With so deﬁned ϕ, ˜ we express ϕ as
Thus, the boundary value problem is transformed into ∇ 2 ϕ1 = 0 on A, ϕ1 = 0 on x = ±a,
(11.32)
1 ϕ1 = − H(x 2 − a 2 ) on y = ±b. 2 We seek a solution by separation of variables as ϕ1 (x, y) = f (x)g(y).
(11.33)
Upon substitution into (11.32), we ﬁnd ∇ 2 ϕ1 = d2 f (x)/dx 2 g(y) + f d2 g(y)/dy2 = 0,
(11.34)
which, when rearranged, yields 1 2 1 d f/dx 2 = − d2 g/dy2 = −λ2 , f g
(11.35)
where λ is a constant. The two equations that follow for f (x) and g(y) are d2 f/dx 2 + λ2 f = 0, f (x) = Acos(λx) + B sin(λx),
(11.36)
and d2 g/dy2 − λ2 g = 0, g(y) = C cosh(λy) + Dsinh(λy).
(11.37)
11.3. Rectangular Cross Section
219
To proceed, we recall the connections to stresses and note that σxz should be an odd function of y, because of symmetry, and that σ yz should be an odd function of x, for the same reason. Thus, since σxz = ∂ϕ/∂ y = ∂ϕ1 /∂ y, and σ yz = −∂ϕ/∂ x = ∂ϕ1 /∂ x − Hx, we have B = D = 0 in (11.36) and (11.37). This means that ¯ cosh(λy) . ϕ1 (x, y) = Acos(λx)
(11.38)
Furthermore, by imposing the boundary condition on x = ±a, it is found that ϕ1 = 0 on x = ±a ⇒ nπ , n = 1, 3, 5, . . . . 2a
cos(λa) = 0 ⇒ λ =
(11.39)
The general solution is, therefore, ∞
ϕ1 (x, y) =
An cos
n=1,3,5,...
nπ x 2a
cosh
nπ y 2a
.
Imposing the boundary condition on y = ±b leads to ∞ nπ x nπb 1 cosh An cos = − H(x 2 − a 2 ). 2a 2a 2 n=1,3,5,...
(11.40)
(11.41)
x The constants An are easily determined by multiplying both sides of (11.41) by cos mπ 2a and integrating over [−a, a]. This yields a ∞ mπ x nπ x nπb cos dx An cosh cos 2a 2a 2a −a n=1,3,5,... (11.42) a mπ x 1 2 2 =− H dx. (x − a ) cos 2 2a −a Noting that
a
−a
cos
we deduce
Am cosh
nπ x 2a
cos
mπ x 2a
dx =
0,
if m = n,
a,
if m = n,
a mπ x mπb 1 (x 2 − a 2 ) cos dx , a=− H 2a 2 2a −a
(11.43)
(11.44)
i.e., Am =
16Ha 2 (−1)(m−1)/2 b . π 3 m3 cosh mπ 2a
(11.45)
Consequently, the function ϕ is 1 ϕ(x, y) = H(x 2 − a 2 ) 2 y x ∞ cosh nπ (−1)(n−1)/2 cos nπ 16Ha 2 2a 2a + . π 3 n=1,3,5,... n3 cosh nπb 2a
(11.46)
220
11. Torsion and Bending of Prismatic Rods
The corresponding stresses are 8Ha σxz = 2 π
∞
(−1)(n−1)/2 cos
nπ x
n=1,3,5,...
and ∞
8Ha σ yz = −Hx + 2 π
sinh
nπ y
2a b n2 cosh nπ 2a
(−1)(n−1)/2 sin
nπ x
2a
cosh
2a n2 cosh nπb 2a
n=1,3,5,...
,
(11.47)
nπ y 2a
.
(11.48)
Assume, with no loss in generality, that a ≤ b. The maximum shear stress then occurs at x = ±a, y = 0, and is equal to " # ∞ (−1)(n−1)/2 sin nπ 8 2 τmax = σ yz(a, 0) = −Ha 1 − 2 , (11.49) π n=1,3,5,... n2 cosh nπb 2a or, since sin
nπ 2
= 1 for the odd integer values of n involved, " # ∞ 1 8 b . τmax = σ yz(a, 0) = −Ha 1 − 2 π n=1,3,5,... n2 cosh nπ 2a
(11.50)
Here, it is convenient to write τmax = −Hak, k=1− The applied moment is
8 π2
∞ n=1,3,5,...
(11.51)
1 b . cosh nπ 2a
n2
ϕ dA
M=2 A
= H2b +
a
−a
(x 2 − a 2 ) dx
32Ha 2 π3
where
I(a, b, n) =
∞
(−1)(n−1)/2 I(a, b, n) , n3 cosh nπb n=1,3,5,... 2a
a −a
(11.52)
cos
nπ x 2a
dx
b
−b
cosh
nπ y 2a
dy.
When the simple integrations are done, we ﬁnd " b# ∞ tanh nπ 1 (2a)3 (2b) 192 a 2a M=− H . 1− 5 2 3 π b n=1,3,5,... n5
(11.53)
(11.54)
Once again, it is convenient to deﬁne a factor ∞ tanh nπb 192 a 2a k1 (b/a) = 1 − 5 , π b n=1,3,5,... n5
(11.55)
11.4. Elliptical Cross Section
221
so that 1 (2a)3 (2b) k1 (b/a). M=− H 2 3 With these, the maximum shear stress can be expressed as τmax = −Hak =
2Mak M (k/k1 ) = (2a)3 (2b)k1 (2a)2 (2b) M 1 , = k2 (2a)2 (2b)
(11.56)
(11.57)
where k2 = k1 /k. We list a table of computed values for the factors k, k1 and k2 . b/a 1.0 2.0 3.0 4.0 5.0 ∞
k 0.675 0.930 0.985 0.997 0.999 1.0
k1 0.1406 0.229 0.263 0.281 0.291 0.333
k2 0.208 0.246 0.267 282 0.291 0.333
11.4 Torsion of a Rod with Elliptical Cross Section Consider a rod with an elliptical cross section as shown in Fig. 11.4. The rod’s periphery is given as y2 x2 + − 1 = 0. a2 b2 A suitable stress function is
(11.58)
x2 y2 ϕ = B 2 + 2 −1 , a b
(11.59)
where the constant B is readily determined by substitution of (11.59) into the governing equation developed previously. The result of this is H = ∇ 2 ϕ = 2B
a 2 + b2 , a 2 b2
a 2 b2 . ⇒ B=H 2(a 2 + b2 ) The torsional moment is computed from
M=2
ϕ dA, A
y
A
Figure 11.4. Elliptical cross section of a rod subjected to torsion.
b a
x
(11.60)
(11.61)
222
11. Torsion and Bending of Prismatic Rods
which gives H=−
2(a 2 + b2 ) M. a 3 b3 π
(11.62)
For the stresses, we obtain σxz =
∂ϕ 2y M, =− ∂y πab3
2x ∂ϕ = σ yz = − M. ∂x πab3
(11.63)
Without loss of generality, assume that b < a; in that case the maximum shear stress occurs at y = b, and is given by τmax =
2M . πab2
(11.64)
The evaluation of the displacement function, uz(x, y), is straightforward and leads to the result uz(x, y) =
M b2 − a 2 xy. G πa 3 b3
(11.65)
In the case of a circular cross section, i.e., where a = b, there is no longitudinal displacement so that uz(x, y) = 0. The only nonvanishing component of stress is the shear stress
σzθ =
M r, I0
I0 =
πa 4 . 2
(11.66)
11.5 Torsion of a Rod with Multiply Connected Cross Sections We have shown that the stress function, ϕ, must be constant on the boundary (or boundaries) of a rod whose side surfaces are stress free. For a simply connected shaft, i.e., a solid shaft, the constant was set to 0. For a multiply connected cross section in a hollow shaft, ϕ is also to be constant, but the constant values on the various contours of the cross section are not the same. Such a geometry is depicted in Fig. 11.5.
y
A2
C2
R C1
x
Figure 11.5. Cross section of a multiply connected rod subject to torsion. R denotes the area of the load bearing cross section between in the inner surface contour C2 , and the outer surface contour C1 . Note the continuous sense of the contour integration.
11.5. Multiply Connected Cross Sections
223
To establish the augmented boundary conditions on ϕ, consider the contour integral of the warping displacement, ∂uz ∂uz dx + dy . (11.67) duz = 0 = ∂x ∂y C2 C2 The integral is equal to 0 because uz is a single valued function. If we substitute from (11.7), we obtain 1 duz = (σxz dx + σ yz dy) − θ (x dy − y dx) G C2 C2 C2 (11.68) 1 τ ds − 2θA2 . = G C2 In (11.68) the third integral is easily seen, via Green’s theorem, to be equal to 2 A2 , where A2 is the area bounded by the inner contour C2 . To recall Green’s theorem in this context, we write ∂M ∂N − (M dy + N dx) dx dy = ∂x ∂y A2 C2 and set M = x and N = −y. The quantity τ is the magnitude of the shear stress, i.e., τ = −σxzn y + σ yznx , along the tangent to the contour, which becomes τ =−
dϕ , dn
(11.69)
where n is the unit normal to the contour C2 . As the stress function must be constant on both the inner and outer contours, (11.68) supplies the additional condition to determine its constant value ϕ0 on C2 . The value of ϕ on the outer boundary, C1 , may still be taken as 0. Thus, in addition to the boundary condition ϕ = 0 on C1 , ϕ must satisfy τ ds = 2GθA2 on C2 . (11.70) C2
The moment is readily computed from (σ yz x − σxz y) dx dy M= R
=− R
∂ϕ ∂ϕ x+ y dx dy. ∂x ∂y
(11.71)
This may be rewritten as M=− R
∂(xϕ) ∂(yϕ) + dx dy + 2 ϕ dx dy, ∂x ∂y R
(11.72)
and transformed, via Green’s theorem, to M = − (xϕ dy − yϕ dx) − (xϕ dy − yϕ dx) C1
C2
ϕ dx dy.
+2 R
(11.73)
224
11. Torsion and Bending of Prismatic Rods
y
R
A2
b
kb
Figure 11.6. Cross section of a hollow ellipsoidal rod.
x ka k b.
(11.77)
This solution may readily be veriﬁed by substitution into the governing equation and boundary conditions developed earlier in this chapter.
11.6. Bending of a Cantilever
225 Figure 11.7. A cantilever beam under bending by a concentrated force at its end z = l. The principal centroidal axes of the cross section are x and y. The shear force V passes through the shear center S.
11.6 Bending of a Cantilever Consider a cantilever beam under a transverse force V at its right end, parallel to one of the principal centroidal directions of the beam’s cross section (y direction in Fig. 11.7). The force passes through the socalled shear center S of the cross section, causing no torsion of the beam. The centroid of the cross section is the point O. The reactive force and bending moment at the left end of the beam are V and Vl, where l is the length of the beam. The bending moment at an arbitrary distance z from the left end of the beam is Mx = −V(l − z) .
(11.78)
Adopting the SaintVenant’s semiinverse method, assume that the normal stress σzz is distributed over the cross section in the same manner as in the case of pure bending, i.e., σzz =
Mx V(l − z) y=− y, Ix Ix
(11.79)
where Ix = A y2 dA is the moment of inertia of the crosssectional area A for the x axis. Because the lateral surface of the beam is traction free, we also assume that throughout the beam σxx = σ yy = σxy = 0 .
(11.80)
The objective is, thus, to determine the remaining nonvanishing stress components σzx and σzy . In the absence of body forces, the equilibrium equations reduce to ∂σzy ∂σzx = 0, = 0, ∂z ∂z ∂σzy ∂σzx V + = − y. ∂x ∂y Ix
(11.81)
These are satisﬁed by introducing the stress function =
(x, y) ,
(11.82)
such that σzx =
∂ , ∂y
σzy = −
V 2 ∂ − y + f (x) , ∂x 2Ix
(11.83)
where f (x) is an arbitrary function of x. To derive the governing equation for , we resort to the Beltrami–Michell’s compatibility equations (8.86). Four of them are identically
226
11. Torsion and Bending of Prismatic Rods
satisﬁed by the above assumptions, whereas the remaining two are 1 1+ν 1 ∇ 2 σzy + 1+ν
∇ 2 σzx +
∂σzz = 0, ∂ x∂z ∂σzz = 0. ∂ y∂z
(11.84)
Upon the substitution of (11.83), these become ∂ (∇ 2 ) = 0 , ∂y ∂ ν V + f (x) . (∇ 2 ) = − ∂x 1 + ν Ix
(11.85)
Thus, ∇2
=−
ν V x + f (x) + c . 1 + ν Ix
(11.86)
The constant c can be given a geometric interpretation. By using Hooke’s law and the above stress expressions, it can be shown that the longitudinal gradient of the material rotation ωz = (u y,x − ux,y )/2 is ∂ezy ∂ezx 1 ∂σzy ∂σzx 1 ν V ∂ωz = − = − =− x−c , ∂z ∂x ∂y 2G ∂ x ∂y 2G 1 + ν Ix where G is the shear modulus. We can deﬁne bending without torsion by requiring that the mean value of the relative rotation of the cross sections ∂ωz/∂z over the crosssectional area is equal to zero, 1 ∂ωz dA = 0 . (11.87) A A ∂z In the considered problem, this is fulﬁlled if we take c = 0 in (11.86). The local twist at the point of the cross section is then ν V ∂ωz =− x. ∂z E Ix
(11.88)
The traction free boundary condition on the lateral surface of the beam nx σzx + n y σzy =
dy dx σzx − σzy = 0 , ds ds
(11.89)
where n = {nx , n y } is the unit outward normal to the boundary C of the cross section, gives dx V 2 d = − . (11.90) y + f (x) ds 2Ix ds An inﬁnitesimal arc length along the boundary c is ds. In each particular problem (shape of the cross section), the function f (x) will be conveniently chosen, such that along the boundary C, V 2 y − f (x) = 0 . 2Ix
(11.91)
11.7. Elliptical Cross Section
227
This yields = const. along the boundary. Since stresses depend on the spatial derivatives of , the value of the constant is immaterial, and we may take = 0 on C. Thus, the boundaryvalue problem for the stress function is =−
∇2
ν V x + f (x) 1 + ν Ix
within C ,
(11.92)
= 0 on C . After solving this boundaryvalue problem, the shear stresses follow from (11.83). At the end cross sections of the cantilever, they must satisfy the integral boundary conditions
σzx dA = 0 ,
σzy dA = V ,
A
A
(11.93)
(xσzy − yσzx ) dA = Ve , A
where e represents the horizontal distance between the shear center S and the centroid O of the cross section.
11.7 Elliptical Cross Section The equation of the boundary of an elliptical cross section is x2 y2 + 2 − 1 = 0, 2 a b
(11.94)
where a and b are the semiaxes of the ellipse. The boundary condition choosing f (x) =
Vb2 2Ix
1−
x2 a2
= 0 is met by
.
(11.95)
The partial differential equation (11.92) reads
∇
2
ν b2 + 2 =− 1+ν a
V x. Ix
(11.96)
Both, the boundary condition and this equation can be satisﬁed by taking = Bx
x2 y2 + − 1 . a2 b2
(11.97)
The constant B is readily found to be
Vb2 B=− 2Ix
b2 +
ν
1+ν 3b2 + a 2
a2 .
(11.98)
228
11. Torsion and Bending of Prismatic Rods
The corresponding shear stresses are obtained from (11.83) as
σzx
σzy
Vxy =− Ix ⎡ Vb2 = 2Ix
b2 +
ν
1+ν 3b2 + a 2 1
a2
a ⎢ 2b + ⎢ 1+ν ⎢ ⎣ 3b2 + a 2 2
, 2
1−
y2 b2
⎤ x2 ⎥ 1 − 2ν ⎥ − ⎥. 1 + ν 3b2 + a 2 ⎦
(11.99)
The magnitude of the maximum shear stress component σzx is ν a2 b2 + Vab 1 + ν max σzx = , (11.100) 2Ix 3b2 + a 2 √ √ and it occurs at the points x = ±a/ 2, y = ±b/ 2. The maximum shear stress component σzy is
max σzy
Vb2 = 2Ix
2b2 +
1
1+ν 3b2 + a 2
a2 ,
(11.101)
occurring at the point x = y = 0 (center of the ellipse). In the case of a circular cross section (a = b = R), we have V 1 + 2ν xy , π R4 1 + ν
1 V 2 2 2 (3 + 2ν)(R = − y ) − (1 − 2ν) x . 2π R4 1 + ν
σzx = − σzy
(11.102)
11.8 Suggested Reading Cook, R. D., and Young, W. C. (1999), Advanced Mechanics of Materials, 2nd ed., Prentice Hall, Upper Saddle River, New Jersey. FilonenkoBorodich, M. (1964), Theory of Elasticity, P. Noordhoff, Groningen, Netherlands. Landau, L. D., and Lifshitz, E. M. (1986), Theory of Elasticity, 3rd English ed., Pergamon Press, New York. Little, R. W. (1973), Elasticity, Prentice Hall, Englewood Cliffs, New Jersey. Sokolnikoff, I. S. (1956), Mathematical Theory of Elasticity, 2nd ed., McGrawHill, New York. Timoshenko, S. P., and Goodier, J. N. (1970), Theory of Elasticity, 3rd ed., McGrawHill, New York.
12 SemiInﬁnite Media
In this chapter solutions involving general types of loading on halfspaces are considered. Such solutions are developed using Fourier transforms. The media are taken to be elastically isotropic. Solutions for anisotropic elastic media are considered in subsequent chapters.
12.1 Fourier Transform of Biharmonic Equation Consider a biharmonic function, φ, that satisﬁes the equation ∇ 4φ =
∂ 4φ ∂ 4φ ∂ 4φ + 2 + = 0. ∂ x4 ∂ x 2 ∂ y2 ∂ y4
Introduce the Fourier transform in y, viz., ∞ φ(x, y)eiαy dy, (x, α) = −∞
and its inverse φ(x, y) =
1 2π
∞
−∞
(x, α)e−iαy dα.
(12.1)
(12.2)
(12.3)
It is noted here that the transform of φ is formed without the factor of (2π)−1/2 ; accordingly the inverse transform contains a factor (2π)−1 . Apply the Fourier transform to the biharmonic equation (12.1), i.e., ∞ 2 2 ∞ 4 ∞ 4 ∂ φ iαy ∂ ∂ ∂ φ iαy iαy e dy + 2 φe dy + e dy = 0. (12.4) 4 2 2 4 −∞ ∂ x −∞ ∂ x ∂ y −∞ ∂ y The differentiation with respect to x may be taken outside the integrals, and after applying the Fourier transform results from above, it is found that 2 ∂4 2∂ + 2(−iα) + (−iα)4 ∂ x4 ∂ x2 2 ∂4 2∂ − 2α + α4 ∂ x4 ∂ x2
= 0, (12.5)
= 0. 229
230
12. SemiInﬁnite Media y r θ
Figure 12.1. Normal loading on the surface of a halfplane.
x
With α > 0, the general solution is (x, α) = (A+ Bx)e−αx + (C + Dx)eαx .
(12.6)
When concerned with developing solutions to other problems in solid mechanics, such solutions will occasionally be written as (x, α) = (A+ Bx)e−αx + (C + Dx)eαx .
(12.7)
The transforms of the stresses are ∞ ∂ 2φ σxx = ⇒ σxx eiαy dy = (−iα)2 (x, α) = −α 2 (x, α), ∂ y2 −∞ σxy
∂ 2φ ⇒ =− ∂ x∂ y
σ yy =
∂ 2φ ⇒ ∂ x2
∞ −∞
∞
−∞
−
∂ 2 φ iαy ∂ e dy = iα , ∂ x∂ y ∂x
(12.8)
∂ 2 φ iαy ∂2 e dy = . ∂ x2 ∂ x2
The inverse transforms follow immediately as ∞ 1 σxx = − α 2 (x, α)e−iαy dα, 2π −∞ σxy
1 = 2π
σ yy
1 = 2π
∞
−∞
∞
−∞
iα
∂ (x, α) −iαy e dα, ∂x
(12.9)
∂ 2 (x, α) −iαy e dα. ∂ x2
12.2 Loading on a HalfPlane Consider the half space deﬁned by x ≥ 0, as depicted in Fig. 12.1. The loading is speciﬁed by σxx = − p(y) on x = 0,
(12.10)
which describes a state of general normal loading on the external surface of the half space. There are no shear forces on this external surface, so that the other boundary condition is σxy = 0 on
x = 0.
(12.11)
12.2. Loading on a HalfPlane
231
The nature of the loading, p(y), is such that it produces bounded stresses. Inﬁnitely far into the bulk of the medium the stresses must be bounded, so that σαβ ∞
as
x → ∞.
(12.12)
As there are no body forces or temperature gradients, the Airy stress function satisﬁes the simple form of the biharmonic equation ∇ 4 φ = 0.
(12.13)
Introduce the Fourier transform of φ in the spatial variable y, viz., ∞ (x, α) = φ(x, y)eiαy dy, −∞
with an inverse 1 φ(x, y) = 2π
∞
(x, α)e−iαy dα.
−∞
The acceptable solutions for the transform,
(12.14)
(12.15)
(x, α), are of the form
(x, α) = (A+ Bx)e−αx + (C + Dx)eαx .
(12.16)
Next, invoke the boundary conditions speciﬁed above. First, form the Fourier transform of the normal loading boundary condition on x = 0, we have ∞ 2 ∞ ∂ φ iαy σxx eiαy dy = e dy 2 −∞ −∞ ∂ y (12.17) ∞ = −α 2 (x = 0, α) = −
−∞
p(y)eiαy dy = −P(α),
and
∞
−∞
σxy e
iαy
dy = −
∞
−∞
∂ (x, α) ∂ 2 φ iαy e dy = iα = 0. ∂ x∂ y ∂x x=0
(12.18)
Since the stresses need to be bounded at x → ∞, it is clear that C = D = 0,
(12.19)
whereas the transformed boundary conditions of (12.17), and (12.18) require that −α 2 A = −P(α) and
0 = B − αA.
(12.20)
This leads to A = P(α)/α 2 The result for
and
B = P(α)/α.
(12.21)
(x, α) is then (x, α) =
P(α) (1 + αx) e−αx . α2
(12.22)
232
12. SemiInﬁnite Media
The solution for the stresses is consequently ∞ 1 σxx (x, y) = − P(α) ( 1 + αx ) e−αx−iαy dα, 2π −∞ ∞ i xα P(α)e−αx−iαy dy, σxy (x, y) = − 2π −∞ ∞ 1 P(α) ( 1 − αx ) e−αx−iαy dα. σ yy (x, y) = − 2π −∞
(12.23)
There are two special cases of particular interest, viz., that arising if P(α) is symmetric or antisymmetric. If symmetric, P(α) = P(−α), then 2 ∞ P(α) ( 1 + αx ) e−αx cos(αy) dα, σxx (x, y) = − π 0 2x ∞ (12.24) σxy (x, y) = − α P(α)e−αx sin(αy) dα, π 0 2 ∞ P(α) ( 1 − αx ) e−αx cos(αy) dα, σ yy (x, y) = − π 0 with
∞
P(α) =
p(y) cos(αy) dy.
(12.25)
0
If, conversely, P(α) = −P(−α), the integrals in (12.23) become 2 ∞ P(α) ( 1 + αx ) e−αx sin(αy) dα, σxx (x, y) = − π 0 2x ∞ α P(α)e−αx cos(αy) dα, σxy (x, y) = π 0 2 ∞ P(α) ( 1 − αx ) e−αx sin(αy) dα, σ yy (x, y) = − π 0 with
P(α) =
(12.26)
∞
p(y) sin(αy) dy.
(12.27)
0
12.3 HalfPlane Loading: Special Case As a particularly interesting special case, consider loading on the external surface of a halfplane of the form p0 , if y ≥ 0, (12.28) p(y) = 0, if y < 0. The planar polar coordinates, to be used later to express the resulting stresses, are shown in Fig. 12.2. Consider the auxiliary function deﬁned as δ+ (α) =
1 1 δ(α) − , 2 2πiα
(12.29)
12.3. HalfPlane Loading
233
y r
p o
Figure 12.2. Normal loading on a halfplane surface.
θ x
where δ(α) is the Dirac delta function (see Chapter 3), and note that ∞ 1, if y ≥ 0 1 ∞ sin(αy) 1 −iαy dα = δ+ (α)e dα = + 2 π 0 α 0, if y < 0. −∞
(12.30)
Thus, take P(α) = 2π p0 δ+ (α), so that 1 p(y) = 2π
∞
−∞
(12.31)
2π p0 δ+ (α)e
−iαy
dα =
p0 ,
if y ≥ 0
0,
if y < 0.
(12.32)
From (12.23), the stresses become ∞ δ+ (α)e−αx−iαy ( 1 + αx ) dα σxx = − p0 −∞
p0 p0 =− − 2 π
∞ 0
(1 + αx) e−αx sin(αy) dα. α
(12.33)
Reducing this integral results in 1 xy σxx = − p0 1 − tan−1 (x/y) + . π π (x 2 + y2 )
(12.34)
Because θ = tan−1 (y/x), i.e., x = r cos θ and y = r sin θ, and noting that cot θ = tan(π/2 − θ), we can rewrite (12.34) as 1 θ 1 + + sin(2θ) . (12.35) σxx = − p0 2 π 2π By a similar set of manipulations, it is found that θ 1 1 + − sin(2θ) , σ yy = − p0 2 π 2π
(12.36)
and σxy =
p0 cos2 θ. π
(12.37)
Note that on the external surface, x = 0, i.e., θ = π/2, σxx = − p0 ,
σ yy = − p0 ,
σxy = 0.
(12.38)
234
12. SemiInﬁnite Media y r1
(x,y)
a θ r2 θ2
p o
r θ1 Figure 12.3. Symmetric loading on a halfplane surface.
x
a
This means that on the loading plane there exists a state of inplane hydrostatic pressure. It is also noted that rays emanating from the origin, at constant θ, are contours of equal stress.
12.4 Symmetric HalfPlane Loading Consider the case where the loading on the halfplane is conﬁned to a region symmetrically located about y = 0. By simple shifting of the position of the origin along the line x = 0, any situation involving a patch of loading as shown in Fig. 12.3 is embodied in this solution. Thus, if the loading is speciﬁed as
− p0 , if − a ≤ y ≤ a,
σxx =
0,
otherwise,
(12.39)
we have P(α) =
∞
−∞
p(y)eiαy dy =
∞
p(y) cos(αy) dy 0
=
0
a
sin(αa) . p0 cos(αy) dy = p0 α
(12.40)
The use of (12.24) results in σxx = −
2 p0 π
0
∞
1 + αx −αx e sin(αa) cos(αy) dα, α
2 p0 x ∞ −αx e sin(αa) sin(αy) dα, π 0 2 p0 ∞ 1 − αx −αx e =− sin(αa) cos(αy) dα. π 0 α
σxy = − σ yy
(12.41)
In terms of the polar angles in Fig. 12.3, it is readily shown that σxx = −
p0 [ cos(2θ2 ) − cos(2θ1 ) ] , 2π p0 =− [ 2(θ1 − θ2 ) + sin(2θ1 ) − sin(2θ2 ) ] . 2π
σxy = σ yy
p0 [ 2(θ1 − θ2 ) − sin(2θ1 ) + sin(2θ2 ) ] , 2π (12.42)
12.5. Alternative Approach
y
θ x r
235
Figure 12.4. Normal loading on a halfplane surface.
As r → ∞, θ1 → θ2 and thus σi j → 0. Note also that the maximum shear stress, 1/2 1 2 (σxx − σ yy )2 + σxy τmax = , (12.43) 4 becomes
p0 (12.44) τmax = sin(θ1 − θ2 ) . π Thus, contours of sin(θ1 − θ2 ) = constant are contours of equal maximum shear stress.
12.5 HalfPlane Loading: Alternative Approach The boundary value problem speciﬁed on a halfplane by (12.10)–(12.12) is revisited here and solved via application of the convolution theorem discussed in Chapter 3. To emphasize the alternative √ approach, a change in coordinate deﬁnitions is used. In addition, the use of the factor 1/ 2π is made both in the deﬁnition of the Fourier transform and its inverse. Recall that the state of general loading on the external surface of the halfplane y = 0 (Fig. 12.4) is speciﬁed as σ yy =
∂ 2φ = p(x), ∂ x2
(12.45)
σxy = 0 . The Fourier transform of the Airy stress function, φ(x, y), and its inverse are ∞ 1 φ(x, y)eiβx dx, (β, y) = √ 2π −∞ ∞ 1 φ(x, y) = √ (β, y)e−iβx dβ. 2π −∞ In the absence of body forces, the transform tion
(12.46)
satisﬁes the transformed biharmonic equa
2 ∂4 2∂ − 2β + β4 ∂ y4 ∂ y2
= 0.
(12.47)
The boundary conditions on y = 0 result in − β2
= P(β), (12.48)
∂ = 0, ∂y where P(β) is the transform of p(x), viz., 1 P(β) = √ 2π
∞ −∞
p(x)eiβx dx.
(12.49)
236
12. SemiInﬁnite Media
As in the previous section, it is noted that solutions of (12.47) that give rise to bounded stresses at x, y → ∞ are of the form (β, y) = ( A+ Cβy ) e−βy .
(12.50)
Upon application of (12.48), this leads to A = C = −P(β)/β 2 ,
(12.51)
and (β, y) = −
P(β) ( 1 + βy ) e−βy . β2
(12.52)
The transformed stresses are, therefore, (xx =
∂2 = P(β) ( 1 − βy ) e−βy , ∂ y2
(xy = iβ
∂ = P(β) ( iβy ) e−βy , ∂y
( yy = −β 2
= P(β) ( 1 + βy ) e−βy .
The inverse transform of ( 1 − βy )e−βy is
F −1 ( 1 − βy )e−βy = 23/2 π −1/2 x 2 y(x 2 + y2 )−2 = g(x, y), that is 1 G(β) = √ 2π 1 g(x, y) = √ 2π
∞ −∞
(12.55) G(β, y)e
−iβx
dβ.
Similarly, for σ yy we obtain
F −1 ( 1 + βy )e−βy = 23/2 π −1/2 y3 (x 2 + y2 )−2 , whereas for σxy ,
(12.54)
g(x, y)eiβx dx = ( 1 − βy )e−βy ,
∞ −∞
(12.53)
F −1 iβye−βy = 23/2 π −1/2 xy2 (x 2 + y2 )−2 .
Next, recall the convolution theorem from Chapter 3, ∞ ∞ −iβx F(β)G(β)e dβ = g(η) f (x − η) dη, −∞
−∞
(12.56)
(12.57)
(12.58)
and make the association of the functions for σxx , i.e., g(η) ⇔ p(η) and This gives σxx
G(β) ⇔ P(β).
∞ 1 =√ P(β) ( 1 − βy ) e−βy e−iβx dβ 2π −∞ 2y ∞ (x − η)2 p(η) dη. = π −∞ [(x − η)2 + y2 ]2
(12.59)
12.6. Additional Solutions
237
Similar manipulations, involving the stresses σxy and σ yy , result in σxy =
2y2 π
∞ −∞
(x − η) p(η) dη, [(x − η)2 + y2 ]2
(12.60)
p(η) dη. [(x − η)2 + y2 ]2
(12.61)
and σ yy
2y3 = π
∞ −∞
A particularly interesting example that lies within this framework is a point force (actually a line of concentrated forces). Without loss of generality, place the coordinate origin at the point of the application of the force. Taking p(x) to be p(x) = p0 δ(x), we ﬁnd σxx = −
2 p0 x 2 y 2 p0 cos2 θ sin θ = − , π(x 2 + y2 )2 π r
σxy = −
2 p0 xy2 2 p0 cos θ sin2 θ , = − π(x 2 + y2 )2 π r
σ yy = −
2 p0 y3 2 p0 sin3 θ . = − π(x 2 + y2 )2 π r
(12.62)
12.6 Additional HalfPlane Solutions This section offers additional solutions involving loading on a halfplane bounding a semiinﬁnite medium. The approach is different than used in the above two sections and thus the development details are provided, along with still another choice of variable names. This is done to distinguish the alternative approach employed. The general solutions are used vis`avis other speciﬁc forms of the loading function, p(y), as indicated in Fig. 12.1. Again, begin with the biharmonic equation ∇ 4 φ = 0,
(12.63)
and recall the deﬁnition of the Fourier transform ∞ φ(x, y)eiξ y dy, (x, ξ ) = F [φ(x, y)] = −∞
with its inverse φ(x, y) = F −1 [ (x, ξ )] =
1 2π
∞
(x, ξ )e−iξ y dy.
−∞
(12.64)
(12.65)
Since ∂2 = (−iξ )2 , ∂ y2 we have
∞
−∞
∇ φ(x, y)e 2
iξ y
dy =
∂2 − ξ2 ∂ x2
(12.66)
∞
−∞
φ(x, y)eiξ y dy.
(12.67)
238
12. SemiInﬁnite Media
To form the biharmonic form, we apply the operator ∇ 2 again to obtain 2 2 ∞ ∞ ∂ 4 iξ y 2 ∇ φ(x, y)e dy = −ξ φ(x, y)eiξ y dy. ∂ x2 −∞ −∞
(12.68)
Thus, ∇ 4 φ = 0 implies
∂2 − ξ2 ∂ x2
2 (x, ξ ) = 0.
(12.69)
This has been seen to have solutions of the form (x, ξ ) = (A+ Bx)e−ξ x + (C + Dx)eξ x . For the transformed stresses we then obtain ∞ ∞ 2 ∂ φ iξ y (xx = σxx eiξ y dy = e dy = −ξ 2 (x, ξ ), 2 −∞ −∞ ∂ y ∞ ∞ ∂ 2 φ iξ y ∂ (x, ξ ) (xy = e dy = iξ , σxy eiξ y dy = − ∂ x∂ y ∂x −∞ −∞ ∞ ∂ 2φ σ yy eiξ y dy = . ( yy = ∂ x2 −∞ The inversions are
∞ 1 ξ 2 (x, ξ )e−iξ y dξ, 2π −∞ ∞ 1 ∂ −iξ y e iξ dξ, σxy (x, y) = 2π −∞ ∂ x ∞ 2 ∂ 1 e−iξ y dξ. σ yy (x, y) = 2π −∞ ∂ x 2
(12.70)
(12.71)
σxx (x, y) = −
(12.72)
12.6.1 Displacement Fields in HalfSpaces For the case of plane strain, the isotropic elastic constitutive laws lead to E ∂v = σ yy − ν(σxx + σ yy ), 1 + ν ∂y
(12.73)
where v is the ycomponent of displacement. The Fourier transform of this displacement gradient is ∞ ∞ ∞ E ∂v iξ y e dy = σ yy eiξ y dy − ν (σxx + σ yy )eiξ y dy, (12.74) −∞ 1 + ν ∂ y −∞ −∞ which yields iξ E − 1+ν
∞
−∞
iξ E ν v(x, y) 1+ν ∂2 ∂2 2 = − ν −ξ + . ∂ x2 ∂ x2
v(x, y)eiξ y dy = −
(12.75)
12.6. Additional Solutions
239
By taking the inverse, we have E 1 v(x, y) = 1+ν 2π
∞
−∞
∂2 (1 − ν) 2 + νξ 2 ∂x
ie−iξ y
dξ . ξ
In view of the deﬁnition of shear strain and the elastic constitutive relation, ∂u ∂v E = σxy , + 2(1 + ν) ∂ y ∂ x we thus obtain 1 E u(x, y) = 1+ν 2π
∂3 dξ 2∂ (1 − ν) 3 + (2 + ν)ξ e−iξ y 2 . ∂ x ∂ x ξ −∞
(12.76)
(12.77)
∞
(12.78)
12.6.2 Boundary Value Problem As in the earlier sections, boundary conditions are applied that correspond to normal loading on the external surface on a semiinﬁnite medium. They are, in the context of the deﬁnitions used here, σxx = − p(y), σi j
σxy = 0
bounded as
on
x = 0,
x, y → ∞.
(12.79)
The latter of (12.79) leads to the conclusion that, with reference to (12.70), C = D = 0. The ﬁrst two conditions of (12.79) lead to ∞ 2 − ξ A= − p(y)eiξ y dy = P(ξ ), −∞ (12.80) B − ξ A = 0. Consequently, A = P(ξ )/ξ 2 ,
B = P(ξ )/ξ ,
(12.81)
P(ξ ) [1 + ξ x] e−ξ x . ξ2
(12.82)
and (x, ξ ) =
The stresses may now be calculated as ∞ 1 P(ξ )e−ξ x−iξ y (1 + ξ x) dξ, σxx (x, y) = − 2π −∞ ∞ 1 P(ξ )e−ξ x−iξ y (1 − ξ x) dξ, σ yy (x, y) = − 2π −∞ ∞ i σxy (x, y) = − xξ P(ξ )e−ξ x−iξ y dξ. 2π −∞ Since there is an imposed state of plane strain here, σzz = ν(σxx + σ yy ), we have ∞ σzz(x, y) = −ν P(ξ )e−ξ x−iξ y dξ. −∞
(12.83)
(12.84)
240
12. SemiInﬁnite Media
For the displacements, it is found that dξ 1+ν ∞ u= , P(ξ )e−ξ x−iξ y [2(1 − ν) + ξ x] 2π E −∞ ξ  1+ν ∞ dξ . v=− i P(ξ )e−ξ x−iξ y [(1 − 2ν) − ξ x] 2π E −∞ ξ 
(12.85)
The above relations take on a rather simpliﬁed form when there exists symmetry in the loading function, p(y). For example, if p(y) = p(−y), then 2 ∞ σxx (x, y) = − P(ξ ) (1 + ξ x) e−ξ x cos(ξ y) dξ, π 0 2 ∞ (12.86) P(ξ ) (1 − ξ x) e−ξ x cos(ξ y) dξ, σ yy (x, y) = − π 0 2x ∞ σxy (x, y) = − ξ P(ξ )e−ξ x sin(ξ y) dξ. π 0 Correspondingly, the displacements are cos(ξ y) 2(1 + ν) ∞ dξ, u(x, y) = P(ξ )e−ξ x [2(1 − ν) + ξ x] πE ξ 0 2(1 + ν) ∞ sin(ξ y) v(x, y) = dξ, P(ξ )e−ξ x [1 − 2ν − ξ x] πE ξ 0
(12.87)
with P(ξ ) =
∞
p(y) cos(ξ y) dy.
(12.88)
0
Note that a factor of 2 has been placed on all of (12.86) and accordingly removed from (12.88).
12.6.3 Speciﬁc Example As a speciﬁc example, consider the loading function ⎧ ⎨ p0 2 (a − y2 )−1/2 , p(y) = π ⎩ 0, if y > a.
if
0 ≤ y ≤ a,
(12.89)
Note that
∞
−∞
p(y)dy =
p0 π
a
−a
(a 2 − y2 )−1/2 dy = p0 .
(12.90)
The transform of p(y) is P(ξ ) = 0
a
p0 cos(ξ y) dy = 1/2 p0 J0 (ξ a), π (a 2 − y2 )1/2
(12.91)
12.6. Additional Solutions y r1
(x,y)
a p o
πa
241
r θ1
θ r2 θ2
Figure 12.5. Coordinate system for the complex variable, z.
x
a
where J0 (...) is a well known Bessel function. By combining terms for the various components of stress it is found that 2 p0 ∞ J0 (ξ a)e−ξ x cos(ξ y) dξ, σxx + σ yy = − π 0 (12.92) 2 p0 ∞ −ξ z ξ J0 (ξ a)e dξ, σ yy − σxx + 2iσxy = − π 0 where z = x + i y is the complex variable, and e−ξ z = e−ξ x−iξ y .
(12.93)
From standard handbooks and the properties of Bessel functions, ∞ ξ J0 (ξ a)e−ξ z dξ = z(a 2 + z2 )−3/2 0
=
z , 3/2 (z + ia) (z − ia)3/2
(12.94)
and thus σ yy − σxx + 2iσxy =
z 2 p0 x . π (z + ia)3/2 (z − ia)3/2
(12.95)
With reference to Fig. 12.5, we have z − ia = r1 eiθ1 ,
z + ia = r2 eiθ2 ,
(12.96)
and σ yy − σxx + 2iσxy =
r eiθ 2 p0 x π (r1r2 )3/2 ei3/2θ1 ei3/2θ2
r 2 p0 x = eiθ−3/2i(θ1 +θ2 ) . π (r1r2 )3/2
(12.97)
Consequently, σxy (x, y) = It is also found that σxx + σ yy = −
2 p0 π
∞
p0r 2 cos θ sin[θ − 3/2(θ1 + θ2 )]. π(r1r2 )3/2 eξ z J0 (ξ a) dξ = −
0
2 p0 cos[1/2(θ1 + θ2 )] =− , π (r1r2 )1/2
2 p0 2 (a − z2 )−1/2 π
(12.98)
(12.99)
242
12. SemiInﬁnite Media y p(x) Figure 12.6. Symmetrically loaded inﬁnite strip.
h h
x p(x)
and σ yy − σxx =
2 p0 r 2 cos θ cos[θ − 3/2(θ1 + θ2 )]. π (r1r2 )3/2
(12.100)
From these relations, it readily follows that σ yy (x, y) = −
σxx (x, y) = −
' ( p0 r2 cos[1/2(θ + θ )] − cos θ cos[θ − 3/2(θ + θ )] , 1 2 1 2 π(r1r2 )1/2 r1 r2 '
2
p0 r cos[1/2(θ1 + θ2 )] + 1/2 π(r1r2 ) r1 r2
(12.101) ( cos θ cos[θ − 3/2(θ1 + θ2 )] . (12.102)
Finally, we return to the displacements to ﬁnd that 2(1 + ν) ∞ cos(ξ y) dξ, P(ξ )e−ξ x [2(1 − ν) + ξ x] u(x, y) = πE ξ 0 which, when differentiated with respect to y, gives ∂u 2(1 − ν 2 ) p0 ∞ = J0 (ξ a) sin(ξ y) dξ ∂ y x=0 πE 0 0, if y ≤ a, = 2 p0 (1−ν 2 ) − π E(y 2 −a 2 )1/2 , if y > a.
(12.103)
(12.104)
Thus, for the assumed normal loading function, the x component of displacement is constant under the load; this is as though the surface was indented by a rigid punch.
12.7 Inﬁnite Strip In this case we consider an inﬁnite strip loaded on both sides with symmetrical loads as shown in Fig. 12.6. We begin with the biharmonic equation ∇ 4 φ = 0,
(12.105)
and the boundary conditions σ yy = ∂ 2 φ/∂ x 2 = − p(x), σxy = −∂ 2 φ/∂ x∂ y = 0,
on − ∞ ≤ x ≤ ∞, y = ±h, on y = ±h.
(12.106)
12.7. Inﬁnite Strip
243
Deﬁne the Fourier transform 1 (β, y) = √ 2π and its inverse 1 φ(x, y) = √ 2π
∞ −∞
∞ −∞
φ(x, y)eiβx dx,
(12.107)
(β, y)e−iβx dβ.
(12.108)
The transformed biharmonic equation becomes, as before, d4 d2 − 2β 2 2 + β 4 4 dy dy
= 0.
Setting the boundary condition for σ yy according to the ﬁrst of (12.106), yields ∞ 1 p(x)eiβx dx = −P(β). −β 2 = − √ 2π −∞
(12.109)
(12.110)
To illustrate the procedure, consider loading functions, p(x), that are symmetric, so that p(x) = p(−x). In this case ∞ 2 p(x)eiβx dx. (12.111) P(β) = √ 2π 0 Similar conversions of integrals involving symmetric functions will be made in what follows. The boundary condition for σxy leads to ∂ /∂ y = 0, for y = ±h.
(12.112)
Solutions that meet these conditions are of the form (β, y) = Acosh(βy) + B sinh(βy) + Cβy sinh(βy) + Dβy cosh(βy). The symmetry of φ in y requires that B = D = 0. The boundary condition for σxy yields
∂ /∂ y y=±h = β Asinh(βh) + C [βh cosh(βh) + sinh(βh)] = 0, i.e., A = −C[1 + βh coth(βh)].
(12.113)
The boundary condition for σ yy gives the additional relation −C
1 βh + sinh(βh) cosh(βh) = 2 P(β). sinh(βh) β
(12.114)
Thus, (β, x) =
1 [βh cosh(βh) + sinh(βh)] cosh(βy) − βy sinh(βh) sinh(βy) . P(β) β2 βh + sinh(βh) cosh(βh)
12.7.1 Uniform Loading: −a ≤ x ≤ a If p(x) is deﬁned as
p(x) =
p0 ,
−a ≤ x ≤ a,
0,
x > a,
(12.115)
244
12. SemiInﬁnite Media
then 1 P(β) = √ 2π
a
2 p0 sin(βa) . p0 cos(βx) dx = √ β 2π
−a
(12.116)
It is convenient to deﬁne nondimensional variables ζ = βh, η = y/ h, ξ = x/ h, and α = a/ h. Using these deﬁnitions, it is found that φ=
1 π
∞ −∞
2 p0 h2 sin(ζ α) ζ 3 [2ζ + sinh(2ζ )]
× [ζ cosh(ζ ) + sinh(ζ )] cosh(ζ η) − ζ η sinh(ζ ) sinh(ζ η) cos(ζ ξ ) dζ. Note that here the factor h2 is to be annihilated upon forming the stresses which involve second derivatives with respect to x and y. In fact, performing these derivatives, and noting the symmetry of the integrands involved, we obtain σxx = − ×
σxy
4 p0 π
∞
0
[sinh(ζ ) + ζ cosh(ζ )] cosh(ζ η) − ζ η sinh(ζ ) sinh(ζ η) 2ζ + sinh(2ζ )
sin(ζ α) cos(ζ ξ ) dζ, ζ
4 p0 =− π ×
0
∞
ζ η sinh(ζ ) cosh(ζ η) − ζ cosh(ζ ) sinh(ζ η) 2ζ + sinh(2ζ )
sin(ζ α) sin(ζ ξ ) dζ, ζ
(12.117)
and σ yy = −
4 p0 π
∞ 0
[sinh(ζ ) − ζ cosh(ζ )] cosh(ζ η) + ζ η sinh(ζ ) sinh(ζ η) 2ζ + sinh(2ζ )
sin(ζ α) × cos(ζ ξ ) dζ. ζ Strains may be calculated in a straightforward manner, and then the displacements. Because the system is fully equilibrated, the displacements will be set without the problem of undetermined rigid body displacements. Note also that the problem solved above [see (12.40) for the boundary conditions] should be recoverable by taking limits as h → ∞, although taking such limits may be a formidable task.
12.7.2 Symmetrical Point Loads If the distribution of force, p(x), above is reduced to a concentrated point force, P, we let p0 = P/2a, and take the limit lim
a→0
P P sin(ζ α) = . 2a ζ 2h
(12.118)
12.8. Suggested Reading
245
Using the previously derived results, we obtain σxx = −
2Px 2 y , π(x 2 + y2 )2
σ yy = −
2Py3 , π(x 2 + y2 )2
σxy = −
2Pxy2 . π(x 2 + y2 )2
(12.119)
12.8 Suggested Reading Little, R. W. (1973), Elasticity, Prentice Hall, Englewood Cliffs, New Jersey. Muskhelishvili, N. I. (1963), Some Basic Problems of the Mathematical Theory of Elasticity, Noordhoff, Groningen, Netherlands. Sokolnikoff, I. S. (1956), Mathematical Theory of Elasticity, 2nd ed., McGrawHill, New York. Sneddon, I. N. (1951), Fourier Transforms, McGrawHill, New York. Timoshenko, S. P., and Goodier, J. N. (1970), Theory of Elasticity, 3rd ed., McGrawHill, New York.
13 Isotropic 3D Solutions
13.1 DisplacementBased Equations of Equilibrium Recall the Cauchy equations of equilibrium in terms of stresses ∂σi j + b j = 0, ∂xj
(13.1)
along with the deﬁnition of small strains ei j =
1 2
∂u j ∂ui + ∂xj ∂ xi
,
and the constitutive relations for isotropic thermoelastic media E ν ekkδi j − KαTδi j . σi j = ei j + 2(1 + ν) 1 − 2ν
(13.2)
(13.3)
The coefﬁcient of thermal expansion is α, and K the elastic bulk modulus, K = E/3(1 − 2ν). The temperature difference from the reference temperature is T = T − T0 . When (13.3) are used in (13.1), we obtain ∂ 2 ui ∂ 2 uk E E + 2(1 + ν) ∂ x j ∂ x j 2(1 + ν)(1 − 2ν) ∂ xi ∂ xk = −bi +
∂T Eα . 3(1 − 2ν) ∂ xi
(13.4)
In direct tensor notation, this is written as E E ∇ 2u + grad div u 2(1 + ν) 2(1 + ν)(1 − 2ν) Eα grad T. = −b + 3(1 − 2ν)
(13.5)
Because the curl of a vector can be written as curl u = pqr 246
∂ur ep , ∂ xq
(13.6)
13.2. Boussinesq–Papkovitch Solutions
247
it is straightforward to construct the vector identity ∇ 2 u = grad div u − curl curl u.
(13.7)
When this is used in (13.5), it is found that E E(1 − ν) grad div u − curl curl u (1 + ν)(1 − 2ν) 2(1 + ν) Eα = −b + grad T, 3(1 − 2ν)
(13.8)
or 3 (1 − 2ν) 3(1 − ν) grad div u − curl curl u (1 + ν) 2 (1 + ν) 3(1 − 2ν) =− b + α grad T. E
(13.9)
These are the displacement based equations of equilibrium for isotropic thermoelastic media.
13.2 Boussinesq–Papkovitch Solutions There are a variety of methods for obtaining solutions to (13.9) or its alternative, (13.5). One of the methods for obtaining general solutions is as follows. In the absence of body forces and thermal gradients, (13.5) becomes grad div u + (1 − 2ν)∇ 2 u = 0.
(13.10)
υ = grad φ,
(13.11)
Now, if
where φ is any scalar function satisfying ∇ 2 φ = 0, then υ is a solution of (13.10), because div υ = ∂υi /∂ xi = ∇ 2 φ = 0,
(13.12)
∇ 2 υ = grad ∇ 2 φ = 0.
(13.13)
ω = 4(1 − ν)ψ − grad (x · ψ),
(13.14)
and thus
Next, if
where ψ is any vector ﬁeld satisfying ∇ 2 ψ = 0, then ω is also a solution to (13.10). To see this note ﬁrstly that components of the grad (x · ψ) are (xkψk), = ψ + xkψk, ,
(13.15)
ω = (3 − 4ν)ψ − xkψk, ,
(13.16)
because xk, = δk . Thus,
248
13. Isotropic 3D Solutions x3
θ r
Figure 13.1. Spherical coordinate system.
x 2 x1
ϕ
and ω, = div ω = (3 − 4ν)ψ, − xkψk, − ψ, = 2(1 − 2ν)ψ, ,
(13.17)
having regard to ψk, = (∇ 2 ψ)k = 0.
(13.18)
div ω = 2(1 − 2ν)div ψ.
(13.19)
Therefore,
But, ω,kk = (3 − 4ν)ψ,kk − (ψk, + xmψm,k)k = −2ψk,k ,
(13.20)
and so ∇ 2 ω = −2 grad div ψ.
(13.21)
Finally, by combining (13.21) and (13.19), we ﬁnd that ω is a solution to (13.10). Thus, general solutions to the homogeneous equation (13.10) can be constructed as u = υ + ω.
(13.22)
Such solutions are known as Boussinesq–Papkovitch solutions.
13.3 Spherically Symmetrical Geometries Considerable simpliﬁcation, incorporating nonetheless interesting and important problems, is achieved when the problem’s geometry suggests a solution in which the displacement ﬁeld depends only on a radial coordinate directed from a ﬁxed point. Such geometries are most naturally described by a spherical coordinate system, as sketched in Fig. 13.1.
13.3. Spherically Symmetrical Geometries
249
With respect to spherical coordinate system, the components of strain are ur ∂ur 1 ∂uθ , eθ θ = + , ∂r r ∂θ r 1 ∂uφ uθ ur eφφ = + cot θ + , r sin θ ∂φ r r 1 ∂uφ 1 ∂uθ − uφ cot φ + , = r ∂θ r sin θ ∂φ err =
2eθ φ
(13.23)
uθ 1 ∂ur ∂uθ − + , ∂r r r ∂θ 1 ∂ur ∂uφ uφ = + − . r sin θ ∂φ ∂r r 2er θ =
2eφr
Suppose, for example, that the displacement vector and the body force vector are of the form u = ur er ,
b = br er ,
where er is the unit vector directed radially. Then, u x u r r div u = div ur = div x + x · grad r r r dur ur ur + − =3 r dr r 1 d 2 (r ur ). = 2 r dr Also,
u x ur r = grad ×x+ curl x. curl u = curl ur r r r
(13.24)
(13.25)
(13.26)
But curl x = 0, and grad(ur /r ) is parallel to er x. These facts lead to the conclusion that, with such radial symmetry, curl u = 0.
(13.27)
Consider the equilibrium equation (13.18) and retain just the body force term. The substitution of the results (13.25)–(13.27) gives d 1 d 2 E(1 − ν) r u (13.28) = −br . r (1 + ν)(1 − 2ν) dr r 2 dr A similar development goes through if a radially symmetric temperature distribution is included on the r hs of (13.5) or (13.9). 13.3.1 Internally Pressurized Sphere Consider a hollow sphere with internal radius r1 , and external radius r2 . The sphere is internally pressurized at a pressure p1 and subject to an external pressure p2 (Fig. 13.2a). This geometry is clearly spherically symmetric and thus, with an origin at the sphere’s
250
13. Isotropic 3D Solutions p
p2
p1
Figure 13.2. (a) Spherical hole and (b) an inclusion subject to pressure.
(b)
(a)
center, the displacement u is purely radial and a function of r alone. Thus, curl u = 0 and (13.9) becomes grad div u = 0,
(13.29)
which leads directly to div u =
1 d(r 2 ur ) = 3a, r2 dr
(13.30)
where 3a is a constant (the 3 being incorporated for convenience). Upon integration, ur = ar + b/r 2 ,
(13.31)
where b is another integration constant. The components of strain are easily derived as err = a − 2b/r 3 ,
eθ θ = eφφ = a + b/r 3 .
(13.32)
The constants a and b are calculated by applying the stated boundary conditions to the radial stress, σrr =
2E b E E a− . [(1 − ν)err + 2νeθ θ ] = (1 + ν)(1 − 2ν) 1 − 2ν 1 + ν r3
(13.33)
The result of applying σrr (r1 ) = − p1 and σrr (r2 ) = − p2 is a=
p1r13 − p2r23 1 − 2ν , E r23 − r13
b=
r13r23 ( p1 − p2 ) 1 + ν . 2E r23 − r13
If, for example p1 = p and p2 = 0, we have pr 3 pr 3 r3 r3 σrr = 3 1 3 1 − 23 , σφφ = σθ θ = 3 1 3 1 + 23 . r r r2 − r1 r2 − r1
(13.34)
(13.35)
Limiting solutions for thin walled spherical shells, i.e., when r2 = r1 + h and h/r1 1, are readily obtained. Another case of interest is a void in an inﬁnite medium (r2 → ∞) subject to external pressure p2 = p. In this case, with p1 = 0, we obtain r13 r13 σrr = − p 1 − 3 , σφφ = σθ θ = − p 1 + 3 . (13.36) r 2r
13.4. Pressurized Sphere: StressBased Solution
251
13.4 Pressurized Sphere: StressBased Solution Another route of deriving the previous solution is as follows. In a threedimensional problems with spherical symmetry, the only displacement component is the radial displacement u = u(r ). The corresponding strain components are err =
du , dr
eθ θ = eφφ =
u , r
(13.37)
with the SaintVenant compatibility equation 1 deθ θ = (err − eθ θ ) . dr r
(13.38)
The nonvanishing stress components are the radial stress σrr and the hoop stresses σθ θ = σφφ . In the absence of body forces, the equilibrium equation is dσrr 2 + (σrr − σθ θ ) = 0 . dr r
(13.39)
The Beltrami–Michell compatibility equation is obtained from (13.38) by incorporating the stressstrain relations err =
1 (σrr − 2νσθ θ ) , E
eθ θ =
1 [σθ θ − ν(σrr + σθ θ )] , E
(13.40)
and the equilibrium equation (13.39). This gives d (σrr + 2σθ θ ) = 0 , dr
(13.41)
which implies that the spherical component of stress tensor is uniform throughout the medium, 1 (σrr + 2σθ θ ) = A = const. 3
(13.42)
Combining (13.39) and (13.42) it follows that 3 dσrr 3 + σrr = A. dr r r
(13.43)
The general solution of this equation is σrr = A+
B . r3
(13.44)
The corresponding hoop stresses are σθ θ = σφφ = A−
B . 2r 3
(13.45)
The boundary conditions for the Lame´ problem of a pressurized hollow sphere are σrr (R1 ) = − p1 ,
σrr (R2 ) = − p2 .
(13.46)
These are satisﬁed provided that A=
p1 R13 − p2 R23 , R23 − R13
B=−
R13 R23 ( p1 − p2 ) . R23 − R13
(13.47)
252
13. Isotropic 3D Solutions
Consequently, the stress components are R13 R13 R23 p1 3 − p2 − ( p1 − p2 ) 3 , σrr = 3 r R2 − R13 R2 σθ θ
R13 R13 R23 = 3 p1 3 − p2 + ( p1 − p2 ) 3 . 2r R2 − R13 R2
(13.48)
(13.49)
The corresponding hoop strain is obtained by substituting (13.48) and (13.49) into the stressstrain relation (13.40). The result is eθ θ =
B 1 A − , 3K 4µ r 3
(13.50)
where the elastic bulk modulus is K = E/3(1 − 2ν), and the elastic shear modulus is µ = E/2(1 + ν). Thus, the radial displacement u = r θ θ is u=
R13 R23 1 1 p1 R13 − p2 R23 1 ( p r + − p ) . 1 2 3κ 4µ R23 − R13 R23 − R13 r 2
(13.51)
For the nonpressurized hole ( p1 = 0) under remote pressure p2 at inﬁnity, the previous results give R13 R13 σrr = − p2 1 − 3 , σθ θ = σφφ = − p2 1 + 3 , (13.52) r 2r u=−
R3 p2 2(1 − 2ν) r + 21 . 4µ 1+ν r
(13.53)
The displacement is here conveniently expressed by using the Poisson’s ratio ν. For the pressurized cylindrical hole in an inﬁnite medium with p2 = 0, we obtain σrr = − p1
R13 , r3 u=
σθ θ = σφφ = p1
R13 , 2r 3
p1 R13 . 4µ r 2
(13.54)
(13.55)
13.4.1 Pressurized Rigid Inclusion Imagine that the cavity of the previous solution is a rigid inclusion so that the displacement at its periphery were to vanish (Fig. 13.2b). The inclusion is to be loaded by a uniform pressure applied at the outer boundary at r2 , and the inclusion’s radius is still r1 . The earlier found form for the displacement ﬁeld (13.31) still holds, but now we have the boundary condition that at r = r1 , ur (r1 ) = ar1 + b/r12 = 0
⇒
a = −b/r13 .
(13.56)
With this we apply the same boundary condition at r = r2 , viz., σrr (r2 ) = − p,
(13.57)
13.4. Pressurized Sphere: StressBased Solution
253
to ﬁnd
E 2E b= p 3 + 3 r1 (1 − 2ν) r2 (1 + ν)
−1
.
(13.58)
The complete solution for the displacements, stresses and strains follows by simple calculation. Here we look at the limit as r2 becomes very large, i.e., lim b =
r2 → ∞
r13 (1 − 2ν) p . E
(13.59)
The radial stress is then σrr = − p − 2 p
1 − 2ν (r1 /r )3 . 1+ν
(13.60)
Note that for an incompressible material, with ν = 1/2, the radial stress is everywhere constant and equal to − p. In addition, at the inclusion surface σrr (r1 ) = −3 p
1−ν , 1+ν
(13.61)
which reveals an interesting effect of Poisson’s ratio on the concentration or virtual removal of pressure on the surface of the inclusion. The complete stress and strain ﬁeld can be easily computed from the results listed above. 13.4.2 Disk with Circumferential Shear It is possible to generate singular solutions of physical interest using the techniques introduced here. For example, consider the displacement ﬁeld u = C grad θ,
(13.62)
where θ = tan−1 (x2 /x1 ), and C is a constant to be determined by suitable boundary conditions. Note some properties of the nonzero components of displacement gradient. Since u1 = −
Cx2 , x12 + x22
u2 =
Cx1 , x12 + x22
(13.63)
the normal strains are u1,1 = 2C
x2 x1 , (x12 + x22 )2
u2,2 = −2C
x2 x1 . (x12 + x22 )2
(13.64)
This shows, inter alia, that the deformation described by this displacement ﬁeld involves no volume change, because u3 = 0 and u1,1 + u2,2 = 0. Also, the equilibrium equations are satisﬁed because ∇ 2 u = 0 and div u = 0. The other relevant components of displacement gradient are u1,2 = − u2,1
x22 C + 2C , x12 + x22 (x12 + x22 )2
x12 C = 2 − 2C , x1 + x22 (x12 + x22 )2
(13.65)
254
13. Isotropic 3D Solutions
τ M
Figure 13.3. Disklike region subject to shear.
and thus the shear strain is e12 =
x 2 − x12 1 (u1,2 + u2,1 ) = C 22 . 2 (x1 + x22 )2
(13.66)
Consequently, σ12 = 2GC
x22 − x12 , (x12 + x22 )2
(13.67)
and x1 x2 . + x22 )2
(13.68)
1 1 = 2GC 2 . 2 r + x2
(13.69)
σ11 = −σ22 = 4GC
(x12
The circumferential shear stress is σθr = 2GC
x12
Thus, the peculiar displacement ﬁeld of the problem gives rise to a singular stress ﬁeld associated with uniform shear stress acting on the periphery of a disklike region. If for example, this region were a disc of radius r = r1 with applied shear stress σθr = τ on its edge, then C = τr12 /2G. The concentrated couple in the center of the disk, needed to equilibrate this shear stress on the periphery of the disk, is M = 2πr12 τ (Fig. 13.3). 13.4.3 Sphere Subject to Temperature Gradients Here we consider a sphere of radius r2 subject to a radial temperature gradient. Again the displacement ﬁeld is assumed to be purely radial. Thus, curl u = 0 and (13.9) reduces to 1 + ν dT d 1 d(r 2 ur ) . (13.70) =α dr r 2 dr 3(1 − ν) dr We let T(r2 ) = 0 such that if the sphere were uniformly cooled to that temperature no stresses would result. If (13.70) is integrated, we ﬁnd r r2 1 1+ν 2(1 − 2ν) r 2 2 T(r )r dr + T(r )r dr . (13.71) ur = α 3(1 − ν) r 2 0 1 + ν r23 0
13.5 Spherical Indentation In this section we examine the problem of indentation of an elastic halfplane by a rigid spherical indenter. The process of indentation is essentially that associated with the Brinell hardness test using a spherical indenter. We shall analyze the problem using the approach
13.5. Spherical Indentation
255
(a') 2 = δ D a (sinking in) < a' < a (piling up) piling up
a sinking in
r
r δ
a' δ a
original surface
Figure 13.4. Geometry of an indentation. Note the phenomenology of either sinking in or piling up depending on the degree of nonlinearity of the indented material.
introduced by Love (1944) and later generalized in terms of the Galerkin vector potential. The geometry of indentations, in its most general form in materials that are elasticplastic, is as sketched in Fig. 13.4. For nonlinear materials, indented material generally tends to either sinkin or pileup beneath or around the indenter. The trends are that for materials that are linear or that display high rates of strain hardening indented material sinks away from the indenter, whereas for materials that are weakly hardening piling up is observed. The effect is that the actual contact radius will be smaller in the case of sinking in behavior and larger for the case of piling up. This, of course has an important effect on the intensity of the pressure that develops beneath the indenter and for the quantitative assessment of hardness. For the case considered here, viz., that of linear elastic materials, we will ﬁnd the characteristic Hertzian sinking in. 13.5.1 DisplacementBased Equilibrium Begin with the isotropic elastic constitutive relations expressed, using Lame´ constants λ and µ, as σi j = λemmδi j + 2µei j .
(13.72)
Recall the connections among the isotropic elastic constants E= ν=
µ(3λ + 2µ) , λ+µ
λ , 2(λ + µ)
G=
µ = G, E , 2(1 + ν)
(13.73)
and the equations of equilibrium ∂σi j + bi = 0. ∂xj
(13.74)
Since ekk = ∂uk/∂ xk = div u, it is readily veriﬁed that 2
∂ei j ∂ekk = ∇ 2 ui + . ∂xj ∂ xi
(13.75)
∂ div u + µ∇ 2 ui + bi = 0. ∂ xi
(13.76)
Thus, (λ + µ)
256
13. Isotropic 3D Solutions
Using the relation λ+µ=
µ , 1 − 2ν
(13.77)
the equilibrium equations can be rewritten as ∇ div u + (1 − 2ν)∇ 2 u +
1 − 2ν b = 0, µ
(13.78)
where µ = G is the shear modulus. In the absence of body forces, this becomes ∇ div u + (1 − 2ν)∇ 2 u = 0.
(13.79)
13.5.2 Strain Potentials We have already seen that a suitable displacement function can be constructed from the gradient of a scalar ﬁeld as 1 ∇φ. G
(13.80)
∇ ∇ 2 φ = 0,
(13.81)
∇ 2 φ = const.
(13.82)
u= To satisfy (13.79), φ must be such that
which leads to the conclusion that
We note that (13.80) is not the most general form of displacement solution. A more general form is one in which the displacement is constructed from the second derivatives of a potential. As there are no operators of this type that transform a scalar into a vector, the potential must be a vector potential. The Galerkin vector potential, G, is thus introduced and the most general form for the displacement u is given as u=
1 2 c∇ − ∇ div G. 2G
(13.83)
When (13.83) is inserted into (13.79), it is found that c = 2(1 − ν), and u=
1 2(1 − ν)∇ 2 G − ∇ div G . 2G
(13.84)
The Galerkin vector potential G must satisfy the biharmonic equation ∇ 4 G = 0.
(13.85)
For the axisymmetric problem considered, we make use of one component of G, viz., Gz; we call Gz = . In the (r, z) coordinate system, we then have 1 ∂ 2 1 ∂ 2 , uz = ur = − 2(1 − ν)∇ 2 − 2 , 2G ∂r ∂z 2G ∂z (13.86) uθ = 0,
= (r, z).
13.5. Spherical Indentation
257
The Laplacean in the (r, z) coordinates is ∇2 = The stresses are
∂2 1 ∂ ∂2 + . + ∂r 2 r ∂r ∂z2
(13.87)
∂ ∂ 2 2 σrr = , ν∇ − ∂z ∂r 2 ∂ 1 ∂ ν∇ 2 − , σθ θ = ∂z r ∂r ∂ ∂ 2 σzz = (2 − ν)∇ 2 − 2 , ∂z ∂z ∂ ∂ 2 (1 − ν)∇ 2 − 2 , σr z = ∂r ∂z
(13.88)
where the Love’s potential satisﬁes ∇ 4 = 0.
(13.89)
Use has been made of the deﬁnitions of strain in a cylindrical system, viz., err = and
∂ur , ∂r
eθ θ =
ur , r
ezz =
∂uz , ∂z
∂uz 1 ∂ur er z = + . 2 ∂z ∂r
(13.90)
(13.91)
13.5.3 Point Force on a HalfPlane The Love’s potential for a concentrated point force of intensity p0 is p0 z 1 + 2ν 1 + r 2 /z2 + (1 − 2ν) ln 1 + 1 + r 2 /z2 − ln z . = 2π The corresponding displacements, from (13.86), are 1 r 2 /z2 p0 (1 − 2ν) 1 1 ur = + − 1 , 4π G r 1 − 2ν (1 + r 2 /z2 )3/2 (1 + r 2 /z2 )1/2 and uz =
1 p0 1 1 + 2(1 − ν) . 4π G z (1 + r 2 /z2 )3/2 (1 + r 2 /z2 )1/2
(13.92)
(13.93)
Of particular interest is the z component of displacement, which we denote by ω when z = 0. In general, 2 z p0 1 , (13.94) + 2(1 − ν) uz = 4π G ρ 3 ρ
258
13. Isotropic 3D Solutions
r
Figure 13.5. A hemispherical distributed load over the halfspace.
z
and on the surface, z = 0, ω=
p0 (1 − ν) 1 p0 (1 − ν) 1 = , 2π G ρ 2π G r
(13.95)
where ρ = (z2 + r 2 )1/2 is the distance from the point force to the ﬁeld point. 13.5.4 Hemispherical Load Distribution Consider now the application of a distributed force whose intensity has a hemispherical form (Fig. 13.5), 1/2 r2 q(r ) = q0 1 − 2 . (13.96) a The displacements are found by the using the solutions given in (13.95) as a Green’s function, so that (1 − ν)q0 π/2 2 (a − r 2 sin2 ϕ) dϕ , r ≤ a , (13.97) ω= 2aG 0 ω=
(1 − ν)q0 2aG
α
(a 2 − r 2 sin2 ϕ) dϕ ,
r ≥a.
(13.98)
0
The angles ϕ and α are deﬁned in Fig. 13.6. The results of integration are r2 ω = ωmax 1 − 2 , r ≤ a , 2a " 1/2 # a a2 ωmax r 2 a2 −1 a + 2 2 − 1 sin , r ≥a. ω= 1− 2 π a2 r r r r
(13.99)
The maximum displacement at the center of the distributed load, ωmax = ω(0, 0), is twice greater than the displacement at the periphery of the load, ωa = ω(a, 0), i.e., ωmax = 2ωa ,
ωmax =
πq0 (1 − ν) a. 4G
(13.100)
13.5. Spherical Indentation n
259
n ϕ
O
m ϕ α
M
r
m
r
O
Figure 13.6. Integration angles. Note “M” signiﬁes the typical ﬁeld point, either inside or outside the circle.
M
The total force is
a
P = 2π
q0 0
r2 1− 2 a
1/2 r dr =
2 πa 2 q0 , 3
(13.101)
so that P=
2 3G a ωmax . 3 1−ν
(13.102)
13.5.5 Indentation by a Spherical Ball The solution for the spherical load is an essential ingredient for constructing the Hertz solution for the elastic indentation of a halfspace by a spherical indenter. Denoting by R the radius of the ball, and by δ the depth of the indentation, the equation of the sphere, on the surface of contact, is r 2 + [z + (R − δ)]2 = R2 .
(13.103)
For shallow indentations δ/R 1 and z/R 1, where in the second inequality the coordinate z is meant to be on the indented surface. Thus, when (13.103) is expanded, terms such as z2 and δz are neglected so that, with z replaced by ω on the surface, (13.103) yields ω(r ) = δ −
r2 , 2R
r ≤ a.
Because a is a geometric mean of δ/2 and 2R − δ/2, we have δ δ a2 = 2R − , a 2 ≈ Rδ , 2 2
(13.104)
(13.105)
and thus (13.104) can be rewritten as r2 ω(r ) = δ 1 − 2 , 2a
r ≤ a,
(13.106)
in agreement with the displacement ﬁeld at the surface given in (13.99) for a hemispherical load distribution. Alternatively, consider the displacement at the periphery of the contact circle (r = a). Call this δa = ω(a, 0). Then, ω(r ) = δa +
1 (a 2 − r 2 ), 2R
(13.107)
260
13. Isotropic 3D Solutions
Figure 13.7. The displacement proﬁle of the indented surface.
with a simple connection δ = δa +
a2 . 2R
(13.108)
√ Note that aˆ ≈ 2Rδ would be the “apparent radius of contact” of the sphere that was ideally pressed into the surface to a depth δ, assuming that the indented material simply did not deﬂect or distort. The quantity c2 = a 2 /aˆ 2
(13.109)
is an invariant of such indentation processes, and for this linear elastic case c2 = 1/2.
(13.110)
If (13.105) is used in (13.102), we obtain P=
8 G R1/2 δ 3/2 , 3 1−ν
(13.111)
8 G 1 3 a . 3 1−ν R
(13.112)
or, in terms of the radius of contact, P=
An indentation hardness can be deﬁned as 8 G 8 G a P = = H= πa 2 3 1−ν R 3 1−ν
1/2 δ . R
The displacement of the indented surface (Fig. 13.7) is a2 r2 ω= 1− 2 , r ≤a, R 2a " 1/2 # a r2 a2 a2 −1 a , ω= + 2 2 − 1 sin 1− 2 πR r r r r
(13.113)
(13.114) r ≥a.
Alternatively, the displacement can be expressed in terms of the depth δ of the indentation (Fig. 13.8) as √ r2 , r ≤ Rδ , 2R √ √ " # 2 r Rδ Rδ Rδ Rδ 1/2 −1 ω= , + 2 2 − 1 sin 1− 2 πR r r r r ω=δ−
(13.115) r≥
√
Rδ .
13.6. Point Forces on Elastic HalfSpace
261
R
r
O δ 2
δ
Figure 13.8. The width a and the depth δ of the indentation by a spherical ball.
z The slope of the indented surface is continuous at the periphery of the contact circle and equal to δ dω =− , dr a
(13.116)
which is unlike indentation with a rigid ﬂat punch (where there is a slope discontinuity). On the other hand, the hemispherical loading considered here prescribes a normal stress that vanishes at the periphery of contact, in contrast to that of a ﬂat punch (for which the normal stress is inﬁnite at the periphery).
13.6 Point Forces on Elastic HalfSpace Here we summarize the solutions for point force loading on elastic halfspaces for 3D inﬁnite media. The coordinate system used is shown in Fig. 13.9. We consider both normal and tangential point forces imposed on the surface of an elastically isotropic media. Relations (13.86)–(13.87) gave the radially symmetric displacement ﬁelds for a normal point force in polar coordinates. We list here the same displacement components in the Cartesian coordinate frame of Fig. 13.9. They are xz p0 x − (1 − 2ν) , ux (x, y, z) = 4π G ρ 3 ρ(ρ + z) yz p0 y − (1 − 2ν) u y (x, y, z) = , (13.117) 4π G ρ 3 ρ(ρ + z) 2 z p0 2(1 − ν) + , uz(x, y, z) = 4π G ρ 3 ρ
p
o
qo x y z
Figure 13.9. Normal and tangential point forces on elastic halfspace.
262
13. Isotropic 3D Solutions
where ρ = (x 2 + y2 + z2 )1/2 . It is of speciﬁc interest to form these on the surface of the halfspace, where r 2 = x 2 + y2 . The displacements there are p0 (1 − 2ν)x , 4π G r2 p0 (1 − 2ν)y , u¯ y (x, y) = − 4π G r2 p0 2(1 − 2ν) . u¯ z(x, y) = 4π G r
u¯ x (x, y) = −
(13.118)
The stresses are then readily calculated by the straightforward procedure of forming the strains and invoking the isotropic elastic constitutive relations. The solution for the case of a tangential point load of magnitude q0 is obtained using similar techniques as described in the previous section on spherical indentation. The results for the displacements are ! x2 x2 1 1 q0 + 3 + (1 − 2ν) − , ux (x, y, z) = 4π G ρ ρ ρ + z ρ(ρ + z)2 xy q0 xy (13.119) u y (x, y, z) = − (1 − 2ν) , 4π G ρ 3 ρ(ρ + z)2 q0 x xz + (1 − 2ν) . uz(x, y, z) = 4π G ρ 3 ρ(ρ + z) When expressed on the surface z = 0 of the halfspace, these displacements are 2(1 − ν) 2νx 2 q0 + 3 , u¯ x (x, y) = 4π G r r q0 2νxy , 4π G r 3 q0 (1 − 2ν)x u¯ z(x, y) = . 4π G r2
u¯ y (x, y) =
(13.120)
Again, the elastic strains and then the stresses can be readily calculated from (13.119). For later reference, we note that if a general set of point loads f = { fx , fy , fz} were applied to the surface, the displacements on the surface could be expressed as u¯ α (x, y) = %αβ (x, y, z) fβ , where
(α, β = x, y, z),
⎧ ⎫ 2(1 − ν) 2νx 2 (1 − 2ν)x ⎪ 2νxy ⎪ ⎪ ⎪ ⎪ ⎪ + 3 − ⎪ ⎪ ⎪ ⎪ r r r3 r2 ⎪ ⎪ ⎨ ⎬ 2 1 2νxy 2(1 − ν) 2νy (1 − 2ν)y . Π= + 3 − ⎪ 4π G ⎪ ⎪ ⎪ r3 r r r2 ⎪ ⎪ ⎪ ⎪ ⎪ (1 − 2ν)x (1 − 2ν)y 2(1 − 2ν) ⎪ ⎪ ⎪ ⎩ ⎭ 2 2 r r r
(13.121)
(13.122)
This form will be useful in solving for the elastic ﬁelds at the surfaces of halfplanes subject to general loading via superposition techniques.
13.7. Suggested Reading
263
13.7 Suggested Reading FilonenkoBorodich, M. (1964), Theory of Elasticity, Noordhoff, Groningen, Netherlands. Fung, Y.C. (1965), Foundations of Solid Mechanics, Prentice Hall, Englewood Cliffs, New Jersey. Little, R. W. (1973), Elasticity, Prentice Hall, Englewood Cliffs, New Jersey. Love, A. E. H. (1944), A Treatise on the Mathematical Theory of Elasticity, Dover, New York. Novozhilov, V. V. (1961), Theory of Elasticity, Pergamon, New York. Sokolnikoff, I. S. (1956), Mathematical Theory of Elasticity, 2nd ed., McGrawHill, New York. Timoshenko, S. P., and Goodier, J. N. (1970), Theory of Elasticity, 3rd ed., McGrawHill, New York.
14 Anisotropic 3D Solutions
14.1 Point Force For the time being we refer to the case of generally anisotropic elastic media, and later specialize to the case of isotropic elastic media. Recall the equilibrium equations σi j, j + bi = 0,
(14.1)
where bi are the components of the body force per unit volume. The constitutive equations that connect the stresses to small elastic strains are σi j = Ci jkl ekl = Ci jkl uk,l .
(14.2)
Thus, combining (14.1) and (14.2), we obtain Ci jkl uk,l j = bi .
(14.3)
Suppose b is concentrated at a “point.” Next let b act only in the xm direction and, for now, let the magnitude of this concentrated force be unity. If the force acts at x = x , we can write 0, if i = m, bi = δ(x − x ), if i = m, where δ(x) is the Dirac delta function, deﬁned in Chapter 3. The above can be rewritten by using the Kronecker δ as bi = δim δ(x − x ),
(i = 1, 2, 3).
(14.4)
14.2 Green’s Function Using (14.4), equation (14.3) becomes Ci jkl uk,l j = −δim δ(x − x ). (m)
264
(14.5)
14.2. Green’s Function
265
bm xx
x'
'
Figure 14.1. Displacement caused by a unit point force.
x u
k
(m)
The direct physical interpretation of uk (m)
uk
is
= the component of displacement in the kth direction at the point x caused by a point force acting in the mth direction at x .
(m)
We note that uk is a tensor as it associates a vector, u, with another vector, b (Fig. 14.1). (m) Thus, the component of tensor G is Gmk = uk , and (14.5) becomes Ci jkl Gkm, jl (x, x ) = −δim δ(x − x ).
(14.6)
The function Gkm is called a Green’s function. It is clearly symmetric, i.e., Gkm = Gmk. When integrating (14.6) we demand that the inﬂuence of the point force vanish sufﬁciently rapid, and in particular we demand that G vanish at least as fast as G∼
1 1 = x − x  r
as r → ∞.
(14.7)
Solution by Fourier transforms provides a direct route to a solution. The Fourier transform of G(x, x ) is obtained from ∞ G(x, x ) exp(iK · x) d3 x, (14.8) g(K) = −∞
where d x ≡ dV = dx1 dx2 dx3 and K is the Fourier vector in Fourier space. The inverse transform is then obtained from ∞ 1 g(K) exp(−iK · x) d3 K. (14.9) G(x, x ) = (2π )3 −∞ 3
To proceed, multiply (14.6) by exp(iK · x) or by (x − x ), because x is a ﬁxed position in the integrations, and integrate over all physical, i.e., x, space to obtain ∞ Ci jkl Gkm, jl (x, x ) exp[iK · (x − x )] d3 x −∞
=−
∞
−∞
(14.10)
δim δ(x − x ) exp[iK · (x − x )] d x. 3
As noted above, d3 x = d3 (x − x ) because of the ﬁxity of x . Integration by parts yields, after taking into account the vanishing of G at afar, ∞ K j Kl Ci jkl Gkm(x, x )d3 (x − x ) = −δim. (14.11) − −∞
266
14. Anisotropic 3D Solutions
To reduce this expression, we deﬁne a unit vector, z, as the unit vector along K, i.e, K = Kz,
K ≡ K.
(14.12)
Then, K j Kl Ci jkl = K2 z j zl Ci jkl = K2 Mik(z).
(14.13)
This, in turn, leads to the deﬁnition of the acoustic tensor, or Christoffel stiffness tensor, M ≡ z · C · z.
(14.14)
Thus, (14.11) becomes ∞ − K2 Mik(z)Gkm(x, x ) exp[iK · (x − x )]d3 (x − x ) = −δim.
(14.15)
Removing items that are constant within the integral, we obtain ∞ 2 Gkm(x, x ) exp[iK · (x − x )]d3 (x − x ) = −δim. −K Mik(z)
(14.16)
−∞
−∞
Therefore, −K2 Mik gkm = −δim,
(14.17)
or, by inversion, gsm =
−1 (z) Msm . 2 K
The inverse transform, or G itself, is thus ∞ −1 Mkm 1 Gkm(x, x ) = exp[−iK · (x − x )] d3 K. (2π)3 −∞ K2 Since G is real, we need only take the real part of (14.19), i.e., ∞ −1 Mkm 1 Gkm(x, x ) = cos[K · (x − x )] d3 K. 3 (2π) −∞ K2
(14.18)
(14.19)
(14.20)
To perform these integrations it is convenient to introduce a unit vector T and a stretched vector λ as follows x − x = x − x T, λ = Kx − x  = Kx − x z. With these, the inverse transform becomes 1 Gkm(x, x ) = 3 8π x − x 
∞ −∞
−1 Mkm (z) cos(λz · T) d3 λ. 2 λ
(14.21)
(14.22)
Note, if T is replaced by −T, we have cos(λz · T) = cos(λz · −T). Accordingly, we can express (14.22) as sgn(s) Gkm(T), (14.23) s where s is an algebraically signed scalar. Thus G scales as 1/x − x . In fact, G depends on x and x strictly as on (x − x ). Gkm(x, x ) = Gkm(sT) =
14.2. Green’s Function
λ z
z θ
267
z ϕ T
T
θ
m
tu
Da
xx'
unit circle z T = 0
z
Figure 14.2. A polar coordinate system aligned with T.
T = 0
We may now inquire about the derivatives of G. For example, we have ∞ −1 zp Mkm (z) −1 sin(λz · T) d3 λ. Gkm, p (x − x ) = 3 2 8π x − x  −∞ λ
(14.24)
Thus, Gkm, p (x, x ) = Gkm, p (sT) =
sgn(s) Gkm, p (T). s2
(14.25)
Gkm, pt (x, x ) = Gkm, pt (sT) =
sgn(s) Gkm, pt (T), s3
(14.26)
Similarly, we ﬁnd
and so on. In general, we obtain Gkm,α1 α2 ...αn (x, x ) = Gkm,α1 α2 ...αn (sT) =
sgn(s) Gkm,α1 α2 ...αn (T). sn
We now return to (14.22) and introduce polar coordinates aligned with T such as in Fig. 14.2. Then d3 λ = λ2 sin φ dλ dφ dθ, and 1 Gkm(x − x ) = 8π 3 x − x 
2π 0
π 0
z · T = cos φ,
0
∞
(14.27)
−1 Mkm (z) cos(λz · T) sin φ dλ dφ dθ.
The integral over λ within the above is ∞ sin[λ(z · T)] . cos(λz · T) dλ = lim λ→∞ (z · T) 0
(14.28)
Recalling that lim λ (z · T) = lim
λ→∞
λ→∞
1 sin[λ(z · T)] = π (z · T) δ(z · T),
we obtain
0
∞
cos(λz · T) dλ = π δ(z · T),
(14.29)
268
14. Anisotropic 3D Solutions
which, when substituted into (14.2), yields 1 Gkm(x − x ) = 8π 2 x − x 
2π 0
−1 Mkm dθ.
(14.30)
The integration over θ is about a unit circle lying on the plane x · T = 0. Note also that δ(z · T) = δ(cos φ) = δ(φ − π/2).
14.3 Isotropic Green’s Function We recall that for the case of isotropic elastic media Ci jkl = λδi j δkl + µ(δikδ jl + δil δ jk)
(14.31)
and thus Mik = Ci jkl z j zl = λδi j δkl z j zl + µ(δikδ jl + δil δ jk)z j zl = λzi zk + µδik zl zl + µzi zk.
(14.32)
But, zl zl = z12 + z22 + z32 = 1,
(14.33)
λ+µ zi zk . Mik = µ δik + µ
(14.34)
because z is a unit vector, so that
Now consider a matrix with components Qli =
1 (δli + Bzl zi ) . µ
(14.35)
We ask, is it possible to choose a value for B such that Qli = Mli−1 , i.e., so that Qli Mik = δlk? To answer the question, evaluate the product λ+µ zi zk Qli Mik = (δli + Bzl zi ) δik + µ λ+µ λ+µ δli zi zk + B zl zi zi zk + Bzl zi δik + Bzl zi δik µ µ λ+µ λ+µ + B+ B = δlk + zl zk . µ µ = δli δik +
(14.36)
Thus, if λ+µ λ+µ + B+ B = 0, µ µ
(14.37)
we have B=− and −1 Mkm
λ+µ , λ + 2µ
1 λ+µ zk zm . = δkm + µ λ + 2µ
(14.38)
(14.39)
14.3. Isotropic Green’s Function
269
x3
x

x'
φ
x1
ψ
Figure 14.3. Spherical coordinate system.
x2
Therefore, to evaluate Gkm(x − x ) we need only express zk zm as a function of θ noting that, for our purposes, zk is the kth direction cosine of a unit vector which is perpendicular to x − x . With reference to the spherical coordinate system in Fig. 14.3, the direction cosines of x − x are λk =
xk − xk , x − x 
(14.40)
with λ1 = sin φ cos ψ,
λ2 = sin φ sin ψ,
λ3 = cos φ,
(14.41)
and λi λi = 1. Then, construct z as zk = ak cos θ + bk sin θ,
(14.42)
where a1 = cos φ cos ψ,
b1 = − sin ψ,
a2 = cos φ sin ψ,
b2 = cos ψ,
a3 = − sin φ,
(14.43)
b3 = 0.
This gives zk zm = (ak cos θ + bk sin θ)(am cos θ + bm sin θ) = akam cos2 θ + bkbm sin2 θ + (akbm + ambk) sin θ cos θ. Hence, for this isotropic case we have 2π ' 1 λ+µ [akam cos2 θ + bkbm sin2 θ δkm + Gkm = 2 8π µx − x  0 λ + 2µ ( + (akbm + ambk) sin θ cos θ] dθ.
(14.44)
(14.45)
Noting that
2π 0
0
we thus obtain
2π
δkm dθ = 2π δkm,
sin θ cos θ dθ = 0,
0 2π
sin2 θ dθ =
2π
cos2 θ dθ = π,
0
1 λ+µ Gkm = (akam + bkbm) . 2δkm − 8π µx − x  λ + 2µ
(14.46)
270
14. Anisotropic 3D Solutions
It is easily veriﬁed that akam + bkbm = δkm − λkλm = δkm − so that
) (xk − xk )(xm − xm , 2 x − x 
(14.47)
! ) (xk − xk )(xm − xm 1 λ+µ . 2δkm − δkm − Gkm(x − x ) = 8π µx − x  λ + 2µ x − x 2
An alternative, useful form of this expression is obtained by observing that ∂ ∂ xm − xm x − x  = [(xl − xl )(xl − xl )]1/2 = . ∂ xm ∂ xm x − x
Then, ∂ ∂ xk
(14.48)
xk − xk ∂ ∂ x − x  = ∂ xm ∂ xk x − x  ) (xk − xk )(xm − xm δkm − 2 x − x  x − x  ) (xk − xk )(xm − xm 1 δkm − . = 2 x − x  x − x 
=
Furthermore, we readily ﬁnd
)(xm − xm ) ∂ ∂ 1 (xm − xm ∇ x − x  = δmm − . x − x  = 2 ∂ xm ∂ xm x − x  x − x  2
(14.49)
Since δmm = 3,
(xm − xm )(xm − xm ) = x − x 2 ,
(14.50)
the previous expression simpliﬁes to ∇ 2 x − x  =
2 . x − x 
Thus, the alternative expression for the Green’s function is ∂2 1 λ+µ 2 Gkm(x − x ) = δkm∇ − x − x . 8π µ λ + 2µ ∂ xk∂ xm
(14.51)
(14.52)
14.4 Suggested Reading Lekhnitskii, S. G. (1981), Theory of Elasticity of an Anisotropic Elastic Body, Mir Publishers, Moscow. Love, A. E. H. (1944), A Treatise on the Mathematical Theory of Elasticity, Dover, New York. Mura, T. (1987), Micromechanics of Defects in Solids, Martinus Nijhoff, Dordrecht, The Netherlands. Ting, T. C. T. (1996), Anisotropic Elasticity, Oxford University Press, New York. Wu, J. J., Ting, T. C. T., and Barnett, D. M., eds. (1991), Modern Theory of Anisotropic Elasticity and Applications, SIAM, Philadelphia.
15 Plane Contact Problems
The basic problem considered in this chapter is one in which a rigid “punch” is forced into the surface of an elastic halfspace of semiinﬁnite extent. If the indenter is idealized as rigid, the problem is displacement driven. We examine the problem by both considering imposed forces on the surface of a halfspace as well as by imposing displacements. Plane strain conditions are assumed to prevail.
15.1 Wedge Problem Consider the problem of a “wedge” loaded at its corner by a force f as shown in Fig. 15.1. The geometry involved suggests that a polar coordinate system be used. We seek solutions of the form σ = f (r )g(θ),
(15.1)
so that all solutions are selfsimilar in angular form. Note that the solutions must be such that σ ∼ 1/r ⇒ f (r ) ∼ 1/r,
(15.2)
since when considering equilibrium, the traction on any arc must decrease as 1/r , because the arc length increases in proportion to r . Thus we seek solutions to the biharmonic equation that lead to stresses corresponding to (15.2). Appealing to the inventory of solutions found earlier in Chapter 10, we try φ = C1r θ sin θ + C2r θ cos θ + C3r ln r cos θ + C4r ln r sin θ.
(15.3)
These give rise to stresses of the form 1 (2C1 cos θ − 2C2 sin θ + C3 sin θ + C4 sin θ) , r 1 = (C3 sin θ − C4 cos θ) , r 1 = (C3 cos θ + C4 sin θ) . r
σrr = σr θ σθ θ
(15.4)
271
272
15. Plane Contact Problems
y r
fx
β α
θ
Figure 15.1. Wedge loaded by corner point forces.
x
fy
The sides of the wedge are stressfree, i.e., σθr = σθ θ = 0 on
θ = α, β,
(15.5)
which leads to C3 = C4 = 0. The constants C1 and C2 are determined by imposing global equilibrium β C1 cos θ − C2 sin θ a cos θ dθ = 0, fx + 2 a α (15.6) β C1 cos θ − C2 sin θ a sin θ dθ = 0. fy + 2 a α Solving (15.6) we obtain (C1 − C2 ) sin2 θβα + (C1 + C2 ) sin θ cos θβα = (C2 − C1 )(β − α)−( fx − fy ), (C1 + C2 ) sin2 θβα + (C2 − C1 ) sin θ cos θβα = (C2 + C1 )(β − α)+( fx − fy ). Since C3 = C4 = 0, all rays are traction free, i.e., σr θ = σθ θ = 0 at each θ. A particularly interesting case is that of a halfplane, obtained by setting α = −π and β = 0. In that case (15.6), or (15.1), yields fx + πC1 = 0, fy − πC2 = 0,
(15.7)
and thus 2 fy sin θ 2 fx cos θ − . (15.8) π r π r We will ﬁnd convenient in the sequel to redeﬁne the convention used to describe the applied forces. In fact, let us redeﬁne the coordinate system as shown in Fig. 15.2. If we call fy = −P, and ignore for the moment the tangential force fx , we obtain σrr = −
σrr = −
2P cos θˆ . π r
P x θ r
^
θ y
Figure 15.2. Redeﬁned polar coordinate system.
(15.9)
15.1. Wedge Problem
273
The Cartesian components of stress for the case of an applied normal load are σxx = σrr sin2 θˆ = −
x2 y 2P , π (x 2 + y2 )2
σ yy = σrr cos2 θˆ = −
y3 2P , π (x 2 + y2 )2
σxy = σrr sin θˆ cos θˆ = −
(15.10)
xy2 2P . π (x 2 + y2 )2
To proceed, recall that the strain components, for the considered twodimensional case, are err =
∂ur 1 − ν 2 2P cos θˆ =− , ∂r E π r
1 ∂uθ ν(1 + ν) 2P cos θˆ ur + = , r r ∂θ E π r ∂uθ uθ σr θ 1 1 ∂ur + − = 0. = = 2 r ∂θ ∂r r 2G
eθ θ = er θ
(15.11)
The above equations can be integrated to obtain the displacement components ur = −
(1 − 2ν)(1 + ν) (1 − ν 2 ) 2P cos θˆ ln r − Pθˆ sin θˆ + a1 sin θˆ + a2 cos θˆ πE πE
(15.12)
and uθ =
ν(1 + ν) (1 − ν 2 ) 2P sin θˆ ln r + 2P sin θˆ πE πE (1 − 2ν)(1 + ν) (1 − 2ν)(1 + ν) Pθˆ cos θˆ + P sin θˆ − πE πE + a1 cos θˆ − a2 sin θˆ + a3r.
(15.13)
If the body does not translate or rotate, then a1 = a2 = a3 = 0. At the surface, where θˆ = ±π/2, we have ur θ=π/2 = −ur θ=−π/2 =− ˆ ˆ uθ θ=π/2 = −uθ θ=−π/2 ˆ ˆ
(1 − 2ν) (1 − 2ν)(1 + ν) P=− P, 2E 4G
(1 − ν 2 ) 2P ln r + a, = πE
(15.14)
where a is a constant combined from the remaining terms in (15.13) that do not involve r . To determine this constant, a reference point is needed from which to measure displacement. If uθ = 0 at say r = r0 , then = −uθ θ=−π/2 =− uθ θ=π/2 ˆ ˆ
(1 − ν 2 ) 2P ln(r0 /r ). πE
(15.15)
Consider next the tangential force fx = F. A similar analysis yields σrr = −
2F cos θ , π r
σθ θ = σr θ = 0.
(15.16)
274
15. Plane Contact Problems
The corresponding Cartesian stress components are σxx = −
x3 2F , 2 π (x + y2 )2
σ yy = −
xy2 2F , 2 π (x + y2 )2
σxy = −
x2 y 2F . 2 π (x + y2 )2
(15.17)
Analysis of the displacements reveals that 1 − ν2 2F ln r + b, πE (1 − 2ν)(1 + ν) = F. 2E
ur θ=0 = −ur θ=π = − uθ θ=0 = uθ θ=π
(15.18)
Equation (15.18) shows an interesting effect that the entire surface at x > 0 is depressed by an amount proportional to F, whereas the surface behind the point force is raised by an equal amount. In a manner similar to the angular displacement due to a point normal force, the constant b in (15.18) can be determined by selection of a reference point rt , so that ur θ=0 = −ur θ=π = −
(1 − ν 2 ) 2F ln(rt /r ). πE
(15.19)
15.2 Distributed Contact Forces The solutions listed above can be used as Green’s functions for constructing the solutions to the elastic ﬁelds of distributed forces on the surface of an inﬁnitely extended halfplane. Let the contact area be −a ≤ x ≤ a, and let the distributed normal and tangential forces be p(x) and f (x), respectively. The resulting stresses are obtained via superposition as σxx = −
2y π 3
σ yy = −
2y π
σxy = −
2y2 π
a −a
p(s)(x − s)2 ds 2 − 2 2 2 [(x − s) + y ] π
a −a a −a
a
−a 2
p(s) ds 2y − 2 2 2 [(x − s) + y ] π p(s)(x − s) ds 2y − 2 2 2 [(x − s) + y ] π
f (s)(x − s)3 ds , [(x − s)2 + y2 ]2 a −a a
−a
f (s)(x − s) ds , [(x − s)2 + y2 ]2
(15.20)
f (s)(x − s)2 ds . [(x − s)2 + y2 ]2
This generalizes the result for normal force loading given earlier to include tangential force loading. Note, however, that the sign convention for the normal load is reversed here. When the radial displacement is given in terms of the Cartesian coordinates, the ln r terms become sgn(x) ln x. Thus, using the means employed by Johnson (1985) to handlethe sign change in uθ at the surface, we ﬁnd
15.2. Distributed Contact Forces
275
x a (1 − 2ν)(1 + ν) p(s) ds − p(s) ds 2E −a x 2 a 2(1 − ν ) f (s) ln x − s ds + a1 − πE −a
u¯ x = −
(15.21)
and 2(1 − ν 2 ) u¯ y = − πE
a −a
p(s) ln x − s ds
(1 − 2ν)(1 + ν) + 2E
x −a
a
f (s) ds −
(15.22)
f (s) ds + a2 ,
x
where u¯ x , u¯ y are the displacements on the surface. Note how splitting the range of integration of the integrals handles the sign switch inherent in uθ , as discussed above. The integration constants, here listed as a1 and a2 , have already been discussed and do yield an arbitrary rigid body translation that is undetermined. When the distortions are computed, however, there is no ambiguity, so that (1 − 2ν)(1 + ν) 2(1 − ν 2 ) a f (s) ∂ u¯ x =− p(x) − ds, ∂x E πE −a x − s (15.23) ∂ u¯ y 2(1 − ν 2 ) a p(s) (1 − 2ν)(1 + ν) =− ds + f (x). ∂x πE E −a x − s The integrals in (15.23) are interpreted as Cauchy principal values where needed, that is in −a ≤ x ≤ a. Some interesting features arise. For example, let f (x) = 0 and consider for the moment only normal applied forces. The normal strain on the surface, e¯ xx , is in this case e¯ xx =
(1 − 2ν)(1 + ν) ∂ u¯ x =− p(x). ∂x E
(15.24)
On the other hand, from the elastic constitutive relation in plane strain, e¯ xx =
1 (1 − ν 2 )σ¯ xx − ν(1 + ν)σ¯ yy . E
(15.25)
If the two expressions are to be equal, we must have σ¯ xx = σ¯ yy = − p(x).
(15.26)
This simple result is interesting. Since in plane strain σ¯ zz = ν(σ¯ xx + σ¯ yy ) and ν is, say, in a typical range 1/3 ≤ ν ≤ 1/2, the state of stress under the indenter that applies p(x) is one of nearly pure hydrostatic stress. This, in turn, means that plastic deformation tends to be suppressed just under the contact surface. 15.2.1 Uniform Contact Pressure Here we consider the problem of uniform loading over the strip −a ≤ x ≤ a with the normal stress p0 , as depicted in Fig. 15.3. This problem has been already considered in
276
15. Plane Contact Problems po a
a
θ1
θ2
r 2
x
r1
Figure 15.3. Uniform contact pressure on a halfplane.
(x,y) y
Chapter 12 (see Fig. 12.3), where the stresses were found to be given by p0 [2(θ1 − θ2 ) + sin(2θ1 ) − sin(2θ2 )] , 2π p0 =− [2(θ1 − θ2 ) − sin(2θ1 ) + sin(2θ2 )] , 2π p0 = [cos(2θ1 ) − cos(2θ2 )] . 2π
σxx = − σ yy σxy
(15.27)
The deﬁnitions of the angles θ1 and θ2 are indicated in Fig. 15.3. Here we compute the corresponding displacements and displacement gradients. From (15.23), as long as −a ≤ x ≤ a, we have (1 − 2ν)(1 + ν) ∂ u¯ x =− p0 . ∂x E
(15.28)
Care must be taken to note that, from (15.21), u¯ x no longer changes beyond x > a or x < −a because of the fact that p(x) = 0 for x > a. Then, if the origin is taken as ﬁxed, and x ≤ a, (1 − 2ν)(1 + ν) p0 x, E
(15.29)
(1 − 2ν)(1 + ν) sgn(x) p0 a. E
(15.30)
u¯ x (x) = − and, if x > a, u¯ x (x) = − As for u¯ y , we have
∂ u¯ y 2(1 − ν 2 ) =− ∂x πE
a −a
p0 ds , x−s
where the principal value is to be taken if x ≤ a. Thus, we form x− a a ds ds ds = lim − →0 x−s −a x − s −a x+ s − x
x− = lim − ln(x − s)−a − ln(s − x)ax+
(15.31)
(15.32)
→0
= ln(x + a) − ln(a − x). Therefore, ∂ u¯ y 2(1 − ν 2 ) =− p0 [ln(a + x) − ln(a − x)], ∂x πE
(15.33)
15.3. DisplacementBased Contact fo
a
x
a
θ1 r1
θ2
r 2
277
Figure 15.4. Uniform tangential force on a halfplane.
x,y y
and, upon integrating, " # a−x 2 (1 − ν 2 ) a+x 2 p0 (a + x) ln u¯ y (x) = − + (a − x) ln + C. πE a a We note that this expression holds for any range of x.
15.2.2 Uniform Tangential Force Consider the case of a halfplane loaded on the patch −a ≤ x ≤ a by a uniform tangential stress f0 . With the angles as deﬁned in Fig. 15.4, the relations (15.20) yield the stresses f0 [4 ln(r1 /r2 ) − cos(2θ1 ) + cos(2θ2 )], 2π f0 [cos(2θ1 ) − cos(2θ2 )], = 2π f0 [2(θ1 − θ2 ) + sin(2θ1 ) − sin(2θ2 )]. =− 2π
σxx = σ yy σxy
(15.34)
where r1,2 = [(x ∓ a)2 + y2 ]1/2 . When the equations (15.22) are examined it becomes obvious that the relations obtained for the displacements produced by uniform normal pressure give the displacements for the tangential stress if we make the following transitions (u¯ x )tangential (u¯ y )normal , (u¯ y )tangential (u¯ x )normal .
(15.35)
15.3 DisplacementBased Contact: Rigid Flat Punch Instead of imposing forces on the contact surface, suppose that displacements are imposed, say by a rigid punch of a prescribed shape. This would be equivalent to the imposition of du¯ x /dx and du¯ y /dx by the curved surface of the punch. The relations (15.23) now read
a
−a
a
−a
π(1 − 2ν) πE f (s) ds = − p(x) − u¯ (x), x−s 2(1 − ν) 2(1 − ν 2 ) x π(1 − 2ν) πE p(s) ds = f (x) − u¯ (x), x−s 2(1 − ν) 2(1 − ν 2 ) y
where u¯ x (x) = du¯ x /dx and u¯ y (x) = du¯ y /dx.
(15.36)
278
15. Plane Contact Problems
For a frictionless ﬂat rigid punch, with f (x) = 0 and u¯ y prescribed, we have
a
−a
πE p(s) ds = − u¯ (x). x−s 2(1 − ν 2 ) y
(15.37)
In this case, as in (15.28), we have u¯ x (x) = −
(1 − 2ν)(1 + ν) p(x). E
(15.38)
Note that the integral equation in (15.37) is singular. Its solutions of a general nature are given in Section 19.8. Here we simply note that the singular integral equation a ζ (s) ds = g(x) (15.39) PV x −s −a has the solution, if unbounded at the end points, given by ζ (x) =
1 2 2 π (a − x 2 )1/2
a
−a
C (a 2 − s 2 )1/2 g(s) ds + 2 2 , x−s π (a − x 2 )1/2
(15.40)
where C=π
a
−a
ζ (x) dx.
(15.41)
For the rigid punch, u¯ y (x) = 0 on −a ≤ x ≤ a, and
a
−a
p(s) ds = 0, x−s
(15.42)
which gives p(x) =
π(a 2
p0 , − x 2 )1/2
(15.43)
where p0 is the total load applied by the force distribution of the punch. The derived result is, of course, the same force distribution as used earlier in Chapter 12 (see Fig. 12.5). The displacement distribution outside the punch can be found readily from (15.21). The result is 2(1 − ν 2 ) a u¯ y (x) = − p(s) ln x − s ds + δ y πE −a " (15.44) 2 1/2 # x x 2(1 − ν 2 ) p0 ln + =− + δy, πE a a2 where δ y is an integration constant determined by selecting a datum from which to measure displacement. The displacement component, u¯ x is found from (15.21) to be u¯ x (x) = −
(1 − 2ν)(1 + ν) p0 sin−1 (x/a). πE
(15.45)
15.4. Suggested Reading
279
15.4 Suggested Reading FischerCripps, A. C. (2000), Introduction to Contact Mechanics, SpringerVerlag, New York. Galin, L. A. (1961), Contact Problems in the Theory of Elasticity, School of Physical Sciences and Applied Mathematics, North Carolina State College. Gladwell, G. M. L. (1980), Contact Problems in the Classical Theory of Elasticity, Alphen aan den Rijn, The Netherlands. Johnson, K. L. (1985), Contact Mechanics, Cambridge University Press, New York. Timoshenko, S. P., and Goodier, J. N. (1970), Theory of Elasticity, 3rd ed., McGrawHill, New York.
16 Deformation of Plates
The deformation of thin plates is considered here. Plates are assumed to be thin when their thickness is very small compared to their other two dimensions in their plane. Deformations and strains are assumed to be small and the material of the plates is isotropic linear elastic.
16.1 Stresses and Strains of Bent Plates Plates, when bent, develop a transition from one side to the other from tension to compression and thus contain a neutral surface. If homogeneous, this neutral surface may be assumed to pass through the middle of the plate thickness (see Fig. 16.1). The coordinate system is accordingly taken so that the normal to the plane of the plate is the z axis, whereas the plane of the plate is in the xy plane. Displacement components within the plane are assumed to be negligible compared to those normal to the plate. The displacement normal to the plate, along the z axis, is designated as w. Thus, along the neutral plane (0) u(0) x = u y = 0,
u(0) z = w(x, y).
(16.1)
For small deﬂections of the plate, the displacement w is assumed to be small compared to the thickness h of the plate. Because plate is assumed to be so thin, the forces acting on the plate surface that induce deformation are typically small. Stresses within the plate, however, due to bending and shear are not. Accordingly, the plate surface is approximated as being stress free so that, if n is the normal to the plate, n · σ = 0 σi j n j = 0.
(16.2)
Moreover, since the deformations are small, i.e., the plates are but slightly bent, it may be assumed that, n ≈ ez where ez is the unit base vector along the z axis. Thus we take as an approximation that σxz = σ yz = σzz = 0. The linear elastic constitutive relations yield E E exz, e yz, σ yz = 1+ν 1+ν E [(1 − ν)ezz + ν(exx + e yy )]. σzz = (1 + ν)(1 − 2ν)
σxz =
280
(16.3)
16.2. Energy of Bent Plates
281
z
h/2
x
w
Figure 16.1. Coordinate geometry of a thin plate that undergoes deﬂection w.
h/2
When the deﬁnitions of the small strains are recalled, and if we take uz = w(x, y), it is found that ∂u y ∂w ∂w ∂ux =− , =− , ∂z ∂x ∂z ∂y ν ezz = − (exx + e yy ) . 1−ν
(16.4)
Thus, plane cross sections remain plane and orthogonal to the midsurface of the plate. The ﬁrst two of (16.4) are integrated wrt z to ﬁnd that ux = −z
∂w , ∂x
u y = −z
∂w . ∂y
(16.5)
The constants of integration were made equal to zero, so that the displacements would be zero at z = 0. Now, the nonzero strain components can be calculated as exx = −z
∂ 2w , ∂ x2
exz = e yz = 0,
∂ 2w ∂ 2w , , exy = −z 2 ∂y ∂ x∂ y 2 ν ∂ w ∂ 2w . z ezz = + 1−ν ∂ x2 ∂ y2 e yy = −z
(16.6)
It may be noticed, in retrospect, that from the last expression for ezz and the relationship ezz = ∂uz/∂z, the integration gives uz =
ν z2 2 ∇ w + w(x, y) . 1−ν 2
(16.7)
Because the plate is thin, this is approximately equal to w, in accord with the initial assumption uz = w(x, y). The same order of approximation is common in the beam bending theory. The underlying assumptions used in the above formulation of thin plate theory are known as the Kirchhoff hypotheses.
16.2 Energy of Bent Plates The elastic strain energy density of a plate can be expressed as #& 2 " 2 2 2 ∂ w ∂ w ∂ 2w 1 ∂ 2w ∂ 2w 1 2 E W = σi j ei j = z + + − . 2 1 + ν 2(1 − ν) ∂ x 2 ∂ y2 ∂ x∂ y ∂ x 2 ∂ y2 The total elastic energy is obtained by integrating this expression throughout the plate. If the thickness of the plate is h, so that z runs from z = − 12 h to z = 12 h, and because the deformations are small, it may be assumed that the area element in the plane of the plate
282
16. Deformation of Plates
is still just dxdy. Therefore, the total elastic energy of the plate is
W=
Eh3 (16.8) 24(1 − ν 2 ) V " #& 2 2 2 ∂ 2w ∂ w ∂ 2w ∂ 2w ∂ 2w × + + 2(1 − ν) − dx dy. ∂ x2 ∂ y2 ∂ x∂ y ∂ x 2 ∂ y2 A W dV =
The plate is assumed to be thin and to deform uniformly through the thickness.
16.3 Equilibrium Equations for a Plate Imagine a variation in deﬂection, δw; we wish to calculate the accompanying variation in strain energy δW. To begin, examine the ﬁrst term in the integral in (16.8), i.e., the integral of 12 (∇ 2 w)2 . The factor 1/2 is placed for later convenience. It follows that 1 δ 2
(∇ w) dx dy = 2
∇ 2 w∇ 2 δw dx dy
2
A
A
∇ 2 w div (grad δw) dx dy
=
A
(16.9)
div (∇ 2 w grad δw) dx dy −
=
grad δw · grad ∇ 2 w dx dy.
A
A
The above transformation is veriﬁed with the help of the following identity, phrased in component form as ∂ div ∇ 2 w grad δw = ∂xj
∇ 2w
∂δw ∂xj
=
∂∇ 2 w ∂δw + ∇ 2 w ∇ 2 δw. ∂xj ∂xj
The divergence theorem enables an immediate transformation of the ﬁrst integral in (16.9), i.e.,
div(∇ 2 w grad δw) dx dy = A
∇ 2 w(n · grad δw) d = C
∇ 2w C
∂δw d, ∂n
(16.10)
where ∂/∂n denotes a derivative along the outward pointing normal to C, the curve bounding the plate area A. The second integral in (16.9) is transformed as
grad δw · grad ∇ w dx dy =
div (δw grad∇ w) dx dy −
2
A
δw ∇ 4 w dx dy
2
A
A
δw (n · grad ∇ 2 w) d −
= C
∂∇ 2 w δw d − = ∂n C
δw ∇ 4 w dx dy A
δw ∇ 4 w dx dy. A
16.3. Equilibrium Equations for a Plate y
283
n θ
Figure 16.2. Coordinates for a plate’s edge.
x
The above transformation can be veriﬁed by forming the following identity ∂ ∂∇ 2 w div δw grad ∇ 2 w = δw ∂xj ∂xj =
∂ ∂ 2 ∂δw ∂∇ 2 w + δw ∇ w, ∂xj ∂xj ∂xj ∂xj
where the operator ∂∂x j ∂∂x j ∇ 2 w = ∇ 4 w is the biharmonic operator. When these results are combined, there follows ∂∇ 2 w ∂δw 1 2 2 4 d + ∇ 2 w d. (16.11) (∇ w) dx dy = δw∇ w dx dy − δw δ 2 ∂n ∂n A A C C Attention is now turned to the second term in (16.8). We want to evaluate # " 2 2 ∂ w ∂ 2w ∂ 2w δ − dx dy ∂ x∂ y ∂ x 2 ∂ y2 A 2 ∂ w ∂ 2 δw ∂ 2 w ∂ 2 δw ∂ 2 δw ∂ 2 w − = − 2 dx dy. ∂ x∂ y ∂ x∂ y ∂ x 2 ∂ y2 ∂ x 2 ∂ y2 A
(16.12)
The integrand can be rewritten as the divergence of a certain vector, viz., ∂δw ∂ 2 w ∂δw ∂ 2 w ∂ ∂δw ∂ 2 w ∂ ∂δw ∂ 2 w − − I= + . ∂ x ∂ y ∂ x∂ y ∂ x ∂ y2 ∂ y ∂ x ∂ x∂ y ∂ y ∂ x2 Thus, after using the Stokes formula (2.3), we have # " 2 2 ∂ w ∂ 2w ∂ 2w δ − dx dy ∂ x∂ y ∂ x 2 ∂ y2 A ∂δw ∂ 2 w ∂δw ∂ 2 w = − d cos θ ∂ y ∂ x∂ y ∂ x ∂ y2 C ∂δw ∂ 2 w ∂δw ∂ 2 w , − + d sin θ ∂ x ∂ x∂ y ∂ y ∂ x2 C
(16.13)
where θ is the angle that the outward pointing normal to the edge of the plate makes with the x axis. The derivatives appearing in the expression for I are expressed in terms of n and (Fig. 16.2) as ∂ ∂ = cos θ − sin θ ∂x ∂n ∂ ∂ = sin θ + cos θ ∂y ∂n
∂ , ∂ ∂ . ∂
(16.14)
284
16. Deformation of Plates
When these are used in (16.13), and terms rearranged, the result is assembled and combined with the contributions from (16.11). The total variation in W is found to be δW = where
Eh3 (I1 + I2 + I3 ), 12(1 − ν 2 )
(16.15)
I1 =
∇ 4 w δw dx dy, A
I2 = −
δw C
−
δw(1 − ν) C
and
I3 = C
∂∇ 2 w d ∂n
2 ∂ w ∂ 2w ∂ ∂ 2w 2 2 − θ − sin θ) + (cos sin θ cos θ d , ∂ ∂ y2 ∂ x2 ∂ x∂ y
∂δw 2 ∂ 2w ∂ 2w ∂ 2w − sin2 θ 2 − cos2 θ 2 d. ∇ w + (1 − ν) 2 sin θ cos θ ∂n ∂ x∂ y ∂x ∂y
The variation we wish to perform to determine the equilibrium conﬁguration of the plate is that of the potential energy. For this we seek conﬁgurations that minimize %. We thus require pδw dx dy = 0. (16.16) δ% = δW − A
This variation includes both surface and line integral terms, which must both vanish. For the surface integrals we obtain Eh3 4 w − p δw dx dy = 0. (16.17) ∇ 2 A 12(1 − ν ) Since the variation in δw is arbitrary, this integral can only vanish if Eh3 ∇ 4w − p = 0 , 12(1 − ν 2 )
(16.18)
i.e., ∇ 4w =
p , D
D=
Eh3 . 12(1 − ν 2 )
(16.19)
The coefﬁcient D is the socalled ﬂexural rigidity of the plate. The distributed load over the plate in the z direction is p = p(x, y). Boundary conditions are obtained by setting the line integrals to zero. If the edges of the plate are free, i.e., no external forces act on them, δw and δ∂w/∂n are arbitrary and thus the integrands of the line integrals must vanish at each point on the plate’s edge. This gives 2 ∂ ∂ w ∂ 2w ∂ 2w ∂∇ 2 w 2 2 + (1 − ν) − θ − sin θ) sin θ cos θ = 0, (16.20) + (cos ∂n ∂ ∂ y2 ∂ x2 ∂ x∂ y
16.4. Shear Forces and Bending and Twisting Moments b
285
Figure 16.3. (a) Clamped vs. (b) simply supported edge conditions.
a
and
2 2 ∂ 2w 2 ∂ w 2 ∂ w − sin θ − cos θ ∇ w + (1 − ν) 2 sin θ cos θ = 0. ∂ x∂ y ∂ x2 ∂ y2 2
(16.21)
If, instead, the plate’s edges are clamped, we have w = 0 and ∂w/∂n = 0 (Fig. 16.3). The shear force and moment are readily calculated as follows. For example, the force Q acting on an edge point of the plate is given by Q = ∂W/∂w, because δW = Qδw. But, looking at I2 in (16.16), we see that its integrand is just this derivative devided by −D, because of the sign ahead of the integral. Likewise, the moment M at an edge point is related to energy changes as δW = M∂δw/∂n because ∂δw/∂n represents, in an inﬁnitesimal strain theory, the variation in rotation angle the moment acts on. But this is just the integrand of I3 in (16.3) devided by D. It can be shown, with the use of (16.14) and taking θ = 0 after differentiation, that these reduce to 3 ∂θ ∂ 2 w ∂ w , + ν Q= D ∂n3 ∂ ∂n2 (16.22) ∂ 2w M= D 2 . ∂n A third type of condition is where the edges lie on ﬁxed supports so that w = 0, but the edges are free to rotate and thus support no moment. Also δw = 0, but ∂δw/∂n = 0. Thus (16.21) remains valid, but (16.22) no longer holds, in general. The reaction force is still given by the ﬁrst of (16.22) at points where the edge is supported, but at such points the reaction moment is zero. The boundary condition (16.21) can be simpliﬁed by noting that w = 0 when the edges are supported, and that ∂w/∂ = 0 and ∂ 2 w/∂2 = 0 as well. In that case, w = 0,
∂θ ∂w ∂ 2w = 0. +ν 2 ∂n ∂ ∂n
(16.23)
In deriving these formulas, as in (16.22), the angle θ may, without loss of generality, be set to zero after differentiation. This simply means that we choose to measure θ from the normal at the point at which the boundary condition is invoked.
16.4 Shear Forces and Bending and Twisting Moments The following expressions hold for the shear forces and bending and twisting moments per unit length of a rectangular plate (Fig. 16.4), Qx = D
∂ 2 ∇ w , ∂x
Qy = D
∂ 2 ∇ w , ∂y
∂ 2w ∂ 2w +ν 2 , Mx = D ∂ x2 ∂y
(16.24)
286
16. Deformation of Plates
Figure 16.4. Positive directions of the shear force, bending and twisting moments in a rectangular plate element.
My = D
∂ 2w ∂ 2w , + ν ∂ y2 ∂ x2
Mxy = D(1 − ν)
(16.25)
∂ 2w . ∂ x∂ y
From equilibrium conditions they are related by ∂ Qy ∂ Qx + = p, ∂x ∂y ∂ Mxy ∂ Mx + = Qx , ∂x ∂y
(16.26)
∂ Mxy ∂ My + = Qy . ∂x ∂y The effective shear forces (that need vanish at free edges) are Vx = Qx +
∂ Mxy , ∂y
Vy = Qy +
∂ Mxy . ∂x
(16.27)
Finally, the stress components in the plate are σxx = −
12Mx z, h3
σ yy = −
12My z, h3
σxy = −
12Mxy z. h3
(16.28)
If we deﬁne M=
1 (Mx + My ) , 1+ν
(16.29)
we also have M , ∇2 M = p , D ∂M ∂M , Qy = . Qx = ∂x ∂y
∇ 2w =
(16.30)
In the case of circular plate, the shear forces (per unit length) can be determined from Qr = D
∂ 2 ∇ w , ∂r
Qθ = D
1 ∂ 2 ∇ w . r ∂θ
(16.31)
16.5. Examples of Plate Deformation
287
Figure 16.5. Positive directions of the shear force, bending and twisting moments in a plate element in polar coordinates.
The bending and twisting moments per unit length (Fig. 16.5) are 2 1 ∂ 2w ∂ w 1 ∂w , + Mr = D + ν ∂r 2 r ∂r r 2 ∂θ 2 Mθ = D
1 ∂w 1 ∂ 2w ∂ 2w + 2 + ν , r ∂r r ∂θ 2 ∂r 2
(16.32)
1 ∂w 1 ∂ 2w − 2 Mr θ = D(1 − ν) . r ∂r ∂θ r ∂θ
The effective shear forces are given by Vr = Qr +
1 ∂ Mr θ , r ∂θ
Vθ = Qθ +
∂ Mr θ . ∂r
(16.33)
The corresponding stress components are σrr = −
12Mr z, h3
σθ θ = −
12Mθ z, h3
σr θ = −
12Mr θ z. h3
(16.34)
16.5 Examples of Plate Deformation 16.5.1 Clamped Circular Plate Consider a circular plate of radius a, clamped around its edge, and loaded under the action of gravity. Let the mass density be ρ, and the plate’s thickness h. We seek a solution for the deﬂection of the plate. In the equation of equilibrium (16.19), we identify p = −ρhg, where g is the gravitational acceleration constant. Thus, ∇ 4 w = 64β,
(16.35)
where β = −3ρg(1 − ν)/16h2 E is a constant factor, made for convenience. Since the plate is circularly symmetric, w = w(r ) only, and we have 1 d dw ∇ 2w = r , (16.36) r dr dr and 1 d d ∇ w= r r dr dr 4
1 d r dr
! dw r . dr
(16.37)
288
16. Deformation of Plates
As noted in Chapter 10, and in particular in equation (10.58), the general integral of (16.35) is r r (16.38) w(r ) = βr 4 + Ar 2 + B + Cr 2 ln + F ln . a a The particular solution βr 4 is included to account for the righthand side of (16.35). We can set F = 0 because w is bounded everywhere, including at r = 0. Also, we set C = 0 since its term produces a singularity at r = 0 in ∇ 2 w. The boundary conditions are that at r = a, w = 0 and dw/dr = 0. With these, A and B are determined easily with the end result for the deﬂection, w(r ) = β(a 2 − r 2 )2 .
(16.39)
16.5.2 Circular Plate with Simply Supported Edges Consider a circular plate, again loaded by gravity force, whose edges are simply supported so that the boundary conditions (16.23) apply. Because for this circular plate dθ/d = 1/r , the conditions in (16.23) become w = 0,
d2 w ν dw = 0, + dr 2 r dr
on r = a.
(16.40)
The solution for w is similar as in previous case, and by invoking the conditions (16.40), it is found that 5+ν 2 a − r2 . w(r ) = β(a 2 − r 2 ) (16.41) 1+ν 16.5.3 Circular Plate with Concentrated Force If a clamped circular plate is loaded by a concentrated force of magnitude f at its center, we can write p = f δ(r ). The integration of (16.19) then yields a 12(1 − ν 2 ) 12(1 − ν 2 ) 4 r ∇ w dr = f δ(r ) dA = f. (16.42) 2π Eh3 Eh3 0 A In this case of a concentrated point force, the term involving the coefﬁcient C is retained so that the solution for w becomes r (16.43) w(r ) = Ar 2 + B + Cr 2 ln . a When (16.43) is used in (16.42), it is found that C = 3(1 − ν 2 ) f/2π Eh3 . The clamped boundary conditions, w = 0 and dw/dr = 0 at r = a, yield the coefﬁcients Aand B, so that 3 f (1 − ν 2 ) 1 2 a 2 2 (a w(r ) = − r ) − r ln . (16.44) 2π Eh3 2 r 16.5.4 Peeled Surface Layer Imagine a thin surface layer peeled off a thick elastic body, as shown in Fig. 16.6. The resistance is due to adhesive forces between the layer and the block. We seek a relation between the surface energy and a measurable feature of the process, such as the shape of the peeled layer. Note that the work done in decohering the layer is given by γ¯ = 2γ0 − γa ,
16.6. Rectangular Plates
289
z h
x
w
Figure 16.6. Peeled layer.
where γ0 is the surface energy of a newly created interface (of which there are two with a surface energy of γ0 ), and γa is the surface energy of the initial adhesive layer (which is destroyed by the peeling process). The layer is treated as a thin plate with one edge clamped at the edge being torn off. As above, the angle made by the layer, to ﬁrst order, is ∂w/∂ x, and its variation is ∂δw/∂ x. Thus the increment of work done by the moment M, given by the second of (16.22), and working through an increment of extension δx, is M
δx∂ 2 w ∂δw =M . ∂x ∂ x2
(16.45)
By equating this increment of work to γ¯ δx, we ﬁnd Eh3 γ¯ = 12(1 − ν 2 )
∂ 2w ∂ x2
2 .
(16.46)
16.6 Rectangular Plates There are cases, other than those involving circular plates, where closed form solutions are possible. Notable among them are cases concerning plates with rectangular shapes such as illustrated in Fig. 16.7. We will take as a speciﬁc example cases where the edges are simply supported, so that displacements normal to the plate and moments vanish at the edges. The equation of equilibrium for a plate is ∇ 4 w(x, y) = p(x, y)/D,
(16.47)
where D = Eh3 /12(1 − ν 2 ) is the plate ﬂexural rigidity. To meet the boundary conditions of w = 0 at x = 0, a and y = 0, b, as well as the condition of vanishing moment there, w is expanded in a double Fourier sine series w(x, y) =
∞ ∞ m=1 n=1
wmn sin
nπ y mπ x sin . a b
y b Figure 16.7. Geometry of a rectangular thin plate with simply supported edges.
x a
(16.48)
290
16. Deformation of Plates
The boundary conditions, w(0, y) = w(a, y) = w(x, 0) = w(x, b) = 0,
(16.49)
are naturally satisﬁed. The moments are computed from the normal stresses, that in turn are computed from the second derivatives of w(x, y), viz., w,xx and w,yy , which likewise vanish along the edges. To satisfy the plate equilibrium equation, we expand the load function, p(x, y), in a similar double sine series, viz., p(x, y) =
∞ ∞
pmn sin
m=1 n=1
nπ y mπ x sin . a b
(16.50)
The usual procedure, outlined below in a speciﬁc example, is used to compute the Fourier coefﬁcients pmn . When (16.50) and (16.48) are substituted into (16.47), and the coefﬁcients of like harmonics equated, it is found that wmn =
1 pmn . π 4 D [(m/a)2 + (n/b)2 ]2
(16.51)
Thus, w(x, y) =
∞ ∞ nπ y pmn mπ x 1 sin . sin π 4 D m=1 n=1 [(m/a)2 + (n/b)2 ]2 a b
(16.52)
16.6.1 Uniformly Loaded Rectangular Plate For a uniformly loaded plate we let p(x, y) = p0 , and (16.50) becomes p0 =
∞ ∞ m=1 n=1
pmn sin
nπ y mπ x sin . a b
(16.53)
To obtain the coefﬁcients, multiply both sides by sin(r π x/a) sin(sπ y/b), where r and s are integers, and integrate over the area of the plate. Then, a b sπ y rπx sin dx dy p0 sin a b 0 0 b a ∞ ∞ mπ x nπ y rπx sπ y sin dx sin dy. pmn sin sin = a a b b 0 0 m=1 n=1 To evaluate the above integrals, recall that a a/2, mπ x rπx sin dx = sin a a 0, 0 Since,
p0
a
sin 0
rπx dx a
b
sin 0
r = m, r = m.
(16.54)
sπ y dy b
⎧ ⎨ 0, r or s even, b a = p0 [cos(r π) − 1] [cos(sπ ) − 1] = 4ab ⎩ rπ sπ p0 , r and s odd, π 2r s
(16.55)
16.7. Suggested Reading
291
we obtain pmn =
16 p0 , π 2 mn
m, n = 1, 3, 5, . . . ,
(16.56)
and w(x, y) =
∞ 16 p 0 π 6 D m=1,3,5
∞
1 nπ y 1 mπ x sin . sin 2 2 2 mn [(m/a) + (n/b) ] a b n=1,3,5
(16.57)
16.7 Suggested Reading Cook, R. D., and Young, W. C. (1999), Advanced Mechanics of Materials, 2nd ed., Prentice Hall, Upper Saddle River, New Jersey. Landau, L. D., and Lifshitz, E. M. (1986), Theory of Elasticity, 3rd English ed., Pergamon Press, New York. Szilard, R. (2004), Theories and Applications of Plate Analysis: Classical, Numerical, and Engineering Methods, Wiley, Hoboken, New Jersey. Timoshenko, S. P., and WoinowskyKrieger, S. (1987), Theory of Plates and Shells, 2nd ed., McGrawHill, New York. Ugural, A. C. (1999), Stresses in Plates and Shells, 2nd ed., McGrawHill, Boston.
PART 4: MICROMECHANICS
17 Dislocations and Cracks: Elementary Treatment
17.1 Dislocations Consider the plane strain deformation and the Airy stress function of the form φ = Cr ln r cos θ,
C = const.
(17.1)
The corresponding stresses are obtained by using the general expressions from Chapter 10, i.e., (10.4)–(10.6). They give 1 ∂ 2φ 1 ∂φ cos θ + 2 2 =C , r ∂r r ∂θ r sin θ ∂ 1 ∂φ , =C =− ∂r r ∂θ r
σrr = σr θ
σθ θ =
(17.2)
∂ 2φ cos θ . =C ∂r 2 r
The elastic strains may then be deduced from stresses by Hooke’s law. The displacements are then obtained from strains by integration. The end result is C [(1 − ν)θ sin θ − 1/4 cos θ + 1/2(1 − 2ν) ln r cos θ], G C uθ = [(1 − ν)θ cos θ − 1/4 sin θ − 1/2(1 − 2ν) ln r sin θ]. G
ur =
(17.3)
Details of the derivation are given in the subsection below. The shear modulus is G, and ν is the Poisson’s ratio. Clearly, the displacement ﬁeld in this case is nonsingle valued, because ur (θ = 0) − ur (θ = 2π ) = 0, uθ (θ = 0) − uθ (θ = 2π) = −
2πC(1 − ν) ≡ b. G
(17.4)
The physical scenario associated with this is illustrated in Fig. 17.1, which shows that the dislocation is created, in a heuristic manner, by ﬁrst making a cut, and then creating a gap of width b, or removing a slab of material of thickness b, and then rejoining the two sides of the cut. In the case where material has been removed the empty gap would be ﬁlled with 293
294
17. Dislocations and Cracks
y r uθ(0)
θ
gap=b
x
Figure 17.1. Dislocation created by a displacement discontinuity uθ (0) − uθ (2π) = b.
uθ(2π)
material of identical properties. The body is left in the state of stress σrr = −
cos θ Gb , 2π (1 − ν) r
σr θ = −
sin θ Gb , 2π (1 − ν) r
σθ θ = −
cos θ Gb . 2π (1 − ν) r
(17.5)
The magnitude of the socalled Burgers vector of the dislocation is b. The stresses are singular at the center of dislocation (r = 0), and have both a shear and hydrostatic component. For plane strain, σzz = ν(σrr + σθ θ ),
(17.6)
and thus the average normal stress is 1 Gb(1 + ν) cos θ (σrr + σθ θ + σzz) = − . 3 3π (1 − ν) r
σh =
(17.7)
Note that if the dislocation were to move, say along the x axis, this motion would result in a displacement, u = be y across the sections of plane so spanned by this motion. This feature allows for the construction of the stress ﬁeld of a crack, as demonstrated in the next section. The vital role played by dislocations in the process of plastic deformation is dealt with in detail in later chapters of this book. 17.1.1 Derivation of the Displacement Field Since the displacement ﬁeld associated with (17.1) is nonsingle valued, the approach to derive Eqs. (17.3) is outlined here. The reader is directed to Tables 23.1–23.5 in Chapter 23 for further details on stress and displacement ﬁelds in polar coordinates. The radial strain component is 1 ∂ur = [σrr − ν(σθ θ + σzz)], ∂r E which, in the present case of plane strain, becomes err =
∂ur C(1 − 2ν) cos θ = . ∂r 2G r
(17.8)
(17.9)
When integrated this yields ur =
C(1 − 2ν) ln r cos θ + f (θ) , 2G
where f (θ) is the integration function.
(17.10)
17.2. Tensile Cracks
295
Next consider the circumferential component of strain eθ θ . From its deﬁnition in terms of the displacement components, we ﬁnd ∂uθ = r eθ θ − ur . ∂θ
(17.11)
When eθ θ is constructed and (17.10) used in (17.11), the integration gives uθ = with F(θ) =
C(1 − 2ν) C(1 − 2ν) sin θ − ln r sin θ − F(θ) + g(r ) , 2G 2G
f (θ)dθ. Furthermore, recalling the deﬁnition of the shear strain ∂uθ uθ 1 1 ∂ur er θ = + − , 2 r ∂θ ∂r r
(17.12)
(17.13)
and observing that F (θ) = f (θ), there follows F (θ) F(θ) 2C(1 − ν) sin θ g(r ) = + + g (r ) − , G r r r r
(17.14)
or F (θ) + F(θ) −
2C(1 − ν) sin θ = rg (r ) − g(r ) = K , G
(17.15)
where K is a constant. The solution for F(θ) and g(r ) are, accordingly, F(θ) = −
C(1 − ν) AC BC θ cos θ + sin θ + cos θ + K , G G G
(17.16)
and g(r ) = Kr + H .
(17.17)
The additional constants K and H correspond to rigid body motion and can be disregarded. The constants A and B, associated with the homogeneous solution to (17.15) are ﬁxed by imposing the consistency of f (θ) with the known strains. Since f (θ) = −
C(1 − ν) AC BC C(1 − ν) cos θ + θ sin θ + cos θ − sin θ , G G G G
(17.18)
if (17.10) and (17.12) is to reproduce the known strains err , eθ θ , and er θ , we must have A=
1 (3 − 4ν) , 4
B = 0.
(17.19)
This speciﬁes F(θ) and thus the displacement components ur and uθ , with the end results as in (17.3).
17.2 Tensile Cracks Consider the boundary value problem associated with a slitlike crack of length 2a, illustrated in Fig. 17.2. The crack lies within an inﬁnite medium. We assume, as in the case of of the dislocation described above, a plane strain state. Thus the crack is inﬁnitely deep in
296
17. Dislocations and Cracks σο
y
Figure 17.2. Center cracked panel.
a
a
x
σο
the direction normal to the xy plane. The block is subject to a far ﬁeld tensile stress of magnitude σ0 . Boundary conditions are then σxy = σ yy = 0 on σ yy → σ0
− a ≤ x ≤ a, y = 0,
at r → ∞,
(17.20)
σxx , σxy → 0 at r → ∞. This may be solved using a simple method of linear superposition of two companion problems. For the ﬁrst problem we take a simple homogeneous solution (1) σ yy = σ0 ,
(1) (1) σxx , σxy = 0.
(17.21)
For the second problem, we require (2) σxy = 0,
(2) σ yy = −σ0
on
− a ≤ x ≤ a, y = 0,
(2) (2) (2) , σ yy , σxy → 0 at r → ∞. σxx
(17.22)
Clearly, the stress state created as σ = σ (1) + σ (2) will satisfy the crack boundary conditions expressed in (17.20). Problem (2) will be solved by the linear superposition of dislocation solutions obtained in the previous section. This is described next. Let B(ξ )dξ represent a continuous density of dislocations distributed between ξ and ξ + dξ (Fig. 17.3). The coordinate ξ is to lie on the x axis, between −a ≤ ξ ≤ a. This density will produce the stress σ yy (x, 0) = σθ θ (r, 0) = −
GB(ξ )dξ . 2π (1 − ν)(x − ξ )
(17.23)
The stress produced by the distribution of dislocations along the entire length of the crack is a B(ξ ) dξ G = −σ0 , σ yy (x, 0) = − (17.24) 2π(1 − ν) −a x − ξ and thus
a
−a
2π(1 − ν)σ0 B(ξ ) dξ = , x−ξ G
−a ≤ x ≤ a.
σο Figure 17.3. Distribution of dislocations.
σο
(17.25)
17.2. Tensile Cracks
297
To solve this singular integral equation introduce the variables φ and θ, such that x = a cos φ,
ξ = a cos θ.
The equation (17.25) then becomes π 2π(1 − ν)σ0 B(θ) sin θ dθ = , cos φ − cos θ G 0
0 ≤ φ ≤ π.
(17.26)
(17.27)
Call 2π (1 − ν)σ0 G
(17.28)
π sin(nθ) cos(nθ) dθ =− . cos φ − cos θ sin φ
(17.29)
A= for brevity, and note the result π 0
Having this in mind, let B(θ) be expanded in a Fourier series, viz., B(θ) =
∞ n=0
Then,
π
pn
cos(nθ) . sin θ
(17.30)
,∞
pn cos(nθ) dθ = A, cos φ − cos θ n=0
0
(17.31)
i.e., ∞ n=0
π
0
pn cos(nθ) dθ = A. cos φ − cos θ
(17.32)
Using the result from (17.29), this becomes −
∞ n=0
pn
π sin(nφ) = A. sin φ
(17.33)
In fact, with n = 1, we have p1 = −A/π and C 2σ0 (1 − ν) cos θ + , G sin θ sin θ
(17.34)
2σ0 (1 − ν) ξ C . + G sin θ a2 − ξ 2
(17.35)
B(θ) = − or B(ξ ) = −
But the dislocation distribution is an odd function of ξ , as there are no net dislocations on −a ≤ ξ ≤ a. Consequently, a B(ξ ) dξ = 0 ⇒ C = 0, (17.36) −a
and B(ξ ) = −
2σ0 (1 − ν) ξ . G a2 − ξ 2
(17.37)
298
17. Dislocations and Cracks
This means that (2) σ yy
G =− 2π(1 − ν)
a
−a
σ0 B(ξ ) dξ = x−ξ π
ξ dξ −a (x − ξ ) a 2 − ξ 2 x = σ0 −1 + √ , x ≥ 0, y = 0. x2 − a 2 a
Now, recall that the full solution is σ = σ (1) + σ (2) . For example, on the crack line ahead or behind the crack tip, we obtain σ yy = √
σ0 x x2 − a 2
,
x ≥ a, y = 0.
Near the tip, say at x = a + , where a, we have a σ0 (a + ) , ∼ σ0 σ yy → √ 2 2 2a +
on y = 0.
(17.38)
(17.39)
If we write that on the crack line, just ahead of the tip, KI , σ yy (r, 0) = √ 2πr
(17.40)
where r is measured from the crack tip, then
√ KI = σ0 πa ,
(17.41)
which is the socalled stress intensity factor for this center cracked panel geometry. Other components of stress may be generated by integration of those associated with individual dislocations.
17.3 Suggested Reading Broek, D. (1987), Elementary Engineering Fracture Mechanics, 4th ed., Martinus Nijhoff, Dordrecht, The Netherlands. Cherepanov, G. P. (1979), Mechanics of Brittle Fracture, McGrawHill, New York. Friedel, J. (1964), Dislocations, Pergamon, New York. Gdoutos, E. E. (1993), Fracture Mechanics: An Introduction, Kluwer Academic, Dordrecht, The Netherlands. Hull, D., and Bacon, D. J. (1999), Introduction to Dislocations, 3rd ed., ButterworthHeinemann, Boston.
18 Dislocations in Anisotropic Media
18.1 Dislocation Character and Geometry Imagine a cut made within an otherwise unbounded elastic medium, where the cut is over an open surface, Scut , that is bounded by a line, C (see Fig. 18.1). To create the dislocation, material is displaced everywhere across the cut surface by a constant vector, b. The displacement vector b is called the Burgers vector. Where such a displacement would cause a gap, extra material is imagined inserted so as to make the body continuous. Where such displacement would cause material to interpenetrate, the excess material is imagined scraped away. At all points on Scut , the surface is rebonded so that all further displacements are continuous. We note that this process causes the displacement ﬁeld to be nonsingle valued across Scut . In fact, if C is the line bounding the cut surface, and R is a closed circuit surrounding C at any point on C, then ∂u dxm = b, (18.1) ∂ R xm where u is the displacement, and the integral is taken counterclockwise with t, the unit tangent to C, taken in the positive sense. Note that the unit tangent t is continuous as the dislocation line, C, is traversed. At points on the dislocation line, where t b, t · b = ±b, whereas at points where t ⊥ b, t · b = 0. We say that at the former type of point the dislocation line has screw dislocation character, whereas at the latter type of point the line has edge dislocation character. In general, the dislocation line has a mixed character and has both edge and screw character. The ﬁgure illustrates a dislocation line that has extended screw segments and hairpin type loop segments that, at points, have primarily edge character. The elastic ﬁeld is caused by the displacement jump across Scut as measured speciﬁcally by (18.1); there are no body forces or applied traction. Thus, the dislocation represents a purely internal source of stress. To construct the elastic ﬁeld, consider the identity ∞ δimδ(x − x )ui (x ) d3 x (18.2) um(x) = −∞
and recall that δimδ(x − x ) = −Ci jkl
∂ 2 Gkm , ∂ xl ∂ x j
(18.3) 299
300
18. Dislocations in Anisotropic Media
e cut surface
e
2 e
3 (+)
1 t
()
t
Figure 18.1. Dislocation loop and cut surface.
(1)
t
b b t
(2)
C
where G is the Green’s function. Thus, formally, the displacement ﬁeld of the dislocation can be written as ∞ 2 ∂ Gkm um(x) = −Ci jkl ui (x ) d3 x . (18.4) −∞ ∂ xl ∂ x j Since G is a function of x − x , we may write ∂ ∂ Gkm(x − x ) = − Gkm(x − x ), ∂xj ∂xj and um(x) = Ci jkl
−∞
= Ci jkl
∞
∞
−∞
∂ ∂ xl ∂ ∂ xl
"
# ∂Gkm(x − x ) ui (x ) d3 x ∂ x j
(18.5)
(18.6)
& ∂ui (x ) ∂ d3 x . [Gkm(x − x )ui (x )] − Gkm ∂ x j ∂ x j
We next examine the second integral in (18.6), viz., ∞ ∂ ∂ui Gkm d3 x . I = −Ci jkl ∂xj −∞ ∂ xl
(18.7)
First note that the stress ﬁeld of the dislocation is calculated from the linear elastic constitutive relation as σkl (x ) = Ci jkl
∂ui (x ) , ∂ x j
(18.8)
because of the inherent symmetry in elastic moduli C. Noting (18.5) again, along with the fact that σkl,l = 0 by equilibrium, the integral I may be rewritten as ∞ ∂ 3 Gkmσkl (x ) dS , (18.9) I= (Gkmσkl ) d x = S∞ −∞ ∂ xl where S∞ is a bounding surface that retreats to inﬁnity in the unbounded medium. But the dislocation is actually a loop, as illustrated in Fig. 18.1, and thus possesses both positive a negative segments, i.e., segments for which t · b > 0 and t · b < 0. At a distance, then, the elastic ﬁelds must fall off at least as fast as 1/r 2 , where r is the radial distance
18.1. Dislocation Character and Geometry
301
n
S+
Figure 18.2. Cross section of the cut surface.
n+
S
from the centroid of the loop. This is shown via speciﬁc example below. In fact, the fall off of the ﬁeld is more like 1/r 3 , as will be veriﬁed. Moreover, the Green’s function G falls off as 1/r . Thus the integrand of the second integral of (18.9) falls off at least as fast as 1/r 3 , or even as fast as 1/r 4 . Thus I → 0. The result for u is then ∞ ∂ ∂ 3 (18.10) um(x) = Ci jkl [Gkmui (x )] d x , −∞ ∂ xl ∂ x j or, for the distortions, ∞ ∂um(x) ∂2 ∂ = um,r (x) = Ci jkl [Gkmui (x )] d3 x ∂ xr ∂ x ∂ x ∂ x j l r −∞ ∞ ∂2 ∂ = Ci jkl [Gkmui (x )] d3 x . ∂ xl ∂ xr −∞ ∂ x j An application of the divergence theorem yields ∂2 um,r (x) = Ci jkl Gkmui (x )n j dS , S ∂ xl ∂ xr
(18.11)
(18.12)
where S = Scut + S∞ . Since Gkm,lr ∼ 1/r 3 and, as it happens, u also falls off with distance, the integral over S∞ vanishes. What remains is the integral over Scut . But across Scut the displacement jump is u− − u+ = b, on account of relation (18.1). Also, the outward pointing − , n− , points in the positive normal to the inﬁnite medium is such that the unit normal to Scut direction as illustrated in Fig. 18.2. Thus we take n = n− as the common unit normal to Scut , and write um,r (x) = Ci jkl Gkm,lr (x − x )bi n j dS . (18.13) Scut
This is known as the Volterra’s integral. The surface integral may be converted to an integral over the bounding line C of the dislocation using Stoke’s theorem in the form l jkϕr,kn j dS = ϕr tl ds, (18.14) C
Scut
where t is the running unit tangent vector to C, and ds is an element of arc length. The integral in (18.13) may be rephrased as Gkm,lr (x − x )bi n j dS um,r (x) = Ci jkl Scut
= Scut
ψ mr j n j dS .
(18.15)
302
18. Dislocations in Anisotropic Media
Letting mr ϕ mr j = nj p Xn ψ p ,
Xn = xn − xn ,
(18.16)
it follows that mr mr ϕ mr j,k = nj p Xn,kψ p + nj p Xn ψ p,k mr = kj p ψ pmr + nj p Xn ψ p,k ,
(18.17)
and mr mr jks ϕ mr j,kns = jks kj p ψ p ns + jks nj p Xn ψ p,kns mr − 2ψsmr ns − ψ p,k Xkn p .
Since ψ pmr is homogeneous of degree −3, we have mr Xi ψ pmr ,i = 0, Xkψ p,k = −3ψ pmr .
(18.18)
(18.19)
Then, mr jks ϕ mr j,kns = ψ p n p ,
and
Scut
jks ϕ mr j,kns dS =
Scut
(18.20)
jks nj p Xn ψ pmr ,k ns dS
=− Consequently,
um,r (x) = −
C
C
(18.21) nj p Xn ψ pmr t j
ds .
nj p (xn − xn )t j bi Ci psq Gmq,sr ds.
(18.22)
Note that this conversion demonstrates an important fact that dislocations are characterized by the line as described by t and their Burgers vector b; the cut surface used to create them then becomes arbitrary, as expected.
18.2 Dislocations in Isotropic Media In this section expressions are derived for the stress ﬁelds of inﬁnitely long and straight dislocations in isotropic elastic media. As such the ﬁelds correspond to either states of antiplane strain or plane strain. 18.2.1 Inﬁnitely Long Screw Dislocations The dislocation line is taken to be t = e3 , i.e., along the unit base vector of the x3 axis. The Burgers vector is taken such that bs · t = +bs ; the dislocation is accordingly said to be a righthanded screw dislocation. In other words, bs t. The jump condition expressed in (18.1) is met with u3 =
bs x2 bs θ= tan−1 . 2π 2π x1
(18.23)
18.2. Dislocations in Isotropic Media
303
This displacement ﬁeld is sufﬁcient to satisfy the equations of equilibrium. Indeed, σ13 = G∂u3 /∂ x1 and σ23 = G∂u3 /∂ x2 , the single equilibrium equation reads ∂σ13 ∂σ23 + = G∇ 2 u3 = 0, ∂ x1 ∂ x2
(18.24)
which of course is satisﬁed by the harmonic function, u3 ∼ θ. The stresses are, therefore, σ13 (x1 , x2 ) = −
x2 Gbs , 2 2π x1 + x22
σ23 (x1 , x2 ) =
x1 Gbs . 2 2π x1 + x22
(18.25)
It is seen that the stress ﬁelds fall off as 1/r from an isolated inﬁnitely long straight segment, but for two parallel segments that are part of the same loop, the ﬁelds fall off as 1/r 2 . Indeed, consider the two screw dislocation segments shown earlier in the ﬁgure. Let them be separated by a distance . The Burgers vector is the same for the two segments, but their unit tangents are antiparallel. Thus the stress ﬁelds are of opposite sign. Consider, for example, the stresses on the plane x2 = 0. Then, Gbs 1 1 Gbs σ23 ∼ − − . (18.26) ∼− 2π x1 x1 + 2π x12 18.2.2 Inﬁnitely Long Edge Dislocations The edge dislocation is characterized by the property that be = be e1 , whereas t = e3 . The corresponding displacement ﬁeld is u1 (x1 , x2 ) =
x1 x2 be be tan−1 (x2 /x1 ) + , 2π 2π (1 − ν) x12 + x22
x12 − x22 be 1 − 2ν ln r − u2 (x1 , x2 ) = − , 2π 2(1 − ν) 4(1 − ν)(x12 + x22 )
(18.27)
whereas the stresses are σ11 = − σ22 = σ12
x2 (3x12 + x22 ) Gbe , 2π (1 − ν) (x12 + x22 )2
x2 (x12 − x22 ) Gbe , 2π(1 − ν) (x12 + x22 )2
x1 (x12 − x22 ) Gbe = , 2π(1 − ν) (x12 + x22 )2
σ33 = −
(18.28)
x2 Gbe ν = ν(σ11 + σ22 ) . π(1 − ν) x12 + x22
18.2.3 Inﬁnitely Long Mixed Segments The elastic ﬁeld of an inﬁnitely long and straight dislocation of mixed character is simply obtained by the linear superposition of the solutions obtained above. Here, however, we consider an inﬁnitely long curved dislocation line lying in the plane x3 = 0 with a Burgers vector as illustrated in Fig. 18.3. Our perspective is that the Burgers vector is given and ﬁxed, but the character of the line varies because of varying orientation of the line tangent t.
304
18. Dislocations in Anisotropic Media
x2 λ
t b φ
θ
Figure 18.3. Inﬁnitely long curved dislocation with a Burgers vector b.
x1
Thus as t varies, i.e., as θ or (θ − φ) varies, the edge vs. screw dislocation character varies. Now let the Burgres vector be b, so that b = b cos φe1 + b sin φe2 , t = cos θe1 + sin θe2 .
(18.29)
This means that bs = b cos(θ − φ) = bt , be = −b sin(θ − φ) = bλ ,
(18.30)
where bs and be are the screw and edge components of b respectively. We now use the solutions obtained above to construct the inplane ﬁeld of this mixed dislocation. Let d be the normal distance from the line as reckoned by “looking right” while sighting down t. Then in the plane x3 = 0, we ﬁnd Gb cos(θ − φ), 2π d Gb sin(θ − φ), =− 2π d
σt3 = σλ3
(18.31)
where t and λ are used as indices corresponding to rotated axes aligned with the dislocation line and orthogonal to it (Fig. 18.3). With respect to the ﬁxed coordinates (x1 , x2 ), we have σ13 = σt3 cos θ − σλ3 sin θ =
Gb Gb cos(θ − φ) cos θ + sin(θ − φ) sin θ, 2πd 2π (1 − ν)d
(18.32)
and σ23 = σt3 sin θ + σλ3 cos θ =
Gb Gb cos(θ − φ) sin θ − sin(θ − φ) cos θ. 2πd 2π (1 − ν)d
(18.33)
We note for later use that the inplane stresses can be expressed as σαβ =
1 1 (αβ (θ; φ) = (αβ (θ), d d
(18.34)
18.3. Planar Geometric Theorem
305
where in the second rendering of this relation the dependence on φ has been omitted on account of the perspective of ﬁxed φ, i.e., ﬁxed b. In fact, 1 cos(θ − φ) cos θ + sin(θ − φ) sin θ , 1−ν Gb 1 sin(θ − φ) cos θ . cos(θ − φ) sin θ − (23 (θ) = 2π 1−ν Gb (13 (θ) = 2π
(18.35)
18.3 Planar Geometric Theorem Here we consider the case of a dislocation loop lying entirely within a plane, and seek to construct its elastic ﬁeld in that plane. Let the plane be deﬁned as x3 = 0. The dislocation line is C and its cut surface can be taken to lie entirely in the plane, without loss of generality. Then, Gkm,lr (x − x )bi n j dS , (18.36) um,r (x) = Ci jkl Scut
as found earlier. The ﬁeld point of interest lies in the plane x3 = 0, and thus has coordinates (x1 , x2 ). Let X = x1 − x1 ,
Y = x2 − x2 .
(18.37)
If we introduce a unit vector, T, deﬁned to be parallel to (x − x ) then x − x = sT, where s = x − x . Note that s is algebraically signed. Recall that the Green’s function has symmetry, such that Gkm(sT) =
sgn(s) Gkm(T) s
(18.38)
sgn(s) Gkm,lr (T), s3
(18.39)
and Gkm,lr (sT) =
i.e., both G and its second derivative are symmetric with respect to the sense of T. Thus, if θ is the angle that T makes with a datum drawn in the plane, we may write Gkm(x − x ) =
1 1 Gkm(θ) = Gkm(θ + π), R R
(18.40)
where R = x − x  = s,
T = T(θ) = −T(θ + π ).
(18.41)
Similarly, Gkm,lr (x − x ) =
1 1 Gkm,lr (θ) = 3 Gkm,lr (θ + π ). 3 R R
(18.42)
306
18. Dislocations in Anisotropic Media
But θ is a function of X/R and Y/R, and so the above may be expressed as a power series of the form m n X Y 1 ¯ mn , Gkm = R n,m R R (18.43) m n X Y 1 Gkm,lr = 3 mn = I. R n,m R R Call the second of (18.43), as noted, I, and write 1 1 )(θ) = 3 )(θ + π ), R3 R m n X Y mn . )(θ) = R R n,m I=
(18.44)
To proceed, examine the expression I=
∂ ∂ (XI) + (YI). ∂X ∂Y
(18.45)
Since R2 = X2 + Y2 , we have ∂R X = , ∂X R
∂R Y = , ∂Y R
3X 3Y ∂(1/R3 ) ∂(1/R3 ) =− 5 , =− 5 , ∂X R ∂Y R m+n (m + n)X (m + n)Y ∂(1/R ) ∂(1/Rm+n ) = − m+n+2 , = − m+n+2 . ∂X R ∂Y R Thus, (18.45) becomes
m n X2 X Y mn R5 m,n R R m n m−1 n X Y X Y Y2 X −3 5 mn + 3 mmn m R m,n R R R m,n R R X m Yn−1 X (m + n)X m Y n Y − 3 + 3 nmn mn m+n+2 X R m,n R Rn R m,n r R X m (m + n)Y Y − 3 mn m+n+2 Yn = −I. R m,n r R
I =I + I −3
Therefore, −I(X, Y) =
∂ ∂ (XI) + (YI). ∂X ∂Y
(18.46)
Now return to (18.36) and incorporate the terms involving bi and Ci jkl , as they are constants. Further, the sums over repeated subscripts are implied (and implemented), so that (18.36) is expressed as ∂ ∂ (XImr ) + (YImr ) dX dY. (18.47) um,r = − ∂Y Scut ∂ X
18.3. Planar Geometric Theorem x
307
2 t x
C α
P ds
x'
Figure 18.4. Geometry of a planar loop.
R θ x1
Next, recall Stokes theorem in the form ∂Q ∂P − (P dX + Q dY) = dX dY, ∂ X ∂Y C S
(18.48)
where C is the line that bounds the open surface S. Let Q = XImr and P = −YImr to convert the surface integral into one along the bounding line C. Also note that the loop C is characterized by the parametric equations for x1 (s) and x2 (s). Consider the typical point such as P. At this point, dx1 /ds = cos α and dx2 /ds = sin α, where ds is an element of arc length and, as before, t is the variable unit tangent to C (see Fig. 18.4). Thus, taking the ﬁeld points x1 , x2 to be ﬁxed in the integration, we have that X = dX/ds = −dx1 /ds, with a similar consideration for Y = dY/ds. Consequently, the integral in (18.47) becomes um,r (x) = (X Y − Y X)Imr (X, Y) ds. (18.49) C
With reference to the ﬁgure, we can write X = − cos α,
Y = − sin α,
X = R cos θ,
Y = R sin θ.
(18.50)
Using these it follows that (X Y − Y X)ds = R(− cos α sin θ + sin α cos θ)ds = −R sin(θ − α)ds, and thus
um,r (x) = −
C
)mr (θ) sin(θ − α) ds. R2
(18.51)
Recall that )(θ) = )(θ + π), θ, α, and R are all functions of the parameter s and therefore dependent on the size and shape of the dislocation loop. Also note that the formula expressed in (18.51) applies to any loop. We may then reinterpret (18.51) as an integral equation for the as yet unknown function, )(θ), in terms of the solution, um,r (x). We now want to choose a somewhat convenient choice for C; we choose C to be an inﬁnitely long and straight dislocation as depicted in Fig. 18.5. Using the geometry of the ﬁgure, we observe the following identities x1 = s cos α,
x2 = s sin α,
s = −d cot(θ − α), ds =
R = d/ sin(θ − α),
d sin2 (θ − α)
dθ .
(18.52)
308
18. Dislocations in Anisotropic Media x' 2
x
t d
R
α
θ θ− α
Figure 18.5. Coordinates for an inﬁnitely long, straight dislocation.
x' 1
x'
With these, (18.51) becomes 1 um,r (d, α) = − d
θ=α+π
θ=α
)(θ) sin(θ − α) dθ.
Derivatives wr t to α leads to a convenient interpretation, viz., α+π 1 ∂um,r = )(θ) cos(θ − α) dθ, ∂α d α and ∂ 2 um,r 1 1 = − [)(α) + )(α + π)] + 2 ∂α d d
α+π α
)(θ) sin(θ − α) dθ.
(18.53)
(18.54)
(18.55)
The addition of (18.53) and (18.55) yields the desired result, um,r (d, α) +
∂ 2 um,r (d, α) 1 = − [)(α) + )(α + π )] , ∂α 2 d
(18.56)
∂ 2 um,r (d, α) um,r (d, α) + . ∂α 2
(18.57)
and thus )(α) = −
d 2
We have already shown that the ﬁeld of an inﬁnitely long and straight dislocation can be cast as um,r =
(mr (ζ ) , d
(18.58)
where ζ would be an angle representing the dislocation’s orientation in the plane (assuming its Burgers vector is ﬁxed). Thus, the expression for the ﬁeld at an arbitrary point becomes (mr (θ) + ∂ 2 (mr (θ)/∂θ 2 1 um,r (x) = sin(θ − α) ds. (18.59) 2 C R2
18.4 Applications of the Planar Geometric Theorem Considerable simpliﬁcation can be achieved by approximating dislocation loops as being polygonal, i.e., as having faceted sides such as sketched in Fig. 18.6. The geometry sketched in the ﬁgure will be used to reduce the integral given in (18.59) above. Figure 18.7 indicates a typical segment of the loop. As we integrate about the loop, R = x − x  =
d , sin(θ − α)
s = −d cot(θ − α),
(18.60)
18.4. Applications of Planar Geometric Theorem
309
α n
α+ n
Rm
θn
Figure 18.6. Geometry of a loop vertex.
so that ds d x − x  = . = dθ sin(θ − α) sin2 (θ − α)
(18.61)
Thus, upon changing the integration variable from s to θ in (18.59), we obtain um,r (x) = 1/2
C
(mr (θ) + ∂ 2 (mr (θ)/∂θ 2 sin(θ − α) dθ. d
(18.62)
Integration by parts from θ1 to θ2 , as indicated in Fig. 18.7 for the typical segment, yields um,r (x) =
1 [−(mr (θ) cos(θ − α) + ∂(mr /∂θ sin(θ − α)]θθ21 2d θ2 − [∂(mr /∂θ cos(θ − α) + ∂(mr /∂θ cos(θ − α)] dθ.
(18.63)
1 [−(mr (θ) cos(θ − α) + ∂(mr /∂θ sin(θ − α)]θθ21 . 2d
(18.64)
θ1
Thus, um,r (x) =
Clearly by summing over all such segments, the ﬁeld of the entire loop may be constructed. Recalling the ﬁrst of (18.60), the integral in (18.63) may be recast as (mr (θ) + ∂ 2 (mr (θ)/∂θ 2 1 dθ. (18.65) um,r (x) = 2 C x − x  Examine the second term in the integrand, viz., C
∂(mr (θ)/∂θ 1 ∂ 2 (mr (θ)/∂θ 2 ∂(mr (θ)/∂θ cot(θ − α) dθ = dθ, − x − x  x − x  x − x  C 1
d
R
Figure 18.7. Dislocation segment.
θ1
θ2
α Datum
(18.66)
310
18. Dislocations in Anisotropic Media
where the limits of evaluation on the ﬁrst integral indicate evaluation from a point labeled 1 to itself, and where it was noted that dx − x  = −x − x  cot(θ − α). dθ
(18.67)
The second integral on the rhs of (18.66) is ∂(mr (θ)/∂θ cot(θ − α) cot(θ − α) 1 − dθ = − (mr (θ) x − x  x − x  1 C (mr (θ) cot2 (θ − α) dθ + x − x  C (mr (θ) − csc2 (θ − α) (1 − dα/dθ) dθ.  x − x C By recognizing that cot2 (θ − α) − csc2 (θ − α) = −1, we have 1 2
C
1 ∂ 2 (mr (θ)/∂θ 2 dθ = − x − x  2
C
1 (mr (θ) dθ + x − x  2
(mr (θ)dα/dθ C
x − x  sin2 (θ − α)
dθ.
When this result is incorporated into (18.65), the remarkably simple result follows, viz., (mr (θ)dα/dθ 1 dθ um,r (x) = 2 C x − x  sin2 (θ − α) (18.68) (mr (θ) 1 dα. = 2 C x − x  sin2 (θ − α) Note that dα = 0 along each segment until a corner is reached, at which point α undergoes a “jump” from, say α − to α + (Fig. 18.6). But during such jumps, θ and x − x  remain ﬁxed. Thus, noting that dα = cot(θ − α), sin2 (θ − α) it is found that each corner, say the nth corner, contributes a term such as χ=
1 (mr (θn ) α+ [cot(θn − α)]αnn− . 2 x − x n
(18.69)
Therefore, for the entire loop, we have um,r (x) =
N (mr (θn ) 1 α+ [cot(θn − α)]αnn− . 2 n=1 x − x n
(18.70)
There is a modiﬁcation if the ﬁeld point x happens to be colinear with one side, because along such a side θ = 0, and θs+1 (mr (θ) + ∂ 2 (mr /∂θ 2 dθ = 0. (18.71) x − x  θs
18.4. Applications of Planar Geometric Theorem x
l2 (2)
λ
α(2) = α
l1
(1) α(1)=0
311
θ
Figure 18.8. An angular dislocation.
Datum
It is assumed here that the side in question connects the s and s + 1 corner. In this case (18.70) would have to be modiﬁed so that the segment between corners s and s + 1 does not contribute. The result of removing this is N (mr (θn ) 1 α+ [cot(θn − α)]αnn− 2 n=1 x − x n
um,r (x) =
n =s,s+1
−
+ ) (mr (θs+1 ) cot(θs+1 − αs+1 (mr (θs ) − cot(θ − α ) − s s x − x s x − x s+1
+
∂(mr (θs )/∂θ ∂(mr (θs+1 )/∂θ − . x − x s x − x s+1
(18.72)
We can recast (18.60) or (18.65) using the fact that dα = κds, When this is done, we obtain 1 um,r (x) = 2
ds = dθx − x  csc(θ − α).
(18.73)
C
κ(mr (θ) csc3 (θ − α) dθ.
(18.74)
18.4.1 Angular Dislocations As a further application of the previous results, consider the angular dislocation shown in Fig. 18.8. Using (18.64), it is found that, for the segment labeled 1, we have θ
1 (1) um,r = (mr (θ) + ∂ 2 (mr (θ)/∂θ 2 sin θ dθ 21 0 (18.75) 1 = [−(mr (θ) cot θ + (mr (0) csc θ + ∂(mr (θ)/∂θ ] . 2λ Similarly, for the segment labeled 2 it is found that α+π
1 (mr (θ) + ∂ 2 (mr (θ)/∂θ 2 sin(θ − α) dθ (18.76) u(2) = m,r 22 θ 1 [(mr (α) csc(θ − α) + (mr (θ) cot(θ − α) − ∂(mr (θ)/∂θ ] . 2λ When added, they yield for the full ﬁeld =−
um,r (x) =
1 [(mr (α) csc(θ − α) + (mr (0) csc(θ)] 2λ sin α 1 + (mr (θ) , 2λ sin(θ − α) sin θ
where we have used the fact that (mr (α) = (mr (α + π ).
(18.77)
312
18. Dislocations in Anisotropic Media
18.5 A 3D Geometrical Theorem Consider again the line integral yielding the distortion ﬁeld for a dislocation loop, viz., um,r (x; C) = − bi nj p t j (xn − xn )C pisk Gsm,kr (x − x ) ds. (18.78) C
m Upon using the symmetry inherent in the components C pisk, let P pi = C pisk Gsm,k be the pi component of stress at x, caused by a unit point force acting at x in the m direction. m m and P pi,r will possess all the symmetry and scaling properties of the Green’s Note that P pi function G. The integral above becomes m (x − x ) ds. (18.79) um,r (x, C) = − bi nj p t j (xn − xn )P pi,r C
Let C be an inﬁnitely long and straight dislocation line. Then, xn = tn s,
x = ts,
nj p xn t j = nj p tn t j s = 0, so that
um,r (x, C∞ ) = −
∞
−∞
m bi nj p xn t j P pi,r (x − st) ds.
(18.80)
(18.81)
m , we have But, because of the scaling and symmetry properties of P pi,r m P pi,r (x − st) =
sgn(s) m P pi,r (x/s − t). s3
(18.82)
Deﬁne η = 1/s, dη = −1/s 2 ds, and observe that ∞ m um,r (x, C∞ ) = − bi nj p xn t j (1/s 3 )P pi,r (x/s − t) ds 0+
+ =
0−
−∞ 0+
m bi nj p xn t j ηP pi,r (ηx − t) dη
∞
−
m bi nj p xn t j (1/s 3 )P pi,r (x/s − t) ds
−∞ 0−
m bi nj p xn t j ηP pi,r (ηx − t) dη.
Then, upon identifying this inﬁnitely long and straight dislocation line by its constant tangent, t, we can write ∞ ∞ m bi nj p xn t j ηP pi,r (ηx − t) dη um,r (x; t) = − + =
0+
0− −∞
∞
−∞
m bi nj p xn t j ηP pi,r (ηx − t) dη
m bi nj p xn t j η sgn(η)P pi,r (ηx − t) dη.
(18.83)
18.5. 3D Geometrical Theorem
313
Operate on this equation with (xα ∂/∂tα )2 , while noting that xα
∂ ∂ m P m (ηx − t) = − P pi,r (ηx − t). ∂tα pi,r ∂η
It is found that xβ xα
∂2 u∞ = 2 ∂tα ∂tβ m,r
∞
−∞
−
bi nj p xn x j η sgn(η)
∞ −∞
bi nj p xn t j η sgn(η)
m ∂P pi,r
∂η
(18.84)
dη
m ∂ 2 P pi,r
∂η2
(18.85) dη.
The ﬁrst integral is clearly zero by virtue of nj p xn x j = 0. The second may be integrated by parts, using the result m ∞ ∂P pi,r η sgn(η) = 0. ∂η −∞ The ﬁrst integration then yields ∞ m d sgn(η) ∂P pi,r ∂2 ∞ dη. xβ xα u = bi nj p xn t j sgn(η) + η ∂tα ∂tβ m,r dη ∂η −∞ But, d sgn(η) = 2δ(η), dη and the second term in the square bracket above makes zero contribution to the integral. Integrating by parts again, and noting that
m ∞ sgn(η)P pi,r = 0, −∞ now gives xβ xα
∂2 u∞ = −2 ∂tα ∂tβ m,r
∞
−∞
m bi nj p xn t j δ(η)P pi,r (ηx − t) dη
m (−t) = −2bi nj p xn t j P pi,r
(18.86)
m (t). = −2bi nj p xn t j P pi,r
Finally, let t ← x − x
and
x ← t,
(18.87)
where x is a ﬁxed point. Then, the integrand of (18.79) becomes m bi nj p tn (x j − x j )P pi,r (x − x ) = −tα
and, consequently,
um,r (x; C) = −
C
tα
∂ ∂ ∞ tβ u (t; x − x ), ∂ xα ∂ xβ m,r
∂ ∂ ∞ tβ u (t; x − x ) ds. ∂ xα ∂ xβ m,r
(18.88)
(18.89)
314
18. Dislocations in Anisotropic Media
18.6 Suggested Reading Indenbom, V. L., and J. Lothe, J. (1992), Elastic Strain Fields and Dislocation Mobility, NorthHolland, Amsterdam. Hirth, J. P., and Lothe, J. (1982), Theory of Dislocations, 2nd ed., Wiley, New York. Nabarro, F. R. N., ed. (1979), Dislocations in Solids, NorthHolland, Amsterdam. Nabarro, F. R. N. (1987), Theory of Crystal Dislocations, Dover, New York. Mura, T. (1987), Micromechanics of Defects in Solids, Martinus Nijhoff, Dordrecht, The Netherlands. Teodosiu, C. (1982), Elastic Models of Crystal Defects, SpringerVerlag, Berlin. Ting, T. C. T. (1996), Anisotropic Elasticity, Oxford University Press, New York.
19 Cracks in Anisotropic Media
An elementary development of crack tip mechanics was given in Chapter 17. Here we provide a more advanced construction of the elastic ﬁelds at crack tips and extract from our construction some particularly important quantities that enter prominently into the physics of crack growth and crack interaction with other defects that exist within the elastic medium surrounding the crack. Of primary importance is the theoretical determination of the total mechanical energy of a cracked body and the negative of its derivative with respect to crack extension, i.e., the energy release rate, G, or the generalized force on the crack tip vis`avis the concept further developed in subsequent chapters. The elastic medium is taken to be arbitrarily anisotropic. The dislocation solutions and methods developed for dealing with the elastic ﬁelds of dislocations are used to construct the crack solutions.
19.1 Dislocation Mechanics: Reviewed In Chapter 21 we show that the energy of an inﬁnitely long and straight dislocation can be written as E = Kmg bmbg ln(R/r0 ),
(19.1)
where R and r0 were outer and inner cutoff radii respectively. The components of the dislocation’s Burgers vector are bi , and Kmg are the components of a positive deﬁnite secondrank tensor called the energy factor. K depends only on the direction of the dislocation line within the elastic medium and on the elastic moduli tensor C, i.e., its components Ci jkl . For an isotropic medium K is diagonal, when phrased with respect to the basis {e1 , e2 , e3 } on the coordinate frame with axes (x1 , x2 , x3 ), and when the dislocation line is parallel to x3 axis, t e3 . In that case, we obtained K11 = K22 = G/4π(1 − ν),
K33 = G/4π.
(19.2)
We have already shown in Chapter 17 how a slit like crack in an elastic medium can be represented by a continuous distribution of dislocations distributed with an appropriate density along the crack line. This was done, speciﬁcally for the case of a Mode I crack. As noted in that development, the calculation of the crack tip ﬁeld involves ﬁrst solving a singular integral equation for the dislocation distribution and then using linear superposition to construct the ﬁeld. It will be shown here that the crack extension force can 315
316 X1
19. Cracks in Anisotropic Media
x2
X3
X2
x1
Figure 19.1. Slitlike crack and crystal frame.
2c
also be calculated knowing the distribution of dislocations in the crack, or more particularly knowing the displacement discontinuity across the crack face that is caused by the distribution of dislocations. In fact, it is shown that the crack extension force, G, can be calculated knowing only the inverse of the energy factor matrix, K−1 , for a single straight dislocation. Two types of cracks are considered, viz., freely slipping cracks and cracks whose faces are not traction free but are subject to applied traction. Furthermore, the following universal result is derived: when the displacement discontinuity at the tips of the crack vanishes, the traction and stress concentration on the plane of the crack are independent of the elastic anisotropy and are, accordingly, the same as predicted by the isotropic theory. The same is true of the stress intensity factors. The same is not the case for the angular dependence of the ﬁelds around the crack or of the crack extension force, G.
19.2 Freely Slipping Crack Consider a slit like crack lying on the plane x2 = 0, as shown in Fig. 19.1. The crack lies in the region, x1  ≤ c, x2 = 0, −∞ < x3 < ∞ in an inﬁnite elastic medium. For later reference, let X = {X1 , X2 , X3 } be a coordinate frame in which the elastic moduli tensor, C, and its components, Ci jkl , are displayed in their simplest form, e.g., for a cubic crystalline medium these would be the cube axes. As r 2 = x12 + x22 → ∞, the state of stress is uniform and thus lim σi j = σiAj .
r →∞
(19.3)
We are assuming small strains so that, using the convention that commas denote differentiation, the strains are deﬁned by 2ei j = ui, j + u j,i .
(19.4)
In the absence of body forces, equilibrium requires that σi j, j = 0.
(19.5)
Since the crack is freely slipping there are no tractions on the crack faces, i.e., σi j n j = 0,
on
x2 = 0, x1  ≤ c,
(19.6)
where n is the unit normal to the crack plane. The convention is that on the upper crack surface (x2 = 0+ ), n1 , n3 = 0, n2 = −1. On the lower crack surface (x2 = 0− ), n1 , n3 = 0, n2 = 1. This means that the freely slipping boundary conditions become σ12 = σ22 = σ32 = 0,
for x1  ≤ c, x2 = 0, x3  ≤ ∞.
(19.7)
19.2. Freely Slipping Crack b x1
1
S b2
S x3
317
type 1 type 2 edge edge
b 3 x2
Figure 19.2. Dislocation types distributed over the crack.
type 3 screw
This boundary value problem is solved using the method of continuously distributed dislocations as introduced earlier. Let the solution be written in the form ui = uiA + uiD ,
ei j = eiAj + eiDj ,
σi j = σiAj + σiDj ,
(19.8)
where the D ﬁelds are constructed from the linear superposition of those of the continuously distributed dislocations of three types; these are indicated in the Fig. 19.2. The A ﬁelds refer to the uniformly stressed uncracked solid, so that, excluding arbitrary rigid body translations, uiA = eiAj x j ,
A eiAj = Si jmn σmn ,
(19.9)
where the Si jmn are the components of the elastic compliance tensor (the inverse of the elastic stiffness tensor). The A ﬁelds are everywhere continuous. We note that σiDj → 0 as r → 0,
(19.10)
because the stress ﬁelds of individual dislocations vanish as r 2 → 0. Since the A and D ﬁelds are each admissible solutions to the equilibrium and compatibility equations, we can complete the solution by choosing σiDj so that (19.7) is satisﬁed, i.e., D A σ12 = −σ12 = −T1A ,
on
x1  < c, x2 = 0,
D A σ22 = −σ22 = −T2A ,
on
x1  < c, x2 = 0,
D A σ32 = −σ32 = −T3A ,
on
x1  < c, x2 = 0.
(19.11)
The D ﬁeld is constructed by an integral superposition of three types of straight dislocations, the dislocations being parallel to the x3 axis and lying in the region x1  < c, x2 = 0. If we denote by bs f (s) (t)dt (no sum on s) the amount of Burger’s vector in the xs direction, distributed between t and t + dt, then σiDj (x1 , x2 )
=
3 s=1
c −c
(s)
f (s) (t)σi j (x1 , x2 ; t, 0) dt,
(19.12)
(s)
where σi j (x1 , x2 ; t, 0) is the stress ﬁeld at (x1 , x2 ) due to a single straight dislocation of type s (s = 1, 2, 3), piercing the planes x3 = const. at the point (t, 0). Thus equations (19.11) may be written as 3 s=1
c
−c
(s)
f (s) (t)σi2 (x1 , 0; t, 0) dt = −TiA ,
for x1  < c, i = 1, 2, 3.
(19.13)
318
19. Cracks in Anisotropic Media
In an inﬁnite elastic medium, (s)
(s)
σi j (x1 , 0; t, 0) = σi j (x1 − t),
(19.14) (s)
and, from what has been developed in Chapters 17 and 18, σi j (x1 − t) ∼ (x1 − t)−1 . Now consider a single dislocation parallel to the x3 axis and piercing the planes x3 = const. at (t, 0). Let its Burger’s vector have components b1 , b2 , b3 . The energy per unit length can be written as t+R (x1 − t)−1 dx1 . (19.15) E = Kmq bmbq ln(R/r0 ) = Kmq bmbq t+r0
But the formula 3 1 E= 2 s=1
t+R
t+r0
(s)
σm2 (x1 − t)bm dx1
(19.16)
is also valid. If a dislocation is of type 1 (i.e., s = 1, b2 = b3 = 0), a comparison of (19.15) and (19.16) yields (1)
σ12 (x1 − t) = 2K11 b1 /(x1 − t).
(19.17)
(3)
(19.18)
Similar reasoning gives (2)
σ22 (x1 − t) = 2K22 b2 /(x1 − t),
σ32 (x1 − t) = 2K33 b3 /(x1 − t).
If we consider the case s = 1, 2 and b3 = 0, and note that (1)
(2)
σ12 (x1 − t)b2 = σ12 (x1 − t)b1 ,
(19.19)
(because one can calculate the interaction energy between a dislocation of type 1 and type 2 by looking at the interaction of one on the other or vice versa), a comparison of (19.15) and (19.16) again shows that (1)
σ22 (x1 − t) = 2K21 b1 /(x1 − t),
(2)
σ12 (x1 − t) = 2K12 b2 /(x1 − t).
(19.20)
Note that (19.19) essentially follows from Betti’s reciprocal theorem. In general, (s)
σi2 (x1 − t) = 2Kis bs /(x1 − t),
(no sum on s).
(19.21)
If we use (19.21) to deﬁne Fs (t) = bs f (s) (t),
(no sum on s),
(19.13) may be concisely expressed as c 2Ki j (x1 − t)−1 F j (t) dt = −TiA , −c
or
c
1 A (x1 − t)−1 F j (t) dt = − K−1 ji Ti , 2 −c
(19.22)
for x1  < c,
(19.23)
for x1  < c,
(19.24)
with the sum over the repeated index. The integrals in question, as will be the case with all singular integrals appearing in this development, are deﬁned by their Cauchy principal values.
19.3. Crack Extension Force
319
We recall that the components of the inverse of K ji are given by −1 K−1 ji = Ki j = jmn ir s Kmr Kns /2αβγ K1α K2β K3λ ,
(19.25)
−1 K−1 ji Kis = K ji Kis = δ js .
(19.26)
so that
Since we expect stress singularities at the crack tip, we require F j (±c) to be unbounded with a weak singularity. Moreover, if we demand that there be no relative displacement of the crack faces at x1 = ±c, then c F j (t) dt = 0. (19.27) −c
It is noteworthy that implicit in this analysis is the convention that the displacement discontinuity across the crack faces at (x1 , 0) is given by x1 x2 =0− D u j (x1 ) = u j (x1 , x2 )x2 =0+ = F j (t) dt. (19.28) −c
The solution of (19.24) is A F j (t) = K−1 ji Ti
2π(c2
t . − t 2 )1/2
(19.29)
A rather important result can be extracted from the above when we consider the traction σi2 on the plane of the crack ( x1  > c, x2 = 0). We have 3 c Fs (t) Kis bs dt, x1  > c. σi2 x2 =0 = σi2A + 2 (19.30) bs (x1 − t) s=1 −c Since TiA = σi2A ,
(19.31)
using (19.26) and (19.29), yields
t dt 1 c σi2 x2 =0 = σi2A 1 + π −c (c2 − t 2 )1/2 (x1 − t) =
σi2A
x1  , 2 (x1 − c2 )1/2
(19.32)
x1  > c.
As x1 → ±c, (19.32) reduces to the familiar isotropic expression for stress concentration, viz., σi2 ≈ σi2A (c/2r )1/2 , where r = x1  − c. Hence, the traction and stress concentrations on the plane of the crack are independent of the elastic constants and the anisotropy of the medium, i.e., they are identical with those for a crack in an isotropic medium loaded by stresses σiAj at inﬁnity. It is shown below that this is also true for the case of a crack that is arbitrarily but symmetrically loaded on its faces by selfequilibrating stresses, provided that (19.27) is true.
19.3 Crack Extension Force The energy of deformation and crack extension force may now be easily calculated. The change in total mechanical energy per unit length in the x3 direction between the stressed
320
19. Cracks in Anisotropic Media
cracked solid and the uncracked solid stressed homogeneously by σi j = σiAj , is 1 c A D E = σ ui dx1 . 2 −c i2
(19.33)
Combining (19.28), (19.29), and (19.33), we obtain 1 A −1 E = − c2 σi2A σs2 Kis . 8 The crack extension force is deﬁned as
(19.34)
1 ∂(E) A −1 = cσi2A σs2 Kis . (19.35) ∂c 4 The appropriate Grifﬁth criterion for brittle fracture in the anisotropic medium is obtained by requiring that G be greater or equal to 4γ , where γ is the surface energy associated with the plane x2 = 0 (the crack is assumed to extend on both ends, so that 2 × 2γ = 4γ ). Thus, the applied stress state required to propagate the crack is determined from G=−
A −1 Kis ≥ 16γ /c. σi2A σs2
Using (19.2) allows a recovery of the isotropic Grifﬁth criterion, A 2
A 2 (1 − ν) (σ12 ) + (σ22 ) + (σ32 )2 ≥ 4Gγ /π c.
(19.36)
(19.37)
A method is presented below for calculating Kis , and hence Kis−1 , using the coordinate frame denoted earlier by X = {X1 , X2 , X3 }. If all quantities are referred to the X frame, then (19.35) becomes 1 A A c σ n j σsm nm Kis−1 , (19.38) 4 ij where nm are components of the unit normal to the crack surface in the X frame. As an example, imagine a cleavage crack lying in the (001) plane of a cubic crystal such as αFe, or an ionic crystal such as KCl or NaCl, which is stressed by far ﬁeld tension pA . The crack’s normal, then, lies in the x3 direction. The crack extension force would be given in this case by G=
G=
1 A 2 −1 ( p ) cK33 . 4
(19.39)
−1 with angle in the (001) plane of three cubic materials. Figure 19.3 shows the variation of K33 The effects of anisotropy appear to be modest and are appreciable only for Fe. In fact, us−1 = 0.103 × 10−10 cm3 /erg, which ing Voigt average isotropic elastic constants for αFe, K33 differs by between 10 and 20% of our anisotropic calculations (recall that 1 erg= 10−7 J).
19.4 Crack Faces Loaded by Tractions The extension of the results for a freely slipping crack to the case of a crack whose faces are loaded by tractions −Ri (x1 ) is readily done. The same analysis sufﬁces if we replace the boundary condition (19.7) by −Ri (x1 ), for x2 = 0+ , x1  < c, (19.40) σi j n j = Ri (x1 ), for x2 = 0− ,
19.4. Crack Faces Loaded by Tractions
321
0.94
1 (cm 3 erg x 10 10) K 33
0.92 KCl 0.90 0.63 0.62
NaCl
0.12
Fe
−1 Figure 19.3. Variation of K33 with angle within the (001) plane.
0.11 0 [100]
30
60 90 (Degrees) [010]
so that we assume that the traction on the upper and lower crack faces are equal in magnitude but opposite in direction. Clearly, the loading is symmetrical about x2 = 0 and thus selfequilibrating. For example, if the loading were internal pressure of magnitude P, then R1 = R3 = 0, R2 = −P. Hence the distribution function F j (t) must now satisfy c A
1 Ti − Ri (x1 ) , x1  < c. (x1 − t)−1 F j (t) dt = − Ki−1 (19.41) j 2 −c It is again required that (19.27) be satisﬁed when F j (±c) is unbounded. The integral equation may be easily solved once we specify Ri (x1 ). For our purposes it is sufﬁcient to note that 2F j (t) = K−1 ji Qi (t), where Qi (t) is independent of the anisotropy of the medium and satisﬁes c
(x1 − t)−1 Qi (t) dt = − TiA − Ri (x1 ) , x1  < c. −c
(19.42)
(19.43)
If F j (±c) is to be unbounded, then TiA t 1 Qi (t) = + 2 2 π(c2 − t 2 )1/2 π (c − t 2 )1/2
c −c
Ri (x1 )(c2 − x12 )1/2 dx1 . x1 − t
(19.44)
For cracks with no stress singularities at x1 = ±c, as in simple models of cracks relaxed by plastic deformation, F j (±c) must vanish, and c 1 2 2 1/2 (c2 − x12 )−1/2 (x1 − t)−1 R(x1 ) dx1 , (19.45) Qi (t) = 2 (c − t ) π −c provided that the subsidiary condition c (c2 − s 2 )−1/2 Ri (s) ds = π TiA −c
(19.46)
322
19. Cracks in Anisotropic Media
is satisﬁed. The traction σi2 acting on the plane of the crack (x1  > c, x2 = 0) is then given by (19.32) which, after using (19.26) and (19.42), reduces to c (x1 − t)−1 Qi (t) dt, x1  > c. (19.47) σi2 x2 =0 = σi2A + −c
Since Qi (t) depends only on the loading TiA − Ri (x1 ), the traction and also the stress concentrations, if any, on the plane of the crack are independent of the elastic anisotropy. Stress intensity factors for cracks with singular ﬁelds are computed in the next section. If (19.27) is not satisﬁed, there exists a net dislocation content in the crack, i.e., c F j (t) dt = Nj . (19.48) −c
In this event, we must add to F j (t), as given by (19.29) or (19.42) and (19.44), the term F j∗ (t) = Nj /π (c2 − t 2 )1/2 .
(19.49)
The traction on the crack plane is in this case no longer independent of the anisotropy because the distribution (19.49) induces an extra traction σi2∗ x2 =0 = 2Kis Ns (x12 − c2 )−1/2 sgn(x1 ),
x1  > c.
(19.50)
19.5 Stress Intensity Factors and Crack Extension Force The three stress intensity factors, called ki here, are most simply deﬁned by noting that if the stresses are singular at the crack tip, i.e., at x1 = c, then σi2  x1 → c, x2 =0 = ki /(2πr )1/2 + nonsingular terms,
(19.51)
where r = x1 − c, so that ki (c) = lim (2πr )1/2 σi2 x2 =0 , x1 → c
x1 > c.
(19.52)
When (19.27) is satisﬁed, the use of (19.44) and (19.47) yields c c 1 dt Ri (s)(c2 − s 2 )1/2 ds A 1/2 1/2 ki (c) = σi2 (π c) + lim (2πr ) . 2 2 2 1/2 x1 → c s−t −c x1 − t π (c − t ) −c (19.53) Interchanging the order of integration and noting that 1 1 1 1 = − , (x1 − t)(s − t) s − x1 x1 − t s−t c dt = 0, s < c (Cauchy principal value), 2 2 1/2 (s − t) −c (c − t ) c π dt = 2 sgn(x1 ), x1  > c, 2 − t 2 )1/2 (x − t) (c (x − c2 )1/2 1 −c 1 the limit of (19.53) as x1 → c gives ki (c) =
σi2A (π c)1/2
− (πc)
−1/2
c
−c
c+s Ri (s) c−s
(19.54)
1/2 ds.
(19.55)
19.5. Stress Intensity Factors
323
In a similar fashion one deduces that at the tip x1 → −c, ki (−c) = σi2A (πc)1/2 − (πc)−1/2
c
−c
Ri (s)
c−s c+s
1/2 ds.
(19.56)
Thus ki (±c) is independent of the anisotropy of the medium. It can now be shown that the crack extension force is easily calculated from only knowing ki and Ki−1 j . When the crack extends from x1 = c to x1 = c + δc, the change in energy is given by 1 δE = 2
c+δc
dx1 σi2 (x1 , 0)
c
x1 −δc
Fi (t) dt.
−c
(19.57)
Using (19.44), (19.51), and (19.55) and letting δc → 0 (see the next subsection for details), the crack extension force is found to be 1 δE −1 = ki km Kim , δ → 0 δc 8π
G = − lim
(19.58)
which is the desired result. Had we considered the crack tip at x1 = −c extending from −c to −(c + δc), we would have obtained (19.58) with ki given by (19.56). Since in deriving (19.58) we considered extension of only one end of the crack, in this instance the proper Grifﬁth criterion for brittle fracture would be G = 2γ . Equations (19.55) and (19.56) may also be used to derive formulae for the applied stress at which an equilibrium crack becomes mobile. In this instance we interpret the Ri (x1 ) as restraining stresses acting on the crack surfaces due to cohesive forces; usually one imagines that Ri (x1 ) differs appreciably from zero only in regions c − d < x1  < c, where d c, and d is independent of c. Such a crack will propagate when ki (±c) ≥ 0, i.e., when σi2A ≥
1 πc
c −c
Ri (s)
c±s c∓s
ds.
(19.59)
The upper and lower signs correspond to the tips x1 = c and x1 = −c, respectively. The fracture criterion expressed in (19.59) depends on anisotropy only through the dependence of Ri (s), the cohesive forces, on anisotropy. The utility of (19.58) for the crack extension force is that the stress intensity factors, ki , need be calculated only once, using either (19.55) or (19.56), for a given crack conﬁguration, because anisotropic effects appear only through the Ki−1 j . The determination of G may also be executed in the X frame. This would be most easily done by calculating Ki−1 j in the X frame and computing ki (X frame) = Aimkm(crack frame), where Aim is the cosine of the angle between the Xi and xm directions.
19.5.1 Computation of the Crack Extension Force In this section the procedure for evaluating G is developed in detail. We wish to evaluate δE , δc → 0 δc
G = − lim
(19.60)
324
19. Cracks in Anisotropic Media
where 1 4
δE =
c+δc
σi2 (x1 , 0)dx1
c
1 −1 = (8π)−1/2 ki Kim 2
x1 −δc
−c
c+δc
−1 Kim Qm(t) dt
(x1 − c)
−1/2
dx1
c
(19.61)
x1 −δc
−c
Qm(t) dt,
with ki given by (19.55). If we let s = x1 − c and integrate by parts, noting that c Qm(t) dt = 0 −c
(19.62)
when (19.27) is satisﬁed, there follows −1 δE = −(8π )−1/2 ki Kim
δc
s 1/2 Qm(c − δc + s) ds.
(19.63)
0
The further substitution of s = (1 − λ)δc reduces (19.63) to 1 δE −1 = (8π)−1/2 ki Kim − (δc)1/2 (1 − λ)1/2 Qm(c − λδc) dλ. δc 0 For the crack with singular stresses at x1 = ±c, we have c t Rm(s)(c2 − s 2 )1/2 1 A 1 ds. + Qm(t) = σm2 2 π (c − t 2 )1/2 π 2 (c2 − t 2 )1/2 −c s−t
(19.64)
(19.65)
As δc → 0, the ﬁrst term in (19.65) on the r hs yields a contribution to −δE/δc given by c 1 1 − λ 1/2 1 −1 A 1 −1 A −1/2 1/2 (8π) ki Kim ki Kim σm2 (δc) dλ = σm2 (π c)1/2 . (19.66) π 2δc 0 λ 8π Interchanging the order of integration, the second term on the r hs of (19.65) becomes c 1 1 c + s 1/2 −1 Rm(s) ds, (19.67) lim χ = − ki Kim δc → 0 8π (π c)1/2 −c c−s where −1 χ = (8π)−1/2 ki Kim
× 0
1
1−λ λ
1 (δc)1/2 π2
1/2
1 2cδc
1/2
c
−c
Rm(s)(c2 − s 2 )1/2 ds
dλ . c − s + λδc
In obtaining (19.67) we have noted that 1 π dλ 1 − λ 1/2 lim =− . δc → 0 0 λ s − c + λδc 2(c − s)
(19.68)
Comparing (19.66) and (19.67) with (19.55) yields the crack extension force in the form G=
1 −1 ki Kim km. 8π
(19.69)
Equation (19.69) is also valid for the crack extension force at the crack tip at x1 = −c, provided we use ki as given in (19.56).
19.7. Energy Factor Matrix
325
c ζ
Figure 19.4. Crack tip opening.
19.6 Crack Tip Opening Displacement Of particular interest is the result given in (19.28) for the crack tip opening displacement. Here we simply list some results for the case of isotropic elastic media. Recall that the displacement discontinuity at the crack tip is given as x1 − = F j (t) dt, (19.70) ui = uiD (x1 , x2 )xx22 =0 =0+ −c
with A F j (t) = K−1 ji Ti
1 . − t 2 )1/2
(19.71)
dt . (c2 − t 2 )1/2
(19.72)
2π (c2
Thus, ui =
A K−1 ji σi2
2π
x1
−c
Simple integration yields −ui = ui (x1 , 0+ ) − ui (x1 , 0− ) =
A K−1 ji σi2
2π
(c2 − t 2 )1/2 .
(19.73)
Now, let δi (x1 ) = ui (x1 , 0+ ) − ui (x1 , 0− ) and consider the case of isotropic media. Recalling the expressions in (19.2), we have, for a Mode II crack stressed by inplane shear, δ1 (x1 ) =
2(1 − ν) A 2 σ12 (c − x12 )1/2 . G
(19.74)
Consider the region just behind the crack tip, say at a distance ζ behind the tip (Fig. 19.4). √ A πc, we ﬁnd Noting that k1 = σ12 δ1 (ζ ) =
4k1 (1 − ν) 1/2 ζ . √ 2π G
δ2 (x1 ) =
4k2 (1 − ν) 1/2 ζ , √ 2π G
(19.75)
By identical reasoning, we have
4k3 δ3 (x1 ) = √ ζ 1/2 . 2π G
(19.76)
19.7 Dislocation Energy Factor Matrix In this section a simple and convenient method for calculating the dislocation energy factor matrix, K, is developed. We begin with the line integral giving the solution for the displacement gradient of a dislocation line, i.e., ∂ Gir (x − x ) dx j . (19.77) ui, p (x) = − pjw bmCwmr s ∂ xs C
326
19. Cracks in Anisotropic Media
x3
P(x 1,x 2 ,x3 ) ρ
t Figure 19.5. Coordinate frame for dislocation.
x2 x1
The integral is taken over the dislocation line, C. We also recall that, in general, analytic solution for the Green’s function does not exist, but its Fourier transform is given as 2π 1 Mir−1 (z) dθ, (19.78) Gir (x − x ) = 8π 2 x − x  0 where the Christoffel stiffness tensor is M = z · C · z, and in this context z(θ) is a unit vector lying in the plane perpendicular to x − x . In terms of the unreduced Fourier transform of G, we have ∞ M−1 i ∂ Gir (x − x ) = − d3 K zs ir e−iK·(x−x ) . (19.79) ∂ xs 8π −∞ K Here K is the Fourier vector and z is the unit vector along K. Consequently, (19.77) may be rewritten as ∞ Mir−1 (x) −iK·x i 3 e pjw bmCwmr s d K zs eiK·x dx j . (19.80) ui, p (x) = 2 8π K −∞ C For an inﬁnitely long and straight dislocation line, laying along the unit vector t, ∞ iK·x e dx j = t j eiK·ts ds = 2π t j δ(K · t), (19.81) C
−∞
where s is the distance along the line. Hence, only those Fourier vectors perpendicular to the dislocation line contribute to the displacement gradient ﬁeld, and (19.81) becomes ∞ Mir−1 (z) 1 2 sin(Kz · x). (19.82) ui, p (x) = t b C d K z pjw j m wmr s s 4π 2 K −∞ The integral in (19.82) extends over the plane deﬁned by z · t = 0, and for this plane z · x = z · ρ,
(19.83)
where ρ is the polar radius vector from the dislocation line to the point x, as illustrated in Fig. 19.5. Accordingly, we may replace x with ρ in (19.82) and thereby show that the ﬁeld is independent of position along the dislocation line, as it should be for an inﬁnitely long and straight line. In the plane z · t = 0 we deﬁne a polar coordinate system centered about the dislocation line, such that d2 K = KdKdψ,
(19.84)
zs = αs cos ψ + βs sin ψ,
(19.85)
where 0 ≤ ψ ≤ 2π. Then
19.7. Energy Factor Matrix
327
where α and β are two orthogonal unit vectors in the plane z · t = 0. In particular, we may choose them such that α1 = sin θ,
α2 = − cos θ,
α3 = 0,
β1 = cos ϕ cos θ,
β2 = cos ϕ sin θ,
β3 = − sin ϕ.
(19.86)
Similarly the vector ρ is written as ρm = ρ(αm cos ψ0 + βm sin ψ0 ),
(19.87)
sin(Kz · ρ) = sin[Kρ cos(ψ − ψ0 )].
(19.88)
so that
The integral in (19.82) is now rewritten in terms of this polar coordinate system, and the integration over K yields ∞ 1 sin[Kρ cos(ψ − ψ0 )] dK = sec(ψ − ψ0 ). (19.89) ρ 0 The expression for the displacements becomes 2π 1 pjw bmt j Cwmr s ui, p (ρ) = zs Mir−1 (ψ) sec(ψ − ψ0 ) dψ. 4π 2 ρ 0 The integral in (19.90) is deﬁned by its Cauchy principal value. The elastic energy is given by 1 R E= (C f gi p ui, p bg N f ) dρ, 2 r0
(19.90)
(19.91)
where N f = −α f sin ψ0 + β f cos ψ0 =
1 f sr ts ρr ρ
(19.92)
are the components of the unit normal to the planar cut surface used (arbitrarily as usual) to create the dislocation, and across which the displacement jumps by b. Clearly, the energy E is independent of ψ0 , so that 2π 1 E= E dψ0 . (19.93) 2π 0 If we integrate (19.92) over ψ0 , interchange the order of integration, and note that sec ζ = 2
∞ (−1)h cos(2h + 1)ζ, h=0
we obtain
2π
ζ = −
3π π 3π , , ,..., 2 2 2
N f sec(ψ − ψ0 ) dψ0 = 2π n f ,
(19.94)
(19.95)
0
with n f = −α f sin ψ + β f cos ψ = dz f /dψ.
(19.96)
328
19. Cracks in Anisotropic Media
This yields 1 E= 8π 2
2π R zs n f Mir−1 (ψ) dψ. ln bmbg pjw t j C f gi pCwmr s r0 0
(19.97)
Next, we recognize that αs β f − βs α f = vs f tv ,
(19.98)
so that
1 vs f tv + (αs β f + βs α f ) cos(2ψ) + (β f βs − α f αs ) sin(2ψ) . 2 Finally, we obtain zs n f =
(19.99)
E = Kmg bmbg ln(R/r0 ),
(19.100)
∗ ∗ Kmg = (Kmg + Kgm ) = Kgm,
(19.101)
where
and ∗ Kmg =
π π 1 −1 t C C t M dψ + (α β + β α ) Mir−1 cos(2ψ) dψ pjw j f gi p wmr s vs f v s f s f ir 16π 2 0 0 π + (β f βs − α f αs ) Mir−1 sin(2ψ) dψ . 0
19.8 Inversion of a Singular Integral Equation Certain solutions were given above for the singular integral equations involved with determining the equilibrium distributions of dislocations. Here we list a brief summary of some techniques given by Muskhelishivili (1960) for inverting integral equations of the form f (t) dt = σ (x), (19.102) p.v. D t −x where p.v. signiﬁes the principal value of the integral. If f (t) and σ (x) are functions that are continuous in the interval D, and if D consists of p ﬁnite segments of which at q of the 2 p ends f (t) is bounded, then 1 R1 (x) 1/2 R2 (x) 1/2 σ (t) dt R1 (x) 1/2 + p.v. Pp−q−1 (x), (19.103) f (x) = − 2 π R2 (x) t−x R2 (x) D R1 (x) provided p − q ≥ 0. Here R1 (x) =
q . i=1
(x − ei ),
R2 (x) =
2p .
(x − ei ).
(19.104)
i=q+1
The polynomial Pp−q−1 (x) is an arbitrary polynomial of degree ≤ p − q − 1, with P−1 = 0. The end points of the segments are ei . When p − q < 0, the same solution is valid with the necessary and sufﬁcient condition R2 (x) 1/2 m x σ (x) dx = 0, m = 0, 1, . . . , q − p − 1. (19.105) D R1 (x)
19.9. Stroh Formalism
329
19.9 2D Anisotropic Elasticity – Stroh Formalism For the sake of completeness, in this section we give a brief summary of the Stroh formalism for twodimensional anisotropic elasticity. Consider a twodimensional anisotropic elasticity problem in which the deformation ﬁeld is independent of the x3 coordinate, so that the displacement components are uk = uk(x1 , x2 ),
k = 1, 2, 3.
(19.106)
The corresponding stresses are σi j = Ci jkl uk,l ,
(19.107)
where Ci jkl are the components of the anisotropic elastic moduli tensor (with respect to selected coordinate directions x1 , x2 , x3 ). They are assumed to possess the usual symmetry properties with respect to the interchange of indices i j and k l, as well as reciprocal symmetry Ci jkl = Ckli j . In the absence of body forces, the equilibrium equations are σi j, j = 0 ,
(19.108)
Ci jkl uk, jl .
(19.109)
or, after using (19.107),
A general solution of (19.109) can be cast in the form uk = ak f (z),
z = x1 + px2 ,
(19.110)
where ak and p are complexvalued constants, and f is an arbitrary function of z. Since uk,l = f ak(δ1l + pδ2l ),
f = d f/dz ,
uk, jl = f ak(δ1 j + pδ2 j )(δ1l + pδ2l ),
f = d2 f/dz2 ,
we obtain from (19.109)
Ci1k1 + p(Ci1k2 + Ci2k1 ) + p2 Ci2k2 ak = 0 ,
(19.111)
whereas (19.107) gives σi j = f (Ci jk1 + pCi jk2 )ak .
(19.112)
In particular, σi1 = f (Ci1k1 + pCi1k2 )ak , σi2 = f (Ci2k1 + pCi2k2 )ak .
(19.113)
In view of the reciprocal symmetry of Ci jkl , we now deﬁne the symmetric 3 × 3 matrices Q and T with components Qik = Ci1k1 ,
Tik = Ci2k2 ,
(19.114)
and the nonsymmetric 3 × 3 matrix R with components Rik = Ci1k2 .
(19.115)
330
19. Cracks in Anisotropic Media
Since the elastic strain energy is positive, the matrices Q and T are positivedeﬁnite. With so deﬁned matrices Q, T, and R, (19.111) and (19.113) can be rewritten in the matrix form as
(19.116) Q + p R + RT + p2 T · a = 0 and
t2 = f RT + pT · a ,
t1 = f (Q + pR) · a , where
⎡
⎡ ⎤ a1 ⎣ a = a2 ⎦ , a3
⎤ σ11 t1 = ⎣σ21 ⎦ , σ31
(19.117)
⎡
⎤ σ12 t2 = ⎣σ22 ⎦ . σ32
(19.118)
The equilibrium equations (19.108) can be cast in the vector form as t1,1 + t2,2 = 0 .
(19.119)
This suggests the introduction of the vector stress function ϕ, such that t1 = −
∂ϕ , ∂ x2
∂ϕ , t2 = ∂ x1
∂ϕi , ∂ x2
i.e.,
σi1 = −
i.e.,
∂ϕi σi2 = . ∂ x1
(19.120)
When these are introduced in (19.117), there follows −
∂ϕ = f (Q + pR) · a , ∂ x2 ∂ϕ = f (RT + pT) · a . ∂ x1
(19.121)
Since z = x1 + px2 , and ∂f = f , ∂ x1
∂f = pf , ∂ x2
equations (19.121) can be integrated to give f ϕ = − (Q + pR) · a = f RT + pT · a . p
(19.122)
ϕ = f (z)b ,
(19.123)
1 b = RT + pT · a = − (Q + pR) · a . p
(19.124)
Thus,
where
It was shown by Stroh (1958) that the constants p, ak, and bk can be determined simultaneously from the sixdimensional eigenvalue problem as follows. From the ﬁrst of (19.124), upon the multiplication with T−1 , we have (19.125) − T−1 · RT · a + T−1 · b = p · a .
19.9. Stroh Formalism
331
By multiplying this with R, we obtain pR · a = R · T−1 · b − R · T−1 · RT · a .
(19.126)
The second of (19.124) can be rearranged as −Q · a − pR · a = pb ,
(19.127)
R · T−1 · RT − Q · a − R · T−1 · b = p · b .
(19.128)
or, by using (19.126),
Equations (19.125) and (19.128) together constitute a sixdimensional eigenvalue problem N · υ = pυ , where
−T−1 · RT R · T−1 · RT − Q
N=
(19.129) T−1 −R · T−1
(19.130)
is a real nonsymmetric 6 × 6 matrix, and
a υ= b
(19.131)
is a sixdimensional vector with components {a1 , a2 , a3 , b1 , b2 , b3 }. The eigenvalue problem (19.129) delivers six eigenvalues p(α) and six corresponding eigendirections υ (α) (α = 1, 2, . . . , 6). They depend only on the type of elastic anisotropy and the values of elastic moduli. The positive deﬁniteness of the strain energy requires the six eigenvalues to appear as three pairs of complex conjugates. It is convenient to arrange them so that p(1) , p(2) , and p(3) have positive imaginary parts, i.e., Im p(α) > 0 ,
α = 1, 2, 3 ,
p(α+3) = p¯ (α) ,
α = 1, 2, 3 ,
(19.132)
where overbar denotes the complex conjugation and Im the imaginary part. Correspondingly, we have a(α+3) = a¯ (α) ,
α = 1, 2, 3 ,
b(α+3) = b¯ (α) ,
α = 1, 2, 3 .
(19.133)
The general solution can now be expressed by superposition as u=
3 a(α) f (α) (z(α) ) + a¯ (α) f (α+3) (¯z(α) ) ,
(19.134)
α=1
ϕ=
3
b(α) f (α) (z(α) ) + b¯ (α) f (α+3) (¯z(α) ) ,
(19.135)
α=1
in which f (α) are arbitrary functions of their argument, and z(α) = x1 + p(α) x2 , (α = 1, 2, . . . , 6). Equations (19.134) and (19.135) are Stroh’s solutions for twodimensional
332
19. Cracks in Anisotropic Media
anisotropic elasticity. See also Eshelby, Read, and Shockley (1953) and, for an alternative approach, Lekhnitskii (1981). In many applications, the functions f (α) assume the same function form, differing only by complex scaling parameters q(α) , such that f (α) (z(α) ) = q(α) f (z(α) ) ,
(19.136)
f (α+3) (¯z(α) ) = q¯ (α) f¯(¯z(α) ) . Thus, by introducing the matrices
A = a(1) a(2) a
(3)
⎡ (1) a ⎢ 1 = ⎣a2(1) (1) a3 ⎡
B = b(1) b(2)
(1)
b
⎢ 1 b(3) = ⎣b2(1) (1) b3
(2)
a1 (2) a2 (2) a3 (2)
b1 (2) b2 (2) b3
⎤ (3) a1 (3) ⎥ a2 ⎦ , (3) a3
(19.137)
⎤ (3) b1 (3) ⎥ b2 ⎦ , (3) b3
(19.138)
⎡
⎤ f (z(1) ) 0 0 F=⎣ 0 0 ⎦, f (z(1) ) 0 0 f (z(1) )
(19.139)
⎡ (1) ⎤ q q = ⎣q(2) ⎦ , q(3)
(19.140)
and the vector
the solution (19.134) and (19.135) can be compactly expressed as u = 2Re (A · F · q) ,
(19.141)
ϕ = 2Re (B · F · q) ,
(19.142)
where Re stands for the real part. For example, for a Grifﬁth crack of length 2c, subject to uniform tractions −t02 over the crack faces which are parallel to x1 direction, it can be shown that (e.g., Ting, 1991) f (z) =
q=B
1 2 (z − c2 )1/2 − z , 2
(19.143)
⎡ 0⎤ σ21 0⎦ . = ⎣σ22 0 σ23
(19.144)
−1
·
t02
,
t02
19.9.1 Barnett–Lothe Tensors Equations (19.141) and (19.142) are genearal solutions, provided that the state of anisotropy is such that there are indeed six independent eigenvectors υ (α) . This is, for
19.9. Stroh Formalism
333
√ example, not the case with isotropic materials, for which p = i = −1 is a triple eigenvalue with only two independent eigenvectors. Barnett and Lothe (1973) constructed a method to derive the solution which circumvent the need of solving the sixdimensional eigenvalue problem. They introduced the real matrices S, H, and L, which are related to complex matrices A and B by S = i(2A · BT − I), and showed that S=− 1 H= π L=
1 π
1 π
0 π
π
H = 2iA · AT ,
L = −2iB · BT ,
(19.145)
T−1 (θ) · RT (θ) dθ ,
T−1 (θ) dθ ,
(19.146)
0
π
Q(θ) − R(θ) · T−1 (θ) · RT (θ) dθ ,
0
where Qik(θ) = Ci jkl n j nl , Rik(θ) = Ci jkl n j ml ,
(19.147)
Tik(θ) = Ci jkl m j ml , and n = {cos θ, sin θ, 0}, m = {− sin θ, cos θ, 0}. It is clear that H and H are symmetric (because T−1 and Q are). It can also be shown that the products S · H, L · S, H−1 · S, and S · L−1 are antisymmetric tensors. There is furthermore a connection H · L − S · S = I. The explicit representations for Barnett–Lothe tensors S, H, and L have been reported in the literature for various types of anisotropic materials, such as cubic and orthotropic (e.g., Chadwick, and Smith, 1982; Ting, 1996). For example, along the plane coinciding with the crack faces of the Grifﬁth crack, loaded over its crack faces by uniform tractions, one has (Ting, 1991) (x12 − c2 )1/2 , x1  > c, (19.148) (z2 − c2 )1/2 = 2 1/2 2 ±i(c − x1 ) , x1  < c, x2 = ±0 . The displacement and traction vectors for ±x1 > c are
u(x1 , 0) = ± x1  − (x12 − c2 )1/2 S · L−1 · t2 0 ,
t1 (x1 , 0) = − x1 (x12 − c2 )−1/2 − 1 G2 · t2 0 ,
t2 (x1 , 0) = x1 (x12 − c2 )−1/2 − 1 t2 0 , while, for x1  < c,
u(x1 , ±0) = ±(c2 − x12 )1/2 I + x1 S · L−1 · t2 0 ,
t1 (x1 , ±0) = ±x1 (c2 − x12 )−1/2 G1 − G2 · t2 0 ,
(19.149)
(19.150)
t2 (x1 , ±0) = −t2 0 . The G matrices are here deﬁned by G1 = R · T−1 · RT − Q · L−1 ,
G2 = R · T−1 + G1 · L · S · L−1 .
(19.151)
334
19. Cracks in Anisotropic Media
From the ﬁrst of (19.149) or (19.150) it is observed that u(c, 0) is in general not equal to zero, unless S · L−1 · t2 0 = 0. Furthermore, the traction vector t2 (x1 , 0) is independent of the type of elastic anisotropy or the values of the elastic moduli. This was already demonstrated by (19.47).
19.10 Suggested Reading Barnett, D. M., and Asaro, R. J. (1972), The Fracture Mechanics of SlitLike Cracks in Anistropic Elastic Media, J. Mech. Phys. Solids, Vol. 20, pp. 353–366. Barnett, D. M., and Lothe, J. (1973), Synthesis of the Sextic and the Integral Formalism for Dislocation, Green’s Functions and Surface Waves in Anisotropic Elastic Solids, Phys. Norv., Vol. 7, pp. 13–19. Cherepanov, G. P. (1979), Mechanics of Brittle Fracture, McGrawHill, New York. Eshelby, J. D., Read, W. T., and Shockley, W. (1953), Anisotropic Elasticity with Applications to Dislocation Theory, Acta Metall., Vol. 1, pp. 251–259. Freund, L. B. (1990), Dynamic Fracture Mechanics, Cambridge University Press, Cambridge. Gdoutos, E. E. (1990), Fracture Mechanics Criteria and Applications, Kluwer, Dordrecht, The Netherlands. Lekhnitskii, S. G. (1981), Theory of Elasticity of an Anisotropic Elastic Body, Mir Publishers, Moscow. Kanninen, M. F., and Popelar, C. H. (1985), Advanced Fracture Mechanics, Oxford University Press, New York. Mura, T. (1987), Micromechanics of Defects in Solids, Martinus Nijhoff, Dordrecht, The Netherlands. Rice, J. R. (1968), Mathematical Analysis in the Mechanics of Fracture. In Fracture – An Advanced Treatise (H. Liebowitz, ed.), Vol. II, pp. 191–311, Academic Press, New York. Stroh, A. N. (1958), Dislocations and Cracks in Anisotropic Elasticity, Phil Mag., Vol. 3, pp. 625–646. Ting, T. C. T. (1996), Anisotropic Elasticity, Oxford University Press, New York. Wu, J. J., Ting, T. C. T., and Barnett, D. M., eds. (1991), Modern Theory of Anisotropic Elasticity and Applications, SIAM, Philadelphia.
20 The Inclusion Problem
The problem considered here has found application to a legion of physical applications including, inter alia, the theory of solid state phase transformations where the transformation (arising from second phase precipitation, allotropic transition, or uptake of solutes, or changes in chemical stoichiometry) causes a change in size and/or shape of the transformed, included, region; differences in thermal expansion of an included region and its surrounding matrix, which in turn causes incompatible thermal strains between the two; and, perhaps surprisingly, the concentrated stress and strain ﬁelds that develop around included regions that have different elastic modulus from those of their surrounding matrices. For the reason that the results of this analysis have application to such a wide variety of problem areas, and because the solution approach we adopt has heuristic value, we devote this chapter to the inclusion problem.
20.1 The Problem In an inﬁnitely extended elastic medium, a region – the “inclusion” – undergoes what would have been a stress free strain. Call this strain the “transformation strain,” eT . Due to the elastic constraint of the medium, i.e., the matrix, there are internal stresses and elastic strains. What is this resulting elastic ﬁeld and what are its characteristics? In particular, can an exact solution be found for this involved elastic ﬁeld? The region of interest is shown in Fig. 20.1 and is denoted as VI ; the outward pointing unit normal to VI is n. The stress free transformation, i.e., change in size and shape, can be viewed as occurring while the inclusion has been hypothetically removed from the medium, as depicted in Fig. 20.1. Thus the transformation indicated by eT involves a displacement within the inclusion of the form b(x) = eT · x, bi = eiTj x j .
(20.1)
The size and shape change associated with this transformation have caused no stresses and elastic strains if it were not for the constraint of the matrix. We consider here the case where eT is uniform, i.e., does not depend on position. We denote the elastic constants as C, so that the linear connection between stress and elastic strain, eel , is σ = C : eel In the discussion that follows, the distinction between elastic strain 335
336
20. The Inclusion Problem step 0
step
1 >
eT
ep
VI
VI
st
Vm
2 >
VI
n SI
T
VI
Figure 20.1. Eshelby’s heuristic scheme for the inclusion setup.
VI I
Vm
rep l e V ac
>
T
p 3
ste
ficticious ste body force p 4 re m o ve body force
cancell T
T VI T = T
and total strain will be made clear in speciﬁc context. For the inﬁnitesimal strain formulation considered here the total strain is simply the sum of the elastic and the “nonelastic” strains.
20.2 Eshelby’s Solution Setup We consider the following heuristic solution approach originally devised by Eshelby (1957). The approach will involve a series of heuristic steps, each accompanied by a change in stress or strain. The concept of linear superposition is used to “build the solution.” Step 1: It is explicitly understood that the inclusion is embedded and bound to the matrix and its interface purely continuous with the matrix (medium). Thus all ﬁnal displacements must be so continuous, and, as our procedure will show, they are. We imagine removing the inclusion from the medium by a purely heuristic process that produces no stress in the inclusion or in the medium. This means, of course, that no elastic strain has been induced in either region. Now let the inclusion transform, i.e., let it undergo a homogeneous strain as prescribed by (20.1). This will induce a total strain in VI of eT . At this stage, the stresses in both the inclusion, VI , and the medium, Vm , are zero. Also, the total strain in the medium is zero at this stage. To be formal, we say eI1 = eT , em1 = 0,
σ I1 = 0, σ m1 = 0.
(20.2)
The convention will be that the ﬁrst superscript, (..)I or (..)m , represents ﬁeld quantities that belong to the inclusion and medium, respectively, and the second superscript indicates the contribution of that ﬁeld quantity from the “step” in question. Step 2: Now the inclusion in its hypothetically separated, yet transformed, state will no longer “ﬁt” within the “hole” in the medium that it came from. But it has undergone a
20.2. Eshelby’s Solution Setup
337
uniform strain, eT . To replace it within the medium, we may imagine applying a uniform set of boundary traction, T, such that T = −C : eT · n, T Ti = −Ci jkl ekl nj.
(20.3)
This has the result of producing a uniform state of elastic strain, and therefore uniform stress, in the inclusion. No strain, or stress, has yet to be caused in the matrix. The contributions to total stress and strain from this step is eI2 = −eT , em2 = 0,
σ I2 = −C : eT , σ m2 = 0.
(20.4)
Step 3: At this point the inclusion will ﬁt perfectly into the “hole” from which it came, and therefore it may be reinserted, and the interface between it and the medium made continuous again. At this stage the state of strain and stress is eI3 = eI1 + eI2 = 0, em3 = 0,
σ I3 = −C : eT , σ m3 = 0.
(20.5)
It is important to recall, however, that the elastic strain in the inclusion is at this stage, −eT , which of course accounts for the state of stress in the inclusion. Note, as explained above, that at this point all displacements are to be continuous across the interface between the inclusion and matrix – and at this point they already are! The ﬁnal step will produce additional displacements in both the matrix and inclusion which are inherently continuous. Although the inclusion now ﬁts within its original “hole,” there are what now appears to be an embedded layer of body force T = −C : eT · n distributed around the interface SI . To remove these ﬁctitious body forces we apply a layer of annulling forces, −T = C : eT · n around SI , as indicated in Fig. 20.1. The application of these forces will cause displacements, elastic strains, and additional stresses, in both the medium and the inclusion; call these the “constrained ﬁeld,” as they occur under the constraint of the inﬁnite elastic medium. Thus the superscript 4 will be replaced by c to specially designate this. Step 4 or c: The last step involves the removal of the unwanted layer of body force, T. Formally this is accomplished by applying a layer of body force −T around SI . However, as already explained, this occurs while the inclusion is bound to the medium. Thus, all displacements that occur in this step will be continuous across the interface between the inclusion and matrix. Call these displacements, inside and outside VI , uc . It is this constrained or c ﬁeld we will now solve for. However, the ﬁnal state for the total ﬁeld quantities within the inclusion and medium will be eI4 = eI1 + eI2 + ec = ec , em4 = ec ,
σ I4 = −C : eT + σ c , σ m4 = σ c ,
(20.6)
where the strains ec are calculated from the constrained displacements, and the stresses σ c are calculated as σ c = C : ec .
338
20. The Inclusion Problem
It is also important to explicitly note the total displacements in the inclusion and the medium at this ﬁnal stage; they are in both VI and Vm .
u = uc
(20.7)
On the other hand, the displacements that cause elastic strains, and thus stresses, are u = −b + uc
in VI , and u = uc in Vm .
(20.8)
Thus, the elastic strains in the inclusion are e = eel = ec − eT
in VI .
(20.9)
20.3 Calculation of the Constrained Fields: u c , ec , and σ c To calculate the displacements caused by the application of the layer of body force, −T = C : eT · n, we simply use linear superposition and the Green’s function to write c T u p (x) = Ci jkl ekl n j Gi p (x − x ) dS
SI
=
SI
T (Ci jkl ekl Gi p )n j dS
=
T Ci jkl ekl
VI
∂ Gi p (x − x ) dV . ∂ x j
We note that Gi p = Gi p (x − x )
⇒
∂ ∂ Gi p (x − x ) Gi p (x − x ) = − ∂xj ∂xj
and thus ucp (x)
∂ = ∂xj
VI
T Ci jkl ekl Gi p (x − x ) dV .
For the distortion, i.e., the displacement gradient, we have ∂ucp ∂2 T = Ci jkl ekl Gi p (x − x ) dV . ucp,s (x) = ∂ xs ∂ xs ∂ x j VI We recall that the Green’s function is given by ∞ Mi−1 1 p (z) 3 Gi p (x − x ) = d k exp[−ik · (x − x )], 3 8π −∞ k2 where k is the Fourier vector and z is a unit vector aligned along k. Thus, ∞ Mi−1 ∂ucp ∂2 p T 1 3 =− Ci jkl ekl d k exp(−ik · x) ∂ xs ∂ xs ∂ x j 8π 3 −∞ k2 exp(ik · x ) dV . × VI
Consider the last integral ﬁrst, i.e., VI
exp(ik · x ) dV .
(20.10)
(20.11)
(20.12)
(20.13)
(20.14)
20.3. Calculation of the Constrained Fields
339
k φ Ω
x' Figure 20.2. A polar coordinate system aligned with k.
θ
Let VI be an ellipsoidal volume with axes a1 , a2 , a3 , for reasons that will be clear in what follows. Deﬁne expanded variables and a polar coordinate system aligned with k (see Fig. 20.2), as follows Ki = ki ai and Ri = xi /ai
(no sum on i),
k · x = K · R = K R cos φ, dV = d3 x = a1 a2 a3 d3 R, d3 x = a1 a2 a3 R2 sin φ dφ dR dθ. Then,
exp(ik · x ) dV = a1 a2 a3
1
R2 dR 0
VI
exp(i K R cos φ) sin φ dφ dθ.
(20.15)
Note that is a unit sphere such that 0 ≤ θ ≤ 2π and 0 ≤ φ ≤ π . The integral over θ is trivial, so that 1 π 2 (20.16) exp(ik·x ) dV = 2πa1 a2 a3 R dR exp(i K R cos φ) sin φ dφ. 0
VI
0
The standard integral tables reveal that π (2π)1/2 exp(i K R cos φ) sin φ dφ = J1/2 (K R), (K R)1/2 0
(20.17)
where J1/2 (K R) is a fractional Bessel function. Thus, π 2πa1 a2 a3 (2π )1/2 1 3/2 exp(i K R cos φ) sin φ dφ = R J1/2 (K R) dR K1/2 0 0 =
2πa1 a2 a3 (2π )1/2 J3/2 (K), K3/2
with K = K = (k12 a12 + k22 a22 + k32 a32 )1/2 .
(20.18)
Consequently, ucp,s = −
1 ∂2 T a1 a2 a3 (π/2)1/2 Ci jkl ekl ∂ xs ∂ x j 2π 2
∞ −∞
d3 k
Mi−1 p (z) k2
exp(−ik · x)
J3/2 (K) . K3/2 (20.19)
340
20. The Inclusion Problem
If we again deﬁne Ki = ki ai ,
(no sum on i),
K2 = ki2 ai2 ,
d3 k =
(20.20)
1 d3 K, a1 a2 a3
then Ki ki νi = = , K Kai ai
(no sum on i), (20.21)
k 21 + k 22 + k 23 ν2 ν2 ν2 = 12 + 22 + 32 , 2 K a1 a2 a3 so that k · x = Kν · R,
Ri = xi /ai ,
(no sum on i).
(20.22)
Now, take the real part of (20.19) to obtain ∞ d3 KM−1 ∂2 1 pi cos[K(ν · R)]J3/2 (K) T . ucp,s = − 2 π/2 Ci jkl ekl 2 3/2 2π ∂ x j ∂ xs −∞ K K [(ν1 /a1 )2 + (ν2 /a2 )2 + (ν3 /a3 )2 ]
(20.23)
Next, introduce another polar coordinate system aligned with R, so that d3 K = k2 dK sin φ dφ dθ, and note
0
∞
√ cos[K(ν · R)]J3/2 (K) dK = 1/2 π/2 1 − (ν · R)2 , 3/2 K
(20.24)
if (ν · R) ≤ 1. It follows that ucp,s =
1 T Ci jkl ekl 4π
2π
0
π 0
sin φ M−1 pi (ν)(ν j /a j )(νs /as ) [(ν1 /a1 )2 + (ν2 /a2 )2 + (ν3 /a3 )2 ]
dφ dθ, (20.25)
(no sum on j, s), = Constants, if ν · R ≤ 1 . To form the strains we take the symmetric part of ucp,s , or ecp,s =
1 T Ci jkl ekl 8π
0
2π
0
π
−1 sin φ dφ dθn j [M−1 pi (ν)ns + Msi (ν)n p ]
[(ν1 /a1 )2 + (ν2 /a2 )2 + (ν3 /a3 )2 ]
,
(20.26)
where n p = (ν p /a p ),
(no sum on p).
We can conveniently deﬁne the components of the tensor S as 2π π −1 sin φ dφ dθn j [M−1 1 pi (ν)ns + Msi (ν)n p ] Ci jkl , S pskl = 8π [(ν1 /a1 )2 + (ν2 /a2 )2 + (ν3 /a3 )2 ] 0 0
(20.27)
such that T ecps = S pskl ekl .
(20.28)
20.4. Eshelby Tensor for Ellipsoidal Inclusion
341
x2
a2
x1
a1
Figure 20.3. An ellipsoidal inclusion with its principal axes parallel to coordinate axes.
a3 x3
The fourthorder tensor with components Si jkl is known as the Eshelby tensor. In summary, it is worth recalling that: In the Inclusion: σiIj = Ci j ps (ecps − eTps ), T , ecps = S pskl ekl c T eI,el ps = e ps − e ps ,
(20.29)
uiI,el = uic − bi , eIps = ecps . In the medium: σimj = Ci j ps ecps , c em ps = e ps ,
(20.30)
uim = uim,el = uic .
20.4 Components of the Eshelby Tensor for Ellipsoidal Inclusion The components of the Eshelby tensor Si jkl obey the symmetry Si jkl = S jikl = Si jlk .
(20.31)
When written with respect to coordinate axes parallel to principal axes of the ellipsoidal inclusion (Fig. 20.3), these components are S1111 =
3a12 1 − 2ν I11 + I1 , 8π(1 − ν) 8π (1 − ν)
S1122 =
a22 1 − 2ν I12 − I1 , 8π(1 − ν) 8π (1 − ν)
S1133
a32 1 − 2ν I13 − I1 , = 8π(1 − ν) 8π (1 − ν)
S1212 =
(20.32)
a12 + a22 1 − 2ν I12 + (I1 + I2 ) . 16π(1 − ν) 16π(1 − ν)
The remaining nonzero components are obtained by cyclic permutations of (1, 2, 3). All other components vanish.
342
20. The Inclusion Problem
The Ii integrals appearing in above expressions can be expressed in terms of elliptic integrals. Assuming that a1 > a2 > a3 , we have I1 =
4πa1 a2 a3 [F(θ, k) − E(θ, k)], (a12 − a22 )(a12 − a32 )1/2
4πa1 a2 a3 I3 = 2 (a2 − a32 )(a12 − a32 )1/2
"
# a2 (a12 − a32 )1/2 − E(θ, k) , a1 a3
(20.33)
I1 + I2 + I3 = 4π , where F(θ, k) and E(θ, k) are elliptic integrals of the ﬁrst and second kind, and 2 1/2 1/2 2 a1 − a32 a1 − a22 θ = arcsin , k= . a12 a12 − a32
(20.34)
The Ii j integrals can be calculated from 3I11 + I12 + I13 =
4π , a12
3a12 I11 + a22 I12 + a32 I13 = 3I1 , I12 =
a12
(20.35)
1 (I2 − I1 ) , − a22
and their cyclic counterparts. The stress components in an ellipsoidal inclusion due to uniform transformation (eigenstrain) eiTj are a12 1−ν σ11 ν = 3I11 + (I21 + I31 ) 2µ 8π(1 − ν) 1 − 2ν 1 − 2ν ! 1 − 2ν 1−ν ν 1−ν + I1 − (I2 + I3 ) − eT 8π(1 − ν) 1 − 2ν 1 − 2ν 1 − 2ν 11 a22 1−ν ν I12 + (3I22 + I32 ) + 8π(1 − ν) 1 − 2ν 1 − 2ν (20.36) ! 1−ν 1 − 2ν ν ν T I1 − (I2 − I3 ) − − e 8π(1 − ν) 1 − 2ν 1 − 2ν 1 − 2ν 22 a32 1−ν ν I13 + (3I33 + I23 ) + 8π(1 − ν) 1 − 2ν 1 − 2ν ! 1 − 2ν 1−ν ν ν − I1 − (I3 − I2 ) − eT , 8π(1 − ν) 1 − 2ν 1 − 2ν 1 − 2ν 33 2 a1 + a22 1 − 2ν σ12 T = I12 + (I1 + I2 ) − 1 e12 , 2µ 8π(1 − ν) 8π (1 − ν)
(20.37)
with other stress components obtained from the above two expressions by cyclic permutations of (1, 2, 3).
20.6. Inhomogeneous Inclusion
343
20.5 Elastic Energy of an Inclusion The elastic energy of the entire body, i.e., inclusion and medium is 1 E= 2
1 σi j ei j dV = 2 V
σi j ui, j dV.
(20.38)
V
Formally, we may divide the body into the inclusion volume and the volume of the medium, so that 1 1 I I,el σ u dV + σ m um dV. (20.39) E= 2 VI i j i, j 2 Vm i j i, j Since there are no body forces, i.e., ∇ · σ = 0, the divergence theorem shows that 1 1 (σiIj uiI ), j dV + (σ m um ), j dV E= 2 VI 2 Vm i j i 1 1 1 σiIj n j uiI,el dS + σiIj nˆ j uiI,el dS + σ m n∞ um dS. = 2 SI 2 SI 2 S∞ i j j i Furthermore,
S∞
m σimj n∞ j ui dS → 0,
because of the way in which the stresses and displacements fall off with distance. Thus, 1 (σ I n j uiI,el + σiIj nˆ j uim ) dS E= 2 SI i j 1 σ I n j (uiI,el − uim ) dS = (20.40) 2 SI i j 1 T σ I n j eis xs dS, =− 2 SI i j because uiI,el − uim = −bi . From (20.40) it then follows, with another use of the divergence theorem, that 1 σ I eT dV. (20.41) E=− 2 VI i j i j
20.6 Inhomogeneous Inclusion: Uniform Transformation Strain We next consider the problem of an inﬁnite medium containing an inclusion of a material different from that of the medium. The inhomogeneous inclusion, which occupies the volume VI , as before, is to undergo what would be, without the constraint of the surrounding medium, a stress free strain, e∗ . The elastic moduli tensor for this inclusion is designated as C∗ . For the case of a homogeneous inclusion, i.e., one having the same elastic constants as the medium, after undergoing a transformation strain, eT , the ﬁnal inclusion strain is ec = S : eT , and the resulting inclusion stress is σ = C : (S : eT − eT ). We recall, if the inclusion were of ellipsoidal shape, and if eT were uniform, the resulting stresses and strains in the inclusion were also uniform. We have omitted the superscript I for the
344
20. The Inclusion Problem
ε C C*
Figure 20.4. Inhomogeneous inclusion subject to far ﬁeld strains.
ε inclusion ﬁeld variables for brevity and because we will only require discussion of ﬁeld quantities within the inclusions for our development. With the above in mind, imagine applying surface forces to the inhomogeneous inclusion so as to produce a strain, ec − e∗ , where we will associate ec here with that of a companion homogeneous inclusion shortly. The resulting stresses in the inclusion are σ ∗ = C : (ec − e∗ ). Note that −e∗ strain will cancel the stress free strain, e∗ , which now leaves the total strain of the inhomogeneous inclusion to be ec . At this stage both the homogeneous and inhomogeneous inclusions have experienced the same total strains and thus have the same size and shape. If the stresses within the two inclusions are also identical, then we may replace the homogeneous inclusion with the inhomogeneous inclusion. This is so because the traction that would be computed from these stresses would be identical, and thus traction continuity would be maintained with the medium. For the stresses to be the same, we must be able to solve for a companion set of transformation strains for a homogeneous inclusion, eT , given the prescribed transformation strains, e∗ . The resulting equations are C : (S : eT − eT ) = C∗ : (S : eT − e∗ ), T T T ∗ Ci jkl (Sklmn emn − ekl ) = Ci∗jkl (Sklmn emn − ekl ).
(20.42)
The set (20.42) can indeed be solved for eT . Consider the problem of an inﬁnite medium containing an inclusion of a different material and subject to a far ﬁeld strain e∞ (Fig. 20.4). Suppose we ﬁrst solve the problem of a homogeneous inclusion with the same elastic constants as the medium and the same initial size and shape, which undergoes a uniform transformation strain eT . We recall that in the case of this companion homogeneous inclusion, the resulting state of stress and strain would be such that the total strain would be ec ; the elastic strain would, however, be ec − eT . Now, superimpose a uniform strain, e∞ , on this homogeneous inclusion as well as on the medium. The stress in the inclusion is σ hom,I = C : (ec − eT + e∞ ).
(20.43)
Next, subject the inhomogeneous inclusion, with elastic constants C, to a uniform strain ec + e∞ . Note at this point that the size and shape change undergone by this inhomogeneous inclusion is identical to that of the fully transformed companion homogeneous inclusion. The stresses in the inhomogeneous inclusion are σ inhom,I = C∗ : (ec + e∞ ).
(20.44)
20.7. Nonuniform Transformation Strain
345
If the stresses in both inclusions are the same, we may replace the companion homogeneous inclusion with its inhomogeneous counterpart. If the inclusions are of ellipsoidal shape this is possible because ec = S : eT , where S is a constant Eshelby tensor. Thus, given e∞ , C, C∗ , we may solve for the companion homogeneous eT from C : (S : eT − eT + e∞ ) = C∗ : (S : eT + e∞ ), T ∞ ∞ Ci jkl (Sklr s erTs − ekl + ekl ) = Ci∗jkl (Sklr s erTs + ekl ).
(20.45)
Note that the stresses and strains are everywhere the same for both the medium with the inhomogeneous and the companion homogeneous inclusions.
20.7 Nonuniform Transformation Strain Inclusion Problem As before, we imagine a volume element – that we will later, for clear advantage, take to be of ellipsoidal shape – undergo what would be a stressfree change in size and shape while it is embedded within an inﬁnite medium. The inclusion and its medium have the same elastic constants, C. The stressfree change in size and shape is described by a transformation strain, eT , as discussed in the previous sections. LEMMA 20.1: If an ellipsoidal region in an inﬁnite anisotropic linear elastic medium undergoes, in the absence of its surroundings, a stressfree transformation strain which is a polynomial of degree M in the position coordinates, x p , then the ﬁnal stress and strain state of the transformed inclusion, when constrained by its surroundings, is also a polynomial of degree M in the coordinates x p .
This generalization of Eshelby’s original theorem for the uniform inclusion in an isotropic elastic medium has far reaching consequences  viz., that all the developments of the previous section regarding the inhomogeneous inclusion hold true, as can be veriﬁed by direct analysis. Clearly, the above results for the uniform transformation strain are included in this generalization. Proof: We start almost from the beginning. Imagine cutting out the volume element VI in an undeformed inﬁnite anisotropic linear elastic medium. As this process is heuristic, let VI undergo a stressfree transformation strain eT (x), where x denotes position within the inclusion. The strain eT (x) is assumed to be continuous and differentiable, but is otherwise T be the stress derived from Hook’s law as above, i.e., if arbitrary. Now let piTj (x) = Ci jkl ekl T the uniform strain e were applied unconstrained to VI . The construction of the constrained elastic ﬁeld is accomplished by ﬁrst applying − piTj (x)n j to the surface SI bounding VI [and distributing body forces (∂/∂ x j ) piTj (x) throughout VI ]. With this nomenclature, we can move to the general expression, i.e., (20.11), for the components of displacement gradient, ∂uic ∂2 =− ∂ xp ∂ x p∂ x j
VI
T Gik(x − x ) pkj (x ) dV .
(20.46)
346
20. The Inclusion Problem
Take the Fourier transform of (20.46) to obtain, with K again being a Fourier vector, ∂uic T = K2 zp z j g jk(K) pkj (x ) exp(i Kz · x ) dV ∂ xp VI −1 T = zp z j Mik (z) pkj (x ) exp(i Kz · x ) dV . VI
We recall that the Fourier transform of G is g(K) = M−1 /K2 ,
(20.47)
where M ≡ z · C · z, and z = K/K. In other words, −1 gik(K) = Mik (K)/K2 .
(20.48)
Using the Fourier inversion described in Chapter 3, along with the spherical coordinate system, yields ∞ ∂uic −1 T = (2π)−3 zp z j Mik (z) d K2 exp(−i Kz · x) dK pkj (x ) exp(i Kz · x ) dV . ∂ xp 0 VI (20.49) Again, d = sin φ dφ dθ is the surface area over the unit sphere, as described in the previous section. We are interested in only the real part of (20.49), and we note that ∇x2 cos[Kz · (x − x)] = −K2 cos[Kz · (x − x)],
(20.50)
∇x2 ≡ ∂ 2 /∂ xs ∂ xs .
(20.51)
cos(Ks) dK = π δ(s).
(20.52)
where
We also recall that
∞
0
Thus, an interchange of the order of integration yields ∂uic 1 −1 =− 2 zp z j Mik (z) d ∇x2 pTjk(x )δ(z · x − z · x) dV . ∂ xp 8π VI
(20.53)
We now specialize to the case of an ellipsoidal inclusion, 3 (xα /aα )2 = 1,
(20.54)
α=1
which means that x lies in VI , and eT (x ) and hence pTjk(x ) are polynomials of degree M in x . We have, for convenience, chosen the xi axes to coincide with the principal axes of the ellipsoid; this can be done without loss of generality because a polynomial of degree M in xi remains a polynomial of degree M in the coordinates of any rectangular Cartesian system obtained by rotation and translation from other rectangular Cartesian system. T (x ) is the sum of M + 1 terms, with a typical r th term of the form In general, pkj Akjmn..,s xm xn . . . xs ,
20.7. Nonuniform Transformation Strain
347
where 0 ≤ r ≤ M and the Akjmn..,s xm xn . . . xs are r 2 constants, whereas xm xn . . . xs are r products. Consider such a term substituted into (20.53), namely the integral (r ) Ikj = Akjmn...s xm xn ...xs δ(z · x − z · x) dV , (20.55) VI
with 3 (xα /aα )2 ≤ 1.
(20.56)
α=1
Then, ∂uic 1 = ∂ xp 8π 2
−1 zp z j Mik (z) d
M r =0
(r )
∇x2 Ikj .
(20.57)
Now, introduce the change in variables tα = xα /aα , tα = xα /aα ,
(20.58)
which will convert the integral over the ellipsoid in (20.55) to an integral over the unit sphere, t  ≤ 1. When x lies within the ellipsoid, t ≤ 1 and (20.55) become
3
(r )
Ikj =
Akjαβ...γ aα aβ ...aγ (a1 a2 a3 )
t ≤1
α,β,...γ =1
tα tβ ...tγ δ[µ(s · t − s · t)] dV ,
(20.59)
where 1/2 µ = a12 z12 + a22 z22 + a32 z32 > 0, sα = zα aα /µ,
(no sum on α),
(20.60)
s = 1. The delta function in (20.59) is nonzero only for those t of the form t = T(m cos ψ + n sin ψ) + (s · t)s,
1/2 , 0 ≤ T ≤ 1 − (s · t)2
(20.61)
and m and n are any two ﬁxed unit vectors normal to s. The angle ψ is a polar angle in the plane of m and n. Thus, the volume integral in (20.59) is reduced to an integral over a plane circular region of radius [1 − (s · t)2 ]1/2 . Since δ(µf ) =
1 δ( f ), µ
(20.62)
we have (r )
Ikj =
a1 a2 a3 µ ×
3
2π
dψ 0
Akjαβ...γ aα aβ ...aγ
α,β,..,γ =1
0
[1−(s·t)2 ]1/2
[T Rα + (s · t)sα ] . . . [T Rγ + (s · t)sγ ]T dT.
(20.63)
348
20. The Inclusion Problem
In here, Rα = mα cos ψ + nα sin ψ,
(20.64)
and TdT is the polar element of area in the plane of integration. The integrand in (20.63) can be expanded using the binomial theorem and is of the form r r (w) T w+1 (s · t)r −w (20.65) fαβ...γ (ψ), w w=0 where
⎧ (0) ⎪ ⎪ ⎨ fαβ...γ (ψ) = sα sβ ...sγ , (1) fαβ...γ (ψ) = sα sβ ...Rγ + sα Rβ ...sγ + Rα sβ ...sα , ⎪ ⎪ ⎩ f (r ) (ψ) = R R ...R , α
αβ...γ
β
(20.66)
γ
(w)
i.e., each term in fαβ...γ (ψ) contains the product of w R s. Since
2π
sinm ψ cosn ψ dψ = 0,
if m + n is odd or if both m and n are odd,
0
one easily veriﬁes that
2π
0
(w)
fαβ...γ (ψ) dψ = 0,
if w is odd.
(20.67)
Thus, (r ) I jk
a1 a2 a3 = µ ×
2 r r Akjαβ...γ aα aβ ...aγ (s · t)r −2w 2w w=0 α,β,...γ =1 1
3
2π
(2w)
fαβ...γ (ψ) dψ
0
(20.68)
[1−(s·t)2 ]1/2
T 2w+1 dT, 0
where 12 r denotes the greatest integer not greater than 12 r . Since, from (20.58) and (20.61), s · t = z · x/µ,
(20.69)
and having in mind the fact that
[1−(s·t)2 ]1/2
T 2w+1 dT =
0
w+1 1 1 − (s · t)2 , 2(w + 1)
we obtain (r ) I jk
a1 a2 a3 = 2µ
2π 2 r r (2w) Akjαβ...γ aα aβ ...aγ fαβ...γ (ψ) dψ 2w 0 w=0 α,β,...γ =1
1 × w+1
3
z·w µ
1
r −2w " #w+1 z·x 2 . 1− µ
(20.70)
20.7. Nonuniform Transformation Strain
349
Clearly, each term in here is a polynomial in z · x of degree r − 2w + 2(w + 1) = r + 2. (r ) Thus I jk is a polynomial in xi of degree r + 2, and (r )
(r )
∇x2 I jk = Pjk (z · x),
(20.71)
(r )
where Pjk (z · x) is a polynomial of degree r in xi . Finally, M r =0
(r )
(M)
∇x2 I jk = F jk (z · x),
(20.72)
(M)
where F jk (z · x) is a polynomial of degree M in xi . Using (20.57) we immediately conclude that inside the ellipsoid the constrained elastic displacement gradients, and thus the strains and stresses, are polynomials in xi of degree M. The total elastic strain inside the ellipsoid is given by (20.57) and −eT (x), which is, of course, also a polynomial in xi of degree M. Thus the proposition of the lemma is proven. 20.7.1 The Cases M = 0, 1 The theorem will be illustrated for the cases where M = 0, 1. For M = 0, we have f (0) (ψ) = 1 and " # z·x 2 a1 a2 a3 (0) I jk = π . (20.73) Akj 1 − µ µ Now, ∇x2
z·x µ
2 = 2/µ2 ,
(20.74)
so that inside the inclusion # " −1 −1 (z z M + z z M ) a a a p j i j ik pk 1 2 3 d Akj = Si pkj Akj , eicp = 8π µ
(20.75)
where the Si pkj may be evaluated by simple numerical integration. For instance, using the fact that 1 −1 = isr r mn Msm Mr n /, = mns M1m M2n M2s , (20.76) Mik 2 we can use spherical coordinates z1 = cos φ cos θ,
z2 = sin φ sin θ,
z3 = cos φ.
(20.77)
When M = 1, in addition to the term in (20.75), we obtain a term corresponding to f (0) (ψ) = sα . Then, " 2 # 3 z · x z · x a1 a2 a3 (1) I jk = π Akjα zα aα2 . (20.78) 1− µ2 α=1 µ µ Since
∇x2
z·x µ
2 =6
z·x , µ3
(20.79)
350
20. The Inclusion Problem
in addition to the term in (20.75), we obtain a contribution " # −1 3 zp z j Mik + zi z j M−1 3a1 a2 a3 pk c 2 zs Akjα zα aα d xs . ei p = 8π µ5 α=1 The integrals may be easily evaluated by numerical integration.
20.8 Inclusions in Isotropic Media Eshelby’s (1957,1959) original development of the problem of an inclusion in a elastic medium contained insight and results of considerable interest for exploring physical phenomena. Here we present some of these. The general framework for this has already been presented and is accordingly utilized here. 20.8.1 Constrained Elastic Field Recall the expression derived for the Green’s function for an inﬁnitely extended isotropic elastic medium, viz., ∂2 1 λ+µ 2 (20.80) x − x . δkm∇ − Gkm(x − x ) = 8π µ λ + 2µ ∂ xk∂ xm Using the result ∇ 2 x − x  =
2 , x − x 
(20.81)
(20.80) may be rewritten as follows. The displacement at the point x due to a unit point force with components fi acting at the point x , is uˆ j (x − x ) =
fj 1 ∂2 1 − f x − x . 4π µ x − x  16π µ(1 − ν) ∂ x ∂ x j
(20.82)
The stress associated with the uniform transformation strain, eT , is σiTj = λeT δi j + 2µeiTj ,
(20.83)
where eT ≡ tr eT . The constrained elastic ﬁeld is constructed by applying traction σi j n j to the surface of the inclusion, i.e., (20.84) ucj (x) = σiTj uˆ j (x − x )nk dS , (no sum on j). S
The strain in the matrix and inclusion, if measured from the original, untransformed state, is eicj =
1 c (u + ucj,i ). 2 i, j
(20.85)
The stress in the matrix arises solely from this constrained ﬁeld and is given by σicj = λec δi j + 2µeicj .
(20.86)
σiIj = λ(ec − eT )δi j + 2µ(eicj − eiTj ).
(20.87)
The stress in the inclusion is
20.8. Inclusions in Isotropic Media
351
Because the σiTj are constant, and by applying the divergence theorem to (20.84), we obtain Eshelby’s result uic = where
1 1 T σ jk σ T φ, k , ψ, i jk − 16π µ(1 − ν) 4π µ ik
φ(x) = V
dV , x − x 
and
x − x  dV
ψ(x) =
(20.88)
(20.89)
V
are the Newtonian harmonic and biharmonic potentials, respectively; V is the volume of the inclusion. Note the fact that ∂/∂ x = −∂/∂ x has been used. Now, since φ(x) is the gravitational potential of a constant unit mass density in the volume V, we have −4π, inside V, (20.90) ∇ 2 φ(x) = 0, outside V. Furthermore, it is evident that ∇ 2 ψ(x) = 2φ(x), ∇ 4 ψ(x) = 2∇ 2 φ(x).
(20.91)
An interesting result follows immediately. Suppose we wish to know the dilatation, ui,c i . Since ψ, i jki = ψ, ii jk = ∇ 2 (ψ, jk) = 2φ, jk, we can construct ui,c i from (20.88) as ui,c i = ec = −
1 − 2ν σ T φ, ik. 8π µ(1 − ν) ik
Suppose further, as an example, that eT =
1 3
(20.92)
eT I. Then,
1 1+ν eT φ, i j , 4π 3(1 − ν)
(20.93)
1+ν eT = ζ eT . 3(1 − ν)
(20.94)
eicj = − and ec =
Thus, the factor ζ is a measure of the constraint of the matrix against free expansion of an inclusion. 20.8.2 Field in the Matrix The ﬁeld in the matrix is generally more difﬁcult to determine in a simple form. The Green’s function can be expressed as # " (xi − xi )(x j − x j ) fj 1 . (3 − 4ν)δi j + uˆ i (x − x ) = 16π µ(1 − ν) x − x  x − x 2
352
20. The Inclusion Problem x
l x' V
Figure 20.5. Field point in the matrix “far” from the inclusion.
r
Insert this into (20.84) and apply the divergence theorem to obtain uic (x) =
T σ jk
dV hi jk() r2
16π µ(1 − ν) V eTjk dV gi jk(), = 8π (1 − ν) V r 2
(20.95)
where r is the distance from x to x, and is a unit vector parallel to x − x , as shown in Fig. 20.5. Furthermore, hi jk = (1 − 2ν)(δi j k + δik j ) − δ jki + 3i j k, gi jk = (1 − 2ν)(δi j k + δik j − δ jki ) + 3i j k.
(20.96)
Suppose x is far removed from the inclusion. Then, we may remove everything from the integrand, except dV, to obtain T uic (x) ∼ Vσ jk hi jk
1 1 = VeTjk gi jk . 2 16π µ(1 − ν)r 8π (1 − ν)r 2
(20.97)
20.8.3 Field at the Interface Now once again the σiTj are constant, and thus ui,c =
1 1 σiTj ψ, i jk − σ T φ, k . 16π µ(1 − ν) 4π µ ik
(20.98)
Consider the jump in ui,c across the interface S of the inclusion. This involves [[ψ, i jk ]]
and
[[φ, k ]].
It is readily shown that [[φ, k ]] = ui,c (out) − ui,c (in) = 4πnkn .
(20.99)
It is left as an exercise to demonstrate this but the steps involve starting with the deﬁnition of φ and noting that the connection ∂/∂ xi = −∂/∂ xi can be used within the integral when forming a second derivative such as φ, k . Use of the divergence theorem, and a bit of elementary geometry, settles the proof. The same argument can be applied to ψ, i j , which is the potential obtained by using the density −2φ, i j /4π . Thus, [[ψ, i jk ]] = 8πni n j nkn .
(20.100)
20.8. Inclusions in Isotropic Media
353
Using the results such as (20.92), there follows 1 1 + ν T 1 − 2ν T e − e ni n j , 3 1−ν 1 − ν ij 1 c T T e T n j nkni n − eik ]] = nkn − ek nkni [[ei 1 − ν jk 1 − 2ν T 1 1+ν T 1 e n j nkδi − e ni n − δi , + 3(1 − ν) jk 3 1−ν 3 [[ec ]] = −
(20.101)
where ei Tj = eiTj − 13 eT δi j is a deviatoric part of the strain tensor. These are Eshelby’s results. Several aspects of the results should be noted. First, since both eicj and eiTj are related to σicj and σiTj by the isotropic elastic constitutive law given in (20.86), the relations in (20.101) are readily expressed in terms of the stresses. Second, by evaluating the elastic ﬁeld within the inclusion, the elastic ﬁeld just outside is known via (20.101). This allows for the determination of stress and strain concentrations at the interface. Third, and quite obviously, the result in (20.101) is available for [[ui,c ]] itself. This makes it useful for evaluating such quantities as surface forces, discussed earlier. Clearly, the strain energy density, W(e), at points on either side of the interface can be evaluated once the ﬁeld within the inclusion is known; this process is quite tractable for inclusions that are ellipsoidal in shape. 20.8.4 Isotropic Spherical Inclusion Eshelby lists his results for an isotropic spherical inclusion and we close by providing them below. One has ec = αeT ,
ei cj = βei Tj ,
1 1+ν , 3 1−ν
β=
(20.102)
with α=
2 4 − 5ν . 15 1 − ν
(20.103)
For a spherical inhomogeneous inclusion with elastic constants κ ∗ and µ∗ , subject to a far ﬁeld applied strain ei∞j , the equivalent transformation strain is given by eT = Ae∞ ,
ei Tj = Bei ∞ j ,
(20.104)
where A=
κ∗ − κ , (κ − κ ∗ )α − κ
µ∗ − µ . B= (µ − µ∗ )β − µ
(20.105)
Recall that κ = λ + 23 µ is a bulk modulus governing the relation between pressure and dilatation, i.e., σ = 3κe. Of particular interest is the ﬁeld that exists just outside the inclusion. The hydrostatic and deviatoric parts of the stress are readily found to be σ = σ∞ −
1+ν Bσi j∞ ni n j , 1−ν
(20.106)
354
20. The Inclusion Problem
and B σ ∞ n j nkni n 1 − ν jk 1 − 2ν 1 − 2ν 1 ∞ Bσ jk Aσ ∞ (ni n − δi ). + n j nkδi − 3(1 − ν) 3(1 − ν) 3
∞ ∞ σi = (1 + β B)σi ∞ − B(σik nkn + σk nkni ) +
(20.107)
A particularly interesting case of an inhomogeneous inclusion in an applied remote ﬁeld is that of a spherical cavity, where κ ∗ = 0 and µ∗ = 0. In that case (20.106) and (20.107) yield 15 ∞ ∞ ∞ nkn − σk nkni ) + σ jk n j nkni n σi = (1 − ν)(σi∞ − σik 7 − 5ν (20.108) 1 − 5ν ∞ ∞ σ (ni n − δi ) . − νσ jk n j nkδi + 10 An elementary check on Eshelby’s (1957) solution is to consider the case where the spherical cavity is subject to far ﬁeld hydrostatic tension of magnitude σ ∞ . Consider the hole’s surface, and note that the circumferential (hoop) normal stress, tangential to the hole is indeed 3 (20.109) σtt = σ ∞ , 2 where the subscript tt simply indicates a tangential direction to the hole’s surface. The hydrostatic tension is, of course, elevated in magnitude by the same factor of 3/2.
20.9 Suggested Reading Asaro, R. J., and Barnett, D. M. (1974), The NonUniform Transformation Strain Problem for an Anisotropic Ellipsoidal Inclusion, J. Mech. Phys. Solids, Vol. 23, pp. 77–83. Eshelby, J. D. (1957), The Determination of the Elastic Field of an Ellipsoidal Inclusion, and Related Problems, Proc. Roy. Soc. Lond. A, Vol. 241, pp. 376–396. Eshelby, J. D. (1961), Elastic Inclusions and Inhomogeneities. In Progress in Solid Mechanics (I. N. Sneddon and R. Hill, eds.), Vol. 2, pp. 87–140. Mura, T. (1987), Micromechanics of Defects in Solids, Martinus Nijhoff, Dordrecht, The Netherlands. NematNasser, S., and Hori, M. (1999), Micromechanics: Overall Properties of Heterogeneous Materials, 2nd ed., Elsevier, Amsterdam. Willis, J. R. (1964), Anisotropic Inclusion Problems, Q. J. Mech. Appl. Math., Vol. 17, pp. 157–174.
21 Forces and Energy in Elastic Systems
21.1 Free Energy and Mechanical Potential Energy Elasticity is concerned with the state of deformation, stress, and resulting energy in bodies subject to applied loads, displacements, or, as illustrated by the chapters on dislocations, incompatible or discontinuous displacements. For example, two such sources of stress in a body are indicated in Fig. 21.4 as S and A. Because of the presence of Aand S the internal energy and the Hemholtz free energy, i.e., the isothermal strain energy, are altered; in addition, the potential energy of external loading mechanisms responsible for traction, T, on the external surfaces, would have been altered as well. In considerations of equilibrium it is not enough to simply consider energy or free energy changes of the body itself, because changes in, say, defect conﬁguration or position cause changes in the potential energy of the external loading mechanisms. The thermodynamic potential that is appropriate to use to seek equilibrium states, or to construct forces from, therefore, must take both the energetic changes of the body and the loading mechanism into account. To begin, then, consider the socalled total energy, Etot = Eel + Eext ,
(21.1)
where Eel is the isothermal elastic energy, or Hemholtz free energy, and Eext is the potential energy of the loading mechanism. We now write a Gibbs equation for the change in this total energy of a body which is assumed to be at constant temperature and subject to ﬁxed loads (i.e., ﬁxed traction). The body is thus assumed to be surrounded by a medium that serves as a heat bath maintaining constant temperature, and a loading mechanism exerting constant boundary traction. The body and the surrounding medium are in thermal contact and can exchange heat; together they are thermally isolated from the remainder of the universe. We also consider an external source of work, Wext , that may do work on the body, but cannot exchange heat with either the body or medium (Fig. 21.1). The total change in internal energy of the body following an incremental process is Ti δui dS − T (0) δS(0) , (21.2) δU = δWext + S0
where we have explicitly noted the dual character of the medium. First, it serves as a heat bath and thus the heat given to the body is the heat it loses in a pure thermal transfer of 355
356
21. Forces and Energy
T
medium
body
So Figure 21.1. Adiabatically isolated body and medium. The traction vector is T and the temperature is T.
T
W ext heat; this means that the heat lost to the body is just −T (0) δS(0) . The absolute temperature is T, and S the entropy. The superscript 0 pertains to the medium, unscripted variables in context pertain to the body, and we recall that T = T (0) . The integral accounts for the other role of the medium as a loading mechanism capable of performing mechanical work on the body. As the body plus medium together comprise a thermally isolated system, the second law of thermodynamics states that δS + δS(0) ≥ 0,
(21.3)
−T (0) δS(0) ≤ T (0) δS,
(21.4)
because δSext = 0. Thus,
and
δU ≤ δWext +
Ti δui dS + TδS,
(21.5)
S0
or, since S = S0 ,
δWext ≥ δU − TδS −
Ti δui dS.
(21.6)
S
The work that must be performed externally by the external “engine” to produce this change in state is δWext . When the change occurs reversibly, the equality holds and (21.7) δWext = δ − Ti δui dS, δ = δU − TδS . rev
S
The Helmholtz free energy δ contains the “locked in” elastic strain energy within the body, whereas the surface integral describes the work effects associated with the external loading mechanism. It is common to deﬁne the potential energy of the body as WdV − T · u dS, (21.8) %= V
S
where W is the strain energy density, and we seek the conﬁguration, under a given set of boundary conditions, that minimizes it. This will be a solution technique we will use in later
21.2. Forces of Translation
357
sections. Thus, at equilibrium, % is a minimum. Generalized forces acting on the system can be thereby deﬁned as fα = −
∂% ∂Etot =− , ∂ξα ∂ξα
(21.9)
where α represents a generalized displacement such as the movement of a defect like dislocation or the deﬂection of a plate under prescribed loading.
21.2 Forces of Translation The objective here is to calculate the force acting on a defect, for example, a crack tip, from the formalism described above. Thus, we want the force inducing translation, which is f = −
∂Etot . ∂ x
(21.10)
We calculate the energy change in two parts. First consider the elastic energy change. As the defect translates a small distance in the x direction, it “drags along with it” its elastic ﬁeld. After the translation, the ﬁeld quantities are given as ui (x j ) = ui (x j − δ j ), σij (xk) = σi j (xk − δk ),
(21.11)
where the superscript denotes the quantities after the translation. The strain energy density is, accordingly, 1 1 σ (xk)eij (xk) = σi j (xk − δk )ei j (xk − δk ). 2 ij 2 We can expand W , excluding regions of singularity, as W =
1 {[σi j (xk) − σi j, (xk)][ei j (xk) − ei j, (xk)]} + O( 2 ) 2 1 1 = σi j ei j − (σi j ei j ), + O( 2 ) 2 2
(21.12)
W =
(21.13)
= W − W, + O( 2 ). Therefore, the energy change in this ﬁrst step is (1) δEel = (W − W) dV = − W, dV + O( 2 ).
(21.14)
The divergence theorem may be used to obtain, to ﬁrst order in , (1) δEel = − Wn dS.
(21.15)
V
V
S
Now, by simply translating the elastic ﬁeld, a state of stress within the body will be created that does not satisfy the boundary conditions. That is, on a boundary with unit normal n, we have σij n j = (σi j − σi j, )n j + O( 2 ).
(21.16)
Step 2: then involves applying a traction σi j, n j + O( 2 ) = O() to annul the error. At the end of step 1 the surface displacements are ui − ui, + O( 2 ), and after step 2 they
358
21. Forces and Energy
attain the values ui (ﬁnal), which of course is unknown. Therefore, the change in elastic energy during step 2 is (2) (21.17) δEel = σi j [ui (ﬁnal) − ui + ui, ]n j dS + O( 2 ). S
The difference [ui (ﬁnal) − ui ] is of O(), because the set of tractions imposed in step 2 is of O(). We now consider the change in energy associated with the loading mechanism. To ﬁrst order in , this is (21.18) δEext = − σi j [ui (ﬁnal) − ui ]n j dS + O( 2 ), S
and thus (1)
(2)
δEtot = δEel + δEel + δEext = − (Wn − σi j ui, n j ) dS,
(21.19)
S
where conveniently the unknown quantity, [ui (ﬁnal) − ui ], drops out! Therefore, appealing to the deﬁnition of force in (21.10), we ﬁnd that f = (Wn − σi j ui, n j ) dS.
(21.20)
S
This may be rephrased as f =
(Wδ j − σi j ui, )n j dS.
(21.21)
S
The generalized force developed here is often called the J integral (Rice, 1968a, 1968b). The tensor P j = Wδ j − σi j ui,
(21.22)
is called the energy momentum tensor (Eshelby, 1956). Thus, f = P j n j dS, f = n · P dS. S
(21.23)
S
It is a rather straightforward exercise to show that the divergence of P is zero, that is (Wδ j − σi j ui, ), j = 0.
(21.24)
Thus, if S and S are two surfaces that surround the defect s, enclosing a volume V (Fig. 21.2), it is found that div P dV = 0 = n · P dS + n · P dS . (21.25) V
S
S
Therefore, since n = −n,
n · P dS = S
S
n · P dS .
(21.26)
Thus, the value of the generalized force on a defect does not depend on the choice of surface S surrounding the defect used to evaluate the integral in (21.21).
21.2. Forces of Translation
V'
359
n S
n' s
Figure 21.2. Path independence of the energy momentum tensor, or J integral. A defect labeled s is indicated as surrounded by S and S .
S'
21.2.1 Force on an Interface Eshelby has extended the above development of a translational force on a defect to the consideration of a force acting on an interface. Consider the interface between two phases α and β. The surface element is to move by an incremental vector, δξ. For example, this may represent the result of a phase transformation β → α, where the transformation involves a change in size and shape of the material. Such problems are dealt with in detail in subsequent chapters, but for now we want to consider the possibility that due to such discontinuities in displacement, induced by a transformation, there may be net mechanical forces on the interface between the two phases.The described total energy change can be computed using the two heuristic steps, as described earlier. First, cut out the material lying between the old surface element, S, and the new element, S , and discard the material. We imagine that suitable tractions are applied to the freshly cut surface to prevent relaxation. This results in a change in elastic energy, (1)α (21.27) δEel = − δξ Wα n dS. S
The direction of the unit normal n is taken as pointing from β → α. At this stage the fα α . Now, alter the displacements to their ﬁnal value, ui . displacement on S is uiα + δξ ui, The work required to do this is fα (2)α α δE = − σiαj (ui − uiα − δξ ui, )n j dS. (21.28) S
For phase β, similar arguments lead to (1)β δEel
and
δE
(2)β
S
(21.29)
S
β
=−
δξ Wβ n dS,
=
fβ
β
β
σi j (ui − ui − δξ ui, )n j dS. fα
(21.30) β
But during this process of interface motion, ui − uiα = ui − ui , so that β δEtot = − n j (P αj − P j )δξ dS. fβ
(21.31)
S
Thus, the force on the interface becomes αβ f = n j [[P j ]] dS. S
(21.32)
360
21. Forces and Energy α n
β
S'
S ξ
Figure 21.3. Moving interface.
αβ
If we form f n , we can deﬁne F = [[W]] − T · [[∂u/∂n]],
(21.33)
as the normal force per unit area acting on the interface. This result should be extended in two obvious ways. In the ﬁrst place, the energy considered so far has only included the elastic energy of deformation. If, however, the interface is one between two phases undergoing the transformation α → β, then the chemical part of the free energy change needs to be included. This would add a contribution to the free energy change δξ (Gβ − Gα )n dS = − δξ [[G]]n dS. (21.34) S
S
The second contribution to the total energy change is that due to the surface energy, γ , per unit area. This contributes a term δξ κn γ n dS, (21.35) S
where κ is the double mean curvature of the surface. Note that this curvature is measured positive for a surface as seen from the α side in Fig. 21.3, i.e., where the radii of curvature are constructed on the α side. Including these two effects yields for the total normal force on the interface F = [[W]] − T · [[∂u/∂n]] − κγ ,
(21.36)
where W = W + G. With the sense of the curvature as taken here, the surface energy term induces a retarding effect on interface motion if κ > 0, i.e., if additional surface area is created by forward motion.
21.2.2 Finite Deformation Energy Momentum Tensor The energy momentum tensor also exists for ﬁnite elastic deformations, and has similar form to that derived for the inﬁnitesimal strain case. The development was originally also due to Eshelby (1970,1975). Recall that the position of a material particle in the deformed conﬁguration, x, is given in terms of its position in the reference conﬁguration by x(X) = X + u(X).
(21.37)
In component form this gives for the displacement ui (Xm) = xi (Xm) − Xi .
(21.38)
21.2. Forces of Translation
361
The equilibrium equations with respect to the nominal stress, P, and without body forces, are ∂ Pi j = 0. (21.39) ∂ Xj Denoting the strain energy density per unit reference volume by W, we have W = W(Grad u, X), and Pi j =
∂W . ∂ui, j
(21.40)
Recall that P is not symmetric, but satisﬁes Pi − Pj = Pji u,i − Pi u j,i .
(21.41)
The energy momentum tensor is derived by considering the set of ﬁeld equations that result from causing the ratio of the current volume and reference volume to be stationary (extreme). This gives ∂ ∂W ∂W = , ∂ Xj ∂ui, j ∂ui
(21.42)
with W = W(ui , ui, j , Xi ). Consider the gradient of W with components ∂ W/∂ X , and then the partial derivative of W holding the displacements and displacement gradients ﬁxed, i.e., ∂W ∂W = . (21.43) ∂ X exp ∂ X ui ,ui, j ,Xm = If the material were homogeneous and free of singularities or dislocations, then ∂W = 0. ∂ X exp But now we have ∂W ∂W ∂W = ui, + ui, j + ∂ X ∂ui ∂ui, j
∂W ∂ X
(21.44)
.
(21.45)
exp
When (21.42) is used to replace ∂ W/∂ui with ∂(∂ W/∂ui, j )/∂ Xj , the ﬁrst two terms on the r hs of (21.45) become ∂ ∂W ui, . ∂ Xj ∂ui, j Thus, since formally ∂ W/∂ Xi = ∂(Wδi j )/∂ Xj , we can write ∂P j ∂W = , ∂ Xj ∂ X exp
(21.46)
where P j = Wδ j −
∂W ui, ∂ui, j
(21.47)
is the energy momentum tensor. Also, because of (21.40), we have P j = Wδ j − Pi j ui, .
(21.48)
362
21. Forces and Energy
A
n
II I
n
s
Σ Figure 21.4. Two sources of stress, labeled A and S, in an elastic medium.
Σο
The integral deﬁned by
F =
P j n j dS,
(21.49)
S ∂W is equal to zero if S encloses a volume in which ∂u ui, = 0, i.e., one that is homogeneous i, j and free of defects. The argument shows that, in the case that S does enclose a defect, i.e., a singularity or displacement discontinuity, the integral given in (21.49) represents the force of translation acting on the defect. The proof follows the same route as detailed in the previous section.
21.3 Interaction Between Defects and Loading Mechanisms We return to the general situation of two sources of stress that are called A and S in Fig. 21.4. As noted earlier, for internal sources of stress such as dislocations or inclusions, the elastic ﬁelds are caused by discontinuous displacement ﬁelds, but even in those cases the stresses and strains are continuous. Since linear superposition applies, the total ﬁeld is the sum of the ﬁelds due to all sources, i.e., σi j = σiAj + σiSj ,
ei j = eiAj + eiSj .
(21.50)
Equilibrium applies to each ﬁeld separately, so that σiAj, j = σiSj, j = 0. The total elastic energy is then 1 (σ A + σiSj )(eiAj + eiSj ) dV Eel = 2 V ij 1 1 1 σiAj eiAj dV + σiSj eiSj dV + (σ A eS + σiSj eiAj ) dV = 2 V 2 V 2 V ij ij
(21.51)
(21.52)
A−S = EsA + EsS + Eint .
Here, EsA and EsS are “selfenergies” of the A and S systems, as if they were isolated, A−S is the interaction energy of the two sources. Clearly, all forces that these two and Eint A−S , which we examine now. The systems are to exert on each other derive from Eint interaction energy is 1 A−S (σ A eS + σiSj eiAj ) dV. (21.53) Eint = 2 V ij ij
21.3. Interaction Between Defects and Loading Mechanisms
363
In general, we expect that uA and/or uS may be discontinuous. Since σi j = Ci jkl ekl , we can write A S A ei j = σiAj eiSj = σklS ekl , Ci jkl ekl
(21.54)
because of the symmetry Ci jkl = Ckli j . Thus, the two terms in the integrand of (21.53) are equal. Now construct a surface, (0 , surrounding S such that outside this surface uS is continuous. Then, we may rewrite (21.53) as A−S S A σiAj eiSj dV, (21.55) Eint = σi j ei j dV + I
II
where, as seen in Fig. 21.4, I and I I are the two volume elements so formed by the separator (0 . Recognizing that the integrands of (21.55) can be put into the form σi j ui, j = (σi j ui ), j , because of the equilibrium stated in (21.51), the application of the divergence theorem leads to S A σi j ei j dV = σiSj n j uiA dS,
I
II
σiAj eiSj dV =
(0
(
σiAj nˆ j uiS dS −
(0
(21.56) σiAj n j uiS dS.
ˆ and the minus sign of the last integral The outward pointing normal to the surface ( is n, appears because the outward pointing normal on (0 from volume I has been used in the integrand. The nature of ( will be deﬁned by application to speciﬁc examples below. For now, we ﬁnd that A−S S A A S (σi j n j ui − σi j n j ui ) dS + σiAj nˆ j uiS dS. (21.57) Eint = (0
(
Suppose that A is an internal source of stress, so that on (, which is now taken as the external surface of the body containing A and S, σiAj nˆ j = 0. Then, not only is the last integral in (21.57) zero, but the integral that would be associated with the potential energy of the external loading mechanism, as well. Thus, we obtain that A−S (σiSj uiA − σiAj uiS ) n j dS (21.58) Eint = Etot = (0
is the total energy of interaction between A and S. A−S Now let A be an external source of stress, so that σiAj nˆ j = 0. Then, to Eint we add the potential energy associated with the loading mechanism, i.e., TiA uiS dS = − σiAj nˆ j uiS dS, (21.59) − (
(
and arrive again at the conclusion that the total interaction energy is given by A−S = Etot = (σiSj uiA − σiAj uiS ) n j dS. Eint (0
(21.60)
Furthermore, in this case we can let (0 → ( and, since S is an internal source of stress so that σiSj nˆ j = 0, we have A−S Eint = Etot = − σiAj nˆ j uiS dS. (21.61) (
364
21. Forces and Energy n
x2
I
λ
D I
Σ
Σο
nI
II
Figure 21.5. Dislocation and inclusion.
x 1
21.3.1 Interaction Between Dislocations and Inclusions Consider the interaction of an inﬁnitely long and straight dislocation line and an inclusion. The stress ﬁeld σiIj of an inclusion vanishes with distance from it as 1/r 3 . Let superscripts I and D denote ﬁeld quantities associated with the inclusion and dislocation, respectively. The interaction energy is then 1 I−D = (σ I uD + σiDj ui,I j ) dV. (21.62) Eint 2 V i j i, j The reciprocity σiIj ui,Dj = σiDj ui,I j within the above integrand is observed, as before. The total volume is divided via the construction of a surface (0 made so that in the two volume elements so created one or the other of uI or uD is continuous (Fig. 21.5). Then, I−D D I σiIj ui,Dj dV Eint = σi j ui, j dV +
I
= =
I
II
(σiDj uiI ), j dV +
(0
σiDj nIj uiI dS −
II
(0
(σiIj uiD ), j dV
(21.63)
σiIj nIj uiD dS +
(
σiIj uiD n j dS.
We note that the outer surface of region II may be taken as the free surface of the body (at least as far as the inclusion’s stress ﬁeld is concerned). Moreover, we may ﬁrst choose the halfplane deﬁned by x2 = 0 and x1 ≥ 0 as the cut surface of the dislocation, Scut , and let (0 → Scut . The displacement ﬁeld of the inclusion is continuous across (0 and so is the stress ﬁeld of the dislocation. We note that on (0 , σiDj n+j = −σiDj n−j , where the normals are deﬁned in the ﬁgure; thus along those parts of (0 called (0+ and (0− the combined integrals cancel. Now, around the loop of vanishing radius , the displacement of the inclusion is uniquely deﬁned, and σiDj n j dS = 0, (21.64)
because this would be, in fact, just the total content of body force at that point, which is zero for the dislocation. Thus, the total contribution to the interaction energy is D(+) D(−) I−D I D I dS σi j ui n j dS = − σiIj n+j ui − ui Eint = − =
(0
(0
σiIj n+j bi dS.
(0
(21.65)
21.3. Interaction Between Defects and Loading Mechanisms
365
t
ds
δn Figure 21.6. Dislocation segment movement.
dS
To calculate a force from this interaction energy we ﬁrst consider this integral per unit length normal to the plane of the ﬁgure, and write ∞ ∞ D(+) D(−) I−D I + Eint = − dS = σi j n j ui − ui σiIj n+j bi dS. (21.66) λ
λ
It follows that fλ = −
I−D ∂Eint = σiIj (λ)n+j bi . ∂λ
(21.67)
The normal n+ is nI oriented upward. This result can be generalized in terms of the force acting on an arbitrary segment of curved dislocation, which is discussed next.
21.3.2 Force on a Dislocation Segment The above result can be used to readily generate an expression for the force on an arbitrary segment of dislocation. Consider a segment of dislocation depicted in Fig. 21.6. The dislocation is acted on by a stress ﬁeld labeled A. Let the arc length of this segment be initially ds and let it move by the normal vector distance δn, thus traversing the planar ˆ we have element dS. In terms of the force acting on this segment, f, −δEtot = fˆ · δn = −σiAj bi δS j ,
(21.68)
where dS j = η j dS, and η would be the unit normal to the area element traversed. But, δS j = (δn × ds) j + O(κδn2 ),
ds = tds,
(21.69)
where κ is the curvature at the point in question on the segment, and t is the unit tangent to the loop at the point of the segment. Thus, dS j = jkl dsl δnk = jkl tl δnkds.
(21.70)
fkδnk = −σiAj bi jkl tl δnk,
(21.71)
Consequently,
where fk = fˆk/ds. Therefore, the force per unit length of dislocation segment is fk = jlkσiAj bi tl . This is called the Peach–Koehler force.
(21.72)
366
21. Forces and Energy
r no
n S+ cut
ϕ
Figure 21.7. Dislocation cut surface and integration path.
So
n+
S cut S
n
21.4 Elastic Energy of a Dislocation Consider an inﬁnitely long and straight dislocation indicated in Fig. 21.7. Per unit length, the elastic energy can be written as 1 σi j ei j dV E= 2 V 1 1 (21.73) = σi j ui, j dV = (σi j ui ), j dV 2 V 2 V 1 σi j ui n j dS, = 2 S where S is the surface that bounds the total volume V and is constructed so that the dislocation’s displacement ﬁeld is single valued within V. This is illustrated in the ﬁgure, where the outward pointing normal, n, to S is also shown. Now, the integrals are divided as 1 1 1 σi j ui n j dS + σi j ui n j dS + σi j ui n j dS. (21.74) E= ± 2 Scut 2 S∞ 2 S0 Considering the angle ϕ, we note that σi j = (i j (ϕ)/r, n j = n j (ϕ) and thus Ti = σi j n j = hi (ϕ)/r . As there are no body forces, we have 2π hi (ϕ) dϕ = 0. (21.75) 0
However,
2π
ui (ϕ) dϕ = bi .
(21.76)
0
The second two integrals cancel, because dS = r dϕ, and hi∞ = −hi0 (the directions of the outward pointing normals are opposite). The integrals left on Scut become 1 1 σi j n±j ui± dS = σi j n−j (ui− − ui+ ) dS E= ± 2 Scut 2 S (21.77) 1 − = σi j n j bi dS, 2 S where we have used n− to describe the normal and b = u− − u+ . Since again σi j = (i j (ϕ)/r , this can be rewritten as 1 ∞ (i2 (0)bi dx1 . (21.78) E= 2 0 x1
21.5. InPlane Stresses
367
Note from the geometry that n x2 . The integral is logarithmicaly singular and we introduce the socalled cutoff radii, r0 and R, to write 1 E= 2
R
r0
(i2 (0)bi 1 dx1 = (i2 (0)bi ln(R/r0 ). x1 2
(21.79)
Recalling that (i2 ∝ Ki j b j , (21.79) may be rewritten as E = Ki j bi b j ln(R/r0 ).
(21.80)
For the inﬁnitely long and straight screw dislocation in an isotropic medium, our previous results show that Gbs2 ln(R/r0 ), 4π
(21.81)
Gbe2 ln(R/r0 ). 4π (1 − ν)
(21.82)
Escrew = whereas for the edge dislocation Eedge =
For an inﬁnitely long and straight dislocation with t x3 and b = be e1 + be e2 + bs e3 , we ﬁnd ⎞ ⎛ b /(1 − ν) 0 0 G ⎝ e (21.83) K= 0 be /(1 − ν) 0 ⎠ 4π 0 0 bs
21.5 InPlane Stresses of Straight Dislocation Lines The energy factor matrix introduced in the previous section, K, has an interesting and useful connection to the traction caused by a dislocation in planes that contain the dislocation line. We explore that connection herein. Recall two expressions for the energy of a straight dislocation line, i.e., E = Ki j bi b j ln(R/r0 ), and 1 E= 2
σi j ui, j V
1 dV = 2 1 = 2
(21.84)
σi j ui dS
S R
r0
1 σi j n j bi dS = 2
R
(21.85) σi j n j bi dx1 .
r0
In (21.85) the cut has been taken along the x1 axis, that is on the plane where x2 = 0; the dislocation is lying along the x3 axis. Consider a dislocation with a Burgers vector with a nonzero component b1 (b2 = b3 = 0). From (21.84) then R K11 b1 b1 dx1 . (21.86) E = K11 b1 b1 ln(R/r0 ) = x1 r0
368
21. Forces and Energy
But, from (21.85), the energy is also given as 1 R (1) 1 R (1) E= σi j n j bi dx1 = σ b1 dx1 , 2 r0 2 r0 12
(21.87)
(1)
where σ12 is the stress component in the plane x2 = 0 caused by the dislocation with Burgers vector b1 . When (21.87) is compared to (21.86), we ﬁnd that (1)
σ12 =
2K11 b1 . x1
(21.88)
Similarly, we ﬁnd that for a dislocation with Burgers vector b2 (b1 = b3 = 0), (2)
σ22 =
2K22 b2 , x1
(21.89)
(2)
where σ22 is the stress component on the plane x2 = 0 caused by the dislocation with Burgers vector b2 . Finally, if the Burgers vector had only a nonzero component b3 , we would ﬁnd that (3)
σ23 =
2K33 b3 . x1
(21.90)
Note that the above results were arrived at by considering the selfenergy of individual dislocations with single nonzero components of Burgers vector. Now consider interaction effects between two dislocations or between the stresses arising from different components of Burgers vector of a single dislocation. Let a dislocation line be again along the x3 axis, but with a Burgers vector b = b1 e1 + b2 e2 . From (21.84), the energy is E = Ki j bi b j ln(R/r0 ) = K11 b1 b1 ln(R/r0 ) + K22 b2 b2 ln(R/r0 ) + (K12 b1 b2 + K21 b2 b1 ) ln(R/r0 ).
(21.91)
Since K12 = K21 , this becomes E = Ki j bi b j ln(R/r0 ) = K11 b1 b1 ln(R/r0 ) + K22 b2 b2 ln(R/r0 ) + 2K12 b1 b2 ln(R/r0 ). (21.92) Alternatively, we could write that this energy is 1 R σi j n j bi dx1 E= 2 r0 1 R (1) (2) σi j n j + σi j n j bi dx1 = 2 r0 1 R (1) (1) (2) (2) σ12 b1 + σ22 b2 + σ12 b1 + σ22 b2 dx1 . = 2 r0 (1)
(2)
(21.93)
Comparing (21.93) with (21.92), having in mind that σ12 and σ22 are already known, we ﬁnd that R 2K12 b1 b2 1 R (1) (2) σ22 b2 + σ12 b1 dx1 = dx1 . (21.94) 2 r0 x1 r0
21.6. Chemical Potential
369
x 2 T n Figure 21.8. Arbitrary cut surface.
λ
x 1
(1)
(2)
Furthermore, the reciprocity σ22 b2 = σ12 b1 holds. To see this, write 1 1 (1) (2) (2) (1) σi j ei j dV = σ e dV 2 V 2 V ij ij 1 1 (1) (2) (1) (2) = σi j ui, j dV = σ n j bi dS 2 V 2 S ij 1 R (1) (2) 1 (2) (1) = σ b dx1 = σ u dV 2 r0 22 2 2 V i j i, j 1 R (2) (1) σ b dx1 . = 2 r0 12 1
(21.95)
Hence, we ﬁnd that (2)
σ12 = (1) σ22
2K12 b2 , x1
2K21 b1 = . x1
(21.96)
In general, we obtain by using this kind of analysis that σi2 =
2Kis bs . x1
(21.97)
It should be noted at this point that our arguments and procedures would be true for any cut plane that contains the dislocation line, and that could have been used to calculate the energy. Thus, for any plane containing the dislocation line, and with λ as the distance from that line, σi j n j = Ti =
Kis bs , λ
(21.98)
i.e., the traction is the same on any plane containing the dislocation line (Fig. 21.8).
21.6 Chemical Potential The chemical potential is deﬁned as the differential change in Gibbs free energy with respect to the addition of a unit amount of a chemical specie, or in the case considered here, of matter. We wish to speciﬁcally evaluate the inﬂuence of stress and elastic strain state on that quantity. Thus we consider the addition of a small amount of material to the surface of a stressed body.
370
21. Forces and Energy
Consider the potential of two states, 1 and 2, before and after the addition of matter. We have (1) (1) (1) W(ei j )dV − Ti ui dS, %1 = (1
V1
%2 =
V2
(2) W(ei j )dV
−
(1
(21.99) (2) (2) Ti ui
dS.
The system is to act at constant temperature and state of applied traction on its external surface. The latter constraint sets T(1) = T(2) . Thus, considering the change in potential, %2 − %1 , the surface integrals of (21.99) contribute (1) (1) (2) (2) (1) (2) (1) (1) (2) (1) Ti ui dS − Ti ui dS = − Ti [ui − ui ] dS − Ti [ui − ui ] dS, (1
(2
(1
(
where ( is the increment of surface area to which matter was added. Naturally, if ( should lie on a traction free part of the surface, the last integral would vanish. Next, focus attention on an inﬁnitesimal volume element at the site of (; in state 1 it is v1 and in state 2 it is v2 . The goal is to let v2 − v1 → 0. Then, (2) ¯ i(2) ) dV + W(ei j ) dV %2 − %1 = W(e j v2
(1)
¯ ij ) − W(e +
(1
Ti
(1)
V2 −v2
v1
dV −
(1) [ui
−
(1)
V1 −v1
(2) ui ] dS
W(ei j ) dV
−
(1)
(
(21.100) (2)
(1)
Ti [ui − ui ] dS,
(1,2)
¯ i j ) is the mean value of strain energy density in these vanishingly small volume where W(e elements. But, after combining terms, (21.100) is equivalent to ¯ i(1) %2 − %1 = W(e j )(v2 − v1 ) +
'
(1) [σi j
(2) ei j
V2
(
(1)
ei j
− σi j ]dei j dV −
(1)
(
(2)
(1)
Ti [ui − ui ] dS, (21.101)
or, by using the divergence theorem, to ¯ i(1) %2 − %1 = W(e j )(v2 − v1 ) +
'
[Ti
(2) ui
(
(1)
(
(1)
ui
− Ti ]dui dS −
(1)
(
(2)
(1)
Ti [ui − ui ] dS. (21.102)
The result may be rewritten as ¯ i(1) %2 − %1 = W(e j )(v2 − v1 ) + ¯ i(1) = W(e j )(v2 − v1 ) +
'
(2) ei j
v2 −v1
(1) ei j (2)
ei j
(1)
ei j
(1)
( (1) [σi j − σi j ]dei j dV −
[σi j − σi j ] dei j −
(1)
(
(2)
(1)
(21.103)
(1)
(
(2)
(1)
Ti [ui − ui ] dS.
But (2)
(1)
Ti [ui − ui ] dS
[ui − ui ] dS = (v2 − v1 )ni dS,
21.6. Chemical Potential
371
h
n Σ
Figure 21.9. Movement of an internal source of stress by the removal and addition of matter to the external surface.
defect
because the change in volume on the surface is (2)
(1)
v2 − v1 = [ui − ui ]ni dS,
(21.104)
where n is the unit normal on (. Now, divide by v2 − v1 and let v2 − v1 → 0. The integral over strain vanishes as the two states merge, and ∂% (1) = W(ei j ) − Tn(1) , ∂v
(21.105)
(1)
where Tn is the normal traction at the point on the surface where mass is added, i.e., (1) (1) Tn = Ti ni . Therefore, we have deduced that the chemical potential is µ = W(e) − Tn .
(21.106)
21.6.1 Force on a Defect due to a Free Surface Consider a purely internal source of stress, such as a defect within a body whose external surface is traction free, as depicted in Fig. 21.9. If the surface did have applied traction, then by ignoring it we would be calculating only that contribution to the total force arising from the free surface. This is the socalled image force. From the energy momentum tensor, this force would be calculated from the integral (21.107) J = (Wn − σi j n j ∂ui /∂ x ) dS. C
Now take the contour C to be (, the external surface of the body. On ( we have σi j n j = 0, and hence W(e)n dS. (21.108) J = (
The movement of such an internal source of stress could be accomplished by imagining a process of mass removal and addition to the external surface as illustrated in the ﬁgure. In particular, if mass is removed in the direction x from the surface element whose outward pointing normal is n, and if the distance along x where mass is removed is h, then the change in free energy is, by using (21.106), h W(ei j )n dS dh. (21.109) % = − 0
(
Thus, the “force” on the defect can be constructed as f = −∂%/∂h = W(ei j )n dS, (
which reproduces the result obtained from the energy momentum tensor.
(21.110)
372
21. Forces and Energy
c
d
a C' b g
j
C1
Figure 21.10. Crack in a strip clamped at its upper and lower edges and subject to extension normal to the crack line.
h e
f
21.7 Applications of the J Integral Here we present some applications of the J integral to calculate the force on particular defects in solid bodies. 21.7.1 Force on a Clamped Crack Consider a crack in a strip, shown in Fig. 21.10, that is loaded via the action of applying a displacement to the upper and lower surfaces, i.e., the surfaces along the lines cd and ef are displaced away from each other by a distance δ. As the original height of the strip is h, this action produces a strain e = δ/ h. The force acting on the crack tip would be computed by evaluating J1 along the contour C1 (axis x1 being parallel to crack faces). Path independence, however, allows the alternate evaluation of J1 along the contour C . This is rather straightforward in this case. First, note that along the paths bc and fg, the stresses vanish, as does the strain energy density and the traction; thus, there is no contribution from these segments. Next, along the paths cd and ef, the normal is orthogonal to the direction of propagation of the crack and the displacement is conﬁned by the rigid clamp such that ui,1 vanishes; thus, there is no contribution from these segments, either. Finally, along the segment de, the strain energy density is given, assuming a state of plane stress, as 2 δ E . (21.111) W= 2(1 − ν 2 ) h Integration of this along the segment de gives 2 Eh δ , W dy = 2(1 − ν 2 ) h
(21.112)
which is the only contribution to the total contour integral. Thus, we obtain J1 =
δ2 E . 2 2(1 − ν ) h
(21.113)
21.7.2 Application of the Interface Force to Precipitation As an application of the concept of a force on an interface, consider the case of the precipitation of a second phase particle within an elastic matrix. We idealize the situation by ignoring any inelastic deformation, i.e., dislocation activity. Further, let this process occur in an inﬁnite matrix (the parent phase) under the inﬂuence of a remotely applied hydrostatic stress state of intensity σ∞ . The process is driven (that is, if it is spontaneous) by the combination of a negative change in the chemical part of the Gibbs free energy, G < 0, and the interaction energy between the remotely applied stress ﬁeld and the transformation
21.7. J Integral
373
σ
r
σ
Figure 21.11. Formation of a critical nucleus and growing precipitate in an elastic matrix.
σ
strain associated with the phase change. Here we assume that the transformation strain is purely dilatational, i.e., eiTj =
1 T e δi j . 3
(21.114)
Of course, it is possible that, even if G > 0, the transformation may be driven forward by an intense enough remote stress, and this is conventionally mapped on “pressure vs. temperature” phase diagram for single component systems. As the phase forms, an elastic ﬁeld is created along with its energy. This problem was dealt with in great detail in previous chapter and will not be included here. The results are only used. Speciﬁcally, we consider the precipitate to be spherical and of radius r (Fig. 21.11). The solution for the elastic ﬁeld can be determined by the methods developed in Chapter 20. The matrix and precipitate are considered to be isotropic in their elastic properties and of the same modulus. With this in mind, the normal interface force from (21.36) becomes F = −G −
2 E ( T )2 + T σ∞ − γ , 9(1 − ν) r
(21.115)
where γ is the surface energy of the α/β interface. Of course, for growth we must have F > 0, or, more speciﬁcally, −G + T σ∞ >
E (T )2 . 9(1 − ν)
(21.116)
We note that, even if (21.116) were satisﬁed, there is the nucleation problem to face, because if γ is signiﬁcant in magnitude, the surface energy term dominates (in a negative way) for small values of r ; that is, we must acquire a nucleus of critical size, r ∗ . This is readily attained by setting F = 0 in (21.115), which yields r ∗ (T) =
2γ . −G − E/[9(1 − ν)](T )2 + T σ∞
(21.117)
We have explicitly noted the very important temperature dependence of the process, coming most strongly through the term involving G, and more weakly through the
374
21. Forces and Energy
temperature dependence of E, ν, T , and γ . Now, if r < r ∗ , the nucleus is unstable and the work done on the system to attain the nucleus of radius r > r ∗ is r∗ G∗ = − 4πr 2 F dr. (21.118) 0
In (21.118) we have employed the often used nomenclature G∗ to denote the magnitude of the activation energy of nucleation. This energy arises through statistical ﬂuctuations and is of paramount importance with respect to the kinetics of the nucleation process. The evaluation of (21.118) for particular cases is left to the reader’s interest.
21.8 Suggested Reading Eshelby, J. D. (1951), The Force on an Elastic Singularity, Phil. Trans. R. Soc. A, Vol. 244, pp. 87–112. Eshelby, J. D. (1956), The Continuum Theory of Lattice Defects. In Solid State Physics (F. Seitz and D. Turnbull, eds.), Vol. 3, Academic Press, New York, pp. 79–144. Eshelby, J. D. (1970), Energy Relations and the EnergyMomentum Tensor in Continuum Mechanics. In Inelastic Behavior of Solids (M. F. Kanninen, W. F. Adier, A. R. Rosenﬁeld, and R. I. Janee, eds.), pp. 77–115, McGrawHill, New York. Eshelby, J. D. (1975), The Elastic EnergyMomentum Tensor, J. of Elasticity, Vol. 5, pp. 321–335. Kienzler, R., and Maugin, G. A., eds. (2001), Conﬁgurational Mechanics of Materials, SpringerVerlag, Wien. Maugin, G. A. (1993), Material Inhomogeneities in Elasticity, Chapman & Hall, New York. Mura, T. (1987), Micromechanics of Defects in Solids, Martinus Nijhoff Publishers, Dordrecht, The Netherlands. Rice, J. R. (1968), Mathematical Analysis in the Mechanics of Fracture. In Fracture – An Advanced Treatise (H. Liebowitz, ed.), Vol. II, pp. 191–311, Academic Press, New York. Rice, J. R. (1985), Conserved Integrals and Energetic Forces. In Fundamentals of Deformation and Fracture (B. A. Bilby, K. J. Miller, and J. R. Willis, eds.), Cambridge University Press, Cambridge.
22 Micropolar Elasticity
22.1 Introduction In a micropolar continuum the deformation is described by the displacement vector and an independent rotation vector. The rotation vector speciﬁes the orientation of a triad of director vectors attached to each material particle. A particle (material element) can experience a microrotation without undergoing a macrodisplacement. An inﬁnitesimal surface element transmits a force and a couple vector, which give rise to nonsymmetric stress and couplestress tensors. The former is related to a nonsymmetric strain tensor and the latter to a nonsymmetric curvature tensor, deﬁned as the gradient of the rotation vector. This type of the continuum mechanics was originally introduced by Voigt (1887) and the brothers Cosserat (1909). In a simpliﬁed micropolar theory, the socalled couplestress theory, the rotation vector is not independent of the displacement vector, but related to it in the same way as in classical continuum mechanics. The physical rationale for the extension of the classical to micropolar and couplestress theory was that the classical theory was not able to predict the size effect experimentally observed in problems which had a geometric length scale comparable to material’s microstructural length, such as the grain size in a polycrystalline or granular aggregate. For example, the apparent strength of some materials with stress concentrators such as holes and notches is higher for smaller grain size; for a given volume fraction of dispersed hard particles, the strengthening of metals is greater for smaller particles; the bending and torsional strengths are higher for very thin beams and wires. The classical theory was also in disagreement with experiments for highfrequency ultrashort wave propagation problems, if the wavelength becomes comparable to the material’s microstructural length. In the presence of couplestresses, shear waves propagate dispersively (with a frequency dependent wave speed). Couplestresses are also expected to affect the singular nature of the crack tip ﬁelds. The couplestress and related nonlocal and straingradient theories of elastic and inelastic material response are also of interest to describe the deformation mechanisms and manufacturing of micro and nanostructured materials and devices, as well as inelastic localization and instability phenomena.
375
376
22. Micropolar Elasticity
22.2 Basic Equations of CoupleStress Elasticity In a micropolar continuum the deformation is described by the displacement vector and an independent rotation vector. In the couplestress theory, the rotation vector ϕi is not independent of the displacement vector ui but is subject to the constraint ϕi =
1 1 i jk ω jk = i jk uk, j , 2 2
ωi j = i jk ϕk ,
(22.1)
as in classical continuum mechanics. The skewsymmetric alternating tensor is i jk, and ωi j are the rectangular components of the inﬁnitesimal rotation tensor. The latter is related to the displacement gradient and the symmetric strain tensor by u j,i = ei j + ωi j , where ei j =
1 (u j,i + ui, j ) , 2
ωi j =
1 (u j,i − ui, j ) . 2
(22.2)
The comma designates the partial differentiation with respect to Cartesian coordinates xi . A surface element dS transmits a force vector Ti dS and a couple vector Mi dS. The surface forces are in equilibrium with the nonsymmetric Cauchy stress ti j , and the surface couples are in equilibrium with the nonsymmetric couplestress mi j , such that Ti = n j t ji ,
Mi = n j m ji ,
(22.3)
where n j are the components of the unit vector orthogonal to the surface element under consideration. In the absence of body couples, the differential equations of equilibrium are t ji, j + fi = 0 ,
m ji, j + i jk t jk = 0 .
(22.4)
The body forces are denoted by fi . By decomposing the stress tensor into its symmetric and antisymmetric part, ti j = σi j + τi j ,
(σi j = σ ji ,
τi j = −τ ji ) ,
(22.5)
from the moment equilibrium equation it readily follows that the antisymmetric part can be determined as 1 τi j = − i jkmlk,l . 2
(22.6)
If the gradient of the couplestress vanishes at some point, the stress tensor is symmetric at that point. The rate of strain energy per unit volume is ˙ = σi j e˙i j + mi j κ˙ i j , W
(22.7)
κi j = ϕ j,i
(22.8)
where
is a nonsymmetric curvature tensor. In view of the identity ωi j,k = ekj,i − eki, j ,
(22.9)
the curvature tensor can also be expressed as κi j = − jkl eik,l .
(22.10)
22.3. Displacement Equations of Equilibrium
377
These are the compatibility equations for curvature and strain ﬁelds. In addition, there is an identity κi j,k = κkj,i (= ϕ j,ik) ,
(22.11)
which represents the compatibility equations for curvature components. The compatibility equations for strain components are the usual SaintVenant’s compatibility equations. Since ei j is symmetric and i jk skewsymmetric, from (22.10) it follows that the curvature tensor in couplestress theory is a deviatoric tensor (κkk = 0). Assuming that the elastic strain energy is a function of the strain and curvature tensors, W = W(ei j , κi j ), the differentiation and the comparison with (22.7) establishes the constitutive relations of couplestress elasticity, σi j =
∂W , ∂ei j
mi j =
∂W . ∂κi j
(22.12)
In the case of isotropic material, with the quadratic strain energy, W=
1 λ ekkell + µ ekl ekl + 2α κkl κkl + 2βκkl κlk , 2
(22.13)
where µ, λ, α, and β are the Lametype ´ constants of isotropic couplestress elasticity. The stress and couplestress tensors are in this case σi j = 2µ ei j + λ ekk δi j ,
mi j = 4α κi j + 4β κ ji .
(22.14)
By the positivedeﬁniteness of the strain energy, it follows that α + β > 0 , and α − β > 0 . Thus, α is positive, but not necessarily β. Since the curvature tensor is deviatoric, from the second (22.14) it follows that the couplestress is also a deviatoric tensor (mkk = 0). In some problems the curvature tensor may be symmetric, and then the couplestress is also symmetric, regardless of the ratio α/β. If the displacement components are prescribed at a point of the bounding surface of the body, the normal component of the rotation vector at that point cannot be prescribed independently. This implies (e.g., Mindlin and Tiersten, 1962; Koiter, 1964) that at any point of a smooth boundary we can specify three reduced stress tractions T¯i = n j t ji −
1 i jk n j (n p mpq nq ),k , 2
(22.15)
and two tangential couplestress tractions ¯ i = n j m ji − (n j m jknk)ni . M
(22.16)
22.3 Displacement Equations of Equilibrium The couplestress gradient can be expressed, from (22.10) and (22.14), as mlk,l = −2α kpq u p,qll ,
(22.17)
independently of the material parameter β. The substitution into (22.6) gives an expression for the antisymetric part of the stress tensor τi j = −2α ωi j,kk = −2α ∇ 2 ωi j ,
(22.18)
378
22. Micropolar Elasticity
which is also independent of β. The Laplacian operator is ∇ 2 = ∂ 2 /∂ xk∂ xk. Consequently, by adding (22.14) and (22.18), the total stress tensor is ti j = 2µ ei j + λ ekk δi j − 2α ∇ 2 ωi j .
(22.19)
Incorporating this into the force equilibrium equations (22.4), we obtain the equilibrium equations in terms of the displacement components 1 ∂ 2 2 4 2 2 (∇ · u) + l ∇ (∇ · u) = 0 , ∇ ui − l ∇ ui + (22.20) ∂ xi 1 − 2ν where ∇ · u = uk,k . The biharmonic operator is ∇ 4 = ∇ 2 ∇ 2 , and l2 =
α , µ
1+
λ 1 = . µ 1 − 2ν
(22.21)
The Poisson coefﬁcient is denoted by ν. Upon applying to (22.20) the partial derivative ∂/∂ xi , there follows ∇ 2 ekk = 0 . Thus, the volumetric strain is governed by the same equation as in classical elasticity, without couplestresses. The substitution into (22.20) yields the ﬁnal form of the displacement equations of equilibrium ∇ 2 ui − l 2 ∇ 4 ui +
∂ 1 (∇ · u) = 0 . 1 − 2ν ∂ xi
(22.22)
Three components of displacement and only two tangential components of rotation may be speciﬁed on the boundary. Alternatively, three reduced stress tractions and two tangential couplestress tractions may be speciﬁed on a smooth boundary. The general solution of (22.22) can be cast in the form ui = Ui − l 2
∂ ∂ 1 (∇ · U) − ϕ + x · (1 − l 2 ∇ 2 )U , ∂ xi 4(1 − ν) ∂ xi
(22.23)
where the scalar potential ϕ and the vector potential Ui are solutions of the Laplace’s and Helmholtz partial differential equations (22.24) ∇ 2 ϕ = 0 , ∇ 2 Ui − l 2 ∇ 2 Ui = 0 . The general solution of the latter equation can be obtained by observing that Ui − l 2 ∇ 2 Ui = Ui0
(22.25)
must be a harmonic function, satisfying the Laplacian equation ∇ 2 Ui0 = 0 . Thus, the general solution can be expressed as Ui = Ui0 + Ui∗ , where Ui∗ − l 2 ∇ 2 Ui∗ = 0 .
(22.26)
22.4 Correspondence Theorem of CoupleStress Elasticity For equilibrium problems of couplestress elasticity with prescribed displacement boundary conditions, and with no body forces or body couples present, we state the following theorem.
22.5. Plane Strain Problems
379
Theorem: If ui = uˆ i is a solution of the Navier equations of elasticity without couplestresses, ∇ 2 uˆ i +
∂ 1 ˆ = 0, (∇ · u) 1 − 2ν ∂ xi
(22.27)
then uˆ i is also a solution of differential equations (22.22) for couplestress elasticity. Proof: It sufﬁces to prove that uˆ i is a biharmonic function. By applying the Laplacian operator to (22.27), we obtain ∇ 4 uˆ i +
∂ 2 1 ˆ = 0. ∇ (∇ · u) 1 − 2ν ∂ xi
(22.28)
Since ∇ · uˆ is a harmonic function, as can be veriﬁed from (22.27) by applying the partial derivatives ∂/∂ xi , equation (22.28) reduces to ∇ 4 uˆ i = 0 .
(22.29)
This shows that uˆ i is a biharmonic function, which completes the proof. We now prove that the stress tensor in couplestress elasticity with prescribed displacement boundary conditions, and without body forces or body couples, is a symmetric tensor. From (22.27) it readily follows by partial differentiation that the rotation components are harmonic functions (∇ 2 ωi j = 0 , ∇ 2 ϕi = 0), and substitution into (22.18) gives τi j = 0. In general, the couplestress tensor is still nonsymmetric, although in the case of antiplane strain with prescribed displacement boundary conditions it becomes a symmetric tensor.
22.5 Plane Strain Problems of CoupleStress Elasticity In plane strain elasticity the displacement components are u1 = u1 (x1 , x2 ) ,
u2 = u2 (x1 , x2 ) ,
u3 = 0 .
(22.30)
The nonvanishing strain, rotation, and curvature components are ∂u1 ∂u2 1 ∂u2 ∂u1 , e22 = e12 = + , e11 = ∂ x1 ∂ x2 2 ∂ x1 ∂ x2 ϕ3 = ω12 =
κ13 =
1 2
∂ϕ3 , ∂ x1
∂u2 ∂u1 − ∂ x1 ∂ x2 κ23 =
,
(22.31)
∂ϕ3 . ∂ x2
The stressstrain relations are σ11 = (2µ + λ)e11 + λe22 , σ12 = 2µe12 ,
σ22 = (2µ + λ)e22 + λe11 ,
τ12 = −2α∇ 2 ϕ3 .
(22.32)
The normal stress σ33 = λ(e11 + e22 ). The couplestress–curvature relations are m13 = 4ακ13 ,
m31 = 4βκ13 ,
m23 = 4ακ23 ,
m32 = 4βκ23 .
(22.33)
380
22. Micropolar Elasticity
The elastic strain energy per unit volume is 2 1 1 1 2 2 2 σ11 + σ22 (m2 + m223 ) . W= + − 2νσ11 σ22 − σ33 σ12 + 2µ 2(1 + ν) 8α 13
(22.34)
Equations (22.31)–(22.34) can be easily rewritten in terms of polar coordinate components. For example, we have ∂uθ ∂ur 1 ∂uθ 1 ∂ur , eθ θ = + ur , er θ = +r − uθ , err = ∂r r ∂θ 2r ∂θ ∂r 1 ∂(r uθ ) ∂ur ∂ϕ3 1 ∂ϕ3 ϕ3 = ωr θ = − , κθ3 = . , κr 3 = 2r ∂r ∂θ ∂r r ∂θ 22.5.1 Mindlin’s Stress Functions The rectangular components of stress and couplestress tensors can be expressed in terms of the functions and as t11 =
∂2 ∂ 2 − , 2 ∂ x1 ∂ x2 ∂ x2
t22 =
t12 = −
∂2 ∂ 2 − , ∂ x1 ∂ x2 ∂ x22
t21 = −
m13 = where the functions
∂ , ∂ x1
∂2 ∂ 2 + , 2 ∂ x1 ∂ x2 ∂ x1
m23 =
∂2 ∂ 2 + , ∂ x1 ∂ x2 ∂ x12
(22.35)
∂ , ∂ x2
and satisfy the partial differential equations ∇4
= 0,
∇ 2 − l 2∇ 4 = 0 .
The curvaturestrain compatibility equations require that the functions by ∂ ∂ − l 2 ∇ 2 = −2(1 − ν)l 2 (∇ 2 ) , ∂ x1 ∂ x2 ∂ ∂ − l 2 ∇ 2 = 2(1 − ν)l 2 (∇ 2 ) . ∂ x2 ∂ x1
(22.36) and be related
(22.37)
The solution of the equation for in (22.36) can be expressed as = 0 + ∗ , where ∇ 2 0 = 0 ,
∗ − l 2∇ 2 ∗ = 0 .
(22.38)
Thus, (22.37) can be rewritten as ∂ ∂0 = −2(1 − ν)l 2 (∇ 2 ) , ∂ x1 ∂ x2 ∂0 ∂ = 2(1 − ν)l 2 (∇ 2 ) . ∂ x2 ∂ x1 The counterparts of (22.35) and (22.39) in polar coordinates are trr =
1 ∂2 1 ∂ 1 ∂ 1 ∂ 2 + 2 + 2 , − 2 r ∂r r ∂θ r ∂r ∂θ r ∂θ
(22.39)
22.6. Edge Dislocation in CoupleStress Elasticity
tθ θ =
tr θ = −
381
1 ∂ ∂2 1 ∂ 2 − 2 , + 2 ∂r r ∂r ∂θ r ∂θ
1 ∂ 1 ∂ 1 ∂ 2 1 ∂2 + 2 − − 2 , r ∂r ∂θ r ∂θ r ∂r r ∂θ 2
tθr = −
(22.40)
1 ∂ ∂ 2 1 ∂2 + 2 + , r ∂r ∂θ r ∂θ ∂r 2
mr 3 =
∂ , ∂r
mθ3 =
1 ∂ , r ∂θ
and ∂ ∂r 1 ∂ r ∂θ
1 ∂ − l 2 ∇ 2 = −2(1 − ν)l 2 (∇ 2 ) , r ∂θ ∂ − l 2 ∇ 2 = 2(1 − ν)l 2 (∇ 2 ) . ∂r
(22.41)
22.6 Edge Dislocation in CoupleStress Elasticity For an edge dislocation in an inﬁnite medium, the only boundary condition is the displacement discontinuity b, imposed for example along the plane x1 > 0, x2 = 0. Thus, by the correspondence theorem, the displacement ﬁeld is as in classical elasticity, i.e., x1 x2 x2 b 1 tan−1 , + u1 = 2π x1 2(1 − ν) x12 + x22 (22.42) x12 − x22 x12 + x22 b 1 + 2 u2 = − (1 − 2ν) ln . 2π 4(1 − ν) b2 x1 + x22 The stresses are σ11 = − σ22 = σ12
x2 (3x12 + x22 ) µb , 2π(1 − ν) (x12 + x22 )2
x2 (x12 − x22 ) µb , 2π(1 − ν) (x12 + x22 )2
x1 (x12 − x22 ) µb = , 2π(1 − ν) (x12 + x22 )2
σ33 = −
(22.43)
x2 νµb . 2 π(1 − ν) x1 + x22
The rotation and curvature components are ϕ3 = − κ13
x1 b , 2 2π x1 + x22
b x12 − x22 = , 2π (x12 + x22 )2
κ23
2x1 x2 b = . 2 2π (x1 + x22 )2
(22.44)
382
22. Micropolar Elasticity
The corresponding couplestresses are m13 =
2αb x12 − x22 , π (x12 + x22 )2
m31 =
2αb 2x1 x2 m23 = , π (x12 + x22 )2
2βb x12 − x22 , π (x12 + x22 )2
2βb 2x1 x2 m31 = . π (x12 + x22 )2
(22.45)
In polar coordinates, the displacements are ur =
b 2π
! 1 r2 1 − (1 − 2ν) ln 2 sin θ , 4(1 − ν) b ! 1 r2 θ sin θ + 1 + (1 − 2ν) ln 2 cos θ , 4(1 − ν) b
θ cos θ +
b uθ = − 2π
(22.46)
and the stresses σrr = σθ θ = − σr θ =
µb sin θ , 2π (1 − ν) r
cos θ µb , 2π (1 − ν) r
σ33 = −
(22.47)
νµb sin θ . π(1 − ν) r
The rotation and curvature components are ϕ3 = −
b cos θ , 2π r
b cos θ , 2π r 2
κr 3 =
κθ3 =
b sin θ , 2π r 2
(22.48)
with the corresponding couplestresses 2αb π 2αb = π
mr 3 = mθ3
cos θ , r2 sin θ , r2
2βb cos θ , π r2 2βb sin θ = . π r2
m3r = m3θ
(22.49)
The stress components decay with a distance from the center of dislocation as r −1 , whereas the couplestresses decay as r −2 . These also specify the orders of the singularities at the dislocation core when r → 0. The displacement and rotation ﬁelds for an edge dislocation in polar elasticity, without the constraint (22.1), can be found in Nowacki (1986).
22.6.1 Strain Energy The strain energy (per unit length in x3 direction) stored within a cylinder bounded by the radii r0 and R (Fig. 22.1) is E=
R 2π
r0
0
W r dr dθ ,
(22.50)
22.6. Edge Dislocation in CoupleStress Elasticity
383
b
σrθ
T
r0
Figure 22.1. A material of the dislocation core is removed and its effect on the remaining material represented by the indicated stress and couplestress tractions over the surface r = r0 . The slip discontinuity of amount b is imposed along the cut at an angle ϕ.
ϕ
σrr mr3
where the speciﬁc strain energy (per unit volume) is
1 2 1 2 σr θ + (1 − 2ν)σrr2 + mr 3 + m2θ3 2µ 8α αb2 1 µb2 1 2 θ + . = 1 − 2ν sin 8π 2 (1 − ν)2 r 2 2π 2 r 4
W=
(22.51)
Upon the substitution into (22.50) and integration, there follows R αb2 µb2 ln + E= 4π(1 − ν) r0 2π
1 1 − 2 ro2 R
.
(22.52)
The second term on the righthand side is the strain energy contribution from the couplestresses. The presence of this term is associated with the work done by the couplestresses on the surfaces r = r0 and r = R. This can be seen by writing an alternative expression for the strain energy, 1 E= 2
R
r0
1 σr θ (r, 0) b dr + 2
0
2π
1 M3 ϕ3 R dθ − 2
2π
M3 ϕ3 r0 dθ ,
(22.53)
0
with M3 = mr 3 given by (22.49), and ϕ3 given in (22.48). The work of the tractions σrr and σr θ on the displacements ur and uθ over the surface r = R cancels the work of the tractions σrr and σr θ over the surface r = r0 . These terms are thus not explicitly included in (22.53). The second term in (22.52) is the strain energy contribution due to last two work terms in (22.53). For example, in a metallic crystal with the dislocation density ρ = 1010 cm−2 , the radius of inﬂuence of each dislocation (deﬁned as the average distance between dislocations) is a = 0.4 nm, of the order of ρ −1/2 = 100 nm. For an fcc crystal with the lattice parameter √ and the Burgers vector along the closed packed direction b = a/ 2, the radius R can be approximately √ taken as R = 200b. By choosing the material length l to be the lattice parameter (l = 2b), the couplestress modulus is α = 2µb2 , and by selecting r0 = 2b and ν = 1/3, the strain energy contribution from couplestresses in (22.52) is 14.5% of the strain energy without couple stresses. The calculations are sensitive to selected value of the dislocation core radius; larger the value of r0 smaller the effect of couplestresses in the region beyond r0 (Lubarda, 2003a). The strain energy contribution from couplestresses is likely to be lowered by inclusion of the micropolar effects. It is known that the effect of couplestresses on stress concentration is less pronounced if the microrotations are assumed to be independent of the displacement ﬁeld (Eringen, 1999).
384
22. Micropolar Elasticity
r0
Figure 22.2. A slip discontinuity of amount b is imposed along the horizontal cut from the inner radius r0 to the outer radius R. The inner and outer surface of the cylinder are free from stresses and couplestresses.
b
R
22.7 Edge Dislocation in a Hollow Cylinder The socalled hollow dislocation along the axis of a circular cylinder with inner radius r0 and the outer radius R is shown in Fig. 22.2. Both surfaces of the cylinder are required to be stress and couple stress free. The displacement discontinuity of amount b is imposed along the horizontal cut from r0 to R. The solution is derived from the inﬁnite body solution by superposing an additional solution that cancels the stresses and couplestresses over the inner and outer surface associated with the solution for an edge dislocation in an inﬁnite medium. Thus, we require that the superposed solution satisﬁes the boundary conditions trr (R, θ) =
tr θ (R, θ ) = −
sin θ µb , 2π(1 − ν) R
cos θ µb , 2π(1 − ν) R
mr 3 (R, θ ) = −
trr (r0 , θ ) =
tr θ (r0 , θ ) = −
2αb cos θ , π R2
sin θ µb , 2π (1 − ν) r0
cos θ µb , 2π (1 − ν) r0
mr 3 (r0 , θ ) = −
(22.54)
2αb cos θ . π r02
This can be accomplished by using the following structure of the Mindlin stress functions 1 3 = A0r + B0 sin θ , (22.55) r r r 1 + DK1 cos θ . = Ar + B + C I1 r l l
(22.56)
From the conditions (22.41) it readily follows that A = −16(1 − ν)l 2 A0 ,
B = 0.
(22.57)
The stress and couplestress components of the superposed solution are accordingly r 1 1 1 r − D K2 trr = 2A0r − 2B0 3 + C I2 sin θ , r rl l rl l tr θ
r 1 1 1 r − D K2 cos θ , = − 2A0r − 2B0 3 + C I2 r rl l rl l
(22.58)
r r ( ' 1 r 1 r mr 3 = − 16(1 − ν)l 2 A0 − C I0 + I2 +D K0 + K2 cos θ. 2l l l 2l l l
22.7. Edge Dislocation in a Hollow Cylinder
385
The expressions for the derivatives of the modiﬁed Bessel functions with respect to r/l are used (Watson 1995). After a lengthy but straightforward derivation, it follows that R2 − r02 µb 2αb l Rb1 − r0 b2 − , 2π(1 − ν) Ra1 − r0 a2 π R2 Ra1 − r0 a2 Ra2 − r0 a1 µb 1 2αb l a2 b1 − a1 b2 , − B0 = Rr0 2 2π(1 − ν) Ra1 − r0 a2 π R2 Ra1 − r0 a2
(22.59)
c1 2αb l c2 A0 − , c π R2 c d1 2αb l d2 D = −16(1 − ν)l 3 A0 + . c π R2 c
(22.60)
A0 =
and C = 16(1 − ν)l 3
The introduced parameters are a1 = 2R3 − 16(1 − ν)
l3 (c1 d3 − d1 c3 ) , c
a2 = 2r03 − 16(1 − ν)
l3 (c1 d4 − d1 c4 ) , c
b1 = where c1 =
c2 = −
1 (c2 d3 − d2 c3 ) , c
1 (c2 d4 − d2 c4 ) , c
r R R 1 r0 1 0 K0 + K2 , K0 + K2 − 2 l l 2 l l r R R R2 1 r0 0 K0 + K2 + 2 K0 + K2 , 2 l l l l 2r0 c3 =
and d1 = −
d2 =
b2 =
(22.61)
R R K2 , l l
c4 =
(22.62)
r r0 0 K2 , l l
r R R 1 1 r0 0 I0 + I2 , I0 + I2 + 2 l l 2 l l
r R R R2 1 r0 0 I0 + I2 − 2 I0 + I2 , 2 l l l l 2r0 R R , d3 = − I2 l l
d4 = −
r0 r0 I2 . l l
(22.63)
386
22. Micropolar Elasticity
The parameter c is deﬁned by r 1 R R r0 0 I0 + I2 c= K0 + K2 4 l l l l r R R 1 r0 0 + I2 . K0 + K2 I0 − 4 l l l l
(22.64)
If R → ∞, we obtain the solution for an edge dislocation with a stress free hollow core in an inﬁnite medium. In this case A0 = A = B = D = 0, and B0 = − D=
µbr02 4π(1 − ν)
−
K2 (r0 /l) , π K0 (r0 /l) + K2 (r0 /l)
2αb 1
4αbl
πr02 K0 (r0 /l) + K2 (r0 /l)
(22.65)
.
If couplestresses are neglected, (22.59) and (22.60) yield A0 =
1 µb , 2 4π(1 − ν) R + r02
B0 = −R2r02 A0
A= C = D = 0.
(22.66)
The corresponding stresses are R2r02 1 1 µb − 2 σrr = − r+ 3 sin θ , 2π(1 − ν) r r R + r02 σr θ =
σθ θ
R2r02 1 1 µb − 2 r + cos θ , 2π(1 − ν) r r3 R + r02
(22.67)
R2r02 1 µb 1 − 2 =− 3r − 3 sin θ , 2π(1 − ν) r r R + r02
in agreement with the solution for the Volterra edge dislocation from classical elasticity (Love, 1944).
22.8 Governing Equations for Antiplane Strain For the antiplane strain problems, the displacements are u1 = u2 = 0 ,
u3 = w(x1 , x2 ) .
(22.68)
The nonvanishing strain, rotation, and curvature components are e13 = e31 =
ϕ1 = ω23 =
κ11 = −κ22 =
1 ∂w , 2 ∂ x1 1 ∂w , 2 ∂ x2
1 ∂ 2w , 2 ∂ x1 ∂ x2
e23 = e32 =
1 ∂w , 2 ∂ x2
ϕ2 = ω31 = −
κ12 = −
1 ∂ 2w , 2 ∂ x12
1 ∂w , 2 ∂ x1 κ21 =
(22.69) 1 ∂ 2w . 2 ∂ x22
22.8. Governing Equations for Antiplane Strain
387
It readily follows that ∇ 2 ω13 =
1 ∂ 2 ∇ w , 2 ∂ x1
∇ 2 ω23 =
1 ∂ 2 ∇ w , 2 ∂ x2
(22.70)
so that, from (22.18), τ31 = −τ13 = α
∂ 2 ∇ w , ∂ x1
τ32 = −τ23 = α
∂ 2 ∇ w . ∂ x2
(22.71)
Consequently, from (22.19), ∂ w − l 2 ∇ 2w , ∂ x1 ∂ w − l 2 ∇ 2w , =µ ∂ x2
t13 = µ t23
∂ w + l 2 ∇ 2w , ∂ x1 ∂ w + l 2 ∇ 2w . =µ ∂ x2
t31 = µ t32
(22.72)
The couplestresses are related to the curvature components by m11 = 4(α + β)κ11 = 2(α + β)
∂ 2w , ∂ x1 ∂ x2
m22 = 4(α + β)κ22 = −2(α + β) m12 = 4ακ12 + 4βκ21 = −2α m21 = 4ακ21 + 4βκ12 = 2α
∂ 2w = −m11 , ∂ x1 ∂ x2
∂ 2w ∂ 2w + 2β , 2 ∂ x1 ∂ x22
(22.73)
∂ 2w ∂ 2w − 2β . 2 ∂ x2 ∂ x12
It is noted that m12 − m21 = 2(β − α)∇ 2 w .
(22.74)
Since displacement ﬁeld is isochoric (∇ · u = 0), the displacement equations of equilibrium (22.22) reduce to a single equation ∇ 2w − l 2 ∇ 4w = 0 .
(22.75)
The general solution can be expressed as w = w0 + w∗ ,
(22.76)
where w0 and w ∗ are the solutions of the partial differential equations ∇ 2 w0 = 0 , w∗ − l 2 ∇ 2 w∗ = 0 .
(22.77)
In view of (22.76) and (22.77), the following identities hold ∇ 2w =
1 ∗ w , l2
(22.78)
and w − l 2 ∇ 2 w = w0 ,
w + l 2 ∇ 2 w = w0 + 2w∗ ,
which can be conveniently used to simplify the stress expressions (22.72).
(22.79)
388
22. Micropolar Elasticity
22.8.1 Expressions in Polar Coordinates When expressed in terms of polar coordinates, the general solutions of (22.77), obtained by separation of variables, are w 0 = (A0 + B0 ln r )(C0 + θ) +
∞
An r n + Bn r −n (Cn cos nθ + sin nθ) ,
(22.80)
n=1
r r + B0∗ K0 (C0∗ + θ) w ∗ = A∗0 I0 l l ∞ r r + Bn∗ Kn (Cn∗ cos nθ + sin nθ) . + A∗n In l l n=1
(22.81)
The functions In (ρ) and Kn (ρ) (with ρ = r/l) in (22.81) are the modiﬁed Bessel functions of the ﬁrst and second kind (of the order n). The nonvanishing strain, rotation, and curvature components in polar coordinates are 1 ∂w 1 ∂w , er 3 = e3r = , 2r ∂θ 2 ∂r 1 ∂w 1 ∂w , ϕθ = ω3r = − , = 2r ∂θ 2 ∂r
eθ3 = e3θ = ϕr = ωθ3 and κrr =
1 ∂ ∂ϕr = ∂r 2 ∂r κθr =
κθ θ
1 ∂w , r ∂θ
κr θ =
1 ∂ 2w ∂ϕθ =− , ∂r 2 ∂r 2
ϕθ 1 ∂ 2w 1 ∂ϕr 1 ∂w − = 2 , + r ∂θ r 2r ∂θ 2 2r ∂r
ϕr 1 ∂ 1 ∂ϕθ + =− = r ∂θ r 2 ∂r
(22.82)
1 ∂w r ∂θ
(22.83)
= −κrr .
Note that 1 κr θ − κθr = κ12 − κ21 = − ∇ 2 w . 2
(22.84)
The corresponding couplestress components are (Fig. 22.3) ∂ 1 ∂w mrr = −mθ θ = 2(α + β) , ∂r r ∂θ mr θ = −2(α + β)
∂ 2w + 2β ∇ 2 w , ∂r 2
mθr = −2(α + β)
∂ 2w + 2α ∇ 2 w . ∂r 2
(22.85)
The shear stresses are ∂ ∂r ∂ =µ ∂r
tr 3 = µ t3r
w − l 2 ∇ 2w ,
w + l 2 ∇ 2w ,
1 r 1 =µ r
tθ3 = µ t3θ
∂ ∂θ ∂ ∂θ
w − l 2 ∇ 2w ,
w + l 2 ∇ 2w .
(22.86)
22.8. Governing Equations for Antiplane Strain
389
m 22
t23 m 11
t13
t13 m 12
m12
θ
tr3
tθ3
m11
m rr
m rθ
mθr
mθθ
m 21
tr3
tθ3
m rθ
m θr
t23 m 21
mθθ
m rr m 22
(b)
(a)
Figure 22.3. (a) A material element with sides parallel to coordinates directions x1 and x2 under conditions of antiplane strain; (b) The corresponding element with sides parallel to polar directions r and θ.
In view of (22.79), the stress components tr 3 and tθ3 (or t13 and t23 ) do not depend explicitly on w∗ , i.e., ∂w0 1 ∂w0 , tθ3 = µ , ∂r r ∂θ (22.87) ∂w ∗ 1 ∂w∗ , t3θ = tθ3 + 2µ . t3r = tr 3 + 2µ ∂r r ∂θ The couplestresses, however, affect the values of tr 3 and tθ3 through the imposed boundary conditions. For example, along an unstressed circular boundary r = R around the origin, the reduced tractions must vanish, tr 3 = µ
t¯r 3 = tr 3 −
1 ∂mrr = 0, 2R ∂θ
mr θ = 0 .
(22.88)
Also note that mr θ = −2(α + β)
∂ 2 w 2β ∗ + 2w , ∂r 2 l
mθr = −2(α + β)
∂ 2 w 2α ∗ + 2w . ∂r 2 l
(22.89)
The elastic strain energy per unit volume is '
( 1 1 1 2 2 2 σr 3 + σθ3 mrr α(mr2θ + m2θr ) − 2βmr θ mθr . (22.90) + + W= 2µ 4(α + β) 2(α − β) 22.8.2 Correspondence Theorem for Antiplane Strain For antiplane strain problems with prescribed displacement boundary conditions, the correspondence theorem of couplestress elasticity reads: If w = w 0 is a solution of differential equation of elasticity without couplestresses ∇ 2 w0 = 0, then w 0 is also a solution of differential equations (22.75) for couplestress elasticity. The proof is simple. Since w0 is a harmonic function, it is also a biharmonic function, satisfying (22.75). For prescribed displacement boundary conditions, the function w 0 speciﬁes the displacement ﬁeld in both nonpolar and couplestress elasticity.
390
22. Micropolar Elasticity
w=0
σ 0r3 = const. m 0rθ = 0
R
Figure 22.4. A circular annulus of inner radius R and outer radius R0 under shear stress σr03 over the outer surface. The inner surface of the cylinder is ﬁxed (w = 0).
R0
The stress and couplestress tensors in antiplane strain problems of couplestress elasticity, in the case of prescribed displacement boundary conditions, are symmetric tensors. Indeed, since the displacement ﬁeld is a harmonic function, the antisymmetric stress components in (22.72) vanish, i.e., τ13 = τ23 = 0. Thus, the total stress tensor is a symmetric tensor. From (22.8) it further follows that the curvature tensor is a symmetric tensor (κ12 = κ21 ). This implies from (22.73) that the couplestress tensor is also symmetric (m12 = m21 ), regardless of the ratio α/β.
22.9 Antiplane Shear of Circular Annulus A simple but illustrative problem of couplestress elasticity is the antiplane shearing of a circular annulus. Suppose that the inner surface r = R is ﬁxed, whereas the constant shearing stress σr03 is applied on the outer surface r = R0 (Fig. 22.4). The corresponding displacement ﬁeld is independent of θ and given by r r r + DK0 . (22.91) w(r ) = R0 Aln + B + C I0 R l l The integration constants are speciﬁed from the boundary conditions w(R) = 0 ,
tr 3 (R0 ) = σr03 ,
mr θ (R0 ) = 0 .
(22.92)
The fourth boundary condition is obtained by specifying an additional information about the bonded interface, such as the magnitude of slope dw/dr or the couplestress mr θ at r = R. We will proceed by adopting the ﬁrst choice, i.e., by assuming that the rotation 1 dw ϕθ (R) = − = ϕˆ θ (22.93) 2 dr r =R is known at the interface. It readily follows from (22.87)–(22.89) that σ0 R R A = r 3 , B = −C I0 − DK0 , µ l l and
R
0 R0 σr 3 ˆ l K1 l − b R µ − 2b ϕθ R R , C= R0 b I1 l + a K1 l R
0 R0 σr 3 l I1 l + a R µ + 2a ϕˆ θ D= , R0 b I1 Rl + a K1 Rl
(22.94)
(22.95)
22.10. Screw Dislocation in CoupleStress Elasticity
where
R0 R0 α R0 I0 − I1 , a= α+β l l l
391
R0 R0 α R0 b= K0 + K1 . α+β l l l
Consequently, tr 3 (r ) =
t3r (r ) =
R0 0 σ , r r3
r r ( R0 ' 0 r σr 3 + 2µ C I1 − DK1 , r l l l
(22.96)
r l r ' R σ0 R0 α 0 r3 −C 2 I0 − I1 mr θ (r ) = 2(α + β) 2 r µ l α+β l r l ( α R0 l r r −D 2 K0 + K1 , l α+β l r l r l r ' R σ0 R0 β 0 r3 mθr (r ) = 2(α + β) 2 −C 2 I0 − I1 r µ l α+β l r l r l r ( β R0 K0 + K1 . −D 2 l α+β l r l
(22.97)
If the bonded interface cannot support the couplestress mr θ , we set the righthand side of the above expression for mr θ equal to zero and calculate the corresponding rotation ϕˆ θ .
22.10 Screw Dislocation in CoupleStress Elasticity The displacement ﬁeld for a screw dislocation with imposed displacement discontinuity b along the plane x1 > 0, x2 = 0 is as in classical elasticity, i.e., w=
b x2 b tan−1 θ. = 2π x1 2π
(22.98)
This follows from the correspondence theorem, since only the displacement boundary conditions are prescribed. The stresses and couplestresses associated with (22.98) are σ13 = −
x2 µb , 2π x12 + x22
m11 = −m22 = −
m12 = m21 = −
σ23 =
x1 µb , 2π x12 + x22
(α + β)b x12 − x22 , π (x12 + x22 )2
(22.99)
(α + β)b 2x1 x2 . π (x12 + x22 )2
The components of the stress and couplestress tensors along the polar directions are µb 1 , σr 3 = 0 , 2π r (α + β)b 1 =− , mr θ = mθr = 0 . π r2 σθ3 =
mrr = −mθ θ
(22.100)
392
22. Micropolar Elasticity
The stress components decay with a distance from the center of dislocation as r −1 , whereas the couplestresses decay as r −2 . These also specify the orders of the singularities at the dislocation core when r → 0. 22.10.1 Strain Energy The strain energy (per unit length in x3 direction) stored within a cylinder bounded by the radii r0 and R is R E= W 2πr dr , (22.101) r0
where the speciﬁc strain energy (per unit volume) is W=
1 µb2 1 (α + β)b2 1 1 2 2 σθ3 + mrr = + . 2µ 4(α + β) 8π 2 r 2 4π 2 r4
Upon the substitution into (22.101) and integration, there follows R (α + β)b2 1 1 µb2 ln + . − E= 4π r0 4π ro2 R2
(22.102)
(22.103)
The second term on the righthand side is the strain energy contribution from the couplestresses. The presence of this term is associated with the work done by the couplestresses on the surfaces r = r0 and r = R. This can be seen by writing an alternative expression for the strain energy, 1 2π 1 2π 1 R σθ3 (r, 0) b dr + Mr ϕr R dθ − Mr ϕr r0 dθ , (22.104) E= 2 r0 2 0 2 0 with Mr = mrr given by (22.100), and with 1 b 1 ∂w = (22.105) 2r ∂θ 4π r being the r component of the rotation vector. Since σr 3 = 0, there is no work of stress traction on the displacement w over the surfaces r = r0 and r = R. The second term in (22.103) is the strain energy contribution due to last two work terms in (22.104). For example, if we set R = 200b, r0 = 2b, and α + β = 2µb2 , the energy contribution from couplestresses in (22.103) is 10.9% of the strain energy without couplestresses. In the classical elasticity a cylindrical surface around the screw dislocation at its center is stress free. On the other hand, the solution derived in this section is characterized by the presence of the constant couple stress mrr along that surface. However, since mrr in (22.100) does not depend on θ, the reduced traction t¯r 3 vanishes on the cylindrical surface r = const. ϕr = ωθ z =
22.11 Conﬁgurational Forces in CoupleStress Elasticity Returning to general theory of couplestress elasticity, it is appealing to extend the energy considerations from Chapter 21 to the framework of couplestress theory. Thus, we now derive expressions for the interaction energy between the stress systems due to internal and external sources of stress, the conﬁgurational force on a singularity or the source of internal stress, and the energymomentum tensor of elastic couplestress ﬁeld.
22.11. Conﬁgurational Forces
393
22.11.1 Reciprocal Properties Consider two equilibrium elastic ﬁelds, designated by the superscripts Aand B. Clearly, in analogy with (21.54), σ jiAe Bji = σ jiBe A ji ,
mAji κ jiB = mBji κ jiA,
(22.106)
and (t jiA − τ jiA)ui,Bj = (t jiB − τ jiB)ui,Aj .
(22.107)
The equilibrium equations (22.4) provide the relationships t jiAui,Bj − t jiB ui,Aj = (t jiAuiB − t jiB uiA), j + fi AuiB − fi BuiA, τ jiAui,Bj − τ jiBui,Aj = −(mAji ϕiB − mBji ϕiA), j ,
(22.108)
so that the substitution into (22.107) gives (t jiAuiB + mAji ϕiB − t jiB uiA − mBji ϕiA), j = fi BuiA − fi AuiB.
(22.109)
Integrating over the volume of the body and using the Gauss divergence theorem, we thus obtain A B A B t ji ui + m ji ϕi n j dS + fi AuiBdV =
S
S
t jiB uiA +
A
mBji ϕi
V
n j dS + S
(22.110) fi BuiAdV,
which is Betti’s reciprocal theorem of couplestress elasticity. In the absence of body forces, from (22.109) it follows that the vector v j (A, B) = t jiAuiB + mAji ϕiB − t jiB uiA − mBji ϕiA has zero divergence. Thus,
(22.111)
v j (A, B)n j dS = S1
v j (A, B)n j dS,
(22.112)
S2
for any two surfaces S1 and S2 which do not embrace any singularity of v j (A, B). In particular, if there are no singularities of v j (A, B) within a surface S, v j (A, B)n j dS = 0. (22.113) S
If the material is homogeneous, in addition to (22.106) we have A B e ji = σ jiBe A σ ji,k ji,k,
A mAji,kκ jiB = mBji κ ji,k .
(22.114)
Consequently, for a homogeneous material (22.113) also applies when v j (A, B) is replaced by A A A uiB + mAji,kϕiB − t jiB ui,k − mBji ϕi,k . ϑ jk(A, B) = t ji,k
(22.115)
394
22. Micropolar Elasticity
22.11.2 Energy due to Internal Sources of Stress Suppose that there are two systems of internal stresses in the body of volume V bounded by the surface S. The sources of internal stress system A lie entirely within the surface S0 , and those of the system B lie entirely outside of S0 . If EA and EB are the values of the elastic strain energy when A and B alone exists in the body, we may write the total strain energy as E = EA + EB + EAB when the sources coexist in the body. Here, A B 1 B A (22.116) σ e + mAji κ jiB + σ jiBe A EAB = ji + m ji κ ji )dV 2 V ji ji is the interaction energy between A and B. Noting that eiBj = 12 (ui,Bj + u Bj,i ) and κiBj = ϕ Bj,i A in the volume V0 within the surface S0 , and eiAj = 12 (ui,Aj + u Aj,i ) and κiAj = ϕ j,i in the volume V − V0 (but not conversely), and in view of the reciprocity properties, (22.116) can be rewritten as A B B A A B σ ji e ji + m ji κ ji dV + σ ji e ji + mBji κ jiA dV. (22.117) EAB = V0
V−V0
Furthermore, σ jiAe Bji = σ jiAui,Bj = (t jiA − τ jiA)ui,Bj , and since from equilibrium equations without body forces t jiAui,Bj = (t jiAuiB), j ,
τ jiAui,Bj = −mAji, j ϕiB,
(22.118)
we obtain σ jiAe Bji + mAji κ jiB = (t jiAuiB + mAji ϕiB), j .
(22.119)
An analogous equation holds when the superscripts Aand B are interchanged in (22.119). Substituting these two equations into (22.117) and applying the Gauss divergence theorem gives A B EAB = t ji ui + mAji ϕiB − t jiB uiA − mBji ϕiA n j dS, (22.120) S0
where n j is the outward normal to S0 . The surface integral over S vanishes, because no load is there applied. Thus, the interaction energy between two internal stress systems can be expressed by the integral over any surface S0 that separates the two stress sources. Note that the bracketed terms of the integrand in (22.120) are equal to v j (A, B) by (22.111). 22.11.3 Energy due to Internal and External Sources of Stress Denote by A the stress system due to internal sources within the volume V, and by B the stress system due to external surface load Ti B and MiB applied over S. The total potential energy of the system is % = % A + % B + % AB, where 1 (σ Ae A + mAji κ jiA)dV, % A = EA = 2 V ji ji (22.121) B B B B % B = EB − (Ti ui + Mi ϕi )dS S
22.11. Conﬁgurational Forces
395
represent the potential energies of two systems when they act alone, and % AB = EAB − (Ti BuiA + MiBϕiA)dS
(22.122)
S
is the interaction potential energy between the two systems. The interaction strain energy EAB between stress systems due to internal and external stress sources is equal to zero. Indeed, in this case uiB and ϕiB exist throughout the volume V, and from (22.116) and the reciprocity property we have A B σ ji e ji + mAji κ jiB dV = (t jiAuiB + mAji ϕiB), j dV. (22.123) EAB = V
V
Thus, upon application of the Gauss theorem, we obtain EAB = 0, because Ti A = 0 and MiA = 0 on S. The response of the body to external loading in couplestress theory is, therefore, the same whether the body is selfstressed or not, as in classical elasticity. The interaction potential energy between external and internal stress systems is consequently (22.124) % AB = − (t jiB uiA + mBji ϕiA)n j dS. S
The righthand side of (22.124) can be rewritten in the same form as the righthand side of (22.120), provided that S0 is taken to be any surface that entirely encompasses the sources of internal stress A. This follows from the Gauss divergence theorem applied to the region V − V0 , noting that Ti A = MiA = 0 on S, and that v j (A, B) is divergence free in the region between S and S0 . In fact, if (uiC , ϕiC , tiCj , miCj ) is any elastic ﬁeld free of singularities within S0 (thus v j (B, C) is divergence free in S0 ), we can write A (t ji − t Cji )uiB + (mAji − mCji )ϕiB % AB = S0 (22.125)
B A C B A C − t ji (ui − ui ) − m ji (ϕi − ϕi ) n j dS, Since the ﬁeld C is arbitrary ﬁeld without singularities within S0 , (A− C) ﬁeld in (22.125) can be any ﬁeld which has the same singularities within S0 as does the ﬁeld A. In applications it is convenient to take (A− C) to be the elastic ﬁeld of internal sources A, considered to be emerged in an inﬁnite body. Thus, the interaction potential energy between the internal system A and external system B can be written as ∞ B B B ∞ B ∞ t ji ui + m∞ (22.126) % AB = ji ϕi − t ji ui − m ji ϕi n j dS. S0
This is a generalization of the corresponding Eshelby’s result from classical elasticity. 22.11.4 The Force on an Elastic Singularity The force on a singularity A due to external system B can be deﬁned as the negative gradient of interaction energy with respect to the location of the singularity, i.e., Jk = −
∂% AB . ∂ xkA
(22.127)
396
22. Micropolar Elasticity
To elaborate on this expression, it is convenient to use (22.126) for the interaction energy % AB. The stress ﬁeld in an inﬁnite body due to singularity at A evidently satisﬁes the property A A ∞ A A (22.128) ti∞ j xk, xk + dxk = ti j xk − dxk , xk , because moving the singularity for dxkA toward the point of observation xk, or approaching the point of observation toward the singularity by dxkA, equally effects the stress at the point of observation. Thus, ∂ti∞ j ∂ xkA
=−
∂ti∞ j ∂ xk
.
(22.129)
Analogous expressions apply to couplestress, displacement and rotation gradients. Substitution into (22.127), therefore, gives ∞ B B B ∞ B ∞ t ji,kui + m∞ (22.130) Jk = ji,kϕi − t ji ui,k − m ji ϕi,k n j dS. S0
ti∞ j
= + (and similarly for other ﬁelds), where the superscript I denotes the Since image ﬁeld, free of singularities within S0 , (22.130) can be rewritten as A B A A t ji,kui + mAji,kϕiB − t jiB ui,k n j dS. − mBji ϕi,k (22.131) Jk = tiAj
tiIj
S0
The terms within the brackets in the integrand are equal to ϑ jk(A, B), deﬁned by (22.115). Recall that ϑ jk(I, B) is divergence free within S0 . The righthand side of (22.131) is symmetric with respect to superscripts Aand B. Thus, the force on a singularity can also be expressed as B A B B t ji,kui + mBji,kϕiA − t jiAui,k n j dS. − mAji ϕi,k (22.132) Jk = S0
To see that the righthand sides of (22.131) and (22.132) are equal, we can form their difference, which is
v j,k(A, B)n j dS = v j, j (A, B)nkdS. (22.133) ϑ jk(A, B) − ϑ jk(B, A) n j dS = S0
S0
S0
The last integral is equal to zero, because from (22.111) we obtain v j, j (A, B) = 0, in view of the reciprocity properties and (22.118). In (22.133) we also assumed that uiA is singlevalued on S0 .
22.12 EnergyMomentum Tensor of a CoupleStress Field As in classical elasticity, it is possible to develop a general expression for the force on an elastic singularity. To that goal, consider a body of volume V, loaded by the force traction Tk and couple traction Mk over its external surface S. The body contains a singularity which is a source of internal stress (e.g., a dislocation, an interstitial atom, or other lattice defect). The total potential energy is %= WdV − Tj u j + Mj ϕ j dS, (22.134) V
S
22.12. EnergyMomentum Tensor
397
where W is the elastic strain energy density, deﬁned in linear couplestress theory by (22.13). If the singularity is moved a small distance in the direction nk, the potential energy alters due to the change of the elastic strain energy and the load potential. The change of the elastic strain energy is Tj δku j + u j,k + Mj δkϕ j + ϕ j,k dS, WdV = − WnkdS + δk (22.135) V
S
S
to within linear terms in . This can be established by the same consideration as in the original Eshelby’s derivation of classical elasticity. The symbol δk indicates a variation associated with an inﬁnitesimal displacement of the singularity in the direction nk. The change of the load potential due to displacement of the singularity is Tj u j + Mj ϕ j dS = Tj δku j + Mj δkϕ j dS + O( 2 ). (22.136) δk S
S
Thus, the total change of the potential energy becomes δk% = − Wnk − Tj u j,k − Mj ϕ j,k dS + O( 2 ).
(22.137)
S
Since the force on the singularity can be deﬁned as Jk = − lim
→0
we obtain, from (22.137),
Jk =
δk % ,
Wnk − Tj u j,k − Mj ϕ j,k dS.
(22.138)
(22.139)
S
This can be rewritten as
Jk =
Pikni dS,
(22.140)
S
where Pik = Wδik − ti j u j,k − mi j ϕ j,k
(22.141)
is the energymomentum tensor of the couplestress elastic ﬁeld. Pursuing Eshelby’s (1956) analysis further, assume that in addition to a considered singularity A and external load B, there are other sources of internal stress, collectively denoted by C. Each of the elastic ﬁelds in the body, such as the displacement ﬁeld ui , can be represented as ui = ui∞ + uiI + uiB + uiC ,
(22.142)
where the superscript I designates the image ﬁeld of the singularity A, considered to be in an inﬁnite medium. The total force on the singularity A is then Jk = JkI + JkB + JkC , where
JkX
= S
X ∞ X X ∞ X ∞ t∞ ji,kui + m ji,kϕi − t ji ui,k − m ji ϕi,k n j dS,
(22.143)
(22.144)
398
22. Micropolar Elasticity
for each of the superscripts X = I, B, C. Indeed, a typical cross term in (22.139) is X Y 1 X Y X Y Y σlk ekl + mlk (X, Y) = (22.145) n j dS. ϕk,l ni − t jk uk,i + mXjkϕk,i S 2 This can be rewritten, by using (22.119), as X Y 1 X Y X Y Y (X, Y) = tlk uk + mlk n j dS. ϕk ,i nl − t jk uk,i + mXjkϕk,i S 2
(22.146)
The property was employed that the surface integral of ,l ni is equal to that of ,i nl for any tensor ﬁeld deﬁned within S. Thus, upon differentiation, it follows that 1 (X, Y) = ϑ ji (X, Y)n j dS. (22.147) 2 S This is equal to zero because ϑ ji (X, Y) is a divergence free ﬁeld, unless one or other of the labels X and Y stands for ∞. The term (∞, ∞) also vanishes because the products of the elastic ﬁelds in an inﬁnite medium rapidly approach zero at large distances from the singularity. Returning to (22.139), if S does not embrace a singularity, a conservation law Jk = 0 of couplestress elasticity is obtained. There is also a conservation law Lk = 0, where Lk = ki j Wx j ni + Ti u j + Mi ϕ j − Tl ul,i x j − Ml ϕl,i x j dS, (22.148) S
i.e., written more compactly by using the energymomentum tensor, Lk = ki j Pli x j + tli u j + mli ϕ j nl dS.
(22.149)
S
22.13 Basic Equations of Micropolar Elasticity In the inﬁnitesimal micropolar elasticity the deformation is described by the displacement vector ui and an independent rotation vector ϕi , which are both functions of the position vector xi . A surface element dS transmits a force vector Ti dS and a couple vector Mi dS. The surface forces are in equilibrium with the nonsymmetric Cauchy stress ti j , and the surface couples are in equilibrium with the nonsymmetric couplestress mi j , such that Ti = n j t ji ,
Mi = n j m ji ,
(22.150)
where n j are the components of the unit vector orthogonal to the surface element under consideration. In the absence of body forces and body couples, the integral forms of the force and moment equilibrium conditions are Ti dS = 0 , (i jk x j Tk + Mi )dS = 0 . (22.151) S
S
Upon using (22.150) and the Gauss divergence theorem, equation (22.151) yields the differential equations of equilibrium t ji, j = 0 ,
m ji, j + i jk t jk = 0 .
(22.152)
22.13. Basic Equations of Micropolar Elasticity
399
For elastic deformations of micropolar continuum, the increase of the strain energy is due to external work done by the surface forces and couples, i.e., ˙ dV = (Ti u˙ i + Mi ϕ˙ i ) dS . W (22.153) V
S
The strain energy per unit volume is W, and the superposed dot denotes the time derivative. Incorporating (22.150) and (22.152) and using the divergence theorem gives ˙ = ti j γ˙i j + mi j κ˙ i j , W
(22.154)
where γi j = u j,i − i jk ϕk ,
κi j = ϕ j,i
(22.155)
are the nonsymmetric strain and curvature tensors, respectively. The symmetric and antisymmetric parts of γi j are γ(i j) = ei j =
1 (u j,i + ui, j ) , 2
(22.156) 1 γ = ωi j − ei jk ϕk , ωi j = (u j,i − ui, j ) . 2 In general, both ekk and κkk are different from zero. In addition, there is an identity κi j,k = κkj,i = ϕ j,ik. Assuming that the strain energy is a function of the strain and curvature tensors, W = W(γi j , κi j ), the differentiation and the comparison with (22.154) establishes the constitutive relations of micropolar elasticity ti j =
∂W , ∂γi j
mi j =
∂W . ∂κi j
(22.157)
In the case of material linearity, the strain energy is a quadratic function of the strain and curvature components 1 1 Ci jkl γi j γkl + Ki jkl κi j κkl . (22.158) 2 2 The fourthorder tensors of micropolar elastic moduli are Ci jkl and Ki jkl . Since the strain and curvature tensors are not symmetric, only reciprocal symmetries hold Ci jkl = Ckli j and Ki jkl = Kkli j . The stresses associated with (22.158) are ti j = Ci jkl γkl and mi j = Ki jkl κkl . In the case of isotropic micropolar elasticity, we have W=
Ci jkl = (µ + µ) ¯ δik δ jl + (µ − µ) ¯ δil δ jk + λ δi j δkl , Ki jkl = (α + α) ¯ δik δ jl + (α − α) ¯ δil δ jk + β δi j δkl ,
(22.159)
where µ, µ, ¯ λ and α, α, ¯ β are the Lametype ´ constants of isotropic micropolar elasticity. The symmetric and antisymmetric parts of the stress tensors are then t(i j) = 2µ ei j + λ ekk δi j , m(i j) = 2α κ(i j) + β κkk δi j ,
t = 2µ¯ (ωi j − i jk ϕk) , m = 2α¯ κ .
(22.160)
More generally, suppose that the elastic strain energy of a nonlinear isotropic material is given by (22.161) W = W Iγ , II γ , II¯ γ , III γ , Iκ , II κ , II¯ κ , III κ ,
400
22. Micropolar Elasticity
where Iγ = γkk , II γ = γi j γi j , II¯ γ = γi j γ ji , III γ =
1 i jk lmn γil γ jm γkn , 6
and similarly for the ﬁrst, second, and thirdorder invariants of the curvature tensor κi j . It follows that ti j = c1 δi j + c2 γi j + c¯2 γ ji + c3 ikl jmn γkm γln , mi j = k1 δi j + k2 κi j + k¯ 2 κ ji + k3 ikl jmn κkm κln ,
(22.162)
with c1 =
∂W , ∂ Iγ
∂W k1 = , ∂ Iκ
1 ∂W , 2 ∂ III γ
∂W , ∂ II γ
c¯2 = 2
∂W , ∂ II¯ γ
c3 =
∂W k2 = 2 , ∂ II κ
k¯ 2 = 2
∂W , ∂ II¯ κ
1 ∂W k3 = . 2 ∂ III κ
c2 = 2
(22.163)
22.14 Noether’s Theorem of Micropolar Elasticity The original Noether’s (1918) theorem on invariant variational principles states that there is a conservation law for the Euler–Lagrange differential equations associated with each inﬁnitesimal symmetry group of the Lagrangian functional. A comprehensive treatment of the general and various restricted forms of Noether’s theorem, with a historical outline, can be found in the book by Olver (1986). Noether’s theorem was applied by Gunther ¨ (1962), and Knowles and Sternberg (1972) to derive the conservation integrals of inﬁnitesimal nonpolar elasticity. When evaluated over a closed surface that does not embrace any singularity, these integrals give rise to conservation laws Jk = 0, Lk = 0, and M = 0. The law Jk = 0 applies to anisotropic linear or nonlinear material, the law Lk = 0 to isotropic linear or nonlinear material, and M = 0 to anisotropic linear material. If the surface embraces a singularity or inhomogeneity (defect), Eshelby (1951,1956) has shown that the value of Jk is not equal to zero but represents a conﬁgurational or energetic force on the embraced defect (vacancy, inclusion, dislocation). As discussed in Chapter 21, the pathindependent J integral of plane fracture mechanics has proved to be of great practical importance in modern fracture mechanics, allowing the prediction of the behavior at the crack tip from the values of the remote ﬁeld quantities (Rice, 1968a, 1968b). Budiansky and Rice (1973) interpreted the Lk and M integrals as the energetic forces (potential energy release rates) conjugate to rotation (by erosion/addition of material) and selfsimilar expansion (erosion) of the tractionfree void. Freund (1978) used the M conservation law for certain plane elastic crack problems to calculate the elastic stress intensity factor without solving the corresponding boundary value problem. Consider a family of coordinate mappings deﬁned by a vectorvalued function xˆ = f(x, η) ,
η ∈ (−η∗ , η∗ ) ,
(22.164)
such that f(x, 0) = x for all position vectors x. Consider also the families of the displacement and rotation mappings uˆ = g(u, η) ,
ϕ ˆ = h(ϕ, η) ,
(22.165)
22.14. Noether’s Theorem of Micropolar Elasticity
401
such that g(u, 0) = u and h(ϕ, 0) = ϕ for all displacement and rotation vectors u = u(x) and ϕ = ϕ(x). Finally, introduce a oneparameter family of functionals W(γˆi j , κˆ i j ) dVˆ , (22.166) Eη = Vˆ
where γˆi j =
∂ uˆ j − i jk ϕˆ k , ∂ xˆ i
and
dVˆ = det
κˆ i j =
∂ ϕˆ j , ∂ xˆ i
∂ xˆ j dV = det( f j,i ) dV . ∂ xi
When the parameter η is equal to zero, we have E0 = E = W(γi j , , κi j ) dV ,
(22.167)
(22.168)
(22.169)
V
which is the total strain energy within the volume V. The family Eη is, therefore, the family of functionals induced from the functional E by the families of mappings f, g, and h. Deﬁnition: The functional E is considered to be invariant at (u, ϕ) with respect to f, g, and h, if Eη = E ,
η ∈ (−η∗ , η∗ ) ,
(22.170)
and inﬁnitesimally invariant if
∂ Eη ∂η
η=0
= 0.
Theorem: If u and ϕ satisfy the equilibrium equations ∂W ∂W ∂ ∂ = 0, + i jk t jk = 0 , ∂ x j ∂γ ji ∂ x j ∂κ ji
(22.171)
(22.172)
for all x in V, then the total strain energy E is inﬁnitesimally invariant at (u, ϕ) with respect to mappings f, g, and h, if and only if ∂ (ai W + b j ti j + c j mi j ) = 0 , ∂ xi
(22.173)
where ai = fi (x, 0) , bi = gi (u, 0) − fk (x, 0) ui,k , ci = hi (ϕ, 0) − fk (x, 0) ϕi,k .
(22.174)
402
22. Micropolar Elasticity
The prime designates the derivative with respect to the parameter η, such that ∂ fi (x, η) . fi (x, 0) = ∂η 0
(22.175)
For brevity, the subscript 0 is used to indicate that the quantity within the brackets is evaluated at η = 0. The condition (22.173) implies the conservation law in the integral form (ai ni W + Ti bi + Mi ci ) dS = 0 , (22.176) S
for every surface S bounding a regular subregion of V. Proof: By differentiating (22.166) with respect to η and then setting η = 0, there follows ∂ Eη ∂ W ∂ γˆi j ∂ W ∂ κˆ i j = + W fk,k(x, 0) + dV . (22.177) ∂η 0 ∂γi j ∂η 0 ∂κi j ∂η 0 V The partial derivatives with respect to η appearing in (22.177) can be evaluated by using (22.167) and (22.168). This gives ∂g j (u, 0) ∂ γˆi j = uk,i − fk,i (x, 0)u j,k − i jk h k(ϕ, 0) , ∂η 0 ∂uk
∂ κˆ i j ∂η
=
∂h j (ϕ, 0) ∂ϕk
0
"
ˆ ∂(dV) ∂η
κik − fk,i (x, 0)κkj ,
(22.178)
# = fk,k (x, 0) dV . 0
The integrand in (22.177) is continuous on V, so that the integral vanishes if and only if its integrand vanishes at each x. The leading term of the integrand can be eliminated by using the identity ∂W ∂ ∂W γi j,k + κi j,k . [W fk(x, 0)] = W fk,k(x, 0) + fk(x, 0) ∂ xk ∂γi j ∂κi j Accordingly, the integrand in (22.177) becomes ∂W ∂W ∂ + di j = 0, [W fk (x, 0)] + Di j ∂ xk ∂γi j ∂κi j where
Di j = di j =
∂ γˆi j ∂η ∂ κˆ i j ∂η
− fk (x, 0) γi j,k ,
0
(22.179)
(22.180) − fk (x, 0) κi j,k .
0
Introducing the vectors bi and ci , deﬁned by (22.174), it can be readily veriﬁed that b j,i = Di j + i jk ck ,
c j,i = di j .
(22.181)
22.15. Conservation Integrals
403
Thus, there is an identity ∂W ∂ ∂W ∂W ∂W bj + cj = Di j + di j ∂ xi ∂γi j ∂κi j ∂γi j ∂κi j ∂W ∂ + i jk ck + ∂γi j ∂ xi
∂W ∂γi j
∂ bj + ∂ xi
∂W ∂κi j
(22.182) cj .
In view of the equilibrium equations (22.172), the last two terms on the righthand side of (22.182) are together equal to −c j jkl tkl , so that ∂W i jk ck − c j jkl tkl = 0 . ∂γi j
(22.183)
Consequently, (22.182) reduces to ∂ ∂W ∂W Di j + di j . (ti j b j + mi j c j ) = ∂ xi ∂γi j ∂κi j
(22.184)
Substituting (22.184) into (22.179) gives the desired result of (22.173). The conservation law (22.176) follows by applying the Gauss divergence theorem. The Knowles and Sternberg’s (1972) proof for inﬁnitesimal nonpolar elasticity follows by taking W = W(ei j ) and by setting mi j = 0 and t = 0.
22.15 Conservation Integrals in Micropolar Elasticity The strain energy in micropolar elasticity is invariant under the mappings xˆ i = xi0 η + Qi j (η) x j ,
uˆ i = Qi j (η) u j ,
ϕˆ i = Qi j (η) ϕ j ,
(22.185)
where xi0 is a constant vector, Qi j (η) is an orthogonal tensor in the case of an isotropic material, and Qi j = δi j (Kronecker delta) in the case of a fully anisotropic material. Thus, since the invariance necessarily implies an inﬁnitesimal invariance, the corresponding conservation laws follow from (22.176). Indeed, we have fi (x, 0) = xi0 + qi j x j ,
gi (u, 0) = qi j u j ,
hi (ϕ, 0) = qi j ϕ j ,
(22.186)
and ai = xi0 + qi j x j , 0 + qmn xn ) ui,m , bi = qi j u j − (xm
(22.187)
0 + qmn xn ) ϕi,m , ci = qi j ϕ j − (xm
where qi j = Qi j (0). When this is substituted into (22.176), we obtain xi0 (W ni − Ti ui, j − Mi ϕi, j ) dS S
(W ni x j + Ti u j + Mi ϕ j − Tl ul,i x j − Ml ϕl,i x j ) dS = 0 .
+ qi j S
For a fully anisotropic material qi j = 0, and by choosing the vector xi0 to be a unit vector in the direction k (xi0 = δik, for each value of k = 1, 2, 3), the above equation gives Jk = (Wnk − Tk uk, j − Mk ϕk, j ) dS = 0 . (22.188) S
404
22. Micropolar Elasticity
For an isotropic material qi j are the components of an orthogonal tensor, and we can take qi j = i jk for k = 1, 2, 3, so that, in addition to (22.188), there is a conservation law Lk = i jk (Wni x j + Ti u j + Mi ϕ j − Tl ul,i x j − Ml ϕl,i x j ) dS = 0 . (22.189) S
If the micropolar terms are omitted, the above conservation laws reduce to those of the classical nonpolar elasticity (Knowles and Sternberg, 1972; Budiansky and Rice, 1973). Using the energymomentum tensor of micropolar elastic ﬁeld, Pi j = W δi j − tik uk, j − mik ϕk, j , the derived conservation integrals can be recast as Jk = P jk n j dS ,
(22.190)
(22.191)
S
Lk = i jk
(Pli x j + tli u j + mli ϕ j ) nl dS .
(22.192)
S
22.16 Conservation Laws for Plane Strain Micropolar Elasticity In twodimensional plane strain problems within (x1 , x2 ) plane, the components ϕ3 , M3 , m13 , and m23 are generally different from zero, whereas other rotation, moment, and couplestress components are equal to zero. By taking S to be a cylindrical surface with its generatrix parallel to x3 axis and with its two ﬂat bases bounded by a curve C, integration in (22.191) and (22.192) gives (per unit length in x3 direction) Pβα nβ dC , (22.193) Jα = C
L = αβ3
(Pγ α xβ + tγ α uβ ) nγ dC .
(22.194)
S
The energymomentum tensor of the plane strain micropolar elasticity is Pαβ = W δαβ − tαγ uγ ,β − mα3 ϕ3,β .
(22.195)
The summation in repeated Greek indices is over 1 and 2. The J1 integral from (22.193) was used by Atkinson and Leppington (1974) to calculate the energy release rate for a semiinﬁnite crack within a strip of thickness h. Xia and Hutchinson (1996) also used the J1 integral to study the elastoplastic crack tip ﬁeld in a straingradient dependent material described by the deformationtype theory of plasticity (see Chapter 26).
22.17 M Integral of Micropolar Elasticity In contrast to classical elasticity, there is no M conservation law of micropolar elasticity. In twodimensional case this was originally observed by Atkinson and Leppington (1977), and elaborated in the threedimensional context by Lubarda and Markenscoff (2003). Consider a family of scalechanges η (22.196) ui . xˆ i = (1 + η)xi , uˆ i = 1 − 2
22.17. M Integral of Micropolar Elasticity
405
It is easily veriﬁed that the total strain energy of a nonpolar elastic material with a quadratic strain energy representation is inﬁnitesimally invariant under (22.196). This is, however, not so in the case of micropolar elasticity, because the material length parameter, whose square is the ratio of the representative micropolar elastic moduli l2 = [K]/[C], remains unaltered by the transformation (22.196). Indeed, since the angle change corresponding to (22.196) is ϕˆ i =
1 − η/2 ϕi , 1+η
(22.197)
which follows from a simple dimensional argument (u ∼ xϕ, uˆ ∼ xˆ ϕ), ˆ we have 1 − η/2 γi j , 1+η
γˆi j =
κˆ i j =
1 − η/2 κi j . (1 + η)2
(22.198)
We assume here that η∗ < 1. Thus, for a linear micropolar material with a quadratic strain energy representation, 1 1 η 2 1− mi j κi j dV , (1 + η) ti j γi j + (22.199) Eη = 2 2 1+η V so that Eη = E0 = E, and
∂ Eη ∂η
=−
0
mi j κi j dV = 0 .
(22.200)
V
This shows that the total strain energy E is not inﬁnitesimally invariant with respect to the considered family of scale changes. Consequently, there is no M conservation law in micropolar elasticity. Actually, the value of the M integral is equal to the expression in (22.200). This follows from 3 hi (ϕ, 0) = − ϕi , 2
(22.201)
1 3 W xi ni − Ti ui − Mi ϕi − Ti x j ui, j − Mi x j ϕi, j dS . 2 2
(22.202)
fi (x, 0) = xi , and
M= S
1 gi (u, 0) = − ui , 2
Upon using the Gauss divergence theorem, the evaluation of the last integral gives (22.203) M = − mi j κi j dV . V
In the derivation it is noted that W,k = ti j γi j,k + mi j κi j,k ,
(22.204)
and that, for the quadratic strain energy representation, the identities hold ti j γi j,k = ti j,k γi j ,
mi j κi j,k = mi j,k κi j .
(22.205)
In terms of the energymomentum tensor (22.190), the M integral of (22.202) can be rewritten as 1 3 (22.206) Pi j x j − ti j u j − mi j ϕ j ni dS . M= 2 2 S
406
22. Micropolar Elasticity
The plane strain counterpart is
M=
(Pαβ xβ − mα3 ϕ3 ) nα dC .
(22.207)
C
If the polar effects are neglected, the couplestress vanishes and the conservation law M = 0 of the classical linear isotropic elasticity is obtained. This is 1 W xi ni − Ti ui − Ti x j ui, j dS = 0 (22.208) M= 2 S for threedimensional nonpolar elasticity, and M= (W xα nα − Tα xβ uα,β ) dC = 0
(22.209)
C
for twodimensional nonpolar elasticity.
22.18 Suggested Reading Brulin, O., and Hsieh, R. K. T., eds. (1982), Mechanics of Micropolar Media, World Scientiﬁc, Singapore. Dhaliwal, R. S., and Singh, A. (1987), Micropolar Thermoelasticity. In Thermal Stresses II (R. B. Hetnarski, ed.), pp. 269–328, Elsevier, Amsterdam. Eringen, A. C. (1999), Microcontinuum Field Theories, SpringerVerlag, New York. Jasiuk, I., and OstojaStarzewski, M. (1995), Planar Cosserat Elasticity of Materials with Holes and Intrusions, Appl. Mech. Rev., Vol. 48, pp. S11–S18. Koiter, W. T. (1964), CoupleStresses in the Theory of Elasticity, Proc. Ned. Akad. Wet. (B), Vol. 67, I: pp. 17–29, II: pp. 30–44. Lubarda, V. A. (2003), Circular Inclusions in AntiPlane Strain Couple Stress Elasticity, Int. J. Solids Struct., Vol. 40, pp. 3827–3851. Lubarda, V. A., and Markenscoff, X. (2003), On Conservation Integrals in Micropolar Elasticity, Phil. Mag. A, Vol. 83, pp. 1365–1377. Mindlin, R. D., (1964), MicroStructure in Linear Elasticity, Arch. Ration. Mech. Anal., Vol. 16, pp. 51–78. Mindlin, R. D., and Tiersten, H. F. (1962), Effects of CoupleStresses in Linear Elasticity, Arch. Ration. Mech. Anal., Vol. 11, pp. 415–448. Nowacki, W. (1986), Theory of Asymmetric Elasticity, Pergamon, Oxford, UK. Stojanovi´c, R. (1970), Recent Developments in the Theory of Polar Continua, CISM Lecture Notes, SpringerVerlag, Wien. Toupin, R. A. (1962), Perfectly Elastic Materials with Couple Stresses, Arch. Ration. Mech. Anal., Vol. 11, pp. 385–414.
PART 5: THIN FILMS AND INTERFACES
23 Dislocations in Bimaterials
23.1 Introduction This chapter contains a detailed analysis of straight (edge and screw) dislocations near the bimaterial interface or near the free surface of a semiinﬁnite medium. A general elastic study of straight dislocations and dislocation loops was presented earlier in Chapter 18. Here, we focus on those aspects of the dislocation analysis that are of importance to study the strain relaxation in thin ﬁlms. We ﬁrst derive the stress ﬁelds for straight dislocations near bimaterial interfaces and then specialize these results to dislocations near the free surfaces or rigid boundaries. An energy analysis of dislocations beneath the free surface of a semiinﬁnite body is also presented.
23.2 Screw Dislocation Near a Bimaterial Interface Consider a screw dislocation near a bimaterial interface at a distance h from it (Fig. 23.1a). The Burgers vector of dislocation is in the z direction and has the magnitude bz. The shear modulus and Poisson’s ratio of the material (1) are µ1 and ν1 ; those of material (2) are µ2 and ν2 . A complete adherence between the two materials is assumed, so that the displacement and traction components are continuous across the interface. The only nonvanishing displacement component is the outofplane displacement bz (θ1 − c θ2 ) , 2π
(23.1)
bz [(1 + c)θ1 − cπ ] , 2π
(23.2)
u(1) z = u(2) z =
where the constant c is a nondimensional shear modulus mismatch parameter, deﬁned by c=
µ1 − µ2 . µ1 + µ2
(23.3)
The above displacement ﬁeld is continuous across the interface, and the slip discontinuity of amount bz is imposed along the cut from x = h to x → ∞. The two sets of polar coordinates 407
408
23. Dislocations in Bimaterials
y
y (x,y) r2 θ2
h
h
r1
S
(x,y) r
θ1
S
x
(1)
(2)
θ
x
(1)
(2)
(a)
(b)
Figure 23.1. (a) A screw dislocation with the Burgers vector bz at a distance h from the bimaterial interface. (b) An interface screw dislocation.
shown in Fig. 23.1a are related to the Cartesian coordinates (x, y) by r12 = (x − h)2 + y2 , tan θ1 =
r22 = (x + h)2 + y2 ,
y , x−h
tan θ2 =
y . x+h
(23.4)
The utilized angles have the range 0 ≤ θ1 ≤ 2π ,
−π ≤ θ2 ≤ π .
(23.5)
The stress components associated with the displacement ﬁeld in (23.1) and (23.2) are obtained from Hooke’s law as (1) µ1 bz y ∂uz y (1) =− , (23.6) = µ1 − c σzx ∂x 2π r12 r22 (1)
(1) σzy
µ1 bz ∂uz = = µ1 ∂y 2π
x−h x+h −c , r12 r22
(23.7)
and (2)
(2) = µ2 σzx
µ2 bz y ∂uz =− (1 + c) 2 , ∂x 2π r1
(23.8)
(2)
(2) σzy = µ2
µ2 bz x−h ∂uz = (1 + c) 2 . ∂y 2π r1
(23.9)
The force exerted by the interface on the dislocation is (1) (h, 0) . Fx = bzσzy
(23.10)
Excluding the divergent part of the stress at the core center of the dislocation, this gives µ1 bz2 . (23.11) 4π h Depending on the sign of c, the dislocation may be attracted or repelled by the interface. Fx = −c
23.2. Screw Dislocation Near an Interface
409
23.2.1 Interface Screw Dislocation For an interface screw dislocation (Fig. 23.1b) we take h = 0, r1 = r2 = r , θ1 = θ, and θ, y ≥ 0+ , θ2 = (23.12) θ − 2π , y ≤ 0− , with 0 ≤ θ ≤ 2π . The displacement ﬁeld is u(1) z = u(1) z =
bz (1 − c)θ , 2π
y ≥ 0+ ,
bz [(1 − c)θ + 2π c] , 2π
u(2) z =
y ≤ 0− ,
bz [(1 + c)θ − cπ] . 2π
(23.13)
(23.14)
(23.15)
The corresponding stresses are (1) σzx =−
(1) σzy =
µ1 bz (1 − c)y , 2π r2
µ1 bz (1 − c)x , 2π r2
(23.16)
(23.17)
and (2) =− σzx
(2) = σzy
µ2 bz (1 + c)y , 2π r2
µ2 bz (1 + c)x . 2π r2
(23.18)
(23.19)
23.2.2 Screw Dislocation in a Homogeneous Medium If two materials have the same shear modulus (e.g., homogeneous medium), the parameter c = 0 and, with h = 0, the results reduce to uz = σzx = − σzy =
bz θ, 2π
(23.20)
µbz y , 2π r 2
(23.21)
µbz x . 2π r 2
(23.22)
23.2.3 Screw Dislocation Near a Free Surface If a dislocation is near the free surface of a semiinﬁnite homogeneous medium, we take µ2 = 0 and c = 1. The displacement and stress ﬁelds in this case are uz =
bz (θ1 − θ2 ) , 2π
(23.23)
410
23. Dislocations in Bimaterials
σzx
σzy
µbz =− 2π
µbz = 2π
y y − 2 2 r1 r2
,
x−h x+h − . r12 r22
(23.24)
(23.25)
The displacement discontinuity is imposed along the cut from x = 0 to x = h. The ﬁelds are recognized to be the superposition of two inﬁnite medium ﬁelds, one for a dislocation at the point x = h, y = 0 and the other for an opposite (image) dislocation at the point x = −h, y = 0. The force exerted by the free surface on the dislocation is Fx = −
µ1 bz2 . 4π h
(23.26)
The dislocation is attracted by the free surface. 23.2.4 Screw Dislocation Near a Rigid Boundary If the second material is rigid, we take µ2 → ∞ and c = −1. The displacement and stress ﬁelds are bz bz (θ1 + θ2 ) − , (23.27) uz = 2π 2 µbz y y σzx = − , (23.28) + 2π r12 r22 µbz x − h x + h . (23.29) σzy = + 2π r12 r22 The displacement vanishes along the rigid boundary, and the discontinuity is imposed along the cut from x = h to x → ∞. The ﬁelds are recognized to be the superposition of two inﬁnite medium ﬁelds, one for a dislocation at the point x = h, y = 0 and the other for an alike dislocation at the point x = −h, y = 0. The force exerted by the rigid boundary on the dislocation is Fx =
µ1 bz2 . 4π h
(23.30)
The dislocation is repelled by the rigid boundary.
23.3 Edge Dislocation (bx ) Near a Bimaterial Interface Two edge dislocations near the bimaterial interface, one with the Burgers vector bx and the other with the Burgers vector by , are shown in Figs. 23.2a and b. Consider ﬁrst the stress ﬁeld for an edge dislocation with the Burgers vector bx . The corresponding Airy stress functions are (Dundurs, 1969) (1)
(2)
= − k1 bx [r1 ln r1 sin θ1 + (a − 1)r2 ln r2 sin θ2 sin θ2 − qh sin 2θ2 − 2h + aβr2 θ2 cos θ2 , r2
(23.31)
= −ak1 bx [r1 ln r1 sin θ1 − β(r1 θ1 cos θ1 + 2hθ1 )] .
(23.32)
23.3. Edge Dislocation (bx ) Near an Interface
411
y
y
(x,y)
(x,y) r2
r1
θ2
θ1
θ1
x
h
h
(1)
(2)
r1
θ2
x
h
h
r2
(1)
(2)
(a)
(b)
Figure 23.2. (a) An edge dislocation with the Burgers vector bx at a distance h from the bimaterial interface. (b) The same for an edge dislocation with the Burgers vector by .
The parameters are introduced µ1 , k1 = 2π(1 − ν1 )
a=
1+α , 1 − β2
q=
α−β , 1+β
(23.33)
and α=
(1 − ν1 )µ2 − (1 − ν2 )µ1 , (1 − ν1 )µ2 + (1 − ν2 )µ1
2β =
(1 − 2ν1 )µ2 − (1 − 2ν2 )µ1 . (1 − ν1 )µ2 + (1 − ν2 )µ1
(23.34)
The Airy stress function yields the stress components according to σxx =
∂2 , ∂ y2
σ yy =
∂2 , ∂ x2
σxy = −
∂2 . ∂ x∂ y
(23.35)
The polar coordinates counterparts are 1 ∂2 1 ∂ σrr = + 2 , r ∂r r ∂θ 2
σθ θ
∂2 = , ∂r 2
σr θ
∂ =− ∂r
1 ∂ r ∂θ
.
(23.36)
The Tables 23.1–23.5 (reproduced from the results listed by Dundurs and Mura, 1964) give the displacement and stress components corresponding to some typical forms of the Airy stress function. In these tables, ϑ is the Kolosov constant deﬁned, as in (8.136), by ⎧ ⎪ ⎨3 − 4ν , plane strain , (23.37) ϑ = 3−ν ⎪ ⎩ , plane stress . 1+ν By using the results from Table 23.4, we obtain
(1) σxx
3(x − h)2 + y2 3(x + h)2 + y2 +q 4 r1 r24 3(x + h)2 − y2 1 + 4qhx + aβ 2 , r2 r26
= − k1 bx y
(23.38)
412
23. Dislocations in Bimaterials
Table 23.1. Rectangular displacement components 2Gux
2Gu y
r ln r cos θ
1 2 (ϑ
r ln r sin θ
− 12 (ϑ + 1)θ −
r θ cos θ
1 2 (ϑ
r θ sin θ cos θ r sin θ r cos 2θ sin 2θ θ ln r
1 2 (ϑ
1 r2
x2
− 1) ln r −
− 1)θ +
r2 xy r2
xy
+
+ 1)θ −
1 2 (ϑ
− 1) ln r +
x2 r2
1 2 (ϑ
2x 2
2xy
r4
r4
2xy
1
r4
r2
(ϑ − 3) (ϑ − 1)
x r2 y r2
+ +
4x 3 r4 4x 2 y r4
y x
−
x2 r2
r2
r4 y r2
x r2
−
+
4x 2 y r4
4x 3 r4
x r2 y r2
2µur r ln r cos θ
1 2 [(ϑ
+ 1)θ sin θ + (ϑ − 1) ln r cos θ − cos θ]
r ln r sin θ
1 2 [−(ϑ
r θ cos θ
1 2 [(ϑ
− 1)θ cos θ − (ϑ + 1) ln r sin θ + sin θ]
r θ sin θ
1 2 [(ϑ
− 1)θ sin θ + (ϑ + 1) ln r cos θ − cos θ]
cos θ
sin θ r
sin θ
+ 1)θ cos θ + (ϑ − 1) ln r sin θ − sin θ]
r2 r2
cos 2θ
(ϑ + 1)
cos 2θ r
sin 2θ
(ϑ + 1)
sin 2θ r
θ
0
ln r
−
1 r
r2
xy
Table 23.2. Radial displacement component
cos θ r
x2
2x 2
(ϑ + 3)
−
r2
− 1)θ −
−(ϑ + 1)
−
r2 −
r2
− 12 (ϑ + 1) ln r −
r2
+ 1) ln r −
xy
1 2 (ϑ
23.3. Edge Dislocation (bx ) Near an Interface
413
Table 23.3. Circumferential displacement component 2µuθ r ln r cos θ
1 2 [(ϑ
+ 1)θ cos θ − (ϑ − 1) ln r sin θ − sin θ]
r ln r sin θ
1 2 [(ϑ
+ 1)θ sin θ + (ϑ − 1) ln r cos θ + cos θ]
r θ cos θ
1 2 [−(ϑ
r θ sin θ
1 2 [(ϑ
cos θ r
sin θ
sin θ r
− 1)θ sin θ − (ϑ + 1) ln r cos θ − cos θ]
− 1)θ cos θ − (ϑ + 1) ln r sin θ − sin θ]
r2 cos θ
−
r2
cos 2θ
−(ϑ − 1)
sin 2θ
(ϑ − 1)
θ
−
ln r
0
sin 2θ r
cos 2θ r
1 r
Table 23.4. Rectangular stress components σxx r ln r cos θ r ln r sin θ r θ cos θ r θ sin θ
−
x
y
+
2x 2 y
y
r4
r2 −
−
r4
12x 2 r4 4xy r4 − −
r6 8x 2 y
−
r4
−
r6 −
−
−
2y r2
r4 2y r4
4
r6
r2
16x 3 y r6
−
r4
r4
r2
+
2x 2
1
r4
r2
−
2x 2 y
−
r4
+ +
r4
2x 3
−
r4
2x
+
r2
2x 3 r4
2x 2 y
r4
r4
8x 3
2y
r6
r4
8x 2 y
−
r6
20x 2 r4
12xy
2xy
1
x r2
2x 2 y
+
r2
r4
2x 3
r4
y
2x 2 y
+
−
2xy
−
r4
−
6x
16x 4
2x 3
−
r2 8x 3
σxy −
2x
r4
2y
ln r
r2
2x 3
sin θ r
θ
3x
r4
r4
6x
sin 2θ
2x 3
2x 2 y
cos θ r
cos 2θ
+
r2
r2 −
σ yy
+
+
−
6x r4
16x 4
8xy
r6
r4
16x 3 y
2
r6
r2 −
r2
2x 2
2xy
r4
r4
r6
+
−
− 1
8x 2 y 8x 3 r6 16x 3 y r6
16x 2 r4 +
2x 2 r4
+
16x 4 r6
414
23. Dislocations in Bimaterials
Table 23.5. Polar stress components σrr
σθ θ cos θ r sin θ r
cos θ r sin θ r sin θ −2 r cos θ 2 r cos θ −2 3 r sin θ −2 3 r cos 2θ −4 r2 sin 2θ −4 2 r
r ln r cos θ r ln r sin θ r θ cos θ r θ sin θ cos θ r sin θ r cos 2θ sin 2θ θ
0
0
0 cos θ r3 sin θ
2
r3
(1) σ yy = k1 bx y
2
sin θ
r3 cos θ
−2
0
2
r3 sin 2θ
r2 cos 2θ r2
1 r2
−
r2
−2
0
0
1
sin θ r cos θ − r
0
2
0
ln r
σr θ
1
0
r2
(x − h)2 − y2 (x + h)2 − y2 1 +q + aβ 2 4 4 r1 r2 r2
2(x + h)3 − 3x(x + h)2 + 2(x + h)y2 + xy2 , − 4qh r26 (1) = k1 bx σxy
(x − h)[(x − h)2 − y2 ] (x + h)[(x + h)2 − y2 ] + q r14 r24
! (x + h)4 − 2x(x + h)3 + 6x(x + h)y2 − y4 x+h − 2qh + aβ , r22 r26 and
(2) σxx = −ak1 bx y
(2) = ak1 bx y σ yy
(2) σxy
= ak1 bx
3(x − h)2 + y2 x 2 − h2 + 2β , r14 r14
(x − h)2 − y2 2h(x − h) − y2 , + 2β r14 r14
(x − h)[(x − h)2 − y2 ] h(x − h)2 − xy2 + 2β . r14 r14
(23.39)
(23.40)
(23.41)
(23.42)
(23.43)
The force exerted by the interface on the dislocation is obtained from (1) (h, 0) , Fx = bx σxy
(23.44)
23.3. Edge Dislocation (bx ) Near an Interface
y
415
y (x,y)
(x,y)
r
r
θ
θ
x
x
(1)
(2)
(1)
(2)
(a)
(b)
Figure 23.3. (a) An interface dislocation with the Burgers vector bx , and (b) with the Burgers vector by .
by excluding the divergent part of the stress at the core center of the dislocation. This gives Fx = −(1 − a)
k1 bx2 . 2h
(23.45)
Depending on the value of a, the dislocation may be attracted or repelled by the interface. 23.3.1 Interface Edge Dislocation The Airy stress functions for an interface dislocation with the Burgers vector bx (Fig. 23.3a) are (1)
= −ak1 bx [r ln r sin θ + βr θ cos θ] ,
(23.46)
(2)
= −ak1 bx [r ln r sin θ − βr θ cos θ] .
(23.47)
The rectangular stress components in the material (1) are (1) = −ak1 bx y σxx
(3 − 2β)x 2 + y2 , (x 2 + y2 )2
(23.48)
(1) σ yy = ak1 bx y
x 2 − (1 − 2β)y2 , (x 2 + y2 )2
(23.49)
(1) σxy = ak1 bx x
x 2 − (1 − 2β)y2 . (x 2 + y2 )2
(23.50)
The same expressions apply for the material (2), provided that β is replaced with −β. The expressions have simple counterparts in polar coordinates. The radial stresses are σrr(1) = −ak1 bx (1 − 2β)
sin θ , r
(23.51)
σrr(2) = −ak1 bx (1 + 2β)
sin θ . r
(23.52)
416
23. Dislocations in Bimaterials
The hoop and shear stresses in both media are σθ θ = −ak1 bx
sin θ , r
σr θ = ak1 bx
cos θ . r
(23.53)
These expressions can be deduced by using the results listed in Tables 23.4 and 23.5. The radial displacements are ak1 bx r [1 − 2ν1 − 2β(1 − ν1 )] ln sin θ 2µ1 bx
µ1 (1 + β) sin θ , − [2(1 − ν1 ) − β(1 − 2ν1 )]θ cos θ − 2µ2
ur(1) = −
(23.54) +
y≥0 ,
ak1 bx r [1 − 2ν1 − 2β(1 − ν1 )] ln sin θ 2µ1 bx
µ1 − [2(1 − ν1 ) − β(1 − 2ν1 )](θ − 2π) cos θ − (1 + β) sin θ , 2µ2
ur(1) = bx cos θ −
ur(2) = −
(23.55) −
y≤0 ,
ak1 bx r sin θ [1 − 2ν2 + 2β(1 − ν2 )] ln 2µ2 bx
1 − [2(1 − ν2 ) + β(1 − 2ν2 )]θ cos θ − (1 + β) sin θ . 2
(23.56)
These expressions satisfy the continuity across the interface and give a slip discontinuity across y = 0, x > 0. The circumferential displacements are (1)
uθ = −
ak1 bx r [1 − 2ν1 − 2β(1 − ν1 )] ln cos θ 2µ1 bx
+ [2(1 − ν1 ) − β(1 − 2ν1 )]θ sin θ
µ1 + [1 − β − (1 + β)] cos θ , y ≥ 0+ , 2µ2 (1)
uθ = −
ak1 bx r [1 − 2ν1 − 2β(1 − ν1 )] ln cos θ 2µ1 bx
+ [2(1 − ν1 ) − β(1 − 2ν1 )]θ sin θ − C2 sin θ
µ1 + [1 − β − (1 + β)] cos θ , y ≤ 0− , 2µ2 (2)
uθ = −
(23.57)
ak1 bx r [1 − 2ν2 + 2β(1 − ν2 )] ln cos θ 2µ2 bx
+ [2(1 − ν2 ) + β(1 − 2ν2 )]θ sin θ −
C2
1 sin θ + (1 + β) cos θ . 2
(23.58)
(23.59)
The continuity conditions across the interface specify the constants C2 and C2 as
µ1 C2 = π 2(1 − ν1 ) − β(1 − 2ν1 ) − [2(1 − ν2 ) + β(1 − 2ν2 )] , µ2
π µ2 2(1 − ν2 ) + β(1 − 2ν2 ) − C2 = [2(1 − ν1 ) − β(1 − 2ν1 )] . 2 µ1
(23.60)
23.3. Edge Dislocation (bx ) Near an Interface
417
It is recalled that the rigid body displacements in polar coordinates are ur = C1 cos θ + C2 sin θ ,
uθ = −C1 sin θ + C2 cos θ + C3r ,
(23.61)
with the rectangular counterparts ux = C1 + C3 y and u y = C2 − C3 x. 23.3.2 Edge Dislocation in an Inﬁnite Medium If two materials have the same elastic properties, the introduced parameters are α = β = q = 0 and a = 1. Taking h = 0, the Airy stress function becomes µ , (23.62) = −kbx r ln r sin θ , k = 2π (1 − ν) with the corresponding stresses σxx = −kbx y
The displacements are
3x 2 + y2 , (x 2 + y2 )2
(23.63)
σ yy = kbx y
x 2 − y2 , (x 2 + y2 )2
(23.64)
σxy = kbx x
x 2 − y2 . (x 2 + y2 )2
(23.65)
1 xy bx −1 y + ux = , tan 2π x 2(1 − ν) x 2 + y2
bx uy = − 2π
x 2 + y2 1 1 − 2ν x 2 − y2 . ln + 4(1 − ν) bx2 4(1 − ν) x 2 + y2
(23.66)
(23.67)
The counterparts in polar coordinates are σrr = σθ θ = −kbx
sin θ , r
σr θ = kbx
cos θ , r
(23.68)
with the displacements
kbx 1 r ur = − sin θ − 2(1 − ν)θ cos θ − sin θ , (1 − 2ν) ln 2µ bx 2
(23.69)
kbx 1 r cos θ + 2(1 − ν)θ sin θ + cos θ . (1 − 2ν) ln 2µ bx 2
(23.70)
uθ = −
23.3.3 Edge Dislocation Near a Free Surface For an edge dislocation near a free surface (Fig. 23.4a) we take µ2 = 0, so that α = q = −1 and a = 0. The Airy stress function becomes = − kbx [r1 ln r1 sin θ1 − r2 ln r2 sin θ2 sin θ2 + h sin 2θ2 − 2h . r2
(23.71)
418
23. Dislocations in Bimaterials
h θ2
h θ2
y r2
h θ1
x
y r2
h
r1
θ1
(x,y)
x
(a)
r1 (x,y)
(b)
Figure 23.4. (a) A dislocation with the Burgers vector bx at a distance h from the free surface. (b) Same for a dislocation with the Burgers vector by .
The corresponding stresses are 3(x − h)2 + y2 3(x + h)2 + y2 3(x + h)2 − y2 σxx = −kbx y , − − 4hx r14 r24 r26 (x − h)2 − y2 (x + h)2 − y2 − σ yy = kbx y r14 r24 2(x + h)3 − 3x(x + h)2 + 2(x + h)y2 + xy2 , + 4h r26 (x − h)[(x − h)2 − y2 ] (x + h)[(x + h)2 − y2 ] − r14 r24 ! (x + h)4 − 2x(x + h)3 + 6x(x + h)y2 − y4 . + 2h r26
(23.72)
(23.73)
σxy = kbx
(23.74)
These expressions were originally derived by Head (1953a, 1953b). The force exerted by the free surface on the dislocation is Fx = −
k1 bx2 , 2h
(23.75)
which is an attraction toward the free surface. 23.3.4 Edge Dislocation Near a Rigid Boundary In this case we take µ2 → ∞, and with µ1 = µ and ν1 = ν, we have α = − 1,
2β =
8(1 − ν)2 , a= 3 − 4ν
1 − 2ν , 1−ν
q=
1 , 3 − 4ν
4(1 − ν)(1 − 2ν) aβ = . 3 − 4ν
(23.76)
The Airy stress function is
= −kbx r1 ln r1 sin θ1 + (a − 1)r2 ln r2 sin θ2
sin θ2 − qh sin 2θ2 − 2h r2
+ aβr2 θ2 cos θ2 .
(23.77)
23.4. Edge Dislocation (by ) Near an Interface
419
The corresponding stresses are
3(x − h)2 + y2 3(x + h)2 + y2 + q r14 r24 3(x + h)2 − y2 1 + 4qhx + aβ 2 , 6 r2 r2
σxx = −kbx y
σ yy = kbx y
(x − h)2 − y2 (x + h)2 − y2 1 +q + aβ 2 4 r1 r24 r2
2(x + h)3 − 3x(x + h)2 + 2(x + h)y2 + xy2 , − 4qh r26 (x − h)[(x − h)2 − y2 ] (x + h)[(x + h)2 − y2 ] + q r14 r24
σxy = kbx
! (x + h)4 − 2x(x + h)3 + 6x(x + h)y2 − y4 x+h . − 2qh + aβ r22 r26
(23.78)
(23.79)
(23.80)
23.4 Edge Dislocation (by ) Near a Bimaterial Interface Consider next an edge dislocation with the Burgers vector by (Fig. 23.2b). The corresponding Airy stress functions are (1)
= k1 by [r1 ln r1 cos θ1 + (a − 1)r2 ln r2 cos θ2 cos θ2 − qh 2 ln r2 − cos 2θ2 + 2h − aβr2 θ2 sin θ2 , r2
(23.81)
= ak1 by [r1 ln r1 cos θ1 + β(2h ln r1 + r1 θ1 sin θ1 )] .
(23.82)
(2)
This gives (1) = k1 by σxx
(x − h)[(x − h)2 − y2 ] (x + h)[(x + h)2 − y2 ] + q r14 r24
! (x + h)4 + 2x(x + h)3 − 6x(x + h)y2 − y4 x+h − 2qh − aβ , r22 r26 (1) = k1 by σ yy
(x − h)[(x − h)2 + 3y2 ] (x + h)[(x + h)2 + 3y2 ] +q 4 r1 r24
! (x + h)4 − 2x(x + h)3 + 6x(x + h)y2 − y4 x+h − 2qh + aβ , r22 r26 y[(x − h)2 − y2 ] y[(x + h)2 − y2 ] +q 4 r1 r24 ! 3(x + h)2 − y2 y − 4qhxy − aβ , r22 r26
(23.83)
(23.84)
(1) σxy = k1 by
(23.85)
420
23. Dislocations in Bimaterials
and
(x − h)[(x − h)2 − y2 ] x(x − h)2 − hy2 , + 2β r14 r14
(23.86)
(x − h)[(x − h)2 + 3y2 ] h(x − h)2 − xy2 − 2β , r14 r14
(23.87)
(2) σxx = ak1 by
(2) = ak1 by σ yy
(2) σxy
= ak1 by
y[(x − h)2 − y2 ] x 2 − h2 . + 2βy r14 r14
(23.88)
23.4.1 Interface Edge Dislocation The Airy stress functions in this case (Fig. 23.3b) are (1)
= ak1 by [r ln r cos θ − βr θ sin θ] ,
(23.89)
(2)
= ak1 by [r ln r cos θ + βr θ sin θ] .
(23.90)
The stress components in the material (1) are (1) σxx = ak1 by x
(1 − 2β)x 2 − y2 , (x 2 + y2 )2
(23.91)
(1) = ak1 by x σ yy
x 2 + (3 − 2β)y2 , (x 2 + y2 )2
(23.92)
(1) σxy = ak1 by y
(1 − 2β)x 2 − y2 . (x 2 + y2 )2
(23.93)
The same expressions hold in material (2), provided that β is replaced with −β. The expressions have simple counterparts in polar coordinates. The radial stresses are σrr(1) = ak1 by (1 − 2β)
cos θ , r
(23.94)
σrr(2) = ak1 by (1 + 2β)
cos θ . r
(23.95)
The hoop and shear stresses in both media are given by σθ θ = ak1 by
cos θ , r
σr θ = ak1 by
sin θ . r
(23.96)
The circumferential displacements are (1)
uθ = −
ak1 by r [1 − 2ν1 − 2β(1 − ν1 )] ln sin θ 2µ1 by
− [2(1 − ν1 ) − β(1 − 2ν1 )]θ cos θ
µ1 + (1 + β) sin θ , y ≥ 0+ , 2µ2
(23.97)
23.4. Edge Dislocation (by ) Near an Interface (1)
uθ = by cos θ −
421
ak1 by r sin θ [1 − 2ν1 − 2β(1 − ν1 )] ln 2µ1 by
− [2(1 − ν1 ) − β(1 − 2ν1 )](θ − 2π ) cos θ
µ1 + (1 + β) sin θ , y ≤ 0− , 2µ2 (2)
uθ = −
ak1 by r [1 − 2ν2 + 2β(1 − ν2 )] ln sin θ 2µ2 by
− [2(1 − ν2 ) + β(1 − 2ν2 )]θ cos θ +
(23.98)
(23.99)
1 (1 + β) sin θ . 2
These expressions satisfy the continuity across the interface and give a displacement discontinuity of amount by across y = 0, x > 0. The radial displacements are ur(1) =
ak1 by r [1 − 2ν1 − 2β(1 − ν1 )] ln cos θ 2µ1 by + [2(1 − ν1 ) − β(1 − 2ν1 )]θ sin θ
µ1 − [1 − β − (1 + β)] cos θ , y ≥ 0+ , 2µ2
ur(1) =
ak1 by r [1 − 2ν1 − 2β(1 − ν1 )] ln cos θ 2µ1 by + [2(1 − ν1 ) − β(1 − 2ν1 )]θ sin θ − C2 sin θ
µ1 − [1 − β − (1 + β)] cos θ , y ≤ 0− , 2µ2
ur(2) =
(23.100)
(23.101)
ak1 by r [1 − 2ν2 + 2β(1 − ν2 )] ln cos θ 2µ2 by + [2(1 − ν2 ) + β(1 − 2ν2 )]θ sin θ − C2 sin θ −
(23.102)
1 (1 + β) cos θ . 2
The continuity conditions across the interface specify the constants C2 and C2 , as given by (23.60). The force exerted by the interface on the dislocation is obtained from (1) (h, 0) , Fx = by σ yy
(23.103)
by excluding the divergent part of the stress at the core center of the dislocation. This gives Fx = −(1 − a)
k1 b2y 2h
.
(23.104)
Depending on the value of a, the dislocation may be attracted or repelled by the interface.
422
23. Dislocations in Bimaterials
23.4.2 Edge Dislocation in an Inﬁnite Medium The Airy stress function is = kbyr ln r cos θ ,
(23.105)
with the corresponding stress components
The displacements are by ux = 2π
"
σxx = kby x
x 2 − y2 , (x 2 + y2 )2
(23.106)
σ yy = kby x
x 2 + 3y2 , (x 2 + y2 )2
(23.107)
σxy = kby y
x 2 − y2 . (x 2 + y2 )2
(23.108)
# x 2 + y2 x 2 − y2 1 1 − 2ν ln , − 4(1 − ν) b2y 4(1 − ν) x 2 + y2
by 1 xy −1 y uy = − . tan 2π x 2(1 − ν) x 2 + y2
(23.109)
(23.110)
The counterparts in polar coordinates are σrr = σθ θ = kby
cos θ , r
σr θ = kby
sin θ , r
with the displacements by r 1 1 − 2ν ur = ln cos θ , cos θ + θ sin θ − 2π 2(1 − ν) by 4(1 − ν) uθ = −
by 2π
r 1 − 2ν 1 ln sin θ . sin θ − θ cos θ + 2(1 − ν) by 4(1 − ν)
(23.111)
(23.112)
(23.113)
23.4.3 Edge Dislocation Near a Free Surface In this case (Fig. 23.4b) we take µ2 = 0, so that α = q = −1 and a = 0. The Airy stress function becomes = kby [r1 ln r1 cos θ1 − r2 ln r2 cos θ2 cos θ2 + h 2 ln r2 − cos 2θ2 + 2h . r2
(23.114)
The stresses are (x − h)[(x − h)2 − y2 ] (x + h)[(x + h)2 − y2 ] − r14 r24 (x + h)4 + 2x(x + h)3 − 6x(x + h)y2 − y4 + 2h , r26
σxx = kby
(23.115)
23.5. Strain Energy of Dislocation Near an Interface
(x − h)[(x − h)2 + 3y2 ] (x + h)[(x + h)2 + 3y2 ] − r14 r24 (x + h)4 − 2x(x + h)3 + 6x(x + h)y2 − y4 + 2h , r26
423
σ yy = kby
y[(x − h)2 − y2 ] y[(x + h)2 − y2 ] − r14 r24 3(x + h)2 − y2 . + 4hxy r26
(23.116)
σxy = kby
(23.117)
The force exerted by the free surface on the dislocation is Fx = −
k1 b2y 2h
.
(23.118)
The dislocation is attracted by the free surface. 23.4.4 Edge Dislocation Near a Rigid Boundary In this case we take µ2 → ∞, which implies (23.76). The Airy stress function is = kby [r1 ln r1 cos θ1 + (a − 1)r2 ln r2 cos θ2 cos θ2 − aβr2 θ2 sin θ2 . − qh 2 ln r2 − cos 2θ2 + 2h r2
(23.119)
The corresponding stresses are σxx = kby
(x − h)[(x − h)2 − y2 ] (x + h)[(x + h)2 − y2 ] +q 4 r1 r24
(x + h)4 + 2x(x + h)3 − 6x(x + h)y2 − y4 x+h , − 2qh − aβ r22 r26 σ yy = kby
(x − h)[(x − h)2 + 3y2 ] (x + h)[(x + h)2 + 3y2 ] + q r14 r24
(x + h)4 − 2x(x + h)3 + 6x(x + h)y2 − y4 x+h − 2qh + aβ , r22 r26 y[(x − h)2 − y2 ] y[(x + h)2 − y2 ] + q r14 r24 3(x + h)2 − y2 y − 4qhxy − aβ . r22 r26
(23.120)
(23.121)
σxy = kby
(23.122)
23.5 Strain Energy of a Dislocation Near a Bimaterial Interface The elastic strain energy per unit dislocation length within a large cylinder of radius R >> h around the core of the dislocation, excluding the core itself, can be calculated by using the
424
23. Dislocations in Bimaterials
h
(2)
Figure 23.5. The dislocation core surface of radius ρ, the remote contour of radius R, and the cut surface from ρ to R used to create a dislocation near the bimaterial interface.
R ρ
(1)
divergence theorem. The energy consists of the work done by the traction on the slip discontinuity along the surface of the cut used to create a dislocation, and the work done by tractions on the corresponding displacements along the surface of the dislocation core and the surface of the remote contour (Fig. 23.5). Thus, for a dislocation with the Burgers vector bx , R 1 (1) σxy (x, 0)dx + ER + Eρ , (23.123) E = bx 2 h+ρ (1)
where ρ is a selected small radius of the dislocation core. The shear stress σxy (x, 0) is obtained from (23.40) as 1 x−h 1 (1) . (23.124) + (q + aβ) + 2qh σxy (x, 0) = k1 bx x−h x+h (x + h)3 The substitution into (23.123) and integration gives 1 2h R q E = k1 bx2 ln + a ln + + ER + Eρ . 2 ρ 2h 2
(23.125)
For a sufﬁciently small radius (ρ p, (24.18) gives Ed = [2b2y + (1 − ν)bz2 ]
π kh , p
(24.19)
which is proportional to h. This is so because for h >> p the stress ﬁeld in the layer above the dislocation array becomes essentially uniform σ yy = −
4πkby , p
σzy = −
µbz , p
as if the array consists of continuously distributed inﬁnitesimal dislocations.
(24.20)
24.3. StrainedLayer Epitaxy
431
Figure 24.3. A threading dislocation segment across the layer and a long misﬁt dislocation left behind at the interface between the layer and its substrate.
The energy for an isolated dislocation near the free surface is obtained when h 0. Alternatively, for a given dislocation spacing of the array, the condition F = 0 speciﬁes the smallest ﬁlm thickness required to support the array at the interface. Thicker ﬁlm could also support the considered array, but they would correspond to F > 0. Since Ed is positive, in order that F ≥ 0, the interaction energy Ed,m must be negative, and its magnitude greater or equal to Ed .
24.4. Conditions for Dislocation Array Formation
433
In the limit ϕ0 → 0 , the condition F = 0 reduces to the Matthews–Blakeslee (1974) equation for the critical ﬁlm thickness, associated with the introduction of an isolated dislocation. In this case F = −(E0d + Ed,m ), where E0d is given by (24.21). If ϕ0 → ∞, i.e., h >> p, from (24.28) it follows that the smallest dislocation spacing of the interface array for a very thick layer, is independent of h and is given by m −1 m by + σzy bz . (24.29) p = kπ[2b2y + (1 − ν)bz2 ] σ yy Physically, the independence of h is a consequence of the fact that for h >> p the stress ﬁeld in the layer becomes essentially constant, and both energies, far ahead and far behind the threading dislocation segments, are proportional to the layer thickness. The misﬁt dislocation, far behind the threading dislocation segment, must be under a force directed away from the free surface, so that misﬁt dislocations are not pulled out to the free surface. This force is given by the negative gradient of the energy difference E − Em with respect to the ﬁlm thickness. Although this must be positive, the misﬁt dislocation will not advance into the substrate, because the external stress in a thick substrate is zero, whereas the free surface exerts only an attractive force on the misﬁt dislocation. As an illustration, consider the layer and substrate that share the same cubic lattice and orientation, with the interface parallel to their (001) crystallographic planes. If the lattice parameters of the layer and substrate are al and as , the fractional mismatch of the lattice parameter is em =
as − al . al
(24.30)
The associated misﬁt strain components are m m em yy = ezz = e ,
m ezy = 0,
(24.31)
and the biaxial stress state is m m = σzz = 4πk(1 + ν)em , σ yy
m σzy = 0.
(24.32)
If the layer/substrate system is Gex Si1−x /Si , where x is the fraction of lattice sites in the layer occupied by Ge atoms, the lattice parameter of the layer is (approximately, by Vegard’s rule) al = xaGe + (1 − x)aSi ,
(24.33)
and of substrate as = aSi . Since aSi = 0.54305 nm and aGe = 0.56576 nm, the misﬁt strain is em ≈ −0.042x. For x = 0.25, this gives em ≈ −0.01. The dislocation array consists of ¯ crystallographic direction on the (111) glide planes (Fig. 24.4). dislocations along [110] ¯ so that relative to the (xyz) coordinate The dislocation Burgers vector is along the [011], √ √ system bx = −b/ 2, by = −b/2, and bz = b/2, where b is equal to al / 2. Consequently, (24.18) becomes 3ϕ02 kb2 5 − 2ν sinh ϕ0 − − ϕ coth ϕ + Ed = (4 − ν) ln , (24.34) 0 0 8 ρ0 4(1 − ν) 2 sinh2 ϕ0 whereas (24.27) gives Ed,m = 2πk(1 + ν)em bh .
(24.35)
434
24. Strain Relaxation in Thin Films [001]

b
[011]
[010]

Figure 24.4. A cubic lattice and orientation, with the interface parallel to (001) crystallographic plane. The Burgers vector ¯ The coordinate of dislocation is b = 12 [011]. axes y and z are along the diagonals of the lattice cube. The x axis is parallel to the crystallographic direction [001].
[110]
z [100]
y
[110]
The relaxation occurs, because Ed,m is negative. Relaxation actually proceeds with the formation of two orthogonal dislocation arrays; the other array consists of dislocations ¯ glide planes. Since the incorporation of the contribution along [110] direction on the (111) from the second array is straightforward, we proceed with the consideration of one array only (the relaxation via the formation of two orthogonal dislocations arrays is considered is Problems 24.2 and 24.3 of Chapter 34). With ν = 0.3, and with the core radius ρ equal to the length of the Burgers vector b, the critical layer thickness is hcr = 19.25 b, where b = 0.388 nm. This satisﬁes the condition Fx > 0 , which requires h > 5.66 b. The relationship between the dislocation spacing and the layer thickness, resulting from the condition F = 0, is shown in Fig. 24.5. The dislocation spacing p tends to inﬁnity when h → hcr . The thickness h0 = 29.25 b corresponds to a dislocation spacing p0 = −(b/2)em = 50 b at which the array completely relaxes the initial mismatch strain.
24.5 Frank and van der Merwe Energy Criterion Frank and van der Merwe proposed that, for a given layer thickness h, dislocations in the array will arrange themselves by choosing the periodicity p which minimizes the energy per unit area of the free surface. This energy is E/ p, and the criterion requires dE d E = E. (24.36) = 0 , i.e., p dp p dp Since E is given by (24.25), from the above condition it follows that p
dEd = Ed + Ed,m . dp
(24.37)
The righthand side of (24.37) is equal to −F. Deﬁning the force f by f = −p
dEd , dp
(24.38)
the Frank and van der Merwe energy condition can be expressed as F= f,
(24.39)
24.5. Frank and van der Merwe Criterion
435
where f =
ϕ02 k ' 2 (bx + b2y )ϕ0 coth ϕ0 − 2b2y 2 sinh2 ϕ0
( + 2b2y + (1 − ν)bz2 ϕ0 coth ϕ0 − bx2 + b2y + (1 − ν)bz2 .
(24.40)
It can be veriﬁed that f is always positive (or equal to zero in the limit ϕ0 → 0), as expected, because from the criterion E ≤ Em , we reason that F cannot be negative. A physical interpretation of f can be given as follows. The force on a single threading dislocation entering alone into an epitaxial layer which already contains an array of spacing p is the negative gradient of the speciﬁc energy with respect to dislocation density, i.e., (Gosling et al. 1992), G=−
d(E/ p) , d(1/ p)
(24.41)
Indeed, if n is the large number of dislocations in the array before one additional dislocation is inserted, the force can be written as G = nE( p) − (n + 1)E( p + d p) .
(24.42)
Since dislocations distribute within the same domain, np = (n + 1)( p + d p). Thus, upon expanding, G= p
dE − E=F− f . dp
(24.43)
The force f is, therefore, the difference between the force F on a threading dislocation associated with a simultaneous formation of all dislocations in the array of spacing p, and the force G on a single dislocation when it alone enters an epitaxial layer already containing an array of spacing p. In the latter case, it is assumed that the array remains periodic upon the introduction of new dislocation by appropriate adjustment of its spacing (if necessary, by dislocation climb). Since f is never negative, it follows that F ≥ G (equality sign applying only at inﬁnitely large dislocation spacing). From this we can again conclude that the equilibrium spacing predicted by the Frank and van der Merwe criterion (G = 0) must be greater than that obtained from the condition F = 0. Indeed, if for an array F = 0, then G < 0, and one dislocation would tend to leave the array, which would increase the spacing among the remaining dislocations. The process would gradually continue until the condition G = 0 is reached, which gives the equilibrium array conﬁguration according to Frank and van der Merwe criterion. For the layer/substrate system under consideration, the predictions based on the condition F = f , and the condition F = 0, are shown in Fig. 24.5. As previously discussed, for a given ﬁlm thickness, a larger spacing is predicted by the Frank and van der Merwe criterion. If the array with dislocation spacing according to Frank and van der Merwe would be formed by a simultaneous threading of all dislocations, the corresponding force F on the threading segments would not be zero, but large and positive. Arrays are observed that do not correspond to the minimum energy, or the most relaxed conﬁguration, so that the actual spacing may indeed be greater or smaller than that predicted by the Frank and van der Merwe criterion. One reason for this is that during the process of their gradual introduction, dislocations cannot easily readjust their positions to minimize the total energy.
436
24. Strain Relaxation in Thin Films 200.0 180.0 160.0 F=0 F=f1 F=f2 F=f
140.0
p/b
120.0 100.0 80.0 60.0 40.0 20.0 0.0 0.0
10.0
20.0
30.0
40.0
50.0
60.0
70.0
80.0
90.0
100.0
h/b Figure 24.5. Dislocation spacing p vs. layer thickness h (scaled by the length of the Burgers vector) according to the condition based on simultaneous array formation, F = 0; Frank and van der Merwe energy minimum condition, F = f ; and the conditions based on two different processes of gradual array formation, F = f1 , and F = f2 (0 < f1 < f2 < f ). From Lubarda (1999).
Experiments, however, indicate that for a ﬁlm thickness that exceeds the critical thickness by a factor of 2 or 3, the dislocation spacing is substantially greater than that predicted by the condition F = 0 (Freund, 1993). The critical layer thicknesses according to the Matthews and Frank and van der Merwe criteria are identical. The critical thickness according to the Frank and van der Merwe criterion follows from (24.39) in the limit p → ∞, which implies that very few dislocations are introduced in the ﬁlm. Because f goes to zero as p goes to inﬁnity, the condition (24.39) reduces to F = 0, which is the Matthews condition for the critical layer thickness. It is interesting to note that at this value of the layer thickness, the stationary value of the speciﬁc energy E/ p, reached asymptotically in the limit p → ∞, is actually a local energy maximum. There is also an energy minimum (being very slightly lower than the local energy maximum), which occurs at a large but ﬁnite value of the dislocation spacing. This was originally observed by Jain et al. (1992). However, by taking the critical ﬁlm thickness to be just slightly smaller than that associated with the condition F = 0, the value of the energy in the limit of inﬁnite spacing becomes an energy minimum, and a single dislocation can be deposited at the interface in a stable manner.
24.6 Gradual Strain Relaxation During the ﬁlm growth beyond its critical thickness, dislocations gradually enter to form the misﬁt dislocation array at the interface between the ﬁlm and its substrate. To uniformly
24.6. Gradual Strain Relaxation
437
relax the ﬁlm, dislocations tend to form periodic arrays. A misﬁt dislocation already deposited at the interface on a particular glide plane relaxes the elastic strain on adjacent glide planes, reducing a tendency for another misﬁt dislocation there. The gradual relaxation is a difﬁcult process, which involves time effects and the kinetics of dislocation nucleation and motion for any given temperature of the ﬁlm growth. A simpliﬁed model of gradual relaxation was suggested by Freund (1993). Imagine that in the process of the formation of an array of spacing p, at some instant the array of uniform spacing 2 p is ﬁrst formed. Denote the corresponding energy within the width 2 p by E(2 p). The ﬁlm is assumed to be thick enough for the energy difference F(2 p) = 2Em − E(2 p) = −Ed (2 p) − Ed,m
(24.44)
to be positive. This is required to make the conﬁguration energetically preferred relative to the ﬁlm conﬁguration without dislocations. The actual order by which dislocations entered the ﬁlm to form the considered array is irrelevant for the present discussion, because the energy E(2 p) does not depend on that order. Thus, the value of F(2 p) is also independent of the order, although F(2 p) can be interpreted as a driving force on each threading dislocation in the array, if they would simultaneously form. For F(2 p) to be positive, the ﬁlm thickness must be greater than the thickness associated with the condition F(2 p) = 0. The second set of dislocations is next introduced by the glide of their threading segments along the planes midway between the glide planes of the ﬁrst set. After this set is introduced, an array of dislocation spacing p is formed. The corresponding elastic strain energy per unit length of dislocation, stored within the width 2 p, can be written as 2E( p) = E(2 p) + Ed (2 p) + Ed,m + Ed,d (2 p) .
(24.45)
Here, E( p) is the energy within the width p, given by (24.18), and Ed,d (2 p) is the interaction energy between the two sets of dislocations (two arrays of spacing 2 p). The ﬁlm of a given thickness will prefer the array of spacing p rather than the array of spacing 2 p, if 2E( p) < E(2 p), regardless of the order by which the second set is introduced. The difference F1 = E(2 p) − 2E( p)
(24.46)
is a driving force on each threading dislocation from the second set, if they all were introduced simultaneously. Substituting (24.44) and (24.45) into (24.46), we obtain F1 = F( p) − f1 ,
f1 =
1 d,d E (2 p) . 2
(24.47)
The force F( p) is given by (24.28). An expression for the interaction energy Ed,d (2 p) can be conveniently obtained by using the fact that the elastic strain energy does not depend on the sequence by which dislocations are introduced in the array. Thus, the energy within the width 2 p, associated with sequential formation of the array, given by (24.45), must be equal to the energy associated with simultaneous formation of the whole array, which is 2E( p) = 2Ed ( p) + Em + 2Ed,m . By equating this to the righthand side of (24.45), we ﬁnd Ed,d (2 p) = 2[Ed ( p) − Ed (2 p)] .
(24.48)
438
24. Strain Relaxation in Thin Films
h p
p
p/2 p/2
Figure 24.6. An array of nonuniform dislocation spacing, which alters between p and p/2.
Substituting (24.18), this becomes explicitly ϕ02 ϕ0 1 2 Ed,d (2 p) = k [bx2 + b2y + (1 − ν)bz2 ] ln cosh + (bx + b2y ) 2 8 cosh2 (ϕ0 /2) ! 1 ϕ0 − (bx2 − b2y )ϕ0 tanh . 2 2 For the previously considered GeSi layer/substrate system, (24.6) simpliﬁes to 3ϕ02 kb2 ϕ0 1 ϕ0 ϕ + Ed,d (2 p) = tanh − (4 − ν) ln cosh . 0 4 2 2 8 cosh2 (ϕ0 /2) 2
(24.49)
It can be veriﬁed that this energy is always positive. It is also observed that Ed,d is a monotonically increasing function of ϕ0 , so that Ed,d ( p) > Ed,d (2 p). The plot of the relationship between the dislocation spacing p and the layer thickness h, associated with the condition F1 = 0, i.e., F( p) = f1 , is shown in Fig. 24.5. For a given ﬁlm thickness, the predicted dislocation spacing is greater in the case of sequential, rather than simultaneous, array formation, associated with the condition F( p) = 0. An additional increase in predicted dislocation spacing is obtained if the relaxation process is more gradual. For example, imagine that, in the transition from the array of spacing 2 p to the array of spacing p, an intermediate conﬁguration is ﬁrst reached which contains a periodic array of period 4 p. The dislocation spacing in this array is nonuniform, and it varies from p to 2 p. The array is shown in Fig. 24.6, if p there is replaced by 2 p. This conﬁguration can be obtained by the introduction of a new dislocation between every second pair of dislocations of the array of spacing 2 p, i.e., by an appropriate introduction of an additional array of spacing 4 p. The corresponding energy, within the width 4 p, is E2 = 2E(2 p) + Ed (4 p) + Ed,m + Ed,d (2 p) .
(24.50)
The driving force for the transition from the conﬁguration with the array of spacing 2 p to the considered intermediate conﬁguration is 2E(2 p) − E2 , which is assumed to be positive. The driving force from the intermediate conﬁguration to the conﬁguration with the array of spacing p is F2 = E2 − 4E( p), which gives F2 = F( p) − f2 ,
f2 = 3Ed ( p) − 2Ed (2 p) − Ed (4 p) − Ed,d (2 p) .
(24.51)
The plot of the relationship between the ﬁlm thickness and the dislocation spacing, resulting from the condition F2 = 0, i.e., F( p) = f2 is shown in Fig. 24.5. The results demonstrate that, for a given ﬁlm thickness, the predicted spacing is greater than that associated with
24.8. Stronger Stability Criteria
439
the condition F1 = 0. Thus, the more gradual the relaxation process, the less dense is the array deposited at the interface.
24.7 Stability of Array Conﬁgurations Consider a periodic array of spacing p at the interface between the ﬁlm and its substrate. If the ﬁlm is sufﬁciently thick, additional dislocations will enter to relax the ﬁlm. If the ﬁlm is too thin, some dislocations will recede. For example, if enough dislocations enter so that, from the array of spacing p, an array of spacing p/2 is formed, the driving force for the transition is E( p) − 2E( p/2) = F( p) − Ed,d ( p). If the ﬁlm resists the transition, this force must be negative, hence F( p) < Ed,d ( p) .
(24.52)
On the other hand, if the ﬁlm is too thin, it may not support the array of dislocation density as high as 1/ p, and some dislocations will recede. Imagine that every second dislocation from the array leaves the ﬁlm. The driving force for this recession is −F1 = −F( p) + Ed,d (2 p)/2, as given by (24.47). If the recession is not preferred, the force must be negative, and F( p) >
1 d,d E (2 p) . 2
(24.53)
Combining the inequalities (24.52) and (24.53), we obtain the bounds that deﬁne the range of the ( p, h) values for which the array can stably exist at the interface, at least regarding the considered perturbations of its structure. The bounds are shown in Fig. 24.7, where they are designated by B1. Recall that the stable range was previously bounded from below by the condition F > 0, which deﬁnes the lowest lower bound. A higher lower bound can be obtained from the condition F2 > 0, associated with the recession in which every fourth dislocation leaves the array of uniform spacing p. From (24.51), we have F( p) > 3Ed ( p) − 2Ed (2 p) − Ed (4 p) − Ed,d (2 p) .
(24.54)
On the other hand, a lower upper bound can be obtained by considering a possible transition of the array of spacing p into the array of nonuniform spacing, which is obtained by the entrance of additional dislocation midway between every second pair of dislocations in the array of uniform spacing p (Fig. 24.6). The energy of this conﬁguration, within the width 2 p, is 2E( p) + Ed (2 p) + Ed,m + Ed,d ( p) . Thus, if the transition should not occur, F( p) < Ed,d ( p) + Ed (2 p) − Ed ( p) .
(24.55)
The bounds deﬁned by (24.54) and (24.55) are also shown in Fig. 24.7, designated there by B2, and they are within the previously deﬁned bounds B1.
24.8 Stronger Stability Criteria Stronger stability conditions and restrictions on possible bounds can be obtained by using the analysis of Gosling et al. (1992), who introduced the criterion based on the conditions for the entrance, or recession, of a single dislocation from the periodic array. If the dislocation
440
24. Strain Relaxation in Thin Films 200.0 180.0 B1 B2 B3 B4
160.0 140.0
p/b
120.0 100.0 80.0 60.0 40.0 20.0 0.0 0.0
10.0
20.0
30.0
40.0
50.0
60.0
70.0
80.0
90.0
100.0
h/b Figure 24.7. Four sets of bounds (B1 through B4) which deﬁne range of stable array conﬁgurations with respect to assumed perturbations in the periodic array structure, as described in the text (from Lubarda, 1999).
spacing can adjust so that the array maintains its periodicity upon the entrance of a new dislocation, the force on a threading dislocation entering the array would be G = F − f . Because the adjustment of spacing generally requires dislocation climb (which may not be operative at low temperatures), it may be assumed that dislocations in the array remain ﬁxed as the new misﬁt dislocation deposits at the interface. The array is then considered to be stable if this deposition is resisted. The driving force on a threading dislocation, midway between the two dislocations of the periodic array of spacing p, is the difference between the energies of the two conﬁgurations: the energy of the conﬁguration with a periodic array, and the energy of the same conﬁguration with an inserted new dislocation. The latter is equal to the former, plus the energy of the added dislocation E0d , given by (24.21), plus the work done to introduce the new dislocation against the stress of the existing array and the misﬁt stress, which is Ed,d ( p) + Ed,m . Thus, the force to drive a dislocation into the array is F(+) = −Ed,d ( p) − Ed,m − E0d = F( p) − Ed,d ( p) + Ed ( p) − E0d .
(24.56)
If the introduction of new dislocation is resisted, then F(+) < 0, and F( p) < Ed,d ( p) − [Ed ( p) − E0d ] .
(24.57)
It was additionally proposed by Gosling et al. (1992) that the recession of a single dislocation from the array (creation of a vacancy in its periodic structure), should also be resisted. A simple way to calculate the force that tends to drive a dislocation out of the array, while all other dislocations remain ﬁxed, is to imagine that a negative dislocation (whose Burgers vector is opposite to that of dislocations in the array) is introduced to
24.9. Further Stability Bounds
441
p
Figure 24.8. A perturbed array conﬁguration used to derive a lower bound of the stable array conﬁgurations (designated by B4 in Fig. 24.7).
p
3p/2
3p/2
annihilate one of dislocations from the array. The energy difference between the two conﬁgurations is then equal to the energy of the added negative dislocation, E0d , plus the work done to introduce the negative dislocation against the stress of the existing periodic array and the misﬁt stress. This work is h−ρ [bx σxy (x, 0) + by σ yy (x, 0) + bzσzy (x, 0)]dx + 2Eρ − Ed,m = −2Ed ( p) − Ed,m. 0
(24.58) Equation (24.16) was used to express the integral in (24.58) in terms of other introduced energy contributions. Thus, the force to drive dislocation out of the array is F(−) = 2Ed ( p) + Ed,m − E0d = Ed ( p) − E0d − F( p) .
(24.59)
A dislocation will not recede from the array if F(−) < 0, i.e., F( p) > Ed ( p) − E0d .
(24.60)
For the considered layer/substrate system, the bounds deﬁned by (24.57) and (24.60) are shown in Fig. 24.7, where they are designated by B3. These bounds are within the bounds B1. This was clear for the upper bounds, because Ed ( p) − E0d is positive. It was also expected for the lower bounds on physical grounds, because the array may be in a stable conﬁguration regarding the recession of every second dislocation from the array, but in an unstable conﬁguration regarding a slighter disturbance, due to recession of a single dislocation. For example, suppose the ﬁlm is in the state corresponding to a point on the lower bound curve. With further ﬁlm growth, dislocation spacing remains constant until the point on the upper bound curve is reached, at which instant a new dislocation can enter the ﬁlm.
24.9 Further Stability Bounds A new set of bounds which deﬁne possible range of stable array conﬁgurations can be constructed by comparing the array conﬁguration with two perturbed neighboring conﬁgurations, as follows. 24.9.1 Lower Bound Consider a perturbed array conﬁguration, which contains one dislocation at a distance 3 p/2 from the two neighboring dislocations, whereas the rest of the array has uniform spacing p (Fig. 24.8). This conﬁguration can be obtained from a perfectly periodic array of spacing p
442
24. Strain Relaxation in Thin Films
y
O h (1)
(2)
y
Figure 24.9. Two dislocations with different Burgers vectors, beneath the free surface at the horizontal distance y between each other.
x
by recession of two neighboring dislocations and by injection of one new dislocation along the slip plane midway between the two receding dislocations. One may also think that one dislocation has receded, whereas one dislocation, ahead or behind the receding dislocation, has subsequently positioned itself in the middle between the two dislocations of the perturbed array. The change of energy between the perturbed and unperturbed conﬁgurations can be calculated as follows. First, introduce a new dislocation midway between the two neighboring dislocations of the perfect array. As previously shown, the energy increases by E0d + Ed,d ( p) + Ed,m . Introduce next two negative dislocations to annihilate two dislocations, ahead and behind the inserted dislocation. This further increases the energy by 2[E0d − 2Ed ( p) − Ed,m ], plus the interaction energy among the three dislocations, which is Ein = E(−,−) + 2E(+,−) . The interaction energy between two dislocations, both at depth h below the free surface of a semiinﬁnite body, and at the horizontal distance y from each other (Fig. 24.9), can be calculated from h (1) (1) (2) (1) bx(2) σxy (x, y) + b(2) (24.61) E(1,2) = − y σ yy (x, y) + bz σzy (x, y) dx . 0
One dislocation has the Burgers vector b(1) and the other b(2) . The substitution of the Head’s stress expressions for a single dislocation beneath the free surface (see Chapter 23) into (24.61), and integration gives k ' (1) (2) (2) (1) (2) bx bx + b(1) ln(1 + η2 ) b + (1 − ν)b b E(1,2) = y y z z 2 2η3 (1) (2) − b b − bx(1) b(2) (24.62) y y x (1 + η2 )2 ( η2 (2) , − (1 + 3η2 )bx(1) bx(2) − (3 + η2 )b(1) b y y (1 + η2 )2 where η = 2h/y. The energy E(−,−) is obtained from (24.62) by taking b(1) = b(2) = −b, and y = p. The energy E(+,−) is obtained if b(1) = −b(2) = b, and y = p/2. Therefore, we obtain
k ' 2 bx + b2y + (1 − ν)bz2 ln(1 + η2 ) E(−,−) = 2 (24.63) (
η2 2 2 2 2 , − (1 + 3η )bx − (3 + η )by (1 + η2 )2 where now η = 2h/ p. The interaction energy between the positive and negative dislocation E(+,−) is given by the same expression, with η replaced by 2η, and k by −k. The force which
24.9. Further Stability Bounds
p
2p/3 2p/3 2p/3
443
p
Figure 24.10. A perturbed array conﬁguration used to derive an upper bound of the stable array conﬁgurations (designated by B4 in Fig. 24.7).
drives the perfect array into the perturbed array is the negative of the corresponding energy change, which gives F∗ = −F( p) + 3[Ed ( p) − E0d ] − Ed,d ( p) − Ein .
(24.64)
If the perturbation is resisted, F∗ < 0 , i.e., F( p) > 3[Ed ( p) − E0d ] − Ed,d ( p) − Ein .
(24.65)
This deﬁnes a lower bound for the stable conﬁguration of the perfect array (B4 in Fig. 24.7), which is slightly higher than the lower bound B3 deﬁned by (24.60). This was expected to be the case, because the symmetric conﬁguration in Fig. 24.8 is more relaxed than the conﬁguration with the array containing the vacancy in its periodic structure, with the surrounding dislocations being ﬁxed. Since dislocation adjustment may require climb, it is supportive to the above consideration to give an additional or alternative interpretation of the condition F∗ < 0. Imagine that the periodic array of uniform spacing p is completed, except for two missing dislocations next to each other. Denote the corresponding energy by E. (Total energies of inﬁnite arrays are inﬁnitely large, but their differences are ﬁnite, and will only be needed in this discussion). If two dislocations enter and complete the perfect array, the energy becomes Ea , and the driving force for this to occur would be Fa = E − Ea . If, instead of two, only one dislocation enters, midway between the two missing dislocations of the perfect array, the energy is Eb , and the corresponding force would be Fb = E − Eb . If Fa > Fb , the case (a) is preferred, because then Ea < Eb . On the other hand, the force that would drive the conﬁguration (a) into (b) is F∗ = Ea − Eb = Fb − Fa . Thus, the condition F∗ < 0 again gives Fa > Fb , which means that the perfect array (a) would be preferred to the perturbed array (b). 24.9.2 Upper Bound A lower upper bound can be obtained by considering a perturbed array conﬁguration shown in Fig. 24.10. This conﬁguration can be obtained from the perfectly periodic array of spacing p by recession of one dislocation, and by symmetric injection of two new dislocations at the distance p/3 from the receding dislocation. Alternatively, one may consider that a perfect array was created, except for one missing dislocation, and the competition is taking place whether one more dislocation will enter and complete the perfect array or
444
24. Strain Relaxation in Thin Films y
y
O x
h p
Figure 24.11. A dislocation at the position (x, y) approaching a dislocation array of spacing p, beneath the free surface.
p
x
whether two dislocations will symmetrically enter to form the perturbed array in Fig. 24.10. Imagine that a negative dislocation is introduced to cancel one dislocation from the perfect array and two additional dislocations are then injected. The energy change relative to the perfect conﬁguration is equal to the energy of the added negative dislocation, E0d , plus the work done to introduce the negative dislocation against the stress of the perfect array and the misﬁt stress, which is given by (24.58), plus the energy associated with the introduction of the two dislocations. This is 2E0d + 2Ed,m , plus the interaction energy of the two dislocations with the perfect array 2Eint ( p/3), plus the interaction energy among the three added dislocations, Ein = E(+,+) + 2E(+,−) . Thus, the force that would drive the perfect array into the perturbed array is p (24.66) F∗ = F( p) + 3[Ed ( p) − E0d ] − 2Eint ( ) − Ein . 3 The interaction energy E(+,+) is given by (24.63), with η = 3h/ p. The interaction energy E(+,−) is given by the same expression, with η replaced by 2η, and k by −k. The general expression for the interaction energy associated with the introduction of an additional dislocation into the periodic array, anywhere between two dislocations in the array (Fig. 24.11), can be calculated from x [bx σxy (x, y) + by σ yy (x, y) + bzσzy (x, y)]dx . (24.67) Eint (x, y) = − 0
The substitution of the stress expressions (24.1)–(24.3) gives upon integration the following expression for the interaction energy Eint (x, y) = k[bx2 Ix + b2y Iy + bx by Ixy + (1 − ν)bz2 Iz] ,
(24.68)
where Ix = Iz −
1 ϕ sinh ϕ ϑ sinh ϑ 1 1 − cosh ϕ cos ψ + + ϕ0 (ϕ − ϕ0 ) , 2 cosh ϕ − cos ψ 2 cosh ϑ − cos ψ (cosh ϕ − cos ψ)2 ϑ sinh ϑ ϕ sinh ϕ − , cosh ϕ − cos ψ cosh ϑ − cos ψ 1 1 − = ϑ sin ψ , cosh ϑ − cos ψ cosh ϕ − cos ψ
Iy = Ix + Ixy
Iz =
1 cosh ϕ − cos ψ ln . 2 cosh ϑ − cos ψ
(24.69)
24.9. Further Stability Bounds y
445
y
O h p
Figure 24.12. A dislocation injected between two neighboring dislocations from a dislocation array of spacing p.
p
x
The interaction energy for x = h (Fig. 24.12) is consequently Eint (y) = k [bx2 Ix + b2y Iy + (1 − ν)bz2 Iz] ,
(24.70)
where Ix = Iz −
ϕ 2 (1 − cosh 2ϕ0 cos ψ) ϕ0 sinh 2ϕ0 + 0 , cosh 2ϕ0 − cos ψ (cosh 2ϕ0 − cos ψ)2 Iy = Ix + Iz =
2ϕ0 sinh 2ϕ0 , cosh 2ϕ0 − cos ψ
(24.71)
1 cosh 2ϕ0 − cos ψ ln . 2 1 − cos ψ
In (24.9.2)–(24.9.2), ϕ0 = 2π h/ p, and ψ = 2π y/ p. The interaction energy Eint ( p/3) is obtained by taking ψ = 2π/3. Having Eint ( p/3) calculated, the perturbation is resisted if F∗ < 0, i.e., p (24.72) F( p) < 2Eint ( ) + Ein − 3[Ed ( p) − E0d ] . 3 This deﬁnes an upper bound for the stable conﬁguration of the perfect array (B4 in Fig. 24.7), which is lower than the upper bound B3 deﬁned by (24.57), because the symmetric conﬁguration in Fig. 24.10 is more relaxed than the perfect array conﬁguration with an additional dislocation exactly midway between the two dislocations of the array. It is interesting to note that the four lower bounds shown in Fig. 24.7 are closer to each other than the four upper bounds, so that bounds are more sensitive to perturbation modes involving the entrance of new dislocations, than the recession of some of the dislocations from the array. From a purely energetic point of view, which does not take into account possible mechanisms by which conﬁgurations can alter, the stable conﬁguration would be unique and given by the Frank and van der Merwe criterion. The corresponding curve is always between the upper and lower bound of any considered set of bounds, because f in (24.39) is always between these bounds. However, during ﬁlm growth dislocations may be entering in such a way that the minimum energy spacing cannot actually be attained at a given ﬁlm thickness, because complete readjustment of already taken dislocation positions would be required (either by climb or recession of some and entrance of other dislocations). In view of this, then, any spacing between derived upper and lower bounds could in principle correspond to a given ﬁlm thickness, depending on the sequence or the order by which
446
24. Strain Relaxation in Thin Films
dislocations entered in the process of ﬁlm growth. Inevitably, the dislocation spacing will be more or less nonuniform, although dislocations will try their best to form, as nearly as possible, periodic arrays and minimize the total energy of the system. Furthermore, the order by which dislocations enter depends on the location and strength of available dislocation sources. The rate of ﬁlm growth has also an obvious effect on dislocation spacing that is eventually taken by the array at the ﬁnal ﬁlm thickness.
24.10 Suggested Reading Fitzgerald, E. A. (1991), Dislocations in StrainedLayer Epitaxy: Theory, Experiment, and Applications, Mater. Sci. Reports, Vol. 7, pp. 87–142. Freund, L. B. (1993), The Mechanics of Dislocations in StrainedLayer Semiconductor Materials, Adv. Appl. Mech., Vol. 30, pp. 1–66. Freund, L. B., and Suresh, S. (2003), Thin Film Materials: Stress, Defect Formation and Surface Evolution, Cambridge University Press, New York. Gosling, T. J., Jain, S. C., Willis, J. R., Atkinson, A., and Bullough, R. (1992), Stable Conﬁgurations in Strained Epitaxial Layers, Phil. Mag. A, Vol. 66, pp. 119–132. Lubarda, V. A. (1999), Dislocations Arrarys at the Interface between an Epitaxial Layer and Its Substrate, Math. Mech. Solids, Vol. 4, pp. 411–431. Matthews, J. W. (1979), Misﬁt Dislocations. In Dislocations in Solids (F. R. N. Nabarro, ed.), Vol. 2, pp. 461–545, NorthHolland, Amsterdam. Nix, W. D. (1969), Mechanical Properties of Thin Films, Metall. Trans. A, Vol. 20A, pp. 2217– 2245. Van der Merwe, J. H. (1991), Strain Relaxation in Epitaxial Overlayers, J. Electr. Mat., Vol. 20, pp. 793–803.
25 Stability of Planar Interfaces
The breakdown of an initially ﬂat, or smooth, surface into one characterized by surface roughness is an important type of phenomena occurring, inter alia, during the growth of thin ﬁlms or at surfaces of solids subject to remotely applied stress in environments that induce mass removal or transport. In the case of thin ﬁlms, stresses arise due to lattice mismatch and/or differences in coefﬁcients of thermal expansion. The sources of stress are, indeed, legion but the effect can be to induce roughness, and surface restructuring, that may be either deleterious, or in some cases desirable, if the patterning can be controlled. The phenomena was ﬁrst studied by Asaro and Tiller (1972) and has since been pursued by others. Our purpose is to develop some of the guiding principles, but we note that the topic is far from being thoroughly worked out. In particular, we make many simplifying assumptions, one being the assumption of surface isotropy. We also ignore some important physical attributes of surfaces, such as surface stress, which have recently been added to the description of surface patterning (Freund and Suresh, 2003).
25.1 Stressed Surface Problem We consider here the phenomena of the breakdown of planar interfaces subject to stress into interfaces characterized by undulated topology. The phenomena is governed by those same driving forces that lead to crack growth and the growth of defects, such as inclusions, that cause internal stresses. Figure 25.1 illustrates such a process occurring under the action of a remotely applied tensile stress, although the same process can be driven by remotely applied shear stress. Moreover, attention will be conﬁned to cases where mass transport is effected by surface diffusion and dissolution followed by diffusion through a bulk medium. An exactly parallel development can be made where mass transport is via bulk solid diffusion. The process involves the development of stress concentrations at the troughs of the (slightly) rough surface; this, in turn, causes higher levels of strain energy density and chemical potential (deﬁned in the next section). The gradients of chemical potential cause mass ﬂow, via diffusion, from the troughs to the hills, thus leading to deepening of the troughs and an increase in undulation. The impediment is the the energy required to create additional surface area. This leads to a stability problem as described below. We begin by considering a halfplane whose free surface has become slightly undulated; the 447
448
25. Stability of Planar Interfaces ny
n nx Figure 25.1. Undulated stressed surface.
x σο
y
σο
surface proﬁle is assumed to be sinusoidal with a form y = a cos(ωx). The slope of the surface is assumed small and the intent is to create an asymptotic solution of order O(aω). The normal to the surface is n, where nx = sin[tan−1 (−aω sin(ωx)] ∼ −aω sin(ωx) + O(a 2 ω2 ), n y = cos[tan−1 (−aω sin(ωx)] ∼ 1 + O(a 2 ω2 ).
(25.1)
This surface is traction free. Once again the total problem will be solved by superposing two companion problems. The ﬁrst problem is simply a halfplane subject to far ﬁeld tension of magnitude σ0 – this will create tractions on the sinusoidal surface, T, that we shall evaluate. The second problem is one in which the opposite tractions −T are applied to the surface of the halfplane; when these are added the effect is to annihilate those existing in the ﬁrst problem, thereby creating a sinusoidal surface that is traction free, as desired. Clearly, the potential (1) for the ﬁrst problem is φ (1) = σ0 y2 , with the stress σxx = σ0 . For problem (2), we proceed as follows. Consider the potential φ (2) = aσ0 ye−ωy cos(ωx).
(25.2)
The corresponding stresses are (2) = σxx
∂ 2 φ (2) = −2aωσ0 e−ωy cos(ωx) + aω2 σ0 ye−ωy cos(ωx), ∂ y2 (2) = σ yy
σxy = −
∂ 2 φ (2) = −aω2 σ0 ye−ωy cos(ωx), ∂ x2
(25.3)
∂ 2 φ (2) = aωσ0 e−ωy sin(ωx) − aω2 σ0 ye−ωy sin(ωx). ∂ x∂ y
On the surface, which is taken asymptotically to be at y = a cos(ωx), the traction components are, to ﬁrst order in aω, (2) (2) Tx(2) = σxx nx + σxy n y = aωσ0 sin(ωx) + O(a 2 ω2 ), (2) (2) n y + σxy nx = 0 + O(a 2 ω2 ). Ty(2) = σ yy
(25.4)
Note from problem (1) that these traction components are, again to ﬁrst order in aω, Tx(1) = −aωσ0 sin(ωx) + O(a 2 ω2 ), Ty(1) = 0 + O(a 2 ω2 ).
(25.5)
Thus, to ﬁrst order in aω, the full solution for the stress potential is φ(x, y) =
1 σ0 y2 + aσ0 ye−ωy cos(ωx). 2
(25.6)
25.2. Chemical Potential
449
S + δS δε
Figure 25.2. Surface area and curvature.
S
The corresponding stresses are σxx = σ0 − σ0 (ω2 y − 2ω)e−ωy cos(ωx), σ yy = −ω2 aσ0 ye−ωy cos(ωx),
(25.7)
σxy = −ωaσ0 (1 − ωy)e−ωy sin(ωx). The strain energy density on y = a cos(ωx) is given, to ﬁrst order in aω, by W(x) = σ02 [1 + 4aω cos(ωx)]/2E + O(a 2 ω2 ).
(25.8)
The above will be used to construct the chemical potential for matter on the undulated surface and to set up the equations of diffusion that govern the evolution of the surface proﬁle.
25.2 Chemical Potential The Gibbs free energy was introduced in previous chapters. Here we introduce the chemical potential µ as the partial molar derivative of G. Accordingly, µ is deﬁned as the work required to add a unit amount of material at constant temperature to the body. Moreover, we are speciﬁcally concerned with the chemical potential on the surface of the body. When material is added to a surface it is necessarily added normal to the surface, and if the surface has curvature this will change the surface area and thus require additional free energy associated with the surface energy, γ . This energy is to be added to that associated with the elastic strain energy. Consider the addition of mass to a surface as depicted in Fig. 25.2. The increment in area is related to curvature by δS = Sκδ,
(25.9)
where δ is the normal growth of the surface, S is the area to which material is being added, and κ is the curvature at the point where material is added. In two dimensions, the curvature is given as d2 y/dx 2
κ=
1 + (dy/dx)2
2 2
3/2 ≈ −aω cos(ωx) + O(a ω ).
(25.10)
Now, the surface area change can also be written as δS = κ(Sδ) = κδv,
(25.11)
where δv is the increment of volume of added material. Thus, the extra amount of work required to add material associated with surface energy is γ κδv. Let the unit amount be per atom, and deﬁne v0 as the atomic volume. Then, the amount of work required to create (or destroy) surface area is, per atom, γ κv0 . Recall that the body is elastically strained. To add a unit amount of material at a point, it is necessary to bring it to the same state of elastic strain – this adds an additional amount
450
25. Stability of Planar Interfaces
of required work, W(x)v0 . The total chemical potential is, therefore, µ = µ0 + W(x)v0 + γ κv0 ,
(25.12)
where µ0 represents all other contributions to µ, not affected by position on the surface. It is gradients in µ that cause mass ﬂow, which we assume occurs by surface diffusion.
25.3 Surface Diffusion and Interface Stability Suppose that the body contains β atoms per unit area. Gradients in the chemical potential give rise to a diffusive ﬂux, J , calculated from J =−
D ∇µ, kT
(25.13)
where kis Boltzman’s constant, T is the absolute temperature, and Dis the surface diffusion constant. For the case considered, ∇µ =
∂µ + O(a 2 ω2 ). ∂x
(25.14)
Deﬁne rn as the rate of normal motion of the surface. Then, rn = v0 divJ = −
Dβv0 ∂ 2 µ . kT ∂ x 2
(25.15)
The rate of normal advance is related to the time change in the curve y(x) deﬁning the surface as dy −1/2 dy rn = 1 + , (25.16) dx dt and so, to ﬁrst order, Dβv0 ∂ 2 µ ∂y =− . ∂t KT ∂ x 2
(25.17)
The differential equation in (25.17) may be solved using the deﬁnitions in (25.10) and (25.12). At t = 0 and at x = 0, i.e., at the depth of a trough at time t = 0, we ﬁnd that 2σ02 3 da 2 4 V= = B −γ ω + ω , (25.18) dt E where B = av02 β D/kT. For V ≥ 0, that is for the interface to become unstable, in the sense that its undulated amplitude begins to grow, we must have √ 2π Eγ 1/2 1/2 2 σ0 ≥ (Eγ ω) = , (25.19) λ where λ is the wavelength of the sinusoidal surface. Assume that all wavelengths are possible and that the one that dominates is that which grows fastest, i.e., set ∂V = 0 and ∂ω
∂2V < 0, ∂ω2
(25.20)
25.4. Interface Stability
451
1.0
V Vmax Figure 25.3. Velocity of surface amplitude growth vs. frequency.
ω / ω ∗ 1.0
to obtain ω =
3 σ0 , 2 Eγ
(25.21)
and V = Vmax = 0.1B
σ08 . γ 3 E4
(25.22)
Relations such as (25.21) and (25.22) certainly suggest a very strong sensitivity of interface stability to the material properties involved in the process, such as interface energy and elastic modulus (Fig. 25.3).
25.4 Volume Diffusion and Interface Stability The chemical potential on the surface of the stressed solid was given in (25.12), and in full it is µ − µ0 =
v0 σ02 [1 + 4aωe−ωy cos(ωx)] − γ v0 aω2 cos(ωx), 2E
(25.23)
where the expression for strain energy density was evaluated on y = 0. Now we assume that the stressed solid is in contact with a ﬂuid that is capable of dissolving the solid and forming with it a perfect solution. With that assumption, we take the chemical potential of the solid constituent in the ﬂuid to be µ − µ0 = kT ln c,
(25.24)
where c is the concentration. If c0 is the equilibrium concentration between an unstressed ﬂat solid and the liquid, we obtain the relation kT ln
v0 σ02 c 1 + 4aωe−ωy cos(ωx) − γ v0 aω2 cos(ωx), = c0 2E
(25.25)
which can be expressed as c = c0 e f (σ0 ,ω) .
(25.26)
452
25. Stability of Planar Interfaces
Since f (σ0 , ω) is typically much less that unity, we may expand (25.26) to ﬁrst order and obtain
v0 σ02 c 1 + 4aωe−ωy cos(ωx) =1− c0 kT 2E v 0 +γ ω2 cos(ωx). kT
(25.27)
This relation is the interface boundary condition for a ﬂuid diffusion problem wherein matter will dissolve at the valleys and deposit at the peaks, or vice versa, depending on the sign of the chemical potential gradient. Assuming that equilibrium is maintained between the solid and the ﬂuid, and that the interface moves sufﬁciently slowly that the transport is nearly steady state at all times, the solution to the transport problem, subject to (25.27) as the boundary condition, is given by !
v0 σ02 1 + 4aωe−ωy0 cos(ωx) e−ωy c − c0 = − c0 kT 2E (25.28) v 0 2 −ωy aω cos(ωx) e . + c0 γ kT The rate of change of the amplitude, a, is ∂y ∂c a˙ = = v0 DL y=0 ∂t x=0 ∂ y x=0 2 σ0 ω v2 + 4ω2 − γ ω3 , = DLc0 0 a kT 2E a
(25.29)
with DLc0 v02 a/kT = B∗ for later reference. For growth of the wave, we must have σ02 ω + 4ω2 > γ ω3 , 2E a
(25.30)
i.e., σ0 > (2Eγ ω)
1/2
1 +4 aω
−1/2
.
The frequency, ω∗ , yielding a maximum in a˙ is obtained from σ2 1 ∂ a˙ + 8ω∗ − 3γ ω2 , =0= 0 ∂ω ω∗ 2E a as ω∗ =
σ02
1 2 ± 3 2E 2
3
4 σ02 3 Eγ
2 +4
σ02 . 6a Eγ
(25.31)
(25.32)
(25.33)
For very small values of a, the second term within the radical will be comparable to the ﬁrst and no real simpliﬁcation is possible. It is best to leave the expression as it is. Thus, (25.33) provides us with ω∗ for Mode I type loading and, with (25.29), we have 2 ∗ ω ∗ ∗ σ0 ∗2 ∗3 + 4ω )=V=B a(ω ˙ − γω . (25.34) 2E a
25.4. Interface Stability
50,000
10,000
σ0 (psi) 75,000 87,500100,000 25
×1 0e rg s/c m2
1020
453
Volume diffusion Surface diffusion
50
Y
75
0 10
1019
00
(v/B*) 10
50
Figure 25.4. Velocity normalized with B (from Asaro and Tiller, 1972).
0
15
00
1018
100
0
1017
1016 .07
.17
.27
.37 .47 .57 σ0 × 1010 (dynes/cm)
.67
.77
In Figs. 25.4 and 25.5, the results for V/B∗ have been plotted as a function of σ0 for a range of values of γ and compared with the similar predictions for growth via surface diffusion as described earlier; see (25.23). We note that the dependence on applied stress is not as strong for this case of volume diffusion as was the case for surface diffusion
1026
σ0(psi) 50,000 75,000 87,500 100,000
10,000
×1
0e
rg
s/c
m2
Volume diffusion Surface diffusion
25
Y
1025
50 75
1024
0 10
(V/B*)
Figure 25.5. Velocity normalized with B continued (from Asaro and Tiller, 1972).
1023
1022
0
10
50
1021 .07
.17
.27
.37
.47
.57
σ0 × 1010 (dynes/cm2)
.67
.77
454
25. Stability of Planar Interfaces σ0 (psi) 10,000 20
50,000
75,000 87,500100,000
Volume diffusion Surface diffusion 0 ergs
/cm 2
18
Y × 10
16
500
14 12 (ω* × 104)
Figure 25.6. Optimal wave frequency (from Asaro and Tiller, 1972). 10
8
00
10
0
10
6
15
00
4 500 0 100 0 150
2 0 .07
.17
.27
.37
.47
.57
.67
.77
σ0 × 1010 (dynes/cm2)
at high values of γ , but is quite comparable in this dependence at low values of γ . The strong dependence on γ should, of course, also be noted. For these calculations, the value of E = 1012 dynes/cm2 and a = 10−5 cm were used (1 dyne = 10−5 N). For a complete comparison between the volume diffusion (i.e., dissolution) case and the surface diffusion case we must also consider the relative magnitude of B∗ and the coefﬁcient B of (25.22); we recall that for surface diffusion V = 0.1Bsd σ08 /γ 3 E4 , Bsd = av02 β Ds /kT,
(25.35)
where β is the surface density of atoms. We have renamed the surface diffusion coefﬁcient Ds for clarity. Thus, if we similarly rename B∗ = Bvd , we must consider the ratio Bsd /Bvd = β Ds /c0 DL. If this ratio were small, the two mechanisms would give comparable rates of growth of the rough surface. If this ratio were near unity, the surface diffusion mechanism is strongly dominant over the volume/dissolution mechanism. Of course, in reality both mechanisms operate concurrently. The presence of surface adsorption leading to a reduction in γ will produce a strong increase in V unless there is a compensatory reduction in B. For the surface diffusion case, β may be reduced, so that Bsd may also be reduced. For the case of dissolution/volume diffusion, a signiﬁcant affect on Bvd is not anticipated, but there may be an interference with the assumption of surface equilibrium that would have a negative effect on the overall kinetics. Such effects of surface adsorption may, of course, be marked at a liquid/metal interface. In Fig. 25.6 the optimum frequency ω∗ has been plotted as a function of σ0 and it is noted that the dissolution mechanism produces a comparable, but smaller optimum wavelengths,
25.5. 2D Surface Proﬁles and Surface Stability
455
y x
Figure 25.7. 2D surface roughness.
z
λ∗ , than the surface diffusion mechanism for similar stress levels. Depending on the surface energy, there seems to be a critical stress range beyond which ω∗ increases very sharply. For example, for γ ∼ 100 erg/cm2 , and σ0 ≤ 50, 000 to 75,000 psi, λ∗ decreases rapidly and the roughness sharpens drastically (1 erg = 10−7 J and 1 psi =6.895 kPa). Finally, it should be noted that the analysis of volume diffusion as considered here should also apply to the case of diffusion via vacancy diffusion in the volume of the solid beneath the undulated surface. Equations (25.27) and (25.28) are still applicable, but with c0 being the equilibrium vacancy concentration in the solid in the unstressed state. Equations (25.29) to (25.34) also hold, with Dbd replacing Dvd in the expression for B. Thus, the ﬁgures also hold, with B changing via D and c0 .
25.5 2D Surface Proﬁles and Surface Stability As seen in the above discussion of 1D surface proﬁles, modeled as sinusoidal perturbations, the tendency for an initially nearly smooth surface in a stressed body to break down into one characterized by growing roughness, is a competition between the release of strain energy and the creation of surface energy. The driving force for the process is properly described by the gradient in chemical potential, as originally introduced in this context by Asaro and Tiller (1972). Thus we want to evaluate µ = µ0 + W(x, y)v 0 + κγ .
(25.36)
The coordinate geometry for the 2D surface proﬁles is as illustrated in Fig. 25.7. The surface energy γ is so far taken to be isotropic and independent of orientation and state of surface stress; W(x, y) is the surface strain energy density. Alternatively, we could calculate the rate of change of the total free energy, Gtot , due to growth of the surface, ˙ Gtot = µvn dS, (25.37) S
where vn is the normal growth rate described earlier and inquire as to its algebraic sign. This in itself would be sufﬁcient to assess stability, but an evaluation of µ would be desirable to carry out detailed kinetic simulations, as dictated by the appropriate mechanisms of mass transport such as surface diffusion, bulk diffusion, and dissolution and bulk transport. Since our purposes here are illustrative only, we will examine stability only. To calculate µ it is necessary to evaluate the elastic ﬁeld at the surface and evaluate the strain energy density W(x, y). A general procedure by Asaro and Tiller (1972) to accomplish this is based on a linear superposition. The method was described previously for 1D sinusoidal surface proﬁles; here we extend the analysis to a 2D sinusoidal proﬁle. Let the surface take on the perturbed shape given by z = a cos(ωx x) cos(ω y y),
(25.38)
456
25. Stability of Planar Interfaces
where ωx = 2π/λx and ω y = 2π/λ y are the respective frequencies. We assume that the surface is shallow, i.e., aωx , aω y 1. The body is loaded by a biaxially applied uniform stress, σ0 , rather than by the uniaxial stress as in the case of 1D surface proﬁles. A uniform state of stress of this type produces a traction on a so perturbed surface of the form Tx = −σ0
∂z , ∂x
Ty = −σ0
∂z , ∂y
Tz = 0,
(25.39)
to ﬁrst order in the aω’s. Thus, if we write the total stress ﬁeld as σ = σ (1) + σ (2) (x, y, z),
(25.40)
where σ (1) = σ0 ex ex + σ0 e y e y is the uniform biaxial stress state, then the perturbed ﬁeld, σ (2) , is obtained by solving the problem of applying the negative traction, given by (25.39) above, to the surface; this has the effect of producing a traction free perturbed surface, as desired. The solution for the surface displacements is ∞ ∂z ∂z (2) + %αy (x − ξ, y − η) %αx (x − ξ, y − η) dξ dη, u¯ α (x, y) = σ0 ∂x ∂y −∞ where the surface is taken as z = z(x, y), and the matrix Π has been given earlier in (13.122) as ⎧ ⎫ 2(1 − ν) 2νx 2 2νxy (1 − 2ν)x ⎪ ⎪ ⎪ ⎪ ⎪ ⎪ + 3 − ⎪ ⎪ ⎪ ⎪ 3 2 r r r r ⎪ ⎪ ⎨ ⎬ 2 1 2νxy 2(1 − ν) 2νy (1 − 2ν)y . (25.41) Π= + 3 − ⎪ 4π G ⎪ ⎪ ⎪ r3 r r r2 ⎪ ⎪ ⎪ ⎪ ⎪ (1 − 2ν)x (1 − 2ν)y 2(1 − 2ν) ⎪ ⎪ ⎪ ⎩ ⎭ 2 2 r r r Freund and Suresh (2003) have carried out this analysis and found by straightforward integration that 2σ0 aλ y u¯ (2) sin(ωx x) cos(ω y y), x =− 4 E¯ λ2x + λ2y 2σ0 aλx cos(ωx x) sin(ω y y), u¯ (2) y =− 4 E¯ λ2x + λ2y
(25.42)
u¯ (2) z = 0. The stresses follow immediately by calculating the strains and using the isotropic constitutive relations. The change in energy is the energy involved with creating the perturbation and the perturbed ﬁeld. This was also calculated by Freund and Suresh (2003). Per period over the perturbation it is found that λx λ y 1 (2) (2) [u¯ σxz + u¯ (2) δEel = y σ yz] dx dy 2 x 0 0 (25.43) π σ02 a 2 4 2 2 =− λx + λ y . 2 E¯
25.6. Asymptotic Stresses
457
The change in energy due to the creation of surface is calculated by noting that, to ﬁrst order, " 2 # ∂z ∂z 2 1 + dx dy. (25.44) d(δS) = 2 ∂x ∂y Thus, this contribution to the energy change is λx λ y " 2 2 # ∂z 1 ∂z + dx dy δEsurface = γ 2 ∂x ∂y 0 0 π 2 γ a 2 λ2x + λ2y = . 2 λx λ y
(25.45)
Therefore, if (2)
δE = δEel + δEsurface = 0
(25.46)
deﬁnes the condition for stability, i.e., for growth versus decay of the perturbation, the critical stress is obtained as 4 3 2 λ2x + λ2y σ0 1 1 = γπ = γπ + 2. (25.47) 2 ¯ λx λ y λx λy E cr Deﬁning 1 = λ∗ the stability condition (25.47) becomes 2 σ0 γπ = ∗ ¯ λ E cr
3
1 1 + 2, λ2x λy
⇒
2σ02 E¯
(25.48)
= γ ω∗ .
(25.49)
cr
This may be compared to the original criterion of this type developed by Asaro and Tiller (1972), which is ω∗ = 2π/λ∗ = 2σ02 /(γ E). The difference is simply the change from a uniaxial stress state to one of uniform biaxial stress. An interesting observation is that these results suggest that initially surface proﬁles may tend to take on a 1D shape. For example, look at the stability criterion by forming the ratio of the magnitude of the released elastic energy to the positive surface energy, viz., 3 (2) δEel λ∗ λ2 = 1 + 2x . (25.50) δEsurface λx λy When this ratio becomes greater than unity, the perturbation may grow. The smallest value of λx for which this happens is when λx = λ∗ and λ y → ∞. Of course, after initial growth the patterning may, and probably will, become multidimensional.
25.6 Asymptotic Stresses for 1D Surface Proﬁles In the previous section a general procedure was developed for calculating the asymptotic stresses on 2D surface proﬁles. Here we revisit the 1D case given out at the outset of the
458
25. Stability of Planar Interfaces
n y = a cos ω x
initial free surface
x
σο
Figure 25.8. Creation of a perturbed free surface.
y
chapter via the original analysis of Asaro and Tiller (1972). We simply seek to establish the similar procedure for constructing the surface stress ﬁeld and strain energy density required to calculate the surface chemical potential. The procedure is developed via the general sinusoidal proﬁle y = a cos(ωx). Consider the surface to be in a state of uniform biaxial stress of magnitude σ0 . If the surface was perturbed in shape with the proﬁle y = a cos(ωx), (aω 1), then we would write the stress state as σ = σ0 ex ex + σ (2) ,
(25.51)
where, as before, σ (2) is the perturbed ﬁeld. The goal is to determine σ (2) to O(aω). The traction induced over the sketched surface in Fig. 25.8 by the biaxial stress is, to ﬁrst order, Tx = σ0 nx ∼ σ0 ∂ y/∂ x ∼ −aωσ0 sin(ωx) + O(a 2 ω2 ), Ty = 0 + O(a 2 ω2 ).
(25.52)
To render the perturbed surface traction free we need to impose a shear traction −Tx = aωσ0 cos(ωx) = −σ0
∂y . ∂x
(25.53)
This deﬁnes the perturbed ﬁeld, called (2) above. Recalling the point force solution given by (15.17), yields ∞ ∂ y(ξ )/∂ξ 2σ0 (2) σxx dξ + O(a 2 ω2 ), (x) = π x−ξ −∞ (25.54) (2) σ yy (x) = 0. (2)
Of course, σxy is already speciﬁed as (2) = aωσ0 sin(ωx) = −σ0 σxy
∂y . ∂x
This procedure holds for general proﬁles so long as ∂ y/∂ x 1. When applied to the case where y = a cos(ωx), we ﬁnd ∞ sin(ωξ ) 2σ0 aω (2) dξ. σxx = − π −∞ x − ξ The (real) Cauchy principal value is needed, which is ∞ sin(ωξ ) PV dξ = −π cos(ωx). −∞ x − ξ
(25.55)
(25.56)
25.7. Suggested Reading
459
This yields the Asaro–Tiller ﬁeld, viz., (2) ∼ 2aωσ0 cos(ωx) + O(a 2 ω2 ), σxx (2) σ yy ∼ 0 + O(a 2 ω2 ),
(25.57)
(2) ∼ aωσ0 sin(ωx) + O(a 2 ω2 ). σxy
The surface strain energy density is readily computed as (2) σ02 σxx 1 (2) σ0 + σxx + O(a 2 ω2 ), + W(x) = Eb 2 E¯
(25.58)
where Eb = E/(1 − ν) is the biaxial modulus and E¯ = E/(1 − ν 2 ) is the plane strain modulus. Note that the O(a 2 ω2 ) term embedded in (25.58) would be omitted from consideration in an asymptotic analysis, but is nonetheless retained for completeness. Indeed, if one had (2) the general ﬁeld σxx = σ0 + σxx , then (25.58) would be the energy density.
25.7 Suggested Reading Asaro, R. J., and Tiller, W. A. (1972), Interface Morphology Development during Stress Corrosion Cracking. Part I: Via Surface Diffusion, Metall. Trans., Vol. 3, pp. 1789–1796. Cammarata, R. C. (1994), Surface and Interface Stress Effects in Thin Films, Progress in Surface Science, Vol. 46, pp. 1–38. Freund, L. B., and Suresh, S. (2003), Thin Film Materials: Stress, Defect Formation and Surface Evolution, Cambridge University Press, New York. Gao, H., and Nix, W. D. (1999), Surface Roughening of Heteroepitaxial Thin Films, Ann. Rev. Mater. Sci., Vol. 29, pp. 173–209. Suo, Z. (1997), Motions of Microscopic Surfaces in Materials, Adv. Appl. Mech., Vol. 33, pp. 193–294.
PART 6: PLASTICITY AND VISCOPLASTICITY
26 Phenomenological Plasticity
When stressed beyond a critical stress, ductile materials such as metals and alloys display a nonlinear plastic response. This is sketched in Fig. 26.1 for a uniaxial tensile test of a smooth specimen, where some relevant terms are deﬁned. In general, plastic yielding is gradual when resolved at typical strain levels (e.g., ∼ 10−4 ). A critical stress, called the yield stress, is deﬁned, which is the stress in uniaxial tension, or compression, required to cause a small, yet ﬁnite, permanent strain that is not recovered after unloading. It is common to take this onset yield strain as e y = 0.002 = 0.2%. Some common general features of plastic ﬂow, with reference to stress vs. strain curves, are: r The σ vs. e response is nonlinear and characterized by a decreasing intensity of strain hardening, measured by the slope dσ/de, as the strain increases. Generally, dσ/de ≥ 0. r Unloading is nearly elastic. r Plastic deformation of nonporous metals is essentially incompressible, i.e., volume preserving. A discussion of the physical basis for plastic deformation in subsequent chapters will explain why this is so. As noted, a schematic stressstrain curve during uniaxial loading and unloading of an elastoplastic material is shown in Fig. 26.1. The initial yield stress is Y (later terms such as σ y will be used to denote yield stress). Note that the yield stress is now ideally represented as a stress level at which an abrupt transition from linear, purely elastic, to nonlinear, elasticplastic deformation occurs. Below this stress level the deformation is elastic, i.e., reversible upon the removal of stress. For linear elasticity, Hooke’s law relates the stress and strain by σ = Ee, where E is Young’s modulus of elasticity (the slope of the linear portion of the curve in Fig. 26.1). When the stress is increased beyond the initial yield limit, the material deforms plastically. The nonlinear portion of the stressstrain curve is associated with plastic mechanisms of deformation due to dislocations (in metals) and is referred to as the work or strain hardening of the material. At an arbitrary state of stress σ > Y, the total strain e consists of the elastic part ee = σ/E, which is recoverable upon removal of the stress, and the plastic part e p = e − σ/E, which is the permanent (residual) strain left upon removal of the stress. It is generally assumed that plastic deformation does not affect elastic properties of the material, so that the unloading slope (Young’s modulus E) remains the same as before the plastic deformation took place. The physical basis for 461
462
26. Phenomenological Plasticity
σ
Figure 26.1. The stress strain curve during tensile loading and unloading of an elastoplastic material. The initial yield stress is Y, and the Young’s modulus of elasticity is E. At an arbitrary stage of elastoplastic deformation, the total strain is the sum of elastic and plastic parts (e = ee + e p ).
Y
E
E
0
Y/E
ep
e
ee
this assumption is made clear in the discussion of crystalline plasticity given in subsequent chapters. The concern of this chapter is the formulation of constitutive equations that describe elastoplastic material response under multiaxial states of stress. While purely elastic deformation is a history independent process, in which the current strain depends only on the current stress, elasticplastic states of strain depend on the entire history of loading and deformation. Consequently, elastoplastic constitutive equations are more appropriately expressed in an incremental or ratetype form by relating the rate of deformation to the rate of stress. Derivation of a variety of these equations is presented in this chapter. Various constitutive models are considered, applicable to either metals or geomaterials. Timeindependent response is mainly considered, although an introduction to timedependent constitutive behavior is also given. A more detailed development of strain rate and time dependent elasticplastic deformation is given in the following chapters that are concerned with physically based constitutive theory.
26.1 Yield Criteria for Multiaxial Stress States A central concept in the classical theory of rate independent plasticity is the yield surface, which deﬁnes the multiaxial states of stress at the threshold of plastic deformation. If the stress states are within the yield surface, the corresponding changes of deformation are purely elastic. Plastic deformation is possible only when the stress state is on the current yield surface. The yield surface evolves with the progression of plastic deformation due to strain hardening of the material. We analyze the shape of the initial yield surface ﬁrst, leaving the hardening models for later sections. The yield surface can be expressed as a hypersurface in the sixdimensional stress space f (σi j ) = 0 .
(26.1)
For isotropic material, the onset of plastic deformation does not depend on the directions of principal stresses, but only on their magnitudes. Thus, f can be expressed in terms of the stress invariants as f (I1 , I2 , I3 ) = 0 ,
(26.2)
26.2. Von Mises Yield Criterion
463 hydrostaic axis
von Mises
Tresca
σ3
σ1
Figure 26.2. Von Mises and Tresca yield surfaces in principal stress space. The yield cylinder and the yield prism have their axis parallel to the hydrostatic axis, which is perpendicular to the π plane (σ1 + σ2 + σ3 = 0).
σ2
π pl
ane
where I1 = σii ,
I2 =
1 (σi j σi j − σii σ j j ) , 2
I3 = det(σi j ) .
(26.3)
For nonporous metals at moderate pressures, the yield is not inﬂuenced by hydrostatic pressure, and the yield surface can be expressed in terms of the deviatoric part of stress only, i.e., f (J2 , J3 ) = 0 ,
(26.4)
where J1 = 0 ,
J2 =
1 σ σ , 2 ij ij
J3 = det(σi j ) .
(26.5)
26.2 Von Mises Yield Criterion The most frequently utilized yield criterion is the von Mises criterion J2 = k2 ,
(26.6)
where k is the material parameter (yield stress in pure shear). In an expanded form, J2 =
1 2 2 2 (σ11 − σ22 )2 + (σ22 − σ33 )2 + (σ33 − σ11 )2 + 6(σ12 + σ23 + σ31 ) . 6
(26.7)
If the yield stress in uniaxial tension is Y, then according to the von Mises criterion Y2 /3 = √ k2 , so that k = Y/ 3. The von Mises yield locus in the principal stress space is shown in Fig. 26.2. Two physical interpretations of the von Mises criterion are possible. The elastic strain energy (per unit volume) is 1 1 1 1 ei j + ekkδi j , (26.8) σ + σkkδi j W = σi j ei j = 2 2 ij 3 3
464
26. Phenomenological Plasticity
i.e., 1 1 σi j ei j + σii e j j . (26.9) 2 6 Since σi j = 2µei j , where µ denotes the elastic shear modulus, the portion of the elastic strain energy associated with the deviatoric part of stress and the resulting shape change of the material, is W=
W =
1 1 1 σi j ei j = σi j σi j = J2 . 2 4µ 2µ
(26.10)
Thus, the von Mises yield criterion can be interpreted as the criterion according to which the yield begins when the deviatoric work W reaches the critical value (k2 /2µ = Y2 /6µ). The second interpretation of the von Mises criterion is based on the octahedral shear stress. An octahedral plane is the material plane that makes equal angles with the principal stress directions at the considered point of the material. Thus, with respect to princi√ pal stress axes ei , the unit vector normal to an octahedral plane is n = ±(e1 + e2 + e3 )/ 3. Since the stress tensor can be expressed relative to its principal directions via the spectral decomposition σ = σ1 e1 e1 + σ2 e2 e2 + σ3 e3 e3 ,
(26.11)
where the product such as e1 e1 represents a dyadic product, the traction vector over the octahedral plane is 1 tn = n · σ = ± √ (σ1 e1 + σ2 e2 + σ3 e3 ) . 3
(26.12)
The magnitude of the octahedral traction is obtained from 1 2 (σ + σ22 + σ33 ) , 3 1 whereas the associated normal stress is 1 σn = tn · n = n · σ · n = (σ1 + σ2 + σ3 ) . 3 Therefore, the square of the octahedral shear stress is tn2 =
(26.13)
(26.14)
1 (σ1 − σ2 )2 + (σ2 − σ3 )2 + (σ3 − σ1 )3 . (26.15) 9 It can be shown that the octahedral shear stress is the average shear stress over all planes passing through the considered material point. Since the second invariant of the deviatoric part of stress tensor, expressed in terms of principal stresses, is τn2 = tn2 − σn2 =
J2 =
1 (σ1 − σ2 )2 + (σ2 − σ3 )2 + (σ3 − σ1 )2 , 6
(26.16)
we have the connection 2 J2 . (26.17) 3 Consequently, the von Mises yield criterion can be interpreted as the criterion according to √ which the yield begins when the octahedral shear stress reaches the critical value ( 2/3 k = √ 2 Y/3). τn2 =
26.3. Tresca Yield Criterion
465 uniaxial stress
σ2
σ2  σ3
biaxial stress pure shear
Y
Y
σ1
σ1  σ3
3
Y
Y Y
3
(a)
(b)
Figure 26.3. (a) The von Mises ellipse and the Tresca hexagon in the plane of principal stress differences; (b) the same in the case of plane stress (σ3 = 0).
We note that the von Mises yield criterion can be rewritten as (σ1 − σ3 )2 − (σ1 − σ3 )(σ2 − σ3 ) + (σ2 − σ3 )2 = Y2 .
(26.18)
This is an ellipse at 45◦ relative to the coordinates σ1 − σ3 and σ2 − σ3 (Fig. 26.3a). In the case of plane stress (σ3 = 0), we have σ12 − σ1 σ2 + σ22 = Y2 ,
(26.19)
which is an ellipse at 45◦ relative to the coordinates √ σ1 and σ2 (Fig. 26.3b). Clearly, the yield stress in pure shear (σ2 = −σ1 ) is equal to Y/ 3, whereas the yield stress in biaxial tension (σ2 = σ1 ) is the same as in uniaxial tension (Y). In the combined tensiontorsion (σ, τ ) test (as it occurs in a thinwalled tube under an axial force and a twisting moment), the principal stresses are σ1,2 =
1 σ ± (σ 2 + 4τ 2 )1/2 , 2 2
(26.20)
and the yield criterion (26.19) gives σ 2 + 3τ 2 = Y2 . (26.21) √ This is an ellipse with the semiaxes of length Y and Y/ 3 along the σ and τ axes, respectively (Fig. 26.4).
26.3 Tresca Yield Criterion The Tresca criterion is a maximum shear stress criterion: plastic deformation begins when the maximum shear stress reaches the critical value kT = Y/2, which is the maximum shear stress at yield in uniaxial tension. Analytically, the Tresca yield criterion is τmax =
1 (σmax − σmin ) = kT . 2
(26.22)
466
26. Phenomenological Plasticity
τ Y
3
von Mises Tresca
Y 2 Y
σ
Figure 26.4. The von Mises and Tresca ellipses in the case of combined tension–torsion (σ, τ ) test. According to von√ Mises criterion the yield stress in pure shear is Y/ 3, whereas according to Tresca criterion it is Y/2, where Y is the yield stress in simple tension.
Thus, the intermediate principal stress according to Tresca criterion does not have any effect on the yield. The maximum shear stress criterion can be recast in terms of principal stresses by any of the following forms 1 max σ1 − σ2 , σ2 − σ3 , σ3 − σ1  = kT , 2 1 (σ1 − σ2  + σ2 − σ3  + σ3 − σ1 ) = kT , 4 1 1 1 (σ1 − σ2 )2 − kT2 (σ2 − σ3 )2 − kT2 (σ3 − σ1 )2 − kT2 = 0 . 4 4 4
(26.23)
Since σ1 − σ2 = σ1 − σ2 , and similarly for other principal stress differences, and since the invariants of the deviatoric part of stress are J1 = (σ1 − σ2 ) + (σ2 − σ3 ) + (σ3 − σ1 ) = 0 , J2 =
1 (σ1 − σ2 )2 + (σ2 − σ3 )2 + (σ3 − σ1 )2 , 6
(26.24)
J3 = σ1 σ2 σ3 , the analytical representation of the maximum shear stress criterion (26.3) in terms of the invariants J2 and J3 is 4J23 − 27J32 − 36kT2 J22 + 96kT4 J2 − 64kT6 = 0 .
(26.25)
Because of its complexity, this representation of the yield criterion is rarely used. The Tresca yield locus for plane stress (σ3 = 0) is depicted in Fig. 26.3b. The same plot applies to threedimensional states of stress, but with respect to the stress differences as the coordinates (Fig. 26.3a). In the combined tension–torsion (σ, τ ) test, the Tresca yield criterion gives σ 2 + 4τ 2 = Y2 .
(26.26)
26.4. Mohr–Coulomb Yield Criterion
467
τn τn = c − µ*σn σ3
2α
σ1
σn
φ
Figure 26.5. The Mohr’s circle corresponding to threedimensional state of stress with maximum stress σ1 and minimum stress σ3 , and the Mohr–Coulomb envelope τn = c − µ ∗ σ n .
c µ*
This is an ellipse with the semiaxes of length Y and Y/2 along the σ and τ axes, respectively (Fig. 26.4). The von Mises yield criterion is in better agreement with experimental data than the Tresca criterion. To optimize the ﬁt with experimental data, a generalization of the von Mises criterion in the form α J32 (26.27) 1 − c 3 J2 = k2 J2 has been suggested. Usually, α is taken to be equal to one, and c is an appropriate parameter. Because of uncertainties in the description of the subsequent work hardening, the beneﬁts of using the representation (26.27) over the simple von Mises criterion J2 = k2 are hardly worth. Further discussion can be found in the book by Hill (1950), and review articles by Drucker (1960) and Naghdi (1960).
26.4 Mohr–Coulomb Yield Criterion For geomaterials such as rocks and soils and for concrete, the inelastic deformation occurs by frictional sliding over the plane of shearing, and thus the normal stress over that plane affects the yield. A simple criterion that accounts for this is a Mohr–Coulomb yield criterion τn = τf + c, where τf = −µ∗ σn is the friction stress (µ∗ = tan φ is the coefﬁcient of internal friction, φ being the angle of friction), and c is the cohesive strength of the material. Failure occurs if the Mohr’s circle corresponding to the stress state (σ1 , σ2 , σ3 ) touches the Mohr’s envelope τn = c − µ∗ σn (Fig. 26.5). The corresponding plane of failure has a normal at an angle α from the axis of the least tensile stress (σ3 ). From Fig. 26.5, 2α = π/2 − φ and σ1 − σ3 σ1 + σ3 + cos 2α , 2 2 σ1 − σ3 τn = sin 2α . 2 Thus, the Mohr–Coulomb yield criterion is σn =
(26.28)
σ1 − σ3 + (σ1 + σ3 ) sin φ = 2c cos φ ,
(26.29)
σmax − σmin + (σmax + σmin ) sin φ = 2c cos φ .
(26.30)
or, in all six sextants,
468
26. Phenomenological Plasticity
σ2
σ2 Y+
Y+
σ1 Y
Y
σ1 Y
+
Y+
Y
Y
(a)
(b)
Figure 26.6. (a) The Mohr–Coulomb hexagon for plane stress (σ3 = 0). The yield stress in simple tension is Y+ and in compression Y− . (b) The Drucker– Prager ellipse for plane stress.
It can be easily veriﬁed that, according to this criterion, the yield stress in pure shear is τY = c cos φ, whereas the yield stresses in uniaxial tension and compression are Y+ = 2c tan α and Y− = 2c cot α, respectively. We note that the Mohr–Coulomb yield criterion is of the general form f (J2 , J3 ) = a − bI1 .
(26.31)
Indeed, the criterion (26.29) can be rewritten as σ1 − σ3 +
1 2 [(σ1 − σ2 ) − (σ2 − σ3 )] sin φ = 2c cos φ − I1 sin φ , 3 3
(26.32)
where I1 = σ1 + σ2 + σ3 . The left hand side of the above equation is an isotropic function of deviatoric stress, which can thus be expressed in terms of J2 and J3 . The Mohr–Coulomb yield locus for plane stress (σ3 = 0) is depicted in Fig. 26.6a. 26.4.1 Drucker–Prager Yield Criterion For porous metals, concrete and geomaterials like soils and rocks, plastic deformation has its origin in pressure dependent microscopic processes. The corresponding yield condition depends on both deviatoric and hydrostatic parts of the stress tensor. Drucker and Prager (1952) suggested that yielding in soils occurs when the shear stress on octahedral planes overcomes cohesive and frictional resistance to sliding on these planes, i.e., when 2 k, (26.33) τoct = τf + 3 where
τoct =
2 J2 3
1/2
1 τf = −µ∗ σoct = − µ∗ I1 . 3
,
(26.34)
The yield stress in simple shear is k, the coefﬁcient of internal friction is µ∗ , the ﬁrst invariant of the Cauchy stress tensor is I1 , and J2 is the second invariant of the deviatoric part of the Cauchy stress. The yield condition is consequently 1/2
f = J2
+
1 µ∗ I1 − k = 0 . 3
(26.35)
26.4. Mohr–Coulomb Yield Criterion DruckerPrager
469
MohrCoulomb
σ2 σ2 0
σ3
σ1
σ3
σ1
Figure 26.7. The Drucker–Prager cone and the Mohr–Coulomb pyramid matched along the compressive meridian shown in (a) principal stress space and (b) deviatoric plane.
(b)
(a)
√ A modiﬁed friction parameter µ∗ = 3/2 µ∗ is conveniently introduced. The criterion geometrically represents a cone in the principal stress space with its axis parallel to √ the hydrostatic axis (Fig. 26.7). The radius of the circle in the deviatoric (π ) √ plane is 2 k, where k is the yield stress in simple shear. The angle of the cone is tan−1 ( 2 µ∗ /3). The yield stresses in uniaxial tension and compression are, according to (26.35), Y+ = √
3k 3 + µ∗
,
3k Y− = √ . 3 − µ∗
(26.36)
√ For the yield condition to be physically meaningful, the restriction holds µ∗ < 3. If the compressive states of stress are considered positive (as commonly done in geomechanics, e.g., Jaeger and Cook, 1976), a minus sign appears in front of the second term of f in (26.35). In the case of plane stress (σ3 = 0), the Drucker–Prager criterion reduces to an ellipse in the (σ1 , σ2 ) plane, with the center at the point σ1 = σ2 = −2µ∗ k/(1 − 4µ2∗ /3), Fig. 26.6b. The magnitudes of the yield stresses in simple tension and compression are as in (26.36), whereas the yield stresses in equal biaxial tension and compression are, respectively, σ+ = √
3k 3 + 2µ∗
,
3k σ− = √ . 3 − 2µ∗
(26.37)
When the Drucker–Prager cone is applied to porous rocks, it overestimates the yield stress at higher pressures, and inadequately predicts inelastic volume changes. To circumvent the former, DiMaggio and Sandler (1971) introduced an ellipsoidal cap to close the cone at the certain level of pressure. This cap is described by the equation J2 + K2
1 3
2 I1 + b
(a − b)2
= 1,
(26.38)
where a is the magnitude of the compressive stress that would alone cause the crushing of the material (apex of the cap in Fig. 26.8). Other shapes of the cap were also used. Details can be found in Chen and Han (1988). See also Ortiz (1985) and Lubarda et al. (1996).
470
26. Phenomenological Plasticity 1/2
J2 cap
yield cone K
a
1 I 3 1
k
b
Figure 26.8. The Drucker–Prager yield criterion shown in the coordinates of stress invariants I1 and J2 . The yield stress in pure shear is k, and the frictional parameter is µ∗ . At high pressure a cap is used to close the cone.
k µ
0
26.5 Gurson Yield Criterion for Porous Metals Based on a rigidperfectly plastic analysis of spherically symmetric deformation around a spherical cavity, Gurson (1977) suggested a yield criterion for porous metals in the form I1 2 Y2 = 0, (26.39) f = J2 + υY2 cosh − (1 + υ 2 ) 3 2Y 3 where υ is the porosity (void/volume fraction) and Y is the tensile yield stress of the matrix material (Fig. 26.9). To improve the agreement with experimental data on ductile void growth, Tvergaard (1982) introduced two additional material parameters (q1 , q2 ) in the structure of the Gurson yield criterion, such that q2 I1 2 Y2 2 = 0. (26.40) − (1 + q12 υ 2 ) f = J2 + υY q1 cosh 3 2Y 3 Further reﬁnements of the model were suggested by Tvergaard and Needleman (1984) and Mear and Hutchinson (1985). If there is no porosity (υ = 0), both (26.39) and (26.40) reduce to von Mises yield criterion J2 = Y2 /3.
26.6 Anisotropic Yield Criteria An anisotropic generalization of the von Mises yield criterion, due to Hill (1950), replaces J2 with a general quadratic function of the stress components 1 Ai jkl σi j σkl = k2 , 2
(26.41)
where the anisotropy tensor Ai jkl has the same symmetries as the elastic stiffness tensor (Ai jkl = Ajikl = Akli j ). Decomposing the stress tensor into its deviatoric and hydrostatic parts σi j = σi j − pδi j ,
1 p = − σkk , 3
(26.42)
1/2
J2 Y 3 1 υ I1 2Y ln υ
0
ln υ
Figure 26.9. Gurson yield condition for porous metals with the void/volume fraction υ. The tensile yield stress of the matrix material is Y.
26.7. ElasticPlastic Constitutive Equations
471
the yield criterion (26.41) can be rewritten as 1 1 Ai jkl σi j σkl − pAi jkkσi j + p2 Aii j j = k2 . (26.43) 2 2 Consequently, if the plastic yield is independent of p, we must have Ai jkk = 0, and the yield criterion reduces to 1 Ai jkl σi j σkl = k2 . (26.44) 2 The von Mises isotropic yield condition is recovered if 1 1 (δikδ jl + δil δ jk) − δi j δkl . (26.45) 2 3 The most wellknown anisotropic yield criterion of the type considered in this section is the Hill’s orthotropic yield criterion. Hill (1948) introduced the yield condition, expressed relative to the principal axes of orthotropy, in the form Ai jkl =
2 2 2 F(σ22 − σ33 )2 + G(σ22 − σ11 )2 + H(σ11 − σ22 )2 + 2Lσ23 + 2Mσ31 + 2Nσ12 = 1,
where F, G, H, L, M, N are the material parameters. If the tensile yield stresses in the directions of the principal axes of orthotropy are Y1 , Y2 , and Y3 , then 1 = H+ F, Y22
1 = G+ H, Y12
1 = F + G. Y32
Consequently, the material parameters F, G, and H are speciﬁed by 1 1 1 1 F= + 2− 2 , 2 Y22 Y3 Y1 1 G= 2 H=
1 2
(26.46)
(26.47)
1 1 1 + 2− 2 2 Y3 Y1 Y2 1 1 1 + 2− 2 Y12 Y2 Y3
,
(26.48)
.
(26.49)
Furthermore, if T12 , T23 , and T31 are the yield stresses under pure shear in the corresponding planes of orthotropy, we have L=
1 , 2 2T23
M=
1 , 2 2T31
N=
1 . 2 2T12
(26.50)
In the case of transverse isotropy (with the axis 3 as the axis of transverse isotropy), the relationships hold N = F + 2H = G + 2H ,
L = M.
(26.51)
For a fully isotropic material, L = M = N = 3F = 3G = 3H.
26.7 ElasticPlastic Constitutive Equations In the ratetype theory of plasticity, the rate of deformation tensor D (symmetric part of the velocity gradient L = F˙ · F−1 ) is decomposed into the elastic and plastic parts, such that
472
26. Phenomenological Plasticity
D = De + Dp .
(26.52)
The elastic part gives a reversible part of the strain increment De dt in an inﬁnitesimal loading–unloading cycle of the stress increment τ dt. Thus, if Me is the fourthorder tensor of elastic compliances, we have
De = Me : τ ,
(26.53)
τ = σ˙ + σ trD − W · σ + σ · W
(26.54)
where
is the Jaumann rate of the Kirchhoff stress τ = (det F)σ, with the current state as the reference. For inﬁnitesimally small elastic deformation of isotropic materials, the rectangular components of the elastic compliance tensor (inverse of the elastic moduli tensor) are 1 1 λ (26.55) (δikδ jl + δil δ jk) − δi j δkl . Miejkl = 2µ 2 2µ + 3λ The Lame´ elastic constants are λ and µ, and δi j denotes the Kronecker delta. In the socalled associative theory of plasticity, the plastic part of the rate of deformation tensor is codirectional with the outward normal to the yield surface in stress space, i.e., Dp = γ˙
∂f , ∂σ
γ˙ > 0 .
(26.56)
It can be shown that this normality rule follows from the plasticity postulate, which states that the net work in an isothermal cycle of strain must be positive if a cycle involves plastic deformation at some stage (Ilyushin, 1961; Hill and Rice, 1973). In the context of inﬁnitesimal strain, Drucker (1951, 1959) introduced a plasticity postulate based on stress cycles, which also leads to normality rule and the convexity of the yield surface. Assuming that the response is incrementally linear, the loading index γ˙ can be expressed as 1 ∂f :τ , (26.57) γ˙ = H ∂σ where H is a scalar parameter dependent on the history of deformation. For a given representation of the yield function and its evolution, this parameter can be determined from the consistency condition for continuing plastic deformation f˙ = 0. In the material is in the hardening range (H > 0), three types of response can be identiﬁed, depending on the direction of stress increment. These are ⎧ ⎪ ⎪> 0, plastic loading, ∂f ⎨ : τ = 0, neutral loading, (26.58) ⎪ ∂σ ⎪ ⎩< 0, elastic unloading. Thus, in the case of plastic loading Dp =
1 H
∂f :τ ∂σ
∂f . ∂σ
(26.59)
Physically, the plastic increment of the rate of deformation tensor Dp dt is the residual strain increment left upon a cycle of application and removal of the stress increment τ dt.
26.8. Isotropic Hardening
473
The overall elastoplastic constitutive structure is obtained by combining (26.53) and (26.59). This gives 1 ∂f ∂f D = Me + (26.60) :τ. H ∂σ ∂σ The scalar parameter H can be positive, negative or equal to zero. Three types of response are thus possible within this constitutive framework. They are ∂f : τ > 0, hardening, ∂σ ∂f (26.61) : τ < 0, softening, H < 0, ∂σ ∂f : τ = 0, ideally plastic. H = 0, ∂σ Starting from the current yield surface in stress space, the stress point moves outward in the case of hardening, inward in the case of softening, and tangentially to the yield surface in the case of ideally plastic response. In the case of softening, D is not uniquely determined by the prescribed stress rate τ , because either (26.60) or the elastic unloading expression applies, H > 0,
D = Me : τ .
(26.62)
In the case of ideally plastic response, the plastic part of the strain rate is indeterminate to the extent of an arbitrary positive multiple, since γ˙ in (26.57) is indeterminate. Clearly, from (26.59), 1 ∂f 2 p :τ , τ :D = (26.63) H ∂σ which is positive in the hardening range and negative in the softening range of the material response. The inverted form of (26.60) is ∂f 1 ∂f : D, (26.64) Λe : : Λe τ = Λe − h ∂σ ∂σ where Λe is the elastic stiffness tensor (inverse of Me ), and h= H+
∂f ∂f : Λe : . ∂σ ∂σ
(26.65)
26.8 Isotropic Hardening Suppose that the yield function is an isotropic function of stress throughout the deformation process, i.e., f (σ, K) = 0,
(26.66)
K = K(ϑ)
(26.67)
where
is a scalar function of deformation history which deﬁnes the size of the current yield surface. The hardening model in which the yield surface expands during plastic deformation,
474
26. Phenomenological Plasticity
preserving its shape, is known as the isotropic hardening model. Because f is taken to be an isotropic function of stress, the material is assumed to be isotropic. The history parameter ϑ can be taken to be the generalized plastic strain, deﬁned by t (26.68) ϑ= (2 Dp : Dp )1/2 dt. 0
The consistency condition for continuing plastic deformation, which requires that the stress state remains on the yield surface during plastic deformation, is f˙ =
∂f ∂K ∂f :τ+ ϑ˙ = 0 . ∂σ ∂ K ∂ϑ
(26.69)
Since, from (26.56), (26.57), and (26.68), ϑ˙ = (2 Dp : Dp )1/2 =
1 ∂ f ∂ f 1/2 ∂ f : :τ , 2 H ∂σ ∂σ ∂σ
(26.70)
the substitution into (26.69) gives ∂ f ∂ f 1/2 ∂ f dK : 2 H=− . ∂ K dϑ ∂σ ∂σ
(26.71)
26.8.1 J2 Flow Theory of Plasticity Suppose that the yield criterion is of the von Mises type f = J2 − k2 (ϑ) = 0,
J2 =
1 σ : σ , 2
(26.72)
where σ is a deviatoric part of σ. It readilly follows that ∂f = σ ∂σ
(26.73)
and p
H = 4k2 ht .
(26.74)
The plastic tangent modulus in the pure shear test is p
ht =
dk . dϑ
(26.75)
Equation (26.73) implies that plastic deformation is isochoric, tr Dp = 0. The total rate rate of deformation is 1 σ σ e D= M + p :τ. σ : σ 2ht
(26.76)
(26.77)
The plastic loading condition in the hardening range is
σ : τ > 0.
(26.78)
26.9. Kinematic Hardening
475
σ σy+ σy0 Figure 26.10. Illustration of the Bauschinger effect (σ y−  < σ y+ ) in uniaxial tension.
e 0 −
σy−
The inverse equation is
σ σ 2µ τ = Λ − p 1 + ht /µ σ : σ
e
: D,
(26.79)
which applies for σ : D > 0.
(26.80)
In retrospect, the plastic rate of deformation can be expressed either in terms of the stress rate or the total rate of deformation as
Dp =
1 σ : τ 1 σ : D σ = σ . p p 2ht σ : σ 1 + ht /µ σ : σ
(26.81)
The derivation of elastoplastic constitutive equations within the framework of inﬁnitesimal strain, with a historical perspective, can be found in the books by Hill (1950), Kachanov (1971), and Johnson and Mellor (1973).
26.9 Kinematic Hardening To account for the Bauschinger effect (Fig. 26.10) and anisotropic hardening, and thus provide better description of material response under cyclic loading, a simple model of kinematic hardening was introduced by Melan (1938) and Prager (1955, 1956). According to this model, the initial yield surface does not change its size and shape during plastic deformation, but translates in the stress space according to some prescribed rule (Fig. 26.11). If the yield criterion is pressureindependent, it is assumed that f (σ − α, K0 ) = 0,
K0 = const.,
(26.82)
where α represents the current center of the yield locus in the deviatoric plane (back stress), and f is an isotropic function of the stress difference σ − α (Fig. 26.12). The size of the yield locus is speciﬁed by the constant K0 . The consistency condition for continuing plastic deformation is ∂ f : τ − α = 0. ∂σ
(26.83)
476
26. Phenomenological Plasticity
σ σy0 2 σ 0y
e
0
−
Figure 26.11. Onedimensional stressstrain response according to linear kinematic hardening model.
σy0
Suppose that the yield surface instantaneously translates so that the evolution of back stress is governed by
α = c(α, ϑ) Dp + C(α, ϑ) (Dp : Dp )1/2 ,
(26.84)
where c and C are the appropriate scalar and tensor functions of α and ϑ. This representation is in accord with assumed time independence of plastic deformation, which requires (26.84) to be homogeneous function of degree one in the components of plastic rate of deformation. Since the plastic rate of deformation is Dp = γ˙
∂f , ∂σ
the substitution of (26.84) into (26.83) gives the loading index 1 ∂f :τ . γ˙ = H ∂σ The hardening parameter H is deﬁned by ∂ f ∂ f 1/2 ∂f ∂f ∂f H=c : : C: + . ∂σ ∂σ ∂σ ∂σ ∂σ
(26.85)
(26.86)
(26.87)
If the yield condition is speciﬁed by f =
1 (σ − α) : (σ − α) − k02 = 0, 2
(26.88)
then ∂f = σ − α. ∂σ
(26.89)
The loading index is γ˙ =
1 (σ − α) : τ , H
(26.90)
with H = 2ck02 +
√
2k0 C : (σ − α) .
(26.91)
26.9. Kinematic Hardening
dα ~ D p
477
dα ~ (σ′ α) Figure 26.12. Translation of the yield surface according to kinematic hardening model. The center of the yield surface is the back stress α. Its evolution is governed by dα ∼ Dp according to Prager’s model, and by dα ∼ (σ − α) according to Ziegler’s model.
σ′ 0
α f(σ α,Κ 0) = 0
f(α,Κ 0) = 0
26.9.1 Linear and Nonlinear Kinematic Hardening p
When C = 0 and c = 2ht , the model with evolution equation (26.84) reduces to Prager’s linear kinematic hardening (Fig. 26.12). The corresponding elastoplastic constitutive equation is 1 (σ − α) (σ − α) :τ, (26.92) D = Me + p 2ht (σ − α) : (σ − α) with plastic loading condition in the hardening range
(σ − α) : τ > 0.
(26.93)
The inverse equation is τ = Λe −
(σ − α) (σ − α) 2µ : D, p 1 + ht /µ (σ − α) : (σ − α)
(26.94)
provided that (σ − α) : D > 0.
(26.95)
Alternatively, by using the suggestion by Ziegler (1959), the evolution equation for back stress can be taken in the form
α = β˙ (σ − α).
(26.96)
The proportionality factor β˙ is determined from the consistency condition in terms of σ and α (Fig. 26.12). Detailed analysis is available in the book by Chakrabarty (1987). Duszek and Perzyna (1991) used an evolution equation that is a linear combination of the Prager and Ziegler hardening rules. A nonlinear kinematic hardening model of Armstrong and Frederick (1966) is obtained if C in (26.84) is taken to be proportional to back stress, C = −c0 α, where c0 is a constant material parameter. In this case
α = 2h Dp − c0 α (Dp : Dp )1/2 ,
(26.97)
478
26. Phenomenological Plasticity
σ σ σ0
σ
e
0
fk
k
Figure 26.13. Geometric illustration of isotropic, kinematic, and combined hardening. The initial yield surface ( f0 ) expands in the case of isotropic, translates in the case of kinematic ( fk ), and expands and translates in the case of combined hardening ( fc ).
f0 c
fc fi
i
with h as another material parameter. The added nonlinear term in (26.97), referred to as a recall term, gives rise to hardening moduli for reversed plastic loading that are in better agreement with experimental data. It follows that
(σ − α) : τ 1 (σ − α) , D = 2h(1 − m) (σ − α) : (σ − α) p
(26.98)
where m=
c0 (σ − α) : α . 2 h [(σ − α) : (σ − α)]1/2
(26.99)
If the yield surface expands and translates during plastic deformation, we have a combined isotropic–kinematic hardening (Fig. 26.13). For example, consider 1 (σ − α) : (σ − α) = kα2 (ϑ), (26.100) 2 where α represents the current center of the yield surface and kα (ϑ) is its current radius. If the evolution equation for the back stress α is given by (26.97), we obtain
Dp =
(σ − α) : τ 1 (σ − α) . p 2hα + 2h(1 − m) (σ − α) : (σ − α)
(26.101)
p
The rate of the yield surface expansion is hα = dkα /dϑ, and the parameter m is speciﬁed by p (26.99). For purely kinematic hardening hα = 0, whereas for a purely isotropic hardening p p hα = ht (plastic tangent modulus in simple shear). More involved, multisurface hardening models were proposed by Mroz ´ (1967, 1976), Dafalias and Popov (1975,1976), and Krieg (1975). A review of these models is given in the book by Khan and Huang (1995). See also the books by Lubliner (1990) and Lubarda (2002).
26.10 Constitutive Equations for PressureDependent Plasticity Suppose that the pressuredependent yield criterion is of the type f (J2 , I1 , K) = 0,
(26.102)
where J2 and I1 stand for the second invariant of the deviatoric stress and the ﬁrst invariant of the stress, whereas K designates an appropriate history dependent parameter. If it is
26.10. PressureDependent Plasticity
479
assumed that plastic part of the rate of deformation tensor is normal to the yield surface, we have Dp = γ˙
∂f , ∂σ
∂f ∂f ∂f = σ + I. ∂σ ∂ J2 ∂ I1
(26.103)
The unit secondorder tensor whose components are δi j is denoted by I. The loading index can be expressed from the consistency condition f˙ = 0 as 1 ∂f ∂f σ + I :τ, (26.104) γ˙ = H ∂ J2 ∂ I1 where H is a hardening modulus. The substitution of (26.104) into (26.103) gives 1 ∂f ∂f ∂f ∂f p σ + I σ + I :τ. (26.105) D = H ∂ J2 ∂ I1 ∂ J2 ∂ I1 The volumetric part of the plastic rate of deformation is ∂f 3 ∂f ∂f p tr D = σ + I :τ. H ∂ I1 ∂ J2 ∂ I1
(26.106)
In the case of the Drucker–Prager yield criterion for geomaterials, we have ∂f 1 −1/2 = J2 , ∂ J2 2 and H=
p ht
dk , = dϑ
∂f 1 = µ∗ ∂ I1 3
ϑ=
t
(2 Dp : Dp )
(26.107)
1/2
dt.
(26.108)
0
The relationship k = k(ϑ) between the shear yield stress k under a given superimposed pressure, and the generalized shear plastic strain ϑ, is assumed to be known. Note that ϑ˙ = γ˙ . In the case of the Gurson yield criterion for porous metals, we have I1 ∂f 1 ∂f (26.109) = 1, = υ Y sinh ∂ J2 ∂ I1 3 2Y and H=
2 I1 I1 υ(1 − υ)Y3 sinh υ − cosh . 3 2Y 2Y
(26.110)
The change in porosity during plastic deformation is speciﬁed by the evolution equation, such as υ˙ = (1 − υ) tr Dp .
(26.111)
Other evolution equations, which take into account nucleation and growth of voids, have also been considered (e.g., Tvergaard and Needleman, 1984). From (26.111) and (26.103) it follows that the porosity evolves according to I1 . (26.112) υ˙ = γ˙ υ(1 − υ)Y sinh 2Y
480
26. Phenomenological Plasticity
26.11 Nonassociative Plasticity Constitutive equations in which plastic part of the rate of deformation is normal to the yield surface f = 0, i.e., ∂f , (26.113) Dp = γ˙ ∂σ are referred to as the associative ﬂow rules. A sufﬁcient condition for this constitutive structure is that the material obeys the Ilyushin’s work postulate (Ilyushin, 1961). However, many pressuredependent dilatant materials, with internal frictional effects, are not well described by the associative ﬂow rules. For example, the associative ﬂow rules largely overestimate inelastic volume changes in geomaterials such as rocks and soils (Rudnicki and Rice, 1975; Rice, 1977), and in certain highstrength steels exhibiting the strengthdifferential effect by which the yield strength is higher in compression than in tension (Spitzig, Sober, and Richmond, 1975). For such materials, plastic part of the rate of strain is taken to be normal to the plastic potential surface g = 0,
(26.114)
which is distinct from the yield surface f = 0. The resulting constitutive structure, ∂g , (26.115) Dp = γ˙ ∂σ is referred to as a nonassociative ﬂow rule. The consistency condition f˙ = 0 gives the loading index 1 ∂f :τ , (26.116) γ˙ = H ∂σ where H is a hardening modulus. Thus, 1 ∂ f ∂g :τ . (26.117) Dp = H ∂σ ∂σ The overall elasticplastic constitutive structure is 1 ∂g ∂ f D = Me + :τ. (26.118) H ∂σ ∂σ Because g = f , the elastoplastic compliance tensor in (26.118) does not possess a reciprocal symmetry. In an inverted form, the constitutive equation (26.118) becomes ∂f 1 ∂g e e e :Λ τ = Λ − : D, (26.119) Λ : h ∂σ ∂σ where ∂g ∂f : Λe : . (26.120) h= H+ ∂σ ∂σ
26.12 Plastic Potential for Geomaterials To better describe inelastic behavior of geomaterials whose yield is governed by the Drucker–Prager yield criterion of (26.35), a nonassociative ﬂow rule is used with the plastic potential (Fig. 26.14) given by 1 1/2 (26.121) g = J2 + β I1 − k = 0. 3
26.12. Plastic Potential for Geomaterials
481
J 21/2 p
D ~
g
σ
f
Figure 26.14. Illustration of a nonassociative ﬂow rule. The plastic rate of deformation Dp is normal to the ﬂow potential g = 0, which is distinct from the yield surface f = 0.
σ
g= 0 1 3 I1
f=0
0 The material parameter β is in general different from the friction parameter µ∗ of (26.35). Thus, 1 −1/2 1 ∂g = γ˙ J2 (26.122) σ + βI . Dp = γ˙ ∂σ 2 3 The loading index γ˙ is determined from the consistency condition. Assuming known the relationship k = k(ϑ) between the shear yield stress and the generalized shear plastic strain ϑ, deﬁned by (26.108), the consistency condition f˙ = 0 gives 1 1 −1/2 1 dk p J . (26.123) γ˙ = σ + µ∗ I : τ , H = ht = H 2 2 3 dϑ The substitution of (26.123) into (26.122) yields 1 −1/2 1 1 −1/2 1 1 Dp = J2 J2 σ + βI σ + µ∗ I : τ . H 2 3 2 3 The deviatoric and spherical parts of the plastic rate of deformation are 1 σ σ : τ 1 p + µ∗ tr τ , D = 2H J 1/2 2 J 1/2 3 2
β tr D = H
(26.124)
(26.125)
2
p
σ : τ 1/2
2 J2
1 + µ∗ tr τ . 3
(26.126)
To physically interpret the parameter β, we observe from (26.122) that 1/2
(2 Dp : Dp )
= γ˙ ,
tr Dp = β γ˙ ,
(26.127)
i.e., β=
tr Dp (2 Dp : Dp )1/2
.
(26.128)
Thus, β is the ratio of the volumetric and shear part of the plastic rate of deformation, which is often called the dilatancy factor (Rudnicki and Rice, 1975). The frictional parameter and inelastic dilatancy of the material actually change with the progression of inelastic deformation, but are here treated as constants. This is further analyzed by NematNasser and Shokooh (1980) and NematNasser (1983).
482
26. Phenomenological Plasticity
The deviatoric and spherical parts of the total rate of deformation are, respectively, 1 σ σ : τ τ 1 + D = + µ∗ tr τ , (26.129) 2µ 2H J 1/2 2 J 1/2 3 2
2
β 1 tr τ + tr D = 3κ H
σ : τ 1/2
2 J2
1 + µ∗ tr τ . 3
(26.130)
These can be inverted to give the deviatoric and spherical parts of the stress rate. The results are " # σ σ : D κ 1 tr D , (26.131) τ = 2µ D − + µ∗ c J 1/2 2 J 1/2 2µ 2
3κ tr τ = c
2
# " H σ : D , 1+ tr D − β 1/2 µ J2
(26.132)
where c =1+
H κ + µ∗ β . µ µ
If the friction coefﬁcient µ∗ is equal to zero, (26.131) and (26.132) reduce to σ : D 1 τ = 2µ D − σ , 1 + H/µ 2 J2
(26.133)
(26.134)
σ : D β tr τ = 3κ tr D − . 1 + H/µ J 1/2 2
(26.135)
With a vanishing dilatancy factor (β = 0), (26.134) and (26.135) coincide with the constitutive equations of isotropic hardening pressureindependent metal plasticity.
26.13 RateDependent Plasticity In the modeling of ratedependent plastic response of metals and alloys, there is no yield surface in the model and plastic deformation commences from the onset of loading, although it may be exceedingly small below certain levels of applied stress. In his analysis of ratedependent behavior of metals, Rice (1970, 1971) showed that the plastic rate of deformation can be derived from a scalar ﬂow potential , as its gradient Dp =
∂ (σ, T, H) , ∂σ
(26.136)
provided that the rate of shearing on any given slip system within a crystalline grain depends on local stresses only through the resolved shear stress. The history of deformation is represented by the pattern of internal rearrangements H, and the absolute temperature is T. Geometrically, the plastic part of the strain rate is normal to surfaces of constant
26.13. RateDependent Plasticity
483
ﬂow potential in stress space. Timeindependent behavior can be recovered, under certain idealizations – neglecting creep and rate effects, as an appropriate limit. In this limit, at each instant of deformation there is a range in stress space over which the ﬂow potential is constant. The current yield surface is then a boundary of this range, a singular clustering of all surfaces of constant ﬂow potential. The powerlaw representation of the ﬂow potential is 2γ˙ 0 = m+ 1
1/2
J2 k
m 1/2
J2 ,
J2 =
1 σ : σ , 2
(26.137)
where k = k(T, H) is the reference shear stress, γ˙ 0 is the reference shear strain rate to be selected for each material, and m is the material parameter. The corresponding plastic part of the rate of deformation is 1/2 m J2 σ . (26.138) Dp = γ˙ 0 1/2 k J 2
The equivalent plastic strain ϑ, deﬁned by (26.69), is usually used as the only history parameter, and the reference shear stress depends on ϑ and T according to T − T0 ϑ α exp −β k = k0 1 + 0 . ϑ Tm − T0
(26.139)
Here, k0 and ϑ 0 are the normalizing stress and strain, T0 and Tm are the room and melting temperatures, and α and β are the material parameters. The total rate of deformation is
D = Me : τ + γ˙ 0
1/2
J2 k
m
σ 1/2
J2
.
(26.140)
The instantaneous elastic compliance tensor is Me . From the onset of loading the deformation rate consists of elastic and plastic constituents, although for large m the plastic contribution may be small if J2 is less than k. The inverted form of (26.140), expressing τ in terms of D, is 1/2 m J2 σ τ = Λe : D − 2µγ˙ 0 . (26.141) 1/2 k J 2
Another representation of the ﬂow potential, according to the Johnson–Cook (1983) model, is " 1/2 # J2 2γ˙ 0 k exp a −1 . (26.142) = a k The reference shear stress is k=k
0
ϑ 1+b ϑ0
c " # T − T0 d , 1− Tm − T0
(26.143)
484
26. Phenomenological Plasticity
τ ht
E
Figure 26.15. Nonlinear stressstrain response in pure shear. Indicated are the initial elastic modulus E, the secant modulus hs , and the tangent modulus ht .
hs
γ 0
where a, b, c, and d are the material parameters. The corresponding plastic part of the rate of deformation becomes # " 1/2 J2 σ p 0 −1 . (26.144) D = γ˙ exp a 1/2 k J 2
26.14 Deformation Theory of Plasticity Simple plasticity theory has been suggested for proportional loading and small deformation by Hencky (1924) and Ilyushin (1947, 1963). Assume that the loading is such that all stress components increase proportionally, i.e., σ = c(t) σ ∗ ,
(26.145)
where σ ∗ is the stress tensor at an instant t ∗ and c(t) is a monotonically increasing function of t, with c(t ∗ ) = 1. This implies that the principal directions of σ remain ﬁxed during the deformation process and parallel to those of σ ∗ . Because the stress components proportionally increase, and no elastic unloading takes place, it is assumed that elastoplastic response can be described macroscopically by the constitutive structure of nonlinear elasticity, in which the total strain is a function of the total stress. Thus, we decompose the strain tensor into elastic and plastic parts, e = ee + ep ,
(26.146)
and assume that ee = Me : σ ,
ep = ϕ σ ,
(26.147)
where Me is the elastic compliance tensor, and ϕ is an appropriate scalar function to be determined in accord with experimental data. The prime designates a deviatoric part, so that plastic strain tensor is assumed to be traceless. Suppose that a nonlinear relationship τ = τ (γ )
(26.148)
between the stress and strain is available from the elastoplastic shear test. Let the secant and tangent moduli be deﬁned by (Fig. 26.15) hs =
τ , γ
ht =
dτ , dγ
(26.149)
26.14. Deformation Theory of Plasticity
and let
τ=
1 σ : σ 2
Since
1/2
γ = (2 e : e )
,
485
e =
1/2
.
(26.150)
1 + ϕ σ , 2µ
(26.151)
1 1 . − 2hs 2µ
(26.152)
the substitution into (26.150) gives ϕ=
26.14.1 RateType Formulation of Deformation Theory Although the deformation theory of plasticity is a total strain theory, deformation theory can be cast in the ratetype form. This is important for the comparison with the ﬂow theory of plasticity and for extending the application of the resulting constitutive equations beyond the proportional loading. The ratetype formulation is also needed whenever the considered boundary value problem is being solved in an incremental manner. In place of (26.146) and (26.147), we take D = De + Dp ,
(26.153)
De = Me : τ ,
(26.154)
Dp = ϕ˙ σ + ϕ τ .
(26.155)
The deviatoric and spherical parts of the total rate of deformation tensor are accordingly 1 + ϕ τ , (26.156) D = ϕ˙ σ + 2µ tr D =
1 tr τ . 3κ
(26.157)
To derive an expression for the rate ϕ, ˙ we use τ τ˙ =
1 σ : τ, 2
γ γ˙ = 2 e : D.
(26.158)
In view of (26.149), (26.151), and (26.152), this gives 1 σ : τ = ht σ : D . 2
(26.159)
When (26.156) is incorporated into (26.159), there follows 1 ϕ˙ = 2
1 1 − ht hs
σ : τ . σ : σ
(26.160)
486
26. Phenomenological Plasticity
τ p
ht
Figure 26.16. Shear stress vs. plastic shear strain. The plastic secant modulus is p p hs , and the plastic tangent modulus is ht .
p
hs
0
γ
p
Substituting (26.160) into (26.156), the deviatoric part of the total rate of deformation becomes " # hs σ :τ 1 (26.161) D = τ + −1 σ . 2hs ht σ : σ
Equation (26.161) can be inverted to express the deviatoric part of τ as ht σ : D τ = 2hs D − 1 − σ . hs σ : σ
(26.162)
During the initial, purely elastic, stage of deformation ht = hs = µ. The onset of plasticity, beyond which (26.161) and (26.162) apply, occurs when τ , deﬁned by the second invariant of the deviatoric stress in (26.150), reaches the initial yield stress in shear. The resulting theory is often referred to as the J2 deformation theory of plasticity. If plastic secant and tangent moduli are used (Fig. 26.16), related to secant and tangent moduli with respect to total strain by 1 1 1 1 1 − p = − p = , ht hs µ ht hs
(26.163)
the plastic part of the rate of deformation can be rewritten as 1 D = pτ + 2hs p
1 1 p − p 2ht 2hs
σ : τ σ . σ : σ
(26.164)
26.14.2 Application beyond Proportional Loading Deformation theory agrees with ﬂow theory of plasticity only under proportional loading, because then speciﬁcation of the ﬁnal state of stress also speciﬁes the stress history. For general (nonproportional) loading, more accurate and physically appropriate is the ﬂow theory of plasticity, particularly with an accurate modeling of the yield surface and the hardening characteristics. Budiansky (1959), however, indicated that deformation theory can be successfully used for certain nearly proportional loading paths, as well. The stress rate τ in (26.164) then does not have to be codirectional with σ . The ﬁrst and third term p (both proportional to 1/2hs ) in (26.164) do not cancel each other in this case (as they do for proportional loading), and the plastic part of the rate of deformation depends on both components of the stress rate τ , one in the direction of σ and the other normal to it. In contrast, according to the ﬂow theory with the von Mises smooth yield surface,
26.15. J 2 Corner Theory
487
the component of the stress rate τ normal to σ (thus tangential to the yield surface) does not affect the plastic part of the rate of deformation. Physical theories of plasticity (Batdorf and Budiansky, 1954; Sanders, 1955; Hill, 1967) indicate that the yield surface of a polycrystalline aggregate develops a vertex at its loading stress point, so that inﬁnitesimal increments of stress in the direction normal to σ indeed cause further plastic ﬂow (“vertex softening”). Because the structure of the deformation theory of plasticity under proportional loading does not use any notion of the yield surface, Budiansky suggested that (26.164) can be adopted to describe the response when the yield surface develops a vertex. If (26.164) is rewritten in the form 1 σ : τ 1 σ : τ p σ σ , (26.165) + D = p τ − p σ : σ 2hs 2ht σ : σ the ﬁrst term on the righthand side gives the response to component of the stress increment p normal to σ . The associated plastic modulus is hs . The plastic modulus associated with the p component of the stress increment in the direction of σ is ht . Therefore, for continued plastic ﬂow with small deviations from proportional loading (so that all yield segments which intersect at the vertex are active – fully active loading), (26.165) can be used as a model of a pointed vertex (Storen ¨ and Rice, 1975). The idea was used by Rudnicki and Rice (1975) to model the inelastic behavior of ﬁssured rocks. For the full range of directions of the stress increment, the relationship between the rates of stress and plastic deformation is not necessarily linear, although it is homogeneous in these rates, in the absence of timedependent (creep) effects. A corner theory that predicts continuous variation of the stiffness and allows increasingly nonproportional increments of stress was formulated by Christoffersen and Hutchinson (1979). This is discussed in the next subsection. When applied to the analysis of necking in thin sheets under biaxial stretching, the results were in better agreement with experiments than those obtained from the theory with a smooth yield surface. Further discussion can be found in Section 30.5 of this book.
26.15 J 2 Corner Theory In phenomenological J2 corner theory of plasticity, proposed by Christoffersen and Hutchinson (1979), the instantaneous elastoplastic moduli for nearly proportional loading are chosen equal to the J2 deformation theory moduli, whereas for increasing deviation from proportional loading the moduli increase smoothly until they coincide with elastic moduli for stress increments directed along or within the corner of the yield surface. The yield surface in the neighborhood of the loading point in deviatoric stress space (Fig. 26.17) is a cone around the axis l=
σ (σ :
p Mdef
: σ )1/2
,
(26.166)
p
where Mdef is the plastic compliance tensor of the deformation theory. The angular measure θ of the stress rate direction, relative to the cone axis, is deﬁned by p
cos θ =
l : Mdef : τ
p
(τ : Mdef : τ )1/2
.
(26.167)
488
26. Phenomenological Plasticity
total loading
τ θn θ
θ0
θc
Figure 26.17. Near proportional or total loading range at the yield vertex of J2 corner theory is a cone with the angle θ0 around the axis l ∼ σ . The vertex cone is deﬁned by the angle θc , and θn = θc − π/2.
σ 0
The conical surface separating elastic unloading and plastic loading is θ = θc , so that plastic rate of deformation falls within the range 0 ≤ θ ≤ θn , where θn = θc − π/2. The range of near proportional loading is 0 ≤ θ ≤ θ0 . The angle θ0 is a suitable fraction of θn . The range of near proportional loading is the range of stressrate directions for which no elastic unloading takes place on any of the yield vertex segments. This range is also called the fully active or total loading range. The stressrate potential at the corner is deﬁned by % = %e + %p ,
p
%p = f (θ)%def .
(26.168)
The elastic contribution to the stressrate potential is %e =
1 τ : Me : τ . 2
(26.169)
The plastic stressrate potential of the J2 deformation theory can be written, from (26.161), as hs hs 1 1 σ σ p p p %def = τ : Mdef : τ , Mdef = −1 A+ 1− , 2 2hs µ ht σ : σ where Ai jkl =
1 1 (δikδ jl + δil δ jk) − δi j δkl . 2 3
(26.170)
p
The plastic stressrate potential %def is weighted by the cone transition function f (θ) to obtain the plastic stressrate potential %p of the J2 corner theory. In the range of near proportional loading 0 ≤ θ ≤ θ0 ,
f (θ) = 1,
(26.171)
f (θ) = 0.
(26.172)
whereas in the elastic unloading range θc ≤ θ ≤ π,
26.16. RateDependent Flow Theory
489
In the transition region θ0 ≤ θ ≤ θc , the function f (θ) decreases monotonically and smoothly from one to zero in a way which ensures convexity of the plasticrate potential,
%p (τ 2 ) − %p (τ 1 ) ≥
∂%p
∂τ 1
: (τ 2 − τ 1 ).
A simple choice of f (θ) meeting these requirements is 2 π θ − θ0 f (θ) = cos , θ0 ≤ θ ≤ θc . 2 θc − θ0
(26.173)
(26.174)
The speciﬁcation of the angles θc and θ0 in terms of the current stress measure is discussed by Christoffersen and Hutchinson (1979). The rate independence of the material response requires Dp =
∂%p
∂τ
=
∂ 2 %p
∂τ ∂τ
: τ = Mp : τ
(26.175)
to be a homogeneous function of degree one, and %p to be a homogeneous function of degree two in the stress rate τ . The function %p (τ ) is quadratic in the region of nearly proportional loading, but highly nonlinear in the transition region, because of nonlinearity associated with f (θ). The plastic rate of deformation is accordingly a linear function of τ in the region of nearly proportional loading, but a nonlinear function in the transition region.
26.16 RateDependent Flow Theory In this section we introduce a multiplicative decomposition of the total deformation gradient into elastic and plastic parts to provide an additional kinematical framework for dealing with ﬁnite elastic and plastic deformation. We introduce this in the speciﬁc context of a strain rate, and thus time dependent, J2 ﬂow theory of plasticity. We will introduce a simple description of kinetic behavior for the strain rates and for the strain hardening rates for the purpose of making the discussion explicit. We note, however, that these concepts are developed in far more detail in the chapters to follow concerned with crystalline plasticity. 26.16.1 Multiplicative Decomposition F = Fe · Fp Consider the current elastoplastically deformed conﬁguration of the material sample. Let F be the deformation gradient that maps an inﬁnitesimal material element dX from the initial to dx in the current conﬁguration, such that dx = F · dX. Introduce an intermediate conﬁguration by elastically destressing the current conﬁguration to zero stress (Fig. 26.18). Such conﬁguration differs from the initial conﬁguration by residual (plastic) deformation and from the current conﬁguration by reversible (elastic) deformation. If dxp is the material element in the intermediate conﬁguration, corresponding to dx in the current conﬁguration, then dx = Fe · dxp , where Fe represents the deformation gradient associated with the elastic loading from the intermediate to current conﬁguration. If the deformation gradient
490
26. Phenomenological Plasticity
dx
F
=
F
e
F
p
x
Fe F
p
Figure 26.18. Schematic representation of the multiplicative decomposition of deformation gradient into its elastic and plastic parts. The intermediate conﬁguration is obtained from the current conﬁguration by elastic destressing to zero stress.
X dX x
p p dx
of the plastic transformation is Fp , such that dxp = Fp · dX, the multiplicative decomposition of the total deformation gradient into its elastic and plastic parts follows as F = Fe · Fp .
(26.176)
This decomposition was introduced in the phenomenological rate independent theory of plasticity by Lee (1969). In the case when elastic destressing to zero stress is not physically achievable because of possible onset of reverse inelastic deformation before the state of zero stress is reached, the intermediate conﬁguration can be conceptually introduced by virtual destressing to zero stress, locking all inelastic structural changes that would take place during the actual destressing. The deformation gradients Fe and Fp are not uniquely deﬁned because the intermediate unstressed conﬁguration is not unique. Arbitrary local material rotations can be superposed to the intermediate conﬁguration, preserving it unstressed. In applications, however, the decomposition (26.176) can be made unique by additional speciﬁcations, dictated by the nature of the considered material model. For example, for elastically isotropic materials the elastic stress response depends only on the elastic stretch Ve and not on the rotation Re from the polar decomposition Fe = Ve · Re . Consequently, the intermediate conﬁguration can be speciﬁed uniquely by requiring that the elastic unloading takes place without rotation (Fe = Ve ). An alternative choice will be pursued below. The velocity gradient in the current conﬁguration at time t is deﬁned by L = F˙ · F−1 .
(26.177)
The superposed dot designates the material time derivative. By introducing the multiplicative decomposition of deformation gradient (26.176), the velocity gradient becomes L = F˙ e · Fe−1 + Fe · F˙ p · Fp−1 · Fe−1 . (26.178) The rate of deformation D and the spin W are, respectively, the symmetric and antisymmetric part of L,
(26.179) D = F˙ e · Fe−1 s + Fe · F˙ p · Fp−1 · Fe−1 s ,
W = F˙ e · Fe−1 a + Fe · F˙ p · Fp−1 · Fe−1 a .
(26.180)
26.17. Elastic and Plastic Contributions
491
Since Fe is speciﬁed up to an arbitrary rotation, and since the stress response of elastically isotropic materials does not depend on the rotation, we shall choose the unloading program such that e p p−1 e−1 F · F˙ · F ·F = 0. (26.181) a With this choice, the rate of deformation and the spin tensors become D = F˙ e · Fe−1 s + Fe · F˙ p · Fp−1 · Fe−1 , W = F˙ e · Fe−1 a .
(26.182) (26.183)
26.17 Elastic and Plastic Constitutive Contributions It is assumed that the material is elastically isotropic in its initial undeformed state and that plastic deformation does not affect its elastic properties. The elastic response is then given by τ = Fe ·
∂
e
(Ee ) eT ·F . ∂Ee
(26.184)
The elastic strain energy unstressed volume, e , is an isotropic function of the La eTper unit e e grangian strain E = F · F − I /2. Plastic deformation is assumed to be incompressible (det Fe = det F), so that τ = (det F)σ is the Kirchhoff stress. By differentiating (26.184), we obtain T ˆ e : F˙ e · Fe−1 . τ˙ − F˙ e · Fe−1 · τ − τ · F˙ e · Fe−1 = Λ (26.185) s ˆ e are The rectangular components of Λ e e ˆ iejkl = Fim F jn
∂2 e e Fkp Flqe . e ∂ Ee ∂ Emn pq
Equation (26.185) can be equivalently written as τ˙ − F˙ e · Fe−1 a · τ + τ · F˙ e · Fe−1 a = Λe : F˙ e · Fe−1 s .
(26.186)
(26.187)
The modiﬁed elastic moduli tensor Λe has the components ˆ iejkl + iejkl =
1 (τikδ jl + τ jkδil + τil δ jk + τ jl δik) . 2
In view of (26.183), we can rewrite (26.187) as τ = Λe : F˙ e · Fe−1 s ,
(26.188)
(26.189)
where
τ = τ˙ − W · τ + τ · W
(26.190)
is the Jaumann rate of the Kirchhoff stress with respect to total spin. By inversion, (26.189) gives the elastic rate of deformation as (26.191) De = F˙ e · Fe−1 s = Λe −1 : τ .
492
26. Phenomenological Plasticity
Physically, the strain increment De dt is a reversible part the total strain increment D dt, which is recovered upon loading–unloading cycle of the stress increment τ dt. The remaining part of the total rate of deformation, Dp = D − De ,
(26.192)
is the plastic part, which gives a residual strain increment left after the considered inﬁnitesimal cycle of stress. 26.17.1 RateDependent J 2 Flow Theory Classical J2 ﬂow theory uses the yield surface as generated earlier as a ﬂow potential. Thus the current yield criteria σ¯ = κ deﬁnes a series of yield surfaces in stress space, where κ serves the role of a scaling parameter. Here we rephrase the yield criterion of (26.6) in terms of the effective stress, σ¯ = (3/2σi j σi j )1/2 ; κ is then the uniaxial yield stress Y. J2 ﬂow theory assumes that Dp  σ . This amounts to taking ∂ σ¯ , ∂σ
(26.193)
∂ σ¯ 3 σi j , = ∂σi j 2 σ¯
(26.194)
Dp  or p
Di j  Thus, we can write
Dp = e˙¯ p
3 σ , 2 σ¯
(26.195)
where e˙¯ p is an effective plastic strain rate whose speciﬁcation requires an additional model statement. By incorporating (26.195) we can write, from (26.189), e e e e p p 3 σ ˙ τ = Λ : D = Λ : (D − D ) = Λ : D − e¯ . (26.196) 2 σ¯ For the present we use a simple power law expression of the form 1/m σ¯ ˙e¯ p = e˙ 0 , g
(26.197)
where e˙ 0 is a reference strain rate and 1/m represents a strain rate sensitivity coefﬁcient. We note that for common metals, 50 < 1/m < 200. For values of 1/m ∼ 100, or larger, the materials will display a very nearly rate independent response in the sense that σ¯ will track g, the hardness, at nearly any value of strain rate. Strain hardening is described as an evolution of the hardness function g. As an example, we adopt the model with e¯ p n , (26.198) g(e¯ p ) = σ0 1 + ey where
p e˙¯ =
2 p D : Dp 3
1/2 ,
e¯ =
t
p
0
2 p D : Dp 3
1/2 dt
(26.199)
26.18. A Rate Tangent Integration
493
are the effective plastic strain rate and effective plastic strain, respectively. The remaining parameters are the material parameters; the initial yield stress is σ0 , and n is the hardening exponent.
26.18 A Rate Tangent Integration In this section we introduce an integration method, originally proposed by Peirce et al. (1982) for phenomenological constitutive theories discussed above and by Peirce et al. (1983) for physically based theories that are discussed in the following chapters. The main concern is the estimate of the plastic strain increments over ﬁnite time steps during the integration of relations such as (26.196). Consider, for example, the expression for the plastic part of the rate of deformation in the phenomenological J2 ﬂow theory, viz., ˙¯ e, Dp = e( ¯ βi )p,
(26.200)
where p is the direction of viscoplastic straining, and the effective plastic strain, e, ¯ is deﬁned as t p D : Dp 1/2 dt. (26.201) e¯ = p:p 0 A set of scalar variables βi deﬁne the “strength of the material.” Of course, the effective plastic strain rate depends on the effective stress, σ¯ , as well. For the J2 ﬂow theory, we have p=
3 τ , 2 τ¯
(26.202)
where τ = τ −
1 3 (τ : I)I, τ¯ 2 = τ : τ . 3 2
(26.203)
The total rate of deformation is consequently
˙¯ e, D = D∗ + Dp = Λe −1 : τ + e( ¯ βi )p,
(26.204)
which can be inverted to give
τ = Λe : D − e˙¯ P,
(26.205)
P = Λe : p.
(26.206)
where
As a model evolutionary law for the βi , we assume β˙i = Ai : Dp + Bi : τ .
(26.207)
The Ai and Bi can, in general, depend on the current values of τ , e, ¯ and the βi . The ˙¯ over a small, but ﬁnite time increment t. To that objective is to estimate an effective et goal, we write for an increment in e, ¯ over the time step t, e¯ = t [(1 − θ)e˙¯ t + θ e˙¯ t+t ] .
(26.208)
494
26. Phenomenological Plasticity
We then expand e˙¯ t+t in a Taylor series about the time t to obtain ∂ e˙¯ ∂ e˙¯ ˙e¯ t+t ≈ e˙¯ t + ˙e¯ t t + β˙i,t t. ∂ e¯ ∂βi i The use of (26.207) in (26.209) gives # " ∂ e˙¯ ∂ e˙¯ p 2 e˙¯ + e¯ ≈ t e˙¯ t + θ(t) (Ai : D + Bi : τ ) . ∂ e¯ ∂βi i
(26.209)
(26.210)
Upon the substitution of (26.200) and (26.205) into (26.210), we obtain e¯ ≈ t e˙¯ t + (θ t) " # ∂ e˙¯ ∂ e˙¯ ∂ e˙¯ e e¯ + × Bi : Λ : Dt + (Ai : p − Bi : P)e¯ . ∂ e¯ ∂βi ∂βi i i When this relation is solved for e, ¯ and then divided by t, there follows e˙¯ =
e¯˙ t 1 ξ + Q : D, ¯ 1+ξ H 1+ξ
(26.211)
where Q= H¯ = −
∂ e˙¯ Bi : Λe , ∂β i i
∂ e˙¯ ∂ e˙¯ − (Ai : p − Bi : P), ∂ e¯ ∂βi i
(26.212)
¯ ξ = (θ t) H. For the J2 ﬂow theory itself, take as a speciﬁc model for evolution, ˙¯ e, e˙¯ = e( ¯ σ¯ ),
(26.213)
and note that
σ˙¯ = p : τ .
(26.214)
∂ σ˙¯ P. ∂ σ¯
(26.215)
Then, Q= It follows that H¯ = −
∂ e˙¯ ∂ e˙¯ + (p : Λe : p), ∂ e¯ ∂ σ¯
(26.216)
and Λtan = Λe −
ξ 1 PP. 1+ξ h
(26.217)
Here, −1 ∂ e˙¯ H¯ ∂ e˙¯ =− + p : Λe : p, h= ˙¯ e¯ ∂ e/∂ ∂ e¯ ∂ σ¯
(26.218)
26.19. Plastic Void Growth
495
with
ξ = θ t
∂ e˙¯ ∂ σ¯
h.
(26.219)
We note that Λtan is symmetric, and the constitutive relation takes the ﬁnal form
τ = Λtan : D −
e¯˙ P. 1+ξ
(26.220)
26.19 Plastic Void Growth As an illustration of the application of some of the derived equations in this chapter, we present in this section an analysis of plastic void growth under triaxial tension. More involved studies of plastic void growth under different states of stress, and based on the more involved material models, can be found in Rice and Tracey (1969), Needleman (1972), Budiansky, Hutchinson, and Slutsky (1982), Huang, Hutchinson, and Tvergaard (1991), Needleman, Tvergaard, and Hutchinson (1992), and others. Consider a spherical void of initial radius R0 in an isotropic inﬁnite medium under remote triaxial tension σ . The stress state at an arbitrary point consists of the radial stress σrr and the hoop stress σθ θ = σφφ . Because of spherical symmetry, the stress components depend only on the radial distance r and not on the spherical angles θ and φ. In the absence of body forces the equilibrium equation is 2 dσrr − (σθ θ − σrr ) = 0 . (26.221) dr r If the material response is within the inﬁnitesimal elastic range, the compatibility equation is d (σrr + 2σθ θ ) = 0 , (26.222) dr which implies that the spherical component of stress tensor is uniform throughout the medium, and thus equal to σ , i.e., σrr + 2σθ θ = 3σ . Combining (26.221) and (26.223) it follows that R03 1 R03 σrr = σ 1 − 3 , σθ θ = σ 1 + . r 2 r3 The corresponding radial displacement is R03 1 σ (1 − 2ν)r + (1 + ν) 2 , u= E 2 r
(26.223)
(26.224)
(26.225)
where E is Young’s modulus and ν is Poisson’s ratio of the material. According to either von Mises or Tresca yield criterion, the plastic deformation commences when σθ θ − σrr = Y .
(26.226)
The initial yield stress of the material in uniaxial tension is denoted by Y. Thus, the threshold value of applied stress σ for the onset of plastic deformation at the surface of the void
496
26. Phenomenological Plasticity
plastic
Figure 26.19. The elasticplastic interface around the spherical void of initial radius R0 . The radius of the expanded void is R. The initial and current radii of material elements within the plastic zone are r0 and r . Since deformation is inﬁnitesimal beyond the elasticplastic interface, its deformed and undeformed radii are nearly equal to each other (ρ ≈ ρ0 ).
r0 R0
elastic
r
R
ρ≈ρ0
(r = R0 ) is σ y = 2Y/3. With further increase of stress beyond this value, the plastic zone expands outward and at an arbitrary instant of deformation the elasticplastic boundary has reached the radius ρ (Fig. 26.19). The corresponding radius of the expanded void is R. A material element within the current plastic zone, which was initially at the radius r0 , is currently at the radius r . We assume that ρ is sufﬁciently large, so that large strains take place in the vicinity of the void, whereas inﬁnitesimal strains characterize the elastic zone beyond the radius ρ. This means that ρ ≈ ρ0 and similarly for any radius beyond the elasticplastic boundary. The deformation gradient tensor associated with the spherical expansion of the void, expressed in spherical coordinates, is ⎤ ⎡ dr 0 0⎥ ⎢ ⎥ ⎢ dr0 ⎥ ⎢ r ⎥ ⎢ . (26.227) F=⎢ 0 0⎥ ⎥ ⎢ r 0 ⎥ ⎢ ⎣ r ⎦ 0 0 r0 The corresponding volume change of an inﬁnitesimal material element is 2 dV r dr = det F = . dV0 r0 dr0
(26.228)
If plastic deformation is assumed to be isochoric, the volume change is entirely due to elastic deformation, and 1 − 2ν dV − dV0 = (σrr + 2σθ θ ) . dV E Combining (26.228) and (26.229), there follows r 2 dr 1 − 2ν 0 0 =1− (σrr + 2σθ θ ) . r dr E
(26.229)
(26.230)
Incorporating the equilibrium equation (26.221), rewritten as σrr + 2σθ θ =
1 d 3 r σrr , r 2 dr
(26.231)
26.19. Plastic Void Growth
497
equation (26.230) becomes r02 dr0 = r 2 dr −
1 − 2ν 3 d r σrr . E
Upon integration, using the boundary condition σrr (R) = 0, we obtain 3 R3 − R03 r − r03 E . σrr = − 3(1 − 2ν) r3 r3
(26.232)
(26.233)
This expression holds everywhere in the medium, regardless of the constitutive description in the plastic zone r ≤ ρ. On the other hand, in the elastic zone r ≥ ρ, we have σrr = σ −
2 ρ3 Y , 3 r3
σθ θ = σ +
1 ρ3 Y , 3 r3
(26.234)
which ensures that σθ θ (ρ) − σrr (ρ) = Y, and σrr + 2σθ θ = 3σ everywhere in the elastic region. Thus, σrr (ρ) = σ − 2Y/3, and from (26.233) we obtain 3 R3 − R03 ρ − ρ03 E 2 . (26.235) σ = Y+ − 3 3(1 − 2ν) ρ3 ρ3 Since the strain is elastic and inﬁnitesimal at the elasticplastic interface, there is an approximation ρ 3 − ρ03 1+ν 3(1 − 2ν) σ+ Y, ≈ 3eθ θ (ρ) = ρ3 E E
(26.236)
and the substitution into (26.235) gives R3 = R03 + 3(1 − ν)
Y 3 ρ . E
(26.237)
At the advanced stages of plastic deformation, when R becomes much greater than R0 , the above result implies that the ratio ρ/R approaches a constant value 1/3 E ρ = . (26.238) R 3(1 − ν)Y Equations (26.237) and (26.238) hold for any type of hardening in the plastic zone, but the analysis cannot be pursued further without using the constitutive description of plastic deformation. For an elastoplastic material with a general nonlinear hardening the relationship between the applied stress σ and the size of the plastic zone ρ can be determined only numerically. The closed form solutions are attainable for two particular material models: an elastic ideally plastic material, and an incompressible elastic linearly hardening material. 26.19.1 Ideally Plastic Material In the case of a nonhardening material, we have σθ θ − σrr = Y throughout the plastic zone, and from the equilibrium equation the stress state in the plastic zone (r ≤ ρ) is r2 r2 (26.239) σrr = Y ln 2 , σθ θ = Y 1 + ln 2 . R R
498
26. Phenomenological Plasticity
Since the stress ﬁeld in the surrounding elastic region (r ≥ ρ) is speciﬁed by (26.234), the continuity condition for the radial stress component at the elasticplastic interface gives σ 2 ρ 1 − σ = Y 1 + 3 ln , ρ = R exp . (26.240) 3 R 2Y 3 The substitution of (26.240) into (26.237) furnishes an expression for the current radius of the void in terms of the applied stress −1/3 Y 3σ −1 . R = R0 1 − 3(1 − ν) exp E 2Y At this stress level, the plastic zone has spread to σ 1 exp − 2Y 3 ρ = R0 " #1/3 . 3σ Y −1 1 − 3(1 − ν) exp E 2Y
(26.241)
(26.242)
The inverted form, giving σ in terms of ρ, is 3 ! R0 2Y Y σ = 1 − ln 3 + 3(1 − ν) . 3 ρ E The limiting stress value, obtained as R or ρ increases indeﬁnitely, is ! 2Y Y 1 − ln 3(1 − ν) . σcr = 3 E
(26.243)
(26.244)
The unlimited void growth under this level of stress is referred to as an unstable cavitation. This stress level is also the critical (bifurcation) stress at which a nonhomogeneous deformation bifurcates from the homogeneous by the sudden void formation.
26.19.2 Incompressible Linearly Hardening Material If the material is both elastically and plastically incompressible, we have det F = 1 in (26.228), and r 3 − r03 = R3 − R03 = ρ 3 − ρ03 =
3Y 3 ρ . 2E
(26.245)
The deformation gradient tensor is in this case ⎡
r02
0
⎢ r2 ⎢ ⎢ r F=⎢ ⎢0 r ⎢ 0 ⎣ 0 0
⎤ 0⎥ ⎥ ⎥ 0⎥ ⎥. ⎥ r ⎦ r0
(26.246)
26.19. Plastic Void Growth
499
By using the multiplicative decomposition of the deformation gradient into its elastic and plastic parts, we can write ⎤ ⎡ 2 ⎤ ⎡ 2 r0 rp ⎢ 2 0 0⎥ ⎢ 2 0 0⎥ ⎥ ⎢ rp ⎥ ⎢r ⎥ ⎢ ⎥ ⎢ r ⎢ ⎥ ⎥ ⎢ r p 0 ⎥·⎢ 0 (26.247) F = Fe · Fp = ⎢ 0 ⎥. 0 ⎥ ⎢ ⎥ ⎢ rp r0 ⎥ ⎢ ⎥ ⎢ r ⎦ ⎣ ⎣ rp ⎦ 0 0 0 0 rp r0 The logarithmic strain
⎡
⎤
r
0 0 ⎥ ⎢ −2 ln ⎢ ⎥ r0 ⎢ ⎥ r ⎢ ⎥ E=⎢ ⎥ 0 ln 0 ⎢ ⎥ r0 ⎢ ⎥ ⎣ r ⎦ 0 0 ln r0
(26.248)
can be additively decomposed into its elastic and plastic parts (E = Ee + Ep ) as ⎤ ⎡ ⎤ ⎡ r rp 0 0 ⎥ ⎢ −2 ln 0 0 ⎥ ⎢ −2 ln r p ⎥ ⎢ ⎥ ⎢ r0 ⎢ ⎥ ⎥ ⎢ r rp ⎥ ⎢ ⎥ ⎢ + . (26.249) E=⎢ ⎢ ⎥ 0 ln 0 0 ln 0 ⎥ ⎢ ⎥ ⎥ ⎢ r r0 p ⎥ ⎢ ⎥ ⎢ ⎣ rp ⎦ r ⎦ ⎣ 0 0 ln 0 0 ln r0 rp For the proportional loading, the generalized plastic strain is 1/2 rp 2 p p p ¯ E = E :E = 2 ln . 3 r0
(26.250)
If the material is linearly hardening with respect to this strain measure, the equivalent yield stress at an arbitrary stage of deformation can be expressed as rp r r = Y + 2k ln − ln σθ θ − σrr = Y + 2k ln , (26.251) r0 r0 rp where k is the hardening modulus. By using Hooke’s law for the elastic component of strain, 3 1 e (26.252) E = σ − (tr σ) I , 2E 3 we obtain ln
r 1 (σθ θ − σrr ) . = rp 2E
(26.253)
The substitution of (26.253) into (26.251) yields σθ θ − σrr = Yˆ + 2kˆ ln
r , r0
(26.254)
500
26. Phenomenological Plasticity
with the abbreviations Yˆ =
Y , 1 + k/E
kˆ =
k . 1 + k/E
(26.255)
The distinction between the barred and nonbarred quantities is important for strong hardening rates and high values of the ratio k/E. Physically, the stress Yˆ and the hardening modulus kˆ appear in the relationship between the uniaxial stress and the total strain ˆ (σ = Yˆ + kE), whereas Y and k appear in the relationship between uniaxial stress and plastic strain (σ = Y + kEp ). When (26.254) is introduced into (26.221), the integration gives r 4kˆ r r 3 dr ˆ , (26.256) ln 3 σrr = 2Y ln + R 3 R r0 r or, in view of (26.245),
" n 3 n # ∞ R − R03 R3 − R03 4kˆ 1 r σrr = 2Yˆ ln + . − R 9 n=1 n2 R3 r3
(26.257)
Evaluating at r = ρ, and equating the result with σrr (ρ) = σ − 2Y/3, following from (26.234), provides an expression for the applied stress σ in terms of the plastic zone radius ρ. This is " n # ∞ R3 − R03 ρ 4kˆ 1 3Y n 2 ˆ − . (26.258) σ = Y + 2Y ln + 3 R 9 n=1 n2 R3 2E The radius R of the expanded void is given in terms of ρ by (26.245). If the plastic zone surrounding the void has spread to a large radius ρ, we have R3 >> R03 , and by neglecting higher than linear terms in 3Y/2E, we obtain 2Y/3 2E π 2 k 1 + ln + . (26.259) σcr = 1 + k/E 3Y 9 Y This is the critical stress for cavitation instability in an incompressible elastic linearly hardening material. If the ratio k/E φ 0 , plasticity spreads outward and at an arbitrary stage of deformation before reaching r = b the elasticplastic interface is at r = c. Assuming linear hardening, p
σr θ = σr0θ + 2her θ , where plastic part of the shear strain is p
er θ = er θ − Thus,
1 1 r dϕ σr θ = − σr θ . 2µ 2 dr 2µ
dϕ h 1+ . σr θ = σr0θ + hr µ dr
Recalling that σr θ = C1 /r 2 , we obtain a differential equation h C1 1 dϕ = 1+ − σr0θ , h dr µ r3 r whose solution, satisfying ϕ(a) = 0, is C1 h r a2 h ϕ(r ) = 2 1 + 1 − 2 − σr0θ ln , 2a µ r a
a ≤ r ≤ c.
On the other hand, in the elastic region we have ϕ(r ) = −
C1 1 + C2 , 2µ r 2
c ≤ r ≤ b.
Imposing the boundary condition at r = b and the continuity condition at the elasticplastic interface r = c, ϕ(b) = φ ,
ϕ(c − 0) = ϕ(c + 0) ,
it readily follows that C1 = 2a 2
c hφ + σr0θ ln a , a2 h a2 1− 2 + 1− 2 c µ b
a2 h hC2 = 1 − 2 + c µ
c C1 − σr θ ln . 2 2a a
The relationship between the angle φ and the radius of the elasticplastic interface r = c can be obtained from the condition σr θ (c) =
C1 = σr0θ . c2
This gives h 2h c2 c φ = 2 − 1 − 2 ln + 0 a a µ σr θ
c2 c2 − 2 2 a b
.
796
Problems 26.4–26.5
Plasticity spreads throughout the cylinder (c = b) when φ = φ ∗ , where 2 b 2h ∗ h b φ = 1 + − 1 − 2 ln . µ a2 a σr0θ At this instant 2 2h b r h b2 − 2 ln , ϕ(r ) = 1 + − µ a2 r2 a σr0θ
a ≤ r ≤ b.
The corresponding shear stress is σr θ = σr0θ
b2 , r2
a ≤ r ≤ b.
Problem 26.5. Solve the previous problem by using the rigidplastic J2 ﬂow theory of
plasticity with a linear hardening. Solution: The deformation mapping in cylindrical coordinates is
r = R, θ = ) + ϕ(r, t) , z = Z. The coordinates in the undefomed conﬁguration are (R, ), Z) and in the deformed conﬁguration (r, θ, z); t is a monotonically increasing time like parameter, e.g., the prescribed outer angle of rotation φ during a continuous loading. The corresponding velocity ﬁeld is vr = r˙ = 0 ,
vθ = r θ˙ = r
∂ϕ , ∂t
vz = z˙ = 0 ,
with the components of the rate of deformation tensor Drr = Dθ θ = Dzz = 0 ,
Dr θ =
1 ∂ 2ϕ r , 2 ∂r ∂t
Dr z = Dθ z = 0 .
The constitutive equation of the rigidplastic J2 ﬂow theory is 1 J˙2 σ , 4h J2
D=
J2 =
1 σ : σ . 2
Assuming that the stress tensor is ⎡
σrr σ = ⎣σθr 0
σr θ σθ θ 0
⎤ 0 0 ⎦, σzz
Problem 26.5
797
the deviatoric stress components are σrr =
1 (2σrr − σθ θ − σzz) , 3
σθ θ =
1 (2σθ θ − σzz − σrr ) , 3
σzz =
1 (2σzz − σrr − σθ θ ) , 3 σr θ = σr θ .
Thus, Drr =
1 J˙2 1 (2σrr − σθ θ − σzz) = 0 , 4h J2 3
Dθ θ =
1 J˙2 1 (2σθ θ − σzz − σrr ) = 0 , 4h J2 3
Dzz =
1 J˙2 1 (2σzz − σrr − σθ θ ) = 0 . 4h J2 3
These are satisﬁed if σrr = σθ θ = σzz = − p , where p is an arbitrary pressure. In view of one of the equilibrium equations, i.e., σrr − σθ θ ∂σrr + = 0, ∂r r there follows ∂ p/∂r = 0, so that p = p(t) only. The deviatoric normal stresses are zero, σrr = σθ θ = σzz = 0,
and J2 =
1 σ : σ = σr2θ , 2
J˙2 = 2σr θ
∂σr θ . ∂t
Since Dr θ =
1 J˙2 1 ∂ 2ϕ , σr θ = r 4h J2 2 ∂r ∂t
there follows ∂σr θ ∂ 2ϕ = hr . ∂t ∂r ∂t The integration gives σr θ = h r
∂ϕ + f (r ) . ∂r
798
Problem 26.5
On the other hand, using the assumption of linear hardening, we can write 1/2
J2 where
ϑ=
= k = σr0θ + hϑ ,
t 1/2
(2 D : D)
dt =
0
t
2Dr θ dt = r
0
∂ϕ . ∂r
This gives σr θ = σr0θ + h r
∂ϕ . ∂r
The comparison with the earlier expression reveals that f (r ) = σr0θ . Note also that at the interface r = c between plastic and rigid regions, ∂ϕ/∂r = 0, so that σr θ (c, t) = σr0θ . But, from the remaining equilibrium equation 2 dσr θ + σr θ = 0 , dr r we obtain σr θ =
C(t) . r2
Combining this expression with the previous expression gives C(t) ∂ϕ + σr0θ , = hr 2 r ∂r or, upon integration using the boundary condition ϕ(a, t) = 0, r C(t) a2 1 − − σr0θ ln . h ϕ(r, t) = 2a 2 r2 a Since at r = c ≤ b, we have ϕ(c, t) = φ(t) , it readily follows that C(t) 1 c 0 . h φ(t) + σ = ln r θ 2a 2 1 − a 2 /c2 a Consequently,
c 1 − a 2 /r 2 r σr0θ σ0 ln . − ϕ(r, t) = φ(t) + r θ ln 2 2 h a 1 − a /c h a
The angle φ ∗ at which plasticity ﬁrst reaches the radius r = b is obtained from the condition σr θ (b) = σr0θ , i.e., 2a 2 b ∗ 0 h φ + σr θ ln = σr0θ . b2 − a 2 a This gives ∗
φ =
b2 − a 2 b − ln 2a 2 a
σr0θ . h
Problem 26.6
799
x2
1
Figure 263. Simple shear of a rectangular block.
x1 0
1
kt
Problem 26.6. Consider a simple shear deformation of of rectangular block (see Fig. 263), for which the velocity ﬁeld is
v1 = kx2 ,
v2 = v3 = 0
(k = const.).
Assuming the rigidplastic material, which hardens in a kinematic hardening mode with the von Mises type yield condition, 2 2 σ , 3 0
(σi j − αi j )(σi j − αi j ) =
α i j = cDi j ,
(σ0 = const.),
(c = const.),
determine the stress components at an arbitrary stage of deformation. Solution: The only nonvanishing component of the velocity gradient is L12 = k, with the
corresponding nonvanishing components of the rate of deformation and spin tensors D12 = D21 =
k , 2
W12 = −W21 =
k . 2
Thus, since
α i j = α˙ i j − Wikαkj + αik Wkj = cDi j , we obtain α˙ 11 = −α˙ 22 = kα12 , α˙ 12 = α˙ 21 = k
c 2
− α11 .
Consequently, by combining these two equations, α¨ 12 + k2 α12 = 0 , which has the general solution α˙ 12 = a1 cos kt + a2 sin kt . Since the components of the back stress are initially (t = 0) equal to zero, we have α12 (0) = 0 and α˙ 12 (0) = kc/2, which speciﬁes the integration constants a1 = 0 and a2 = c/2. Thus, α12 =
c sin kt . 2
800
Problems 26.6–26.7
From the differential equation for α11 it then readily follows that α11 =
c (1 − cos kt) , 2
α22 = −α11 .
Now, from the normality rule for the rigidplastic material giving Di j ∼ (σi j − αi j ), we have D22 D12 D11 = = . σ11 − α11 σ22 − α22 σ12 − α12 Since D11 = D22 = 0, we conclude that σ11 = α11 and σ22 = α22 = −α11 . Thus, from the yield condition − α11 )2 + (σ22 − α22 )2 + 2(σ12 − α12 )2 = (σ11
2 2 σ , 3 0
√ we obtain σ12 − α12 = σ0 / 3. The nonvanishing stress components at an arbitrary stage of deformation are therefore c σ0 c = −σ22 = (1 − cos kt) , σ12 = √ + sin kt . σ11 2 2 3 An arbitrary hydrostatic pressure can be superposed to this without affecting the considered simple shear deformation. The obtained spurious oscillation of the stress response corresponding to monotonically increasing shear deformation (γ = kt) is an indication of the limitation of the utilized simple evolution equation for the back stress. More involved representation of this evolution is required to eliminate such oscillations. Problem 26.7. Determine the critical stress for a cylindrical cavitation instability in an
incompressible elasticplastic linearly hardening material. Solution: Consider a cylindrical void of initial radius R0 in an isotropic inﬁnite medium
under remote biaxial tension σ . Assume the plane strain conditions. The stress state at an arbitrary point consists of the radial stress σrr , the hoop stress σθ θ , and the longitudinal stress σzz. Because of cylindrical symmetry, the stress components depend only on the radial distance r . In the absence of body forces the equilibrium equation is 1 dσrr − (σθ θ − σrr ) = 0 . dr r If the material response is within the inﬁnitesimal elastic range, the compatibility equation reduces to d (σrr + σθ θ ) = 0 , dr Combining above equations, it follows that R02 σrr = σ 1 − 2 , r
i.e.,
σθ θ
σrr + σθ θ = 2σ . R02 =σ 1+ 2 . r
The longitudinal stress is σzz = 2νσ , and the radial displacement is R02 σ u= (1 − 2ν)r + . 2G r
Problem 26.7
801
According to the von Mises yield criterion, the plastic deformation commences when σrr + σθ θ 2 3 (σθ θ − σrr )2 + σzz − = Y2 . 4 2 Thus, the threshold value of applied stress σ for the onset of plastic deformation at the surface of the void is σ yy =
Y [3 + (1 − 2ν)2 ]
1/2
.
With an increase of stress beyond this value, the plastic zone expands outward and at an arbitrary instant of deformation the elasticplastic boundary has reached the radius ρ. The deformation gradient tensor, associated with a cylindrical expansion of the void and expressed in cylindrical coordinates, becomes ⎤ ⎡ dr 0 0⎥ ⎢ dr ⎥ ⎢ 0 ⎥. F=⎢ r ⎢ 0 0⎥ ⎣ ⎦ r0 0 0 1 The corresponding volume change of an inﬁnitesimal material element is dV r dr = det F = . dV0 r0 dr0 If plastic deformation is assumed to be isochoric, the volume change is entirely due to elastic deformation, so that 1 dV − dV0 = [(1 − ν)(σrr + σθ θ ) − 2νσzz] . dV E The closed form analysis can be pursued further for an elastically incompressible material (ν = 1/2). The longitudinal stress σzz is then an arithmetic mean of the other two stress components throughout the medium, and r 2 − r02 = R2 − R02 = ρ 2 − ρ02 . In the elastic zone r ≥ ρ, the stress components are Y ρ2 σrr = σ − √ 2 , 3 r
Y ρ2 σθ θ = σ + √ 2 , 3 r
σzz = σ .
They satisfy the yield condition at the elasticplastic interface r = ρ, and the condition σrr + σθ θ = 2σ everywhere in the elastic region. Because the strain is elastic and inﬁnitesimal at the elasticplastic interface, we can write √ ρ 2 − ρ02 3Y , ≈ 2eθ θ (ρ) = ρ2 E and
√ R = 2
R02
+
3Y 2 ρ . E
802
Problem 26.7
At the advanced stages of plastic deformation, when R becomes much greater than R0 , the ratio ρ/R approaches a constant value E 1/2 ρ = √ . R 3Y The last two equations hold regardless of the type of material hardening in the plastic zone. The deformation gradient tensor for the void expansion in an incompressible material is ⎤ ⎡ r0 ⎢ r 0 0⎥ ⎥ ⎢ ⎥ F=⎢ ⎢ 0 r 0⎥ . ⎦ ⎣ r0 0 0 1 By using the multiplicative decomposition of the deformation gradient into its elastic and plastic parts (F = Fe · Fp ), we have ⎤ ⎤ ⎡ ⎡ r0 rp 0 0⎥ 0 0⎥ ⎢ ⎢r ⎥ rp ⎥ ⎢ ⎢ ⎥ ⎢ ⎥·⎢ r F=⎢ ⎥. r p ⎥ ⎢ ⎢0 0 0⎥ ⎦ ⎣0 ⎣ ⎦ rp r0 0 0 1 0 0 1 The corresponding logarithmic strain ⎡
⎤
r
⎢− ln r 0 ⎢ E=⎢ ⎢ 0 ⎣ 0
0 ln
r
r0 0
0⎥ ⎥ ⎥ 0⎥ ⎦ 0
can then be additively decomposed as E = E + E , i.e., ⎤ ⎡ ⎡ r r 0 0⎥ ⎢− ln p ⎢− ln rp ⎥ ⎢ ⎢ r0 ⎢ ⎥ ⎢ E=⎢ r ⎥+⎢ ⎢ 0 ln 0⎥ ⎣ ⎦ ⎣ 0 rp 0 0 0 0 e
p
0 ln
rp
r0 0
⎤ 0⎥ ⎥ ⎥. 0⎥ ⎦ 0
If the material is linearly hardening with respect to the generalized plastic strain 1/2 rp 2 p 2 p p ¯ E = E :E = √ ln , 3 r0 3 √ the equivalent yield stress 3(σθ θ − σrr )/2 at an arbitrary stage of deformation is √ rp 3 2k 2k r r (σθ θ − σrr ) = Y + √ ln = Y + √ ln − ln . 2 r0 r0 rp 3 3 By using Hooke’s type law for the elastic component of strain, ln
3 r (σθ θ − σrr ) , = rp 4E
Problems 26.7–26.8
p
803
Figure 264. A thin circular disk under internal pressure p. The current midradius of the ring is R and its thickness t.
the substitution in the previous equation yields σθ θ − σrr = Yˆ + kˆ ln The abbreviations are here used Yˆ =
√ 2Y/ 3 , 1 + k/E
kˆ =
r . r0
4k/3 . 1 + k/E
When this is introduced into the equilibrium equation, the integration gives " n 2 n # ∞ R − R02 R2 − R02 kˆ 1 r ˆ σrr = Y ln + . − R 4 n=1 n2 R2 r2
√ Evaluating this at r = ρ, and equating the result with σrr (ρ) = σ − Y/ 3, provides an expression for the applied stress σ in terms of the plastic zone radius ρ. This is " n √ n # ∞ R2 − R02 kˆ 1 3Y Y ρ σ = √ + Yˆ ln + − . 2 2 R 4 n=1 n R E 3 If the plastic zone around the void has spread to a large extent, we have √ √ E π 2 3k Y/ 3 σcr = 1 + ln √ + . 1 + k/E 3Y 18 Y This is the critical stress for a cylindrical cavitation instability in an incompressible elastic linearly hardening material. If k E, the result reduces to that for a pressurized cylindrical void in an inﬁnitely extended material (Hill, 1950). Problem 26.8. Determine the pressure at the onset of necking of a thin circular ring
assuming a rigidplastic J2 ﬂow theory. The initial midradius of the ring is R0 and its square cross section has initial size t0 . Solution: The hoop stress in the ring at an arbitrary stage of deformation before necking is σ = pR/t, where Rand t are the current dimensions of the ring (Fig. 264). Thus, p = σ t/R. At the onset of necking, p reaches its maximum, so that
dp = 0
⇒
dt dR dσ + − = 0. σ t R
Since the deviatoric stress components are σθ θ =
2 σ 3
1 =− σ σrr = σzz 3
804
Problem 26.8
we have 1 J˙2 t˙ Drr = Dzz = = t 4h J2 R˙ 1 J˙2 Dθ θ = = R 4h J2
1 − σ , 3
2 σ , 3
where J2 =
J˙2 2σ˙ . = J2 σ
1 2 σ , 3
Evidently, dt 1 dR =− , t 2 R which is a consequence of plastic incompressibility (Rt 2 = R0 t02 ). Thus, at the onset of necking 3 dR dσ = . σ 2 R Since from the ﬂow rule dR 1 dJ2 = R 4h J2
2 σ 3
=
dσ , 3h
we obtain that the hoop stress at the necking is σ = 2h . For the linearly hardening material 1/2
J2
= k = k0 + hϑ
⇒
σ = σ0 +
√
3hϑ ,
where σ0 is the hoop stress at the beginning of plastic deformation, and t √ R ϑ= (2 D : D)1/2 dt = 3 ln . R0 0 Thus, the necking condition becomes σ = σ0 + 3h ln
R = 2h , R0
which gives the radius of the ring at the onset of necking 2 σ0 R = R0 exp − . 3 3h The corresponding pressure is pmax
σ0 2ht0 −1 . = exp R0 2h
An alternative derivation proceeds by writing the function p = p(R) directly from p = σ t/R, and σ = σ0 + 3h ln
R , R0
Rt 2 = R0 t02 .
Problems 26.8–26.9
805
This gives p(R) =
R R−3/2 . R0 t0 σ0 + 3h ln R0
The necking condition is simply d p/dR = 0, i.e., R 2h − σ0 + 3h ln = 0, R0 in accord with the previously derived result. Problem 26.9. Consider a thin cylindrical shell under internal pressure p and axial force
N, such that σθ θ =
Rp , t
σzz =
N Rp + , 2t 2Rπ t
σrr ≈ 0 ,
where R is the current radius of the shell, and t is its thickness. Suppose that N = cpR2 π, where c =const. Assuming a rigidplastic J2 material model and isotropic hardening with constant hardening rate h, determine c such that R = R0 =const. throughout the loading process. Determine in that case the relationship between the pressure p and the thickness t of the deformed shell, and discuss the onset of instability. Solution: For the considered rigidplastic material model, the components of the rate of deformation tensor are
Di j =
1 σkl σ˙ kl σi j . σ 2h σmn mn
The stress components are σθ θ = 2σ ,
σzz = (1 + c)σ ,
σrr ≈ 0 ,
where σ = Rp/2t. The corresponding deviatoric components c 2c c σ , σr = − 1 + σ , σz = σ. σθ = 1 − 3 3 3 It readily follows that c2 c2 σmn σmn =2 1+ σ 2 , σkl σ˙ kl = 2 1 + σ σ˙ , 3 3 so that Di j =
1 σ˙ σ . 2h σ i j
Thus, Dr =
1 σ˙ c t˙ 1 = σr = − 1+ σ˙ , t 2h σ 2h 3
Dθ =
R˙ 1 σ˙ c 1 = σθ = 1− σ˙ , R 2h σ 2h 3
Dz =
l˙ c 1 σ˙ = σz = σ˙ . l 2h σ 3h
806
Problems 26.9–26.10
Clearly, there is no change in radius of the shell ( R˙ = 0) if c = 3. In this case, then, t˙ 1 t0 1 pR0 p0 R0 . = − σ˙ ⇒ ln = − t h t h 2t 2t0 The plastic yielding begins when 0 σ yy 1 1/2 =√ σmn σmn 2 3
⇒
0 σ yy t0 , p0 = √ 3 R0
0 where σ yy is the initial yield stress in simple tension. Consequently, the pressurethickness relationship is 0 σ yy t t0 . p= √ + 2h ln R0 t 3
This is a monotonically increasing function of the ratio t0 /t up to the instability condition 0 σ yy t0 dp =0 ⇒ = exp 1 − √ . d(t0 /t) t 2 3h The corresponding (maximum) pressure is pmax
0 σ yy t0 = 2h exp √ − 1 . R0 2 3h
The hardening rate has to be such that pmax > p0 , which is satisﬁed for any h > 0. For h = 0 (ideal plasticity), we must require σ˙ = 0, which gives p = p0 t/t0 . This implies instability from the onset of deformation (t < t0 ⇒ p < p0 ). Problem 26.10. Consider an elastoplastic deformation process which is characterized by elastic isotropy and plastic incompressibility. Let the elastic strain energy per unit initial volume be 1 eT e F ·F −I , = (Ee ) , Ee = 2
where Fe is the elastic part of the elastoplastic deformation gradient from the multiplicative decomposition F = Fe · Fp . The corresponding symmetric Piola–Kirchhoff stress tensor, corresponding to elastic deformation Fe , is Se = (det Fe ) Fe−1 · σ · Fe−T =
∂ , ∂Ee
where σ is the Cauchy stress. Prove that the symmetric Piola–Kirchhoff stress tensor, corresponding to elastoplastic deformation F, is S=
∂ . ∂E
Solution: The elastoplastic Lagrangian strain is
E=
1 T F · F − I = FpT · Ee · Fp + Ep , 2
Problems 26.10–26.11
807
where the Lagrangian strain corresponding to plastic deformation gradient Fp is deﬁned by Ep =
1 pT p F ·F −I . 2
Thus, Ee = Fp−T · (E − Ep ) · Fp−1 . The elastic strain energy per unit unstressed volume can now be expressed as
p−T · (E − Ep ) · Fp−1 . = (Ee ) = F Thus, by partial differentiation ∂ Ekle ∂ ∂ = . e ∂ Ei j ∂ Ekl ∂ Ei j Since ∂ Ekle p−1 = F p−T ki F jl , ∂ Ei j we obtain ∂ ∂ = Fp−1 · · Fp−T . ∂E ∂Ee By substituting into this the expression ∂ = (det Fe ) Fe−1 · σ · Fe−T , ∂Ee and by using Fp−1 · Fe−1 = F−1 and the plastic incompressibility constraint giving det Fe = det F, we ﬁnally obtain ∂ = (det F)F−1 · σ · F−T = S . ∂E Note also that Se = Fp · S · FpT . Problem 26.11. Prove equation (26.189), i.e., when the current state is taken as the refer
ence state, show that the Jaumann rate of the Kirchhoff stress is
τ = σ + σ trD . Solution: Apply the Jaumann rate to τ = (det F)σ to obtain
τ =
d (det F) + (det F) σ . dt
Since d (det F) = (det F) trD , dt
808
Problems 26.11–26.13
we have
τ = (det F)(σ + σ trD) . When the current state is taken to be the reference state, we have F = I and det F = 1, so that
τ = σ + σ trD = σ˙ + σ trD − W · σ + σ · W . Problem 26.12. The elastoplastic partitions of the rate of deformation tensor and the
Jaumann rate of the Kirchhoff stress are deﬁned such that D = De + Dp ,
De = Λe −1 : τ ,
and
τ =τ e+τ p,
τ e = Λe : D ,
where Λe is the instantaneous elastic moduli tensor. Derive the relationship between the plastic parts τ p and Dp . Solution: By applying a trace product with Λe to
D = Λe −1 : τ + Dp , we obtain
τ = Λe : D − Λe : Dp . Thus p
τ
= −Λe : Dp .
Clearly, there is an identity p
τ
: De = −τ : Dp = −Dp : Λe : De .
Problem 26.13. If the material obeys the Ilyushin’s postulate of nonnegative net work in
an isothermal cycle of strain, then p
τ
: D < 0.
Show that
τ e : Dp > 0 ,
τ e : D > 0,
p
τ
: Dp < 0 ,
τ : De > 0 ,
and
τ : Dp > −Dp : Λe : Dp .
Problems 26.13–26.14
809 p
Solution: Since from Problem 26.13, τ p
τ
= −Λe : Dp , we have
: D = −Dp : Λe : D = −Dp : τ e < 0 .
This proves the ﬁrst inequality. The second inequality follows immediately, because p
τ
: Dp = −Dp : Λe : Dp < 0 ,
the elastic moduli tensor being positive deﬁnite. Similarly, the third and fourth inequality follow from
τ e : D = D : Λe : D > 0 , and
τ : De = De : Λe : De > 0 . The last inequality is deduced from
τ e : Dp = τ − τ p : Dp > 0 .
This gives
τ : Dp + Dp : Λe : Dp > 0 , i.e.,
τ : Dp > −Dp : Λe : Dp .
If elastoplastic material is in the hardening range, then τ : Dp > 0. Problem 26.14. Consider a pressurized hollow sphere. At an instant when the applied
pressure over its internal surface is p, and its inner and outer radii are a and b, determine the stress ﬁeld within the sphere, assuming that it is made from elastically rigid, powerlaw plastic material, governed by the constitutive expression 1/2 m σi j J2 1/2 , m ≥ 1 , J2 < K0 . Di j = γ˙0 1/2 K0 J2 Note that for m = 1 the model corresponds to linearly viscous material, while rigid ideally plastic material is obtained in the limit m → ∞. Solution: The nonvanishing velocity component is the radial velocity vr = vr (r ). The rate
of deformation components are Drr =
dvr , dr
Dθ θ = Dφφ =
vr . r
The incompressibility constraint is Drr + Dθ θ + Dφφ = 0
⇒
vr dvr +2 = 0, dr r
810
Problem 26.14
which can be integrated to give vr =
A . r2
Thus, Drr = −
2A , r3
Dθ θ = Dφφ =
A . r3
The nonvanishing stress components are σrr and σθ θ = σφφ , with the corresponding deviatoric parts 2 σrr = − (σθ θ − σrr ), 3
σθ θ = σφφ =
1 (σθ θ − σrr ) . 3
In the considered problem the radial stress is compressive and the hoop stress tensile, so that 1/2
J2
1 = √ (σθ θ − σrr ) . 3
Thus, from the constitutive expression we can write √ 1/m 1 3 A . √ (σθ θ − σrr ) = K0 γ˙0 r 3 3 On the other hand, the equilibrium equation is dσrr 2 + (σθ θ − σrr ) = 0 dr r
⇒
σθ θ − σrr =
r dσrr . 2 dr
Combining this with the previous expression gives √ 1/m 1 r dσrr 3 A = K0 , √ γ˙0 r 3 3 2 dr and, upon integration, 2m σrr = − √ K0 3
√
1/m 3A r −3/m + B . γ˙0
The boundary conditions at the considered instant of deformation process are σrr (r = a) = − p ,
σrr (r = b) = 0 .
They give 2m B = √ K0 3 2m √ K0 3
√
√
1/m 3A b−3/m + B , γ˙0
1/m p 3A = − −3/m . γ˙0 b − a −3/m
Problems 26.14–27.3
811
The stresses are consequently σrr = − p
b−3/m − r −3/m , b−3/m − a −3/m
σθ θ = σφφ = − p
3 )r −3/m b−3/m − (1 − 2m . −3/m −3/m b −a
The radial velocity is γ˙0 vr = √ 3
"√
p 3 −3/m 2m K0 (b − a −3/m)
#m
1 . r2
CHAPTER 27 Problem 27.1. Consider a uniaxial tension of a single crystal rod of fcc nickel, oriented with the [100] direction parallel to the rod axis. Calculate the Schmid factor for the slip system {111}, involved in the plastic ﬂow of nickel. Solution: The angle between the loading axis [100] and the slip plane normal [111] is
determined from 1 1 1 cos φ = {0, 0, 1} · √ , √ , √ 3 3 3
!
1 =√ , 3
φ = 54.7◦ .
¯ The angle between the loading axis [100] and the slip direction [101] is determined from ! 1 1 1 cos ψ = {0, 0, 1} · − √ , 0, √ = √ , ψ = 45◦ . 2 2 2 Thus, the Schmid factor is 1 1 1 S.F. = cos φ cos ψ = √ √ = √ = 0.408 . 3 2 6 Problem 27.2. It was found that a cylindrical rod of the cross sectional area A = 5 cm2 ,
¯ is oriented made from zinc, yields at the axial load 2.1 kN, if the slip system (0001), [1120] ◦ ◦ such that φ = 83.5 and ψ = 18 . Calculate at what load will the rod yield if the slip system is oriented relative to the axial load such that φ = 13◦ and ψ = 78◦ . Solution: The ﬁrst information speciﬁes the critical resolved shear stress of the slip system
τcr =
2.1 cos 83.5◦ cos 18◦ = 452.2 kPa . 5 × 10−4
The crystal will therefore yield in the second case if the load is F=
Aτcr 5 × 10−4 × 452.2 = = 1.12 kN . cos 13◦ cos 78◦ cos 13◦ cos 78◦
Problem 27.3. Derive the necking condition in a uniaxial tension test. Assuming material
incompressibility, and the stressstrain relationship σ = K n , determine the strain at the onset of necking, and the corresponding maximum force.
812
Problems 27.3–27.4
tn n
F
τb
b s glide plane
Figure 271. A curved segment of dislocation with the Burgers vector b within the glide plane whose unit normal is n. The traction vector at a point of the dislocation is tn .
Solution: The applied force is F = σ A, where σ is the true stress and Athe current cross
sectional area. Thus, dF = dσ A+ σ dA. Necking occurs at the maximum load, where dF = 0 and dA dσ =− . σ A This is the necking condition. If the plastic strain is large and dominates the elastic strain component, one can assume the overall incompressibility, i.e., AL = const., where L is the current length of the specimen. Consequently, dAL + AdL = 0
⇒
−
dA dL = = d . A L
Combining this with the previously derived necking condition, we obtain dσ =σ. d If σ = K n , this gives the necking strain = n. The corresponding maximum force is n n . Fmax = K A0 e Problem 27.4. A glide force on an inﬁnitesimal dislocation segment, which is normal to
the dislocation line, is deﬁned as F = bτb, where b is the magnitude of the Burgers vector b of the curved dislocation, and τb the resolved shear stress over the glide plane and in the direction of b. Derive the expression for this force in terms of the stress tensor σi j . Solution: By the Cauchy relation, the components of the traction vector and the stress
tensor at an arbitrary point of the dislocation line (Fig. 271) are related by tin = σi j n j . Thus, the Peach–Koehler glide force is F = bτb = bi tin = bi σi j n j .
Problems 27.4–27.5
813
τ F1
F2
F3
F4
Fn
Figure 272. A dislocation pileup against a grain boundary. There are n dislocations in the pileup, which is under remote shear stress τ .
...
F0 1
2
3
4
n
τ If s is the unit vector along the dislocation line, the vectorial expression for the glide force is F = bτb(n × s) = (b · σ) × s . Problem 27.5. Consider a dislocation pileup at a strong obstacle, such as grain boundary (Fig. 272). The mutual repulsion of the dislocations tends to spread out the dislocation arrangement, while the applied shear stress drives the dislocations closer together against the obstacle. If there are n dislocations in the pileup, calculate the force F0 exerted on the obstacle. Solution: Let the Burgers vector of the edge dislocations be b, and the applied shear stress τ . The dislocation forces on the dislocations from the pileup are
F1 = τ b + F1,2 + F1,3 + F1,4 + . . . + F1,n , F2 = τ b − F2,1 + F2,3 + F2,4 + . . . + F2,n , F3 = τ b − F3,1 − F3,2 + F3,4 + . . . + F3,n , . . . . . . . . . . . . . . . . . . etc. . . . . . . . . . . . . . . . . . . , Fn = τ b − Fn,1 − Fn,2 − Fn,3 − . . . − Fn,n−1 , where Fi, j is the interaction force on the ith dislocation due to the jth dislocation. Clearly, Fi, j = F j,i . In the equilibrium pileup conﬁguration, each dislocation is in the equilibrium, so that F1 − F0 = 0 ,
F2 = F3 = . . . = Fn = 0 .
Thus, by summing up the expressions for the dislocation forces, we obtain n
Fi = F1 = nτ b ,
i=1
because the interaction forces cancel each other, n n i=1 j=1
Fi, j = 0 .
814
Problems 27.5–28.1
σ
B
Ψ0
Figure 281. Simple shearing along the slip direction, which is at an angle ψ0 in the undeformed conﬁguration, and ψ in the deformed conﬁguration (relative to longitudinal directions of the rod l0 and l). The resulting shear strain is γ = B0 B/ h.
B0
l h
l0 Ψ
B
B0
A0
h
ϕ
A0
σ
(a)
(b)
Therefore, the force exerted on the obstacle is F0 = F1 = nτ b . CHAPTER 28 Problem 28.1. Consider a plastic extension of the rod produced by a single slip of amount
γ as depicted in Fig. 281. Assume that the slip plane normal, the slip direction and the loading axis of the rod are all in one plane. Derive the relationship between the longitudinal stretch ratio l/l0 and the slip induced shear strain γ . Solution: The shear strain in an element of the rod of initial length l0 because of slip of
amount B0 B over the slip plane and in the slip direction is γ = tan ϕ =
B0 B . h
From the geometry of the triangle A0 B 0 B we have h = l0 sin ψ0 = l sin ψ , B 0 B = l cos ψ − l0 cos ψ0 . Since
" #1/2 1/2 l 2 2 2 l cos ψ = l 1 − sin ψ = l0 − sin ψ0 , l0
Problems 28.1–28.2
815
n σ
n
Figure 282. Single crystal under uniaxial tension oriented for single slip along the slip direction s0 in the slip plane with the normal m0 ; parts (a) and (b). The lattice rotates during deformation so that the slip direction s in the deformed conﬁguration makes an angle ψ with the longitudinal direction n; part (c). The angle between the slip plane normal m and the longitudinal direction is φ. The vectors m0 , s0 , and n, in general, do not belong to one plane.
φ m0
m0 s0
m
Ψ
s0
s
σ (a)
(c)
(b)
we can write B0 B = l0
⎧" ⎨ l 2 ⎩
l0
#1/2 − sin2 ψ0
− cos ψ0
⎫ ⎬ ⎭
.
Therefore, the shear strain γ is related to the stretch ratio l/l0 by ⎧" ⎫ #1/2 2 ⎬ l 1 ⎨ γ = − sin2 ψ0 − cos ψ0 . ⎭ sin ψ0 ⎩ l0 If the slip plane normal does not belong to the plane formed by the loading axis and the slip direction, the above expression generalizes to ⎧" ⎫ #1/2 2 ⎬ l 1 ⎨ − sin2 ψ0 − cos ψ0 , γ = ⎭ cos φ0 ⎩ l0 as originally derived by Schmid and Boas. Problem 28.2. Derive an expression for the instantaneous modulus H = dσ/de of a rigid
plastic crystal oriented for single slip under uniaxial tension. Show that the lattice rotation can cause an apparent softening of the crystal, even when the slip direction is still hardening. Solution: Consider a specimen under uniaxial tension oriented for single slip along the
direction s0 , on the slip plane with the normal m0 (see Fig. 282). The corresponding rate of deformation and the spin tensors can be expressed from the equations derived in text as D=
1 (P P) : σ, a
W = W∗ +
1 (Q P) : σ, a
816
Problem 28.2
where a = h − P : (Q · σ − σ · Q), and P=
1 (s m + m s), 2
Q=
1 (s m − m s). 2
Suppose that the specimen is under uniaxial tension in the direction n, which is ﬁxed by the grips of the loading machine. The Cauchy stress tensor is then σ = σ n n, the material spin is W = 0, and
σ = σ˙ n n. It follows that
P : σ = σ˙ (m · n)(s · n) = σ˙ cos φ cos ψ, where φ is the angle between the current slip plane normal m and the loading direction n, while ψ is the angle between the current slip direction s and the loading direction n, as shown in Fig. 282. It is easily found that P : (Q · σ − σ · Q) =
1 1 σ (m · n)2 − (s · n)2 = σ (cos2 φ − cos2 ψ). 2 2
Therefore, upon substitution into the expression for the rate of deformation, D=
σ˙ cos φ cos ψ h − (cos2 φ − cos2 ψ) 1 2
P.
Denoting by e the longitudinal strain in the direction of the specimen axis n, we can write e˙ = n · D · n, and therefore e˙ =
σ˙ cos2 φ cos2 ψ h − 12 (cos2 φ − cos2 ψ)
,
i.e., σ˙ = He˙ ,
H=
h σ (cos2 φ − cos2 ψ) − . cos2 φ cos2 ψ 2 cos2 φ cos2 ψ
Depending on the current orientation of the active slip system, the instantaneous modulus H can be positive, zero, or negative. If the lattice has rotated such that cos2 φ − cos2 ψ >
2h , σ
the current modulus is negative, although the slip direction may still be hardening (h > 0). The resulting apparent softening is purely geometrical effect, due to rotation of the lattice caused by crystallographic slip, and is referred to as geometric softening. In the derivation it was assumed that the lattice rotation does not activate the slip on another slip system.
Problems 28.3–29.1
817
Problem 28.3. Derive the expression (28.78), i.e., show that
˙ ∗ · F∗T + D∗ · τ ∗ + τ ∗ · D∗ . τ ∗ = F∗ · Λ∗ : E Solution: We start from the relationship between the symmetric Piola–Kirchhoff stress relative to the lattice and the corresponding Kirchhoff stress τ ∗ = (det F∗ )σ,
S∗ = F∗ −1 · τ ∗ · F∗ −T . Applying the time like derivative, we obtain . . S˙ ∗ = F∗ −1 · τ ∗ · F∗ −T + F∗ −1 · τ˙ ∗ · F∗ −T + F∗ −1 · τ ∗ · F∗ −T . Since
. F∗ −1 = −F∗ −1 · F˙ · F∗ −1 = −F∗ −1 · L∗ ,
the previous expression can be rewritten as S˙ ∗ = F∗ −1 · τ˙ ∗ − L∗ · τ ∗ − τ ∗ · L∗ T · F∗ −T . The bracketed term is the convected rate of the Kirchhoff stress relative to the lattice,
τ ∗ = τ˙ ∗ − L∗ · τ ∗ − τ ∗ · L∗ T = τ ∗ − D∗ · τ ∗ − τ ∗ · D∗ , where
τ ∗ = τ˙ ∗ − W∗ · τ ∗ + τ ∗ · W∗ is the Jaumann rate corotational with the lattice. Thus, we obtain
τ ∗ = F∗ · S˙ ∗ · F∗T + D∗ · τ + τ · D∗ . Finally, since ˙∗, S˙ ∗ = Λ∗ : E we arrive at the desired result. If plastic deformation is assumed to be volume preserving, then det F∗ = det F and τ ∗ = τ . CHAPTER 29 Problem 29.1. Consider a plane strain bifurcation of an incompressible nonlinear elastic material from the state of biaxial stretch (λ1 = λ, λ2 = λ−1 ). Show that
σ 11 − σ 22 = 2µ∗ (D11 − D22 ) ,
σ 12 = 2µD12 ,
where 2µ =
λ4 + 1 (σ1 − σ2 ) , λ4 − 1
Solution: Let the bifurcation strain rate
D=
D11 D12
4µ∗ = λ
D12 . D22
d (σ1 − σ2 ) . dλ
818
Problem 29.1
be superposed to the biaxially stretched state with the deformation gradient and corresponding Cauchy stress 0 λ λ 0 σ1 0 F= 1 = , σ = . 0 λ2 0 σ2 0 λ−1 The rate of Lagrangian strain is 2 ˙ = FT · D · F = λ D11 E D12
D12 . λ−2 D22
For an incompressible material, the rate of the symmetric Piola–Kirchhoff stress is related to the convected rate of the Cauchy stress by S˙ = F−1 σ − D · σ − σ · D · F−T , i.e.,
S˙ 11 S˙ 12
" −2 S˙ 12 λ (σ 11 − 2σ1 D11 ) = S˙ 22 σ 12 − (σ1 + σ2 )D12
σ 12 − (σ1 + σ2 )D12
#
λ2 (σ 22 − 2σ2 D22 )
The rates of stress and strain are related by S˙ i j = i jkl E˙ kl , which gives S˙ 11 = 1111 E˙ 11 + 1122 E˙ 22 , S˙ 22 = 2211 E˙ 11 + 2222 E˙ 22 , S˙ 12 = 21212 E˙ 12 . The (symmetric) instantaneous elastic moduli are from (7.100) given by 1111 =
1 ∂ S1 , λ1 ∂λ1
1122 =
1 ∂ S1 S1 − S2 + 2 , λ2 ∂λ2 λ1 − λ22
2222 =
1 ∂ S2 , λ2 ∂λ2
2211 =
1 ∂ S2 S1 − S2 + 2 , λ1 ∂λ1 λ1 − λ22
1212 =
S1 − S2 , λ21 − λ22
1112 = 2212 = 0 .
Upon combining of the above results, we obtain S1 − S2 ∂ S1 ∂ S1 D11 , σ 11 = 2σ1 + λ31 − λ1 − 2 ∂λ1 ∂λ2 λ1 − λ22 ∂ S2 ∂ S2 S1 − S2 σ 22 = 2σ2 + λ32 − λ2 − 2 D22 , ∂λ2 ∂λ1 λ1 − λ22 S1 − S2 σ 12 = σ1 + σ2 + 2 2 D12 . λ1 − λ22 To derive the desired results, we recall that σ1 = λ21 S1 ,
σ2 = λ22 S2 ,
(λ1 = λ , λ2 = λ−1 ),
.
Problems 29.1–29.2
819
so that ∂(λ21 S1 ) ∂λ1 ∂(λ21 S1 ) ∂λ2 dσ1 = + . dλ ∂λ1 ∂λ ∂λ2 ∂λ This gives λ
dσ1 ∂ S1 ∂ S1 = 2σ1 + λ31 − λ1 , dλ ∂λ1 ∂λ2
and similarly λ
dσ2 ∂ S2 ∂ S2 = −2σ2 − λ32 + λ2 . dλ ∂λ2 ∂λ1
Recalling that D11 + D22 = 0 by the incompressibility constraint, we ﬁnally obtain 1 d λ (σ1 − σ2 ) (D11 − D22 ) , σ 11 − σ 22 = 2 dλ and
σ 12 =
λ4 + 1 (σ − σ ) D12 . 1 2 λ4 − 1
Problem 29.2. Derive the expressions for the moduli µ and µ∗ of the previous problem if
the strain energy function is of the Mooney–Rivlin type 1 1 1 = µ0 + β (IB − 3) − − β (I IB + 3) . 2 2 2 Solution: Since, in the threedimensional setting,
⎡
λ 0 F = ⎣0 λ−1 0 0
⎤ 0 0⎦ , 1
⎡
λ2 ⎣ B= 0 0
0 λ−2 0
⎤ 0 0⎦ , 1
we obtain IB = tr B = λ2 + λ−2 + 1,
I IB =
1 tr(B2 ) − (tr B)2 = −(λ2 + λ−2 + 1), 2
so that =
1 µ0 (λ2 + λ−2 − 2) . 2
Thus, σ1 = − p0 + λ1
∂ = − p0 + µ0 λ21 , ∂λ1
σ2 = − p0 + λ2
∂ = − p0 + µ0 λ22 . ∂λ2
Consequently, σ1 − σ2 = µ0 (λ2 − λ−2 ) ,
λ
∂ (σ1 − σ2 ) = 2µ0 (λ2 + λ−2 ) , ∂λ
and, therefore, µ = µ∗ =
1 µ0 (λ2 + λ−2 ) . 2
820
Problem 30.1
CHAPTER 30
A polycrystalline aggregate is considered to be macroscopically homogeneous by assuming that local microscopic heterogeneities (because of different orientation and state of hardening of individual crystal grains) are distributed in such a way that the material elements beyond some minimum scale have essentially the same overall macroscopic properties. This minimum scale deﬁnes the size of the representative macroelement or representative cell. The representative macroelement can be viewed as a material point in the continuum mechanics of macroscopic aggregate behavior. To be statistically representative of the local properties of its microconstituents, the representative macroelement must include a sufﬁciently large number of microelements. For example, for relatively ﬁnegrained metals, a representative macroelement of volume 1 mm3 contains a minimum of 1000 crystal grains. The concept of the representative macroelement is used in various branches of the mechanics of heterogeneous materials and is also referred to as the representative volume element. Experimental determination of the mechanical behavior of an aggregate is commonly based on the measured loads and displacements over its external surface. Consequently, the macrovariables introduced in the constitutive analysis should be expressible in terms of this surface data alone. Problem 30.1. Let
F(X, t) =
∂x , ∂X
det F > 0,
be the deformation gradient at the microlevel of description, associated with a (continuous and piecewise continuously differentiable) microdeformation within a crystalline grain, x = x(X, t). The reference position of the particle is X, and its current position at time t is x. Express the volume averages of the deformation gradient, rate of deformation gradient, velocity gradient, and Cauchy and Kirchhoff stress, all in terms of the surface data. Solution: The volume average of the deformation gradient over the reference volume V0
of the macroelement is F =
1 V0
F dV0 = V0
1 V0
x n0 dS0 , S0
by the Gauss divergence theorem. The unit outward normal to the bounding surface S0 of the macroelement volume is n0 . The volume average of the rate of deformation gradient, ∂v ˙ , F(X, t) = ∂X
˙ v = x(X, t),
where v is the velocity ﬁeld, is ˙ = F
1 V0
1 F˙ dV0 = V 0 V0
v n0 dS0 . S0
Problems 30.1–30.2
821
Table 34.1. Designation of slip systems in fcc crystals Plane Slip Rate Slip Direction
¯ (1¯ 11) b1 b2 b3 ¯ 1] ¯ [110] ¯ [011] [10
(111) a1 a2 a3 ¯ [101] ¯ [110] ¯ [011]
¯ (111) c1 c2 c3 ¯ [10 ¯ 1] ¯ [110] [011]
¯ (111) d1 d2 d3 ¯ [1¯ 10] ¯ [011] [101]
If the current conﬁguration is taken as the reference conﬁguration (x = X, F = I, F˙ = L = ∂v/∂x), the above equation gives the volume average of the velocity gradient 1 1 {L} = L dV = v n dS. V V V S The current volume of the deformed macroelement is V, and S is its bounding surface with the unit outward normal n. Enclosure within { } brackets is used to indicate that the average is taken over the deformed volume of the macroelement. Let P = P(X, t) be a nonsymmetric nominal stress ﬁeld within the macroelement. The nominal traction pn is related to the true traction tn by pn dS0 = tn dS. The volume average of the nominal stress is 1 1 P dV0 = X pn dS0 . P = V0 V0 V0 S0 If current conﬁguration is chosen as the reference, (P = σ, pn = tn ), and we have 1 1 {σ} = σ dV = x tn dS. V V V S Note that
τ dV0 = V0
σ dV = V
so that 1 τ = V0
x tn dS = S
x pn dS0 , S0
1 τ dV0 = V0 V0
x pn dS0 . S0
Problem 30.2. The slip in an fcc crystal occurs on the octahedral planes in the directions of the octahedron edges (see Fig. 301). There are three possible slip directions in each of the four distinct slip planes, making a total of 12 slip systems (if counting both senses of a slip direction as one) or 24 (if counting opposite directions separately). The positive senses of the slip directions are chosen as indicated in Table 34.1. The letters a, b, c, and d refer to four slip planes. With attached indices 1, 2, and 3, they designate the slip rates in the respective positive slip directions. If elastic (lattice) strains are disregarded, calculate the components of the rate of deformation tensor, expressed on the cubic axes, due to simultaneous slip rates in 12 slip directions. Solution: The components of the rate of deformation can be calculated from
D=
12 α=1
Pα γ˙ α =
12 1 α=1
2
(sα mα + mα sα ) γ˙ α ,
822
Problems 30.2–30.3
3
] 11 [101]
]
[0
11
]
[0
[101
[1 1
0]
2 ]
[110
Figure 301. Twelve different slip directions in fcc crystals (counting opposite directions as different) are the edges of the octahedron shown relative to principal cubic axes. Each slip direction is shared by two intersecting slip planes so that there is a total of 24 independent slip systems (12 if counting opposite slip directions as one).
1 where mα is the unit slip plane normal and sα is the slip direction. For example, the contribution from the slip rate γ˙ = a1 is obtained by using 1 m = √ (1, 1, 1), 3
1 s = √ (0, −1, 1), 2
which gives ⎛ 0 a 1 α α 1 (s m + mα sα ) a1 = √ ⎝−1 2 2 6 1
−1 −2 0
⎞ 1 0⎠ . 2
An analogous calculation proceeds for other slip rates, which yields the following expressions for the overall rate of deformation components √ 6 D11 = a2 − a3 + b2 − b3 + c2 − c3 + d2 − d3 , √ 6 D22 = a3 − a1 + b3 − b1 + c3 − c1 + d3 − d1 , √ 6 D33 = a1 − a2 + b1 − b2 + c1 − c2 + d1 − d2 , √ 2 6 D23 = −a2 + a3 + b2 − b3 − c2 + c3 + d2 − d3 , √ 2 6 D31 = −a3 + a1 + b3 − b1 + c3 − c1 − d3 + d1 , √ 2 6 D12 = −a1 + a2 − b1 + b2 + c1 − c2 + d1 − d2 . Problem 30.3. Determine the number of independent sets of ﬁve slips in an fcc crystal. Solution: An arbitrary rate of deformation tensor has ﬁve independent components (tr D = 0 for a rigidplastic crystal), and therefore can only be produced by multiple slip
Problem 30.3
823
over a group of slip systems containing an independent set of ﬁve. Of the C512 = 792 sets of ﬁve slips, only 384 are independent. The 408 dependent sets are identiﬁed as follows. First, only two of three slip systems in the same slip plane are independent. The unit slip rates along a1 , a2 , and a3 directions together produce the zero resultant rate of deformation. The same applies to three slip directions in b, c, and d slip planes. We can write this symbolically as a1 + a2 + a3 = 0,
b1 + b2 + b3 = 0,
c1 + c2 + c3 = 0,
d1 + d2 + d3 = 0.
Thus, if the set of ﬁve slip systems contains a1 , a2 , and a3 , there are C29 = 36 possible combinations with the remaining nine slip systems. These 36 sets of ﬁve slips cannot produce an arbitrary D, with ﬁve independent components, and are thus eliminated from 792 sets of ﬁve slips. Additional 3 × 36 = 108 sets, associated with dependent sets of three slips in b, c, and d planes, can also be eliminated. This makes a total of 144 dependent sets corresponding to the above constraints. Of the remaining 648 sets of ﬁve slips, 324 involve two slips in each of two slip planes with one in a third (6 × 32 × 6 = 324), whereas 324 involve two slips in one slip plane and one in each of the other three slip planes (4 × 34 = 324). In the latter group, there are 3 × 8 = 24 sets involving the combinations a1 − b1 + c1 − d1 = 0,
a2 − b2 + c2 − d2 = 0,
a3 − b3 + c3 − d3 = 0.
These expressions can also be interpreted as meaning that such combinations of unit slips produce zero resultant rate of deformation. The 24 sets of ﬁve slips, involving four slip rates according to above, can thus be eliminated (these sets necessarily consists of two slips in one plane and one slip in each of the remaining three slip planes). Additional 12 sets are eliminated, which correspond to conditions obtained from the above equations by adding , , or subtracting ai , . . . , di , one at a time, to each of the equation. A representative of these is a1 − b1 + c1 + d2 + d3 = 0. There are 4 × 33 = 132 dependent sets associated with a1 + b2 + d3 = 0,
a2 + b1 + c3 = 0,
a3 + c2 + d1 = 0,
b3 + c1 + d2 = 0.
Each group of 33 sets consists of 21 sets involving two slips in one plane and one slip in each of other three planes and 12 sets involving two slips in two planes and one slip in one , , , bi , and di , one at plane. Additional 84 sets can be eliminated by subtracting ai , a time, from the ﬁrst of the above set of equation, and similarly for the other three. This makes 12 groups of 7 sets. A representative group is associated with a1 + b2 − d1 − d2 = 0. Four of the 7 sets consist of two slips in two planes and one slip in one plane, whereas 3 sets consist of two slips in one plane and one slip in each of the other three planes. Finally, 12 more sets (making total of 228 dependent sets associated with the above set of equations , , and their equivalents) can be eliminated by subtracting appropriate one of ai , . . . , di from each of the 12 previous group equations. An example is −a1 + b1 + b3 + d1 + d2 = 0. They all involve two slips in each of two planes and one slip in another plane. In summary, there is a total of 408 dependent sets of ﬁve slips: 144 sets with three slips in the same plane, 108 sets with two slips in each of two planes and one in a third, and 156 sets with two slips in one plane and one slip in each of the other three planes. The total number of independent sets of ﬁve slips is 792 − 408 = 384. Taylor (1938a) originally considered only 216 sets as geometrically admissible (involving double slip in each of two
824
Problems 30.3–30.4
planes) and did not observe 168 admissible sets with double slip in only one plane. These were originally identiﬁed by Bishop and Hill (1951b). Problem 30.4. According to the Voigt assumption, when a polycrystalline aggregate is
subjected to the overall uniform strain, the individual crystals will all be in the same state of applied strain. Based on this assumption, calculate the effective elastic constants of an isotropic aggregate of cubic crystals. Solution: For a cubic crystal the elastic moduli can be expressed as
Cicjkl = c12 δi j δkl + 2c44 Ii jkl + (c11 − c12 − 2c44 )Ai jkl , where Ii jkl =
1 (δikδ jl + δil δ jk) , 2
and Ai jkl = ai a j akal + bi b j bkbl + ci c j ckcl . The vectors a, b, and c are the orthogonal unit vectors along the principal cubic axes, and the usual notation for the elastic constants c11 , c12 , and c44 is employed. Two independent linear invariants of Cicjkl are Ciic j j = 3(c11 + 2c12 ) ,
Cicji j = 3(c11 + 2c44 ).
Denote by κ and µ the overall (effective) bulk and shear moduli of an isotropic aggregate of cubic crystals. The corresponding elastic moduli are 2 Ci jkl = 2µIi jkl + κ − µ δi j δkl . 3 According to the Voigt assumption, when a polycrystalline aggregate is subjected to the overall uniform strain, the individual crystals will all be in the same state of applied strain (which gives rise to stress discontinuities across the grain boundaries). Thus, by requiring that the overall stress is the average of the local stresses, there follows Ci jkl = {Cicjkl }. Instead of performing the integration Ci jkl =
1 8π 2
Cicjkl d,
the effective polycrystalline constants can be obtained directly by observing that the linear invariants of Ci jkl and Cicjkl must be equal. Thus, equating the earlier expressions for Ciic j j and Cicji j to Cii j j = 9κ,
Ci ji j = 3κ + 10µ,
we obtain the Voigt estimates κ=
1 (c11 + 2c12 ), 3
µV =
1 (c11 − c12 + 3c44 ). 5
Problems 30.5–31.1
825
Problem 30.5. According to the Reuss assumption, when a polycrystalline aggregate is
subjected to the overall uniform stress, the individual crystals will all be in the same state of stress. Based on this assumption, calculate the effective elastic constants of an isotropic aggregate of cubic crystals. Solution: By requiring that the overall strain in the aggregate is the average of the local
crystalline strains, there follows Si jkl = {Sicjkl }. The components of elastic compliance tensor of cubic crystals (see Problem 14.6) are c12 1 Ii jkl δi j δkl + (c11 − c12 )(c11 + 2c12 ) 2c44 1 1 Ai jkl . + − c11 − c12 2c44
Sicjkl = −
Two independent linear invariants of Sicjkl are Siic j j =
3 , c11 + 2c12
Sicji j =
3 3(c11 + c12 ) + . (c11 − c12 )(c11 + 2c12 ) 2c44
The components of the elastic compliance tensor of an isotropic aggregate of cubic crystals are 1 1 1 1 Ii jkl + − δi j δkl , Si jkl = 2µ 3 3κ 2µ with the corresponding invariants Sii j j =
1 , κ
Si ji j =
1 5 + . 2µ 3κ
Consequently, the Reuss estimates are κ=
1 (c11 + 2c12 ), 3
5
µR =
4 c11 − c12
+
3
.
c44
It can be shown that µV is the upper bound and that µR is the lower bound on the true value of the effective shear modulus, i.e., µR ≤ µ ≤ µV . It can also be shown that the effective Lame´ constant is bounded such that λV ≤ λ ≤ λR . CHAPTER 31 Problem 31.1. Derive the ratetype constitutive equation given by (31.16) of the main
text. Solution: The deformation gradient is decomposed as
F = F∗ · Fp ,
826
Problem 31.1
with F˙ p · Fp−1 =
2
γ˙α sα mα .
α=1
The two Lagrangian strain measures, relative to the initial reference conﬁguration, are E=
1 T F ·F−I , 2
1 pT p F ·F −I , 2
Ep =
whereas E∗ =
1 ∗T ∗ F ·F −I . 2
These strain measures are related by E = FpT · E∗ · Fp + Ep . By differentiating, we obtain the relationship ˙ ∗ · Fp + FpT · C∗ · F˙ p · Fp−1 ˙ = FpT · E · Fp , E sym where C∗ = F∗T · F∗ . The above can be rewritten as ˙ · Fp−1 − C∗ · F˙ p · Fp−1 ˙ ∗ = Fp−T · E E sym The two symmetric Piola–Kirchhoff stress tensors are derived from the strain energy (E∗ ) by the gradient operations S∗ =
∂ , ∂E∗
S=
∂ , ∂E
with the connection S∗ = Fp · S · FpT . The relationship between the rates of the stress tensors S∗ and S is obtained by simple differentiation, which gives
S˙ ∗ = Fp · S˙ · FpT + 2 F˙ p · Fp−1 · S∗ sym . Finally, by taking the time derivative of S∗ = ∂ /∂E∗ , there follows ∂2 . ∂E∗ ∂E∗ When the previously derived expressions for S˙ ∗ and E˙ ∗ are substituted in this relationship, ˙∗, S˙ ∗ = Λ∗ : E
Λ∗ =
we obtain ˙ − S˙ = Λ : E
2
γ˙α Xα ,
α=1
where i jkl = Fim−1 F jn −1 ∗mnpq F pk−1 Fql −1 , p
p
p
p
and Xα = F p−1 · (Λ∗ : Aα + 2Bα ) · F p−1 .
Problems 31.1–32.2
827
The secondorder symmetric tensors Aα and Bα are deﬁned by Aα = [C∗ · (sα mα )]sym ,
Bα = [(sα mα ) · S∗ ]sym .
CHAPTER 32 Problem 32.1. Consider the total body force acting on the body of variable mass, whose
current volume is V and mass density ρ, i.e., b ρ dV , Fb = V
where b is the body force per unit current mass. Derive an expression for the time rate of change of this force. Solution: Applying the time derivative to Fb , we have
d dFb = dt dt
b ρ dV = V
V
d (ρ b dV) = dt
db dV + ρ dt V
b V
d (ρ dV) . dt
Since d(ρdV) = r g dV , dt there follows dFb = dt
db g + r b dV . ρ dt V
In view of the continuity equation dρ + ρ ∇ · v = rg , dt we can also express the rate of the total body force acting on the body of variable mass as dρ dFb db = + + ρ ∇ · v b dV . ρ dt dt dt V If there is no mass growth, dρ + ρ ∇ · v = 0, dt the previous expression reduces to classical expression of the mechanics of constant mass dFb db = dV . ρ dt dt V rg = 0 ,
Problem 32.2. Consider a circumferential growth of a cylindrical blood vessel (Fig. 321). If the opening angle ( < 0 for growth; > 0 for resorption) is assumed to be constant along the thickness of the vessel, and if the plain strain conditions prevail, write down the components of the deformation gradients F, Fg , and Fe . Solution: The deformation mapping from the initial to current state is
r = r (R) ,
θ = ),
z = Z,
828
Problems 32.2–32.3
F
b0
b
a
a0
Fe Fg
b0
Figure 321. Circumferential growth of a cylindrical blood vessel. The opening angle is .
a0 Ω
where (R, ), Z) are the cylindrical coordinates in the initial conﬁguration and (r, θ, z) are those in the current conﬁguration. The corresponding deformation gradient at an arbitrary point of the vessel is ⎤ ⎡ dr/dR 0 0 F=⎣ 0 r/R 0⎦ . 0 0 1 A discontinuous mapping giving rise to an opening angle is ρ = R, ϑ = 1 − ) , ζ = Z, 2π where (ρ, ϑ, ζ ) are the cylindrical coordinates in the intermediate (stress free) conﬁguration. Thus, ⎤ ⎡ 1 0 0 Fg = ⎣0 . ω 0⎦ , ω = 1 − 2π 0 0 1 The elastic part of the deformation gradient Fe now follows composition F = Fe · Fg as ⎡ dr/dR 0 Fe = F · Fg −1 = ⎣ 0 r/(ω R) 0 0
from the multiplicative de⎤ 0 0⎦ . 1
Problem 32.3. Referring to previous problem, derive the expressions for the stress com
ponents in terms of the elastic principal stretches λre , λeθ , λez . Assume that the blood vessel is an incompressible elastic material with the strain energy function 1 α[exp(Q) − 1] − p(λre λeθ λez − 1) , 2 where α is a material parameter and p plays a role of the Lagrangian multiplier corresponding to the incompressibility constraint λre λeθ λez = 1. The function Q depends on the strain components according to W=
Problem 32.3
829
Q = β[(Ere )2 + (Eθe )2 + (Eze )2 ] , where β is another material parameter. The pressures on the inner and outer surface of the vessel, p0 and p1 , are assumed to be known. Solution: The elastic stretches in the previous problem are
λre =
dr , dR
λeθ =
1 r , ω R
λez = 1 .
In view of the incompressibility constraint λre λeθ λez = 1, we have dr r = ω, dR R
i.e.,
r 2 = ω R2 + C1 .
The integration constant is to be determined from the boundary condition at the inner (or outer) surface of the blood vessel. The Cauchy stress components can be expressed in terms of the principal stretches as σrr = λre
∂W − p, ∂λre
σθ θ = λeθ
∂W − p, ∂λeθ
σzz = λez
∂W − p. ∂λez
Since e err =
1 e 2 [(λ ) − 1] , 2 r
eθeθ =
1 e 2 [(λ ) − 1] , 2 θ
Eze =
1 e 2 [(λ ) − 1] , 2 z
we have Q=
1 e 2 β [(λr ) − 1]2 + [(λeθ )2 − 1]2 + [(λez )2 − 1]2 , 2
and ∂Q = 2βλre [(λre )2 − 1] , ∂λre
∂Q = 2βλeθ [(λeθ )2 − 1] , ∂λeθ
∂Q = 0. ∂λez
Consequently, ∂W p = αβλre [(λre )2 − 1] exp(Q) − e , e ∂λr λr p ∂W = αβλeθ [(λeθ )2 − 1] exp(Q) − e . ∂λeθ λθ Therefore, the stress components become σrr = αβ(λeθ )2 [(λeθ )2 − 1] exp(Q) − p , σθ θ = αβ(λeθ )2 [(λeθ )2 − 1] exp(Q) − p , σzz = − p . The explicit determination of the function p = p(r ) requires a numerical solution of the differential equation of equilibrium σrr − σθ θ dσrr + = 0. dr r
830
Problems 32.3–33.1
F n
n
ei
Figure 331. The membrane element of area dS 0 is mapped by the deformation gradient F into an element with area dS. The corresponding unit normal vectors are n0 and n. The inplane membrane vectors ei0 are transformed into ei = F · ei0 (i = 1, 2).
0
e0i
dS
dS0
The integration constant is speciﬁed by imposing the remaining boundary condition on the inner or outer surface of the blood vessel. Problem 32.4. Show that in the case of isotropic uniform growth of a spherical blood
vessel, there are no stresses due to growth alone. Solution: The deformation mapping due to growth alone is
ρ = λg R ,
ϕ=
,
ϑ = ),
where (R, , )) are the spherical coordinates in the initial conﬁguration, and (ρ, ϕ, ϑ) in the intermediate conﬁguration. The growth stretch ratio is λg . The corresponding deformation gradient at an arbitrary point of the vessel is ⎤ ⎡ ⎤ ⎡ g 0 0 λ dρ/dR 0 0 F=⎣ 0 ρ/R 0 ⎦=⎣0 0 ⎦. λg 0 0 ρ/R 0 0 λg This is clearly a pure dilatation. If there is no pressure applied to inner or outer surface of the vessel, we have r = ρ = λg R ,
φ=ϕ=
,
θ = ϑ = ),
where (r, φ, θ ) are the spherical coordinates in the current conﬁguration. Thus, F = Fg and Fe = I. Since Fe = I, there are no stresses in the blood vessel during its isotropic uniform growth alone. CHAPTER 33 Problem 33.1. Derive the relationship for the fractional change in reference area of the
membrane α = λ1 λ2 − 1, where λ1 and λ2 are the principal stretches in the tangent plane of the membrane. Solution: Let n0 = e01 × e02 be the unit normal vector to the membrane element in the
undeformed conﬁguration, where e01 and e02 are the orthogonal unit vectors in the tangent plane of the membrane in the directions of its principal membrane stretches (Fig. 331). Then, the right Cauchy–Green stretch tensor is U = λ1 e01 e01 + λ2 e02 e02 + λ3 n0 n0 . The Nanson’s relation (4.74) provides an expression for the area change of the surface element according to ndS = (det F)F